This book reviews up-to-date ideas of how the luminescence radiation in semiconductors originates and how to analyze it

*509*
*44*
*8MB*

*English*
*Pages 560
[557]*
*Year 2012*

- Author / Uploaded
- Ivan Pelant
- Jan Valenta

*Table of contents : CoverContents1. Introduction References2. Experimental techniques of luminescence spectroscopy 2.1 Emission and excitation spectra 2.2 Types of photodetectors 2.3 Monochromators and spectrographs 2.3.1 Dispersion and resolving power 2.3.2 Throughput of monochromators and spectrographs 2.4 Signal detection methods in luminescence spectroscopy 2.4.1 Phase-synchronous detection 2.4.2 Photon counting 2.5 Signal-to-noise ratio in a scanning monochromator 2.6 Fourier luminescence spectroscopy 2.7 Spectral corrections 2.8 Influence of slit opening on the shape of emission spectra 2.9 Time-resolved luminescence measurements 2.9.1 Direct imaging of the luminescence response 2.9.2 Phase-shift method 2.9.3 Time-correlated photon counting 2.9.4 Boxcar integrator 2.9.5 Streak camera 2.10 Problems References3. Kinetic description of luminescence processes 3.1 Radiative and non-radiative recombination. Luminescence quantum yield 3.2 Monomolecular process 3.3 Bimolecular process 3.4 Stretched exponential 3.5 Multiple processes present simultaneously 3.6 Problems References4. Phonons and their participation in optical phenomena 4.1 Lattice vibrations—phonons 4.2 Electron–phonon and exciton–phonon interactions 4.3 Lattice vibrations associated with point defects 4.4 A localized optical centre in a solid matrix—the configurational coordinate model 4.5 The shape of absorption and emission spectra of a localized centre 4.6 Thermal quenching of luminescence 4.7 Problems References5. Channels of radiative recombination in semiconductors 5.1 Overview of luminescence processes in crystalline semiconductors 5.2 Recombination of free electron–hole pairs 5.2.1 Direct bandgap 5.2.2 Indirect bandgap 5.3 Recombination of a free electron with a neutral acceptor (e–A[sup(0)]) and of a free hole with a neutral donor (h–D[sup(0)]) 5.4 Recombination of donor–acceptor pairs (D[sup(0)]–A[sup(0)]) 5.5 Luminescence excited by two-photon absorption 5.6 Luminescence from transition metal and rare earth ion impurities 5.7 Problems References6. Non-radiative recombination 6.1 Transformation of the excitation energy into heat 6.1.1 Multiphonon recombination 6.1.2 Auger and bimolecular recombination 6.2 Creation of lattice defects 6.3 Photochemical changes 6.4 Problems References7. Luminescence of excitons 7.1 Concept of the Wannier exciton 7.1.1 Absorption spectrum of the Wannier exciton 7.1.2 Direct bandgap: resonant luminescence of free exciton–polaritons 7.1.3 Direct bandgap: luminescence of free excitons with emission of optical phonons 7.1.4 Luminescence of free excitons in indirect-bandgap semiconductors 7.2 Bound excitons 7.2.1 Excitons bound to shallow impurities 7.2.2 Quantitative luminescence analysis of shallow impurities in silicon 7.2.3 Excitons bound to isoelectronic impurities 7.2.4 Self-trapped excitons 7.3 Problems References8. Highly excited semiconductors 8.1 Experimental considerations 8.2 Excitonic molecule or biexciton 8.2.1 Identification of the EM emission line 8.2.2 Determination of biexciton parameters 8.3 Collisions of free excitons 8.4 Electron–hole liquid (EHL) 8.4.1 Luminescence determination of EHL parameters 8.4.2 Identification of the EHL emission band 8.4.3 Coexistence of excitonic molecules with electron–hole liquid 8.5 Electron–hole plasma (EHP) 8.5.1 Mott transition 8.5.2 Luminescence of EHP 8.6 Bose–Einstein condensation of excitons 8.6.1 Properties of the Bose–Einstein distribution 8.6.2 Luminescence experiment: Bose–Einstein condensation yes or no? 8.7 Problems References9. Luminescence of disordered semiconductors 9.1 Densities of states in bands 9.2 Temperature dependence of luminescence 9.3 Distribution of luminescence lifetimes 9.4 Spectral shape of the emission band 9.5 Some other properties of luminescence of disordered semiconductors 9.5.1 Correlation effects 9.5.2 Non-radiative recombination 9.5.3 Luminescence of impurities and defects 9.5.4 Luminescence ‘fatigue’ 9.6 Problems References10. Stimulated emission 10.1 Spontaneous versus stimulated emission. Optical gain 10.2 Optical gain in semiconductors 10.3 Spectral shape of the optical gain 10.4 Stimulated emission in an indirect-bandgap semiconductor 10.5 Participation of excitons in stimulated emission 10.6 Experimental techniques for measuring the optical gain 10.6.1 Variable stripe length (VSL) technique 10.6.2 Pump and probe (P&P) method 10.7 Problems References11. Electroluminescence 11.1 Historical notes 11.2 High-field electroluminescence 11.2.1 Experimental considerations 11.2.2 Mechanisms of high-field electroluminescence 11.2.3 Intensity, spectral and temporal characteristics 11.3 Injection electroluminescence 11.3.1 Electrical properties of a p-n junction 11.3.2 Intensity, spectral and temporal characteristics of LEDs 11.4 Electroluminescence of a p-n junction biased in the reverse direction 11.5 Problems References12. Electronic structure and luminescence of low-dimensional semiconductors 12.1 Basic types of low-dimensional semiconductors 12.1.1 Semiconductor heterostructures 12.1.2 Basic types of quantum-well heterostructures 12.2 Density of states in low-dimensional semiconductors 12.3 Quantum wells (layers)—two-dimensional semiconductors 12.3.1 Single quantum well with in.nite barriers 12.3.2 Quantum well with finite barriers 12.3.3 Excitons in a quantum well 12.3.4 Optical transitions in a quantum well 12.3.5 Luminescence of quantum wells 12.4 Quantum wires 12.5 Quantum dots—nanocrystals 12.5.1 Quantum dot with spherically symmetric potential 12.5.2 Types of quantum dots according to the strength of the quantum con.nement effect 12.5.3 Luminescence of quantum dots 12.6 Exciton–phonon interaction. Phonon bottleneck 12.7 Some special phenomena 12.8 Problems References13. Effects of high excitation in low-dimensional structures 13.1 Excitonic molecule (biexciton) in a quantum well 13.2 Trions in a quantum well 13.3 Collisions of free excitons in a quantum well 13.4 Electron–hole plasma (EHP) and electron–hole liquid (EHL) in 2D structures 13.5 Biexcitons, EHP, and EHL in quantum wires 13.6 Effects of high excitation in quantum dots (nanocrystals) 13.7 Problems References14. Stimulated emission and lasing in low-dimensional structures 14.1 Stimulated emission in quantum wells 14.1.1 Localized excitons 14.1.2 Radiative decay of an exciton with emission of an LO-phonon (X–LO) 14.1.3 Stimulated emission in electron–hole plasma (EHP) 14.2 Stimulated emission in quantum wires 14.3 Stimulated emission in nanocrystals 14.3.1 Nanocrystals dispersed in a matrix 14.3.2 Heterostructures with ordered quantum dots 14.4 Random lasing 14.5 Problems References15. Silicon nanophotonics 15.1 Silicon nanocrystals 15.2 Optical gain in silicon nanocrystals 15.3 Active planar waveguides made of silicon nanocrystals 15.4 Electroluminescence of silicon nanocrystals 15.5 Silicon nanocrystals combined with Er[sup(3+)] ions 15.6 Biological applications of silicon nanocrystals 15.7 Problems References16. Photonic structures 16.1 Photonic crystals 16.1.1 Spontaneous emission 16.1.2 Stimulated emission 16.2 Microresonators 16.3 Microcavities 16.4 Single photon sources 16.5 Problems References17. Spectroscopy of single semiconductor nanocrystals 17.1 Basic principles 17.2 Experimental techniques 17.2.1 Wide-field micro-spectroscopy 17.2.2 Scanning techniques 17.3 Preparation of samples 17.3.1 Electron- and ion-beam lithography 17.3.2 Colloidal dispersions 17.4 Experimental observation of luminescence from individual nanocrystals 17.4.1 Hidden fine structure of luminescence spectra 17.4.2 Changes in spectra: jumps, shifts, blinking 17.4.3 Stark effect 17.4.4 Luminescence polarization 17.4.5 Luminescence intermittency—blinking 17.5 Nanocrystals as sources of non-classical photon flux 17.5.1 Measuring photon statistics 17.5.2 Experimental manifestation of non-classical light emitted by a single nanocrystal 17.6 Problems ReferencesAppendices A: Convolution B: Emission spectrum of free excitons including phonon broadening C: Luminescence of an excitonic molecule D: Kinetic model of exciton condensation E: Bose–Einstein condensation F: Emission band due to strong electron–phonon interaction G: Fitting the optical gain spectral shape in the model of k-relaxation H: Reabsorption of luminescence in semiconductors I: Oscillator strength J: Fitting with a double exponential (Kočka’s summation) K: Absolute quantum yield of luminescent materials L: Basic description of statistics of light from classical and non-classical sources M: Behaviour of multi-component spectral mixtures: the isostilbic pointSubject index A B C D E F G H I J K L M N O P Q R S T U V W X Y ZMaterial index A C G H I P Q R S T Y Z*

L U M I N E S C E N C E S P E C T RO S C O P Y O F SEMICONDUCTORS

This page intentionally left blank

Luminescence Spectroscopy of Semiconductors IVAN PELANT Institute of Physics, v.v.i. Academy of Sciences of the Czech Republic, Prague

JAN VALENTA Department of Chemical Physics and Optics Charles University, Prague

1

3

Great Clarendon Street, Oxford ox2 6DP Oxford University Press is a department of the University of Oxford. It furthers the University’s objective of excellence in research, scholarship, and education by publishing worldwide in Oxford New York Auckland Cape Town Dar es Salaam Hong Kong Karachi Kuala Lumpur Madrid Melbourne Mexico City Nairobi New Delhi Shanghai Taipei Toronto With ofﬁces in Argentina Austria Brazil Chile Czech Republic France Greece Guatemala Hungary Italy Japan Poland Portugal Singapore South Korea Switzerland Thailand Turkey Ukraine Vietnam Oxford is a registered trade mark of Oxford University Press in the UK and in certain other countries Published in the United States by Oxford University Press Inc., New York c Ivan Pelant and Jan Valenta 2012 The moral rights of the authors have been asserted Database right Oxford University Press (maker) First published 2012 All rights reserved. No part of this publication may be reproduced, stored in a retrieval system, or transmitted, in any form or by any means, without the prior permission in writing of Oxford University Press, or as expressly permitted by law, or under terms agreed with the appropriate reprographics rights organization. Enquiries concerning reproduction outside the scope of the above should be sent to the Rights Department, Oxford University Press, at the address above You must not circulate this book in any other binding or cover and you must impose the same condition on any acquirer British Library Cataloguing in Publication Data Data available Library of Congress Cataloging in Publication Data Data available Typeset by SPI Publisher Services, Pondicherry, India Printed and bound by CPI Group (UK) Ltd, Croydon, CR0 4YY ISBN 978–0–19–958833–6 10 9 8 7 6 5 4 3 2 1

To our families: Alena, Irena and Dita Helena, Jakub and David

This page intentionally left blank

Preface Luminescence of semiconductors has been widely used by many physicists, engineers and chemists for multiple purposes: For the study of the macroscopic optical properties of semiconducting materials as well as of their microscopic electronic processes, for the determination of purity and crystalline perfection of newly prepared compounds as well as of industrially grown single crystals, for the evaluation of the application prospects of novel active optoelectronic media, etc. The importance of luminescence techniques has considerably increased hand in hand with the recent rapid progress in low-dimensional semiconductor structures. The ﬁeld of luminescence has been evolving rapidly during recent years also thanks to the advanced and ever developing spectroscopic instrumentation. The purpose of this book is to introduce the reader to the study of the physical principles underlying semiconductor luminescence phenomena from the very beginning. Because, during the past 50 years, work on various types of luminescence radiation in semiconductors has been taking place in different streams, occurring mostly in different time periods, the relevant results are consequently scattered over many special monographs. The present book attempts to summarize the heart of the matter and to treat the whole subject in a unifying way. It is based on our one-semester course on ‘Luminescence spectroscopy of semiconductors’, read by us at the Faculty of Mathematics and Physics of Charles University in Prague for many years. For the purpose of the book we have extended our syllabus to cover a broader scope, by including especially a detailed treatment of experimental instrumentation (Chapter 2) and some theoretical parts, for example in Chapters 9, 10 and 12. Our own present interest has inﬂuenced the inclusion of Chapter 15; all other chapters, we believe, may serve as a general basis for many specialized and newly emerging branches of luminescence. It is understood that Chapters 12–17, devoted to luminescence phenomena of nanostructures, represent, on the one hand, an essential part of the book, and on the other hand, they should be regarded just as a ‘snapshot’ of the rapidly developing and versatile ﬁeld of nanoscience that will very soon be outdated. The level of presentation throughout the book, being based predominantly on verbal and graphical descriptions of the phenomena rather than on a rigorous quantum-mechanical treatment, has been chosen to be comprehensible to graduate university students. Of course, a basic knowledge of solid state physics (the crystalline and amorphous states, kspace, energy band structure, elementary statistics of electrons and holes) is required. We are indebted to many colleagues of ours for countless discussions over the years of cooperation, in particular to R. G. Elliman, B. H¨onerlage, J. Koˇcka, J. Linnros, P. Mal´y, A. Mysyrowicz, J. Oswald and K. Vacek. We appreciate the creative atmosphere in the Group of Thin Films and Nanostructures of

viii

Preface the Institute of Physics and the inspiring long-term tradition of luminescence research in the Department of Chemical Physics and Optics at the Faculty of Mathematics and Physics of Charles University in Prague, Czech Republic. We ˇ illustrate the text in part by our experimental results supported by the MSMT Centre LC510 and the Grant IAA101120804 of GAAVCR. We should like to thank Academia, Prague, for granting us the electronic version of the Czech edition to work from. The book was translated from Czech by K. Herynkov´a, ˇ K. K˚usov´a, J. Valenta, M. Zofka and I. Pelant under the editorial control of the last mentioned. Special thanks are due to V. Havl´ıcˇ ek for his invaluable technical support. The book would never have been accomplished without the helpful cooperation of Oxford University Press, in particular S. Adlung, A. Warman and C. Charles. Prague, May 2011 I. Pelant and J. Valenta

Contents 1 Introduction References

7

2 Experimental techniques of luminescence spectroscopy 2.1 2.2 2.3

Emission and excitation spectra Types of photodetectors Monochromators and spectrographs 2.3.1 Dispersion and resolving power 2.3.2 Throughput of monochromators and spectrographs

2.4

Signal detection methods in luminescence spectroscopy 2.4.1 Phase-synchronous detection 2.4.2 Photon counting

2.5 2.6 2.7 2.8 2.9

Signal-to-noise ratio in a scanning monochromator Fourier luminescence spectroscopy Spectral corrections Inﬂuence of slit opening on the shape of emission spectra Time-resolved luminescence measurements 2.9.1 2.9.2 2.9.3 2.9.4 2.9.5

1

Direct imaging of the luminescence response Phase-shift method Time-correlated photon counting Boxcar integrator Streak camera

2.10 Problems References

3 Kinetic description of luminescence processes Radiative and non-radiative recombination. Luminescence quantum yield 3.2 Monomolecular process 3.3 Bimolecular process 3.4 Stretched exponential 3.5 Multiple processes present simultaneously 3.6 Problems References

9 9 15 31 33 40 44 44 48 53 57 58 63 67 68 70 72 73 76 78 80

82

3.1

82 85 87 89 91 96 96

x

Contents

4 Phonons and their participation in optical phenomena 4.1 4.2 4.3 4.4

Lattice vibrations—phonons Electron–phonon and exciton–phonon interactions Lattice vibrations associated with point defects A localized optical centre in a solid matrix—the conﬁgurational coordinate model 4.5 The shape of absorption and emission spectra of a localized centre 4.6 Thermal quenching of luminescence 4.7 Problems References

5 Channels of radiative recombination in semiconductors 5.1 5.2

Overview of luminescence processes in crystalline semiconductors Recombination of free electron–hole pairs 5.2.1 Direct bandgap 5.2.2 Indirect bandgap

Recombination of a free electron with a neutral acceptor (e–A0 ) and of a free hole with a neutral donor (h–D0 ) 5.4 Recombination of donor–acceptor pairs (D0 –A0 ) 5.5 Luminescence excited by two-photon absorption 5.6 Luminescence from transition metal and rare earth ion impurities 5.7 Problems References

98 98 103 110 112 116 120 121 122

123 123 124 125 128

5.3

6 Non-radiative recombination 6.1

Transformation of the excitation energy into heat

132 135 139 144 146 147

148

6.2 Creation of lattice defects 6.3 Photochemical changes 6.4 Problems References

149 149 153 157 158 159 160

7 Luminescence of excitons

161

6.1.1 Multiphonon recombination 6.1.2 Auger and bimolecular recombination

7.1

Concept of the Wannier exciton 7.1.1 Absorption spectrum of the Wannier exciton 7.1.2 Direct bandgap: resonant luminescence of free exciton–polaritons 7.1.3 Direct bandgap: luminescence of free excitons with emission of optical phonons 7.1.4 Luminescence of free excitons in indirect-bandgap semiconductors

7.2

Bound excitons

162 165 168 171 177 180

Contents 7.2.1 Excitons bound to shallow impurities 7.2.2 Quantitative luminescence analysis of shallow impurities in silicon 7.2.3 Excitons bound to isoelectronic impurities 7.2.4 Self-trapped excitons

7.3 Problems References

8 Highly excited semiconductors 8.1 8.2

Experimental considerations Excitonic molecule or biexciton 8.2.1 Identiﬁcation of the EM emission line 8.2.2 Determination of biexciton parameters

8.3 8.4

Collisions of free excitons Electron–hole liquid (EHL) 8.4.1 Luminescence determination of EHL parameters 8.4.2 Identiﬁcation of the EHL emission band 8.4.3 Coexistence of excitonic molecules with electron–hole liquid

8.5

Electron–hole plasma (EHP) 8.5.1 Mott transition 8.5.2 Luminescence of EHP

8.6

Bose–Einstein condensation of excitons 8.6.1 Properties of the Bose–Einstein distribution 8.6.2 Luminescence experiment: Bose–Einstein condensation yes or no?

8.7 Problems References

9 Luminescence of disordered semiconductors 9.1 9.2 9.3 9.4 9.5

Densities of states in bands Temperature dependence of luminescence Distribution of luminescence lifetimes Spectral shape of the emission band Some other properties of luminescence of disordered semiconductors 9.5.1 9.5.2 9.5.3 9.5.4

Correlation effects Non-radiative recombination Luminescence of impurities and defects Luminescence ‘fatigue’

9.6 Problems References

10 Stimulated emission 10.1 Spontaneous versus stimulated emission. Optical gain 10.2 Optical gain in semiconductors

xi 182 190 194 199 201 202

205 206 207 208 216 218 220 223 226 228 230 230 232 234 234 236 239 240

242 242 244 248 250 255 255 256 258 260 261 262

263 263 267

xii

Contents 10.3 Spectral shape of the optical gain 10.4 Stimulated emission in an indirect-bandgap semiconductor 10.5 Participation of excitons in stimulated emission 10.6 Experimental techniques for measuring the optical gain 10.6.1 10.6.2

Variable stripe length (VSL) technique Pump and probe (P&P) method

10.7 Problems References

11 Electroluminescence 11.1 Historical notes 11.2 High-ﬁeld electroluminescence 11.2.1 11.2.2 11.2.3

Experimental considerations Mechanisms of high-ﬁeld electroluminescence Intensity, spectral and temporal characteristics

11.3 Injection electroluminescence 11.3.1 11.3.2

Electrical properties of a p-n junction Intensity, spectral and temporal characteristics of LEDs

11.4 Electroluminescence of a p-n junction biased in the reverse direction 11.5 Problems References

12 Electronic structure and luminescence of low-dimensional semiconductors 12.1 Basic types of low-dimensional semiconductors 12.1.1 12.1.2

Semiconductor heterostructures Basic types of quantum-well heterostructures

12.2 Density of states in low-dimensional semiconductors 12.3 Quantum wells (layers)—two-dimensional semiconductors 12.3.1 12.3.2 12.3.3 12.3.4 12.3.5

Single quantum well with inﬁnite barriers Quantum well with ﬁnite barriers Excitons in a quantum well Optical transitions in a quantum well Luminescence of quantum wells

12.4 Quantum wires 12.5 Quantum dots—nanocrystals 12.5.1 12.5.2 12.5.3

Quantum dot with spherically symmetric potential Types of quantum dots according to the strength of the quantum conﬁnement effect Luminescence of quantum dots

12.6 Exciton–phonon interaction. Phonon bottleneck 12.7 Some special phenomena 12.8 Problems References

271 278 282 287 287 295 299 300

302 302 304 304 308 316 321 322 327 333 336 337

339 340 340 342 344 347 347 351 353 355 357 359 363 363 365 368 371 374 378 379

Contents

13 Effects of high excitation in low-dimensional structures 13.1 13.2 13.3 13.4

Excitonic molecule (biexciton) in a quantum well Trions in a quantum well Collisions of free excitons in a quantum well Electron–hole plasma (EHP) and electron–hole liquid (EHL) in 2D structures 13.5 Biexcitons, EHP, and EHL in quantum wires 13.6 Effects of high excitation in quantum dots (nanocrystals) 13.7 Problems References

14 Stimulated emission and lasing in low-dimensional structures 14.1 Stimulated emission in quantum wells 14.1.1 Localized excitons 14.1.2 Radiative decay of an exciton with emission of an LO-phonon (X–LO) 14.1.3 Stimulated emission in electron–hole plasma (EHP)

14.2 Stimulated emission in quantum wires 14.3 Stimulated emission in nanocrystals 14.3.1 Nanocrystals dispersed in a matrix 14.3.2 Heterostructures with ordered quantum dots

14.4 Random lasing 14.5 Problems References

15 Silicon nanophotonics 15.1 Silicon nanocrystals 15.2 Optical gain in silicon nanocrystals 15.3 Active planar waveguides made of silicon nanocrystals 15.4 Electroluminescence of silicon nanocrystals 15.5 Silicon nanocrystals combined with Er3+ ions 15.6 Biological applications of silicon nanocrystals 15.7 Problems References

xiii

381 382 384 386 387 392 395 398 399

400 400 401 404 405 408 410 410 416 418 420 421

423 424 426 428 431 434 437 438 439

16 Photonic structures

441

16.1 Photonic crystals

441 443 446 447 449 451

16.1.1 Spontaneous emission 16.1.2 Stimulated emission

16.2 Microresonators 16.3 Microcavities 16.4 Single photon sources

xiv

Contents 16.5 Problems References

17 Spectroscopy of single semiconductor nanocrystals 17.1 Basic principles 17.2 Experimental techniques 17.2.1 17.2.2

Wide-ﬁeld micro-spectroscopy Scanning techniques

17.3 Preparation of samples 17.3.1 Electron- and ion-beam lithography 17.3.2 Colloidal dispersions

17.4 Experimental observation of luminescence from individual nanocrystals 17.4.1 17.4.2 17.4.3 17.4.4 17.4.5

Hidden ﬁne structure of luminescence spectra Changes in spectra: jumps, shifts, blinking Stark effect Luminescence polarization Luminescence intermittency—blinking

17.5 Nanocrystals as sources of non-classical photon ﬂux 17.5.1 17.5.2

Measuring photon statistics Experimental manifestation of non-classical light emitted by a single nanocrystal

17.6 Problems References

Appendices A B C D E F G H I J K L M

Convolution Emission spectrum of free excitons including phonon broadening Luminescence of an excitonic molecule Kinetic model of exciton condensation Bose–Einstein condensation Emission band due to strong electron–phonon interaction Fitting the optical gain spectral shape in the model of k-relaxation Reabsorption of luminescence in semiconductors Oscillator strength Fitting with a double exponential (Koˇcka’s summation) Absolute quantum yield of luminescent materials Basic description of statistics of light from classical and non-classical sources Behaviour of multi-component spectral mixtures: the isostilbic point

Subject index Material index

453 454

455 456 457 458 460 465 465 466 467 467 469 470 472 478 485 485 487 490 491

493 493 495 497 502 503 505 507 511 513 514 515 521 526 530 538

Introduction

Terminological notes By the term ‘luminescence of solids’ we understand a surplus of the electromagnetic (light) radiation, emitted by a solid, over its equilibrium radiation that can be described by Planck’s law.1 At the same time this radiation has to have a decay time much longer than the period of light oscillations (10−14 –10−15 s). Above all, it follows from this deﬁnition that, from the thermodynamical point of view, the luminescence is a non-equilibrium radiation. This means that the solid needs to be supplied in some way with extra energy (with respect to that being exchanged by the solid with its surroundings through the equilibrium electromagnetic radiation). This extra energy is transformed inside the medium into the luminescence radiation. The supplied extra energy is called excitation energy, and the luminescence can be classiﬁed according to the way the excitation energy is applied, as follows: Photoluminescence is excited with light (of wavelength λex , which is usually shorter than the emission wavelength λem . The relation λex ≤ λem is called Stokes’ law). Electroluminescence originates as a consequence of the application of an electric ﬁeld and the relevant electric current ﬂow through the material (do not confuse this with the thermal radiation due to the Joule heat!). Chemiluminescence accompanies certain types of exothermic chemical reactions—the released heat or part of it is radiated in the form of light. Bioluminescence coexists in a similar way with certain physiological biochemical reactions. Cathodoluminescence arises when a high-energy electron beam (102 –103 eV) impinges on a luminescent screen. Mechanoluminescence is light (usually a short ﬂash) emitted in some cases during mechanical deformation of a solid. Thermoluminescence occurs when a solid is ﬁrst cooled to a low temperature, then illuminated (excited) using short-wavelength electromagnetic 1 The notion of light should be understood here in a wider sense, namely, not only visible radiation, but also the near-infrared and ultraviolet regions.

1

2

Introduction radiation and ﬁnally its temperature is allowed to increase slowly, which is accompanied by emission of the luminescence radiation. Sometimes one can also encounter terms like X-ray luminescence (excitation by X-rays), sonoluminescence (excitation by acoustic or ultrasound vibrations), triboluminescence (luminescence due to friction when the material is scratched or crushed), etc. In recent years, light induced through injecting lowenergy electrons or holes (energy of the order of 1 eV) into a semiconductor or metal in a scanning tunnelling microscope is being investigated. In the case of metals, however, the term luminescence seems inappropriate, as luminescence in solid-state physics is—for historical reasons—connected with non-metallic solids, insulators and semiconductors. Therefore, here the term photon emission is used instead. The second part of the deﬁnition of luminescence, dealing with its ﬁnite decay time, differentiates luminescence from other types of so-called secondary radiation: reﬂected light, various types of scattered light (Rayleigh, Raman and Brillouin scattering) and Cerenkov radiation. The thing is that these kinds of radiation originate as an act of very fast photon–matter interaction and there is virtually no exchange of energy between the impinging photon and the electronic system of the solid. On the contrary, during the process of luminescence the electrons are excited to higher energy states, which entails genuine absorption of the excitation energy in the material and its subsequent gradual transformation. Consequently, the succession of all involved events lasts a relatively long time. For this reason, upon cessation of the excitation the luminescence continues to decay for some time. The lower bound of this time period gets shorter with the development of time-resolved spectroscopy techniques. Nowadays it can be considered to amount to hundreds of femtoseconds. (Of course, the scale of luminescence decay times is much broader and ranges from nanoseconds up to tens of hours.) The study of luminescence has a long history, in the course of which the relevant terminology has also been developing. Radiating rotten stumps or certain kinds of luminescent insect and ﬁsh have been known in Nature from time immemorial. Probably more than a thousand years ago the Chinese and Japanese knew about luminescent dyes. In the seventeenth century, the ‘Bolognian stone’ was described, emitting red light upon prior exposure to sunlight (nowadays we know that it was barium sulphide, BaS). This and similar stones were given the name phosphors and the relevant effect, i.e. long-term light emission after cessation of the excitation radiation, was named phosphorescence.2 Later on, in order to distinguish from phosphorescence, the term ﬂuorescence was introduced to designate light emission with an immeasurably short decay after stopping the excitation; this was observed for the ﬁrst time in ﬂuorite, CaF2 . The general term luminescence, comprising both

2 This has nothing to do with the chemical element P, phosphorus (in the sense that the luminescing substance would have to comprise P atoms), even if historical connection with phosphorus lighting itself can be traced; see Harvey E. Newton (2005). A History of Luminescence. From the Earliest Times until 1900. Dover Publications, Mineola.

Introduction phosphorescence and ﬂuorescence, was ﬁnally introduced towards the end of the nineteenth century. In the literature even the word phosphor occurs nowadays. Even if its meaning is not strictly speciﬁed, it usually denotes a luminescent solid in a wider sense. Also the meaning of the notions of phosphorescence and ﬂuorescence has shifted in time—presently, ﬂuorescence is sometimes understood as light emission occurring in the course of the excitation event, while in speaking of phosphorescence we have in mind non-equilibrium light emission observed during its decay, provided this decay is long enough to be observable by the naked eye. However, these terms are more exactly speciﬁed in the case of luminescence of organic substances. Luminescence of organic and inorganic materials Luminescence occurs in most organic substances (aromatic hydrocarbons like benzene, naphthalene, anthracene, organic dyes, etc.) as well as in many inorganic solids (ionic crystals, semiconductors). Its underlying origin, however, in both cases differs substantially. In organic matter, the role of a characteristic luminescence bearer (luminescence centre) is played by a molecule. This means that the essential features of the luminescence radiation (spectral content, decay time) in the solid state and in a solution are very much alike. This is because organic crystals are composed of molecules, the binding between them being mediated only by weak van der Waals forces. Therefore, the molecules keep their individuality to a large extent; the weak intermolecular forces are not strong enough to modify them substantially. The same, of course, is true in the case of a solution, thus the luminescence spectrum of organic matter has virtually the same shape in solution as well as in the solid state. The basic features of organic luminescence can thus be derived from the electron energy level scheme of large organic molecules (the Jablonski diagram). As is well known, the ground state of such a molecule is represented by a singlet state S0 , higher lying electronic states being mainly excited singlet states (S1 , S2 , S3 , . . . ). The higher excited singlet states S2 , S3 , . . . relax very rapidly to the S1 state and the transition S1 → S0 is accompanied by emission of a luminescence photon. This radiative transition is spin-allowed and, consequently, is fast (the characteristic time is of the order of 10−9 s) and is called ﬂuorescence. There are, however, also excited triplet states T1 , T2 , T3 , . . . The transition T1 → S0 can also be accompanied with photon emission, but is spinforbidden and thus slow (10−3 s). It is called phosphorescence. As for inorganic solids, especially semiconductors, speaking of a ‘molecule’ loses its meaning to a large extent (a molecule of silicon—does it exist?). Physical properties here, above all the development of the forbidden energy gap, etc., are conditioned by the existence of a minimal ensemble of at least several tens of atoms (sometimes called a ‘cluster’). However, real bulk properties can only be achieved in substantially larger objects with lateral dimensions at least 1μm that contain approximately 1010 atoms. We shall treat these bulk semiconductor luminescence properties in Chapters 5–11. Low-dimensional semiconductor structures are examined in Chapters 12– 17.

3

4

Introduction Intrinsic and extrinsic luminescence Solid-state luminescence can be divided into two basic types: • intrinsic (‘proper’); • extrinsic (‘improper’). Intrinsic luminescence originates in an ideal, pure and defect-free crystalline lattice, while extrinsic luminescence has its origin in lattice defects or impurities. (A similar classiﬁcation can be applied also to non-crystalline, disordered solids, provided we have in mind topological disorder of the amorphous network instead of the crystalline lattice.) A luminescence-active impurity (admixture) atom, ion or molecule is frequently called an impurity luminescence centre. Now, a natural question arises. If—in the extrinsic case—the luminescence radiation originates in a microscopic impurity centre, what then is the role of the host solid itself, i.e. the crystalline or amorphous matrix? This matrix fulﬁls multiple functions: (i) First of all, it represents a host medium inside which the luminescence centres are ﬁxed, statistically dispersed and mechanically isolated. However, this is by no means all; if we imagine these centres located in a similar way in a vacuum, they would either not emit any radiation at all or such radiation would be substantially weaker and of different spectral content. This means that (ii) the matrix also serves as an ‘antenna’ capturing the excitation energy and transferring it very efﬁciently to the luminescence centres. Next, (iii) owing to the interaction of the impurity electronic system with the matrix vibrations the electron energy levels undergo important modiﬁcations, which leads to substantial alterations of the optical spectra of the centre. Finally, (iv) in the special case of electroluminescence the matrix must ensure suitable electrical conductivity for exciting the centres. At present we know that in the beginning of the era of the modern quantitative study of luminescence phenomena in solids (dating roughly from the ﬁrst third of the nineteenth century to the 1950s), physicists and chemists were working exclusively with impurity, extrinsic luminescence. At that time, technology was not able to prepare sufﬁciently pure materials, while it is known today that most semiconductors owe their strong luminescence radiation to the presence of impurities. Even a negligible amount of residual impurity (1 ppm or less) can manifest itself in luminescence of enormous intensity, which masks or totally prevents intrinsic emission. This phenomenon, which will be discussed in Chapter 7, forms the basis of a sensitive qualitative and quantitative photoluminescence analysis of impurities in semiconductors. As a typical example of extrinsic emission we quote the luminescence of Cu+ or Mn++ ions in ZnS crystals, while the most characteristic example of intrinsic emission is luminescence due to the radiative decay of free excitons. Examples of luminescence spectra This book contains in its title the word spectroscopy. It follows that we shall largely deal with the interpretation of the emission spectral line shape of semiconductor luminescence. One of our goals is therefore aimed at analysing as much of the characteristic features of the experimentally acquired emission

Introduction

5

spectrum as possible, in order to assign the given spectral line to a speciﬁc microscopic luminescence centre or to some other channel of radiative recombination. Let us introduce here several examples of luminescence spectra. Figure 1.1 shows near-infrared photoluminescence spectra of three crystalline Si samples, measured at liquid-helium temperature (4.2 K) [1]. The A sample represents extremely pure silicon without intentional doping (i.e. without introducing electrically active impurities), with a low concentration of residual unintentional impurities—in the order of 1012 cm−3 only. The B sample contains impurities in the order of ∼ 1014 cm−3 and the sample C has even higher impurity concentration, > 1015 cm−3 . The notations of individual emission lines and bands will be clariﬁed in Chapters 7 and 8. The spectra are rich in structure, comprising both very narrow (almost atomic) lines and relatively broad bands. It might be interesting to draw the reader’s attention to the different characters of the spectral components: e.g. the lines denoted ILO (FE) and ITO (FE) are, as well as the band ILO,TO (EHL), of intrinsic origin, while the lines BTO (BE), PTO (BE), SbTO (BE) are of extrinsic origin.

Fig. 1.1 Photoluminescence spectra of three samples of crystalline silicon close to the bandgap energy. The B and C samples were doped with (Sb + As) and (B + As), respectively; the A sample was not intentionally doped (nominally pure silicon). The samples were immersed in liquid helium (T = 4.2 K) and excited with a continuous-wave (cw) Ar+ -laser, λex = 488 nm. After Valenta [1].

6

Fig. 1.2 (a) Photoluminescence spectra of pure AgCl at liquid-helium temperature under excitation with a pulsed N2 -laser (λex = 337 nm). Numbers near the curves denote temporal delays after the excitation pulse at which the spectra were recorded. After Pelant and H´ala [2]. (b) Photoluminescence spectrum of nominally pure AgBr at T = 7 K. The ﬁne structure superimposed on the broad band is due to interaction with lattice vibrations—phonons. After Wassmuth et al. [3].

Fig. 1.3 Cathodoluminescence spectra of ZnS doped with various metals (Me), the so-called activators: 1. ZnS/Zn, 2. ZnS/Cu, 3. ZnS/Ag, 4. ZnS/Au and 5. ZnS/Mn. T = 295 K. After Markovskii et al. [4].

Introduction Figure 1.2(a) displays photoluminescence spectra of a pure silver chloride, AgCl, crystal, measured also at low temperature, 2 K, and under various modes of excitations [2]. Even if silver halides AgCl, AgBr are not typical semiconductors, their optical and, in particular, luminescence properties render them close to the family of wide-bandgap polar semiconductors. (Interestingly, at the same time, their mechanical properties are similar to those of metals.) In this context, they represent important model substances and throughout the book we shall often refer to their luminescence behaviour. The spectra contain a very broad emission band (full width at half maximum, FWHM, ∼ 0.4 eV) at ∼ 500 nm (2.5 eV) and, besides this, an indication of a weaker band at ∼ 420 nm. Both bands are of intrinsic origin. The spectrum is situated in the visible region—under ultraviolet excitation and at low temperature AgCl exhibits very bright blue-green luminescence. Figure 1.2(b) shows the lowtemperature (7 K) photoluminescence spectrum of nominally pure crystalline silver bromide, AgBr [3]. This material closely resembles AgCl both in chemical composition and in crystalline structure, and also the spectra displayed in Figs 1.2(a) and (b) are very much alike in their spectral position as well in their width. Despite these similarities, there is a fundamental difference in the origin of luminescence: Contrary to AgCl, the emission band at 2.5 eV in AgBr has extrinsic origin (!). (Another interesting observation is the ‘ﬁne structure’ superimposed on the broad emission band in AgBr, which is completely absent in AgCl. The interpretation of these effects will be given in Chapter 7.) Finally, Fig. 1.3 demonstrates room-temperature emission spectra of zinc sulphide ZnS doped with various intentional impurities [4]. These broad extrinsic emission bands cover most of the visible region. From these examples we can already draw several conclusions. First of all, it becomes quite obvious that—unfortunately—neither the shape nor the width of the emission spectrum can be used for judging the intrinsic or extrinsic origin of luminescence. Undoubtedly, this would be very proﬁtable, but Nature does not reveal its mysteries so easily. Next, the reader has probably noticed

Introduction

7

Fig. 1.4 Cathodoluminescence spectrum of edge emission in a nominally pure ZnO crystal. Excitation by bombardment with a 7 keV electron beam, T = 4 K. Adapted from Tomzig and Helbig [5]. The arrow labels the position of the bandgap Eg = 3.436 eV (∼ 360.9 nm).

that most of the presented spectra are photoluminescence spectra, which anticipates the fact that the book is devoted predominantly to photoluminescence spectroscopy; the theory of electroluminescence and its applications are concentrated mainly in Chapter 11. Furthermore, the spectra displayed in Figs 1.1 and 1.2 were measured at very low temperatures. The reason for this is that the luminescence of most solids occurs only upon cooling them considerably below ordinary room temperature. And even if some materials luminesce at room temperature (Fig. 1.3), the intensity of this luminescence, as a rule, grows markedly in the course of cooling. This property contradicts ﬂagrantly the ordinary behaviour of thermal radiation of solids (incandescence), described by the Planck and Stefan–Boltzmann laws, and that is why luminescence is sometimes known as cold light. The drop of luminescence intensity with increasing temperature is called thermal quenching. Finally, in semiconductor luminescence one can encounter the term edge emission. This means luminescence radiation situated in the spectral range around the onset of interband optical absorption (absorption edge). More speciﬁcally, the energy of the luminescence photon hνem is only slightly less than the bandgap energy E g . The edge emission spectrum usually consists of a large number of narrow (excitonic) lines, both intrinsic and extrinsic. An example of the low-temperature edge emission in zinc oxide, ZnO, is shown in Fig. 1.4 [5]. The bandgap energy E g = 3.436 eV is marked by an arrow. The displayed wavelength range is very narrow, about 10 nm (90 meV); the individual lines are shifted with respect to E g by 0.01–0.1 eV only. Similarly, the spectra shown in Fig 1.1 can also be speciﬁed as edge emission.

References 1. Valenta, J. (1994). Photoluminescence characterization of selected semiconductors and insulators. PhD Thesis, Charles University in Prague, Faculty of Mathematics and Physics, Prague. 2. Pelant, I. and H´ala, J. (1991). Solid State Com., 78, 141.

8

Introduction 3. Wassmuth, W., Stolz, H., and von der Osten, W. (1990). J. Phys. C: Cond. Matter, 2, 919. 4. Markovskii, L. J., Pekerman, F. M., and Petoshina, L. N. (1966). Phosphors (in Russian: Ljuminofory). Chimija, Moskva, Leningrad. 5. Tomzig, E. and Helbig, R. (1976). J. Luminescence, 14, 403.

Experimental techniques of luminescence spectroscopy The aim of experimental luminescence spectroscopy is basically the same as that of other types of optical spectroscopy, namely, to disperse luminescence radiation into a spectrum, which is subsequently detected and recorded. Here, as a dispersion device, a monochromator or a polychromator is almost exclusively used; only exceptionally (in the case of Fourier luminescence spectroscopy) is an interferometer applied. Possible application of devices based on multiple-beam interference (Fabry–Perot interferometer, Lummer– Gehrke plate) brings no advantage as the luminescence spectra are usually broad and do not require extreme spectral resolution. Only exceptionally, e.g. in the case of narrow spectral lines of edge emission (Figs 1.1 and 1.4), a highresolution monochromator or possibly a Fourier spectrometer with resolving power R = (λ/λ) amounting at least to ∼ 5 × 103 (λ denotes the minimum separation between two spectral lines around a central wavelength λ that are to be resolved) is indispensible. Generally, what is characteristic for luminescence spectroscopy is typically an extremely low level of detected light ﬂux rather than requirements for extreme spectral resolution. Therefore, the spectral device must have the highest possible throughput, and special care must be devoted to selecting a sensitive photodetector and, in particular, to setting up an efﬁcient optical system to collect the luminescence signal. All these aspects will be discussed in this chapter.

2.1 Emission and excitation spectra The purpose of monochromators in luminescence spectroscopy is, on the one hand, to observe the spectral content of luminescence emission and, on the other hand (in the case of photoluminescence) they can also be applied to select a suitable excitation wavelength from an optical excitation source. The luminescence signal can be measured either as a function of emission wavelength at a ﬁxed excitation wavelength or vice versa. One speaks of emission and excitation spectra, respectively. A general scheme of luminescence experiment is shown in Fig. 2.1(a). The excitation source supplies excitation energy to the sample, emitted

2 2.1 Emission and excitation spectra

9

2.2 Types of photodetectors

15

2.3 Monochromators and spectrographs

31

2.4 Signal detection methods in luminescence spectroscopy

44

2.5 Signal-to-noise ratio in a scanning monochromator

53

2.6 Fourier luminescence spectroscopy

57

2.7 Spectral corrections

58

2.8 Inﬂuence of slit opening on the shape of emission spectra 63 2.9 Time-resolved luminescence measurements

67

2.10 Problems

78

10

Experimental techniques

Fig. 2.1 (a) Block diagram of a luminescence experiment, (b) the ‘transmission’ geometry, (c) the ‘back-reﬂection’ geometry, (d) collection of luminescence from the sample edge using a waveguiding effect.

luminescence radiation is dispersed in a spectral device, a detector converts the optical signal into an electric signal that is then processed by electronic devices and ﬁnally by a control computer. The output in the form of a plot of luminescence intensity Ilum versus emission wavelength λem is called an emission spectrum (all the spectra shown in Figs 1.1–1.4 are emission spectra). Spontaneous luminescence emission emerges from a sample practically in all directions, even if in many cases the sample might not be a perfect isotropic emitter. Various optical systems collecting the emitted light can be implemented. The simplest one is shown in Fig. 2.1(b). This is the so-called transmission geometry, where the optical axes of the excitation and luminescence rays coincide. Luminescence is thus detected from the opposite, nonexcited side of the sample. This geometry is simple and easy to adjust but the luminescence signal could be signiﬁcantly reduced by light scattering and especially by reabsorption in the sample. Since reabsorption may be spectrally dependent, the emission spectrum will be distorted. In addition, a signiﬁcant fraction of non-absorbed excitation light could enter into the monochromator and cause problems by saturating or even damaging the detector. Therefore, the transmission geometry is seldom used. More routinely applied is reﬂection geometry shown in Fig. 2.1(c). Luminescence is collected from the same spot on which the exciting radiation is focused by a lens (or an objective). The excitation beam is directed perpendicular to the optical axis of a collection system and the exciting light is sent towards the sample by means of a small totally reﬂecting prism (when the excitation is provided by a well-collimated narrow laser beam) or a dichroic ﬁlter (which reﬂects short wavelengths, i.e. excitation, and transmits longer wavelengths, i.e. luminescence). One and the same lens (objective) is employed to concentrate excitation light and to collect luminescence emission. The lens should have a very large numerical aperture in order to collect light from a wide solid angle. The collimated luminescence light is then focused by means of a second lens onto the entrance slit of a spectral device. Among merits of this geometry are the above mentioned large collection solid angle (remember that luminescence is weak secondary radiation, so the largest possible portion of the emitted power must be collected for successful spectral analysis, see Section 2.5), reduced reabsorption of luminescence radiation, as well as avoidance of stimulated emission (which will be explained later). As a

Emission and excitation spectra possible drawback, complicated optical adjustment required for achieving both optimum excitation power density on the sample and simultaneous maximum luminescence collection can be mentioned. Another undesirable effect may be possible reﬂection of a signiﬁcant part of the excitation light into a detection system, but that is easily remedied by slightly rotating the sample to reﬂect the exciting beam out of the detection cone. In particular cases, when the sample takes the form of thin layer(s) with high-quality surfaces, the geometry sketched in Fig. 2.1(d) (an extreme case of the reﬂection geometry, excitation and emission axes being perpendicular to each other) may be advantageous. Such samples may act as a waveguide into which luminescence is coupled and thereby concentrated at the output edge. In comparison with the previous case, this scheme enables the excitation and emission optical paths to be adjusted independently, and it avoids reﬂection of the excitation beam into the detection system. The most serious problem that might appear is the possible occurrence of stimulated emission: if population inversion is (unintentionally) achieved, then in semiconductors with high probability of radiative recombination the luminescence (spontaneous emission) guided through the excited volume may be ampliﬁed by stimulated emission. This effect can be reduced or avoided by limiting the size of the excited area, but even a small portion of stimulated emission could signiﬁcantly distort the shape of the emission spectrum [1, 2]. On the other hand, this geometry is convenient especially when stimulated emission and the presence of optical gain are the subjects of investigation. Details on such experiments and measurement techniques are provided in Chapter 10. Two particular set-ups for measurements of photoluminescence emission spectra are presented in Fig. 2.2 [3, 4]. The experimental arrangement in Fig. 2.2(a) represents a particular case of the collection geometry sketched schematically in Fig. 2.1(c). A continuous-wave (cw) Ar+ -laser with the most intense lines at 488 and 514 nm is used as an excitation source. The sample is immersed in liquid helium inside a helium-bath cryostat (the temperature of the boiling point of helium at normal pressure is 4.2 K). Luminescence is spectrally dispersed in a double-grating monochromator and detected by a photomultiplier tube (PMT) placed behind the exit slit. The PMT is cooled down by liquid nitrogen (the temperature of the boiling point at normal pressure is 77 K). The signal from the PMT is processed by a photon counter and plotted, as a function of wavelength, by a computer. Another frequently used set-up is shown in Fig. 2.2(b). The excitation source is represented by a high-pressure mercury lamp which has one of its dominant lines at 365 nm (in the near-UV spectral region) that is almost an ideal universal excitation wavelength for most semiconductors. (Nowadays, mercury lamps have been almost completely replaced by diode lasers or (UV adapted) Ar+ -lasers.) From the point of view of geometry, this set-up is halfway between Figs 2.1(c) and 2.1(d), so-called ‘reﬂection at 45◦ ’. The sample is, again, placed in a cryostat whose single window is replaced by a collection lens. The diameter of the lens deﬁnes the collection solid angle. Another lens focuses the collimated luminescence beam into a point where an optical chopper (a rotating disk with regularly arranged slots) periodically chops the beam.

11

12

Experimental techniques

Fig. 2.2 (a) Experimental set-up for detection of photoluminescence emission spectra in a back-reﬂection geometry with double-lens collection system [3]. (b) Set-up for detection of emission spectra with the collection system combining lenses and two parabolic mirrors. This geometry is called ‘reﬂection at 45◦ ’. Adapted from Bebb and Williams [4]. The apparatus contains an optical chopper inserted into the luminescence beam, enabling application of a lock-in detection technique (Subsection 2.4.1).

The rectangular temporal trace of the luminescence signal is essential for treatment of the signal by a lock-in technique that will be discussed in Subsection 2.4.1 (in the case of chopping an unfocused luminescence beam the temporal proﬁle of the signal would be trapezoidal and, consequently, the ﬁnal signal-to-noise ratio will be degraded). Before entering the monochromator, the luminescence radiation must be refocused onto the entrance slit. This is done by a pair of parabolic mirrors; these cover a smaller area than a lens system that would play the same role, thus saving room on the optical table and, moreover, minimizing optical abberations. The detector behind the exit slit of the monochromator—again a photomultiplier tube—provides the output signal that is processed by a lock-in ampliﬁer. The photoluminescence excitation spectrum is a plot of the photoluminescence intensity IPL (at a ﬁxed emission frequency νem = c/λem ) as a function of the excitation photon energy hνex : IPL (νem ) = f (hνex ); νem = const.

Emission and excitation spectra

13

Fig. 2.3 Block diagram of an apparatus for excitation spectra measurements.

A schematic sketch of an experimental set-up for recording excitation spectra is shown in Fig. 2.3. In order to understand the usefulness of the excitation spectra, let us investigate ﬁrstly the dependence of the photoluminescence intensity IPL (νem ) on the excitation light intensity. Suppose we have a sample in the form of a plane-parallel plate with thickness d and an excitation intensity I0 (hνex ) impinging on it. The transmitted excitation intensity is given by the Lambert–Beer law I (hνex ) = I0 (hνex ) exp [− α(hνex )d] ,

(2.1)

where α(hνex ) is the absorption coefﬁcient. If we consider the correction for reﬂectivity R on the front face of the sample (for the sake of simplicity R is assumed to be independent of wavelength), the absorbed part of the excitation intensity is equal to I0 (hνex ) (1 − R) (1 − exp [− α(hνex )d]). The photoluminescence intensity, being proportional to the absorbed energy (possible nonlinear effects are neglected here) then reads IPL (νem ) ∼ = ηI0 (h νex ) (1 − R) (1 − exp [−α(hνex )d]).

(2.2)

The proportionality coefﬁcient η ≤ 1 introduced here is called the efﬁciency or quantum yield of luminescence. In general it depends on many variables: η = η(hνex , hνem , T , . . . ). Now we should distinguish two extreme cases: 1. Weakly absorbing sample α(hνex )d 1. By applying the common approximation of the exponential function exp(−αd) ≈ (1–αd), we obtain from (2.2) IPL (νem ) ∼ = η I0 (hνex ) (1 − R) d α(hνex ) and, after dividing by a reference spectrum of the excitation source I0 (hνex ), we ﬁnd IPL (νem ) ∼ α(hνex ). I0 (hνex )

(2.3)

This means that the excitation spectrum, normalized in this way, reproduces the shape of the absorption spectrum. This can be applied to obtain (relative) absorption spectra in samples in which standard transmission spectroscopy fails, e.g. in thin semiconductor layers on an opaque (i.e. strongly absorbing or scattering) substrate, in measuring low concentrations of luminescent dopants in a strongly absorbing non-luminescent host material, in quantum wells or

14

Experimental techniques superlattices, etc. This is one of the motivations for investigating photoluminescence excitation spectra. (It is worth pointing out that such measurements of optical absorption spectra can also be performed in samples of a very irregular shape, in small fragments or even in powder materials. This is a general merit of most luminescence measurements—they can be performed without paying special attention and effort to preparing a sample of a perfectly deﬁned shape, size, surface quality, etc.) The second motivation for measuring excitation spectra is purely practical. As mentioned above, luminescence radiation is generally very weak; hence all means of optimizing the luminescence signal should be used. In this sense the excitation spectrum, once acquired, gives a clear hint about the choice of an optimum excitation wavelength—this is a wavelength (or excitation photon energy) at which the excitation spectrum is peaked. As an example of a photoluminescence excitation spectrum we present that of crystalline quartz, containing a pronounced structure (see Fig. 2.4(a) [5]). A narrow excitonic peak around 8.7 eV as well as onsets of indirect and direct absorption edges around 9 eV and 10.7 eV can be identiﬁed. Note that the emission spectrum is signiﬁcantly red-shifted from the deep-UV excitation peaks to the near-UV and blue spectral regions (between 2 and 5 eV, see Fig. 2.4(b)). Such a red-shift between excitation and emission peaks is often called the Stokes shift; a more exact deﬁnition will be given in Section 4.5. A sizeable Stokes shift, of several electron-volts like in Fig. 2.4, indicates low power efﬁciency of luminescence, and most likely also the occurrence of a complicated mechanism of excitation energy transfer from a light-absorbing system to luminescence centres. This is additional interesting information revealed by the excitation spectra. Let us recall that all of the above discussion is valid in the case of weak absorption of excitation light, when relation (2.3) holds true. Now we are going to discuss the opposite case. 2. Strongly absorbing sample α(hνex )d 1, i.e. α ≈ 103 –105 cm−1 and d ≥ 10−2 cm. In this case exp[−α(hνex ) d] 1 and (2.2) is reduced to IPL (νem ) ≈ η I0 (hνex ).

(2.4)

This means that the excitation spectrum basically mimics the shape of the emission spectrum of the excitation source while information about the sample under study is lost. The condition α(hνex )d 1 is valid for most semiconductors under deep band-to-band excitation, i.e. when hνex is much larger than the

Fig. 2.4 (a) Photoluminescence excitation spectrum (PLE) of crystalline SiO2 detected at hνem = 3.0 eV and T = 80 K. (b) Photoluminescence emission spectrum (PL), excited by photons with an energy of hνex = 8.7 eV. Adapted from Itoh et al. [5].

Types of photodetectors bandgap energy E g . Here, excitation spectra no longer bring useful information. In a number of experiments between the extremes 1 and 2, the usefulness of excitation spectra measurements must be assessed from case to case. Note: From the experimental point of view eqn (2.4) can be exploited to monitor excitation intensity variations. When the quantum efﬁciency η of a luminescent material (or its solution—e.g. Rhodamin B in ethylenglycol) strictly satisﬁes the requirement of being independent of excitation wavelength, η = η(hνex ), then this material (the so-called quantum counter) may be applied in combination with a photomultiplier to measure the emission spectrum of an excitation source. The advantage of this mode of measurement against using detectors with a spectrally ﬂat response (thermal detectors) is its much higher sensitivity.

2.2 Types of photodetectors In Fig. 2.2 a photomultiplier tube (PMT) is used to detect the spectrally dispersed luminescence signal. This is the most common highly sensitive photodetector for luminescence spectroscopy, even if nowadays it is often replaced by an avalanche photodiode or by an array of small semiconductor devices—usually by a charge-coupled device (CCD) camera. We shall brieﬂy describe these three types of detectors. Photomultiplier tube Detection of optical radiation in a photomultiplier tube is based on the external photoelectric effect and secondary emission of electrons. A photomultiplier is an evacuated glass (or quartz) tube containing a photocathode (from which incident photons eject electrons—with quantum efﬁciency ηph < 1—due to the external photoelectric effect), an array of dynodes (where primary electrons are multiplied through the emission of secondary electrons) and an anode (the collector of electrons, see Fig. 2.5(a)). The outlets of all electrodes pass through a socket of the photomultiplier. A photon can eject an electron from the photocathode only when the photon energy hν exceeds the work function φ of the given photocathode material, hν ≥ φ. To detect (optical) photons from the visible range (hν ≈ 1–4 eV), the photocathode must be made of either an alloy containing alkali metals with low work function φ (e.g. φ = 1.8 eV in Cs,) or a semiconductor with relatively low values of both the work function φ and bandgap E g (GaAs). The applied photocathode material determines the spectral sensitivity of the detector, especially its long-wavelength cut-off, while the short-wavelength edge is determined mostly by the material of the input window. Photoelectrons are accelerated and focused onto the ﬁrst dynode, where each of these primary electrons can release δ (between 3 and 10) secondary electrons. These secondaries, upon being accelerated, hit the next dynode, and the secondary emission of electrons is repeated there so that an avalanche increase in the number of electrons is achieved: if n is the number of dynodes, the number of electrons that hit the anode will be equal to G = δ n . The quantity G is called the current ampliﬁcation or photomultiplier gain and attains values

15

16

Experimental techniques

Fig. 2.5 (a) General scheme of a photomultiplier tube, (b) circuitry of the resistor voltage divider between dynodes, where Ia denotes the anode current and Ivd is the current ﬂowing across the voltage divider, (c) a Hamamatsu R750 photomultiplier tube (the tube length and diameter are 88 and 20 mm, respectively). Adapted from a Hamamatsu brochure.

of 105 –107 . Dynodes are mostly fabricated from nickel or BeCu and are covered by a material with high coefﬁcient δ of secondary emission (BeO, GaP, or KCsSb). The electron ﬂux, collected by the anode, ﬂows across a load resistance and gives an output electric signal, which is then treated by electronic circuits. In order to accelerate the primaries as well as the secondaries, an electric ﬁeld must be supplied between the relevant electrodes. This is done by applying a high voltage (usually between 1000 and 2000 V) between the photocathode and anode through a resistor voltage divider (Fig. 2.5(b)). The resistors are connected in series; the ratios of their values, deﬁning how the applied voltage is divided between electrodes, are speciﬁed by the manufacturer and must be strictly maintained. Nowadays most manufacturers offer sockets with a built-in resistor divider for any type of photomultiplier tube. A typical value of a single resistor is of the order of 100 k , determining the current through the divider to be in the order of mA (in the case of n = 10 dynodes and an applied voltage of 1000 V). There are many various construction types of photomultiplier tubes. The photomultiplier sketched schematically in Fig. 2.5(a) and an overall view of which is shown in Fig. 2.5(c), has a so-called linear focus multiplier; other common types of multiplier structures are called ‘Venetian blinds’, boxes and grids, and circular cages. Besides, the photocathode may be deposited onto the inner surface of either the front side of the cylindrical tube (head-on type, Fig. 2.5(c)) or its side wall (side-on type). A more detailed description and comparison of different types of photomultipliers goes beyond the scope of this book and can be found in the dedicated literature, e.g. [6, 7].

Types of photodetectors We shall describe concisely the technical parameters of photomultiplier tubes. Photomultipliers owe their widespread use to, ﬁrstly, the already mentioned high gain G and also to their spectral range of sensitivity. This range extends between about 150 and 1100 nm; in special cases it can go up to 1400 nm. It should be stressed, however, that the entire spectral domain cannot be covered by a single type of photomultiplier. The selection of an appropriate photomultiplier type thus has to be based primarily on considerations about the spectral range of the detected light. The anode sensitivity k (λ) is given as the anode current produced by 1 watt (in energy units) or 1 lumen (in photometric units) of incident radiant or luminous ﬂux Φ, respectively: k(λ) =

output signal , incident radiant power

k(λ) =

S S = 2 Φ I W/cm A cm2

(A/W) or (A/lm),

(2.5)

where A denotes the sensitive area of the photomultiplier. Typical values of k(λ) are 103 –105 A/W. The above mentioned quantum efﬁciency ηph of the photomultiplier tube is deﬁned as the probability of ejecting from the photocathode one electron per incident photon (ηph is typically about 0.1–20%). A very important parameter for properly operating a photomultiplier is its maximum anode current Iam , whose typical value is usually 10–100 μA and must not be exceeded (i.e. the incident radiant ﬂux must be kept below a certain level), otherwise the excessive heating of the electrodes will induce permanent damage to the photomultiplier (due, e.g., to partial evaporation of the sensitive layer of the photocathode) which manifests itself as a decrease in sensitivity or an increase in background noise. In addition, for proper functioning of a photomultiplier tube (linearity of its response) the resistors in the voltage divider must be chosen so that the current ﬂowing across the divider is at least an order of magnitude higher than Iam (Problem 2/1). This deﬁnition of sensitivity does not take into account noise and the socalled dark current of the photomultiplier tube. The dark current Id is a current due to the thermionic emission of electrons from the photocathode, which takes place even in darkness when no light strikes the photocathode. The thermionic current density is described by the well-known Richardson–Dushman equation [8], and thus increases exponentially with increasing temperature and decreasing work function φ of the photocathode. Photomultiplier tubes sensitive in the red and near-infrared spectral regions suffer from the highest dark currents, as the work function of their photocathodes must be low. Typical values of the anode dark current lie between a few nA up to hundreds of nA. Dark current at the output of a photomultiplier cannot be distinguished from the real (lightinduced) signal, which is troublesome especially for very low signal levels— dark current obviously increases the limit of the lowest detectable signal (the detection limit of a photomultiplier tube). It is therefore desirable to suppress the dark current as much as possible. The strong (exponential) dependence of the dark current on temperature enables us to reduce it signiﬁcantly by cooling the photomultiplier. The lowest allowed operational temperature is

17

18

Experimental techniques given by the manufacturer and must not be exceeded because mechanical deformations at lower temperatures can induce permanent mechanical damage. Cooling can be provided by means of a thermoelectric (Peltier) element (down to about −25◦ C with a single-stage device) or by liquid nitrogen (boiling point −195◦ C = 77 K). The cooling housings for different types of photomultiplier tubes are commonly offered by manufacturers or they can be home-built (which is not an easy task, though). Sometimes, ‘for less demanding applications’, photomultipliers can be used even without cooling, but that depends on the photomultiplier type and even the particular photomultiplier piece of choice. The dark current Id can thus be suppressed to a large extent by cooling. Alternatively, because the dark current contribution to the resulting output signal has the form of a direct current (DC) component, it can be ﬁltered out when measuring alternating current (AC) signals. A similar approach cannot, unfortunately, be applied to reduce noise in the output signal—see, e.g., Figs 1.1 and 1.2, where we reproduce luminescence spectra as recorded by a plotter after being treated by the electronic part of the detection channel. The spectra in Fig. 1.1 were detected by using a cooled (77 K) photomultiplier tube with a near-infrared sensitive photocathode while the spectra in Fig. 1.2(a) were obtained by an uncooled photomultiplier tube with a semiconductor-type photocathode. In order to characterize the noise properties of a photodetector, the quantity termed noise equivalent power (NEP) (or equivalent noise input— ENI) is introduced. This means the incident light power which would induce an output signal equal to the root mean square of the intrinsic (dark) noise N (Fig. 2.6). The detected noise increases, of course, with increasing transmission bandwidth f of the entire measurement system; it turns out that the noise amplitude scales with the bandwidth like ( f )1/2 . So the detected noise N can be written down as (2.6) N = k(λ) NEP f,

Fig. 2.6 Schematical representation of noise conditions in a DC luminescence emission spectrum. N stands for the root mean square noise value, i.e. 1/2 t0 2 N= n (t) dt /t0 , where n(t) 0

is the instantaneous time-variable value of the noise related to the mean signal value S.

where NEP = (2e Id G)1/2 /k(λ) [7] is a parameter already independent of the measurement system, i.e. solely characterizing the photodetector. According to the deﬁnition, the signal-to-noise ratio (S/N ) is equal to unity when the incident light power is equal to NEP. In other words, NEP represents the lowest signal level (detection limit) which can be detected by a given detector; weaker signals will remain buried in noise. Referring to eqn (2.6), NEP is expressed in W/Hz1/2 . Thus this is not directly power (in watts), but one usually supposes that f = 1 Hz and then NEP( f )1/2 (W) and NEP(W/Hz1/2 ) in (2.6) are numerically equal to each other. A typical value of NEP for photomultipliers amounts to 10−16 –10−15 W. One can also introduce related quantities: the detectivity D and normalized detectivity D ∗ . The detectivity D is simply the reciprocal value of NEP(D = 1/NEP), and the normalized detectivity is deﬁned as √ √ (2.7) D ∗ = A /NEP = D A (cm Hz1/2 /W). A deﬁnition such as this is introduced because for most √ detectors the NEP scales with the sensitive area A of the detector like A . Therefore the

Types of photodetectors normalized detectivity D ∗ enables us to compare detectors of different sizes. A photomultiplier with a photocathode area of A ∼ = 5 cm2 , NEP = 1/2 −16 ∗ ∼ W/Hz , and f = 1 Hz would feature D = 2.3 × 1016 cmHz1/2 /W. 10 Let us note, however, that the detectivities D and D ∗ are most often used to characterize semiconductor detectors rather than photomultipliers. A more detailed analysis of noise is beyond the scope of this book. We should only note that the total photodetector noise has several components: the shot noise of the photocathode, the noise due to the statistical character of the secondary emission from dynodes, Johnson’s noise in the load resistor, the so-called 1/ f noise, and in the case of semiconductor detectors, generationrecombination noise is added, etc. The reader is referred to [6, 9]. On the other hand, the crucial task in luminescence spectroscopy is to optimize the signal-to-noise ratio, S/N . This will be discussed in detail in Section 2.5. Here we shall brieﬂy deal with one type of noise only—shot noise. This noise is a direct result of the quantum (corpuscular) nature of both the photons in the input optical signal and the electric charge generated in a detector. The number of incoming photons per unit time ﬂuctuates around a certain average value. Statistical ﬂuctuations in the stream of photons emitted by a classical source obey Poissonian photon statistics (some special cases violating Poissonian statistics are mentioned in Chapter 17 and Appendix L). Obviously, this photon-related noise component is independent of the particular detector, and represents an inevitable property of the incoming signal and thus also the lowest possible noise level of any optical detection system. An analogous statistical description applies to the internal detector process of photoelectron emission upon absorption of a photon. The current generated by a detector thus ﬂuctuates around an average value (i.e. the signal S) and—in analogy with similar statistical ensembles—the relevant ﬂuctuations are equal to the square root of the signal average. This means that the mean square value of the shot noise N reads √ (2.8) N = S. This kind of noise, increasing at higher signal levels, is shown in Fig. 2.6 and is noticeable also in Figs 1.1 and 1.2 (the noise of the background level is of different origin). To conclude our account of photomultipliers we give several practical hints. A photomultiplier is a sensitive, fragile, and expensive electronic tube that must be handled with care. When not in use, the photomultiplier tube should be stored in a light-tight box. Its installation into a housing must be done under dimmed light and exposure of the photocathode to daylight should be as short as possible. The operational high voltage must be applied at least half an hour prior to measurement in order to stabilize the sensitivity k(λ), the dark current value Id and the noise properties. Varying or even switching on and off the applied high voltage during an experiment (e.g. for fear of exceeding the maximum allowed anode current) is a quite common mistake, which could lead to erroneous results—any change in voltage may disturb the stabilized operation conditions and cause a temporary variation in photomultiplier sensitivity,

19

20

Experimental techniques lasting up to tens of minutes (the so-called photomultiplier hysteresis). The correct approach to avoid overﬂow of Iam is decreasing the incoming light ﬂux (using, e.g., calibrated neutral density ﬁlters). In the case of a cooled photomultiplier, the best practice is to keep cooling and permanently applying the high voltage even between measurements, the photocathode being kept in darkness. In such a way the dark current and the noise amplitude are minimized in the long term. There might be two additional causes of irreversible noise increase (besides the above mentioned overﬂow of Iam ): exceeding the maximum allowed voltage between the photocathode and anode Uam (this value is given by the manufacturer, as well as Iam ) and penetration of moisture into the cooled photomultiplier housing. We recommend the maximum allowed voltage Uam should never be applied to a photomultiplier. First of all, the optimum operational voltage always lies below Uam (sometimes even by hundreds of volts) and increasing the voltage closer to Uam does not lead to better performance. Secondly, a possible inaccuracy of the voltmeter monitoring the applied high voltage can result in an unintentional overﬂow of Uam , entailing consequences much like the case of overﬂowing of Iam . Moisture penetrating towards a cooled photomultiplier can condense in the socket and leakage currents could cause irreversible changes of the properties of the photomultiplier. A good commercially supplied housing should be leakproof, anyhow. Finally, let us remark that a magnetic ﬁeld can be detrimental to the functioning of a photomultiplier as it alters the optimized trajectories of electrons between electrodes. The location of a photomultiplier (and of all auxilliary experimental apparatus) in a laboratory must be chosen to be free of disturbing electromagnetic ﬁelds. A special magnetic shield can possibly be used (these are offered by photomultiplier manufacturers). Avalanche photodiode The basic principle of an avalanche photodiode is the same as in other photovoltaic semiconductor photodetectors, namely, the internal photoelectric effect—the generation of an electron–hole pair through absorption of a photon. The photogenerated charge is then separated in an electric ﬁeld established across the depletion layer of a p-n junction, and a photovoltage is created at the detector output, which is subsequently processed by electronics. Semiconductor photodiodes have a much wider spectral range compared to photomultipliers, especially toward the near-infrared region; their longwavelength cut-off is determined by the bandgap width of the photosensitive semiconductor material. For example, the range of sensitivity of a Ge and InAs diode is 600–1800 nm and 1000–3200 nm, respectively. Despite their relatively low detectivities (D ∗ ≤ 1012 cm Hz1/2 /W), the p-n or p-i-n photodiodes1 are 1 An ultrasensitive germanium detector introduced by Edinburgh Instruments, Ltd., represents an exception suitable to detect low luminescence light ﬂuxes. It is based on a p+ -i-n+ diode made of ultrapure germanium and cooled by liquid nitrogen. The detection range is 800–1700 nm and its normalized detectivity of 5 × 1014 cmHz1/2 /W is comparable to photomultipliers. However, high sensitivity is counterbalanced by a very slow response, big size, considerable weight, and a relatively complicated operation.

Types of photodetectors

21

Fig. 2.7 The principle of an avalanche photodiode. Primary electron–hole pairs are created by absorption of photons hν > E g (1). A pair is dissociated and both the electron and hole are accelerated in opposite directions by the strong electric ﬁeld in the intrinsic layer of the reverse biased p-i-n structure. After gaining enough energy the accelerated electron (hole) can create by impact ionization a new electron–hole pair (2) or (3) and the process can continue in an avalanche-like manner.

applied in luminescence spectroscopy for the detection in the infrared region beyond ∼ 1000 nm, i.e. beyond the red cut-off in sensitivity of the common photomultipliers. However, current photodiodes lack the effect of photocarrier multiplication. Such multiplication is only possible in avalanche photodiodes that have internal gain in the range of G AP ∼ 10–500. The avalanche photodiode detectivity D ∗ is then increased but usually does not reach values comparable to photomultipliers. The principal functional layout of an avalanche photodiode is shown in Fig. 2.7. Basically one deals with a p-i-n semiconductor structure under high reverse bias. Upon absorption of a photon hν > E g an electron–hole pair is created. This pair is dissociated in the strong electric ﬁeld of the intrinsic layer (i) and both the electron and hole are accelerated in opposite directions. If the energy acquired by the accelerated carriers exceeds E g (which is not always the case, because carriers are losing their energy in collisions with the crystal lattice), another electron–hole pair can be generated by impact ionization. Then the whole process may be repeated and an avalanche-like increase in number of carriers takes place. Even if the principle of an avalanche photodiode looks very simple, there are several fundamental and technical obstacles making fabrication of an efﬁcient and reliable device difﬁcult. First of all, contrary to what might seem proﬁtable at ﬁrst sight, simultaneous ampliﬁcation of both the electrons and holes (Fig. 2.7) is not favourable for obtaining high gain. In fact, such a situation is undesirable because this process is unstable and can result in avalanche breakdown and damage to the diode. In addition, the symmetrical ampliﬁcation as a random process gives rise to a higher noise level of the detector and, moreover, prolongs the risetime of the avalanche diode, thereby reducing the frequency bandwidth of the diode. Therefore, avalanche diodes should be made of a material in which only one type of carrier is ampliﬁed. Let us characterize the probability of ionization by electrons (or holes), i.e. the number of ionization events per unit distance, by the ionization coefﬁcient αe (or αh ). Then an important avalanche photodiode parameter can be deﬁned, namely, the ionization ratio κ = αh /αe and it is required that κ tends either to zero κ → 0 (electron multiplication) or to inﬁnity κ → ∞ (hole multiplication). The best

22

Experimental techniques commercial avalanche photodiodes based on silicon have κ ≈ 0.006. In the extreme case of κ = 0 the photodiode gain is simply given by G AP = αe w, where w is the width of the multiplication region. Another difﬁculty one is faced with when designing an avalanche photodiode arises from this simple reasoning: to achieve high diode sensitivity (i.e. to maximize the number of primary electron–hole pairs), the intrinsic (i) layer should be made as thick as possible. On the other hand, the inevitable presence of a high electric ﬁeld across the layer requires this layer to be thin. The last requirement is of a technical rather than essential nature: the volume of the amplifying material should be limited in order to minimize the possible occurrence of material inhomogenities that could cause a local overrun of the breakdown electric ﬁeld, thus creating a microplasma and eventually leading to photodiode damage. This conﬂict of opposite demands is solved by the special design of the avalanche photodiode—the wide photon-absorption layer is separated from the thin electron-multiplication layer (‘separateabsorption-multiplication’). Evidently, fabrication of good avalanche photodiodes involves the use of both a perfect homogeneous material and advanced technology. The ﬁrst avalanche photodiodes produced in the 1970s suffered from excess noise and easy breakdowns but subsequent radical development of semiconductor technologies removed those constraints. Finally, the requirement to minimize the multiplication volume (as well as to achieve fast response) leads to a small size of the sensitive area AAP of the avalanche photodiode (of the order of mm2 or smaller). The structure of an avalanche photodiode together with the proﬁle of the internal electric ﬁeld are presented in Fig. 2.8 (in this case hole multiplication occurs—photon absorption takes place in an i-InGaAs layer from which the holes drift in the weak electric ﬁeld to an intrinsic InP multiplication layer) [10]. Obviously, the highest allowed bias applied to an avalanche photodiode must not be exceeded, similarly to photomultipliers. Let us brieﬂy compare photomultipliers with avalanche photodiodes from the point of view of luminescence spectroscopy. An advantage of avalanche photodiodes as solid-state devices over fragile vacuum tubes is their small compact size and robustness. On the other hand, noise properties of avalanche photodiodes are generally worse as expressed by the mean value of the dark noise [11]

Fig. 2.8 Internal structure of an InGaAs/InP avalanche photodiode with separated absorption and multiplication layers and the corresponding proﬁle of the electric ﬁeld (right). Adapted from Ferrari et al. [10].

Types of photodetectors

1/2 NAP = 2eIdAP G¯ 2AP F(G AP ) f .

(2.9)

When compared to eqn (2.6) which is valid for photomultipliers we notice ﬁrstly in (2.9) the squared mean value of the gain G¯ 2AP and, secondly, an additional noise factor F(G AP ). The squared factor arises as a consequence of the contribution of both types of carriers (electrons and holes) to the photodiode current (even if only one type of carrier is multiplied). The factor F(G AP ) arises from the stochastic nature of the ionization process. For multiplication of electrons this factor is given by F(G AP ) = κ G AP + (2 − 1/G AP )(1 − κ).

(2.10) 6 × 10−3

In the case of an Si avalanche photodiode with parameters κ = and G¯ AP = 100 we obtain F(G AP ) ∼ = 2.6. The NEP of an avalanche photodiode can be expressed, using (2.9), as 2eI dAP G¯ 2AP F(G AP ) NEPAP = kAP (λ) and for the normalized detectivity it follows from (2.7) that √ AAP kAP (λ) ∗ . DAP = 2eI dAP G¯ 2AP F(G AP ) ∗ Finally, the ratio of the normalized detectivity of a typical photomultiplier DPM ∗ 5 (with gain G PM ≈ 10 ) to that of an avalanche photodiode DAP is found to be

√ ∗ DPM APM IdAP kPM (λ) G¯ AP F(G AP ) , (2.11) √ ∗ = DAP AAP IdPM kAP (λ) G PM

where IdAP and IdPM stand for the dark currents of the avalanche photodiode and photomultiplier, respectively, and kAP , kPM are the corresponding sensitivities. If we try to compare, using eqn (2.11), two particular detectors—a Hamamatsu R316 photomultiplier with a Perkin Elmer InGaAs avalanche photodiode (the spectral sensitivities of both detectors overlap in the range ∗ ∼ 50D ∗ . However, a comparison like this must 700–1100 nm), we ﬁnd DPM = AP be considered with care, because all device parameters are strongly dependent on the radiation wavelength as well as on operational conditions. Sometimes even the datasheets for detectors, supplied by the manufacturers, do not contain all the necessary parameters. Nevertheless, in general it holds true that the normalized detectivity of avalanche photodiodes does not attain the photomultiplier values. Moreover, the small size of the sensitive area of the avalanche photodiode is hardly appropriate for luminescence spectroscopy—to ensure tight focusing of luminescence radiation at the exit slit of a monochromator onto a small area of 1 mm2 is basically impossible; a large part of the signal would thus be lost. Here, the optimum choice is indeed a photomultiplier because its photocathode of typically rectangular shape with size about 3 × 12 mm2 ﬁts

23

24

Experimental techniques the cross-section of the light beam emerging from the exit slit quite well. Therefore, avalanche photodiodes are applied in unconventional spectroscopic techniques only, like time-correlated single-photon counting and the determination of photon autocorrelation (see Subsection 2.4.2 and Chapter 17). They can also be used for the detection of extremely low-level luminescence signals from small sources—nanoobjects, like single molecules or nanocrystals, in a microspectroscopy set-up (Chapter 17). Single-photon counting avalanche photodiode modules are produced, e.g., by Perkin Elmer, ID Quantique and Hamamatsu. In these special luminescence measurements, the avalanche photodiode operates in the so-called Geiger mode, the applied bias being higher than the breakdown voltage and the diode gain being very high (G AP ∼ = 105 − 106 ). A particular diode design simultaneously ensures that no current ﬂows across the diode except in the case when an avalanche event is initiated by a released photoelectron; after generating a current pulse the diode is closed again (in analogy with the Geiger–M¨uller counter of radioactive radiation). In this way individual photons may be resolved. Normalized detectivity of photon counting modules based on silicon avalanche photodiodes can be as high as 5 × 1013 cmHz1/2 /W. Obviously, in this case cooling of the avalanche photodiode is of particular importance in order to suppress the dark counts (the dark counts of the best diodes can be below 20 counts/s). Multichannel detectors Photomultipliers and avalanche photodiodes are single-channel photodetectors, which means that they are able to detect, at a given time, the photon ﬂux at a single point (area) in space only. Alternatively, the so-called multichannel detectors, in the form of linear or two-dimensional arrays of tiny photosensitive solid-state devices, are able to detect the photon ﬂux simultaneously at many spatial points. In luminescence spectroscopy, when the single-channel detector is placed behind the exit slit of a monochromator, only a single point from the spectrum is recorded. The entire spectrum is then acquired sequentially, step by step, by rotating the dispersion element (grating or prism) and thereby scanning the spectral image across the exit slit. Such a measurement is, of course, quite lengthy and the obtained spectrum can be distorted owing to, for instance, the long-term instability of both the excitation source and/or the sample (photochemical changes, generation of defects, etc.). On the other hand, multichannel detectors, ﬁxed in the output plane of a spectrograph, simultaneously detect the intensity (photon ﬂux) at many spectral points within some spectral range, or even the whole spectrum without moving the dispersion element (Fig. 2.9). This allows for signiﬁcant shortening of the signal acquisition time, avoiding instability effects, monitoring the entire spectrum in real time, eliminating inaccuracy of the dispersion element scanning mechanism, etc. In addition, this approach considerably simpliﬁes those experiments that apply a pulsed mode of luminescence excitation. It may be worth evoking memories of the ﬁrst type of multichannel detector used in spectroscopy, which was a photographic plate. Its replacement by photomultipliers and scanning monochromators during the 1950s and 1960s

Types of photodetectors

25

Fig. 2.9 Scheme of (a) a monochromator equipped with a rotating dispersion element (prism or grating) and a single-channel detector, (b) a spectrograph with a ﬁxed dispersion element and a multichannel detector.

introduced a qualitative improvement to optical, and especially luminescence, spectroscopy. Even if the photomultiplier is a single-channel detector only, its many times higher sensitivity and reproducibility compared to photographic emulsions enabled researchers to investigate many new semiconductor phosphors. This ﬁnally resulted in the discoveries and inventions of, e.g., injection electroluminescence, light-emitting diodes, semiconductor lasers, and the accelerated development of optoelectronics and its applications. Present-day multichannel detectors combine detection sensitivity— comparable to that of photomultipliers—with the advantages of a ‘photographic plate’ and the mechanical robustness of a solid-state detector. The better noise and detection properties of multichannel detectors arise from the so-called Fellgett (multiplex) advantage, which makes it possible to integrate a weak luminescence spectrum for an arbitrarily long time. Let us give a more detailed explanation. Suppose we have a linear array detector containing n elements (called pixels, an abbreviation of ‘picture element’), the sensitivity of each of them being the same as that of a photomultiplier. In the case of a scanning monochromator and a single-channel detector, the detector (photomultiplier) ‘sees’ any of the n spectral elements separately, say for one second of time, therefore the entire spectrum is recorded within n seconds, featuring a certain signal-to-noise ratio (S/N )0 . A multichannel detector records all of the n pixels simultaneously, therefore, supposing the integration time to be also one second, the resulting signal-to-noise ratio will be the same, i.e. (S/N )0 . The spectrum, nevertheless, is recorded within 1/n th of the time required to be measured (to the same ‘quality’) by the photomultiplier. If we now record (integrate) the spectrum also for the time span of n seconds, we obviously obtain an n-times higher signal nS but—according to eqn (2.8)— √ only nS-times higher noise level. Consequently, the spectrum recorded in this way will feature the signal-to-noise ratio

S N

Fellgett

√ nS =√ = n nS

S N

. 0

(2.12)

26

Experimental techniques

Fig. 2.10 Standard array of silicon photodiodes.

This increase in signal-to-noise ratio is known as Fellgett advantage. Let us consider n ∼ = 1000 (indeed, the number of pixels is often 1024 = 2√10 ); then according to eqn (2.12) the increase in the signal-to-noise ratio is 1000 ≈ 32 × (!). The foregoing example is valid strictly in the case of shot noise only but, as we shall see shortly, most other noise components can be successfully suppressed in multichannel detectors; in particular the thermal noise is effectively suppressed by cooling. Of course, a further increase in S/N can in principle be achieved by further prolonging the acquisition time, as is immediately evident from eqn (2.12). With an acquisition time of m seconds (m > n) the signal-to-noise ratio is √ improved m-times against (S/N )0 . It must be remembered, however, that in this way we deliberately renounce other beneﬁts of multichannel detectors, namely, the elimination of possible sample ‘fatigue’ or of other unwanted variations in time of both the sample and the whole experimental set-up; on the other hand, such a measure is often beneﬁcial because it facilitates successful recording of (‘recovered from the noise’) the spectra of extremely low light ﬂuxes, undetectable by making use of photomultipliers. Two of the most common types of multichannel detectors are photodiode arrays and charge-coupled-device (CCD) cameras. A linear array of photodiodes is made up of a row of tiny (silicon) photodiodes (Fig. 2.10). Every photodiode (pixel) is reverse biased and charged like a capacitor. The incident photons generate electron–hole pairs, increasing electric conductivity in the capacitor and consequently its discharging. Then, a read-out period follows, during which the diodes are charged up by a current that is proportional to the number of absorbed photons. The usual duration of the read-out period in the case of the 1024 diode array shown in Fig. 2.10 is 13 ms. The spectral range of the sensitivity is, similarly to common single Si photodiodes, about 300–1100 nm, and the spectrum acquisition time can be arbitrarily varied. The discrete structure of the photodiode array seemingly imposes certain limits to the achievable spectral resolution. However, luminescence spectra are usually relatively broad and so this fact does not usually pose serious problems. The dark signal in a diode array, given by thermally generated electron–hole pairs, determines the sensitivity threshold of the array but can be substantially reduced by cooling—mostly thermoelectric cooling down to −20◦ C is applied. The sensitivity of the diode array is not necessarily sufﬁcient for the purposes of luminescence spectroscopy. Nowadays, the most sensitive photodetectors, aimed at detecting extremely weak signals and broadly exploited especially in luminescence spectroscopy, are CCD cameras. Their basic principle again consists in the generation of charge carriers by incident photons, but

Types of photodetectors

27

Fig. 2.11 (a) Schematics of a CCD detector. (b) Charge transfer in a CCD detector. Adopted from ISA Jobin-Yvon-Spex ﬂyers [12].

their construction and read-out scheme differ substantially from the photodiode arrays. One deals with a system of discrete small components, in which the individual pixel is usually deﬁned as a set of three electrodes with a variable applied bias [12]. The electrodes are made of conductive (highly doped) polycrystalline silicon and deposited on a photosensitive silicon wafer of lower conductivity; the said materials are separated by a thin layer of insulating SiO2 (Fig. 2.11(a)). The photoelectrons generated by incident light may, depending on the applied bias, be trapped and stored in potential wells that are created in silicon beneath the electrodes. The light-detection process involves three steps: 1. Absorption of incident photons in photosensitive silicon and generation of electron–hole pairs. The number of pairs in each pixel is proportional to the incident light intensity. When positive bias is applied to the pixel central electrode, only the electrons are trapped in the potential well while holes are drained to earth. 2. Transfer of the collected charge from a given pixel to the next one. By applying the bias to the outer electrode of the pixel, the electron cloud is shifted to the pixel edge and eventually to the next pixel in the column, i.e. along the particular spectral line or a speciﬁc wavelength. This process is repeated until the charge from each pixel of a row reaches a read-out register located along the edge of the CCD chip, i.e. in parallel with the wavelength axis. This is accomplished by gradually varying the bias on individual pixels (see Fig. 2.11(b)). It is now clear why a pixel is composed of three electrodes. A great advantage of this mode of information read-out is the extreme reduction of the read-out noise due to the use of a single

28

Experimental techniques

Fig. 2.12 Spectral response of a silicon CCD camera. (a) Sensitivity of a standard front-illuminated CCD detector (extension of the detection range into the IR region—short dashed line—can be achieved by using a thicker substrate that absorbs effectively longer wavelengths). (b) Spectral sensitivity of a back-illuminated chip where absorption of incident light in electrodes is avoided. Extension into the UV region can be obtained for example by depositing a phosphor layer (emitting visible light under illumination by UV light) directly onto the detector. AR means antireﬂection coating. Adapted from the ISA Jobin-Yvon-Spex ﬂyer [12].

common read-out register for all of the pixels instead of employing a readout system in every pixel. 3. Conversion of electric charge into voltage, ampliﬁcation and digitization. The stored charge is transferred row by row into the read-out register and then into an output node, converted to an appropriate voltage, ampliﬁed and turned into a digital signal. Finally, the number of detected photoelectrons in every pixel of a CCD is stored, and the obtained picture (spectrum) can be visualized on a display, numerically treated, etc. The typical area of a pixel in a spectroscopic CCD detector is about 20 × 20 μm2 , and the full size of the sensitive area is, e.g., 26.6 × 6.6 mm2 (1024 × 256 pixels with a pixel size of 26 × 26 μm2 ). The spectral sensitivity of a CCD detector is determined by its material— usually silicon. The typical range of about 400–1000 nm can be modiﬁed to some extent by adjusting the detector surface and thickness and the mode of illumination (front or back-illuminated), see Fig. 2.12. The experimental spectral coverage depends on the physical length of the detector and on the monochromator dispersion, and it can obviously be expressed as λcov = (reciprocal linear dispersion[nm/mm]) × (CCD detector length [mm]). We have to stress that multichannel detectors should not be coupled to a common scanning monochromator, by merely removing its output slit and replacing it by a CCD camera or a diode array. An ordinary monochromator is able to image an aberration-free spectrum (i.e. to create a spectrally resolved projection of the entrance slit into the exit slit plane) of a very narrow wavelength range only, covering roughly the slit width (∼ 1 mm). For application with multichannel detectors, special imaging spectrographs are available. Their optical aberrations must be corrected over the whole size (height and width)

Types of photodetectors of the detector. For example, combination of a Horiba Jobin Yvon iHR 320 imaging spectrograph having a dispersion of 2.64 nm/mm with a CCD chip of 1024 × 256 pixels (pixel size 26 × 26 μm2 ) shows a spectral coverage of λcov = 70.3 nm. In order to measure a wider spectral range the ultimate spectrum must be glued together from several segments with a shifted central wavelength. The sensitivity of the CCD detector is extremely high. Thermal noise can be almost eliminated by cooling down to −90◦ C or even −140◦ C when the dark signal can be suppressed down to an unbelievable 1 electron/pixel/h only (!) (In practise, the recommended temperature is usually above −110◦ C because lower temperatures would decrease the quantum efﬁciency of the detector; efﬁcient cooling is provided either by liquid nitrogen or a multistage thermoelectric Peltier element.) The lowest detectable signal is then limited by the so-called read-out noise, or possibly only by the shot noise originating mostly in the signal itself. Let us put forward a few examples: 1. Suppose the total root mean square noise value NCCD of the detector is given as a combination of three components NCCD = |n shot |2 + |n dark |2 + |n read |2 , (2.13) with n shot , n dark and n read standing for the shot noise, dark signal and the read-out noise, respectively. Assuming a relatively low ﬂux of incident photons of 10 photon/pixel/s entails (in the visible range) a power ﬂux density of ∼ 4 × 10−13 W/cm2 . Considering the quantum efﬁciency of the detector to be 50% we obtain 5 photoelectron/pixel/s. Setting the acquisition time to be 600 s (10 min), the total integrated signal is 5 photoelectron/pixel/s ×600 s = 3000 photoelectron/pixel. Shot noise of such a signal is n shot = (3000)1/2 = 54.77. Suppose further this cooled detector has a dark signal of 1 electron/pixel/min, then the total dark signal accumulated during 600 s is 10 electron/pixel and the corresponding noise component is n dark = 101/2 = 3.16. Finally, the typical read-out noise of a 1024 × 256 pixel CCD detector with slow reading is about n read = 4 electrons (root mean square value). According to (2.13) the overall noise of the detection system is NCCD = (54.77)2 + (3.16)2 + 42 = 55. The signal-to-noise ratio is S/N = 3000/55 = 54.54. Note that, were the detector completely free from both the dark current and read-out noise, then the best achievable signal-to-noise ratio would be S/N = 3000/54.77 = 54.77, i.e. only negligibly higher. We conclude that under an incident photon ﬂux of 10 photon/pixel/s the intrinsic detector noise does not play any detrimental role—such measurement is referred to as ‘shot noise limited’. The same conclusion would hold true even for a ten times lower incident ﬂux of 1 photon/pixel/s! 2. Let us now consider a complelety different situation when an extremely low signal of only 1000 photon/s hits the whole area of a CCD detector

29

30

Experimental techniques (1024 × 256 pixels2 = 676 μm2 ). This means, at a photon energy of 2 eV, an incident power density of 1.7 × 10−17 W/cm2 . Such extremely low photon ﬂuxes take place, for example, when detecting luminescence excited by the tip of a scanning tunnelling microscope (STM) or photoluminescence of single semiconductor quantum dots (see Chapter 17). Suppose we have at our disposal the same CCD detector as in the previous example. This means with quantum efﬁciency of 50%, dark signal of 1 electron/pixel/min, read-out noise of n read = 4 electrons, and we also leave unchanged the acquisition time 600 s. The average photon ﬂux incident on a single pixel is 1000 (photon/s)/ 2.62 × 105 pixels = 3.8 × 10−3 photon/pixel/s; the corresponding number of photoelectrons is 0.5 × 3.8 × 10−3 = 1.9 × 10−3 photoelectron/pixel/s, and after an integration time of 600 s we obtain the total signal as 1.9 × 10−3 photoelectron/pixel/s × 600 √ s = 1.14 photoelectron/pixel. The corresponding shot noise is n shot = 1.14 ≈ 1.07. From the preceding example we remember that n dark = 3.16, n read = 4 and thus the total CCD noise reads NCCD = (1.07)2 + (3.16)2 + (4)2 = 5.21. The signal-to-noise ratio is thus S/N = 1.14/5.21 ≈ 0.22. Taking S/N = 1 as the detection limit criterion, the light ﬂux under consideration is not detectable and will be ‘buried in noise’. Here the experiment is already clearly limited by the detector’s noise itself! Does this example imply that even sensitive CCD detectors are not able to detect photon ﬂuxes of the order of 103 photon /detector/s? No, it does not, as we shall see. The solution could be to set a longer detection time and/or apply a less noisy detector. 3. Let us keep all the parameters from example 2 ﬁxed, except the integration (acquisition) time, which we increase now from 600 s to 1 hour (3600 s). The signal will be increased to 6.84 photoelectron/pixel and the overall noise to (2.61)2 + (7.75)2 + 42 = 9.1. We obtain S/N = 6.84/9.1 ∼ = 0.75 < 1. We can see that even quite substantial prolongation of the acquisition time does not lead to S/N = 1, and further extension of the experimental time is usually out of the question (due to possible instabilities of sample properties or experimental conditions). 4. Let us select the best available CCD detector with a high quantum efﬁciency (90%) and almost zero dark signal (1 electron/pixel/h)—these are typical parameters of a back-illuminated liquid-nitrogen-cooled silicon CCD chip. Let the incident photon ﬂux be the same as in example 2, i.e. 3.8 × 10−3 photon/pixel/s, and integration time is 600 s. Then the signal is 0.9 × 3.8 × 10−3 × 600 = 2.05 photoelectron/pixel, the shot noise is √ 2.05 = √1.43, the dark signal is 1/6 electron/pixel and the corresponding noise is 1/6 = 0.41. The read-out noise remains equal to 4 electrons. Now we have NCCD = (1.43)2 + (0.41)2 + 42 = 4.27, S/N = 2.05/4.27 ∼ = 0.48 < 1. Even now the spectrum remains undetectable, due to the relatively high read-out noise. The last chance is to extend the acquisition time; 40 min (2400 s) is on the limit but still acceptable. The reader then easily

Monochromators and spectrographs ﬁnds that the resulting S/N ratio ﬁnally breaks the detection limit, being S/N = 8.21/4.98 ∼ = 1.65 > 1. The spectrum can thus be recorded within a 40-minute exposure time, even if quite noisy. In conclusion, CCD detectors manage to display the whole spectrum of comparatively strong signals in real time (which, by the way, appears to be an excellent tool to adjust the experimental set-up in this case). The whole spectral range of such signals is detected almost instantaneously (no monochromator scanning is needed), all the wavelengths being recorded simultaneously. The CCD detectors have very low dark signal and their sensitivity is comparable to photomultipliers or even better. For detection of extremely low signals, the S/N ratio can be improved by increasing acquisition times or by binning signals from several neighbouring pixels. One of the drawbacks of a CCD is the relatively narrow spectral coverage, as another possible weakness may be their low read-out speed given by operating a single read-out register (‘serial readout’). CCD detectors must be handled with care, avoiding strong overexposure by light (like photomultipliers) and, in particular, discharge of static electricity into both the disconnected CCD camera and the control electronics connectors.

2.3 Monochromators and spectrographs A monochromator serves to disperse the analysed light signal into a spectrum using a dispersion element (grating or prism), and then to cut out a narrow (quasi)-monochromatic part of the spectrum by the exit slit, located at the rear (output) focal plane. A monochromator can be tuned manually (e.g. for selecting the appropriate excitation wavelength) or scanned automatically by rotating the dispersion element—in this case the spectrum moves continuously across the exit slit and can be recorded using a single-channel detector. A spectrograph projects the spectrum onto a ﬁxed position in its output focal plane. The exit slit is replaced by a photographic plate or a multichannel detector. Most modern spectrographs are equipped with two output channels— a lateral output (selectable by a moving mirror), being ﬁtted with a slit, enables application of the spectrograph in a scanning monochromator mode (Fig. 2.13). An imaging spectrograph is a special type of spectrograph, equipped with purpose-built optics that reduces optical aberrations. The spectral image of the entrance slit is perfectly sharp over a large area at the output image plane (typically 1 cm high and 2 cm wide), not only in its central part (close to the optical axis) as was the case of a monochromator. The terms polychromator and spectrometer can also be encountered in the literature. A polychromator has several parallel monochromatic outputs provided by multiple output slits. A spectrometer is a complete device designed for measurements of optical emission spectra, consisting of a monochromator (or spectrograph) coupled with a detector.2 2 This nomenclature of spectral devices is not employed systematically in the scientiﬁc literature. The terms monochromator, spectrograph or spectroscope are often used arbitrarily like

31

32

Experimental techniques

Fig. 2.13 A HR 320 monochromator– spectrograph. Adapted from Horiba Jobin Yvon ﬂyer.

Fig. 2.14 The most common optical designs of spectral devices. (a) Littrow type with an autocollimating prism, (b) Walsch type with a prism, (c) Ebert construction with a grating, (d) Czerny–Turner type with a grating. The quality of spectral imaging increases from (a) to (d).

There are various designs of optical spectral devices with different levels of compensation for spherical aberration, astigmatism and coma, observed when displaying the spectral elements. Some of these designs are shown in Fig. 2.14. Most of the currently fabricated monochromators suitable for luminescence spectroscopy are of the Czerny–Turner type (Fig. 2.14(d))—see for example the HR 320 monochromator–spectrograph in Fig. 2.13. Other, somewhat less familiar optical schemes are those by Ebert–Fastie, Gillies, Wadsworth, the Rowland’s construction with a concave grating and many others; for more details the reader is referred to the special literature [13, 14, 15]. The basic quantities describing the properties of a monochromator or spectrograph are dispersion, resolving power, and throughput (aperture). We shall

synonyms (originally a spectroscope denoted a device producing an optical spectrum for visual observation).

Monochromators and spectrographs

33

Fig. 2.15 Illustration of the deﬁnition of angular and linear dispersion.

describe them only to the limited extent necessary for the experimental foundations of luminescence spectroscopy.

2.3.1 Dispersion and resolving power Let us consider two light beams whose wavelengths differ by dλ. They leave the dispersion element at angles differing by dθ. We can deﬁne the angular dispersion as dθ (rad/nm). (2.14) dλ The spatial separation d between two spectral lines λ, λ + dλ in the exit slit plane depends on the focal length f of the spectral device, determined by a focusing mirror or lens, see Figs 2.13 and 2.15: D=

d = f dθ.

(2.15)

The linear dispersion L is then deﬁned as dθ d = f = f D. (2.16) dλ dλ More frequently its inverted value, the so-called reciprocal linear dispersion, is used: dλ 1 dλ 1 = = (nm/mm). (2.17) L −1 = d f dθ fD L=

To make an order-of-magnitude estimate, let us consider a simple diffraction grating and light incident at an angle α = α(λ). Light diffraction is described by the the grating equation d(sin α + sin θ ) = kλ (d is the grating constant, k is the diffraction order). By differentiating with respect to λ we obtain k . (2.18) d cos θ In order to estimate D we approximate θ ≈ 0◦ (corresponding to the situation when the analysed light impinges on the grating at an angle α = 0 and the spectrum is observed in a direction almost perpendicular to the grating plane). Then for a grating with 1200 grooves/mm operating in the ﬁrst diffraction order we obtain an angular dispersion D = 1/d = 1.2 × 103 rad/mm = 1.2 × 10−3 rad/nm. A monochromator with f = 500 mm features a linear dispersion D = dθ /dλ =

34

Experimental techniques L = 500 × 1.2 × 10−3 = 0.6 mm/nm and reciprocal linear dispersion L −1 ≈ 1.66 nm/mm. Therefore, in the case of luminescence spectroscopy, when—as we shall specify below—neither very high dispersion nor excessive spectral resolution is required, the spectral devices possess reciprocal linear dispersion in the range of 1–10 nm/mm. The importance of the reciprocal linear dispersion L −1 results from the fact that the spectral bandwidth λ of a given device is simply determined by L −1 (declared by the manufacturer) and the mechanical slit width (set by the experimenter) via the relation λ = L −1

(2.19)

that follows immediately from (2.17). In our example (a monochromator with L −1 = 1.66 nm/mm) for a chosen slit width of = 0.5 mm we thus ﬁnd λ = 0.83 nm. Note that eqn (2.19) is strictly valid only when both the entrance and exit slits are of the same width . This setting is commonly used in spectroscopy for optimizing spectral brightness and facilitating spectral correction procedures (see Section 2.8). The angular dispersion of a prism can be found by differentiating the condition of minimum deviation (see e.g. [14, 16]) which yields D=

2sin (ϕ/2) 1 − N 2 sin2 (ϕ/2)

dN , dλ

(2.20)

where φ is the prism apex angle, and N and dN /dλ are the refractive index and material dispersion of the glass (or other material) from which the prism is fabricated, respectively. In the case of a monochromator, the measurement of the spectra is performed by rotating the dispersion element, thereby scanning the spectral image across the exit slit. Most grating monochromators are equipped with a so-called sine-drive scanning mechanism that ensures linear scanning of the wavelength in time, which means λ = const t. The principle of the sine-drive mechanism is shown in Fig. 2.16. There is a triangle ABC; one of its sides (a) is allowed to vary linearly in time t by means of a precise motor-driven screw, a = a0 + vt. The length of the hypotenuse c, which is anchored by a balljoint at point B, is constant. The second side b is carried in a sliding assembly allowing its length to be varied. Then the angle γ is a function of time, γ = γ (t). By differentiating the goniometric relation sin γ (t) = (a0 + vt)/c we ﬁnd cos γ dγ = (v/c)dt.

(2.21)

A grating can be coupled with this mechanical system in such a way that γ = θ. (Spectroscopic gratings have an asymmetric proﬁle of grooves—the so-called blaze, which enables efﬁcient diffraction of a selected spectral range into the desired angle and diffraction order.) Then eqn (2.21) is replaced by cos θdθ = (v/c)dt and using (2.18) we obtain (k/d)dλ = cos θdθ

or

(k/d)dλ = (v/c)dt,

Monochromators and spectrographs

35

Fig. 2.16 Schematic of a sine-drive mechanism.

therefore, in the given diffraction order k we have λ = const t; the wavelength scan is linear in time. A simple modiﬁcation of the sine-drive (Fig. 2.16) is possible: the length of the hypotenuse c can be varied in time using the screw mechanism while a is kept constant. Then the reciprocal wavelength ν ∗ = 1/λ, called the wavenumber, is a linear function of time ν ∗ = constt. This design is referred to as a cosecant-drive (or just a cosec-drive) since here one deals with a linear temporal variation of the function 1/ sin γ = cosec γ . This drive makes the spectrum to be scanned linear in the photon energy hν = hcν ∗ instead of in wavelength, which could be advantageous for many experiments as well as their physical interpretation. Indeed, it is used in some Raman spectrometers. In the past few decades, most monochromators were provided with sine-drives but modern spectrographs are equipped with direct drives, where a motor rotates the grating directly (through some gear wheels). The number of motor steps per unit wavelength in the course of scanning is not constant and is driven by control software. The beneﬁts of this design are a very high speed of grating rotation from one position to another, possible integration of more selectable gratings in one holder, and use of cheaper mechanical components. Unlike in gratings, there is no simple mechanical way to ensure linear scanning of λ or ν ∗ in a prism monochromator. The angular dispersion of a prism as given by eqn (2.20) contains the dispersion relation N = N (λ) which is strongly nonlinear in glasses and other optical materials. Therefore, spectra measured using a prism monochromator usually have a nonlinear wavelength scale; compare, e.g., Fig. 2.28 (a prism monochromator) with Fig. 1.1 (a grating monochromator). Another important fact contained in relations (2.18) and (2.20) is worth pointing out: the dispersion of a grating or prism is independent of its size— e.g. two prisms made of the same material and having equal apex angles ϕ have equal dispersion regardless of size (Fig. 2.17). In other words, the dispersion of a spectral device is deﬁned in the framework of geometrical optics, where diffraction due to ﬁnite beamwidth is not taken into account. On the other hand, the resolving power R, deﬁned with the aid of the smallest resolvable difference between two closely spaced spectral lines λ as R = λ/λ, is limited just by diffraction of the light beam, whose diameter is driven by the lateral size of the dispersion element. A small prism or grating with a small effective area gives rise to sizeable broadening of spectral lines in

36

Experimental techniques

Fig. 2.17 Illustrating the distinction between dispersion and resolving power. Two prisms (a) and (b) have equal (angular and linear) dispersion but the bigger one (b) has higher resolving power, as shown by the proﬁles of two closely spaced spectral lines in the exit focal plane.

the exit slit plane due to light diffraction. Consequently, taking into account Rayleigh criterion for the resolution of two peaks, the resolving power is decreased (Fig. 2.17). But even having a sufﬁciently large dispersion element, the effective cross-section of the beam to be analysed may happen to be limited by the insufﬁcient diameters of the lenses or mirrors used in the spectral device, and possibly also by improperly collimating the input radiation. Along with diffraction due to the limited diameter of the light beam, another diffraction effect enters the play—diffraction at the entrance slit, which could negatively inﬂuence the output spectral image when the slit width is set too narrow, below some ‘reasonable’ limit.3 Let us discuss both of these phenomena in greater detail. To begin with, suppose we can neglect diffraction at the entrance slit. It is obvious that reducing the width of the monochromator slits leads, according to eqn (2.19), to narrowing of the transmitted spectral bandwidth λ and, consequently, to increased spectral resolution. Let us employ the term theoretical or ultimate resolving power for Rt = λ/λopt , where λopt is the (minimum) spectral bandwidth at which the input slit diffraction does not yet become evident, and thus an ultimate resolution Rt is achieved. Let us consider this situation, as occurring in a prism monochromator, displayed in Fig. 2.18. We remember that the diffraction angle on a circular aperture of diameter W (here the ‘effective aperture stop of the monochromator’) is expressed by the wellknown relation δθ ≈ λ/W,

(2.22)

if we omit the numerical factor 1.22 on the right-hand side for the sake of simplicity. Now, should two closely spaced lines be resolved (λ = λopt ), the condition θ = δθ must be satisﬁed according to Fig. 2.18. The angle θ 3 Note that in spectral devices equipped with a diffraction grating, the interplay between three diffraction effects is taking place—diffraction on the input slit, on the grating and diffraction due to the ﬁnite beam size.

Monochromators and spectrographs

37 Fig. 2.18 Illustrating the resolving power of a simple prism monochromator. (a) Rays leaving the prism and propagating through an exit focusing lens. The lateral size of the beam W is basically determined by the prism dimensions. The images of two spectral lines in the plane of the exit slit have ﬁnite width due to light diffraction. (b) Proﬁles of two closely spaced spectral lines in the plane of the exit slit that meet Rayleigh resolution criterion (i.e. the centre of one linear diffraction pattern falls on the ﬁrst minimum of the diffraction proﬁle of the other line).

is determined by the angular dispersion of the prism; by combining eqns (2.14) and (2.22) we obtain Rt = λ/λopt =

δθ W θ W dθ = ≈ W = W D. λopt λopt dλ

(2.23)

Obviously, this relation is valid for any dispersion element. Importantly, it shows that there is a close relation between the angular dispersion D and the ultimate resolution Rt of a dispersion element, and also supplies a qualitative explanation for Fig. 2.17. By inserting the angular dispersion into eqn (2.23) for the grating (2.18) or prism (2.20), respectively, we obtain, after some simple algebra, for the ultimate resolving power of the grating Rt = m k

(2.24)

and for that of a prism (valid under the assumption that the whole prism entrance face is illuminated) Rt = t

dN . dλ

(2.25)

In eqn (2.24) m stands for the number of illuminated grating grooves (it is easy to show that m = W/d cos θ), and t in eqn (2.25) denotes the width of the prism base, see Fig. 2.17. For example, a grating with 1200 grooves/mm and width of 5 cm has in the ﬁrst diffraction order Rt = 6 × 104 ; a prism made of a heavy ﬂint glass (dN /dλ ≈ 2.7 × 10−4 /nm for blue light) with a base of t = 5 cm features Rt ≈ 1.35 × 104 . In reality, the ultimate resolution power may be decreased by one-third or even more due to imperfections in the mechanical and optical elements, imperfect homogeneity of the optical materials, etc. Coming back to the problem of diffraction at the entrance slit and the determination of the optimum slit width opt , we start with the scheme in Fig. 2.19. The detected light is focused onto the entrance slit under a top angle of 2ϕ and adjusted so that the whole collimating element (lens) of diameter W is covered. Along with the angle ϕ, determined basically by the rules of geometrical optics, the deviation angle due to diffraction at the slit emerges

38

Experimental techniques

Fig. 2.19 The entrance slit of a spectral device should not be set narrower than opt , otherwise, due to diffraction, the incoming light ﬁlls up an angle larger than 2ϕ and part of the signal is lost.

as an independent factor. This diffraction angle ϕd ∼ λ/ increases with decreasing . When setting too small (with the best of intentions to improve resolution), below some optimum value opt , the angle ϕd becomes larger than ϕ and part of the input light fails to meet the lens and is lost for spectral detection. Such a situation has several negative consequences: (i) ﬁrst of all, the brightness of the spectrum drops which might be fatal in studying low-level luminescence signals; in any case the signal-to-noise ratio deteriorates (see Section 2.5); (ii) light passing through the lens hits the internal walls or other parts of the device, thereby producing parasitic reﬂections and thus increasing the background signal (the so-called stray light) which, eventually, (iii) results in futher suppression of the S/N ratio. Moreover, mechanical imperfections, e.g. microscopic damage to the slit blades, can substantially degrade the sharpness of the spectra when setting the slit very narrow. The optimum value opt of the slit width is thus achieved if the diffraction angle ϕd ∼ λ/ opt

(2.26)

is just equal to the angle ϕ given by the geometrical condition ϕ∼

W , 2f

(2.27)

imposed by Fig. 2.19. By comparing (2.26) and (2.27) we obtain opt ≈

2 fλ . W

(2.28)

The reader is, undoubtedly, aware of some oversimpliﬁcation of the discussion given above; in particular relation (2.26) valid for Fraunhofer diffraction of plane waves must be considered as an approximation only. Thus, to make an order-of-magnitude estimate, we neglect also the numerical factor 2 in (2.28), we shall consider a monochromator with focal length of f = 60 cm and effective width of the dispersion element W = 6 cm, we put λ = 1 μm and then we get for the optimum slit width opt ≈ f λ/W ≈ 10 μm. This is a very important message for luminescence measurements: Decreasing the input slit width below approximately 10 μm makes no sense—resolution will not be improved; on the contrary the quality of the spectrum will deteriorate and the S/N ratio will decrease.

Monochromators and spectrographs

39

Of course, in most practical luminescence experiments much wider slits (100 μm or more) are used, partly due to low light ﬂuxes and also because the luminescence spectra are often composed of broad bands that do not require an extremely high resolution, as already stressed above. Nevertheless, one can meet situations where the luminescence emission spectrum of a semiconductor contains a series of narrow, sometimes closely spaced lines (see, e.g., the spectrum of bulk silicon in Fig. 1.1). To resolve such lines, the width of the slits must be chosen very carefully. The optimum width is found as a tradeoff between an acceptable noise level and the requirement to distinguish the closely spaced lines. Here, it appears useful to realize that by opening slits to a real value real > opt , the theoretical limit of the resolving power Rt is relaxed to a real value Rreal called the ‘effective-slit-width-limited resolving power’: Rreal = λ/λreal = λ/L −1 real . An approximate relation between these two resolving powers may be written as opt Rt . Rreal ≤ (2.29) real All this is illustrated schematically in Fig. 2.20. To conclude our discussion of the dispersion properties we shall attempt to compare brieﬂy prism- and grating-based spectral devices. A diffraction grating gives a linear sweep in λ or ν ∗ = 1/λ, which is one of its main merits. Another advantage, as we have seen, is—as a rule—the higher resolving power compared to a prism of comparable size. On the other hand, a grating monochromator or spectrograph has at least two unpleasant properties: Firstly, different wavelengths can be sent to the same diffraction angle, in other words, spectra of different diffraction orders may partially overlap one another. An inexperienced or careless experimenter can consequently come to a completely erroneous interpretation of his observation. The problem is usually solved by inserting appropriate band-pass or edge ﬁlters in front of the input slit in order to restrict the spectral width of the detected signal. A second disadvantage of gratings is less familiar—the diffraction efﬁciency of a grating can often exhibit a sharp local minimum at certain wavelengths. This is known as Wood’s anomaly (the physical origin of which is based presumably on the generation of surface plasmons in the metal coating, but is not known in all its details). Such a minimum is projected onto the measured spectrum and might be misinterpreted as a spectral feature. Therefore, a correction for the spectral response of the apparatus is often necessary; this will be treated in Section 2.7. A prism spectrometer also has its pros and cons. The main advantage over a grating device is that the apparatus is absolutely free from any problems connected with the overlap of different order spectra. In general, prisms may also have a wider dispersion range than gratings; depending on the material the prism is made of (various glasses, ionic crystals, etc.), the application range can extend from the ultraviolet to the far-infrared spectral regions. On the other hand, as the main drawback of the prism, its nonlinear dispersion along with the relevant nonlinear sweep of the spectra inducing a signiﬁcant decrease in resolving power at longer wavelengths—as follows from eqn (2.25)—is usually noted.

Fig. 2.20 Real resolving power of a spectral device as a function of the slit width . The quantity Rt stands for the ultimate resolving power. When is large enough, diffraction effects on the slits may be neglected and the simple relation (R2 /R1 ) = ( 1 / 2 ) holds true.

40

Experimental techniques Even if none of these two types of dispersion elements is ideal, most commercial spectrometers produced during the last 20 or 30 years are based on gratings. The advanced technology of holography has led to striking improvements in the quality of holographic diffraction gratings, which are now available in a wide range of groove densities and sizes for reasonable prices. In order to overcome the disadvantage of the relatively narrow spectral range, several interchangeable gratings are mounted on a revolving table (turret) inside the spectrometer. We shall conclude this subsection with a short note on wavelength calibration of monochromators and spectrographs. The current commercially available spectral devices have an internal control system for rotating the grating. The exit (detected) wavelength is calculated and indicated by control software. Nevertheless, the correctness of the wavelength calibration must be checked from time to time, especially after moving the device or before some highresolution measurements. Wavelength calibration is done using a light source of well-deﬁned wavelengths. For a fast check we can use some lines of gas lasers, e.g. the red line of a He-Ne laser at 632.8 nm. Low-pressure discharge lamps (ﬁlled with Hg, Ar, Kr, Ne, etc.), whose emission wavelengths are tabulated, are considered to be the best sources of calibration spectral lines. Calibration of a monochromator is checked by scanning the spectrum of a calibration lamp using narrow slits and comparing the result with the tabulated wavelength values. Calibration of a spectrograph is more sophisticated: in the ﬁrst step the ‘monochromator-like’ calibration at the centre of a multichannel detector (more precisely, at the point of intersection of the optical axis of a spectrograph with the exit image plane) must be checked, and the second step calibrates the dispersion of wavelengths on the multichannel detector (offaxis points). The appropriate calibration procedures should be integrated in the control software and described in a user manual.

2.3.2 Throughput of monochromators and spectrographs In order to deﬁne the term throughput we begin by recalling the deﬁnition of the brightness (radiance) of an extended emitter, Fig. 2.21(a). The radiant ﬂux φi , emitted by a surface element S of the emitter, is proportional to the size of this element, to the cosine of the angle ϑ between the direction of radiation and the normal to S, and to the magnitude of the pertinent solid angle ω, i.e. φi ∼ S cos ϑω. The proportionality factor in this equation is just the brightness of the emitter B: φi = BS cos ϑω.

(2.30)

Suppose the element S is represented by the uniformly illuminated (effective) area of a monochromator entrance slit. Due to the narrow ﬁeld of view of the collimator optics we can take cos ϑ ≈ 1 and approximate the angle ω via the relation ω ≈ W 2 / f 2 , see Fig. 2.21(b). Equation (2.30) then reads φi ≈ B S (W 2/f 2 ).

(2.31)

Monochromators and spectrographs

41

Fig. 2.21 Illustrating the deﬁnitions of (a) the brightness of an extended ﬂat emitter and (b) the aperture ratio of a spectral device.

Let us ﬁrst consider the case of a monochromator. Here an essential quantity is the (quasi-)monochromatic luminous or radiant ﬂux φλ at the exit slit that induces the photoelectric response of a single-channel detector. The efﬁciency and/or transmittance of all optical elements inside the monochromator (mirror reﬂectivity, lens transmittance, efﬁciency of the diffraction grating, or prism transmittance) at a wavelength λ can be included in the coefﬁcient κ(λ) < 1. Then, based on eqn (2.31), we can write for the output ﬂux

(2.32) φλ = κ(λ) φi = κ(λ) B S W 2/f 2 . The throughput of the monochromator is then deﬁned as ¡ κ(λ) φi = κ(λ) S (W 2 / f 2 ) ≈ κ(λ) S(A/ f 2 ). (2.33) mono = B Here A stands for the effective area of the dispersion element. Note that the throughput is proportional to the maximum solid angle that just illuminates the whole area of the collimator. It should be noted that the deﬁnition of the throughput is not standardized. Sometimes it is taken simply 2 as (A/ f ) or even A/ f 2 ≈ W/ f . Here, in analogy with a photographic camera, the aperture ratio is given by 1/#, where (aperture number) # = f /(diameter of the entrance pupil). Producers of spectral devices usually give the throughput4 in the form of ( f /#), with # = f /W ranging from about 3.5 to 20 (the bigger this number the lower is the throughput of the device!). This simpliﬁed (commercial) deﬁnition of the throughput does not take into account the factor S in eqn (2.33), i.e. the variability of the slit width. In luminescence spectroscopy, dealing mostly with weak signals, spectral devices with a large throughput are usually preferred. However, similar to the mutual interconnection between dispersion and resolving power, there exists a simple relation between the throughput and resolving power of a 4 Unfortunately, the terminology is not universal. Different terms like luminosity, throughput, aperture, aperture ratio, acceptance angle, etc. are used.

42

Experimental techniques device. In what follows we shall derive this relation and discuss its practical consequences. Let w and h be the width and height of the illuminated part of the entrance slit, respectively. Then S = wh and the quantity α = w/ f stands for the angular width of the entrance slit as ‘seen’ from within the device. Analogously, β = h/ f means the angular height of the slit. Consequently, αβ = S/ f 2 and instead of eqn (2.32) we write φλ = κ B α β W 2 .

(2.34)

Using the relations for the linear and angular dispersions (2.19) and (2.17), respectively, the transmitted bandwidth λ determined by the slit width5 w reads 1 λ = L −1 w = w = α D −1 fD and eqn (2.34) takes the form φλ = κ B β λ D W 2 . Fig. 2.22 A continuous spectrum characterized by its spectral brightness Bλ . The entrance slit is illuminated by the spectrally integrated brightness B = Bλ dλ.

(2.35)

In case of a sufﬁciently broad continuous spectrum (common in luminescence) we can introduce the ‘spectral brightness’ of the entrance slit Bλ by replacing B → Bλ λ (see Fig. 2.22). Then, the output ﬂux is given by φλ = κ Bλ β D W 2 (λ)2 ,

(2.36)

which can be further modiﬁed by introducing the real resolving power Rreal φλ =

κ Bλ β D W 2 λ2 . 2 Rreal

(2.37)

The ﬁnal relation between resolving power and throughput Σmono we are looking for is derived from (2.37) using eqns (2.32) and (2.33) and reads Rreal =

κ βD W 2 λ .

(2.38)

mono

This relation shows that the real resolving power and the (real) throughput of a monochromator are, in agreement with intuition, inversely proportional to each other—widening the slits boosts the output signal but reduces the spectral resolution. Again, the experimenter must ﬁnd a viable compromise using his/her experience. However, more interesting conclusions can probably be drawn from eqn (2.37): (a) The transmitted (output) light ﬂux φλ scales with the resolution like (1/Rreal )2 . This means that the output signal decreases quadratically with increasing resolution. In other words, the output signal level increases with the spectral (and thus also mechanical) slit width like (λ)2 ; for that matter see also eqn (2.36). This relation can sometimes be used during an experiment to estimate quantitatively the signal level. If we need (e.g. due 5 We consider a symmetrical device with equal widths of both slits, consistent with the previous

text.

Monochromators and spectrographs

43

to low signal levels at the emission band edges) to increase the ‘detection sensitivity’, one option is to set wider slits. Now, we know that doubling the slit width entails a fourfold increase in signal level. We have to keep in mind, however, that the above quadratic relation holds well for broad structureless spectra only (as follows from the introduction of the spectral brightness Bλ , see Fig. 2.22). Besides, there are plenty of more precise means to increase sensitivity. (b) The output ﬂux φλ scales linearly with β, the angular height of the illuminated slit. Therefore, it appears highly desirable to illuminate the whole height of the entrance slit, which, however, is difﬁcult to arrange because the emitting spot is commonly of circular shape. Nevertheless, when the signal is brought by an optical cable, its termination can be shaped to ﬁt the entire surface of the entrance slit. Also in cases of weakly absorbed or homogeneous two-photon excitation of a sufﬁciently voluminous sample by a laser beam (Chapter 5, Fig. 5.15(b)), the elongated luminescence spot can be oriented so that its image covers the entrance slit. (c) The relation φλ ∼ W 2 implies that a high-throughput monochromator has to be equipped with a large grating or prism. In the case of a spectrograph it is the so-called irradiance of a multichannel detector (the radiant ﬂux at the spectrometer output divided by the illuminated area) that has a crucial role to play, rather than the radiant or luminous ﬂux itself. This quantity determines the exposure time and the signalto-noise ratio. Luminescence radiation, spatially distributed by a dispersion element, projects the entrance slit area S = wh characterized by the spectral brightness Bλ to its image S = w h (in the plane of the multichannel detector, see Fig. 2.23), the dimensions of the slit and its image being identical (w = w , h = h ) in the case of a symmetrical device. In analogy with deﬁnition (2.33) we deﬁne the throughput of the spectrograph Σspectro using the irradiance (κ(λ)φi /S ) on the area S = w h of the slit image created by quasimonochromatic light λ ± λ/2 as 2 2 ¡ φλ φi κ(λ) S W W = = κ(λ) = κ(λ) . spectro = Bλ λ S Bλ λ S S f f (2.39) Now we can express the ‘spectral irradiance’ of the detector with respect to its full height h 0 ≥ h as E λ = φλ / h 0 w, as follows from Fig. 2.23. This expression for E λ can then be easily modiﬁed using eqn (2.32) and the deﬁnition of the aperture number # as 2 φλ κ(λ) Bλ λ S (W/ f )2 h 1 λ . (2.40) = = κ(λ) Bλ Eλ = h0 w h0 w h0 # Rreal Relation (2.40), valid for a spectrograph, is analogous to expression (2.37) relevant to a monochromator. Here, again, are some conclusions important for experiments: (a) The irradiance E λ decreases proportionally to (1/Rreal ), unlike the transmitted ﬂux at the exit slit which scales as (1/Rreal )2 .

Fig. 2.23 Image of the entrance slit on a multichannel detector located in the spectrograph exit plane. h 0 is the height of the sensitive area of the detector, and h and w stand for the height and width of the entrance slit image, respectively.

44

Experimental techniques (b) The irradiance E λ is proportional to (h/ h 0 ). Therefore, it is desirable to choose a combination of spectrograph, multichannel detector and a method to illuminate the entrance slit so that h = h 0 , in order to maximize E λ . Naturally, the case h > h 0 should be avoided because part of the signal ﬂux fails to meet the detector. (c) The irradiance E λ scales like (1/#)2 , i.e. the irradiance of the detector increases with the square of the aperture ratio. This factor is actually the most important one among those aimed at maximizing the detector irradiance.

2.4 Signal detection methods in luminescence spectroscopy Following the discussion of spectral devices and detectors we are now going to describe brieﬂy methods of signal treatment in spectroscopy. Essentially this means dealing with the principles of electronic devices that treat the electric signal from the photodetector. Here we concentrate on single-channel detectors because multichannel ones are quite straightforward and user friendly—the accumulated photoinduced charges, after being digitized, are simply transferred to a computer to be processed by software. For the sake of simplicity we consider in this section only continuous-wave (cw) luminescence signals, i.e. signals excited by a continuously emitting lamp or laser. In particular, we are going to describe two methods: phasesynchronous detection and the photon-counting technique. Experimental methods of pulsed luminescence signals are left to Section 2.9.

2.4.1 Phase-synchronous detection The simplest arrangement of optical cw signal detection is obviously direct current detection—time invariant radiant ﬂux (at the monochromator exit slit) induces in the attached photomultiplier a constant photocurrent, which is subsequently directly measured by a voltmeter connected to a load resistance (Fig. 2.5(b)). In the case of extremely low luminescence photon ﬂuxes a DC preampliﬁer could be inserted between the photomultiplier and the voltmeter. However, in reality such DC measurements are rarely applied, because low photocurrents are commonly comparable in magnitude with the photomultiplier dark current or only slightly higher. The dark current amplitude must be subtracted in this case from the detected signal, which leads to important errors like in any other indirect measurements where two comparable quantities are to be subtracted. The inevitable presence of broad-frequency noise makes the quality of the resulting output even worse because there is no electronic component available for noise suppression. It therefore becomes obvious that weak continuous optical signals can be successfully detected only when applying some electronic device that is able to extract reliably a signal buried completely in the dark current and/or in various types of noise whose amplitude may be higher by several orders of

Signal detection methods in luminescence spectroscopy

45

magnitude. This is possible, ﬁrst and foremost, by employing the method of phase-synchronous detection through a device called a lock-in ampliﬁer. This device is able to measure alternating voltage or currents and to provide a corresponding DC output voltage that scales linearly with the input signal level (the output signal level is usually much higher than the input level, hence the term ‘ampliﬁer’). Here, only certain frequencies of the input signal are detected while virtually all the others are suppressed (mainly all noise with a broad frequency spectrum), hence the term ‘lock-in’. The ability of a synchronous detector to extract and amplify a low synchronous signal buried in noise is characterized by a quantity called the dynamic reserve. This is the ratio of the maximum acceptable amplitude of the asynchronous (noise) signal (i.e. the amplitude value which just starts to induce nonlinearity and saturation of input circuits) to the peak synchronous signal giving a full-scale DC output. The dynamic reserve of up-to-date lock-in ampliﬁers is extremely high, routinely reaching values of 100 dB (!) or even higher. Any lock-in ampliﬁer contains two key parts: a mixer (phase detector) and an integrator. The principle of operation of a lock-in ampliﬁer is illustrated in Fig. 2.24. The input to the mixer (left side of Fig. 2.24) receives two electric signals—the measured sine wave signal e1 from a photodetector and a square wave so-called reference signal e2 (the origin of these particular forms of signals will be described later). The output of the mixer e3 is the product of the input signals: e3 = e1 e2 . The technical solution consists in alternating usage of a direct and an inverting ampliﬁer in the mixer input. The amplitude of the reference signal E 2 can be put equal to unity. Then Fig. 2.24(a) shows immediately that for equal frequencies of both the signals ( f 1 = f 2 ) and provided their relative phase shift is equal to 0, 2π, 4π, etc. the output mixer signal e3 contains a pulsating voltage of positive polarity only. The measured signal is said to be synchronous with the reference. Enabling e3 to pass through the integrator having a time constant τ = RC (right-hand side of Fig. 2.24), a DC output voltage with amplitude E DC proportional to the amplitude of the measured input signal E 1 is obtained.

Fig. 2.24 Principle of a lock-in ampliﬁer. The left-hand side shows a mixer and the right-hand side an integrator (low-pass ﬁlter). (a) For a synchronous input signal f 1 = f 2 we obtain a non-zero DC output signal E DC = 0. (b) Asynchronous input signal f 1 = f 2 along with a sufﬁciently long time constant τ = RC result in a zero DC output level.

46

Experimental techniques

Fig. 2.25 Demonstration of the phase sensitivity of a lock-in ampliﬁer. The input signal from a photodetector e1 and the reference signal e2 have equal frequencies but the DC output is strongly dependent on the phase shift between these two signals.

In the case of an asynchronous signal f 1 = f 2 (Fig. 2.24(b)) the signal e3 contains both positive and negative components compensating each other if a long enough time constant τ is applied, and thus zero DC output results. It can be seen that the lock-in ampliﬁer acts as an extremely selective ﬁlter processing and amplifying only the ‘meaningful’ signal component, i.e. that corresponding to the reference frequency; this is the succinct essence of the principle of the lock-in ampliﬁer. There are, however, additional useful features of synchronous detection that remain to be explained. First of all, these is the phase sensitivity, which strongly inﬂuences the magnitude of the output signal—for certain values of the phase shift between the signal and the reference, the output E DC may be zero even if the measured and reference signals have the same frequency f 1 = f 2 (!). Two examples ( f 1 = f 2 while the phase shift is different from 2πn, n being an integer) are demonstrated in Fig. 2.25: the phase shift φ = 90◦ (or (2n + 1)π/2) induces zero DC output, while under a shift of φ = 180◦ (or (2n + 1)π) the output signal E DC is of the same amplitude as for φ = 0◦ but of negative polarity. This is why a lock-in ampliﬁer is sometimes also called a phase-sensitive detector. The phase sensitivity has several interesting consequences. But prior to entering the relevant discussion we should describe how cw luminescence radiation is converted into a sine-modulated input signal and how the reference signal is generated. Everything is based on simple mechanical chopping of the light beam (as a rule, the excitation beam is chopped, less commonly chopping of the photoluminescence signal is applied—see Fig. 2.2(b)) by a mechanical chopper, which is a rotating disk with periodically arranged slots. (Of course, mechanical chopping itself cannot create the sinusoidal signal shown in Figs 2.24 and 2.25, nevertheless, the input circuits of a lock-in ampliﬁer are able to adapt a chopped cw signal into a sine wave.) The reference signal is generated by an optical pair (a LED and a photodiode) attached to the chopper. In this way the reference and measured signal are modulated by the same mechanical system and undoubtedly f 1 = f 2 holds true. However, there is certainly a non-zero phase shift φ between both signals due to the different response times of the photomultiplier and the reference photodiode along with different delays introduced by wiring and circuits on the path of both signals towards the mixer input. Here, the phase sensitivity of the lock-in ampliﬁer appears to be very useful. The phase shift φ between the two input signals can be continuously tuned

Signal detection methods in luminescence spectroscopy

47 Fig. 2.26 Block diagram of a phase-sensitive detector. Both the modulated input and the reference signal are ﬁrst ampliﬁed and possibly shape-adapted. The reference signal branch contains an adjustable phase shifter. After passing through the RC circuit (low-pass ﬁlter) the signal is ampliﬁed again.

to maximize the output signal amplitude E DC . Up-to-date lock-ins can do this phase tuning automatically. Another useful feature is the possibility of alternating the polarity of the output simply by setting the phase shift to ±180◦ . The converse is also true: if the device, on its own, automatically changes the phase by ±180◦ during measurement, this indicates that the polarity of the input signal has changed, which may carry important experimental information. (While one can hardly meet such a situation in luminescence spectroscopy, it is, however, quite common in photoelectric measurements.) Finally, the phase sensitivity proves very useful in ﬁltering out all kinds of noise, even if their frequencies may happen to be equal f 1 = f 2 , because they have no ﬁxed phase relation to the reference signal, i.e. their phases ﬂuctuate randomly. The time constant τ = RC also deserves a short discussion. The illustrations in Figs 2.24 and 2.25 are oversimpliﬁed. It can be shown that the output of the mixer can contain not only pulsating components with frequency f 1 = f 2 , but also with f 1 = (2n + 1) f 2 where n is an integer. Moreover, asynchronous input frequencies reveal themselves at the mixer output as sum and difference frequency components ( f 1 + f 2 ), ( f 1 – f 2 ) and higher harmonics. These frequencies could possibly appear as noise superimposed on the output voltage E DC but they are mostly ﬁltered out by the RC circuit, which then acts not only as an integrator but also as a low-pass ﬁlter. A block diagram of a lock-in ampliﬁer is shown in Fig. 2.26. Concerning the optimum choice of the time constant τ , smoothing of the DC output is evidently improved with increasing time constant (available values of τ range from microseconds to tens of seconds) but, on the other hand, very high values of τ make the overall response of the device slower. This means that the speed of scanning a spectrum across the exit slit must be adapted to the selected time constant, otherwise the acquired spectral shape may be distorted. Very long time constants can lead to intolerably long acquisition times. This problem will be discussed in more detail in Section 2.5. We shall conclude our discussion of the synchronous detection technique by mentioning the limits of the method. One limit arises from luminescence kinetics and its relation to the chopping rate. If the mechanical chopper modulates the excitation beam, the expected square wave photoluminescence signal may be distorted owing to the ﬁnite speed of the rise and decay of luminescence (Fig. 2.27). If the relevant characteristic time constants are comparable to or even longer than the chopping period T2 = 1/ f 2 , the lock-in ampliﬁer input signal loses its modulated shape and can no longer be processed by the device (Fig. 2.27(d)). Possible solutions are obvious—either decrease the chopping

48

Experimental techniques

Fig. 2.27 Temporal trace of the photoluminescence response excited by a mechanically chopped beam with frequency f 2 . Curve (a) pertains to luminescence with very fast kinetics, i.e. the rise and decay times are short compared to T2 = 1/ f 2 ; curves (b)–(d) illustrate luminescence with slower and slower response. A lock-in ampliﬁer will perceive case (d) as almost an unmodulated DC signal and will not respond to it.

Fig. 2.28 Low-temperature photoluminescence spectrum of AgBr under excitation with a cw UV laser and using low-frequency synchronous detection ( f 2 = 500 Hz). The spectrum contains three bands: luminescence of the electron–hole liquid (EHL) at ∼2.6 eV, a band IodLO (BE) due to radiative recombination of excitons bound to ions of an isoelectronic unintentional dopant (iodine) at ∼2.5 eV, and a band at ∼2.1 eV due to a residual impurity. The inset shows the spectrum obtained under high chopping frequency f 2 = 100 kHz, which eliminates the iodine-related band IodLO (BE) with a decay time of ∼ 25 μs and retains only the fast band of EHL with a decay time of about 20 ns. Adapted from Pelant et al. [17] and Hulin et al. [18].

frequency f 2 (which is not always possible) or modulate the luminescence instead of the excitation beam (which is experimentally not so easy to do). On the other hand, the above drawback can sometimes be turned into an advantage and applied as a simple tool for time-resolved luminescence spectroscopy. Suppose that the material under study shows two luminescence emission bands, partially overlapping spectrally but having substantially different kinetics. Then these spectral peaks may be cleanly separated by performing two measurements with a lock-in ampliﬁer under two different chopping frequencies f 2 f 2 . While the measurement at frequency f 2 reveals a spectrum comprising both the bands, the measurement at frequency f 2 shows only the ‘fast’ band provided this frequency is high enough to eliminate the slow component. An example is shown in Fig. 2.28 [17, 18]. The second limit beyond which application of the lock-in technique serves no useful purpose is detection of very low light ﬂuxes, where the discrete character of both light (photons) and detection events (photoemission from the photomultiplier photocathode) becomes apparent. This situation is nicely illustrated by Fig. 2.29. The lock-in ampliﬁer cannot detect very weak signals since they are formed by an array of random anode pulses (Fig. 2.29(c)) rather than by a DC component processable through chopping into a form suitable for phase-sensitive treatment. Detection of such low photon ﬂuxes requires another method called photon counting.

2.4.2 Photon counting Every current pulse at the output of a photomultiplier, shown in Fig. 2.29(c), corresponds to the impact of one photon on the photocathode, accompanied by emission of one photoelectron. Therefore, the number of pulses Nr registered per unit time is proportional to the number of photons Nh hitting the photocathode during the same time interval, i.e. to the incident light ﬂux or

Signal detection methods in luminescence spectroscopy

intensity. (In quantitative measurements, e.g. those of the quantum efﬁciency of luminescence, we have to keep in mind that these quantities are only proportional to each other, not equal. The number of registered pulses Nr is always lower than the number of incoming photons Nh , the proportionality coefﬁcient being the product of the photocathode quantum efﬁciency ηph and the collection efﬁciency of dynodes αd , which means Nr = ηph αd Nh .) A block diagram of a photon counting apparatus is presented in Fig. 2.30. The output signal from the photomultiplier is composed of single voltage spikes (as already illustrated in Fig. 2.29(c)), generally superimposed on various low- and high-frequency noise and instabilities—circle A. Big pulses are due to photoelectrons emitted from the photocathode while smaller ones come from the thermionic emission in dynodes. This signal is treated by an input ampliﬁer, which multiplies the signal approximately one thousand times and ﬁlters out the low-frequency ripple—circle B. The ampliﬁed pulses enter a discriminator (circle C), which eliminates pulses that are below a certain adjustable discrimination level (dashed line in the circle B). In this way the parasitic pulses originating in the thermionic emission of dynodes are ruled out. Each pulse passing through the discriminator generates at the output a standard TTL voltage pulse (circle C) and these pulses are counted by a common counter. The counter can send out either digital information about the number of pulses per unit time or it can produce an analogue signal (for a plotter) employing a digital-to-analogue converter. The principle of the photon-counting method looks simple but the apparatus requires excellent temporal and noise characteristics of all of its components. The most critical is selection of a suitable photomultiplier tube meeting stringent criteria imposed on its parameters, as well as the selection of its high anode–cathode voltage and of the appropriate discrimination level of the discriminator. These issues deserve to be discussed in more detail.

49 Fig. 2.29 Visualization of the output signal of a photomultiplier (chopped at frequency f 2 ) on an oscilloscope screen for different signal levels. (a) The light ﬂux hitting the detector is high enough, single output voltage pulses are merged together. (b) The number of incoming photons is lower; pulses corresponding to the detection of single photons can already be resolved. (c) Very low signal photon ﬂux. The signal from the detector is composed of discrete voltage pulses; there is almost no continuous component. Therefore the lock-in sees only incoherent noise and the DC output level E DC is zero. The signal has negative polarity, which corresponds to the most common photomultiplier wiring with a grounded anode (Fig. 2.5b). Modiﬁed from Hamamatsu [7].

Fig. 2.30 Block diagram of a simple version of a photon counter.

50 Fig. 2.31 (a) Qualitative illustration of a (differential) distribution of photomultiplier pulse heights. The dashed and solid curves are the height distributions for ‘dark’ pulses (photocathode not illuminated) and for ‘light’ pulses (signal photons hit the photocathode), respectively. Such distributions can be measured by making use of a multichannel analyser or a discriminator with adjustable upper and lower levels (see inset). (b) An integral distribution of pulse heights, which can be experimentally acquired with a single-level discriminator. Adapted after a Hamamatsu brochure [7].

Experimental techniques

By no means is every photomultiplier applicable to the photon-counting method. In selecting a suitable photomultiplier the following factors have a crucial role to play: 1. Temporal width of the output voltage pulses. This width must be sufﬁciently short in order to distinguish the height of pulses due to photoelectrons from that of pulses originating in thermionic emission in dynodes. Excess temporal blurring of the electron packets propagating through the photomultiplier could reduce the contrast in amplitude between the two kinds of pulses so that their separation in the discriminator would be impossible. Moreover, shorter pulses enable the photon-counting technique to be applied to higher pulse rates—the upper limit of pulse counting corresponds to the situation in which adjacent pulses become signiﬁcantly overlapped and thus indistinguishable. A common value of the temporal pulse halfwidth in photomultipliers designed for photon counting is about 10–20 ns. 2. A high quantum efﬁciency ηph of photocathode emission and a low anode dark current. It is evident from the very principle of the method that a high signal-to-noise ratio requires high yield of generation of primary photoelectrons from photons hitting the photocathode, along with minimization of the number of thermally released electrons. Quantum efﬁciencies of suitable photomultipliers are usually around ηph = 20–30%. 3. Appropriate distribution of pulse heights. Firstly, we have to explain what we understand by the distribution of pulse heights. One can hardly expect that all the pulses or counts originating from a single photoelectron event on the photocathode (or ‘dark’ counts initiated by thermally released electrons) would have the same amplitude on the anode; the statistical character of secondary electron emission at the dynodes, individual variations in electron trajectories, etc. make the anode pulse heights of both the signal and ‘dark’ counts ﬂuctuate. The average amplitude of signal counts is expected, naturally, to be higher compared to that of dark counts. This phenomenon is illustrated in Fig. 2.31(a) which shows a histogram S(L) of the occurrence of pulses with height L; this is called the distribution of photomultiplier pulse heights. The centre of gravity of the dark-count distribution (dashed curve) is clearly left-shifted compared to the pulse distribution relevant to an illuminated photomultiplier (signal+dark counts, solid curve). An optimum pulse distribution for the photon-counting technique should have a pronounced—and as narrow as possible—peak with strongly suppressed occurrence of small pulses. The discrimination level is then adjusted close

Signal detection methods in luminescence spectroscopy

51

Fig. 2.32 Number of counts as a function of voltage applied to a photomultiplier in the photon-counting technique (important is the occurrence of a plateau on the curve A/B). Adapted after a Hamamatsu brochure [7].

to the local minimum of the distribution curve (see the arrow in Fig. 2.31(a)) in order to reject efﬁciently the dark pulses. Here, however, the experimenter is faced with a problem. Photomultiplier manufacturers usually do not provide curves of pulse height distributions in their catalogues. Therefore, it appears advisable for the user to perform his/her own measurement of these characteristics prior to application of a particular photomultiplier6 in photon-counting detection. A direct measurement of distributions as shown in Fig. 2.31(a) is possible with a multichannel analyser of pulse heights or using a discriminator that has two adjustable discrimination levels (such a narrow discrimination ‘window’ is scanned from low- to high-amplitude pulses and the occurrence of pulses belonging to this span of heights is recorded). Commonly, however, the discriminator has only one discrimination level. In this case all pulses with amplitude higher (in absolute value) than the adjusted discrimination level are recorded, resulting in the curve shown in Fig. 2.31(b). One can easily infer that this curve can be converted to the peak height distribution via numerical differentiation. Therefore, the curve (b) displayed in Fig. 2.31 is sometimes called an integral representation, while the curve (a) is called a differential representation of the pulse height distribution. 4. The choice of the photomultiplier anode–cathode high voltage and of the discrimination level. Suppose we have already acquired the differential curve of the height distribution and adjusted the discrimination level approximately to the local minimum (the arrow in Fig. 2.31(a)). We are now in a position to ﬁnd a proper operational high voltage. The procedure is as follows: the applied voltage is varied in small steps (allowing the operation conditions to be stabilized adequately), and the number of pulses is recorded at each step. This is done for both non-illuminated and illuminated photomultipliers. Curves similar to those plotted in Fig. 2.32 are obtained. The number of signal pulses (upper curve) increases with increasing voltage faster than the number of dark pulses (lower curve) because the latter are 6 There are photomultiplier types especially fabricated for use in photon-counting applications. But the manufacturer can also select an exeptionally suitable exemplar from other ranges of photomultipliers.

52

Experimental techniques already substantially restricted by the discriminator. The ratio of these two curves (dashed curve in the middle) increases rapidly as the high voltage raises but then saturates, achieving a plateau. (The occurrence of a broad plateau is another prerequisite imposed upon the photomultiplier.) The correct applied high voltage is then situated in the plateau region that starts at a voltage V0 at which the ratio of signal to dark pulses reaches saturation (Fig. 2.32) and that extends basically up to the maximum allowed voltage. The output signal is thus to a large extent independent of the anode–cathode voltage and its ﬂuctuations, featuring an obvious beneﬁt of the photoncounting technique. It is important to realize that proper choice of the operational high voltage may comprise some ambiguities. The distribution of pulse heights shown in Fig. 2.31 was obtained with a certain pre-selected photomultiplier high voltage. If, later, we found that this bias was, unfortunately, outside of the plateau region, another operational voltage must be chosen, which may inﬂuence the shape of the pulse height distribution. Then, in principle, we shall have to remeasure the curves shown in Fig. 2.31, ﬁnd a new discrimination level and determine a new plateau characteristic. Possibly, the operational voltage will then have to be shifted again, etc. and we risk ending up in a closed loop. The solution is a compromise based both on the experimenter’s experience and on the requirements of the particular experiment. Obviously, shifting the discrimination level down (to the left side from the local minimum of the height distribution) increases the overall efﬁciency of pulse counting, while shifting it to higher pulse amplitudes (roughly towards the middle between the local minimum and the distribution peak) rejects more noise pulses and improves the signal-to-noise ratio. We shall close our discussion of photon counting with a few ﬁnal notes. First of all, let us remind ourselves that not only a photomultiplier but also an avalanche photodiode can be applied in the photon-counting method (Section 2.2). In fact, we have also already mentioned the natural limits of application of the technique. The high count rate limit is set by the resolution of two closely following pulses, where both the temporal width of the pulse and the dead time of the detector and discriminator are signiﬁcant. A typical value of the maximum pulse rate is 1–3 × 106 s−1 , which corresponds to a photon ﬂux of about 107 photon/s (i.e. optical power ∼ 3 pW) hitting a photomultiplier with a photocathode quantum efﬁciency of ηph = 20%. The low count rate limit is determined by various noise characteristics and by the rate of dark counts. Using an up-to-date cooled photomultiplier one can easily detect signals of tens of photons per second, but if the entire spectrum is to be recorded in this case, then the overall measurement time already has a decisive role to play, as will be analysed in Section 2.5. A troublesome peculiarity of the photon-counting technique is its excessive receptiveness to external perturbations. A photon-counting apparatus can register, for example, spurious pulses generated by a stepping motor that drives the dispersion element located inside the monochromator or high-frequency perturbations from other laboratory equipment, originating possibly even in neighbouring rooms. The only remedy is perfect shielding of all instruments

Signal-to-noise ratio in a scanning monochromator

53

including usage of well screened cables, good earthing, and sometimes ﬁnding an optimum location of the apparatus within the laboratory. The spheres of applicability of the lock-in and photon-counting techniques overlap over a certain range of photon ﬂuxes. If both techniques are usable, then synchronous detection is usually preferred as it is simpler and less sensitive to external perturbations. For more information on the photon-counting technique, noise analysis, dead times, accuracy, etc. the reader is referred to, e.g., [6, 19].

2.5 Signal-to-noise ratio in a scanning monochromator In the preceding sections we examined the basic characteristics of spectral devices, introduced parameters describing the properties of optical detectors, and analysed the two basic techniques of signal detection in luminescence spectroscopy—synchronous detection and photon counting. Now, we are ready to deduce a relatively simple expression for the signal-to-noise (S/N ) ratio [20] of luminescence spectra. This is of basic importance for laboratory practice. Consider a scanning monochromator, provided at the exit slit with a detector of sensitivity k(λ), normalized detectivity D ∗ and sensitive area A . The detector is illuminated by a monochromatic radiant ﬂux φλ . The deﬁnition (2.7) of D ∗ can be modiﬁed using (2.6) to √ √ √ √ √ A f S A f ∗ = k (λ) . (2.41) D = A /NEP = φλ N N To be speciﬁc, let the output from the detector be treated by a lock-in ampliﬁer. Then the frequency bandwidth f of the detection path is driven by the integrator time constant τ as f ≈ 1/2πτ . This can be understood as a straightforward result of a Fourier transform, or—in a more illustrative way—we can imagine the signal as being recorded by a classical plotter (or traced in real time on an oscilloscope screen) when the time constant τ determines the speed of movement of the recorder pen. Suppose the spectrum contains very sharp features, for example an intense narrow line; then the fast upward movement of the pen is damped by the time constant τ . In the case of excessively long τ , the peak is not well reproduced, is smaller, broader and shifted along the direction of wavelength scanning. It may happen that less intense spectral peaks even disappear entirely from the record. This implies that, in order to detect a spectrum without distortion, the wavelength scanning speed must be adapted to the applied time constant τ . The mathematical formulation of this requirement is simple. Crucial for the scanning speed are the sharpest features in the spectrum. The narrowest peak, if it is to be recorded perfectly, must be scanned for a time T signiﬁcantly longer than τ (Fig. 2.33), which means τ = ε T (ε 1), f ≈ 1/2πτ.

(2.42)

Fig. 2.33 Scanning of emission spectrum in real time. The recording time T of the narrowest peak must be much longer than the time constant τ of the detection system.

54

Experimental techniques Now, the noise level N in eqn (2.41) can be expressed using eqn (2.42) as √ √ A f A k(λ) = ∗ . (2.43) N = k(λ) D∗ D 2πε T The magnitude of the signal S as registered by the detector for the output radiative ﬂux φλ (2.37) is given by S = k(λ) φλ = k(λ)

κ Bλ β D W 2 λ2 . 2 Rreal

(2.44)

Finally, the signal-to-noise ratio we are looking for follows from the last two equations as κ Bλ β D W 2 λ2 2 π ε T ∗ S (2.45) = D . 2 N A Rreal This relation hold true for the narrowest spectral line. Obviously, recording any other spectral feature, like a wider peak or band, will run for even longer time. For the detection time of the whole spectrum thus the relation T > T τ holds. Expression (2.45) for S/N contains several interesting pieces of information and is worth analysing in detail. First of all, the detector sensitivity k(λ) does not enter eqn (2.45). This surprising fact conﬁrms that the S/N ratio is determined predominantly by the detectivity D or D ∗ . Therefore, a responsible choice of a suitable detector should not be just a matter of a cursory glance at the catalogue’s data on sensitivity. Suppose now the entire experimental set-up is ready, which means the detector and monochromator parameters (detectivity D ∗ , transmittance κ, effective area of the dispersion element proportional to W 2 , and angular dispersion D) have been ﬁxed. Then, for the experimenter just four remaining parameters are left to be adjusted in order to maximize S/N : the spectral brightness of the entrance slit Bλ , the angular height of the illuminated slit β, the time constant τ (or acquisition time T ), and the resolving power Rreal . In Subsection 2.3.2 we already saw that homogeneous illumination of the whole slit height is, except in special cases, hardly possible in luminescence spectroscopy. Thus, only three adjustable parameters remain, i.e. Bλ , T , and Rreal . First we pay attention to the resolving power and detection time T ; they are closely related. An increase in resolving power Rreal (e.g. by setting narrower slits) is accompanied, according to eqn (2.45), by a decrease in the S/N ratio. If in this situation we want to keep the S/N constant, we can attempt to increase the time constant τ and simultaneously to set a longer acquisition time T , which means a slower spectrum scan. This method is, however, very limited. Imagine we have recorded a spectrum within T1 = 10 min and found that, in order to resolve better two neighbouring spectral lines, we have to increase the resolving power (i.e. to narrow down the slits), say, 3.3 times. According to eqn (2.45), the S/N ratio remains unchanged provided we prolong the acquisition time to T2 ≈ 100T1 = 1000 min ≈ 16 hours (!). This is not feasible. In other words, the inﬂuence of the detection time on the S/N ratio is strongly limited. √ Obviously, this is because of the weak relationship (S/N ) ∼ T and, on the

Signal-to-noise ratio in a scanning monochromator

2 . Let us note that a other hand, to the strong dependence (S/N ) ∼ 1/Rreal √ similar weak square root relation (S/N ) ∼ T holds true also for the photoncounting technique. We come to the conclusion that the crucial parameter available to the experimenter is the entrance slit brightness Bλ . This can be optimized by setting up an effective optical system to collect luminescence from as wide as possible solid angle (see Figs 2.1 or 2.2, and the relevant discussion). Futhermore, the optical system focusing the luminescence signal on the entrance slit must be well designed. The basic principle is illustrated in Fig. 2.34. Luminescence emission is to be focused by a lens L 1 with minimized spherical and chromatic aberration (an achromatic doublet is preferred) exactly onto the centre of the entrance slit. Moreover, this imaging system should be designed so that the light cone entering the spectroscope just covers the whole area of the collimating lens (or mirror) L 2 . Let the diameter and focal length of the lens L 1 be ρc and f c , respectively; then simple geometrical similarity (Fig. 2.34) implies 1 ρc W = , (2.46) = fc f #

in other words, the aperture ratios of lenses L 1 and L 2 must be equal to one another. This equation represents a recipe for choosing the ratio ρc / f c of the lens L 1 (condenser). In case relation (2.46) is not fulﬁlled, either part of the luminescence emission is lost for spectral analysis (if ρc / f c > 1/#), or the resolving power of the spectrometer is not fully exploited (if ρc / f c < 1/#) as the incoming light cone does not cover the whole area of the dispersion element. It is also desirable to ensure precise positioning of the properly chosen condenser L 1 with respect to the optical axis of the whole system by ﬁxing it to a suitable {x, y, z} translation stage equipped with micrometer adjustment screws. Nowadays, there are many advanced numerical methods (often being part of commercial software packages) that can be applied to ‘improve’ noisy spectra a posteriori, having ﬁnished the experiment. But it is always advisable to pay attention to optimizing the luminescence signal during the experiment, especially to maximize the entrance slit brightness and simulatenously to exploit properly the throughput of the spectral device in the described way. One way to adjust the whole optical path from the source of luminescence emission to the entrance slit is based on the principle of reversibility of light rays, a law known from geometrical optics. Here, the detector is removed

55 Fig. 2.34 Optical system for illuminating the spectrometer entrance slit. A collimated beam of luminescence emission comes from the left-hand side. The parameters of the focusing lens L 1 (condenser) are chosen so that the light cone inside the spectrometer just covers the whole area of the collimating element (here the lens L 2 , but most of today’s spectral devices utilize mirrors). At the same time this design ensures plane parallelism of the beam entering the dispersion element.

56

Fig. 2.35 Adjustment of the optical system for luminescence collection by reversing the direction of light propagating through a monochromator. A piece of ground glass is inserted into the exit slit.

Experimental techniques and the exit slit is illuminated from outside, preferentially with a HeNe laser (633 nm) or other gas or diode laser emitting visible light, as shown in Fig. 2.35. A small piece of ground glass or calking paper is inserted into the plane of the exit slit in order to scatter the low-divergence laser beam into many directions, simulating the passage of the luminescence emission beam through the monochromator. The laser light, after leaving the entrance slit (the monochromator has to be set to the laser wavelength, obviously), maintains its direction going through the collection optical system and is ﬁnally focused onto the sample, where a visible red spot appears. This is the place onto which the excitation light beam is to be directed. Such an arrangement ensures correct focusing of the luminescence emission onto the entrance slit along with the optimized path through the monochromator and the right illumination of the detector. Do not forget to remove the ground glass from the exit slit before remounting the detector (!). A ﬁnal signal maximization prior to recording the spectrum is done via ﬁne adjustment of the positions of the lenses using {x, y, z} translation stages. Achieving maximum brightness at the entrance slit represents the experimental priority also when using a spectrograph in conjunction with a multichannel detector, because Bλ naturally ﬁgures in eqn (2.40), standing for the detector irradiance. Other experimental factors, the spectrum acquisition time and the related S/N ratio, were already described in that part of Section 2.2 dealing with multichannel detectors. Finally, it is worth noting that, nowadays, optical waveguides (ﬁbres) are increasingly applied to guide light signals towards spectrometers. Among numerous beneﬁts, for example, is their capacity to bring the signal from distant and/or badly accessible places. In order to minimize signal losses, one has to choose an appropriate waveguide material with maximum transmittance over the spectral region of interest (common waveguides are made of various glasses, silica, polymers, and liquids) and then correctly couple light in and out of the waveguide. A glass waveguide can be formed by a single ﬁbre or a bundle of ﬁbres. The single-ﬁbre waveguide is mostly of cylindrical shape, the central part of which is called the core (refractive index n 1 ) and is surrounded by a cladding layer with lower refractive index n 2 < n 1 (the change in refractive index may be either step-like or gradual, hence the so-called step-index or graded-index ﬁbres). Coupled light is guided within the core thanks to total reﬂection on the interface between the core and cladding, provided the entrance angle is equal to αa or smaller (see Fig. 2.36(a)). The maximum entrance angle αa is given by sin αa =

1 2 (n − n 22 )1/2 , n0 1

(2.47)

where n 0 is the relative refractive index of the ambient medium (for air we can put n 0 = 1). The same value of maximum angle holds for light leaving the waveguide. Typical values for glass and silica ﬁbres are αa = 34◦ and 12◦ , respectively. The angle αa is called the acceptance or aperture angle and it determines the so-called acceptance (and output) cone of the ﬁbre. The sine of the aperture angle is the numerical aperture (NA), and sometimes also the term

Fourier luminescence spectroscopy

57

Fig. 2.36 (a) Schematic of light rays guided in an optical waveguide, (b) and (c) examples of two optical systems designed to couple correctly light from a ﬁbre to a spectrometer using lenses (a) or mirrors (b). Based on documents by Horiba Jobin Yvon, Ltd.

aperture ratio 1/# ≈ 2NA is used (in analogy with photographic cameras), see Subsection 2.3.2. The numerical apertures of a waveguide and that of a spectrometer only exceptionally happen to match one another. Therefore, a special optical system is required to adapt the output cone of a ﬁbre to the acceptance cone of a spectrometer described by an angle αs (Fig. 2.36(b),(c)). Such coupling adapters for various optical waveguides and spectrometers are usually designed and supplied by spectrometer manufacturers.

2.6 Fourier luminescence spectroscopy We have shown that increasing the resolving power of a scanning monochromator leads either to a decrease in the S/N ratio or to impractically long spectral acquisition times. One possible way to solve this problem— the multichannel detectors—was also mentioned; these devices are indeed increasingly used in modern luminescence spectroscopy. However, if a need for relatively very high resolution (λ ≤ 0.01 nm) arises, we shall be faced with a fundamental limitation: the ultimate resolution of the multichannel detectors is strictly limited by the ﬁnite size of their individual pixels. For example, a typical detector with pixels of 26 μm × 26 μm attached to a spectrometer with a dispersion of L −1 ≈ 3 nm/mm has the resolution limit λ ≈ 3 nm/mm × 26 × 10−3 mm ≈ 0.08 nm. Even if the need for such a very high spectral resolution is not typical for luminescence spectroscopy, it may sometimes appear, as we have already indicated several times. In this case one has no choice but to resort to Fourier luminescence spectroscopy.

58

Experimental techniques A Fourier spectrometer, widely applied in infrared absorption spectroscopy, is basically a scanning Michelson interferometer. The radiation to be analysed (luminescence in our case), upon entering the spectrometer, is split into two arms and, after being reunited again, the beams interfere due to the varying length of one of the arms. The resulting temporal interference signal undergoes Fourier analysis that transforms it into a frequency (or wavelength) spectrum. There are two fundamental differences compared to standard monochromators: (i) all spectral components are analysed simultaneously (the so-called Fellgett (or multiplex) advantage which, however, takes place also in spectrographs equipped with multichannel detectors—see eqn (2.12)), and (ii) the interferometer has no slits and, consequently, its throughput/aperture is much higher than that of a traditional monochromator that shows the same resolving power (the so-called Jacquinot advantage). It is possible to derive the following relation comparing the signal-to-noise ratio of a Fourier spectrometer (S/N )F to that of a scanning monochromator (S/N )scan utilizing the same detector [20] (S/N )F 2π f √ ≈ M, h (S/N )scan

(2.48)

where M is the number of narrow spectral components (lines) that are analysed by a Fourier spectrometer during the same time interval that a scanning monochromator needs to analyse a single component. Other variables have their usual meaning: f is the focal length of the monochromator collimator and h is the illuminated slit height (the ﬁrst factor on the right side of (2.48) thus reﬂects the Jacquinot advantage while the second one results from the Fellgett advantage). The right-hand side of eqn (2.48) has a typical value of 103 . If we consider the highest real resolution of a typical scanning monochromator to be λ ≈ 0.1 nm, then, keeping the same S/N ratio, a Fourier spectrometer can in principle attain a resolution of about three orders of magnitude better, i.e. λ ≈ 10−4 nm. However, since, as a rule, semiconductor photodiodes rather than photomultipliers are used in a Fourier luminescence spectrometer, it appears more realistic to speculate that the right-hand side of eqn (2.48) is one order of magnitude lower. Then, the practically achievable resolution of a Fourier spectrometer is about λ ≈ 10−3 nm; expressed in wavenumbers ν ∗ , which are frequently used here, this corresponds to ν ∗ ≈ 10−2 cm−1 . We shall mention a beneﬁt of this unique property in Subsection 7.2.2. Nevertheless, in general Fourier spectrometers are still rather expensive and their exploitation is as yet worthwhile only in very special applications (e.g. highresolution near-infrared spectroscopy of weak luminescence signals).

2.7 Spectral corrections Suppose we have optimized our optical collection system and our spectral apparatus consists of a high-throughput monochromator and a high-quality cooled detector. Even then, however, the experimental emission spectra of the sample under study, in spite of being minimally noisy, do not correspond—

Spectral corrections as far as their shape is concerned—to the actual luminescence spectrum. The reason for this is due to the fact that the photodetector sensitivity k(λ) as well as the characteristics of other optical elements—the reﬂectivity or transmittance of the dispersion element, mirrors and lenses—are spectrally dependent. Thus, if we denote the luminescence intensity as function of wavelength (which means the actual emission spectrum) as I (λ), then the measured spectrum i(λ) is equal to i(λ) = Q(λ) I (λ),

(2.49)

where Q(λ) is usually called the spectral response of the whole detection system.7 Thus Q(λ) includes both the transmittance of the spectral device κ(λ) and the detector sensitivity k(λ). Sometimes Q(λ) is simply referred to as a correction function (of the detection channel). The function Q(λ) must be determined experimentally, separately for each particular conﬁguration of the detection system (various combinations of a dispersion element and a detector unit). A faithful spectral shape I (λ) is then obtained, according to eqn (2.49), by dividing the measured spectrum i(λ) by the correction function Q(λ). The correction function Q(λ) is determined with the aid of a light source with well-known spectral emittance. A commonly applied calibrated source for the visible and near-infrared regions is a tungsten strip (ﬁlament) lamp, whose emission spectrum bears a close resemblance to blackbody radiation. Such calibrated lamps are supplied, together with a detailed description of their spectral energy density, either in graphical or tabular form (or simply colour temperature), valid under a speciﬁc heating current. Light is emitted by a narrow tungsten strip in a vacuum bulb; this design ensures the distribution of temperature over the entire surface of the light-emitting body to be as homogeneous as possible. (A traditional tungsten spiral in a bulb or other incandescent lamp types do not fully satisfy this condition but even special sources of this type—ﬁlament lamps—can be calibrated and applied for correction purposes.) If an experimentally acquired spectrum of the calibrated source is w(λ) and its actual spectral emittance is W (λ, T ), the required correction function is calculated according to eqn (2.49) simply as Q(λ) =

w(λ) . W (λ, T )

(2.50)

Then, to obtain undistorted results, any measured luminescence spectrum has to be divided by this correction curve. The procedure for determining Q(λ) as described above seems to be quite simple but the opposite is true. First of all, it is not easy to keep the prescribed lamp current stabilized over the whole measurement time, while even small 7 A somewhat more exact formulation of the above debate is that the luminescence intensity means (usually) the photon ﬂux (power) per unit interval of wavelengths, [I (λ)] = photon/s/unit interval of λ. From the point of view of radiometry this corresponds to radiant ﬂux φL (λ) per unit interval of λ, [φL (λ)] = power/unit interval of λ. This ﬂux impinges on the entrance slit creating its irradiance E λ = φL (λ)/S. Then the slit becomes a planar light source for the spectrometer, featuring brightness Bλ = E λ . According to eqn (2.37), the radiant ﬂux at the exit slit is φλ ∼ κ(λ)Bλ and the detector signal reads i(λ) ∼ k(λ)φλ , which means i(λ) ∼ k(λ)κ(λ) Bλ ∼ k(λ)κ(λ) I (λ).

59

60

Experimental techniques deviations from the speciﬁc temperature (usually in the range of 2800–3000 K) cause signiﬁcant changes of the W (λ, T ) spectrum. Too high lamp intensity may appear as another problem, because of possible detector oversaturation. Next, ageing of such lamps may be quite fast and can cause harmful alteration of the original spectrum W (λ, T ). Often, to determine Q(λ) correctly, a diffusion reﬂector (made of, e.g., MgO or BaSO4 ) is recommended, but variations in its spectral reﬂectivity can affect the result. In addition, problems could also arise from polarization effects—light becomes partially polarized or depolarized by reﬂective surfaces, by diffraction gratings, etc. In particular the last mentioned effects are often ignored even if their impact could be signiﬁcant. The correction curve thus has to be determined with due care. Some difﬁculties in determining Q(λ) can be eliminated by using an integration sphere ﬁxed at the entrance of the spectrometer. This ensures correct ﬁlling of the collimator by light and also depolarizes possible partial polarization of the incoming lamp radiation. Nowadays, performing the correction of luminescence spectra for spectral response of the detection path should be commonplace in every laboratory. Any spectrum submitted for publication in international refereed journals may be automatically supposed to have been corrected. Indeed, the difference between a corrected and an uncorrected spectrum can be considerable, as illustrated in Fig. 2.37 [21]. Naturally, the correction becomes imperative when the spectrum is going to be ﬁtted with a theoretical curve. Actually one of the aims of this book is to teach the reader how to identify the microscopic origin of the luminescence centre, based on the corresponding spectral shape and its changes due to controlled variations of experimental parameters: temperature, excitation intensity, etc. Nevertheless, one can admit that sometimes the correction in question is not indispensable—for example, if only a qualitative demonstration of spectral changes (e.g. one spectral band grows at the expense of another during an increase in temperature) is sufﬁcient for a given purpose. Also in the case of very narrow emission lines the spectra can often be left uncorrected and even ﬁtting its shape with a theoretical model is possible. The reason is that the correction curve is usually only slowly varying with wavelength and its change

Fig. 2.37 As measured (full squares) and corrected (empty circles) electroluminescence spectra of amorphous hydrogenated silicon. The pronounced deformation of the measured spectrum at long wavelengths is mainly due to the rapid decrease in photomultiplier sensitivity in this spectral region (S1 photocathode), while the dip at ∼ 790 nm is due to the so-called Wood’s grating anomaly. The spectra are normalized. Adapted from Fojtik [21].

Spectral corrections in a narrow wavelength range (a few nanometres) can be neglected. But always be vigilant! We should stress that this correction does not serve for establishing the absolute number of emitted photons or determining the absolute luminescence quantum yield η—this is a domain of very special and quite difﬁcult techniques, which are described for example in [22] and in Appendix K. Any spectrum corrected using (2.50) ‘only’ faithfully represents (in relative units) the number of photons emitted by the luminescent sample per unit interval of wavelengths or photon energies. It remains to be noted that the described correction procedure is basically the same irrespective of whether a monochromator or spectrograph is used. In the context of corrections of optical emission spectra we must mention another experimental problem, which used to be unjustly neglected. It concerns two alternative modes of plotting the emission spectra—against either wavelengths λ or photon energy hν. Both representations are possible and widely used (sometimes even both modes are applied to the same graph, one at the bottom and the other at the upper axis or vice versa, see e.g. Fig. 1.2), conversion between wavelengths and photon energies being performed simply via the trivial relation c (2.51) hν =h . λ However, such an approach is not always fully justiﬁed. One has to take into account what type of dispersion element and wavelength scan was used during the experiment. Let us consider ﬁrstly a grating monochromator with a linear scan in wavelengths λ (the sine-drive, see Section 2.3). The spectral measurement is carried out using constant slit widths λ, the result being either a raw spectrum i(λ) or, after having performed the correction, the actual spectrum I (λ). However, the elemental step (interval) in photon energy is not kept constant during the measurement, as is clearly seen by differentiating (2.51), |d(hν)| =

hc |dλ|. λ2

(2.52)

Obviously, when increasing the wavelength (keeping dλ = const), the energy interval |d(hν)| drops, because it scales like λ−2 . Therefore, if one wishes to plot the spectrum against the photon energy scale like I (hν), the decrease in the magnitude of the energy interval |d(hν)| should be corrected8 by multiplying each value of I (λ) by λ2 : I (hν) = λ2 I (λ).

(2.53)

This multiplication obviously boosts the long-wavelength wing of the spectrum, causing a red-shift of spectral peaks; see Fig. 2.38(a) [23]. Thus, in principle it is incorrect to convert simply λ into hν while keeping the spectral curve unchanged. However, at the same time one can see that the correction 8 Let us recall that I (λ) means the photon ﬂux per unit interval of wavelength, and by analogy I (hν) is the photon ﬂux per unit (therefore constant) interval of photon energies.

61

62

Experimental techniques

Fig. 2.38 Correction of emission spectra when transforming the wavelength-to-photon energy scale. (a) Photoluminescence spectrum of silicon nanocrystals embedded in an SiO2 matrix. The spectrum was recorded using a grating monochromator with a linear scan of λ (solid line, the spectrum is related to the lower axis). Correction pertinent to transformation into photon energies hν was performed by multiplying by λ2 (open circles, the spectrum is related to the upper axis). Both curves are normalized. Adapted from Dian et al. [23]. (b) Emission spectra of TlBr crystals due to radiative decay of the electron–hole plasma. The solid line is the experimental spectrum measured by making use of a linear scan in λ, and the crosses show the recalculated spectrum connected with axis transformation to photon energies (circles are related to a theoretical ﬁt, which is irrelevant to the present discussion). Both the A and B emission lines being relatively narrow, the correction as regards their spectral shape and position is of minor importance—just the relative intensities of these bands are slightly changed (the intensity of the B line increases relative to the A line). Adapted from Pelant et al. [24].

effect is not large and becomes signiﬁcant for sufﬁciently broad spectra only (full width at half maximum about 100 nm or more). This is illustrated by Fig. 2.38(b) [24]: for emission lines only a few tens of nanometres in width or narrower, the distinction in shape between the recalculated curve and the spectrum as recorded becomes negligible, usually buried in noise. In the case of a grating monochromator with a linear sweep in wavenumbers 1/λ or energy hν (a cosec-drive, which is a much less frequent case) we obtain an experimental spectrum against photon energy like I (hν). For transforming it into wavelengths we again use relation (2.53), but in the opposite direction: the spectrum I (hν) will be divided by λ2 . Monochromators equipped with a prism should in principle require two corrections. Nevertheless, the following discussion is intended to show that the situation there is, in fact, not so serious. First of all, the reciprocal linear dispersion L −1 is a nonlinear function of λ which, according to (2.19), causes an increase in the spectral slit width λ (when keeping the mechanical slit width constant) with increasing λ.

Inﬂuence of slit opening Consequently, the shape of the measured spectrum I (λ) does not exactly correspond to reality. In principle, for each prism device, knowing its particular L −1 (λ) dependence, we should have to determine a speciﬁc correction function9 ξ(λ) = λ0 /λ < 1 to multiply the experimental spectrum I (λ); since ξ(λ) is a decreasing function, the long-wavelength wing of I (λ) would have been slightly suppressed. However, a second correction takes place during the transition from I (λ) to I (hν), namely, multiplication by λ2 according to (2.53), which relatively enhances the long-wavelength side. All in all, both corrections go in opposite directions and may roughly compensate each other. This means that we can practically omit both of them within reasonable accuracy. To conclude, this somewhat arbitrary way of interchanging between the λ and hν axes, found frequently in the literature, is not usually at the expense of the correctness of presentation, except, perhaps, for very broad spectra. For completeness, let us also mention spectrographs, where wavelength scanning is replaced by multichannel detection. Most of these devices employ a diffraction grating whose dispersion is linear in wavelength, i.e. λ = const. This situation is analogous to that of a sine-drive monochromator—transformation from I (λ) to I (hν) is done using eqn (2.53), if necessary.

2.8 Inﬂuence of slit opening on the shape of emission spectra The last important correction of emission spectra we are going to treat here concerns the effect of the ﬁnite width of the instrument slits on the spectral shape. Intuitively, we feel that setting too wide slits can bring about loss of spectral details and blurring or broadening of the spectra. In this section, the inﬂuence of the slit will be described quantitatively. Firstly, the case of a monochromator (a dispersion device with two slits) and then that of a spectrograph (having one entrance slit and a multichannel detector at the output) will be analysed. Monochromator In Appendix A we give an illustrative explanation of the convolution of two functions in terms of a shift of the ﬁrst function over the second one along the independent variable axis, integrating simultaneously the product of the two functions (Fig. A.1). The functioning of a scanning monochromator equipped with a rotating dispersion element ﬁts the above scheme well: the emission spectrum, created with the cooperation of the entrance slit with the dispersion element (and being affected by the spectral variations in reﬂectivity (transmittance) of all elements contained within the device) is projected onto the exit slit plane. Obviously, this is not the true spectrum I (hν) = I (E) but it can be described as κ(E)I (E), where κ(E) comprises all the above mentioned spectral factors (see also (2.32)). If, moreover, we include now also 9 Here λ means the spectral slit width at the short-wavelength boundary λ of the spectral 0 0 range covered by the device, and λ = L −1 (λ) is taken for λ > λ0 .

63

64

Fig. 2.39 The emission spectrum in a scanning monochromator is scanned across the exit slit (its spectral width being E). The joint activity of the entrance and exit slits is described by a function s(E 0 –E). This means that the function Q(E)I (E) is convoluted with s(E 0 –E); FWHM means full width at half maximum of the spectral band.

Experimental techniques the detector spectral sensitivity k(E), then the spectrum projected onto the exit slit corresponds to κ(E)k(E)I (E) ≡ Q(E)I (E). This spectrum is now ‘swept’ or scanned across the exit slit, consistently with rotation of the grating or prism (Fig. 2.39). The exit slit of spectral width E transmits (and so ‘integrates’) slices of the spectrum towards the detector. If we denote, according to eqn (A.1) and Fig. A.1, the product Q(E)I (E) as f 2 , and the function describing the effect of slits as f 1 = s(E), we see that the measured spectrum is given by the convolution of the functions QI and s: +∞

+∞

−∞

−∞

i(E 0 ) = ∫ s(E)Q(E 0 − E)I (E 0 − E)dE = ∫ Q(E)I (E)s(E 0 − E)dE, where we have applied commutativity of the operation of convolution according to eqn (A.3). Thus the measured spectrum i(E 0 ) is, taking into account the effect of the ﬁnite slit opening, given by the convolution +∞

i(E 0 ) = ∫ Q(E)I (E)s(E 0 − E)dE. −∞

(2.54)

The function s(E 0 –E) is usually called the apparatus (instrumental) function of the spectral device. It must comply with the normalization condition +∞

∫ s(E 0 − E)dE = 1.

−∞

(2.55)

We are now in a position to decide under what conditions the convolution (2.54) is to be taken unavoidably into consideration when treating the experimental data; we shall discuss three typical situations. (a) The spectral slit width E is much narrower than the full width at half maximum (FWHM) of the measured spectrum, E FWHM. Then the function s(E 0 –E) can be approximated by the delta function δ(E 0 –E) and (2.54) is reduced straightaway to i(E 0 ) = Q(E 0 )I (E 0 ).

(2.56)

Or, for a broad spectrum and narrow slits the effect of apparatus function need not be taken into account. The true emission spectrum is obtained simply by dividing the experimental result by the correction function Q(E). (b) The spectral slit width E remains smaller than the FWHM of the spectrum but the apparatus function cannot be considered inﬁnitely narrow. Then the measured spectrum and the actual spectrum are not identical, and in order to extract the actual spectrum I (E) from the convolution integral (2.54), one needs to know the function s(E 0 –E). Let us restrict our discussion to the standard case of equal entrance and exit slit widths E, large enough to neglect diffraction effects. Then the geometrical image of the entrance slit in the output focal plane is represented by a homogeneously illuminated area (rectangle). Then an ideal monochromator (i.e. a device free of imperfections and aberrations of optical imaging) features the apparatus function of a triangle shape as described by

Inﬂuence of slit opening s(E 0 − E) =

1 E

0

1−

|E 0 −E| E

for|E 0 − E| ≤ E for|E 0 − E| > E,

65

(2.57)

which is illustrated in Fig. 2.40(b) and whose FWHM is equal to E. Figure 2.40(a) helps us to understand why this is so. When the dispersion element is turning, the monochromatic image of the entrance slit is moving across the exit slit, and the detector records a signal proportional to the overlap area (just the convolution of the entrance slit image with the exit slit). This signal increases linearly from zero to its maximum value (both areas are fully overlapping) and then drops back. As a result, the triangular shape of the function s(E 0 –E) appears. In a real monochromator, however, various imperfections, inhomogeneities of all optical elements, parasitic diffraction effects, imperfect absorption of the internal blackened surfaces of the monochromator, etc. produce a weak light background that can enter the exit slit at wavelengths different from the nominally set value. This effect leads to making the triangle vertices round and the real apparatus function can be approximated by a Gaussian curve, as shown in panel (c) of Fig. 2.40. Its analytical expression takes the form 4 ln2 (E 0 − E)2 , (2.58) s(E 0 − E) = N (E ) exp − (E )2 √ √ where E is the FWHM of the curve and N (E) = 2 ln 2/( πE ) is a normalizing factor. The relatively simple form of the apparatus function (2.58) is advantageous for performing a deconvolution of eqn (2.54) in order to extract the real spectrum I (E) from the experimental one i(E). (We should not forget, however, that also the correction function Q(E) must be known.) There are a large number of deconvolution methods [25] and current progress in computational techniques makes them easily available. Nevertheless, it seems that an inverse approach, the so-called iterative convolution, remains among the most widely applied methods. The principle is based on setting down a suitable model function for the actual spectrum I (E) with some initial parameters and calculating the convolution (2.54). The parameters of I (E) are then iterated until the best correspondence between the calculated spectrum i(E) and the experimental one is achieved. Evidently, the initial selection of an appropriate microscopic model of luminescence centre (and related spectral shape) is crucial and depends strongly on both the experience and intuition of the experimenter. Application of the apparatus function in the form of (2.58) includes one difﬁculty which is not evident at ﬁrst glance, namely, the unknown value of E . Unlike the triangular function (2.57), the halfwidth of the Gaussian peak E (2.58) is not equal to the spectral width of the entrance or exit slit E. This is because of the normalization (2.55) and is illustrated in Fig. 2.40(c): the postulate of a constant area below the curve yields E > E. Therefore, knowledge of the mechanical (and, consequently, also spectral) widths of slits does not enable us to determine the particular shape of the Gaussian instrumental function (2.58). How, then, can the apparatus function shape be obtained?

Fig. 2.40 Illustration of the apparatus function of a monochromator. (a) The monochromatic image of the entrance slit is moving to the right across the exit slit in the focal plane of an ideal device. The detector ‘sees’ an intensity proportional to the overlap area (dark grey rectangle) whose variation as a function of E is the apparatus function s(E 0 –E) plotted in panel (b). This function has a triangular shape with unit area, in order to fulﬁl the condition (2.55). Panel (c) shows the shape of this function in a real monochromator, as inﬂuenced by imperfections in the instrument and optical inhomogeneities. N (E) stands for a normalizing factor.

66

Experimental techniques The answer to this question is related to our last situation to be discussed: (c) The spectral slit width E is much wider than the width of the measured spectrum, E FWHM. Then we put I (E) ≈ δ(E − E 0 ), Q(E) ≈ const, and eqn (2.49) is reduced to +∞

i(E 0 ) ≈ ∫ δ(E − E 0 ) s(E 0 − E) dE ≈ s(E 0 − E 0 ). −∞

(2.59)

Thus, paradoxically, the result of this experiment is the apparatus function rather than the spectrum (spectral peak) itself. Such a situation can be easily realized for example by measuring narrow emission lines from a low-pressure spectral lamp. If such a measurement is performed with the same slit widths as applied during the luminescence experiment, we can thereby use the obtained shape of the Gaussian apparatus function (2.58) for deconvolution (or iterative convolution) to ﬁnd the actual spectral shape I (E). Let us add a ﬁnal technical note: All the functions in the integral (2.54) are non-zero within relatively narrow energy intervals only; then the limits of numerical integration may be strongly restricted. In fact they are given by the narrowest function. Therefore, in the case of (b), applying the Gaussian apparatus function (2.58), reasonable integration limits are E 0 − 5E , E 0 + 5E . Spectrograph Here, assessment of the inﬂuence of the slit opening on the spectral shape is somewhat easier for two reasons. Firstly, there is only a single (entrance) slit. Secondly, the option of acquiring any spectrum for a very long time enables us to set the slit width narrow enough so as not to distort the spectral shape. Nevertheless, we are going to analyse several potential situations. First of all, we should ask about the shape of the apparatus function s(E). The answer is obvious: in any spectrograph, a uniformly illuminated monochromatic image of its entrance slit is created in the exit focal plane. Therefore, the relevant apparatus function is of a rectangular shape described by 1 for |E 0 − E| ≤ E E 2 (2.60) s(E 0 − E) = E 0 for |E 0 − E| > 2 , Fig. 2.41 (a) Apparatus function of a spectrograph. (b) Detection of a broad luminescence spectrum by a multichannel detector and a spectrograph with a wide entrance slit (E means the spectral width of the entrance slit image).

where E is again the spectral slit width (Fig. 2.41(a)). Then the convolution (2.54) takes on the form i(E 0 ) ≈

E 0 +E/2

∫

E 0 −E/2

Q(E)I (E)dE ≈ Q(E 0 )

E 0 +E/2

∫

E 0 −E/2

I (E)dE,

(2.61)

if we exploit the fact that the correction function Q(E) is only slowly varying across the slit width. Application of relation (2.61) to deconvoluting a measured spectrum is then relatively simple. However, a closer inspection of the preceding procedure can raise an objection: we have introduced the convolution (Appendix A) as a relative shift of two functions, which is not completely true here—the grating is not rotating, and the spectrum is not moving. Is then the proposed application of eqn (2.61)

Time-resolved luminescence measurements correct? The response is yes. Although the ‘monochromatic’ images of the entrance slit hit the detector simultaneously, not in sequence like in a monochromator, the ﬁnal effect is the same (see Fig. 2.41(b)). The mechanism of the generation of the spectral image is, however, different, as we shall indicate. Figure 2.41(b) shows the situation when the experimenter has chosen the entrance slit width of a spectrograph10 several times wider than the size of a single pixel. This is a standard situation; in Section 2.3 we have shown that setting the slit width narrower than about 10 μm serves no useful purpose. Therefore, a slit width of = 100–200 μm is a reasonable choice (also in relation to an acceptable acquisition time of the spectrum), being really much larger than the typical CCD pixel size 25 μm. Let us select a ﬁxed photon energy E 0 . If the slit image width exceeds that of a single pixel, the signal level on the pixel at E 0 = hν 0 may ‘get saturated’, but this does not prevent the signal at E 0 from attaining the correct level, because ‘monochromatic’ images of neighbouring spectral elements join the signal. Naturally, this is accompanied by spectral broadening; everything is comprised in eqn (2.61). We shall close Sections 2.7 and 2.8 with a brief evaluation of the effects and corrections just discussed in view of their practical importance. The reader, possibly confused and upset, might have come to the conclusion that any experimental luminescence spectrum is only a relatively useless raw product, which must undergo many mathematical operations prior to being presented and interpreted. This is not the case, though. Among the above mentioned corrections only one is really essential and almost always indispensable, namely, to divide the experimental spectrum by the spectral correction function Q(λ) given in eqn (2.50), in order to correct the effect of spectral sensitivity of the whole detection system. The ‘presentation problem’ of the spectral data, i.e. care about whether to present spectra against wavelength λ or photon energy E = hν, takes place only exceptionally, in the case of very broad spectra (and if one wants to be very careful). Similarly, the correction through making use of the apparatus function s(E 0 –E) in order to remove the effect of the ﬁnite slit width is worth doing only in the case of the measurement of very narrow emission lines, like for instance those typical of radiative recombination of free excitons and biexcitons (Chapters 7 and 8). To a certain extent the corrections Q(λ) and s(E 0 –E) may even be considered disjunctive, because the spectral correction function Q(λ) is important for wide spectra, when the slit-width effect is negligible, while the function s(E 0 –E) is important for narrow lines when, to a good approximation, Q(λ0 ) ≈ const.

2.9 Time-resolved luminescence measurements Knowledge of the temporal behaviour of the luminescence signal, especially the shape of the luminescence decay curve after the excitation is switched off, carries valuable information contributing to the identiﬁcation of the recombination process and the microscopic nature of the relevant luminescence centre (along with an analysis of the excitation and emission spectral shapes 10 We again and again assume equal widths of the entrance slit and of its image.

67

68

Experimental techniques and of the dependence of the pump intensity). However, the techniques of time-resolved luminescence measurements, in particular under pumping with ultrashort laser pulses, represent a largely specialized research ﬁeld that cannot be fully treated within the limited space of this section. Therefore, we shall describe just the basic principles of the most common experimental methods and instruments. A comprehensive treatment of this subject can be found for example in [26] and [27].

2.9.1 Direct imaging of the luminescence response The simplest set-up to study luminescence decay consists of a single-channel detector, usually a photomultiplier, of which the output is connected to the vertical deﬂection plates of an oscilloscope and swept in time by its horizontal time base. The result is either observed on a screen or transferred to a computer. Obviously, in order to record, in this way, the decay of the luminescence radiation in time, either a cw excitation beam must be chopped (then curves similar to those plotted in Fig. 2.27 are obtained) or a pulsed excitation source supplying sufﬁciently short pulses (a lamp or laser) must be used. Since the character of luminescence decay may be strongly dependent on the emission wavelength, the decay curves i λ (t) of a quasi-monochromatic luminescence signal are usually measured after inserting a monochromator or at least narrowband interference ﬁlters in front of the detector. The next step consists in analysing the measured curves i λ (t). In the simplest case, one deals with a single-exponential function i λ (t) = i λ (0) exp(–t/τ ) where τ is referred to as the luminescence decay time or lifetime. However, many other shapes of decay, e.g. double-exponential, hyperbolic, etc. may occur in luminescence spectroscopy. Their detailed study will be presented in Chapter 3. Generally, the mean decay time t¯ can be deﬁned from the point of view of statistics as the mean value of a continuous stochastic varible by ∞ t¯ =

t iλ (t) dt

0 ∞

, i λ (t)dt

0

where iλ (t) plays the role of the occurrence probability density of a time interval t in which an elementary emitter is found in an excited state. In the case of the single-exponential decay i λ (t) = i λ (0) exp(–t/τ ), simple evaluation of the integrals leads to t¯ = τ . For practical purposes and in analogy with the single-exponential decay, as the ‘decay time’ in the case of more complex decay curves i λ (t), the time at which the initial intensity i λ (0) decreases to the value i λ (0)/e ≈ i λ (0)/2.72, is often (somewhat arbitrarily) taken. Although the method of direct decay imaging looks very simple, its practical implementation challenges the quality of the instrumentation and the experimenter’s knowledge of the limits of applicability of the method. First of all, the whole experimental set-up (a pulsed excitation source, a photomultiplier

Time-resolved luminescence measurements

or photodiode, and an oscilloscope) should be fast enough, highly sensitive and perfectly linearly responding to the optical signal, which requirements are difﬁcult to be satisﬁed simultaneously. (For example, a highly sensitive photomultiplier must contain many dynodes, which in turn makes its time resolution worse due to statistical ﬂuctuations of secondary emitted electrons and the long trajectory of the electron packet.) One can easily imagine a number of potential limitations of the method: (i) the insufﬁcient response speed of the photomultiplier; if (ii) a fast p-i-n photodiode is applied, it is inherently less sensitive and a preampliﬁer must be used in connection with the oscilloscope, whose limited bandwidth may pose a problem; (iii) similarly, the frequency bandwidth of the oscilloscope itself may be a limiting factor, etc. The direct measurement of the luminescence response may be easily applied (without any complementary mathematical treatment) to study relatively slow decays only (under a pulsed excitation, for roughly τ ≥ 0.1–1μs). An example is shown in Fig. 2.42 [28]. If photoluminescence is excited by a chopped beam, this limit is pushed to even longer times (τ ≥ 50 μs), considering that the typical maximum frequency of mechanical chopping is of the order of 1 kHz and the excitation pulses are of trapezoidal rather than of perfectly rectangular shape (the slope of the pulse edges is given by the speed of chopper rotation as well as by the diameter of the chopped beam). Under the complementary (a posteriori) mathematical treatment, deconvolution of the measured decay curve is to be understood. In analogy to the inﬂuence of the monochromator slit opening on the shape of the measured emission spectra (Section 2.8), we can deduce that the experimentally determined luminescence time response Rλ (t) is given by a convolution of the actual time response i λ (t) (i.e. the luminescence response to an inﬁnitely short excitation pulse) with the temporal proﬁle of the excitation pulse L(t) measured by the same detection system as that used to obtain Rλ (t): t

Rλ (t) = ∫ L(t − t )i λ (t )dt .

(2.62)

0

Here the integration goes from zero to t. This follows from analogy with the convolution example given in Appendix A, where the actual decay shape i λ (t),

69 Fig. 2.42 An example of direct imaging of the luminescence response by a digital oscilloscope (the signal comes from red electroluminescence (EL) and photoluminescence (PL) of silicon nanocrystals). The upper trace (a) shows a 50μs-long electric injection pulse, which excites electroluminescence, and curve (b) is part of the onset of EL and the subsequent decay. Curve (c) is the photoluminescence response of the same sample to excitation with 3 ns laser pulses (the third harmonics from a Nd:YAG laser). For both EL and PL, the excitation switch-off is fast enough which enables direct determination of decay times without any mathematical treatment (deconvolution). The decay curves (b), (c) are ﬁtted by single-exponential functions with decay times of τEL ≈ 8μs and τPL ≈ 2.5μs. After Luterov´a et al. [28].

70

Experimental techniques which has non-zero values only within an interval 0,∞), substitutes now for the function deﬁned by eqn (A.4). Convolution with the excitation pulse is deﬁned by eqn (A.5), from which eqn (2.62) follows via simple application of the commutativity of convolution (A.3). Often the duration of the excitation pulse L(t) happens to be comparable to the decay time of the luminescence response i λ (t). In this case the actual luminescence response must be determined via deconvolution of relation (2.62).11 This can also be simply formulated as follows: Due to the ﬁnite temporal width of the excitation pulse L(t), the exact (sharp) initial point of decay t = 0 cannot be found and, consequently, the time at which the intensity drops to i λ (0)/e cannot be determined. Only in case the pulse width L(t) is much shorter than the decay time, can we approximate L(t–t ) → δ(t–t ) and we obtain Rλ (t) = i λ (t); this means that the experiment gives the actual shape of the decay curve, in complete analogy with the situation when the spectral slit width is negligible compared to the width of spectral lines and measured emission spectra do not need to be deconvoluted to recover their actual shape. It is worth stressing that the function L(t–t ) appearing in (2.62) does not represent the actual shape of the excitation pulse but its ‘projection’ as seen by the whole detection system. Thus, it is not necessary to apply an extremely fast detection set-up that would be able to detect a distortionfree pulse shape, which might pose problems, especially in experiments with nanosecond and picosecond pulses. On the other hand, the detection system must be fast enough to distinguish reliably the shape of the excitation pulse from the shape of the relevant luminescence response, anyway. The pulse shape L(t) can be most easily measured by detecting reﬂected or scattered excitation light. Note that the above discussion concerns photoluminescence experiments. In the case of electroluminescence the response is determined not only by optical transitions and recombination phenomena but also by electric effects related to charge transport or capacitance of the device under study. Then, the observed electroluminescence kinetics is a combination of electric and optical effects and its analysis may be considerably more difﬁcult.

2.9.2 Phase-shift method The principle of this method consists in excitation of the sample with light, the intensity of which is sinusoidally modulated in time with an angular frequency ω. The luminescence response is obviously expected to be also modulated with the same frequency, but the ﬁnite value of the excited state lifetime τ induces two effects: Firstly, the luminescence response is phase shifted by an angle ϕ with respect to the excitation function and, secondly, its modulation depth is decreased. 11 The relevant methods were mentioned in Section 2.8 when discussing relation (2.58). For the case of luminescence decay curves, a critical review is given by O’Connor, D. V., Ware, W. R., and Andre, J. C. (1979). J. Phys. Chem., 83, 1333.

Time-resolved luminescence measurements

71

Fig. 2.43 Modulation of excitation light and luminescence response in the phase-shift method. Important parameters: modulation frequency ω = 2π × 30 MHz, phase angle ϕ = 59.5◦ , demodulation coefﬁcient m = 0.5 and extracted (single-exponential) decay time τ = 9 ns. Adapted from Lakowicz [27].

The overall picture is displayed in Fig. 2.43. It can be shown that [27] tan ϕ = ωτ, −1/2

= cos ϕ, m = 1 + ω2 τ 2

(2.63a) (2.63b)

where m = (B : A)/(b : a) is the ratio of modulation depths of the luminescence to that of the excitation light (Fig. 2.43). As measured quantities thus ϕ and, possibly, m are obtained; on the basis of these the decay time τ is calculated using (2.63a). It should be stressed that the simple relations (2.63) are strictly valid for pure single-exponential decays only. If this is not the case, eqns (2.63a) and (2.63b) provide values of τ differing slightly from one another. They offer an order-of-magnitude estimate of the decay kinetics but their physical meaning is not evident. To apply this method successfully, the frequency ω must be comparable to 1/τ . In the case of ω 1/τ , the fast luminescence response does follow perfectly the modulations of the excitation light, i.e. ϕ → 0, m → 1, and thus analysis of the experimental curves yields no information about the decay time; if, on the other hand, ω 1/τ , luminescence is not able to follow fast modulation variations, m → 0, ϕ cannot be reliably determined and the method fails again. The applicability of the method usually lies within the modulation frequency range ω/2π ≈ 1–30 MHz, which allows decay times from 10−1 s to ∼ 10−9 s to be measured. The phase-modulation method has been given considerable attention for a long time. Its main beneﬁt consists in the capacity to measure relatively fast luminescence kinetics without the need for any source of short or ultrashort pulses. Excitation can be provided by a cw lamp whose output is modulated at high frequency using, for example, light diffraction on ultrasound waves in crystals (the technique of ultrasound waves in the frequency range of 10 MHz is well mastered and a large variety of modulators are available). Due to the development of reliable picosecond and femtosecond lasers with high repetition rate and good pulse-height stability, the phase-shift method has been put largely in the shade. Also its restriction to a simple single-exponential decay as outlined above had a role to play. A wider spectrum of information on luminescence decay can be obtained using other methods, based on high repetition rate pulsed excitation, like the time-correlated single–photon counting or sampling methods, which are the subject of the following subsections.

72

Experimental techniques

Fig. 2.44 Schematic representation of a luminescence response measured by the time-correlated photon-counting method. A narrow excitation pulse (not shown) is emitted at time t = 0.

2.9.3 Time-correlated photon counting This method is based on the statistical character of luminescence photon emission. Upon excitation of a luminescent material by a very short light pulse, the luminescence emission builds up and then decays. During the decay, the number of emitted photons decreases in time. Photons are emitted randomly in all directions. Suppose we select a narrow solid angle (e.g. using a circular aperture) and record (by a photomultiplier) the arrival time of single photons within this angle, i.e. the time when a pulse appears at the photomultiplier output corresponding to a single photoelectron released from the photocathode (see Subsection 2.4.2); the moment when the excitation pulse was emitted is taken as the time origin t = 0. The pulse excitation of the sample is repeated many times. The luminescence rise and decay curve we are interested in is obtained by plotting a histogram of the pulse occurrence within certain time intervals ti (called time slots), as illustrated in Fig. 2.44. This is based on the fact that the probability of emitting a photon into the selected solid angle at any time is proportional to the number of luminescence centres actually being in an excited state. One should be aware that the curve shown in Fig. 2.44 is accumulated randomly during the experiment, which means not by shifting regularly from the ﬁrst time slot towards the next one in sequence t1 , t2 , t3 , . . . , etc. The detection events arrive randomly into any of the time slots. In order to perform such an experiment, two basic requirements must be satisﬁed: 1. The luminescence intensity must be very low to enable the arrival of single photons to be recorded.12 12 In fact there are two kinds of time-correlated photon counting (TC-PC) experiments: The ﬁrst one is called time-correlated single-photon counting. Here only one (or no) count is detected following each excitation event (actually, the correct proportion is one detected photon per 10 or 100 excitation pulses—if the rate is higher, the shape of the temporal response is distorted). This

Time-resolved luminescence measurements

73

Fig. 2.45 Functioning of a time→voltage amplitude converter.

2. A high number of photons must be detected to obtain conclusive statistics. The repetition rate of special pulsed lamps emitting nanosecond pulses is of the order of 10–100 kHz; repetition rates of mode-locked pulsed lasers can be of the order of 10–100 MHz. Even for such high-repetition excitation, the accumulation of the entire rise/decay curve may take from minutes up to hours. On the instrumental side, the essential part of this apparatus is a time → voltage converter. Its functioning is illustrated in Fig. 2.45. The converter is initiated by the excitation pulse at time t = 0 (start pulse) and begins to generate a DC voltage linearly increasing in time. The voltage rise is stopped by a stop pulse coming from the photomultiplier (which detects single luminescence photons). The resulting voltage amplitude is proportional to the time delay between t = 0 and the stop pulse. This voltage is sorted according to its amplitude and then ranked into the corresponding channel of a multichannel analyser. The immediate result of this measurement thus has the form shown in Fig. 2.44, where the horizontal axis represents channel numbers, not directly the time intervals ti . The time-correlated photon-counting method is very sensitive and accurate, but requires special electronic devices; besides, measurements are sometimes time-consuming. It is mainly applied to the detection of luminescence kinetics at the time-scale of ∼ 10−6 –10−10 s. Obviously, the ﬁnite width of the excitation pulses L(t) must also be taken into account here and the experimental result, if necessary, deconvoluted in order to extract the actual luminescence response, according to (2.62). A special deconvolution method dedicated to the case of very high repetition rates of the excitation pulses (larger than the reciprocal decay time) is described in [29].

2.9.4 Boxcar integrator All of the above mentioned methods enable us to detect the luminescence time response at a ﬁxed wavelength (or a range of wavelengths). Now we are going is used to measure fast nanosecond decays under high-repetition (> MHz) pulsed lasers (in order to accumulate enough statistics in a reasonable time). The second type of TC-PC is applied to measure slow (microsecond) decays. Here more than one count should be detected at each (lowrepetition) excitation pulse, otherwise the statistics cannot be accumulated within a relatively short time period.

74

Experimental techniques

Fig. 2.46 (a) Schematic of boxcar integrator operation. The signal input is loaded by periodic short voltage pulses from a photomultiplier. The trigger input receives synchronous trigger pulses that turn on (via a time base and after a deﬁned delay TD ) a fast sampling switch (gate) for a period TG . The repetition rate of the whole process is f = 1/TP . After Letzter [30]. The attached graph demonstrates the measured proﬁle of N2 -laser pulses (337 nm) with a temporal FWHM of about 10 ns (detection by a photomultiplier, pulse repetition rate f = 50 Hz). (b) Digital EG&G PAR Model 4400 boxcar integrator. Reproduced with permission by Ametek Signal Recovery (formerly EG&G Signal Recovery).

to describe an electronic device called a boxcar integrator (or boxcar averager) which has a much greater diversity of experimental options; of practical importance for us is its capacity to record complete time-resolved luminescence spectra (i.e. emission spectra when the luminescence intensity is registered at a predeﬁned delay after the excitation event). To begin with, we describe the principle of the device, then its application to luminescence kinetics and ﬁnally we shall address the measurement of time-resolved emission spectra. The boxcar integrator was developed by Princeton Applied Research in the middle of the 1960s, mainly in response to demands for the detection of a wide variety of fast optical signals with high repetition rate, emerging due to the rapid development of laser techniques at that time. It can also be classiﬁed as a device aimed at detecting weak repetitive signals unprocessable by the lock-in detection technique. A simpliﬁed scheme of boxcar functioning is shown in Fig. 2.46(a) [30]. There are two inputs: (i) the investigated signal (pulsed output from a photomultiplier or other detector) that is repeated with a period TP , and (ii) a trigger pulse, synchronous with the signal. The signal channel contains a broadband preampliﬁer, a fast sampling unit, and a low-pass RC ﬁlter. With the incoming trigger pulse, the sampling unit (gate) is switched on (with a deﬁned delay Td ) for a time interval TG . Therefore, during this time interval a capacitor Cis being charged and its voltage rises. The whole process is repeated with a frequency f = 1/TP . As far as the delay TD is concerned, two modes of operation are feasible. Either TD is kept constant, or is left to increase linearly in time. The latter mode is applied to measure the temporal shape of the incoming pulse, i.e. the

Time-resolved luminescence measurements

luminescence kinetics. Here the gate samples the temporal proﬁle of signal pulses by shifting the delay by an increment t after each incoming pulse.13 The RC time constant is usually much larger than TG , thus the voltage on the capacitor C increases in small steps (Fig. 2.46(a)). Due to the simultaneous slow discharging of the capacitor the output signal asymptotically approaches the average value of the input pulse amplitude within the given time interval. In other words, the latest signal acquisitions have predominant weight over the earlier ones that fade away gradually and the input signal shape is replicated at the output. This mode of signal treatment is referred to as an exponential averaging. At the same time, an important condition is to ﬁnd an appropriate relation among several experimental parameters—too fast gate scanning distorts the pulse shape while too slow scanning leads to unnecessary prolongation of the experiment and possible errors due to drift of experimental parameters. This means that an optimum time of signal scanning TM must exist; it can be shown that this optimum scanning time is given approximately as TM ≈ 5RCX/TG2 f , where X denotes the overall sampled time interval. The inset in Fig. 2.46(a) shows an example: a N2 -laser pulse shape measured in this way (X = 60 ns, TG = 1 ns, TM = 60 s, f = 50 Hz). Time-resolved emission spectra are measured in the TD = const mode (to be more speciﬁc, using several discrete values of TD ). The experiment can be performed in the set-up shown in Fig. 2.47: for any selected delay value TD the monochromator is let to scan the spectrum. This means that this time the same portion of the temporal proﬁle of luminescence pulse is sampled for a time TG , while the wavelength is being scanned. On condition of a proper setting of all experimental parameters, i.e. the scanning speed in relation to RC, TG and f , exponential averaging takes place and the luminescence spectrum is continuously recorded under a pulsed excitation. (This ability of the boxcar integrator contributed considerably to the fast development of laser spectroscopy in the 1960s and 1970s; till that time, there was practically only one way to detect emission spectra under pulsed excitation, namely, lengthy and uncertain registration on a photographic plate.) Moreover, the signal-tonoise ratio is improved when using a boxcar, because the input noise is not coherent with the trigger pulse rate and its contribution to the integrated output signal is therefore small, likewise in the lock-in technique.

13 In principle, one deals with a stroboscopic method of measurement of periodic events, exploited also in, for example, a sampling storage osciloscope.

75 Fig. 2.47 Single-channel luminescence spectrometer with a pulsed laser excitation. Pulses from a dye laser (pumped by a nitrogen laser) periodically excite luminescence of a sample, a small fraction of the excitation pulse energy (reﬂected on a beam splitter) being applied to generate trigger pulses for a boxcar integrator. The delay line, inserted between the photomultiplier and the boxcar signal input, serves to compensate for internal delay in the triggering circuits of the integrator. Adapted from Letzter [30].

76

Experimental techniques

Fig. 2.48 Time-resolved luminescence spectra of AgBr at a temperature of T = 6 K, measured in an experimental conﬁguration similar to that shown in Fig. 2.47 (only the dye laser was omitted, the sample was excited directly with N2 -laser pulses 337 nm, 2 MW/cm2 , 10 ns). The gate width is TG ∼ 3 ns and the values of the delay TD behind the excitation pulse maximum are indicated on the left-hand side of each spectrum. With increasing delay TD the emission lines ITO (FE) and M are rapidly fading out and a slow band around 490 nm appears (this emission band is shown also in Fig. 1.2(b), but excited with cw UV light). Adapted from Baba and Masumi. [31].

Upon changing the time position of the gate, a new spectrum is registered at another delay TD after the excitation pulse—this is the principle of timeresolved luminescence spectroscopy. An example is presented in Fig. 2.48, showing low-temperature (6 K) time-resolved emission spectra of pure AgBr under pulsed excitation with a N2 -laser (337 nm) [31]. Clearly, the spectra in different time delays (windows) behind the excitation event can differ substantially. Immediately after excitation only two narrow emission lines (‘fast component’), labelled ITO (FE) and M, are observed. They rapidly fade out with increasing delay TD and a new broad emission band (‘slow component’) appears around ∼ 490 nm. The origin of these spectral features will be discussed in Sections 7.1, 7.2, and 8.2.

2.9.5 Streak camera A boxcar integrator is an excellent instrument to study luminescence kinetics and decay times from about 500 ps to hundreds of ns but does not serve this purpose for faster processes taking place on shorter time-scales of 10–100 ps. This constraint is due to the limited speed of the boxcar electronic circuits as well as the relatively slow response of the photomultipliers (even the special fast photomultipliers do not have the signal onset faster than ∼ 500 ps). Similar limitations take place also in oscilloscopes, more speciﬁcally in their input ampliﬁers. For luminescence transients occurring on the time-scale of picoseconds and femtoseconds, either special methods of nonlinear optics (upconversion) or the so-called streak camera should be used. This device enables the measurement of both time evolutions of ultrafast light signals and timeresolved emission spectra, likewise the boxcar integrator. The development of the streak camera at the beginning of the 1970s (Hamamatsu Co. Ltd.) was

Time-resolved luminescence measurements

again motivated by the fast dissemination of lasers emitting picosecond and femtosecond pulses. The streak camera is a device which converts temporal information, originating in a light-emission event, to spatial information. Roughly speaking, the streak camera combines, in a single device, the principles of a photomultiplier with the basic components of an oscilloscope: the external photoelectric effect, deﬂection of an electron beam and a phosphorescence screen. The principle of a streak camera is shown in Fig. 2.49. The analysed light pulse is focused on the entrance (mechanical) slit, whose image is projected onto a photocathode deposited on the internal front face of an evacuated tube. Emitted photoelectrons (whose number is proportional to the intensity of the incident light) are accelerated in an electric ﬁeld and then deﬂected by a high voltage applied in the direction perpendicular to the acceleration voltage. This deﬂection voltage is applied synchronously with the incoming light pulses, the photoelectrons thus being swept with a deﬁned speed and known trajectory (like in an oscilloscope, but without input ampliﬁer here) by which means the time information is converted to spatial information. Then these electrons undergo multiplication via secondary electron emission in the socalled microchannel plate, and ﬁnally they bombard a phosphorescence screen on the opposite end of the vacuum tube. This creates the phosphorescence image, rendering the temporal distribution of intensity of the analysed luminescence pulses in the form of a vertical spatial distribution of phosphorescence intensity on the screen. The phospherescence image is then recorded (e.g. by a photodiode array or a CCD detector), treated and displayed on a computer screen. An example of a measured luminescence transient is presented in Fig. 2.50: luminescence of Hg2 Cl2 (calomel) crystals excited by ∼ 35 ps pulses of second harmonic frequency from a passively mode-locked Nd:YAG laser (532 nm) [32]. As Hg2 Cl2 is an anisotropic uniaxial crystal, its luminescence response exhibits a slightly different temporal shape under polarization of the excitation light perpendicular to the optical axis c (electric ﬁeld vector ⊥c) and parallel with this axis ( ||c). On the left-hand side of the lower curve in Fig. 2.50 one can also see the shape of the excitation pulse; this was enabled by the appropriate setting of an optical delay line for both luminescence and the reﬂected fraction of the excitation light and their simultaneous focusing onto the camera entrance slit.

77 Fig. 2.49 Operation schematic of a streak camera. The light pulse passing through the entrance slit and hitting a photocathode induces emission of photoelectrons inside an evacuated tube. Photoelectrons are accelerated along the horizontal direction (i.e. the direction of the incoming light) by a voltage applied between the photocathode and a metal mesh and subsequently deﬂected by a high voltage in the vertical direction. Upon impinging on a phosphorescence screen, the photoelectrons produce a phosphorescent trace with spatial distribution of intensity corresponding to the temporal proﬁle of the incoming pulse. After materials by Hamamatsu Co. Ltd.

78

Experimental techniques

Fig. 2.50 Luminescence transients measured and displayed by a streak camera (luminescence of Hg2 Cl2 crystals spectrally situated around ∼ 396 nm, excited at T ∼ 80 K via two-photon absorption of second harmonic pulses from a Nd:YAG laser with temporal FWHM ∼ 35 ps). The lower curve shows also (on the left) the excitation pulse proﬁle. Full lines represent experimental data while points show the calculated convolution of the excitation pulse proﬁle with a double-exponential decay. After Svoboda et al. [32].

The open circles in Fig. 2.50 represent the best numerical ﬁt using the model of double-exponential decay i λ (t) = a1 exp(–t/τ1 ) + a2 exp(–t/τ2 ) with parameters: a1 = 0.93, τ1 = (17 ± 5) ps, a2 = 0.07, τ2 = (87 ± 30) ps ( ||c), a1 = 0.82, τ1 = (25 ± 7) ps, a2 = 0.18, τ2 = (77 ± 26) ps ( ⊥c). (2.64) Figure 2.50 indicates that the excitation pulse FWHM and the characteristic times τi are of the same order of magnitude, therefore to ﬁt the experiment properly, numerical convolution of the measured system response to the excitation pulses with a presumed model shape of luminescence decay i λ (t) according to eqn (2.62) was applied. The numerical values given in (2.64) give an idea of the attainable accuracy in extracting the decay times τi by this method. The principle of the measurement of time-resolved luminescence spectra follows from Fig. 2.49. The streak camera can be attached to the spectrograph output in such a way that the spectrum of the luminescence signal is imaged onto the entrance slit. Then the two-dimensional image displayed on the phosphorescence screen represents the temporal evolution of the pulse spectral content while the photoelectrons are vertically swept. Various models of streak cameras are commercially available for various time regimes, with time resolution as short as ≤ 1 ps. Streak cameras can operate in a single-shot mode but also at high repetition rates of the order of 100 MHz (the so-called synchroscan camera).

2.10 Problems 2/1: Photomultiplier nonlinearity. When illuminating a high-gain photomultiplier by too high photon ﬂux, the photocurrent between the last dynodes may attain such high values (without yet inducing irreversible damage to the photomultiplier) that the condition Ia (anode current) Ivd (current through the voltage divider) is no longer fulﬁlled—see Fig. 2.5(b). Consequently, the last stages of the voltage divider are partially ‘short-circuited’ by the current Ia ﬂowing inside the photomultiplier. Then the voltage

Problems from an external high-voltage supply is concentrated predominantly in several ﬁrst stages of the divider (close behind the photocathode). Thus a positive feedback appears, the photomultiplier gain increases and the linearity of the photomultiplier response is violated. Discuss the consequences of this effect for measurements of optical gain according to the paper by Webb [33]. 2/2: Show that the relation between the photomultiplier anode sensitivity k(λ) (expressed in units of A/W) and the photocathode quantum efﬁciency ηph has the form hc k 1240 k ηph (%) = × 100 = × 100, λe G λ G where h is Planck’s constant (Js), c is the speed of light (m/s), e is the electron charge (C), λ denotes the wavelength of the incident light, and G is the photomultiplier gain. 2/3: You are in a position to investigate the emission spectrum of a semiconductor with low luminescence yield. This spectrum is expected to be situated between 600 and 800 nm and composed of spectral bands and lines, the FWHM of the narrowest ones being about 1 nm and that are separated from one another by 2.5 nm. Decide which of the following monochromators is more convenient for this task and justify your selection: 1. Focal length f = 1000 mm, aperture f /7.5, holographic grating 120 × 140 mm2 (blaze at 630 nm), reciprocal linear dispersion L −1 = 0.8 nm/mm, resolving power R = 7×104 (at the slit width of 10 μm). 2. Focal length f = 320 mm, aperture f /4.2, holographic grating 120 × 140 mm2 (blaze at 750 nm), reciprocal linear dispersion L −1 = 2.4 nm/mm, resolving power R = 6×103 (at the slit width of 10 μm). What is the maximum slit width of the selected monochromator you may apply in the experiment? 2/4: A scanning monochromator is used to measure one of the emission lines of the material mentioned in the previous problem. The signal from a photomultiplier is treated by a lock-in ampliﬁer. What is the maximum time constant you can apply (in order to obtain the spectrum as smooth as possible but without distortions), if the wavelength scan speed is 10 nm/min? What is the total acquisition time of the spectrum? Note: The values of the time constant can usually be set in steps 1–3–10, e.g. 1 ms–3 ms–10 ms. 2/5: (a) Show that the FWHM of a bell-shape curve f (x) = x exp(–x/a) is FWHM ∼ 2.45 a. (b) Suppose you excite photoluminescence with optical pulses of temporal FWHM = 5 ns and measure the corresponding luminescence decay. Let the decay curve i(t) be of single-exponential type with the characteristic time constant τ = 15 ns. Estimate the uncertainty in determining τ if no deconvolution of the experimental curve is applied. For the sake of simplicity suppose that the excitation pulse is described by a function L(t) = t exp(–t/a) and use the result of part (a).

79

80

Experimental techniques

References 1. Voos, M., Leheny, R. F., and Shah, J. (1980). Radiative recombination. In: Handbook on Semiconductors (ed. T. S. Moss), Vol. 2 (ed. M. Balkanski), p. 329. North Holland, Amsterdam. 2. Kulakovskii, V. D. and Timofeev, V. B. (1983). Thermodynamics of electron–hole liquid in semiconductors. In: Modern Problems in Condensed Matter Sciences (general ed. V. M. Agranovich and A. A. Maradudin), Vol. 6, Electron–Hole Droplets in Semiconductors (ed. C. D. Jeffries and L. V. Keldysh), p. 95. North Holland, Amsterdam. 3. Valenta, J. (1994). Photoluminescence characterization of selected semiconductors and insulators. PhD. thesis, Charles University in Prague, Faculty of Mathematics & Physics, Prague. 4. Bebb, H. B. and Williams, E. W. (1972). Photoluminescence I. Theory. In: Semiconductors and Semimetals (ed. R. K. Willardson and A. C. Beer), Vol. 8, p. 181. Academic Press, New York. 5. Itoh, C., Tanimura, K., Itoh, N., and Itoh, M. (1989). Phys. Rev. B, 39, 11183. 6. Engstrom, R. W. (1980). Photomultiplier Handbook. RCA/Burle, USA. 7. Photomultiplier Tube. Principle to Application. Hamamatsu Photonics K. K. 1994. 8. Rieke, G. H. (2003). Detection of Light. From Ultraviolet to Submillimeter, 2nd edn, p. 194. Cambridge University Press, Cambridge. 9. Saleh, B. E. A. and Teich, M. C. (2007). Fundamentals of Photonics, 2nd edn. Wiley-Interscience, New York. 10. Ferrari, M., Pavesi, L., and Righini, G. C. (eds) (2002). Micro-Optoelectronics: Materials, Devices and Integration, p. 26. Italian Society of Optics and Photonics, Centro Editoriale Toscano. 11. Mac Intyre, R. J. (1966). IEEE Trans. Elect. Dev., 13, 164. 12. Spectrum One, Spectroscopic CCD Detectors. ISA Jobin Yvon-Spex, Horiba. 13. Michel, P. (1953). La spectroscopie d’emission et ses applications. Collection Armand Colin, Paris. 14. Sawyer, R. A. (1951). Experimental Spectroscopy. Prentice Hall. New York. 15. James, J. and James, J. F. (2007). Spectrograph Design Fundamentals. Cambridge University Press, Cambridge. 16. Demtr¨oder, W. (2003). Laser Spectroscopy: Basic Concepts and Instrumentation, p. 109. Springer, Heidelberg. 17. Pelant, I. , H´ala, J., Parma, L., and Vacek, K. (1980). Solid State Comm., 36, 729. 18. Hulin, D., Mysyrowicz, A., Combescot, M., Pelant, I., and Benoit a` la Guillaume, C. (1977). Phys. Rev. Lett., 39, 1169. 19. Photon Counting using Photomultiplier Tubes (1998). Technical information, Hamamatsu Photonics K. K. ˇ zin, G. N., and Popova, M. N. (1982). 20. Bagdanskis, N. I., Bukreev, V. S., Ziˇ High resolution infrared spectrometers (in Russian: Infrakrasnyje spektrometry vysokogo razreˇsenija). In Current Trends in Spectroscopy Techniques (in Russian: Sovremennyje tendencii v technike spektroskopii, ed. S. G. Rautman), p. 153. Nauka, Novosibirsk. 21. Fojt´ık, P. (1999). Selected photoelectrical properties of amorphous and microcrystalline silicon with respect to lateral resolution (in Czech: Vybran´e fotoelektrick´e vlastnosti amorfn´ıho a mikrokrystalick´eho kˇrem´ıku s pˇrihl´ednut´ım k later´aln´ımu rozliˇsen´ı). Diploma thesis, Charles University in Prague, Faculty of Mathematics & Physics, Prague. 22. Shionoya, S. and Yen, W. M. (eds) (1999). Phosphor Handbook, Chap. 14. CRC Press, Boca Raton. 23. Dian, J., Valenta, J., Luterov´a, K., Pelant, I., Nikl, M., Muller, D., Grob, J. J., Rehspringer, J.-L., and H¨onerlage, B. (2000). Mater. Sci. Engin. B, 69–70, 564. 24. Pelant, I., Kohlov´a, V., H´ala, J., Ambroˇz, M., and Vacek, K. (1987). Solid State Com., 64, 939.

References 25. Bertero, M. and Boccacci, P. (1998). Introduction to Inverse Problems in Imaging. Institute of Physics Publishing, Bristol. 26. Shah, J. (1999). Ultrafast Processes of Semiconductors and Semiconductor Nanostructures. Springer Series in Solid-State Sciences, Vol. 115. Springer, Berlin. 27. Lakowitz, J. R. (1983): Principles of Fluorescence Spectroscopy, Chap. 3. Plenum Press, New York and London. 28. Luterov´a, K., Pelant, I., Valenta, J., Rehspringer, J.-L., Muller, D., Grob, J. J., Dian, J., and H¨onerlage, B. (2000). Appl. Phys. Lett., 77, 2952. 29. Sakai, Y. and Hirayama, S. (1988). J. Luminescence, 39, 145. 30. Letzter, S. (1983). Laser Focus, December 1983. 31. Baba, T. and Masumi, T. (1977). Nuovo Cimento B, 39, 609. ˇ and Pelant, I. (1990). phys. stat. sol. (b), 157, 32. Svoboda, A., Veˇceˇr, J., Barta, C., K69. 33. Webb, C. (2003). Optics & Photonics News, May 2003, 14.

81

Kinetic description of luminescence processes

3 3.1 Radiative and non-radiative recombination. Luminescence quantum yield 82 3.2 Monomolecular process

85

3.3 Bimolecular process

87

3.4 Stretched exponential

89

3.5 Multiple processes present simultaneously

91

3.6 Problems

96

A multitude of characteristic features of luminescence can described and understood using simple kinetic equations, which, from the point of view of mathematics, represent ﬁrst-order differential equations in time. In this chapter, we shall ﬁrst introduce important parameters called the probability of radiative and non-radiative transition and the luminescence quantum yield. We shall discuss their relation to the experimentally established luminescence decay time. Next, we shall formulate kinetic equations for several simple luminescence phenomena. Solving the equations, we shall proceed ﬁrstly to explicate transient luminescence phenomena (i.e. the form of luminescence decay or possibly rise in time) and, secondly, we shall obtain the functional dependence of emission intensity on the optical excitation intensity in the steady state.

3.1 Radiative and non-radiative recombination. Luminescence quantum yield An excited luminescence centre is in a non-equilibrium thermodynamic state and it loses its electron excitation energy after a certain relaxation time and goes into the ground state. The transition can occur in two ways. The excitation energy is either radiated away in the form of a luminescence photon after the mean lifetime τr or the excess energy is transmitted in the form of heat (vibrations) to the crystal lattice after time τnr or it can possibly cause photochemical changes in the crystal matrix or generate a lattice defect. The ﬁrst kind of transition is called a radiative transition, the time τr is the radiative recombination time (radiative lifetime), transitions of the second kind are called non-radiative and τnr is the non-radiative recombination time (non-radiative lifetime). The inverse values (τr )−1 and (τnr )−1 then represent the probability of the corresponding transition per unit time (the recombination rate). The total probability of transition to the ground state is given by 1 1 1 ; = + τ τr τnr

(3.1)

Radiative and non-radiative recombination

83

we can imagine this in analogy to electromagnetism as two parallel conductors, the resulting conductivity of which is given by the sum of the inverse values of their individual resistances (Fig. 3.1). We deﬁne the luminescence quantum yield or quantum efﬁciency, already mentioned in Section 2.1, as η=

1/τr ≤1 1/τr + 1/τnr

(3.2)

i.e. as the ratio of the radiative recombination rate to the total recombination rate. For brightly luminescent materials τr τnr holds true, which means the given excited centre is much more likely to go into the ground state by radiating a photon hνlum than by a non-radiative transition. Neglecting 1/τ·nr in (3.2), we get η → 1 (we also say the quantum yield is 100%). However, such materials almost never occur in nature. In fact, we speak of strongly luminescent materials already if η is of the order of 0.1. The word ‘quantum’ in the deﬁnitions given here implicitly points to the fact that both luminescence excitation and light emission take place through one-photon elementary steps; e.g. η = 0.5 means there is one emitted photon to every two absorbed photons. Thus, multiple-photon phenomena, although feasible in general, are not considered here. Likewise, deﬁnition (3.2) does not allow for the energy difference between the exciting hνex and emitted hνlum photons—in this sense, we sometimes introduce the power efﬁciency ηP = (hνlum / hνex )η. Due to Stokes’ law, we have ηP ≤ η. For injection electroluminescence, η relates not to the number of photons absorbed but to the number of electron–hole pairs injected. What is the physical meaning of the time τ given by expression (3.1)? It characterizes the emptying of the excited-state level in a large ensemble of luminescence centres by radiative and non-radiative transitions simultaneously. Yet, the population decay of an excited level is reﬂected just in a decrease of the luminescence intensity as it decays after the excitation is turned off. Therefore, the time τ is (in accordance with the notation introduced in Section 2.9) an experimentally accessible quantity—the luminescence decay time. By means of this decay time, we can rewrite the expression for quantum efﬁciency (3.2) in the form η=

τ (≤ 1). τr

(3.3)

Let us point out straightaway the occasional erroneous use of the terms we have just introduced. The radiative lifetime (τr ) is not the same as the luminescence decay time (τ ) although the admitted similarity of the terms may tempt us to confuse them! (On the contrary, we shall show shortly that, in a special case, the luminescence decay time may be identical to the non-radiative recombination time!) From the point of view of mathematics, relations (3.1), (3.2), and (3.3) are just trivial fractions but, surprisingly enough, they involve a wide spectrum of physical information. So ﬁrstly, it is interesting that expression (3.3) relates two measurable quantities (η, τ ) to an important quantum-mechanical parameter

Fig. 3.1 Illustration of the deﬁnition of luminescence quantum efﬁciency.

84

Kinetic description of luminescence processes characterizing optical transitions from a theoretical perspective (the reciprocal value of the radiative lifetime τr−1 is proportional to the square of the modulus of the corresponding transition matrix element [1–3]). The magnitude of the matrix element basically cannot be obtained by direct measurements and it is neither simple nor reliable to calculate it. Therefore, the simple formula (3.3) appears to provides a welcome opportunity to obtain τr−1 from two experimentally available quantities and to compare the result to the theory (in a semiconductor with a direct bandgap, τr is of the order of 10−9 s, and with an indirect bandgap, τr ≈ 10−4 to 10−3 s). However, while it is very easy to measure τ —and we have discussed several of the most common experimental methods in Section 2.9—it is, in contrast, extremely difﬁcult to measure the quantum efﬁciency η with sufﬁcient accuracy, as we have, for that matter, also mentioned before. Hence, we should not overestimate the signiﬁcance of expression (3.3) in this sense; nonetheless, it is very important that by measuring the temperature dependence of the luminescence intensity (which we can consider, to a good approximation, proportional to the quantum yield η) and of the luminescence decay time τ we can obtain from (3.3) information on the temperature dependence of the radiative recombination time τr , albeit in relative units. In addition, relations (3.1)–(3.3) enable us to asses quickly a number of situations we may encounter in practice. Let us ﬁrst consider the case τnr −1 , is much higher than τr < ∞. Then the non-radiative recombination rate, τnr the radiative transition rate; nonetheless, some weak luminescence radiation may still be present. Naturally, the quantum yield η will be very low (η ≈ τnr /τr 1 as follows directly from (3.2)) and what is particularly interesting is that—as an immediate consequence of (3.1)—we get τ ∼ = τnr . Thus, measuring the luminescence decay time, we are now actually measuring the non-radiative lifetime. Or, put in still another way, if we reveal in an experiment a weak luminescence decaying very quickly then there will very likely be a strong inﬂuence of non-radiative transitions. The opposite case reads τr τnr . The quantum yield η is close to unity according to (3.2) and τ ∼ = τr holds. Although we encounter this situation much less often than the previous case we must still mention the following possibility. Let us consider a material with a relatively large τr , which, in itself, is thus not a very efﬁcient phosphor. Yet, if we are able to ‘forbid’ somehow all non-radiative transitions then τnr → ∞, τr τnr and the electronically excited system has no other choice but to return—albeit slowly—to the ground state exclusively via radiative transitions. Hence, in this way, we can obtain a material featuring efﬁcient luminescence (η ∼ = 1). The total number of photons emitted per unit of time will be relatively low; nevertheless, this mechanism is thought to be one of the factors contributing to the intense luminescence of so-called porous silicon and of silicon nanocrystals. Silicon is a poor phosphor as a result of its indirect bandgap. The radiative lifetime is long (τr ≈ 10−3 s) and almost all transitions to the ground state occur via much more efﬁcient non-radiative processes. In nanocrystals, however, the non-radiative transitions take place mostly on the surface of the nanocrystal and they can be prevented through efﬁcient passivation of unoccupied surface bonds by attaching, e.g., hydrogen or oxygen atoms.

Monomolecular process

85

3.2 Monomolecular process Let us consider a localized luminescence centre1 in a crystal or possibly in an amorphous matrix, typically represented by an impurity atom. Let us assume the centre can be brought into an electronic excited state by either absorbing light directly or via energy transfer from the optically excited surrounding matrix. Let both processes be described by a quantity G, which is the number of photons absorbed in unit volume per unit time. Subsequently, centres in an excited state return to the ground state, partly radiatively and partly nonradiatively. If the concentration of the excited centres is n(t), the processes under consideration are described by the equation n n dn n =G− , =G− − dt τr τnr τ

(3.4)

where d/dt denotes the derivative with respect to time and G is called the generation term. A schematic is shown in Fig. 3.2(a). We shall now analyse eqn (3.4) in two cases: (a) luminescence decay and (b) steady state. (a) Luminescence decay is characterized by the excitation being switched off (G = 0) at time t = 0. We are interested in the fall-off of the luminescence intensity i(t) at times t ≥ 0. Equation (3.4) has the form dn n =− dt τ and its solution thus reads n(t) = n(0) exp(–t/τ ). The luminescence intensity i(t) (here, the number of photons emitted from unit volume per unit time) is given by the ratio n(t)/τr , and hence the desired intensity falloff is n(t) n(0) −t/τ i(t) = = e = i(0)e−t/τ , t ≥ 0. (3.5) τr τr Here, i(0) denotes the intensity at time t = 0. We can see that in this case (the so-called monomolecular process or a localized centre) the luminescence exhibits strictly single-exponential decay governed by the total lifetime τ , as we have already described in Section 3.1 and as plotted in Fig. 3.2(b). (b) The steady state—when the excitation G is turned on and when, after the initial increase in i(t), the intensity of luminescence settles at a constant value—is determined by the condition dn/dt = 0. From eqn (3.4) and with regard to Fig. 3.2(b), we have G=

n(0) n(0) n(0) + = i(0) + . τr τnr τnr

(3.6)

The generation term G is closely related to the excitation radiation intensity Iex (here, the number of photons incident upon unit surface area per unit time). Let us consider the common case when all excitation radiation 1 By this we shall mean an electron excitation localized at a certain impurity or defect. Free quasi-particles do not participate in recombination phenomena.

Fig. 3.2 (a) The monomolecular luminescence process. Wavy lines represent non-radiative thermalization of the carriers, their capture, and possibly non-radiative recombination. (b) The kinetics of monomolecular luminescence upon turning the excitation source on and off.

86

Kinetic description of luminescence processes is absorbed in the sample (we neglect reﬂection for the sake of simplicity). Absorption occurs in a thin subsurface layer, the depth of which is roughly equal to the reciprocal value of the absorption coefﬁcient of the excitation light α −1 . If the area of the excited luminescence surface is S then there are Iex S photons incident per unit time and the photons are thus absorbed in a volume ∼ Sα −1 . The density of the absorbed photons, or the number of centres excited per unit volume per unit time, is thus G ≈ (Iex S)/Sα −1 = α Iex . From eqn (3.6) we then get i(0) = G −

τr n(0) = α Iex − i(0) τnr τnr

and after some simple algebra and considering deﬁnition (3.2), we immediately have i(0) = ηα Iex .

(3.7)

In the case of monomolecular recombination, the stationary value of the luminescence intensity, i(0), is thus directly proportional to the excitation intensity Iex . Hence, we have obtained two simple and important guidelines facilitating the interpretation of experimental data. Observing a single-exponential decay together with a linear increase in luminescence intensity are rather strong indications that the microscopic origin of the examined luminescence might lie within a localized centre. This is not unambiguous evidence—similar features can be seen in, for example, the luminescence of a kind of free quasi-particle, the free exciton—and yet, such an observation helps us to exclude a number of other types of recombination processes. Let us note further that the presence of two kinds of localized luminescence centres will show itself via a double-exponential decay i(t) = a1 e−t/τ1 + a2 e−t/τ2 ,

(3.8)

where ai (i = 1, 2) denotes the amplitudes of the individual components. Naturally, the prerequisite of observing a dependence of the form (3.8) is that we detect spectrally unresolved luminescence of both centres, e.g. when the emission wavelengths of both centres are close to each other and their spectra overlap. Today, computer-aided ﬁtting of the experimental decay curve enables us to determine the parameters a1 , a2 , and τ1 , τ2 quickly and reliably even in case we need to use deconvolution methods (see (2-64) and Fig. 2.50). One cannot help thinking of generalizing relation (3.8) to a sum of multiple exponential functions. However, when attempting to ﬁt the luminesj cence decay curve using the expression i(t) = i=1 ai e−t/τi ( j ≥ 3), we must be very careful. Of course, from the point of view of mathematics, such a ﬁt is feasible and we usually achieve very good agreement between our calculation and experiment, yet, from the point of view of physics, such a result in itself can hardly be considered as evidence for the presence of three or more luminescence centres. This is because, in principle, any of the

Bimolecular process

87

characteristic forms of decay curve, which we shall discuss below, can be modelled very nicely as a sum of three exponentials with six ﬁtting parameters (ai , τi , i = 1, 2, 3); the informative value of such a ﬁt, however, is highly questionable.

3.3 Bimolecular process Let us consider the process shown in Fig. 3.3. If a semiconductor absorbs a photon of energy above the bandgap, E g , then free electron–hole pairs are produced. Let us denote the concentration of electrons by n and the concentration of holes by p. If there is no impurity atom or possibly a lattice defect nearby where localization of the created photocarriers could occur then electrons and holes will diffuse along the edges of the respective bands and, eventually, electrons will recombine with the nearest holes (as their wavefunctions overlap most), whether radiatively or non-radiatively. The above processes are described by the equation dn = G − β n p, dt

(3.9)

where G again denotes the generation term. The recombination term proportional to the product np represents the fact that recombination requires a free electron to encounter a free hole. The coefﬁcient β is called the bimolecular recombination coefﬁcient and can be expressed as the sum of bimolecular radiative (βr ) and bimolecular non-radiative (βnr ) recombination coefﬁcients: β = βr + βnr .2 If we consider, for the sake of simplicity, an intrinsic semiconductor at low temperatures, then n = p and eqn (3.9) can be rewritten as dn(t) = G − βr n 2 − βnr n 2 = G − βn 2 . dt

(3.10)

Here, the term βr n 2 clearly represents the intensity of luminescence generated by bimolecular recombination (order-of-magnitude values of the coefﬁcients βr are βr ∼ 10−10 cm3 s−1 for direct bandgap semiconductors and βr ∼ 10−15 –10−14 cm3 s−1 in indirect bandgap semiconductors). We shall again analyse both the luminescence decay and steady state. (a) Similarly to the monomolecular process, let us turn off the excitation (G = 0) at time t = 0 and follow the decay. Then, relation (3.10) reduces to dn(t) = −βn 2 , dt

2 It should be clear by now that the terms ‘monomolecular’ and ‘bimolecular’ historically originated from the analogous chemical reactions.

Fig. 3.3 An example of a bimolecular luminescence process.

88

Kinetic description of luminescence processes which is an equation we can solve easily if, for example, we separate the variables, use the substitution 1/n = x, and apply the boundary condition n(t = 0) = n(0). We get n(t) =

n(0) (βn(0)t + 1)

and the luminescence intensity i(t) = βr n 2 (t) comes out immediately as βr n 2 (0) i(0) i(0) = = √ , (3.11) 2 2 (βn(0)t + 1) (βn(0)t + 1) (γ i(0)t + 1)2 √ where i(0) is the intensity at time t = 0 and γ = β/ βr . We can see that the form of the bimolecular luminescence decay differs substantially from the exponential function. It is a power-law function of time and, for late times, we can approximate i(t) ≈ t −2 . (b) The steady state is characterized by the condition dn/dt = 0. From (3.10) we get i(t) =

i(0) = βr n 2 (0) = G − βnr n 2 (0) = G − βnr

i(0) , βr

which can be transformed into the form βr βr G= α Iex . i(0) = βr + βnr βr + βnr

(3.12)

Therefore, in the case of bimolecular recombination, the steady-state luminescence intensity remains a linear function of the excitation intensity Iex . However, let us stress again that this result is valid only if the steady state has been reached, that is, in particular when using continuous excitation radiation of an incandescent lamp, or possibly of a gas or a semiconductor laser. Nevertheless, bimolecular recombination requires a rather high density of electron– hole pairs since its probability scales like the square of this density. This is more likely to occur when using excitation by powerful laser pulses. And under a pulsed excitation, the intensity dependence of bimolecular luminescence can be governed by a law different from the linear relation of the type (3.12) as we now proceed to show. Let us ﬁrst solve a general differential equation of the form (3.10). It is easy to check that the solution reads

√ G 1 − e−2 Gβt √ + const. (3.13) n(t) = β 1 + e−2 Gβt Let us now choose a boundary condition different from the one we have used up to now. Let n(0) = 0 at time t = 0 and now we promptly turn on the excitation G in the form of a rectangular pulse of duration tp (Fig. 3.4(a)). √ If 2 Gβt 1 holds for all 0 ≤ t ≤ tp (i.e. the excitation pulse is sufﬁciently short), then we can approximate the exponential terms in (3.13) using a series expansion exp(–x) ≈ 1–x which yields

Stretched exponential

89

Fig. 3.4 Time-dependent bimolecular luminescence under a pulsed excitation. (a) A short excitation pulse √ tp 1/2 Gβ; (b) luminescence response pulse. The dashed curve represents the evolution of luminescence intensity towards the steady state provided the excitation lasts long enough (tp → ∞).

n(t) ≈

√ G 2 G βt ≈ Gt. √ β 2(1 − Gβt)

(3.14)

Then, the luminescence intensity i(t) = βr n 2 (t) is given by 2 . i(t) = βr n 2 (t) ≈ βr G 2 t 2 ≈ βr α 2 t 2 Iex

(3.15)

Hence, the amplitude of the luminescence response pulse is proportional to the square of the excitation intensity Iex (Fig. 3.4(b)). We leave it to the reader to conﬁrm that we can never get a similar quadratic dependence for a monomolecular process even if we excite using an arbitrarily short pulse tp τ (Problem 3/2). When is the excitation pulse ‘short enough’ so that the quadratic dependence (3.15) can reveal itself? To get a numerical estimate, let us consider, for example, excitation by using a rather weak pulsed lamp with an excitation power density of 100 W/cm2 , bimolecular recombination coefﬁcient β = 10−15 cm3 s−1 , and the excitation photon energy hνex = 3.2 eV. Then the excitation intensity in terms of the relevant photon ﬂux is Iex = 100 (J/cm2 s)/ hνex ≈ 2 × 1020 photon/cm2 s. With absorption√coefﬁcient α = 104 cm−1 we have G = Iex α ≈ 2 × 1024 cm−3 s−1 and √ Gβ = √ 2 × 1024 × 10−15 ≈ 4.5 × 104 s−1 . Thus, the relation tp (1/2 Gβ) ≈ 1 × 10−5 s will hold for pulses of duration of roughly 1 μs and less. Of course, under a higher-intensity excitation G and higher values of β, the duration of pulses leading to the quadratic dependence (3.15) will get substantially shorter; nevertheless, it is still easily achievable with excitation by common laser pulses with durations of the order of nanoseconds or tens of picoseconds.

3.4 Stretched exponential In practice, we observe certain cases when the luminescence decay curve is neither governed by the exponential law (3.5) nor by a dependence of the type (3.11) but, instead, it can be described by the so-called stretched exponential i(t) = i(0) exp[−(t/τ )δ ],

(3.16)

90

Kinetic description of luminescence processes where τ is called the decay time and δ is the dispersion factor with 0 < δ < 1. It is obvious that for the limiting value δ = 0, eqn (3.16) represents a constant function, and for δ = 1 relationship (3.16) reduces to the standard exponential decay. Between the limiting values of the parameter δ, the function (3.16) interpolates these two extremes as shown in Fig. 3.5. This also hints at the origin of the name—as if we ‘stretched’ an exponentially decreasing function towards later times. This decay law is often observed in disordered systems and it is believed to be due to the so-called dispersion diffusion of photoexcited carriers. In particular, eqn (3.16) describes very precisely luminescence decay in amorphous semiconductors or silicon nanostructures. Nevertheless, it is important to realize that, in itself, the presence of the stretched exponential function in luminescence decay does not allow us to identify the luminescence centre in microscopic detail. There exist several plausible explanations—e.g. in a silicon nanocrystal system, this can be the case for photocarrier migration between various localized states either within a single nanocrystal or along multiple closely packed nanocrystals. Moreover, the diffusion itself can occur due to carriers being excited from localized to free states (multiple trapping and release) or hopping directly between the localized states. The degree of the dispersion of motion is measured by δ, which depends on the trap density, the distribution of their depths, etc. Moreover, both δ and τ depend also on the temperature and the wavelength at which the decay is measured.

Fig. 3.5 A plot of the stretched exponential i(t) = i(0) exp[−(t/τ )δ ] for i(0) = 1, τ = 10 ms and several values of the parameter δ. (a) A lin–lin scale; (b) a log–log scale often used to plot the stretched exponential.

Multiple processes present simultaneously

91

3.5 Multiple processes present simultaneously Let us now consider a somewhat more complex situation that, however, comes closer to that from a large variety of possible experimental events. We shall deal with two parallel recombination channels: bimolecular (intrinsic) recombination of free electron–hole pairs produced by optical excitation G = α Iex and monomolecular (extrinsic) recombination of impurity atoms present in a total concentration N0 . These impurity centres are excited primarily via the same optical excitation that produces free electrons and holes. All processes involved are shown in Fig. 3.6. We shall be mainly interested in the character of the dependence of both luminescence lines on the excitation intensity in the steady state. We shall show that in case there are both monomolecular and bimolecular luminescence processes present in the material simultaneously, they can be distinguished by their typical intensity dependences. We divide the free photoelectrons and holes into the so-called ‘optical’, n 0 , and ‘thermal’, n t , electrons and ‘optical’, p0 , and ‘thermal’, pt , holes. Optical electrons and holes represent a population of carriers occupying almost all available states in the conduction and valence bands.3 They can mutually recombine radiatively with a bimolecular recombination coefﬁcient β, emitting a photon hνB ≥ E g . By thermal photocarriers n t or possibly pt , we shall mean electrons and holes in the lowest energy states just above the bottom of the conduction or below the top of the valence band, respectively. These quasiparticles originate from the population of optical carriers via thermalization, which process is described using a rate constant k. They have the highest chance to be captured by an impurity centre, promoting this into an excited state. Let us denote the concentration of the excited centres by N . Let the process of both electron and hole capture be described by the same rate constant a; its occurrence probability is proportional to the product of the

Fig. 3.6 (a) The band scheme of a semiconductor showing the processes of bimolecular (intrinsic) and monomolecular (extrinsic) photoluminescence—see the main text and eqns (3.17)–(3.19). The respective photon energies are hνB ≈ E g , hνM ≈ E g –(E 1 + E 2 ). (b) The corresponding block diagram of the transitions. 3 We can presume their energy distribution to be described by the classical Boltzmann tail of the Fermi–Dirac distribution function with the Fermi energy level being roughly amid the bandgap.

92

Kinetic description of luminescence processes concentration of impurity centres in the ground state (N0 –N ) with the concentration of thermal electrons n t , or holes pt , respectively. The excited impurity atoms then luminesce (emitting a photon of energy hνM ≈ E g –(E 1 + E 2 )), the number of recombination acts per unit volume being given by N /τ . Let us note that, for the sake of simplicity and without loss of universality of our arguments, we shall assume 100% quantum efﬁciency in both luminescence processes, i.e. β = βr and τ = τr . All the above processes can be described by the following kinetic equations: dn 0 dt dn t dt dN dt n0

= α Iex − βn 0 p0 − k n 0 ,

(3.17)

= k n 0 − a(N0 − N )n t ,

(3.18)

= a(N0 − N )n t − = p0 , n t = p t .

N ; τ

N = N0 , N = 0,

(3.19)

In the steady state, d/dt = 0, we obtain βn 20 + k n 0 − α Iex = 0,

(3.20)

a(N0 − N )n t − k n 0 = 0,

(3.21)

a(N0 − N )n t = N /τ.

(3.22)

We rewrite equation (3.22) in the form N a n t N0 = , τ (1 + a n t τ )

(3.23)

having thus obtained a parametric expression for the monomolecular luminescence intensity, IM = N /τ ; for the bimolecular luminescence intensity, we have in accordance with our previous notation IB = β n 20 . Solving the quadratic equation (3.20), we get the equilibrium concentration of optical electrons, n 0 , and hence immediately also IB ; using eqns (3.21) and (3.23), we obtain n t and thus also IM . The solution to (3.20) reads k Iex k2 n0 = 1+ −1 , I0 = . (3.24) 2β I0 4αβ Substituting this expression into (3.21) and taking advantage of (3.23), we get after some simple algebra

Iex k2 1 + − 1 2β I0 (3.25) a nt τ =

. N0 k2 1 + IIex0 − 1 τ − 2β In relations (3.24) and (3.25), I0 = k 2 /4αβ represents a sort of characteristic excitation intensity governed exclusively by the material parameters. We now distinguish two excitation modes, weak excitation and strong excitation, characterized by the relations Iex I0 and Iex I0 , respectively.

Multiple processes present simultaneously (a) Weak√excitation (Iex I0 ). In this case we apply the familiar approximation 1 + x ≈ 1 + x/2 valid for x 1. From eqn (3.24) we then get n0 ≈

α Iex , k

IB = β n 20 =

α2 β 2 I . k 2 ex

(3.26)

Therefore, bimolecular luminescence varies quadratically with excitation intensity. From eqn (3.25), we have a ntτ ≈

α Iex N0 τ

− α Iex

,

a n t N0 ≈

N0 α Iex N0 − ατ Iex

(3.27)

and, ﬁnally, substituting the above relations into (3.23) yields, for the monomolecular luminescence, IM = α Iex ;

(3.28)

thus, IM increases linearly with the excitation. Unlike the situation when there is just a single active luminescence process in a semiconductor (Sections 3.2 and 3.3), the steady-state bimolecular and monomolecular luminescences now depend on the excitation intensity in a markedly different way: IB scales quadratically while IM scales linearly with excitation intensity. This corresponds to the intuitive and rather widespread scheme; we stress, however, that the necessary prerequisite is the parallel occurrence of both phenomena, which is sometimes overlooked just as the weak excitation condition. (Short-pulse excitation, discussed in Section 3.3, is another example of a quadratic demonstration of bimolecular recombination.) It is not difﬁcult to understand what goes on in our model material during weak excitation. Comparing (3.28) with the starting eqn (3.17), we see that basically all the absorbed energy α Iex is radiated in the form of monomolecular impurity luminescence. Thus, under weak excitation, bimolecular emission is substantially weaker than monomolecular emission (IB IM ), which makes sense since the density of the ‘optical’ electron–hole pairs is low and it is difﬁcult for the electrons and holes to ﬁnd one another to recombine. Almost all the photoelectrons are trapped at the impurity centres, which subsequently return to the ground state, emitting an extrinsic luminescence photon hνM ≈ E g –(E 1 + E 2 ). This enables us to formulate now the weak excitation condition alternative to the relationship Iex I0 . Under the circumstances, the low excitation intensity is physically equivalent to the fact that by far not all impurity atoms are brought into the excited state. In other words, the number of all available recombination impurity events, N0 /τ , is much larger than the density of photoexcitation events per second: N0 /τ α Iex . This, of course, then reduces relation (3.27) to the form a nt τ ≈

ατ Iex 1. N0

(3.29)

Indeed, neglecting ant τ as compared to unity in the denominator of eqn (3.23), we immediately obtain IM = N /τ ≈ ant N0 . This, considering (3.29) again yields IM ≈ (α Iex /N0 )N0 = α Iex , which is in accordance with (3.28).

93

94

Kinetic description of luminescence processes Therefore, inequality (3.29) is an alternative expression for the weak excitation condition. (b) Strong excitation. It appears beneﬁcial to formulate the strong excitation condition as a relation opposite to (3.29): ant τ 1. Equation (3.23) then immediately informs us of the monomolecular luminescence intensity IM =

a n t N0 a n t N0 N0 N = ≈ = . τ (1 + a n t τ ) a ntτ τ

(3.30)

This is clearly the maximum achievable intensity in the case when all impurity centres are excited. Its value no longer depends on the excitation intensity. Therefore, the extrinsic radiative recombination channel becomes saturated. What dependence of the bimolecular intrinsic luminescence on the excitation intensity do we get now? Using the strong excitation condition in the form Iex /I0 1, we obtain from eqn (3.24)

Iex k n0 = 2 β I0 or IB = β n 20 ≈

β k 2 Iex = α Iex . 4 β 2 I0

(3.31)

Hence, bimolecular luminescence increases linearly in the strong excitation limit and, in a sense, it basically swaps roles with monomolecular luminescence as can be seen by comparing with eqn (3.28). The overall behaviour of the system on a wide scale of excitation intensities is summarized by the plot in Fig. 3.7(a). We can formulate a system of kinetic equations analogous to eqns (3.17)– (3.19) for a large number of various luminescence centres and photocarrier trap levels. An example of a very successful model is the kinetic model of exciton and biexciton optical creation, which introduces, among other things, exactly the concept of ‘optical’ and ‘thermal’ excitons to explain the experimental data [4]. An older monograph by Antonov-Romanovskij [5] even attempts to cover the basis of all luminescence phenomena in semiconductors by making use of various combinations of unspeciﬁed radiative and non-radiative transitions and a large number of trapping levels. From today’s perspective, however, this approach appears obsolete. To conclude this section, a few more general notes may be in order. The kinetic approach to luminescence phenomena may be useful when analysing experimental data, in the sense that it is able to suggest a basic idea or a hint about what type the examined luminescence radiation might be. Here, both the character of the decay curve and the measured intensity dependence can help us. A speciﬁc model can give us a very good picture of the experimental

Multiple processes present simultaneously

95

Fig. 3.7 (a) A schematic intensity dependence of monomolecular (IM ) and bimolecular (IB ) luminescence for the model shown in Fig. 3.6. (Using the log-log scale, the plot of a linear function is a straight line with slope equal to 1, the plot of a quadratic function is a straight line with slope equal to 2.) (b) The intensity dependence of bimolecular luminescence (electron–hole intrinsic recombination, triangles) and monomolecular luminescence (localized impurity centre, circles) in InSb at temperature T = 4.2 K. Adapted from Mooradian and Fan [6]. Compare to panel (a).

results in a number of cases. For example, the basic features of the curves in Fig. 3.7(b), representing the intensity dependence of intrinsic and impurity low-temperature luminescence in InSb [6], are qualitatively absolutely identical to the attributes of our model curves from Fig. 3.7(a) (the quadratic dependence of intrinsic luminescence and the linear dependence of impurity luminescence in the case of weak excitation; a marked decrease in the slopes and possibly a tendency to saturation at high excitation intensities). On the other hand, we must not overestimate the signiﬁcance of kinetic equations. First of all, they contain no information about the spectral form of the individual luminescence lines. In addition, based on these equations alone we cannot usually draw unambiguous conclusions in the sense of a bilateral mathematical implication. For example, an experimentally established quadratic intensity dependence is evidence (if we disregard possible nonlinear optical phenomena and very high excitation effects) for the presence of a bimolecular recombination mechanism, yet the absence of such a

96

Kinetic description of luminescence processes dependence does not necessarily imply the absence of a bimolecular process— see Fig. 3.7(a) on the side of high excitation intensities. Finally, we must keep in mind that the effects of very high excitation accompanied by the bands ﬁlling (being reﬂected e.g. in spontaneous emission in an electron–hole system of high density, n 0 , p0 ≥ 1017 cm−3 , occurring for instance in LED operation or near the threshold condition of a semiconductor laser) may modify the formulation of the kinetic equations very substantially; e.g. the simple relation (3.10) is no longer valid, etc. [7]. After all, in the case of very high excitation, brand-new luminescence systems appear (they are discussed in Chapter 8), for which it often does not make much sense to distinguish mono- and bimolecular luminescence phenomena.

3.6 Problems 3/1: Show that even if we introduce quantum yields of monomolecular and bimolecular luminescence (η = τ/τr < 1, βr /(βr + βnr ) = (βr /β) < 1) into eqns (3.17)–(3.19), all the salient features of the model shown in Fig. 3.6 remain qualitatively preserved. 3/2: Check that for a monomolecular process we cannot (as against a bimolecular process) obtain a quadratic dependence of the luminescence response to the excitation intensity even if we excite the system by an arbitrarily short pulse tp τ , where τ is the luminescence decay time. 3/3: Prove that the solution to the equation dn/dt = –βn 2 –n/τ is a decay curve n(t) of the form n(t) =

n(0)e−t/τ . 1 + n(0) β τ (1 − e−t/τ )

Show that at later times after the excitation was turned off (when the density of the recombining photocarriers, n(t), has already dropped substantially) the total luminescence decay is governed by a sum of exponential curves. What condition must be satisﬁed for the decay to be described by a single exponential ∼ exp(–t/τ )? 3/4: Show that (a) the solution to eqn (3.10) is (3.13) and that (b) for long excitation pulses and after a transient initial increase in luminescence intensity, i(t), a steady-state value of intensity is established, which is in accord with (3.12). Plot the curve i(t), from the time we turn on the excitation until the emission intensity settles. 3/5: Discuss the kinetic model of exciton and biexciton creation according to [4].

References 1. Bebb, H. B. and Williams, E. W. (1972). Photoluminescence I. Theory. In Semiconductors and Semimetals (ed. R. K. Willardson and A. C. Beer), Vol. 8, p. 181. Academic Press, New York.

References 2. Rice, T. M. (1977). The electron-hole liquid in semiconductors: Theoretical aspects. In Solid State Physics (ed. H. Ehrenreich, F. Seitz, and D. Turnbull), Vol. 32, Chap. 1. Academic Press, New York. 3. Yu, P. Y. and Cardona, M. (1996). Fundamentals of Semiconductors. Springer, Berlin 4. Knox, R. S., Nikitine, S., and Mysyrowicz, A. (1969). Optics Comm., 1, 19. 5. Antonov-Romanovskij, V. V. (1966). Kinetics of photoluminescence of crystalline phosphors (in Russian: Kinetika fotoljuminescencii kristalofosforov). Nauka, Moskva. 6. Mooradian, A. and Fan, H. Y. (1966). Phys. Rev., 148, 873. 7. Bourdon, G., Robert, I., Sagnes, I., and Abram, I. (2002). J. Appl. Phys., 92, 6595.

97

Phonons and their participation in optical phenomena

4 4.1 Lattice vibrations—phonons

98

4.2 Electron–phonon and exciton–phonon interactions 103 4.3 Lattice vibrations associated with point defects 110 4.4 A localized optical centre in a solid matrix—the conﬁgurational coordinate model 112 4.5 The shape of absorption and emission spectra of a localized centre 116 4.6 Thermal quenching of luminescence

120

4.7 Problems

121

Optical and thus also luminescence transitions in a semiconductor occur primarily within its electron system originating from the outer electron shells of the atomic constituents of the crystal lattice. However, interaction of the system with atomic nuclei binding the inner shell electrons is by far no negligible in optical phenomena and reveals itself in a number of effects very easy to observe. This affects the shape of the absorption edge, the width of both the absorption and emission spectral lines, gives rise to their possible ﬁne structure, and it often results in thermal luminescence quenching, etc. In this chapter, we ﬁrst recap concisely the standard facts about crystal lattice vibrations, recalling the notion of phonons. Then we mention the microscopic mechanisms responsible for interactions of excited electronic states with semiconductor lattice vibrations, the so-called exciton–phonon interaction. Next, we point out the possible local vibrations of impurity atoms. Finally, we discuss a model of the interaction between a localized optical centre and lattice vibrations (the concept of conﬁgurational coordinate) and related effects and terms: the Franck–Condon principle, thermal luminescence quenching, the Huang–Rhys factor, and weak and strong interactions with lattice.

4.1 Lattice vibrations—phonons Atomic nuclei in a crystal keep oscillating around their equilibrium positions, determined by lattice point coordinates. The amplitudes of these oscillations rise with increasing temperature; however, they remain small compared to the lattice constant a at temperatures related to the luminescence processes (these range basically from the pumped liquid He temperature, about 1.5 K, up to room temperature of 295 K). In the simplest case of a one-dimensional crystal made of an inﬁnite chain of identical atoms of mass m, we can write the equation of motion in the form m x¨n = − f (xn − x n−1 ) − f (xn − xn+1 ),

(4.1)

Lattice vibrations—phonons

99

Fig. 4.1 (a) An inﬁnite one-dimensional chain of identical oscillating atoms, and (b) the corresponding dispersion relation ω = ω(k).

where xn is the instantaneous deﬂection of the nth atom from its equilibrium position (Fig. 4.1(a)). In (4.1), we only consider interactions of the nearest neighbours. As a further consequence of the small amplitude of the nuclei, we can use a harmonic approximation assuming, similarly to a harmonic oscillator, that the force restoring the nuclei to their equilibrium positions depends linearly on the instantaneous deﬂection with the force constant (or ‘spring constant’) f . It is natural to look for a solution to eqn (4.1) in the form of a wave of frequency ω, running along the chain [1, 2] x n = A eiω(t−na/cs ) = A ei(ωt−kna) ,

(4.2)

where cs = cs (ω) is the velocity of the wave motion, k = |k| = ω/cs is the magnitude of the corresponding wavevector k, and A is the amplitude of the vibrations. Similarly to other cases in wave mechanics, we are interested in the so-called dispersion relation for the given system, i.e. the dependence ω = ω(k). We obtain it simply by substituting (4.2) into (4.1); the result is plotted in Fig. 4.1(b). Here, several facts are worth mentioning. (a) ω = ω(k) ≡ ωk is a periodic function of k and hence it is enough to consider the range k ∈ (–π/a, π/a) only, which is nothing but the ﬁrst Brillouin zone that we encounter, in complete analogy, with the electron band structure of semiconductors. (b) There is a maximum oscillation frequency, ωmax , at which the vibrations can still propagate along the chain. It follows from the solution to eqn (4.1) that ωmax = 2( f /m)1/2 . This is markedly different from a continuum (represented by an oscillating string) where no such restriction on the transmitted frequency occurs. (c) Near the centre of the Brillouin zone (k = 0), i.e. for k π/a, the dispersion relation becomes almost linear: ωk = cs k. This can be easily understood. If, for k π/a, we write the wavevector as k = 2π/λ and combine both expressions, we get the condition λ a, which means that the discrete chain structure vanishes in comparison to the wavelength.

100

Phonons in optical phenomena Therefore, we are in a continuum-type situation for which, as is well known, a linear dependence governs the relationship between ω and k with cs denoting the speed of sound. Regarding the mechanical wave motion discussed above, we can introduce quantization, which is to a large extent analogous to the quantization of an oscillating electromagnetic ﬁeld. If we restrict, as a certain approximation to reality, the number of atoms in the chain to a large but ﬁnite number, N , we can view the chain, regarding the energy, as an ensemble of N harmonic oscillators. The mean energy of a quantized harmonic oscillator ε¯ at a given temperature T is given by the expression that constitutes part of Planck’s blackbody radiation law ε¯ =

h¯ ωk . eh¯ ωk /kB T − 1

(4.3)

Here, kB denotes the Boltzmann constant. Thus, the energy of the entire onedimensional crystal will be E¯ = N ε¯ =

N h¯ ωk . −1

eh¯ ωk /kB T

(4.4)

We can now grasp expression (4.4) as stating that the total vibrational energy of the one-dimensional crystal is given by the sum of the energies of Nk quasiparticles, when Nk =

E¯ N = h ω /k T ; e¯ k B − 1 h¯ ωk

(4.5)

we assign energy h¯ ωk to every quasi-particle. We call these quasi-particles— quanta of the vibrational energy of a solid—phonons.According to statistical physics, the statistical distribution (the distribution function) of the phonons is deﬁned as the mean number of phonons in one quantum state. For a linear chain of N oscillating atoms, the number of allowed quantum states is equal to N [1], hence, from (4.5) we obtain for the phonon distribution function nk =

Nk 1 = h ω /k T . N e¯ k B − 1

(4.6)

Various vibrationally excited states of the crystal are characterized by different values of n k or, in other words, each vibrational state of the lattice can be described as a state of a perfect gas of non-interacting particles—phonons. Equation (4.6) tells us that the phonons are subject to Bose–Einstein statistics and that the chemical potential of an ensemble of phonons is equal to zero. It also follows from the same equation that the phonon population depends very strongly on temperature T —as the temperature drops, the phonon population decays quickly. The analogy to the quanta of electromagnetic radiation—photons—is rather obvious; it is, however, important to realize there is a certain difference. The expression hν for the energy of photons holds exactly, while hωk for the phonons only holds in the harmonic approximation. With large amplitudes of atomic vibrations, we can no longer apply the harmonic approximation

Lattice vibrations—phonons and phonons can undergo mutual interactions. There are well-known macroscopically observable effects that cannot be explained within the context of harmonic oscillations of the lattice (e.g. the thermal expansion of solids). Although the one-dimensional chain of identical atoms provides us with the basic concept of the phonon, it cannot encompass the full reality of a three-dimensional crystal. It is astonishing, however, that it sufﬁces to modify the one-dimensional model just slightly to be able to represent all the basic features of vibrations in a three-dimensional crystal. This modiﬁcation consists in introducing two kinds of atoms into the chain as shown in Fig. 4.2(a). We denote their masses by m and M (m < M). The lattice constant is then equal to 2a and there are two atoms per unit cell. Using an approach analogous to the previous case of identical atoms, we can formulate equations of motion for both kinds of atoms and, by solving them, we can obtain the dispersion relations shown in Fig. 4.2(b). The most important new feature as compared to Fig. 4.1 is the fact that there are now two branches of phonons separated by a frequency gap.1 The lower branch, called the acoustic branch, is characterized by the relation lim ω(k) = 0 while on the boundary of the Brillouin zone, k→0

(a)

it has its maximum value of ω max = (2 f /M)1/2 . On the contrary, the upper branch, called the optical branch, has the highest allowed frequency in the (o) centre of the Brillouin zone (equal to ωmax = [2 f (1/m + 1/M)]1/2 ) and the magnitude of the optical frequency gently decreases towards the boundary of (o) the zone k = ±π/2a where it reaches the value of ωmin = (2 f /m)1/2 . Therefore, we speak of optical and acoustic vibrations or phonons. From the microscopic perspective, the difference between them consists in the fact that—as can be easily shown based on the equations of motion [1, 2]—light and heavy atoms move in counter-phase during optical vibrations, see also Fig. 4.5 below, while for acoustic vibrations both kinds of atoms vibrate in phase. In this case, however, even the centre of mass in each cell moves and there is a deformation wave of ‘compression and expansion’ travelling through the crystal, as for sound propagation. Conversely, optical vibrations— just due to the atoms moving in counter-phase—leave the centre of mass of (o) the unit cell at rest, which allows for a non-zero frequency ωmax even at k = 0. The name ‘optical vibrations’ stems from the fact that if there are two kinds of atoms of opposite charge per unit cell (a partially ionic bond), then the counterphase motion means electric dipole oscillations, which can also be excited by resonance absorption of photons from the mid-infrared region. Besides explaining the fundamental difference between the optical and acoustic vibrations, Fig. 4.2 shows several other facts that are worth emphasizing because of their importance in optical and, particularly, in luminescence phenomena: (a) Near the ﬁrst Brillouin zone boundary (k = ±π/2a), both phonon branches are basically dispersionless, i.e. dω/dk ≈ 0. 1 Again, we can perceive a certain similarity to the electron energy band structure in semiconductors: the existence of allowed energy (frequency) bands and gaps. This is the common characteristic feature of waves propagating in periodic structures.

101

Fig. 4.2 (a) A one-dimensional chain with two kinds of oscillating atoms of masses M and m (M > m); (b) the corresponding dispersion relations ω = ω(k).

102

Phonons in optical phenomena (b) Near the Brillouin zone centre (k = 0), the optical branch reveals itself dispersionless while the acoustic branch has its highest dispersion here. (c) Figure 4.2 considers only atomic oscillations along the chain axis. These are the so-called longitudinal vibrations. In addition to these, however, there are also transverse vibrations when the atoms move perpendicularly to the chain. (Yet, in both cases, the vector k points in the same direction, that is, along the chain.) Therefore, we speak of transverse acoustic (TA), longitudinal acoustic (LA), transverse optical (TO) and longitudinal optical (LO) phonons. Up to this point, we have explored only the single dimension of the linear model. It turns out that in a real three-dimensional crystal, the concept of TA-, LA-, TO-, and LO-phonons remains fully valid, but the phonon dispersion curves acquire somewhat more variable forms as against Fig. 4.2, due to numerous vibrational waves travelling through the crystal lattice in various directions featuring different electron cloud densities, different effective spring constants, etc. An example of actual phonon dispersion curves in a particular semiconductor—crystalline silicon—is shown in Fig. 4.3 [3]. Such curves are most often obtained using inelastic scattering of neutrons as they interact with phonons in various directions within a crystalline sample. These then correspond to different directions of k in the Brillouin zone. Generally, in the three-dimensional case, if a crystal has n atoms per unit cell then there are exactly 3 types of acoustic vibrations characterized by the condition lim ω(k) = 0, and 3n-3 types of optical vibrations with ω(k) = 0 for k→0

k = 0. The transverse vibrations may be doubly degenerate; the degeneration is generally removed in an anisotropic medium. As regards Fig. 4.3, let us ﬁrstly notice that the typical phonon energy in a semiconductor is of the order of 10 meV. It is further interesting to realize that in silicon the gap between the optical and acoustic branches disappears in a certain direction in the Brillouin zone. This is due to the fact that there are two Si atoms per unit cell in the silicon (diamond) structure, and the atoms— naturally—have the same mass. According to Fig. 4.2(b), the acoustic and

Fig. 4.3 Phonon dispersion curves of crystalline silicon in the principal directions of the Brillouin zone at room temperature. The reduced wavevector is plotted in units of ζ = ka/2π, where a is the lattice constant. Adapted from Dargys and Kundrotas [3].

Electron–phonon and exciton–phonon interactions optical curves indeed coincide for m = M at the boundary of the Brillouin zone.2 Finally, a remark on the terminology: Despite their name, acoustic phonons can participate in optical processes in a crystalline solid just like the optical phonons do! For instance, at the onset of the optical absorption edge in a semiconductor with an indirect bandgap (Si, Ge, AgBr), the type of phonons ensuring the quasi-momentum conservation law is determined by selection rules following from the symmetry of lattice vibrations, the symmetry of electron wavefunctions, and the symmetry of the corresponding matrix elements. Luminescence processes in these semiconductors are in a fully analogous situation (Subsection 7.1.4). Primarily, it is thus not of crucial importance whether the phonons are optical or acoustic. However, each of these phonon types may have a different mechanism of interaction with excited electronic states; these mechanisms are brieﬂy treated in Section 4.2.

4.2 Electron–phonon and exciton–phonon interactions In the preceding section, we dealt with phonons as with an isolated system. However, phonon participation in optical processes naturally requires interaction with the system of electrons responsible for the optical properties, which are basically the electrons occupying energy levels in the valence or possibly conduction band. In that case, we speak of the so-called electron–phonon interaction. Clearly, we can expect a similar type of interaction also in case the semiconductor electronic system is in an excited state and returns to the ground state, the phonon system thus participating in emission of luminescence radiation. We shall be primarily interested in this process. If, in this respect, we call the excited electronic system of the crystal an ‘exciton’ then we may call the corresponding interaction an exciton–phonon interaction. We shall discuss a somewhat more detailed view of the exciton–phonon and electron–phonon interactions in an excited semiconductor in Subsection 7.2.4.3 The following example [4] is a clear illustration of how we can imagine the charge carriers may inﬂuence the lattice vibrations. Let us consider a charge, 2 One might then ask whether it actually makes any sense to speak of acoustic and optical vibrations in silicon if the lattice is made up of a single kind of atom. Yes, it does make sense, exactly because there are two atoms per unit cell. Then n = 2 and we have exactly three acoustic and 3n–3 = 3 optical vibration branches. Although the optical branches cannot be excited by infrared radiation here as the bond is fully covalent, this requirement is not a condition necessary to call the lattice vibrations optical. 3 The original meaning of the word ‘exciton’ in a semiconductor was clearly speciﬁed and strictly deﬁned (Wannier, G. H. (1937). Phys. Rev., 52, 191; Elliot, R. J. (1957). Phys. Rev., 108, 1384; Nikitine, S. (1959). Phil. Magazine, 4, 1) as the lowest excited electronic state of a perfect, pure crystal that can propagate freely through the lattice and transfer excitation energy (not electric charge). We shall discuss this quasi-particle, also called a Wannier ‘free exciton’, in connection with its important role in luminescence properties of semiconductors in Chapter 7. At a later time, the term exciton relaxed substantially from its rigour and, at present, it is used rather loosely also to denote an arbitrary bound electron–hole pair generated by light (e.g. an excited state of an impurity atom, a localized electronic excitation in an amorphous material, an electron–hole pair in a semiconductor nanocrystal, and suchlike).

103

104

Phonons in optical phenomena whether bound or free, in a harmonically oscillating lattice made up of two kinds of ions (an ionic crystal or a semiconductor with an ionic contribution to the lattice binding energy). We shall focus on a single mode of these vibrations and we shall write its total energy (in the absence of charge that would introduce interactions) in the well-known form W0 =

1 ˙2 1 m Q + f Q2, 2 2

(4.7)

where Q is the normal coordinate and ( f /m)1/2 denotes the angular frequency of the mode. Now we insert a charge into the lattice, which, due to Coulomb forces, introduces an additional term, –FQ, into (4.7), where F is the force the charge exerts on the mode. Here, we neglect higher-order terms in Q and, likewise, a possible change of the spring constant, f , due to the inserted charge. Hence, the total energy is then equal to W = W0 − F Q, which, after introducing a new coordinate Q˜ = Q − F/ f , can be rewritten in the form W =

1 ˙˜ 2 1 ˜ 2 1 F 2 mQ + f Q − . 2 2 2 f

Physically, this means a shift of the oscillator vibrations to a new equilibrium position Q 0 = F/ f accompanied by the release of relaxation energy WR = F 2 /2 f , as shown in Fig. 4.4. On the whole, there are three main microscopic mechanisms mediating the electron–phonon and exciton–phonon interactions: the deformation potential, the piezoelectric mechanism, and the Fr¨ohlich mechanism. The deformation potential The energy of an electron and a hole, and thus also that of an exciton, is a sensitive function of the interatomic distance in the crystal lattice. It is well known that, for example, a deformation caused by an external force changes the bandgap value of a semiconductor. We can thus expect a similar effect to occur also due to crystal lattice vibrations. The simplest picture corresponds to long-wavelength, longitudinal acoustic vibrations when atomic displacements parallel to the direction of wave propagation occur, inducing periodic expansions and compressions of the medium on a macroscopic distance. These

Fig. 4.4 The parabolic potential energy of harmonic oscillations in an ionic lattice, f Q 2 /2, together with the linear coupling to the inserted electric charge (–FQ) result in a shift of the parabolic curve to a new equilibrium position, Q 0 , and release of relaxation energy, WR . According to Hayes and Stoneham [4].

Electron–phonon and exciton–phonon interactions can be expressed using the relative change in the volume of a sample, δV /V . The relative change then yields a shift in the extreme of the electron energy band δ E kn (k denotes the electron wavevector, n indexes the band). To a ﬁrst approximation, the dependence reads [5] δE k n = a(k, n) (δV /V ),

(4.8)

where a(k, n) is the volume deformation potential of the energy level E kn . It follows from this equation that the deformation potential has the dimension of energy and it is measured in eV. However, it is neither simple to calculate such a (absolute) deformation potential theoretically nor to determine it experimentally. It is much easier to establish the difference between deformation potentials of two energy levels (the relative deformation potential). One of the commonly used experimental techniques is an optical measurement performed under external hydrostatic pressure applied to the sample. This determines the energy difference in optical transitions near the onset of the absorption edge, that is, near the extremes of the valence and conduction bands. To illustrate the situation, Table 4.1 gives the values of the relative deformation potential between extremes of the valence and conduction bands at the point (k = 0) of the ﬁrst Brillouin zone. In semiconductors with a direct bandgap, this energy difference corresponds to the onset of an interband absorption edge; in semiconductors with an indirect bandgap (Si, GaP, AgBr), we in addition need to consider the deformation potential at the relevant points at the boundary of the ﬁrst Brillouin zone. Table 4.1 thus also lists the available values of two absolute deformation potentials u and d , necessary to describe the energy shift according to the generalized relation (4.8) at the point = [k/kmax , 0, 0] in the direction [100], where the conduction band minima are located in silicon and GaP. Based on the data in Table 4.1, we can infer the following facts as regards the electron–phonon interaction. Values of the relative deformation potential given in the table decrease slightly with increasing bond ionicity, i.e. from Si towards AgBr; nevertheless, the dependence is weak and all the deformation potential values are of the same order. Therefore, this electron–phonon Table 4.1 Deformation potentials for extremes of conduction and valence bands in selected semiconductors. The symbols a(1c )–a(15v ) or possibly a(15c )–a( 25v ) denote the relative volume deformation potential for the lowest minimum of the conduction band and the highest maximum of the valence band at the point (k = 0). d and u denote deformation potentials at the minimum of the conduction band in Si and GaP. The volume deformation potential along the [100] direction in the Brillouin zone of silicon is equal to (d + u ). Most data adopted from Yu and Cardona [5]. Values are given in eV. a(1c ) – a(15v ) Si GaP GaAs ZnS ZnSe CdTe AgBr

–9.3 –9 –4 –5.4 –3.4 –2.31

a(15c ) – a( 25v )

d

–10

5

u 8.77 13

105

106

Phonons in optical phenomena interaction mechanism has roughly the same efﬁciency in all semiconductors. Important from the luminescence point of view is that, in addition to mediating the coupling between electrons or excitons and the acoustic phonon ﬁeld that we have mentioned several times already, both the magnitude and sign of the deformation potential have an immediate impact also on the behaviour of luminescence in semiconductors subject to a static mechanical deformation. In this sense, we must understand the data in Table 4.1 as follows. A negative value of the relative deformation potential a(1c ) – a(15v ) means that in hydrostatic pressure experiments (δV /V < 0), the energy separation (1c ) – (15v ), i.e. the width of the bandgap, E g , becomes larger according to (4.8). This means that, as the pressure increases in these experiments, semiconductors with a direct bandgap will show a shift in the wavelength of edge emission luminescence lines towards lower values (a ‘blue-shift’). Experiments conﬁrm this. For indirect semiconductors Si and GaP, Table 4.1 gives positive signs of the deformation potentials at the minimum of the conduction band. As the values of the deformation potential at the conduction band edge commonly turn out to be about one order of magnitude larger than at the valence band maximum, the values shown here deﬁne the character of the indirect bandgap shift and thus also that of the edge emission in Si and GaP; the applied hydrostatic pressure causes a red-shift in the edge emission here. It should be emphasized that the account given above was considerably simpliﬁed and only applies to the long-wavelength longitudinal acoustic phonons. A more detailed discussion of the deformation potentials—additionally including also anisotropic uniaxial deformation of the crystal (or shear deformation of the TA-phonons), which lifts the degeneracy of the conduction band minima in reciprocal space of Si and Ge crystals, and the participation of short-wavelength phonons near the ﬁrst Brillouin zone boundary in optical transitions in Si, Ge, and AgBr—can be found in [5]. An important note: The deformation potential mechanism may be partially related to optical phonons as well, particularly the long-wavelength ones (k π/a). These phonons from around the centre of the Brillouin zone can also induce band edge shifts due to a relation analogous to (4.8) because a relative displacement of two ions in the unit cell induces on macroscopic distances a quickly changing local deformation (Fig. 4.5(a)), which the electron system can feel as well. The exciton–phonon interaction due to the deformation potential occurs in all crystalline solids. The piezoelectric mechanism In materials of lower lattice symmetry, an electric voltage associated with a macroscopic electric ﬁeld inside the material may develop, in particular between opposite sample surfaces under mechanical deformation; this is known as the piezoelectric effect. The same mechanism of generating an electric ﬁeld also works in the case of deformations varying in time and resulting from the relative shift between adjacent atomic layers; that is, most

Electron–phonon and exciton–phonon interactions

107 Fig. 4.5 (a) A long-wavelength TO vibration with a rather strong local deformation between adjacent atoms oscillating in counter-phase with large amplitude. (b) In a cubic crystal with the rock salt structure (e.g. AgBr), planes occupied only by positive ions alternate with planes of negative ions perpendicular to the [111] direction. LO vibrations then represent a vibrating capacitor with a constant charge but varying plate separation. This produces a varying macroscopic electric ﬁeld along the wave propagation direction k || [111]. TO vibrations do not possess this property. We can also imagine an analogous situation to occur in type II-VI and III-V semiconductors with partially ionic bonds.

importantly again in the case of longitudinal acoustic modes of lattice vibrations. The piezoelectric potential ΦPE , describing the generated electric ﬁeld, then changes the energy of a carrier of charge q, an electron or a hole, by the quantity qΦPE ; this is the essence of this electron–phonon coupling. Although the exciton, as a bound electron–hole pair, is electrically neutral, it is affected by the electric ﬁeld, too, as the ﬁeld modulates its energy levels and binding energy. Since the piezoelectric electron–phonon interaction is underlain by (long-range) Coulomb forces, the interaction is strongest for phonons with a small wavevector k (long wavelength), that is, for long-wavelength LA-phonons again. This exciton–phonon interaction only occurs in crystals whose crystallographic point group does not contain the centre of inversion (in semiconducting materials, these are particularly the point groups Td and C6v that govern the crystal structure of the following materials showing signiﬁcant luminescence: GaAs, GaP, GaN, CdS, CdSe, ZnO, ZnS, and ZnTe). It can be rather easily screened by free carriers and it is thus relatively weak; nonetheless, it is stronger than the deformation potential mechanism. The Fr¨ohlich mechanism This is the most important exciton–phonon interaction. However, it only occurs in ionic crystals and in semiconductors with an ionic contribution to the lattice energy (also called polar semiconductors); it is thus completely absent in elemental semiconductors like Ge and Si. Its principle consists in the fact that, due to the opposite orientation of oscillations by oppositely charged ions, longwavelength LO-phonons induce in the vibrating crystal lattice a long-range macroscopic electric ﬁeld along the direction of the wavevector k (Fig. 4.5(b)). This ﬁeld—or equivalently the macroscopic crystal polarization—again enters the Coulomb interaction with charge carriers or excitons. It is worth mentioning that TO-phonons do not produce similar crystal polarization and thus the energy of long-wavelength LO-phonons (i.e. phonons in the neighbourhood of

108 Fig. 4.6 Phonon dispersion curves in a polar semiconductor AgBr at T = 4.4 K. The reduced wavevector is plotted in units of ζ = ka/2π, where a is the lattice constant. Symbols denote experimental points from neutron diffraction measurements, and lines represent the theoretical model. Symmetries of the individual phonon branches are marked by the irreducible representations of the corresponding point groups. It is particularly worth noting that at the point (k = 0), the LO-phonon energy is greater than the TO-phonon energy, which is common behaviour in polar semiconductors. Besides, however, the plot also shows some unexpected features. At the Lpoint, the energy of the TO-phonon L 3 (TO) is lower than the energy of the LA-phonon L 1 (LA) which contradicts the simple Fig. 4.2. This basically means that the heavier ions M(Ag+ ) oscillate with a higher frequency here than the lighter ones m (Br− ). This can only be explained by the effective force constants, f , being considerably different for both modes. This and related effects are discussed in more detail in Problem 4/4. The irreducible representation notation at the L point holds for a negative ion (Br− ) at the origin of coordinates. Adapted from Song and Williams [6].

Phonons in optical phenomena

k = 0) in a polar lattice is always greater than that of TO-phonons, as illustrated, for example, by Fig. 4.6 for AgBr [6]. The Fr¨ohlich mechanism can be well quantiﬁed using the so-called polaron coupling constant α. An electric charge in an ionic lattice polarizes its neighbourhood. The polarization involves two components: electronic and ionic. The potential at a distance r from a point charge e is screened by the dielectric constant. The electronic polarization component (the shift of the electron cloud with respect to the nuclei) and the ionic component (the shift of ions from their equilibrium positions) are jointly associated with a static dielectric constant, εs , that adequately describes screening at low ﬁeld frequencies. The potential energy at a distance r from a point charge then reads 1 e2 4πε0 εs r where ε0 is the dielectric constant or permittivity of free space. Electric ﬁeld screening by the electronic component of the lattice constituents alone is described by a high-frequency or optical dielectric constant ε∞ (< εs ) and leads to the potential energy e2 1 . 4πε0 ε∞ r Ionic polarization itself, which is due to the relative motion of anions and cations (representing the mass of the vibrating lattice), is then characterized by the difference e2 1 1 . − 4πε0 r ε∞ εs −1 − ε −1 ) is a crucial factor for the description of the Fr¨ Obviously, (ε∞ ohlich s mechanism of electron–phonon and exciton–phonon interactions. In practice, one introduces the above-mentioned dimensionless coupling constant α in the form [7]

Electron–phonon and exciton–phonon interactions α=

e2 1 −1 (ε∞ − εs−1 ) . h¯ ωLO 8 πε0 rp

(4.9)

In (4.9), rp = h¯ / 2m p h¯ ωLO stands for the so-called polaron radius. By the polaron term we denote a quasi-particle—an electron or a hole of mass m p — that polarizes and thus locally deforms the ionic lattice as it propagates through it. This manifests itself in an increased mass of the electron or hole—as if they ‘pulled’ along the polarized surrounding lattice that slows them down in their motion. (We speak of an electron–polaron with a coupling constant αe and of a hole–polaron with a constant αh .) Thus, the effective polaron mass, m p , is always larger than the effective mass of a ‘bare’ quasi-particle. The radius rp denotes the very size of the polarization-deformed lattice region around the charge carrier—the polaron; this is basically of the same magnitude in all polar crystals (rp ≈ 1–1.5 nm). The crucial factor when characterizing the Fr¨ohlich interaction using (4.9) is thus the value of the coupling constant, quoted for selected semiconductors in Table 4.2. As expected, the values of αe , αh increase with the fraction of bond ionicity (from homopolar semiconductors Ge, Si towards type I-VII semiconductors). Therefore, we can expect the strongest Fr¨ohlich electron–phonon coupling, i.e. polaron effects, in silver halides AgBr, AgCl and in thallous halides. Experimental results conﬁrm this reﬂection. However, in the case of the exciton–phonon coupling, the situation becomes somewhat different. It is expected that the exciton–phonon interaction will become stronger here, like in the case of the deformation mechanism, with increasing radius of the Wannier exciton ax . (We can infer this on the basis of an analogy between the Wannier exciton and a free atom— the polarizability of an atom increases with its radius.) The exciton Bohr radius decreases, although not completely monotonically, with increasing bandgap E g , as we shall discuss in Chapter 7. Thus, what comes into play here is not only the coupling constant α abut also the last column in Table 4.2. It turns out that the most prominent effects of the exciton–phonon coupling can be Table 4.2 Polaron coupling constants αe (electron–polaron), αh (hole–polaron), and the bandgap width, E g , in selected crystalline semiconductors; (i) denotes the indirect bandgap. αe

Semiconductor Ge Si GaAs GaP GaN CdTe CdSe CdS ZnS AgBr AgCl TlBr

0 0

III-V

II-VI

I-VII

αh 0 0

E g (eV) (i) 0.745 (T = 0 K) (i) 1.17 (T = 0 K)

0.03 0.13 0.4–0.5

1.519 (T = 0 K) (i) 2.35 (T = 0 K) 3.49 (T = 0 K)

0.39 0.46 0.65 0.71

1.606 (T = 4.2 K) 1.829 (T = 80 K) 2.583 (T = 4.2 K) 3.78 (T = 19 K)

1.6 1.86 2.05

2.8 – 3.2

(i) 2.7 (T = 4.2 K) (i) 3.3 (T = 4.2 K) (i) 2.663 (T = 4.2 K)

109

110

Phonons in optical phenomena observed in the luminescence of some II-VI compounds, in particular CdS. This is also partially due to the fact that the piezoelectric interaction here joins the Fr¨ohlich interaction.

4.3 Lattice vibrations associated with point defects In our considerations of phonons and their interactions with charge carriers we had, until now, always had in mind a perfect, pure crystal lattice without impurities and defects. However, we have already emphasized several times that a number of solid-state luminescence processes, very important as regards their application, are conditioned just by the presence of atomic-type impurities. It is thus in order to attempt to analyse now the inﬂuence of point defects in the crystal lattice on its vibrational properties [4]. Let us ﬁrst clarify the differences in approaches used to describe perfect crystal vibrations and those of a crystal containing point defects. Firstly, as we have seen in Section 4.1, the vibrational modes of a perfect, defect-free crystal are characterized by the wavevector k. Secondly, these modes are fully delocalized due to the translational symmetry of the lattice. This means that, knowing the oscillation amplitude in a certain part of the crystal, we ﬁnd the same oscillation amplitude—without being enhanced or damped—in any other macroscopically separated region. We usually assume that the imperfect lattice of crystals containing point defects retains its harmonic character of vibrations and hence we may speak of its vibrational modes and phonons. Yet, we may no longer use the term wavevector and employ fully the concept of the translational symmetry of the lattice. The amplitude of the vibrational mode will be generally different in different sections of the crystal. Let us now assume that the lattice contains a single point defect, e.g. an impurity atom of mass M’ different from the masses of atoms or ions constituting the host crystal. One can imagine three different types of vibrational modes. 1. Certain crystal vibrational modes may happen not to be affected by the presence of the defect at all. If the defect atom indeed only has a different mass M as we assumed and the harmonic force (‘spring’) constant, f , remains unchanged in its neighbourhood, then the modes with a node located at the impurity atom will not feel the presence of the defect. This is because the different mass will stay at rest (Fig. 4.7(a)). 2. The second type of mode can be called a resonance mode. If the mass M is large (a heavy impurity atom) or the force constant f in the neighbourhood of the impurity decreases due to a different type of interatomic bond ( f < f ), or possibly if both effects are present simultaneously, then there appears a mode of a rather low frequency ωR = ( f /M )1/2 (Fig. 4.7(b)). The frequency ωR is usually situated within the band of allowed phonon frequencies of the unperturbed lattice and a resonance transfer of vibrational energy from the unperturbed area leads to an ampliﬁcation of the local

Lattice vibrations associated with point defects

111

Fig. 4.7 Various types of localized vibrations of impurity atoms for the one-dimensional case: (a) an unaffected mode of the basic lattice; (b) a low-frequency resonance mode; (c) a local mode in superposition with the basic lattice mode; (d) a schematic picture of the defect modes in the energy band scheme of phonon branches.

amplitude as compared to the amplitude of vibrations in areas far away from the defect atom; hence the name resonance mode. 3. The third type of mode occurs in the neighbourhood of an impurity atom, the mass M of which is lower than the masses of atoms in the unperturbed crystal (speciﬁcally, e.g. M < M, M < m for a two-atom chain), and the neighbouring force constant f is high, f > f . The frequency of such a mode ωL = ( f /M )1/2 is then located above the highest allowed frequency of perfect lattice vibrations ωmax . It is clear that the resonance energy transfer cannot occur here and the amplitude of such a mode decreases rather quickly away from the defect; the mode is called a local mode (Fig. 4.7(c)). An analogous type of defect vibration can also occur (for various ratios of the values f , f , M , M, and m) within the frequency gap between the acoustic and optical phonon branches. We can call this a gap mode. The frequency position of the modes discussed above in the band scheme of phonon energies is shown in Fig. 4.7(d). It remains to assess the degree of localization of the modes under discussion in a quantitative way, if possible. The mean quadratic value of the oscillation amplitude of a given atom, in a given mode, and how this quantity varies with the distance from an impurity atom, suggest themselves to be suitable parameters. Let us assume there are N atoms oscillating in this mode, with the same amplitudes u. The potential energy V of N oscillating atoms in the

112

Phonons in optical phenomena Table 4.3 Oscillation amplitude u 2 1/2 of various types of modes. Mode Perfect crystal mode Resonance mode Local mode

Close to a defect

Far from a defect

−1/2

∼ N∞ −1/2 ∼ NL −1/2 ∼ NL

−1/2

∼ N∞ −1/2 ∼ N∞ 0

Figure 4.7(a) 4.7(b) 4.7(c)

harmonic approximation is, expressed classically, equal to V = N f u 2 /2. At the same time, the total energy of a quantum harmonic oscillator (representing a given mode) is equal to 2V and is given by relation (4.3), independent of N . Even if we add to it the zero-point energy hω/2 (which is not included in (4.3)), we obtain 2V =

h¯ ω 1 h¯ ω coth , 2 2kB T

(4.10)

which is fully determined by the frequency ω and temperature T and is also independent of N . The only option to comply with the requirement that√the expression (Nfu2 /2) be independent of N is thus the scaling u 2 1/2 ∼ 1/ N . This then supplies us with information on the localization of various modes. If we denote by N∞ the number of atoms in the host crystal and if the point defect affects the oscillation amplitude of NL atoms in its neighbourhood then the relative values of the root mean square u 2 1/2 are given in Table 4.3. Finally, let us note that the defect-induced vibrations modify the selection rules for infrared and Raman spectroscopy. Translational symmetry of the unperturbed crystal leads to the quasi-momentum conservation law and only optical phonons around k ∼ 0 are active in infrared spectra and Raman scattering. The presence of a defect breaks the symmetry and, therefore, modes from almost the entire Brillouin zone (with frequencies from the allowed bands) can participate in infrared and Raman experiments. At the same time, the presence of the defect itself does not appear much in the resulting spectra; they reﬂect primarily the phonon density of states of the perfect host crystal. The typical impurity concentrations to which we can apply the approximation of a single isolated defect discussed above (without the need to consider defect pairs or even clusters) are of the order of 1000 ppm and less. This complies fully with the requirements for extrinsic luminescence in semiconductors, which is characterized by impurity concentrations mostly within the range 10 ppb–100 ppm.

4.4 A localized optical centre in a solid matrix—the conﬁgurational coordinate model In the present section, we shall continue investigating the properties of a point defect (an impurity atom) in a solid. However, we shall now be primarily interested in the electronic properties of such an impurity centre related to its optical excitation and subsequent radiative transition to the ground state—

A localized optical centre in a solid matrix

113

the extrinsic luminescence.4 In Section 3.2 we gave such an optically active area in a solid the name of a localized luminescence centre, in order to distinguish the phenomenon from a process where emission of a luminescence photon is connected with quasi-particles moving freely through the matrix or crystal lattice (e.g. radiative recombination of a free electron–hole pair). We now introduce the concept of a conﬁgurational coordinate, which will enable us to understand how an excited luminescence centre enters into interaction with the defect modes of lattice vibrations in its neighbourhood, how the exciton–phonon interaction affects the shape of the optical spectra, and how this interaction can be quantiﬁed using optical measurements. Let us consider an impurity atom of mass Mp embedded in a host solid; the simplest case of a one-dimensional chain with a single type of atom is shown in Fig. 4.8(a). Such a defect, as we know, leads to a distortion in the equilibrium positions of the nearest neighbours—the host atoms of mass m = Mp . Let the defect be in its ground electronic state. Let us denote by Q g0 the equilibrium distance between the impurity and its nearest neighbours of

Fig. 4.8 (a) A one-dimensional chain of atoms (‘matrix’) containing an optically active impurity atom of mass Mp . (b) Energy of the ground (g) and excited (e) electronic states of a localized centre as a function of the conﬁgurational coordinate Q for the Huang–Rhys factor S = 2. (c) Schematic of the origin of optical absorption and luminescence spectra within the framework of the Franck–Condon principle at T = 0K . INP and IPW denote the integral intensities of a no-phonon line and a phonon wing, respectively.

4 In certain cases, the formalism discussed here can also be applied to intrinsic processes (see Problem 7/4 or the luminescence of pure AgCl in Subsection 7.2.4).

114

Phonons in optical phenomena mass m; this distance generally differs from the unperturbed ‘lattice constant’ a, occurring sufﬁciently far away from the defect. The impurity atoms, just like the host atoms, oscillate around their equilibrium positions at any temperature and (assuming harmonic oscillations) we can write for the total energy of the oscillating impurity E g = E g0 +

1 f g (Q − Q g0 )2 . 2

(4.11)

Here f g is the effective force constant determining the oscillation frequency ωg = ( f g /Mp )1/2 , and (Q–Q g0 ) represents the instantaneous displacement from the equilibrium position Q g0 . We shall call Q a conﬁgurational coordinate and the overall situation is presented in Fig. 4.8(b). The diagram also shows the quantum-mechanical energy levels of a harmonic oscillator, represented by the oscillating atom Mp , as being equidistant with spacing hωg . Let us remind ourselves that the quantum-mechanical probability of ﬁnding the harmonic oscillator in one of these vibronic levels reaches its highest value at the classical turning points where the corresponding vibronic level intersects the parabolic curve. Figure 4.8(b) shows this schematically, plotting the square of the modulus of the wavefunction (shaded curves). The ground vibrational state of energy hωg /2 is an exception to this rule, with its occurrence probability highest for Q = Q g0 (point A). Let us now imagine the impurity atom in an excited electronic state. The classical picture is as follows: one of the valence electrons jumps to a higher energy level with a larger orbital radius; this means that the effective atom radius increases and the excited atomic ‘pushes’ away its nearest neighbours somewhat further off. The equilibrium distance thus grows from the value Q g0 to a value Q e0 (> Q g0 ), the impurity will oscillate around a new equilibrium position, and we can write for its total energy E e = E e0 +

1 f e (Q − Q e0 )2 , 2

(4.12)

where Ee0 = E g0 + E 0 and we usually assume that the force constant f e remains unchanged as the atom goes to the excited electronic state, thus f e = f g . Equation (4.12) is represented by the upper parabola in Fig. 4.8(b), which, under the assumptions, arises by translating the parabola (4.11) into a new origin [Q e0 , E g0 + E 0 ]. The energy E 0 is equal to the electron excitation energy of the impurity atom and is called the zero-phonon or no-phonon energy for reasons that will become clear hereafter. Before entering the discussion on optical transitions with Fig. 4.8 as promised, let us attempt to specify more closely the notion of the conﬁgurational coordinate Q. We introduced it by a visual demonstration—as a coordinate describing in a simple way the relative motion of a point defect and its nearest neighbours. Admittedly, such a picture very often corresponds to reality; on a more general level, however, Q may represent a conﬁguration of multiple atoms as well as of a three-dimensional host matrix in the neighbourhood of a luminescent impurity atom or molecule. In another words, the coordinate Q is generally a combination of normal vibrational modes of a defective

A localized optical centre in a solid matrix periodic atomic structure. The reduction of a three-dimensional conﬁguration to a single coordinate represents a considerable technical simpliﬁcation of the problem. When introducing the term of conﬁgurational coordinate, we nowhere explicitly invoked the translational symmetry of the crystal lattice; we were only speaking of a defect atom and its immediate neighbourhood. Hence, only the short-range order is important here and the conﬁgurational coordinate model can thus be applied to both crystalline and amorphous solids. Let us now consider how the impurity atom can be raised from the ground to an excited electronic state by absorbing a photon of visible radiation. In its ground electronic state, the system is located on the lower parabola around the minimum A. The absorption of a suitable photon proceeds extremely fast, within a time interval of about 10−15 s. During this time, all atoms in the solid keep their momentary positions unchanged since the typical frequencies of lattice vibrations are comparatively low, ω ∼ 1012 –1013 s−1 . Therefore, the absorption event takes place much faster than nuclei around the impurity atom can rearrange into a new equilibrium conﬁguration and, thus, in the diagram of Fig. 4.8(b), it is represented by a vertical transition between points A and B. (Not to be confused with direct optical transitions in the Brillouin zone!) Point B, as the ﬁnal transition state, is determined by that vibronic level of the excited electronic state that has the highest occurrence probability at Q = Q g0 (the ‘turning point’). Therefore, a photon of energy hνa equal to the energy difference between B and A is absorbed. However, point B represents an excited vibrational state of the upper energy curve, which is a non-equilibrium position. Hence, by rearranging the conﬁguration of its adjacent nuclei, the system gradually reaches an equilibrium given by the minimum C of the upper parabola at Q = Q e0 . In addition it releases its excess energy by emitting phonons hωe (= hωg ), belonging to one of the vibrational modes associated with point defects as discussed in Section 4.3. Therefore, the ultimate outcome of the relaxation is to hand over a certain fraction of the electron excitation energy E R = (E B – E C ) to the matrix (lattice) in the form of heat. The energy E R is called the relaxation energy. At point C, the system is still in an excited electronic state of ﬁnite lifetime (10−9 –10−8 s for the allowed dipole transitions); after this time, it drops to point D of the ground electronic state, radiating a luminescence photon of energy hνlum = E C –E D . The verticality of the transition C → D and the choice of point D are driven by the same rules as applied in the case of the absorption transition (A → B). The entire process is again completed by releasing the relaxation energy equal to the energy difference between D and A (which can be easily shown to be equal to E R = E B – E C ) and returning to point A. The approach assuming that atomic nuclei remain at rest in a solid matrix during optical excitation of the electron, and thus leading to verticality of the resulting optical transitions in the conﬁgurational coordinate diagram, is called the Franck–Condon principle. We can immediately see that the principle inherently explains the Stokes’ luminescence law: hνa ≥ hνlum . Thus, the localized luminescence centres are generally ‘transparent’ to their own emitted radiation. Considering Fig. 4.8(b), we deﬁne several additional important terms. First of all, the two parabolic curves intersect at point X . Putting aside zero-point

115

116

Phonons in optical phenomena oscillations, the energy separation E A of point X from the minimum C of the upper parabola is equal to EA =

(E 0 − E R )2 . 4E R

(4.13)

This is the activation energy, the meaning of which will be discussed in Section 4.6. Next, we usually express the relaxation energy E R , supposing hω = hωg = hωe , as E R = S h¯ ω,

(4.14)

where the dimensionless parameter S is called the Huang–Rhys factor. By eqn (4.14), this factor hence represents the mean number of phonons hω emitted as the centre relaxes along the path B → C or D → A. (If ωe = ωg , which is experimentally observed in certain cases, then it is basically possible to deﬁne two different values of the Huang–Rhys factor: Se a Sg .) This factor, S, is an important indicator of the strength of coupling between the centre and the matrix. The larger the parameter S, the larger is the shift (Q e0 – Q g0 ) and thus the stronger is the interaction between the excited centre and its surroundings. Finally, the meaning of the term zero-phonon energy for E 0 should be clearer now: it is the lowest excitation energy to be supplied to the centre to bring it to the excited electronic state. Optically, this will certainly be possible if the axes of both parabolas merge, i.e. Q g0 ≈ Q e0 and E R → 0, or S = 0. We shall show shortly, however, that this is not the only conﬁguration in which such a transition can occur. No phonons are released during such an optical excitation and hence the term zero-phonon energy for E 0 .

4.5 The shape of absorption and emission spectra of a localized centre By making use of Fig. 4.8(b) and employing qualitative arguments, we can now proceed to get an insight into the shape of optical absorption and emission (luminescence) spectra of a localized centre. At ﬁrst glance, it may seem that both the absorption and emission are formed by narrow lines corresponding to the transitions A → B and C → D. The truth is, however, somewhat more complicated. The ‘harmonic oscillators’ of the ground as well as the excited electronic states oscillate incessantly, and so both the initial and the ﬁnal point of an optical transition must respect the spatial distribution of the oscillator probability density. Thus, for instance, although an absorption transition starting from point A will most likely end at point B, it may also—with just a slightly lower probability—terminate on a vibrational level (of the excited electronic state) with an energy higher or lower by hω. Transition to the vibrational levels ±2hω will even have a somewhat lower probability, etc. Obviously, even the transition with zero-phonon energy hνa = E 0 will occur with a certain probability (which, in Fig. 4.8(b), is just the transition –2hω), and it will happen all the more so the smaller the difference Q e0 – Q g0 is. The above considerations thus lead to the following picture of the absorption spectrum: it will consist of a series of narrow lines spaced equidistantly by

Absorption and emission spectra of a localized centre

117

the phonon energy hω, and their intensities will be modulated by a certain probability distribution. Since analogous reasoning may be applied to the emission spectrum as well, only reversing the transition directions, the shape of the emission spectrum is expected to be mirror-like with respect to the absorption spectrum, both spectra sharing a common line at the zero-phonon energy E 0 . All this is shown in the right part of Fig. 4.8(c). What has been said up to now can be, naturally, represented quantitatively by calculating the transition probability [8]; it is proportional to the square of the dipole moment matrix element. Assuming independence of the dipole moment operator of the conﬁgurational coordinate Q, the spectral shape will be determined—in accordance with the above reﬂections—by the overlap integral of the wavefunctions of the vibrating nuclei. At absolute zero temperature, this yields the shape of the absorption spectrum to be given by the Poisson distribution I (n) ≈ e−S S n /n!,

n = 0, 1, 2, . . . ,

(4.15)

where n numbers the vibrational level of the excited electronic state (the upshifted parabola); as T → 0 K, the transition begins from the ground vibrational level (point A) of the ground electronic state. Figure 4.9 represents schematically several spectra of the type (4.15) for various values of the parameter S. One usually distinguishes three cases: weak (S ≤ 1), medium (S ≈ 5–10), and strong (S ≥ 20) exciton–phonon coupling. It immediately follows from relation (4.15) that in the case of an extremely weak bond (S = 0), the spectrum will consist of a single line corresponding to the zero-phonon transition to the n = 0 state (the so-called zero-phonon or no-phonon line). With increasing values of S, gradually more and more lines with a higher n (the so-called phonon replicas or satellites) appear and the intensity of the no-phonon line I (0) = INP decreases; the maximum of the spectral ‘envelope’ occurs roughly at n = S. The energy separation between the maxima of absorption and emission is called the Stokes shift and it is obviously given by 2Shω, as demonstrated by Fig. 4.8(c). Figure 4.9 considers the individual lines to be inﬁnitely narrow. In fact, the lines are already broadened at T = 0 K, as actually shown in Fig. 4.8(c). This happens as a result of the zero-point oscillations and other mechanisms not included in the Franck–Condon principle: homogeneous broadening due to the ﬁnite excited state lifetime and inhomogeneous broadening due to the more or less variable matrix parameters in the vicinity of any localized centre, i.e. because of possible variability in the values of energy hω. Therefore, as the parameter S increases the satellite phonon lines n ≥ 1 gradually merge into a continuum, which is sometimes also called the phonon wing. Let IPW denote the wing integral intensity, shown as the shaded area on the right in Fig. 4.8(c). The ratio of the no-phonon line intensity INP to the total intensity of the absorption (or emission) band (INP + IPW ) is called the Debye–Waller factor u DW =

INP ≤ 1. INP + IPW

(4.16)

Fig. 4.9 Schematic shape of the (absorption) spectrum given by the Poisson distribution (4.15) for several values of the Huang–Rhys parameter S.

118

Phonons in optical phenomena The value of u DW drops quickly with increasing S as one can infer immediately from Fig. 4.9. Furthermore, it also decreases considerably with increasing temperature (here we can refer to the complete analogy with the Debye–Waller factor known from X-ray diffraction on the vibrating lattice). Before discussing typical experimental examples, we shall brieﬂy summarize the typical spectral features for various strengths of the exciton–phonon coupling: • Weak coupling: a distinct no-phonon line and a negligible phonon wing, zero Stokes shift and a large Debye–Waller factor u DW ≈ 1. • Medium coupling: an inconspicuous no-phonon line, a number of phonon satellites (up to n ≈ 10) in the phonon wing, a small factor u DW ≤ 10−2 . • Strong coupling: the no-phonon line missing completely, phonon satellites merging into a broad phonon wing, the spectrum takes the form of a broad, structureless Gaussian band with a large Stokes shift (for n ≥ 10, the Poisson distribution turns into the Gaussian form, see Fig. 4.9), factor u DW ≈ 0. Examples of experimental spectra are given in Fig. 4.10. We shall mainly concentrate on emission spectra since often it is not quite straightforward to measure the absorption spectrum of a localized centre in semiconductors. (Either the absorption measurements are not sufﬁciently sensitive as compared to the luminescence measurement, as we have mentioned already, or the absorption spectrum overlaps with the onset of the matrix absorption edge itself, and so on. In this respect, the situation is much more favourable in widebandgap optical materials such as alkali halides, Al2 O3 , CaF2 , CaO.) As an example of weak exciton–phonon coupling in Fig. 4.10(a), the lowtemperature (4.2 K) luminescence spectrum of phosphorus impurity atoms embedded with a concentration of 1016 cm−3 into crystalline silicon is displayed [9]. This is a pure no-phonon, narrow line (S = 0, u DW ≈ 1). If we give a little more thought to this observation, it may seem strange that in a semiconductor with an indirect bandgap, such as silicon, an optical recombination act without phonon participation can be found; the quasi-momentum conservation law should not enable similar processes to occur. This is a justiﬁed objection, we have not been considering a situation like this so far; in both the present section and Section 4.4, we have tacitly assumed that the semiconductor— matrix—had a direct bandgap and from this point of view, phonons were not indispensable to ensure optical transitions. Now, we really should need them; however, it is the relatively heavy phosphorus doping that breaks the perfect translational symmetry of the lattice and partially removes the ban on nophonon transitions. We can also immediately ask the question why is it just silicon where the experiment points to a weak exciton–phonon interaction. The answer is simple. The only mechanism of this interaction in non-polar, centrosymmetric silicon is the deformation potential and the two most efﬁcient mechanisms of this interaction, the Fr¨ohlich and piezoelectric mechanisms, are thus missing. An example of medium exciton–phonon coupling is displayed in Fig. 4.10(b): the low-temperature (7 K) luminescence spectrum of iodine ions I− in a crystalline AgBr matrix [10]. We can clearly see a number of narrow phonon lines for n = 0 to n = 10, superimposed on a rather broad phonon wing.

Absorption and emission spectra of a localized centre

119

Fig. 4.10 Emission spectra of localized optical centres in semiconductors. (a) Weak exciton–phonon coupling: The (no-phonon) luminescence line of phosphorus atoms in crystalline silicon. We can also see a weak no-phonon line associated with arsenic atoms present at a lower concentration. After Pelant et al. [9]. (b) Medium exciton–phonon coupling: AgBr/I− luminescence. To suppress coupling between the iodine-related I− centre and the lattice vibrations (in order to emphasize the phonon structure), an external hydrostatic pressure was used here. After Wassmuth et al. [10]. The left part shows the corresponding absorption spectrum after Kanzaki and Sakuragi [11]. (c) Strong exciton–phonon coupling: luminescence of a self-trapped exciton in AgCl. After Pelant and H´ala [13]. Note the different wavelength scales.

Therefore, we can estimate the values of the interaction parameters: S ≈ 8 and u DW < 10−2 (because, although the no-phonon line is present, its intensity is minute). Also here, we notice the presence of the no-phonon line in the spectrum even though this is again the case of a semiconductor with an indirect bandgap. The reason for this is analogous to that for doped silicon. The left part of Fig. 4.10(b) also shows the onset of the absorption spectrum as measured in AgBr samples of high optical quality [11]. Comparison of the spectra conﬁrms the correct identiﬁcation of the individual lines—we can clearly see the mirrorsymmetry of the spectra together with the no-phonon lines overlapping in absorption and emission. Let us again note that the presence of no-phonon lines at a localized centre in an indirect semiconductor is not commonplace. For example, ZnSiP2 (with an unknown impurity as the centre) is usually cited as an indirect semiconductor where the no-phonon spectral line is missing and there is an energy separation of 2hω between the onsets of absorption and emission [12]. The low-temperature (4 K) luminescence spectrum of AgCl serves as an example of strong exciton–phonon coupling in Fig. 4.10(c): a smooth, broad curve without any phonon structure [13]. Here, the localized centre

120

Phonons in optical phenomena is represented by the so-called self-trapped hole in the vicinity of an Ag+ ion, which attracts a photoelectron via Coulomb forces, thus producing the so-called self-trapped or auto-localized exciton. Its radiative annihilation then gives rise to a broadband luminescence spectrum. We shall consider these excitons in rather more detail in Subsection 7.2.4. This is an untypical intrinsic localized centre. There is not much difference between the emission spectra of AgBr and AgCl apart from the total absence of both the no-phonon line and ﬁne phonon structure in AgCl. In fact, the interaction of excitons with the lattice vibrations is very strong in both cases due to the efﬁcient Fr¨ohlich mechanism.

4.6 Thermal quenching of luminescence Let us return to Fig. 4.8(b) and explore point X in more detail. At a temperature close to absolute zero, the excited centre is located near point C (and thermal vibrations are negligible). With increasing temperature T , however, the amplitude of vibrations of the centre around its position Q e0 increases, and, consequently, so does the chance of the system to reach point X . In solid-state physics terminology, this means overcoming the potential barrier of height E A . The probability of such a thermally activated process is governed by the wellknown relation p = p0 e−E A /kB T,

(4.17)

where p0 (s−1 ) is the so-called frequency factor, acquiring values of the order of the lattice vibration frequency. After reaching point X , the excited centre now has the option of a non-radiative return to the ground electronic state: at point X , it can pass over the curve of the ground state potential energy and, following the path X → A while emitting phonons, it can reach equilibrium at point A. Thus, all the energy gained via absorption of the excitation photon hνa is converted into the matrix vibrational energy, i.e. into heat. Realizing that the probability (4.17) is thus nothing but the probability of a −1 and assuming that the probability τ −1 of a non-radiative transition p = τnr r radiative transition C → D is independent of temperature, the luminescence quantum efﬁciency (3-2) can be expressed as η=

Fig. 4.11 Luminescence efﬁciency of ZnS:0.015% Ag as a function of temperature. Points—experiment; solid line—calculation according to (4.19) with EA = 3.9meV,E A = 132meV. After Williams [14].

1 , 1 + ξ exp (−E A /kB T )

(4.18)

where ξ = τr p0 . Therefore, η drops with increasing temperature and this effect is called thermal quenching of the luminescence. An example of the temperature dependence of the luminescence efﬁciency, established experimentally in a classical semiconductor phosphor ZnS doped with Ag (which is well-known from the Second World War era when it was used for radar screens), is shown in Fig. 4.11. This is an often-used type of graph where we plot η as a function of reciprocal temperature, 1/T ; this is because for sufﬁciently large T we can usually approximate (4.18) by η ∼ ξ −1 exp(E A /kB T ), and from the slope of such a logarithmic-scale plot we can immediately infer the activation energy E A . At the same time, it can be

Problems seen in Fig. 4.11 that the thermal quenching only occurs here for temperatures T ≥ 310 K (i.e. for 1000/T ≤ 3.2 K −1 )—hence, this phosphor radiates most at room temperature which is highly unusual and which explains why the material is so attractive as regards its applications. It is thus obvious that relation (4.18) does not fully grasp the overall form of the experimental dependence since, when temperature increases from about 200 K to approximately 280 K, the luminescence efﬁciency does not drop but grows instead. A similar increase is generally observed quite often and the simple conﬁgurational coordinate model, as discussed above, can no longer encompass this fact. In order to describe the experimentally found temperature dependence η, eqn (4.18) is sometimes modiﬁed by adding another factor that describes a weakly thermally activated process resulting in an increase of the radiative transition probability. For example, the experimental points in Fig. 4.11 can be very well ﬁtted by the equation

η∼

T e−EA /kB T 1 + ξ e−E A /kB T

(4.19)

(see the curve in Fig. 4.11 with E A ≈ 3.9 meV and E A ≈ 132 meV) [14]. However, in this case, it is just a phenomenological model while currently there are already more exact models based on microscopic concepts. Let us emphasize, however, that any such increase in luminescence intensity with increasing temperature is only temporary and, ultimately, thermal quenching always prevails and luminescence thus fades away completely. And ﬁnally a note regarding the relative position of points B and X in Fig. 4.8(b). Our analysis of thermal quenching was based on the assumption that the intersection point X is at a higher energy than point B. If both points are located on the same level or if X is even lower than B then there will be a steep drop in luminescence intensity since a non-radiative transfer of the electronic excitation energy to the matrix will prevail already at very low temperatures.

4.7 Problems 4/1: Show that the vibrational energy of a one-dimensional ‘crystal’ with N atoms is at high temperatures (hωk kB T ) equal to E¯ = N kB T . (Hint: Transform relation (4.4) into the form −1 E¯ N h¯ ωk h¯ ωk .) = exp −1 kB T kB T kB T 4/2: Show that the total energy of a harmonic oscillator in quantum physics is equal to (hω/2) coth(hω/2kB T ). 4/3: Prove that in the harmonic approximation and assuming f e = f g , the relaxation energies E R in Fig. 4.8(b) in the ground and excited electronic states are the same. Show that the activation energy E A is given by eqn (4.13). 4/4: The lattice vibrations in crystalline silver bromide show a number of peculiarities. This is caused by the deformability of the Ag+ ion and the considerable fraction of both ionic and covalent bonds in the crystal.

121

122

Phonons in optical phenomena These effects lead to very dissimilar force constants for different vibration types, to a low energy of TO-phonons at the L point (Fig. 4.6), and to the inverted character of TO- and TA-phonons near the L point. Discuss these phenomena according to Dorner et al. [15]. 4/5: Conﬁrm that at T = 0 K the Debye–Waller factor u DW and the Huang– Rhys factor S are related by u DW = exp(–S). (Hint: Use eqns (4.15) and (4.16).)

References 1. Dekker, A. J. (1963). Solid State Physics. Chap. 2. Prentice-Hall, Englewood Cliffs, N.J. 2. Peyghambarian, N., Koch, S. W., and Mysyrowicz, A. (1993) Introduction to Semiconductor Optics. Chap. 4. Prentice Hall, Englewood Cliffs, N.J. 3. Dargys, A. and Kundrotas, J. (1994). Handbook on Physical Properties of Ge, Si, GaAs and InP. Science and Encyclopedia Publishers, Vilnius. 4. Hayes, W. and Stoneham, A. M. (1985). Defects and Defect Processes in Nonmetallic Solids. Chap. 1. John Wiley, New York. 5. Yu, P. Y. and Cardona, M. (1996). Fundamentals of Semiconductors. Springer, Berlin. 6. Song, K. S. and Williams, R. T. (1996). Self-Trapped Excitons (Springer series in solid state sciences Vol. 105). Springer, Berlin. 7. B¨oer, K. W. (1990). Survey of Semiconductor Physics. Van Nostrand Reinhold, New York. 8. Vij, D. R. (ed.) (1998). Luminescence of solids. Plenum Press, New York; Yamamoto, H. (1999). Fundamentals of Luminescence. In Phosphor Handbook (ed. S. Shionoya and W. M. Yen), p. 35. CRC Press, Boca Raton. 9. Pelant, I., H´ala, J., Ambroˇz, M., V´acha, M., Valenta, J., Adamec, F., Kohlov´a, V., and Matouˇskov´a, J. (1990). Impurity assessment in Si wafers by photoluminescence method V. Research report for Tesla Roˇznov. Charles University in Prague, Faculty of Mathematics & Physics, Prague. 10. Wassmuth, W., Stolz, H., and von der Osten, W. (1990). J. Phys. C: Cond. Matter, 2, 919. 11. Kanzaki, H. and Sakuragi, S. (1969). J. Phys. Soc. Japan, 27, 109. 12. Shah, J. (1972). Phys. Rev. B, 6, 4592. 13. Pelant, I. and H´ala, J. (1991). Solid State Comm., 78, 141. 14. Williams, F. E. (1948). The mechanism of rate processes in the luminescence of solids. In Preparation and Characteristics of Solid Luminescent Materials. Cornell Symposium 1946, p. 337. John Wiley, New York; Chapman & Hall, London. 15. Dorner, B., von der Osten, W., and B¨uhrer, W. (1976). J. Phys. C: Solid State Phys., 9, 723.

Channels of radiative recombination in semiconductors Various radiative recombination processes have already been mentioned several times in the previous chapters. These processes were, however, not discussed from the point of view of the underlying physics; more emphasis was put on the introduction (or reminder) of the basic concepts and terminology, which will be indispensable later in the book. The conﬁgurational coordinate model, which was described in the previous chapter, for example, is broadly applicable. In this chapter, we are going to show in which particular aspects of luminescence in semiconductors the application of this model is completely straightforward, when, on the other hand, it does not make any sense at all, or when it can be used only formally and with prudence. Now that everything is ready we can move on to giving systematic explanations of known channels of radiative recombination in semiconductors. First, we will list an overview of these channels. Secondly, we will focus in more detail on the spectral shape of the emission line of recombining free electron– hole pairs, and of related recombinations of a free electron with a neutral acceptor or a free hole with a neutral donor. Then we will talk about the shape of the emission spectra of recombining donor–acceptor pairs and ﬁnally we will mention the particularity of exciting luminescence via a two-photon absorption process.

5.1 Overview of luminescence processes in crystalline semiconductors Let us start with the widely accepted classiﬁcation of luminescence processes according to the intensity of excitation. The low-ﬂuence or weak excitation processes (i.e. taking place when a gas-discharge lamp, an incandescent lamp or a continuous-wave gas laser with the output power of the order of 0.01–10 W/cm2 are used for excitation) comprise: • radiative recombination of free excitons (often denoted as FE for a free exciton, or X); • radiative recombination of free excitons with simultaneous emission of an LO phonon (FE–LO, X–LO);

5 5.1 Overview of luminescence processes in crystalline semiconductors

123

5.2 Recombination of free electron–hole pairs

124

5.3 Recombination of a free electron with a neutral acceptor (e–A0 ) and of a free hole with a neutral donor (h–D0 )

132

5.4 Recombination of donor–acceptor pairs (D0 –A0 )

135

5.5 Luminescence excited by two-photon absorption

139

5.6 Luminescence from transition metal and rare earth ion impurities 144 5.7 Problems

146

124

Channels of radiative recombination • radiative recombination of a bound exciton (BE), which can be further subdivided into • radiative decay of an exciton bound to a neutral donor (D0 , X) or (D0 –X); • radiative decay of an exciton bound to a neutral acceptor (A0 , X) or (A0 –X); • radiative decay of an exciton bound to an ionized donor (D+ , X) or (D+ –X); • radiative decay of an exciton bound to an ionized acceptor (A− , X) or (A− –X); • radiative decay of an exciton bound to an isoelectronic impurity; • radiative recombination of donor–acceptor pairs (D0 –A0 ); • radiative recombination of a free hole with a neutral donor (h–D0 ) or a free electron with a neutral acceptor (e–A0 ); • radiative recombination of free electron–hole pairs (e–h), which can also be referred to as band-to-band recombination. At high-ﬂuence (strong) excitation, usually by means of a pulsed laser with excitation intensity of the order of 1 kW–10 MW/cm2 , additional processes occur: • • • • •

radiative decay of an excitonic molecule (EM or XX); luminescence coming from inelastic collisions of excitons (X–X collisions); luminescence of electron–hole liquid (EHL);1 luminescence of electron–hole plasma (EHP); Bose–Einstein condensation of excitons or excitonic molecules and luminescence coming from the condensate.

Obviously, two or more types of these processes can occur simultaneously in a material. In addition, most of these processes can also be observed in low-dimensional semiconductor structures, although the emission of light from low-dimensional structures is in some aspects speciﬁc. The emission of light from amorphous semiconductors, on the other hand, is governed by signiﬁcantly different processes. Later in this chapter, the most important spectral features connected with luminescence processes occurring at low-ﬂuence excitation levels will be treated, deliberatly neglecting any luminescence manifestation of excitons, to which Chapter 7 is devoted. The high-excitation luminescence spectral features will be discussed in Chapter 8 and the luminescence of amorphous and low-dimensional semiconductors will be described in Chapters 9 and 12.

5.2 Recombination of free electron–hole pairs Even though, in reality, this process is not encountered very often, the explanation of the shape of a luminescence emission spectrum will begin here; the 1 This process is sometimes not considered typical for high-level excitations because it can often be observed even when a continuous source of radiation is used.

Recombination of free electron–hole pairs

125

reasons for choosing this particular process will become evident later. (We would like to note here that this process was called ‘bimolecular’ in Chapter 3, where it was treated from the point of view of its kinetics.)

5.2.1 Direct bandgap The process is schematically shown in Figure 5.1. An electron with energy E 2 situated close to the minimum of the conduction band spontaneously recombines with a hole situated at the top of the valence band with energy E 1 and wavector k0 via a direct vertical transition. The physical quantity of interest here is the probability density Isp (hν) of the spontaneous emission of a photon with energy hν = E 2 –E 1 . This is obviously inﬂuenced by three factors: 1. the probability of a suitable conﬁguration of occupancy of conduction and valence band states f e (ν); 2. the quantum-mechanical probability of this transition in the form of the square of the absolute value of the matrix element of the transition (in the dipole approximation) |M|2 ; 3. the joint density of electron and hole states ρ(ν) in the corresponding bands. Thus Isp (hν) ≈ |M|2 f e (ν)ρ(ν) ≈

1 f e (ν) ρ(ν). τr

(5.1)

Ad 1. For the radiative recombination to take place, the corresponding energy state with energy E 2 in the conduction band has to be occupied by an electron while the state with energy E 1 in the valence band has to be empty (i.e. occupied by a hole), as is indicated in Fig. 5.1. Consequently, f e (ν) is given as the product of the occupancy factors fc and f v : f e (ν) = f c f v = f (E 2 )[1 − f (E 1 )],

(5.2)

where f (E) = {exp[(E − E f )/kB T ] + 1}−1 is the Fermi–Dirac distribution function. Let us assume that the semiconductor is intrinsic, has a sufﬁciently wide bandgap E g and the process takes place at low temperature. At lowﬂuence excitation, the semiconductor can be treated as if it is still in thermal equilibrium, i.e. the Fermi level stays localized in the middle of the bandgap at low temperature (Fig. 5.1). As long as the condition of low temperature and wide bandgap kB T (E g /2) ≈ E 2 –E f ≈ E f –E 1 is fulﬁlled, one can write 1 f (E 2 ) = (E −E )/k T ≈ exp [−(E 2 − E f )/kB T ] , e 2 f B +1 [1 − f (E 1 )] = 1 −

1 e(E 1 −Ef )/kB T + 1

≈

e(E 1 −Ef )/kB T e(E1 −E f )/kB T + 1

≈ exp[−(E f − E 1 )/kB T ], which transforms (5.2) into the simple form fe (ν) ≈ exp (−hν/kB T ).

(5.3)

Fig. 5.1 Free electron–hole recombination in a direct bandgap semiconductor. E f stands for the Fermi level.

126

Channels of radiative recombination Ad 2. The matrix element of the optical transition M can be considered to be constant to a very good approximation over a wide range of wavevectors close to the extremes of the bands. In relation to luminescence, the radiative lifetime τr will be treated as inversely proportional to the square of the matrix element τr ∼ |M|−2 . (This simple relation is strictly valid only for atomic transitions. When it comes to semiconductors, the application of this relation is a bit less straightforward; the parameters of the particular band structure as well as the bandgap width come into play. A detailed theoretical discussion can be found in [1]. This approximation, however, is fully sufﬁcient within the framework of this textbook.) Ad 3. The density of states ρ(ν) is pertinent to the difference energy band E c (k)–E v (k), which is obtained—mathematically speaking—by subtracting E v (k) from E c (k). Since these transitions are vertical the subtraction makes sense in this context. The densities of states in the individual bands, i.e. in the conduction band ρc (E) and the valence band ρv (E), are well known (see, e.g., [2, 3]): ρc (E) = ρv (E) =

(2m e )3/2 2π2 h¯ 3 (2m h )3/2 2π2 h¯ 3

(E − E c )1/2 , E ≥ E c ,

(5.4a)

(E v − E)1/2 , E ≤ E v ,

(5.4b)

where m e and m h stand for the effective masses of an electron and a hole, respectively, connected with the curvatures of the corresponding bands close to the extremes. Thus, one can easily get (using the incremental relation ρc (E 2 )dE 2 = ρ(ν)dν) ρ(ν) =

(2m r )3/2 π h¯ 2

(hν − E g )1/2 ;

hν ≥ E g .

(5.5)

Relation (5.5) includes the reduced mass of the electron and hole given by the expression 1 1 1 = + . mr me mh

(5.6)

To derive ρ(ν) by making use of the aforementioned incremental relation, the following expressions, which stem directly from Fig. 5.1 (see Problem 5/1), are employed: mr (hν − E g ), me mr (hν − E g ). E1 = Ev − mh

E2 = Ec +

(5.7) (5.8)

One more thing worth mentioning is that the density ρ(ν) is given per unit frequency, not per unit energy, which causes different fractional prefactors to appear in (5.4) and (5.5).

Recombination of free electron–hole pairs

127

Now, it is possible to get the desired formula for the spectral shape of luminescence coming from the radiative recombination of free electron–hole pairs in a semiconductor with direct bandgap by combining (5.3), (5.5) and (5.1): Isp (hν) ≈ D0 (hν − E g )1/2 exp −(hν − E g )/kB T , (5.9a) where D0 = [(2m r )2/3 /π h¯ 2 τr ]exp(−E g /kB T ) is a parameter independent of the photon energy hν. Disregarding this parameter, Isp (hν) is given by the product of a factor characterizing the joint density of states (hν–E g )1/2 with a term describing basically the occupancy of these states, i.e. exp[−(hν − E g )/kB T ]. The shape of the luminescence spectrum (5.9a) is sometimes also called the Maxwell–Boltzmann distribution. It is interesting to note that the formula describing the radiative band-to-band recombination contains solely the reduced electron–hole mass m r , not the individual effective masses of an electron and a hole m e , m h . In other words, it is impossible to determine the values of the effective masses of the carriers using only luminescence (or absorption) measurements. The spectral shape Isp (hν) is shown in Fig. 5.2(a). The curve is asymmetric with a tail towards the high-energy photon side. The asymmetry stems from the kinetic energy of recombining free electrons and holes, which can be described by an exponential distribution function.2 The full-width

Fig. 5.2 (a) Maxwell–Boltzmann lineshape Isp (hν) ≈ hν − E g exp[−(hν − E g )/ k B T ] at T ≈ 12 K. (b) Asymmetric linewidth broadening with increasing temperature. Curves are normalized. 2 It may be of interest to recall that the formula for the number of molecules of an ideal gas n (out of the total number n), whose kinetic energy falls in the interval (E k , E k + E k ), reads

2 n = √ E k exp(−E k /kB T ). 3/2 n E k π (kB T )

128

Channels of radiative recombination at half maximum (FWHM) of this curve can then be shown to be directly proportional to temperature FWHM ∼ 1.8 kB T.

Fig. 5.3 Emission spectrum of the recombination of free electron–hole pairs in InSb at T = 4.2 K. Solid curve—experiment; circles—theoretical lineshape given by (5.9). After Mooradian and Fan [4].

Thus, the linewidth broadens with rising temperature, as can be seen in Fig. 5.2(b). On the whole, however, the line is very narrow: temperatures T between 4 and 100 K correspond to FWHM ≈ 1–20 meV, which amount to only tenths of nanometres, or nanometres at most, in the visible spectral region. The physical reason underlying the linewidth broadening is obvious: the Boltzmann tail of the Fermi–Dirac distribution broadens with increasing temperature, or in other words, at higher temperatures photoexcited electrons and holes occupy states further from the extremes of the bands. Thus, photons with higher energy are generated by these higher-energy electron–hole pairs, while the low-energy onset of the spectral line is determined by E g and its position remains ﬁxed. (The possible shift of E g with changing temperature leads to a shift of the emission line as a whole.) Figure 5.3 demonstrates the experimentally observed luminescence of electron–hole pairs in InSb at 4.2 K [4]. The dotted curve indicates the theoretical lineshape given by (5.9a) and agrees very well with experiment except for the low-energy side. This slight difference can be due to several factors, including the inﬂuence of the slit of the monochromator as described in Section 2.8, which smears the sharp onset of luminescence. As has already been mentioned, the radiative recombination of free electrons and holes is a scarcely encountered process. Indium antimonide InSb is the exception that proves the rule. Its very narrow bandgap (E g ∼ 0.23 eV at T = 4.2 K) and consequently also the low exciton binding energy ensure that even at low temperatures excitons are thermally dissociated. In nearly all other semiconductive compounds, low-temperature luminescence is dominated by excitonic effects, which means that free electrons and holes and their luminescence are practically absent. In the literature, formula (5.9a) can sometimes be written in the slightly modiﬁed form (5.9b) Isp (hν) ≈ ν 2 (hν − E g )1/2 exp −(hν − E g )/kB T . The factor ν 2 comes from the photon density of states in three dimensions, which equals 4ν 2 /c3 in free space. Taking into account the already mentioned narrow spectral width and high optical frequencies (FWHM/ hν) ≤ 0.01, however, makes it possible to consider ν 2 a constant, and thus to neglect the inﬂuence of this term on the spectral lineshape.

Fig. 5.4 Schematic drawing of radiative recombination of electron–hole pairs in the energy band struture diagram E(k) for a semiconductor with (a) a direct and (b) an indirect bandgap. hν stands for the energy of a photon, h¯ ω for the energy of a phonon.

5.2.2 Indirect bandgap A fundamental difference between the recombination of electron-hole pairs in a semiconductor with a direct and indirect bandgap is shown in Fig. 5.4. This formula implies that the Maxwell–Boltzmann distribution is a fully valid name for (5.9a) and, moreover, the comparison of these two formulas suggests that at low concentrations of free quasiparticles (= 1017 cm−3 , i.e. for weak optical excitation) one can speak of a ‘gas’ of free electrons, holes or excitons in semiconductors.

Recombination of free electron–hole pairs In a direct-bandgap semiconductor, the recombination takes place between electrons and holes with the same wavevector k0 , whereas in an indirectbandgap semiconductor, an excited electron with energy E 2 can recombine with any hole with energy E 1 and varying values of k, as long as the energyconservation rule E 2 –E 1 = hν ± h¯ ω is fulﬁlled. The energy h¯ ω then denotes the energy of a phonon, which takes part in the process in order to ensure the conservation of quasi-momentum: kh¯ ω = |k(E 2 )–k(E 1 )|. Considering the fact that phonon dispersion relations are deﬁned for any k from the ﬁrst Brillouin zone (see, e.g., Fig. 4.3), it is obvious that an appropriate phonon can always be found, unless the transitions are forbidden due to the symmetry of electron and/or phonon states. For the sake of simplicity, only low-temperature cases will be treated hereafter. At low temperatures, only a small number of phonons are present in the semiconductor and the recombination process is accompanied by the emission of a photon and the emission of a phonon, i.e. the electron excitation energy is released both in the form of luminescence and as an additional vibration energy of the lattice: E 2 –E 1 = hν + h¯ ω. in of The calculation of the probability density of spontaneous emission Isp a luminescence photon with energy hν = (E 2 –E 1 )–h¯ ω is then carried out by summing all of the contributions over the curves marked in bold in Fig. 5.4(b), subsequently ‘inﬁnitesimally shifting’ the difference (E 2 –E 1 ) on the energy axis, repeating the summation, etc. Factors which play important roles in the calculation are thus, naturally, not only the densities of states in the bands (5.4), but also the occupancy factors f c , f v .3 In analogy with (5.1), the described procedure leads to the integration over all pairs of states in the conduction and valence bands, whose energies relative to the corresponding band edges will be denoted as E e = E 2 –E c for the electron and E h = E v –E 1 for the hole, respectively (see Fig. 5.5(a)). The mathematical formulation of the described procedure then reads hν+h¯ ω−E g in Isp (hν) ≈ |M|2

ρc (E e ) f c (E e ) ρv (E h ) f v (E h )dE e 0

hν = |M|2

ρc (E e ) f c (E e ) ρv (hν + h¯ ω − E g − E e ) 0

f v (hν + h¯ ω − E g − E e )dE e = |M|

2

hν

E e f c (E e ) hν − E e f v (hv − E e )dE e ,

(5.10)

0

where, as can be seen from Fig. 5.5(a), hν = E g + E e + E h –h¯ ω or E h = hν + h¯ ω–E g –E e . The upper integration limit hν = hν + h¯ ω–E g reﬂects the abovementioned summation of all contributions to the ﬂux of emitted photons hν. 3 The joint density of states (5.5) cannot be applied, since it has a reasonable meaning only for vertical transitions.

129

130

Channels of radiative recombination

Fig. 5.5 Illustrating the calculation of the spectral lineshape of luminescence coming from the recombination of free electron–hole pairs in an indirect-bandgap semiconductor; (a) detail of band structure; (b) convolution of occupied electron and hole states according to (5.10).

On closer inspection, one can easily recognize that what (5.10) represents is the convolution of states occupied by electrons in the conduction band with the states occupied by holes in the valence band. (Let the reader compare formula (5.10) with eqn (A-5) in Appendix A.) The convolution-based calculation (5.10) is schematically shown in Fig. 5.5(b). The matrix element |M|2 this time contains both vertical transitions (via virtual states with higher energies of electrons and holes at the same quasi-momentum) and also electron–phonon scattering ensuring the indispensable alteration of quasi-momentum in the recombination event. If both the photon and phonon parts of the matrix element are symmetry-allowed, this matrix element can be in a very good approximation treated as independent of both E e and E h and its inﬂuence on the emission lineshape can be neglected. The calculation (5.10) can be carried out analytically without being too complicated, although one might not think so at ﬁrst sight. First, we can realize that the product f c (E e ) f v (hν − E e ) under the integration sign is completely analogous to (5.2), but with hν being replaced with (hν + h¯ ω). Similarly to (5.3) the term thus can be approximated f c (E e ) f v (hν − E e ) ≈ exp [−(hν + h¯ ω)/kB T ] .

(5.11)

Since the product fc f v is thus independent of E e , it can be placed outside the integration sign in (5.10). The formula then reads in Isp (hν)

≈e

−(hν+h¯ ω)/kB T

hν 0

E e hν − E e dE e ,

(5.12)

a √ √ where the deﬁnite integral is of the type 0 x (a − x) dx ≈ a 2 (Problem 5/4). The resulting formula for the spectral lineshape of luminescence

Recombination of free electron–hole pairs

131

due to recombination of free electron–hole pairs in a semiconductor with an indirect bandgap thus acquires the form 2 in (hν) ≈ hν − (E g − h¯ ω) exp −(hν − (E g − h¯ ω))/kB T . Isp

(5.13)

Finally, this formula is not very different from the analogous relation for a direct-bandgap semiconductor (5.9a). The ﬁrst difference is represented by the red-shift of the low-energy side of the spectrum by h¯ ω, the second then consists of the replacement of the square-root dependence of the pre-exponential factor in (5.9a) by a quadratic dependence in (5.13). This change in the preexponential factor, however, does not inﬂuence the lineshape radically; it just slightly modiﬁes the low-energy onset of the spectrum (a precise experimental determination of which is, moreover, problematic due to spectral broadening by the slit of the dispersion device as well as by other mechanisms), while the shape of the high-energy tail is most signiﬁcantly inﬂuenced by the exponential factor, which is of identical form in both (5.9) and (5.13). This similarity is documented in Fig. 5.6. Now, it is very important to note that this luminescence process scarcely occurs in reality. The fact that the excited electrons and holes in an indirectbandgap semiconductor live much longer than in direct-bandgap materials causes nearly all electrons and holes at low temperatures to be bound in excitons. The emission spectrum then features only the luminescence line due to the radiative recombination of excitons. Emission coming from the recombination of free electron–hole pairs can only be observed in pure crystals at slightly elevated temperatures (at about 100 K), when some of the excitons are already ionized and when, simultaneously, thermal luminescence quenching is not yet sufﬁciently efﬁcient. The intensity of such luminescence is, however, very low, since the matrix element in (5.10) is of second-order correction in perturbation theory.

Fig. 5.6 Comparison of emission lineshapes of the recombination of free electron–hole pairs (5.9a)—dashed curve—with the lineshape described by (5.13)—solid curve. The curves are normalized both vertically and relative to the origin of the energy axis (i.e. h¯ ω = 0). Typical asymmetry in the high-energy tail is present in both cases.

132

Channels of radiative recombination

5.3 Recombination of a free electron with a neutral acceptor (e–A0 ) and of a free hole with a neutral donor (h–D0 )

Fig. 5.7 (e − A0 ) recombination (top panel) and (h − D0 ) recombination (bottom panel) in a direct-bandgap semiconductor.

An impurity atom in a semiconductor, whose valence is smaller (larger) by one electron than that of the main constituent of the crystal lattice, is referred to as a shallow acceptor (donor). Classic examples of a shallow acceptor (donor) are boron (phosphorus) atoms in silicon. The additional hole or electron arising from the replacement of the main constituent’s atom in its position in the crystal lattice by the impurity atom is weakly bound and can be thermally excited into the valence (conduction) band, thus boosting the electrical conductivity of the material. The corresponding amount of energy needed for the release of the hole or electron is referred to as the ionization (binding) energy of the acceptor E A or donor E D . The acceptor and donor states are usually represented in the band structure diagram by short segments drawn inside the bandgap, just above the maximum of the valence band or below the minimum of the conduction band. As the deﬁnition implies, the difference in energy between the acceptor (donor) level and the extreme of the valence band equals E A (or E D in the case of the conduction band). A neutral acceptor (donor) is a term used to describe an acceptor (donor) with a non-ionized hole (electron); in the opposite case, the impurity will be referred to as an ionized acceptor or donor. The short segment in the band structure demonstrates the fact that the hole or the electron is localized at the neutral acceptor or donor and their quasi-momentum h¯ k is practically zero. This situation is depicted in Fig. 5.7 for an acceptor and a donor in a direct-bandgap semiconductor. Figure 5.7 implies that the presence of a neutral acceptor or donor in the semiconductor can give rise to speciﬁc luminescence. Hereafter, we will focus only on acceptors (Fig. 5.7(a)). If a free electron is present at the bottom of the conduction band, it can recombine with a hole localized on the acceptor level, which leads to the emission of a luminescence photon with approximate energy hν ≈ E g –E A . The luminescence process would not proceed further, however, if it were not for excitation, either optical or by employing other means, resulting in the liberation of other free electron–hole pairs, as is also demonstrated in Fig. 5.7. Excited electrons and holes quickly thermalize and ‘diffuse’ close to the extremes of the bands. The electron remaining after the radiative recombination at the acceptor level recombines (usually nonradiatively) with a hole at the top of the valence band, which restores the neutral state of the acceptor and the whole process of the emission of a luminescence photon can happen again. Next, the spectral shape of luminescence (e–A0 ) in a direct-bandgap semiconductor will be described. Let us start with (5.9a); this relation can be adapted so that it explicitly contains the effective masses m e and m h : Isp (hν) ≈ (hν − E g )1/2 exp −

hν − E g me m e + m h kB T m h hν − E g exp − . m e + m h kB T

(5.14)

(e–A0 ) and (h–D0 ) recombination Assuming a high hole effective mass m h → ∞ and thus m h m e immediately yields, by making use of (5.14), hν − E g 1/2 . (5.15) Isp (hν) ≈ (hν − E g ) exp − kB T We get back to a formula identical to (5.9a) and the whole procedure seems pointless. In reality, however, the transition from (5.14) to (5.15) only once again stresses the fact that optical transitions across the bandgap do not carry information regarding the values of effective masses m e , m h themselves. Importantly now, in the case of recombination of the type (e–A0 ) the hole bound to an acceptor can be viewed as an immobile quasi-particle with an effective mass m h → ∞, which immediately suggests that the lineshape will again correspond to (5.9a), or (5.15), except for the fact that the low-energy onset is determined by (E g –E A ) instead of E g , which can also be easily deduced from Fig. 5.7(a). Consequently, the formula will read 1/2 hν − (E g − E A ) (e−A0 ) ≈ hν − (E g − E A ) exp − . (5.16a) Isp kB T Since similar reasoning (but for the substitution of electrons with holes) applies to the recombination of a free hole with a neutral donor (h–D0 ), one can instantaneously write the formula for the corresponding lineshape 1/2 hν − (E g − E D ) (h−D0 ) . (5.16b) Isp ≈ hν − (E g − E D ) exp − kB T All in all, the Maxwell–Boltzmann lineshape (5.9a), (5.16) (or the analogous formula (5.13)) is shared by all luminescence processes for which at least one of the recombining quasi-particles is free. This similarity in behaviour reﬂects the kinetic energy of a free quasi-particle, which manifests itself in the asymmetry of the spectral line and the broadening of the high-energy tail with increasing temperature.4 An example of an experimentally observed luminescence spectrum (e–A0 ) coming from a high-purity epitaxial GaAs layer at T = 1.9 K is shown in Fig. 5.8 [5]. Both aspects of the experiment, i.e. the high purity and low temperature, are essential for this observation. If the semiconductor is not highly pure (high purity for GaAs stands for the concentration of unintentional (residual) acceptors and donors of the order less than 1015 cm−3 ), several different acceptors and donors with slightly varying ionization energies are present in the sample, their emission lines thus being, according to (5.16), slightly shifted with regard to one another. This may result in the occurrence of two inhomogeneously broadened lines, one representing the unresolved acceptor transitions and the second one unresolved donor transitions, with the typical asymmetry given by (5.16) smeared and consequently lost. The sample whose spectrum is 4 From the point of view of the conﬁgurational coordinate model, the processes (e–A0 ) and (h–D0 ) can be viewed as weakly localized excitation (i.e. only the zero-phonon line is observed), and broadening of the line due to kinetic energy of the quasi-particles taking part in the process goes beyond the scope of this model.

133

134 Fig. 5.8 Photoluminescence spectrum (e–A0 ) of high-purity GaAs containing a single residual shallow acceptor with ionization energy E A ≈ 27 meV. The solid curve denotes the experimental data, and circles stand for the theoretical lineshape (5.16a). The low-energy edge reveals the occurrence of donor–acceptor pair emission (D0 –A0 ), which is, however, more than an order of magnitude lower in intensity (note the logarithmic intensity scale). The bath temperature of liquid helium was TL = 1.9 K, and the effective temperature of the electron gas for the ﬁt of eqn (5.16a) was Tef = 14.4 K. After Ulbrich [5].

Channels of radiative recombination

shown in Fig. 5.8 contains a single type of acceptor only, which is why the typical asymmetry of the experimentally obtained curve towards the highenergy wing is well evidenced. Yet, at the low-energy edge near hν ∼ = E g –E A another emission band (D0 –A0 ), which will be treated in Section 5.4, clearly stands out. The second experimental aspect, i.e. low temperatures, plays an important role not only due to the effect of thermal quenching, which has already been mentioned several times, but even more importantly to prevent the ionization of donors by the thermal energy kB T . Figure 5.8 contains our very ﬁrst notion of two different temperatures in semiconductors: the lattice temperature (TL ) and the so-called effective temperature of a gas of free quasi-particles Tef , introduced in photoluminescence measurements. The concept of the effective temperature indicates that, although the energy distribution of photoexcited free electrons and holes (or excitons) can be described by the Fermi–Dirac distribution function or by its Boltzmann tail, the temperature Tef in the relevant formula is higher than the bath temperature TL at which the sample is kept (liquid helium, nitrogen, etc.). In other words, even if the free quasi-particles are in thermal equilibrium with one another, they are not in thermal equilibrium with the subsystem of atoms (ions) vibrating in the lattice. This effect was found to be quite general and occurs not only at high-ﬂuence excitation with high-power laser pulses, but also at conventional low-ﬂuence excitation levels. The different temperatures of the carriers and the bath are a natural outcome of the relatively short photocarrier or exciton lifetime, the term ‘relatively short’ meaning the fact that the lifetime of carriers and excitons is shorter than the relaxation time necessary for the establishment of full thermodynamic equilibrium between the two described subsystems, i.e. the gas of free quasi-particles and the crystal lattice.5 Naturally, the difference between the temperatures Tef and TL increases if a high-power excitation source is used or when the energy difference between the exciting photons and the bandgap E g rises. Ultrafast semiconductor spectroscopy [6] is the branch of optics dealing with, among other things, the study of the rate of dissipation of this ‘hot carrier’ excess 5 The exception to the rule T > T can sometimes be encountered in indirect-bandgap L ef semiconductors, in which the lifetime of excitons may be sufﬁciently long.

Recombination of donor–acceptor pairs (D0 –A0 )

135

energy (i.e. the decrease of Tef as a function of time after the excitation pulse has ended) after picosecond or femtosecond excitation. The last remark concerns the practical importance of (e–A0 ) luminescence: it enables the ionization energy E A to be spectroscopically determined as the energy difference between the low-energy onset of the line (E g –E A ) and the energy corresponding to the width of the forbidden gap E g . The bandgap energy E g , however, needs to be obtained with sufﬁcient accuracy from another type of measurement, since luminescence measurements rarely allow for its determination (but for the case of band-to-band recombination). It is of the essence, moreover, that a single type of acceptor is present; the alternative would inevitably lead to the smearing of the lineshape. A characteristic feature conﬁrming the proper identiﬁcation of a line being due to (e–A0 ) or (h–D0 ) can, besides the Maxwell–Boltzmann lineshape, be the saturation tendency of the intensity dependence, as discussed in Section 3.5 for extrinsic luminescence. Radiative recombination (e–A0 ), (h–D0 ) is difﬁcult to observe in an indirectbandgap semiconductor due to the negligible concentration of free electrons and holes with respect to the concentration of excitons.

5.4 Recombination of donor–acceptor pairs (D0 –A0 ) If both neutral donor and acceptors are present in a semiconductor simultaneously, another type of radiative recombination might occur, as depicted in Fig. 5.9. In the approximation of effective mass, the neutral donor D0 can be considered as an ‘extra’ electron orbiting all the remaining parts of the atom, i.e. the atomic nucleus, the inner atomic shells and electrons taking part in the covalent bonding with the nearest constituents of the crystal lattice. A neutral acceptor A0 can then be treated analogously, if the extra electron is substituted with a hole. This electron–hole pair can recombine radiatively while emitting a photon hν (Fig. 5.9(a)). The very same process is sketched in Fig. 5.9(b) in the band structure diagram, although the (E, x) system of coordinates, x being the real space coordinate, is used instead of the conventional (E, k) layout. Immediately after the recombination, both the donor and the acceptor become ionized (D+ , A− ), but free electron–hole pairs generated by the bandFig. 5.9 The concept of luminescence arising from the recombination of donor–acceptor pairs (D0 –A0 ): (a) in real space, (b) in the electron energy band structure as a function of the real-space coordinate x. Donor and acceptor atoms are located at different positions of the crystal lattice, separated by the distance R. The quantities rD and r A stand for the radius of the donor and acceptor, and E D and E A are their ionization energies, respectively.

136

Channels of radiative recombination to-band excitation quickly neutralize these ionized donors and acceptors and the whole process resumes. This process is sometimes schematically described as D0 + A0 → D+ + A− + hν. Glancing at Fig. 5.9(b) one could deduce that the energy of the emitted photon is determined as hν(D0 − A0 ) = E g − (E A + E D ).

(5.17)

Nevertheless, this formula is not fully valid. Since a charged pair (D+ , A− ) is generated as a result of the recombination process, the additional energy of its mutual electrostatic attraction e2 /4πε0 εr R needs to be added to (5.17): hν(D0 − A0 ) = E g − (E A + E D ) +

e2 (−J (R)). 4 π εr ε0 R

(5.18)

In this formula, R denotes the distance between the donor and the acceptor and rD stands for the radius of the electron shell in D0 (and, analogously, rA for the hole in A0 ), see also Fig. 5.9(a). Formula (5.18) holds only provided the donor and the acceptor represent point charges, i.e. R rD , rA . The last term J (R) in (5.18) constitutes a non-Coulomb term, correcting for the overlap of the wavefunctions in the case of small distance R and decreasing the additional Coulomb energy. This term disappears when R is sufﬁciently large. The (D0 –A0 ) recombination manifests itself in the emission spectrum in various ways, depending on the strength of the electron–phonon coupling. First we shall discuss semiconductors with weak electron–phonon coupling (which means, according to Table 4.2, the fourth group and III-V group semiconductors, taking into account the polaron coupling constant αe as a measure of this interaction). Since the donors and acceptors replace the main constituents of the crystal lattice in their sites, the values of R can only be discrete and, thus, so will the energies of the emitted photons, according to (5.18). When the electron–phonon interaction is weak, one can consequently expect the emission spectrum to comprise a number of narrow (zero-phonon) lines corresponding to the allowed values of R, or, in other words, to virtual spherical ‘shells’ of partners for radiative recombination around the particular donor or acceptor. A prime example of such an emission spectrum is shown in Fig. 5.10 [7], in which one immediately recognizes an overwhelming number of narrow lines. The depicted luminescence spectrum is that of silicon- and sulphur-doped gallium phosphide, GaP, at liquid helium temperature (1.6 K). In this case, silicon and sulphur are the so-called substitution donors and acceptors of type I, which substitute atoms only in one of the sublattices of the crystal, in this case phosphorus: a phosphorus atom is replaced with a sulphur (donor SP ) or silicon (acceptor SiP ) atom. Zinc and oxygen, on the other hand, is a pair that can serve as an example of substitution donors and acceptors of type II, which are built into both sublattices, i.e. ZnGa –OP . Both the density of lines and their intensity obey general rules. The lines located at the high-energy side of the spectrum are relatively sparse and of low intensity, and in the direction towards lower energies they become more

Recombination of donor–acceptor pairs (D0 –A0 )

densely packed and their intensity increases, whereas at the very low-energy edge the intensity decreases again and the lines merge into a ‘ﬁne-structuremodulated’ wider band. Such behaviour is easily understandable considering relation (5.18): high photon energies correspond to small R, the number of suitable neighbours in the nearest shell being low, though; the corresponding discrete values of R are relatively scarce, resulting in sparse and weak lines on the high-energy side of the spectrum. When the distance R increases, however, more partners can be found in the given shell, and the shells themselves are located closer to one another, which means that the lines become more intense and more densely packed. The situation changes once again when R becomes even larger, as the suitable shells nearly merge and a decrease in the probability of radiative recombination W (R) comes into play owing to the fact that the electron and a hole are too far apart, for one can prove that W (R) = W (0) exp (−2R/a),

137 Fig. 5.10 Photoluminescence spectrum of siliconand sulphur-doped GaP (the doping atoms are the so-called substitution impurities of type I, SP donor and SiP acceptor). The doping level is |ND –NA | ∼ 1018 cm−3 , and measurement temperature 1.6 K. The numbers next to the lines denote the number of the shell, lines marked with Rb come from a rubidium calibration lamp. Lines A, B, C are due to bound excitons. The whole spectrum is located between E g = 2.35 eV and E g –(E D + E A ) ≈ 2.044 eV. After Thomas et al. [7].

(5.19)

where a = max(rD , rA ). This is why the low-energy end of the spectrum gets smeared into a broad band and drops to zero somewhere above the energy limit of E g –(E A + E D ), see Fig. 5.10. This type of emission spectrum contains so many characteristic features that the experimental identiﬁcation of the (D0 –A0 ) radiative channel should not pose any problems (even though some spectral similarity with the luminescence of an electron–hole liquid in a doped semiconductor can appear, see Chapter 8). Nevertheless, two additional characteristic features of this type of luminescence spectrum can be listed, the ﬁrst one being an overall blue-shift of the broad band with increasing excitation intensity, as displayed in Fig. 5.11. This blue-shift is easily noticeable and can be qualitatively understood again on the basis of eqn (5.18): when increasing the excitation intensity, more D0 , A0 atoms closer to one another, i.e. with lower R, get excited, which increases the inﬂuence of the Coulomb term in (5.18). The second attribute of the (D0 –A0 ) luminescence spectrum is then typical behaviour in time-resolved luminescence experiments: the increasing delay after the excitation impulse gives rise to a pronounced red-shift of the emission spectrum. The reason for the behaviour lies in the fact that, according to (5.19), the closest pairs with the lower R are the ﬁrst ones to recombine, while pairs further and further apart start to send out luminescence in longer time delays. This, in agreement with

Fig. 5.11 Position of the maximum of the broad (D0 − A0 ) band from Fig. 5.10 as a function of excitation intensity. Bath temperature of 20 K. Different types of symbols denote different samples and different excitation wavelengths. After Thomas et al. [7].

138

Fig. 5.12 (D0 –A0 ) luminescence spectrum of GaP at T = 20 K (the very same sample as in Figs 5.10 and 5.11). The high-energy tail at ∼ 2.25 eV includes the unresolved lines of D0 –A0 pairs (wide slit, higher temperature) and the peak at 2.20 eV corresponds to the broad band from Fig. 5.10. The structure is periodically repeated with period h¯ ωLO . Note the gradual widening of the monochromator slit for higher-energy phonon replicas and the logarithmic intensity scale. After Thomas et al. [7].

Channels of radiative recombination (5.18), signiﬁes the shift of hν(D0 –A0 ) towards lower energies and evidently also the decrease of the overall emission intensity. In the foregoing discussion we have put the (D0 –A0 ) radiative recombination in the framework of the conﬁgurational coordinate model as a special example of ‘localized excitation’ without the contribution of the kinetic energy of free carriers. The narrow spectral lines in Fig. 5.10 were referred to as ‘zero-phonon’ lines. The arguments that justify the application of such terminology are summarized in Fig. 5.12, which represents the emission spectrum of the very sample of Figs 5.10 and 5.11 measured, however, in a much wider spectral range and at slightly higher temperature (20 K). The spectrum contains an intense zero-phonon component near 2.20 eV and several satellites with decreasing intensities, shifted by multiples of the LO-phonon energy. Such behaviour is a typical manifestation of weak electron–phonon coupling. This time, the densely packed lines from Fig. 5.10 are hidden in the unresolved shoulder at 2.25 eV and the wide low-energy band originally located at 2.215 eV (Fig. 5.10) is shifted to 2.20 eV in Fig. 5.12, as a result of the thermally induced decrease in E g . Under what experimental conditions can the characteristic (D0 –A0 ) recombination luminescence with enormous numbers of narrow lines be observed in a semiconductor with weak electron–phonon coupling? The most important parameter will be a suitable level of concentration of both dopants. If the number of donors and acceptors is too low, D0 and A0 in the pairs will be too far apart from one another and no recombination will take place; on the other hand, when the concentration is too high, the simple Coulomb interaction of D0 and A0 ceases to be valid and, moreover, concentration quenching can set in. Therefore, the typical emission with densely packed lines can be observed in moderately or highly doped materials (e.g. in GaP at |ND –NA | ∼ 1017 –1018 cm−3 ) and under slightly elevated excitation (otherwise, only donors and acceptors far apart from one another will be excited and the spectrum will feature only a band). Furthermore, low temperatures are absolutely essential and, if possible, the number of competing radiative recombination channels should be minimized. The importance of fulﬁlling all of these conditions becomes more obvious if we realize that GaP is, in fact, the only material in which a large number of narrow (D0 –A0 ) lines can be observed. For instance in silicon, whose electron–phonon coupling is even weaker than in GaP (and which, similarly to GaP, is an indirect-bandgap semiconductor), luminescence lines of this origin have never been experimentally observed. In GaAs, just to give another example, whose electron–phonon interaction is comparable to that in GaP, the (D0 –A0 ) emission manifests itself as a single unresolved line. There are, obviously, other factors coming into play; the problem will be further discussed in Section 7.2. Now, let us brieﬂy focus on semiconductors with strong electron–phonon coupling. A typical example of such a semiconductor is, taking into account the Fr¨ohlich constant αe in Table 4.2, direct-bandgap zinc sulphide ZnS with E g ∼ 3.8 eV. A particular case of doping by CuZn acceptors and ClS donors leads to intense green emission, which has been well known for many years [8]. The most recent interpretation of this luminescence consists in the D0 –A0 recombination. As the electron–phonon coupling in this material is particularly

Luminescence excited by two-photon absorption

139 Fig. 5.13 Spectral distribution of cathodoluminescence of ZnS doped (activated) by copper with the addition of a ‘ﬂuxing agent’ in the form of NaCl. This results in the luminescence of donor (ClS )–acceptor (CuZn ) pairs, giving rise to the emission band at ∼ 520 nm. Curves enumerated 1–4 correspond to increasing concentration of copper: 1 – nominally pure ZnS, 2–10−3 % Cu, 3–5 × 10−3 % Cu, 4–10−2 % Cu. Measured at room temperature, curves are normalized. After Espe [8].

strong, the luminescence band is broad, lacks any structure and is located far from edge emission (i.e. with large Stokes shift), near 520 nm (Fig. 5.13). The existence of other dopants, the introduction of which makes it possible to cover an important part of the visible spectral region, has been of great importance for applications in the development of phosphors for cathodoluminescence. Here, it might be of interest to make a small historical detour: the fact that efﬁcient luminescence in zinc sulphide can be achieved only if the material is co-doped with two different elements was empirically discovered as long ago as in the 1940s. Since the D0 –A0 recombination mechanism was not yet known to be responsible for the luminescence, the metal dopant was not called an ‘acceptor’, but an ‘activator’, and the Cl− or Br− ions were not known as ‘donors’, but as ‘co-activators’. A similar type of broadband D0 –A0 emission can also be encountered in ZnSe and CdS and some attempts were also made to interpret the intense lowtemperature blue-green luminescence of AgCl by means of the same mechanism. From the application perspective, D0 –A0 recombination is exploited as a mechanism of efﬁcient emission from GaP light-emitting diodes. One of the proposed models describes the red electroluminescence at 1.8 eV as being due to the recombination of a compact OP –ZnGa pair in highly doped material.

5.5 Luminescence excited by two-photon absorption In the text so far, we have taken for granted that the excitation of the photoluminescence processes takes place via the conventional absorption of a single (suitable) photon with energy hνex > E g which leads to the generation of electron–hole pairs or excitons and is followed by radiative recombination via one of the above-mentioned mechanisms. This kind of absorption is governed by the well-known Lambert–Beer law (2.1) Ihνex (d) = I0 exp (−α (hνex ) d) ,

(5.20)

where α(hνex ) is the absorption coefﬁcient and d stands for the depth under the surface of the sample to which the light penetrates. Unless the experiment has some speciﬁc requirements, the usual energy of the excitation photons

140

Fig. 5.14 Schematic illustration of two-photon absorption in semiconductors. The process is mediated by the presence of a higher lying conduction band c2 , but the energy-conservation law reads E c1 − E v = 2hνex .

Channels of radiative recombination substantially exceeds E g , which guarantees high values of the absorption coefﬁcient and in turn boosts the luminescence intensity. The typical values of absorption coefﬁcient for these cases are in the order of α(hνex ) ≈ 104 –105 cm−1 , which allows the penetration of light only into depths of the order of d ≈ α −1 = 10−5 –10−4 cm = 100 nm–1 μm. Such low values can pose a problem, because radiative recombination can be strongly inﬂuenced by surface and subsurface states, the existence of which is well known in solid-state physics. These states can either quench the luminescence, or, if the semiconductor is prone to oxidation, the surface oxide layer (or a surface layer of adsorbed molecules or radicals) can be the source of luminescence. Under such conditions, the obtained spectra might not in fact reﬂect the properties of the studied material—or, at least, an argument of this kind can be raised by any reviewer of a thesis or manuscript dealing with luminescence of semiconductors. A simple but reliable way to conﬁrm or refute such an argument may consist in comparing emission spectra excited via a one-photon and two-photon process. In order to understand why, it is important to give an explanation of two-photon absorption ﬁrst. This is a nonlinear optical phenomenon, in which two photons are absorbed at the same time in a single elemental act. The special case of absorption of two identical photons hνex in a semiconductor is schematically represented in Fig. 5.14. A condition to be fulﬁlled if this process is to occur reads E g > hνex ≥ E g /2.

(5.21)

The right part of the inequality can be easily understood, as it reﬂects the energy-conservation law. The left part of eqn (5.21) results from the nonlinear nature of this process, since two-photon absorption is described in second-order perturbation theory [9] of quantum mechanics, implying that this process is several orders of magnitude weaker than the conventional onephoton absorption (ﬁrst-order perturbation theory). Thus, were the condition hνex > E g fulﬁlled, intense single-photon absorption over the bandgap would set in and two-photon absorption would cease to be detectable. The formalism of second-order perturbation theory implicitly comprises the so-called ‘virtual intermediate level’, which mediates the transition between the ground (E v ) and ﬁnal (E c1 ) states. The role of the virtual intermediate state in a semiconductor is taken on for example by one of the higher lying conduction bands (c2 in Fig. 5.14). The energy-conservation law, though, is a relation between the ground and ﬁnal states: 2hνex = E c1 –E v . Now, we will derive a relation describing the decrease in light intensity as it passes through a semiconductor in the case when eqn (5.21) holds; in other words, we will derive a two-photon analogue of the Lambert–Beer law (5.20). Let us denote by α (2) (I ) the two-photon absorption coefﬁcient, which evidently depends, unlike its one-photon counterpart, on the intensity of light I . It can be shown that this dependence is linear: α (2) (I ) = aI [9], where the coefﬁcient a is a material constant. The decrease in the intensity of the light beam dI as a function of travel distance dx in a sample can then be described by the differential equation

Luminescence excited by two-photon absorption dI = −α (2) I dx = −a I 2 dx.

141

(5.22)

This equation can be easily solved using separation of variables with the initial condition I (x = 0) = I0 . The result can be written as I (d) =

I0 , (a I0 d + 1)

(5.23)

which is the formulation of the law we were looking for; d again stands for the depth of penetration under the surface of the sample, or its thickness. This relation was derived for the ﬁrst time by Basov [10]. In contrast to the fast exponential decrease as in the case of linear onephoton absorption (5.20), the decrease of light intensity during two-photon absorption is only hyperbolic. This fundamental difference in the rate of decrease is documented in Fig. 5.15(a); the hyperbolic decrease is incomparably slower. In order to induce nonlinear optical phenomena, obviously, the application of a high-power source of light is necessary. Two-photon absorption can only be observed when relatively high-power laser beams are used as excitation sources. Taking into account the typical value of coefﬁcient a(∼ 10−3 cm/MW) and the power density of the incident beam I0 = 10 MW/cm2 , one can immediately see that—according to (5.23)—a sample length of 1 cm(!) is needed so that the intensity could decrease by a single per cent (i.e. I (d)/I0 ) ≈ 0.99)! Two-photon excited luminescence coming from thick samples is then, without doubt, a phenomenon connected with the bulk of the material. (If semiconductor nanostructures with typical dimension of units and tens of nanometres are used as samples, however, the difference in the depth of penetration between one- and two-photon excitation is no longer so signiﬁcant.) An experimental veriﬁcation of the described behaviour can be found in Fig. 5.15(b). The ﬁgure demonstrates a view through a cryostat window (dark circle) of a bulk AgCl sample at T ∼ = 80 K (grey rectangle in the upper part of the window). The ruby laser beam (hνex = 1.78 eV) is coming from the left side and excites the luminescence in AgCl; the forbidden gap width Eg ∼ = 3.2 eV of the silver chloride signiﬁes that condition (5.21) is fulﬁlled. This luminescence can be observed as a bright trace coming through the sample in its middle part along its whole length, i.e. about 1.5 cm. Its brightness only minutely decreases towards the right side of the sample, reﬂecting a very modest decrease of laser intensity during its passage through the sample. Which brings us back to the initial question: ‘What does a two-photon excited, i.e. inherently coming from the bulk, luminescence spectrum look like in comparison with one-photon excitation?’ Although a general and unambiguous answer to this question does not exist, a large number of experiments carried out at different laboratories (including that of the authors of this book) suggest that in the vast majority of cases the emission spectra are almost identical, at least when it comes to the salient features. This similarity is documented in Fig. 5.16, in which emission spectra of (a) a bulk AgCl sample at low temperatures [11] and (b) a thin CdS ﬁlm (thickness of 1.6 μm) at room temperature [12] are compared. Similar comparisons were obtained using a large number of other semiconductors under diverse experimental conditions,

Fig. 5.15 (a) Numerical comparison of the decrease in intensity of a light beam as a function of the penetration depth during one- and two-photon absorption. An unrealistically high value of a = 10−2 cm/MW was chosen in order to make the decrease of intensity during the two-photon absorption process observable to the naked eye. (b) Experimental demonstration: a view through the window of a cryostat (dark circle) of a bulk AgCl sample with a horizontal trace of two-photon excited blue-green luminescence across the whole length of the sample (grey rectangle with a light strip in the middle). The sample temperature was T ∼ = 80 K. The focused beam of the excitation ruby laser 694 nm is coming from the left side, and three green optical ﬁlters with high optical densities were applied when the photograph was taken in order to block the scattered laser light.

142

Channels of radiative recombination

Fig. 5.16 Comparison of emission spectra acquired with one- and two-photon excitations. (a) AgCl single crystal, excited by one-photon absorption with a cw high-pressure lamp (hνex = 3.4 eV) and by two-photon absorption with a pulsed ruby laser (2hνex ∼ = 3.56 eV). After Laibowitz and Sack [11]. (b) Thin-ﬁlm CdS excited at room temperature by one-photon absorption (OPA) with nanosecond pulses of the third harmonic of a Nd:YAG laser (hνex ∼ = 3.49 eV) and by two-photon absorption (TPA) with 200-fs pulses of a Ti:sapphire laser (2hνex ∼ = 3.23 eV). The spectra are shifted with respect to one another because the penetration depth of the femtosecond laser was larger than the thickness of the sample (1.58 μm); that is why the luminescence in this case is strongly inﬂuenced by reabsorption and consequently shifted to lower energies. After Yano and Ulbrich [12].

both in air and under vacuum. This indicates that the inﬂuence of surface states on luminescence is not so pronounced as was commonly supposed in the past. In some cases, some new features, e.g. phonon replicas, appear in the two-photon excited spectrum; these new features, however, are again more closely related to the properties of the material itself than to its surface. When in doubt, though, comparative experiments should be carried out on the material. The last question needing clariﬁcation here is how to recognize undoubtedly that the observed luminescence is, indeed, two- and not one-photon excited. Two characteristic features can be applied, namely the quadratic intensity dependence and an ‘anti-stokes’ shift of the two-photon excited luminescence. The term ‘anti-stokes shift’ actually indicates that the spectral position of the emission spectrum violates Stokes’ law, which states that the luminescence wavelength λlum is always longer than the excitation wavelength λex . This law was formulated in the nineteenth century when one-photon excitation was the only conceivable way to excite luminescence (the very ﬁrst laser was designed as late as in 1960); this mode of excitation, obviously, always leads to a Stokes shift. This shift clearly renders nothing less than the energyconservation law hνex ≥ hνlum . During two-photon excitation, however, the

Luminescence from transition metal and rare earth impurities law reads 2hνex ≥ hνlum or λlum ≥ λex /2 and, in particular, the condition λex ≥ λlum ≥ λex /2 is very likely to occur; this happens very often indeed in semiconductors. Such behaviour is demonstrated in Fig. 5.14 depicting the excitation that takes place not too high above the bandgap, and luminescence photons have an energy very close to E g , meaning that λlum < λex . Thus, when looking at the photograph in Fig. 5.15(b), one should realize that the trace of luminescence across the sample is blue-green (λlum ≈ 500 nm), while the exciting laser beam is red (λex = 694 nm).6 The fact that two-photon excited luminescence depends quadratically on the excitation intensity can be derived from simple energy-based reasoning. The density of the excitation power absorbed in the sample of thickness d equals (if reﬂection losses are neglected), according to eqn (5.23), I0 −

I0 (ad I0 + 1)

=

ad I02 ≈ ad I02 ; (ad I0 + 1)

(5.24)

the last modiﬁcation in (5.24) is justiﬁed by the fact that even when applying the highest power densities of the order of I0 = 10 MW/cm2 , still low enough not to destroy the material with the application of nanosecond laser pulses, and considering typical values of a ≤ 10−3 cm/MW, the condition adI 0 1 easily holds. Making just the natural assumption, namely, that luminescence is proportional to the absorbed power, we see that luminescence is proportional to the squared incident laser intensity I02 according to (5.24). This dependence is illustrated in the inset in Fig. 5.16(a). The reader surely recalls the case of bimolecular (one-photon excited) recombination which can, under certain circumstances, exhibit quadratic dependence on the excitation intensity, as was discussed in Section 3.5. Consequently, even though the experimental determination of such a dependence on its own does not prove that two-photon excitation takes place, the combination of this quadratic excitation-intensity dependence with an anti-stokes luminescence shift cannot be interpreted in any other way. It is important to keep in mind that the realization of a two-photon experiment for a given value of bandgap is to some extent limited by the availability of high-power pulsed lasers complying with (5.21). Due to the growing numbers of tunable parametric generators this requirement is no longer as limiting as it used to be. The very last remark in this section relates to the fact that twophoton excitation can sometimes be applied to ensure excellent homogeneity of photoexcited carriers or excitons in order to compare experimental results with theoretical models, as will be mentioned later on in Chapter 8.

6 To detect two-photon excited luminescence, the ‘transmission geometry’ cannot be applied. The direct laser light is many orders of magnitude more powerful than the luminescence and a direct detection of the beam could easily destroy the detector. The two-photon excited luminescence signal is rarely detected in a different way than at right angles to the excitation beam.

143

144

Channels of radiative recombination

5.6 Luminescence from transition metal and rare earth ion impurities Donors and acceptors are introduced in semiconductors as impurities in order to control their electrical transport properties. A number of impurities, however, are introduced into solids primarily in order to boost the luminescence efﬁciency and achieve a particular emission wavelength. Some of these impurities will be discussed in Chapter 7 (the so-called isoelectronic impurities); this section will deal with two types of speciﬁc impurities active in luminescence, which are exploited in countless commercially produced phosphors (e.g. for various types of reﬂecting surfaces, displays, luminescent signs, etc.): transition metal ions from the fourth period of the periodic table and rare earth ions. These impurities, which cannot be easily classiﬁed from the point of view of their electrical activity as donors or acceptors, are active also in the luminescence of semiconductors. The corresponding channels of radiative recombination, however, will be mentioned only brieﬂy, despite being both efﬁcient and very commonly applied; they are not typical for semiconductors. They can be much more frequently encountered in various glasses, wide-bandgap ionic compounds, polymer-based materials, etc. Anyone more deeply interested in them can consult the chapters in the textbooks [13, 14].

Transition metal ions Transition metal ions exhibit luminescence as a result of transitions of electrons between the levels of the partially ﬁlled 3d shell. Ions having the greatest importance in applications are Cr3+ , Mn4+ and Mn2+ . For example, ZnS : Mn2+ has been a material commonly exploited for the preparation of electroluminescent thin ﬁlm for quite some time; Cr3+ ions present in sapphire, Al2 O3 , were, on the other hand, the active medium for the very ﬁrst ruby laser operating in 1960. It is important to realize that 3dn∗ → 3dn (∗ stands for an excited state) transitions are, from the atomic point of view, dipole-forbidden, since they do not comply with the condition = ±1. When the ions are embedded into the crystal lattice, the interaction with the electric ﬁeld of the crystal makes the transitions partially allowed. This interaction can be described in the framework of so-called ligand-ﬁeld theory, which, among other things, shows that in some crystal lattices the emission spectra of the transition metal impurity ions can consist of both discrete lines (atomic-like emission) and broad bands. The crucial factor determining the spectral shape is the arrangement of the neighbouring ligands, the radius of the d orbitals and the distances between the built-in metal ion and the ligand. The shape of the spectrum can be predicted on the basis of the so-called Tanabe–Sugano diagram [15]. Recently, much effort has been devoted to the study of magnetic semiconductors, i.e. semiconductors with impurities of paramagnetic ions (Mn2+ ), with the view towards applications in spintronics. Spintronics deals with the potential exploitation of spin polarization of charge carriers in informatics. Luminescence spectroscopy is presumed to be an excellent instrument for the study of these materials.

Luminescence from transition metal and rare earth impurities Rare earth ions The most commonly applied rare earth ions are trivalent ions of lanthanides Ce3+ –Yb3+ , in which luminescence comes from 4f n∗ → 4f n transitions. Similarly to the previous case, these transitions are also dipole-forbidden, while the crystal ﬁeld makes them partially allowed. An important difference with respect to the previous case of 3dn∗ → 3dn transitions, however, lies in the fact that the 4f shell is strongly screened from the inﬂuence of the crystal ﬁeld by the external ﬁlled orbitals 5s2 5p6 . The inﬂuence of the crystal ﬁeld is, on the one hand, strong enough to partially alter the character of the transitions, and on the other hand, the screening manifests itself by keeping the atomic-like character of the emission spectrum. In the framework of the conﬁgurational coordinate model in Fig. 4.8 this weak interaction with the lattice can be described as Q = (Q e0 –Q g0 ) → 0. This description implies two important consequences: Firstly, the weak effect of the matrix suggests that the energy levels in ions, and thus also the emission (absorption) spectra, will be independent of the chemical nature and periodic arrangement of the matrix. Secondly, the activation energy E A of the thermal quenching of luminescence (Fig. 4.8(b)) will be high, giving rise to more or less temperature-independent emission. Consequently, the emission can be expected to occur even at room temperature unless a different quenching mechanism, such as an Auger process (see Chapter 6), is present. These aspects of rare-earth-doped semiconductor luminescence are nicely demonstrated in Fig. 5.17, depicting the luminescence of Er3+ ions built into various matrices [16, 17]. The emission is due to 4f11∗ → 4f11 transitions from the excited state 4I13/2 to the ground state 4I15/2 . Comparison of the emission spectra in Fig. 5.17(a), (b) and (c) immediately conﬁrms that the emission of these ions is represented by a relatively narrow line peaking approximately at 1530 nm, regardless of whether they are incorporated in a glass GeO2 –SiO2 matrix or in crystalline or amorphous silicon. Comparison of the emission spectra in Fig. 5.17(c) and (d) further suggests that the intensity of luminescence of Er3+ in hydrogenated amorphous silicon decreases by only about 20% when the temperature increases from 2 K to 300 K. Recently, there has been considerable interest in the luminescence of Er3+ in silicon as the exploitation of such luminescence would allow for the operation of an optoelectronic light source on a silicon basis, a necessity for silicon optoelectronics or photonics. The emission wavelength near 1.53 μm is highly attractive because it lies in the so-called second transmission window of the glass ﬁbres used in optical communications. Apart from the trivalent form, rare earths can be built into the lattice also in the form of divalent ions. In the Eu2+ ion, for example, which is an important activator in a number of phosphors used in applications, luminescence occurs via dipole-allowed 5d → 4f transitions. The reason underlying this difference against the case of Er3+ ions is as follows: the Eu2+ ground state is 4f7 , and it can have for partners in optical transitions both the 4f7∗ excited state and the 4f6 5d excited state. The intensity of the crystal ﬁeld then determines which one of these excited states lies lower in energy; the 4f6 5d level turns out to be the lower one in most Eu2+ -ion-activated phosphors, resulting in

145

Fig. 5.17 Emission spectra of Er3+ ions built into various matrices and measured at different temperatures. (a) A glass GeO2 –SiO2 matrix doped with Al2 O3 (dashed curve) and P2 O5 (solid curve) at T = 295 K. After Martucci et al. [16]. (b) Crystalline silicon matrix at T = 2 K. (c) Hydrogenated amorphous silicon (a-Si:H) matrix at T = 2 K. (d) a-Si:H matrix at T = 300 K. Except for the temperature, the experimental conditions and intensity scales are the same for (c) and (d). Graphs (b)–(d) after Bresler et al. [17].

146

Channels of radiative recombination 4f6 5d → 4f7 being the allowed transition underlying the luminescence in this case. One more difference can be found: the 4f shell is, similarly to trivalent ions, screened from the inﬂuence of the crystal ﬁeld by the ﬁlled 5s2 5p6 shell, but the excited 5d orbital is spatially located outside this shell and as such feels the interaction of the matrix much more strongly. This implies that, on the one hand, the emission spectrum can contain broad bands and, on the other hand, that its spectral position may vary with the chemical composition and spatial symmetry of the matrix. For these reasons, Eu2+ ions provide a wide range of luminescence and absorption bands. The CaF2 : Eu2+ crystal can serve as an interesting example, since it was chosen as the very ﬁrst material for the experimental demonstration of the occurrence of two-photon absorption in solids in 1961. The only laser then available was the ruby laser λ = 694 nm (hν = 1.78 eV); the cubic CaF2 : Eu2+ crystal is transparent at this wavelength and at the same time has a strong absorption band 4f → 5d at 2hν = 3.56 eV. In addition, CaF2 : Eu2+ was known to exhibit intense blue luminescence with a band around 420 nm (∼ 2.95 eV), being due to radiative transitions after the relaxation of the excited electrons. The clever employment of these properties by Kaiser and Garrett [18] led to the actual detection of blue luminescence excited with red ruby laser pulses, with the intensity of this luminescence quadratically rising with the excitation intensity according to (5.24), see Fig. 5.18 (compare with the inset in Fig. 5.16(a)).

Fig. 5.18 Quadratic dependence of the intensity of blue luminescence on red laser excitation in CaF2 : Eu2+ in an original experiment demonstrating two-photon absorption in solids; T = 295 K. After Kaiser and Garret [18].

5.7 Problems 5/1: Derive relations (5.7) and (5.8) by making use of Fig. 5.1. Employ the parabolic approximation E 2 = E c + h¯ 2 k02 /2 m e , E 1 = E v − h¯ 2 k02 /2 m h , along with E 2 –E 1 = hν. 5/2: Relation (5.9) for the luminescence lineshape of electron–hole pair recombination includes a parameter D0 ∼ exp(–E g /kB T ), which increases with rising temperature. Does this mean that the intensity of this luminescence will also rise with temperature? Which important effect was neglected when deriving eqn (5.9)? 5/3: Prove (e.g. graphically) that the halfwidth of the Maxwell–Boltzmann lineshape (5.9) approximately equals 1.8 kB T . a √ √ x (a − x)dx, a ≥ 0, in eqn (5.12). Hint: 5/4: Calculate the integral I = 0

Apply integration by parts and then the substitution x = a sin2 t. (Result: π/2 I = ( 23 sin4 t d t)a 2 .) 0

5/5: Estimate what concentration of donor–acceptor pairs should occur in crystalline silicon so that the discrete D0 –A0 lines appear in its lowtemperature luminescence spectrum. The spectral position of such lines would be determined by the Coulomb term in (5.18). Using Fig. 1.1, ﬁnd the corresponding spectral positions of these lines. Typical binding energies of donors and acceptors in silicon are E D (phosphorus) ∼ = E A (boron) = 45 meV, and consider typical radii rA ∼ = rD ∼ = 3 nm.

References

References 1. Bebb, H. B. and Williams, E. W. (1972). Photoluminescence I. Theory. In Semiconductors and Semimetals (ed. R. K.Willardson and A. C. Beer), Vol. 8, p. 181. Academic Press, New York. 2. Kittel, C. (1976). Introduction to Solid State Physics, 5th edn. John Wiley, New York. 3. Saleh, B. E. A. and Teich, M. C. (1991). Fundamentals of Photonics. John Wiley, New York. 4. Mooradian, A. and Fan, H. Y. (1966). Phys. Rev., 148, 873. 5. Ulbrich, R. (1973). Phys. Rev. B, 8, 5719. 6. Shah, J. (1999). Ultrafast Spectroscopy of Semiconductors and Semiconductor Nanostructures. Springer, Berlin. 7. Thomas, D. G., Gershenzon, M., and Trumbore, F. A. (1964). Phys. Rev. A, 133, 269. 8. Espe, W. (1954). Luminescent Substances in Electrical Engineering (in Czech: Luminiscenˇcn´ı l´atky v elektrotechnice. V´yroba, vlastnosti a pouˇzit´ı). SNTL, Prague. 9. Yariv, A. (1967). Quantum Electronics. John Wiley, New York. 10. Basov, N. G. (1966). International Conference on Physics of Semiconductors, Kyoto 1966. J. Phys. Soc. Japan, 21, Supplement, p. 277. 11. Laibowitz, R. L. and Sack, H. S. (1966). phys. stat. sol., 17, 353. 12. Yano, S. and Ulbrich, B. (2003). Thin Solid Films, 444, 295. 13. Shionoya, S. (1998). Photoluminescence. In Luminescence of Solids (ed. D. R.Vij), p. 95. Plenum Press, New York. 14. Shionoya, S. and Yen, W. M. (eds.) (1999). Phosphor Handbook, p. 141. CRC Press, Boca Raton. 15. Tanabe, Y. and Sugano, S. (1954). J. Phys. Soc. Japan, 9, 753. 16. Martucci, A., Guglielmi, M., Strohh¨ofer, C., Fick, J., Pelli, S., and Righini, G. C. (1999). Germania based sol-gel waveguides doped with Er 3+ . In Innovative Light Emitting Materials. Advances in Science and Technology (ed. P. Vincenzini and G. C. Righini), Vol. 27, p. 197. Techna, Faenza. 17. Bresler, M. S., Gusev, O. B., Kudoyarova, V. Kh., Kuznetsov, A. N., Pak, P. E., Terukov, E. I., Yassievich, I. N., Zakharchenya, B. P., Fuhs, W., and Sturm, A. (1995). Appl. Phys. Lett., 67, 3599. 18. Kaiser, W. and Garrett, C. G. B. (1961). Phys. Rev. Lett., 7, 229.

147

Non-radiative recombination

6 6.1 Transformation of the excitation energy into heat

149

6.2 Creation of lattice defects

157

6.3 Photochemical changes

158

6.4 Problems

159

Luminescence efﬁciency or quantum yield almost never reaches η = 1; even if this were the case, Stokes’ law implies that a portion of the supplied excitation energy is not transformed into luminescence radiation but, during relaxation to the system ground state, changes into other types of energy instead. The relevant transitions are called non-radiative transitions and the relevant electron–hole recombination is called non-radiative recombination. It is mostly an undesirable competing effect, which can even result, under strong pumping, in local overheating and mechanical damage of the material. Depending on the ﬁnal form of the dissipated excitation energy, one can recognize three basic types of non-radiative recombination in semiconductors: 1. recombination when the excitation energy transforms into heat (phonons); 2. recombination leading to a creation of new point defects in the lattice; 3. recombination transforming the excitation energy into photochemical changes of the material under study. The ﬁrst type of non-radiative recombination, which consequently slightly increases the sample temperature, is found most commonly. Within its framework, multiphonon transitions and Auger recombination can be distinguished. Photochemical changes induced by excitation radiation are restricted to only a limited number of compounds such as halides of silver and thallium. Similarly, the formation of lattice defects occurs quite rarely, mainly in some wide-bandgap materials at the border between semiconductors and ionic crystals. Even though the theoretical foundations of non-radiative recombination processes in semiconductors are covered in the monograph by Abakumov et al. [1], in general non-radiative recombination is not as widely studied and understood as the diverse types of radiative recombination.

Transformation of the excitation energy into heat

149

6.1 Transformation of the excitation energy into heat 6.1.1 Multiphonon recombination The simplest idea that comes to mind under the concept of ‘multiphonon nonradiative recombination in semiconductors’ is probably as follows: an excited electron near the bottom of the conduction band, a hole near the valence band maximum and the entire excitation energy is—instead of being emitted in the form of photons hν ∼ = E g owing to radiative e–h recombination—handed over to the lattice through n phonons with energy ¯hω: Eg = n¯hω, as depicted in Fig. 6.1(a). Actually, it is a non-radiative analogy of bimolecular recombination, discussed in Section 3.3. However, this process is highly improbable. From the perturbation theory point of view, it is an nth order process and for its probability 1/τnr a relation like 1/τnr ≈ exp(–E g /¯hω) ≈ exp(–n) can be foreseen. For a typical semiconductor with Eg ≈ 2 eV and ¯hω ≈ 25 meV we obtain n = 80, therefore, the corresponding probability is negligibly small and decreases with increasing forbidden gap E g . Moreover, expression (5-9b) implies that the probability of the radiative transition, considering its proportion to ν 2 , increases strongly in this case with the value of hν(≈ E g ). Therefore, there are two reasons why wide-bandgap semiconductors outperform, as far as the luminescence efﬁciency is concerned, those with a narrow bandgap. The probability of such free electron–hole pair non-radiative bimolecular recombination would increase substantially if a deep energy level occurs

Fig. 6.1 (a) Non-radiative bimolecular recombination of free electron–hole pairs across the bandgap via multiple phonon h¯ ω emission. This process in fact does not occur in reality. (b) Non-radiative transition in a localized luminescence centre C → X → A through the emission of many local phonons h¯ ω(‘cooling transitions’). The centre is assumed to be in strong interaction with the lattice (high local change in the coordinate Q e0 –Q g0 ). (c) Non-radiative transition into the ground electronic state C → C → C → C → A inside a localized centre that has only a weak interaction with the lattice (Q e0 ≈ Q g0 ). The non-radiative recombination is mediated by a deep level d. The thermal activation energy of the transition is denoted by E B .

150

Non-radiative recombination approximately in the middle of the bandgap; this process will be discussed in the next subsection. Now we shall pay attention to how non-radiative multiphonon transitions can be applied in a localized luminescence centre. Actually, we have already addressed the problem for the case of strong exciton– phonon coupling in Section 4.6, with the help of Fig. 4.8(b); its salient features are reproduced here as Fig. 6.1(b). The ordinate of the intersection point X lowers with increasing difference Q g0 – Q e0 (i.e. with increasing exciton– phonon binding) and so does the activation energy E A . The excited centre then reaches point X easily and then, down the trajectory X → A, it may pass non-radiatively to the ground electronic state, emitting local phonons. Notice that the phonon emission here has a character substantially different from the (hypothetical) non-radiative bimolecular recombination depicted in Fig. 6.1(a). While in Fig. 6.1(a) multiphonon emission would be mediated by ‘virtual’ electron levels (much like, for instance, two-photon absorption) and therefore it would be a pure process of nth order perturbation theory, in the case of a localized centre, on the other hand, it proceeds by sequential application of one-phonon processes with participation of a real intermediate level.1 The probability of such processes is then incommensurately higher, and non-radiative recombination of the localized centre via local phonon emission becomes very efﬁcient, provided the centre is in strong enough interaction with the lattice. If the localized centre interacts with the surrounding lattice only very weakly (e.g. rare earth ions), then Q g0 ≈ Q e0 (Fig. 6.1(c)) and the point of intersection X in fact does not exist. In this case, non-radiative recombination with manyphonon emission also becomes improbable, similarly to the case of a free electron–hole pair depicted in Fig. 6.1(a). Apart from other things this is one of the reasons why rare earth ions represent efﬁcient luminescent centres if embedded into any lattice, as we have already discussed in Section 5.6. Here, a very important factor mediating non-radiative recombination proves to be a deep level lying approximately in the middle of the bandgap, which corresponds to a defect located in the vicinity of the luminescent centre. It is signiﬁcant that a defect associated microscopically with the deep level is always in strong interaction with the surrounding lattice, therefore the conﬁgurational coordinate changes from Q e0 to Q d0 during transfer of the excitation energy to this defect (Fig. 6.1(c)). This allows for a gradual dissipation of the electron excitation energy via ‘cooling transitions’ C → C → C . From here, the remaining energy ‘spills’ into the matrix by a pathway of similar character C → C → A, thus completing the non-radiative relaxation of the excited luminescence centre via multiphonon emission. The non-radiative recombination mediated by a defect is sometimes called Shockley–Read recombination. It is worth realizing that, at the same time, the radiative channel of this centre may not be completely blocked (τr → ∞). The transition C → D in Figs 6.1(b) and 6.1(c) comprises the emission of a luminescence photon; transitions to the deep level can therefore be accompanied by weak broadband 1 Such transitions are sometimes called ‘cooling transitions’ because they lead to a decrease of the non-equilibrium amplitude of the vibrations in the excited electronic state, therefore to a decrease of the high effective temperature.

Transformation of the excitation energy into heat luminescence. However, the intensity of such luminescence strongly decreases with decreasing thermal activation energy E B (Fig. 6.1(c))—in other words, the stronger the interaction of the deep defect with the surrounding matrix, the weaker is the luminescence connected with this deep level. We assumed tacitly that the luminescence centre was photoexcited via a path A → C, see Fig. 6.1(c). The excitation energy, however, can be supplied to the centre also via capturing injected free carriers (the case of injection electroluminescence). This presumes, however, a sufﬁcient electric conductivity of the surrounding lattice. Luminescence quenching of this type does indeed occur in light-emitting diodes [2]. What is the microscopic basis of the non-radiative centre constituting the deep level? In many cases this is not known precisely. It may be dislocations or vacancies in the bulk of the semiconductor, or recombination in the proximity of the interface between two materials may be involved (dislocations caused by different lattice constants, aggregated impurity atoms). Nevertheless, what is especially worth mentioning is the so-called surface recombination. Surface recombination is a speciﬁc non-radiative recombination in solidstate phosphors, which takes place only in a thin subsurface layer and is conditioned by the occurrence of deep localized levels located within the forbidden gap (sometimes called Tamm levels or Tamm surface states). It is known that these levels, related to surface electron states, owe their origin to perturbation of the ideal translation symmetry of the inﬁnite lattice by the crystal surface. More exactly, from the microscopic point of view it is unoccupied (dangling) bonds of surface atoms in a semiconductor that give rise to these levels. For the sake of simplicity let us assume an intrinsic semiconductor, excited with a generation rate G. The situation is depicted in Fig. 6.2(a). As a consequence of the existence of the deep levels under discussion, the non-radiative recombination (see Fig. 6.1(c) or possibly Fig. 6.5) will be strongly inhomogeneous along the x coordinate normal to the surface, assuming a maximum at x = 0. This means, however, that the photocarrier concentration n(x) just under the surface will decrease signiﬁcantly, thus creating a concentration gradient driving photocarriers to the surface. Kinetic equations describing the generation and recombination processes then will, in comparison with previous considerations, incorporate an additional term arising from the diffusion current density |j| = –D| grad n(x)| = –D∂n(x)/∂ x, where D stands for the diffusion coefﬁcient of the carriers.2 We now analyse a steady-state regime, i.e. we apply the kinetic equations for ∂/∂t = 0. The diffusion term, containing a derivative with respect to the space coordinate x, thus enters the kinetic equations through Fick’s second law in the form of – ∂/∂ x(–D∂n(x)/∂ x). Thus instead of equation of the type (3.4) we have D

d2 n(x) n(x) − = −G, dx 2 τ

(6.1)

2 Carrier diffusion is in this case governed by slower (heavier) carriers which, via Coulomb interaction, slow down the motion of their faster partners and ensure the electric neutrality of the photoexcited electron–hole system.

151

152

Non-radiative recombination where, considering the steady state conditions, we substituted the total derivative d/dx for the derivative partial ∂/∂ x. Let us remind ourselves that τ is the (total) non-equilibrium carrier lifetime. When solving eqn (6.1) we apply the following boundary condition which tells us that the surface recombination described by the recombination rate S determines the value of the derivative of n(x) at x = 0 according to relation dn(x) = S n(x) |x=0 . (6.2) D dx x=0 Note that S is expressed, as follows from (6.2), in cm/s. An example of the solution of eqn (6.1) using the boundary condition (6.2) is graphically demonstrated in Figs 6.2(b) and (c). Panel (b) shows a strongly inhomogeneous photoexcitation proﬁle G = α I0 exp(–αx) under the common case of one-photon excitation. The second boundary condition here reads n(x → ∞) = 0. Panel (c) refers to the case of a constant excitation proﬁle G = const connected with the second boundary condition n(x → ∞) = Gτ . This may occur, e.g. under two-photon laser excitation or in electric injection in luminescent diodes. It is observed that in both cases a marked decrease of the concentration n(x) close beneath the surface, indeed, occurs which may

Fig. 6.2 Illustration of surface non-radiative recombination. (a) Schematic of photoexcitation and deep levels within the forbidden gap in the proximity of the surface. (b) Proﬁles of the generation rate G(x) ∼ I0 exp(–αx) and of the excited carrier concentration n(x) under one-photon excitation. (c) Carrier concentration proﬁle n(x) under a constant generation rate G = const (e.g. two-photon excitation). Parameters L = (Dτ )1/2 (diffusion length), τ and S were chosen the same for both (b) and (c).

Transformation of the excitation energy into heat give rise to a luminescent ‘dead layer’ with strongly reduced luminescence intensity. The width of this layer can range—depending on the values of the parameters α, τ , S, D—from units to hundreds of micrometres. It should be mentioned that in order to demonstrate clearly the effects depicted in Figs6.2(b) and (c) a rather high surface recombination velocity (S = 106 cm/s) had to be chosen. Under the condition G = const the subsurface decrease of n(x) is more prominent and penetrates deeper. This fact can, on the one hand, be favourable in two-photon luminescence spectroscopy because it contributes to suppressing the spurious surface extrinsic radiative channels (Section 5.5). On the other hand, in applications—light-emitting semiconductor devices—the subsurface dead layer should be regarded as an undesirable effect which decreases the luminescence efﬁciency. In order to suppress the surface recombination special arrangements of the diode active layer are used. In general, the surface nonradiative recombination rate can be reduced by application of various passivation techniques which can decrease substantially the concentration of the subsurface recombination centres in the bandgap.

6.1.2 Auger and bimolecular recombination Non-radiative Auger recombination in semiconductors can be considered parallel to the Auger effect known from electron spectroscopy of atoms and solids or from X-ray generation. In this process, an incident high-energy electron ejects another electron from an atomic core level; if some electron from an outer shell falls into the created vacancy, one X-ray photon is emitted. However, the ﬁlling process of the vacant state can also result in another outcome: the excitation energy is not released in the form of an emitted X-ray photon but, instead, is handed over to another electron from the same outer shell, ejecting it out of the atom. It is obviously a competing non-radiative process accompanying the X-ray generation. As regards electron–hole pair recombination in semiconductors, an analogous Auger process is depicted in Fig. 6.3. It requires the presence of three quasi-particles, either two electrons and one hole (process eeh, see Fig. 6.3(a)) or two holes and one electron (process ehh from Fig. 6.3(b)). The energy released by one electron–hole pair recombination is transferred to the third quasi-particle which is then ‘catapulted’ either higher to the conduction band (e) or lower to the valence band (h). The energy of the recombining pair is passed to the third quasi-particle as its kinetic energy, and for this reason the Auger recombination is sometimes classiﬁed as an independent category of non-radiative transitions, characterized by the fact that the electronic excitation energy is—instead of being emitted as a luminescent photon—delivered to another electronic excitation. In the end, however, the kinetic energy of the third quasi-particle spills very rapidly (in picoseconds or their fractions) into the crystalline or amorphous matrix by multiphonon emission (Fig. 6.3, right column); the ultimate form of energy is therefore again heat. The ejected ‘hot quasi-particle’ (Auger quasi-particle) releases energy by relaxing to lower allowed energy levels in the respective band, taking advantage of the quasicontinuous character of these states.

153

154

Non-radiative recombination

Fig. 6.3 Intrinsic non-radiative Auger recombination: (a) electron–electron–hole (eeh); (b) electron–hole–hole (ehh).

During the Auger process, obviously both energy and quasi-momentum conservation laws have to be satisﬁed. The schematics on the right-hand side of Fig. 6.3 show that the Auger process can occur both with (a) and without (b) involvement of a quasi-momentum conserving phonon h¯ k; the no-phonon Auger process becomes feasible provided the ejected quasi-particle has to its disposal a suitable energy band, attainable without the alteration of wavevector of the (i.e. k = 0). The latter alternative does not happen frequently; the ﬁrst type of Auger process (k = 0) is more common. The Auger mechanisms depicted in Fig. 6.3 can be called intrinsic because their occurrence is not conditioned by the presence of a defect or impurity. A )−1 to be characteristic Let us choose a rate of the non-radiative process (τnr of the Auger recombination. Then we remember the bimolecular recombination described by eqn (3.9) dn(t) = G − βr n p − βnr n p, dt

(6.3)

where G is the generation term and βr (βnr ) stands for the radiative (nonradiative) bimolecular recombination coefﬁcient, see also Fig. 3.3. The Auger effect is a three-particle process, unlike two-particle recombination depicted in Fig. 3.3. We can therefore expect that Auger recombination will be described by a term ∼ np 2 and instead of (6.3) it is possible to write d p(t) = G − An n 2 p dt dn(t) = G − Ap n p 2 dt

(eeh),

(6.4a)

(ehh),

(6.4b)

depending on whether the process (a) or (b) in Fig. 6.3 is under consideration. The so-called Auger coefﬁcients An , Ap in eqn (6.4) will be related to the rate of non-radiative Auger recombination if we rewrite this equation in the form

Transformation of the excitation energy into heat dp p =G− A , dt τnr n

(6.5a)

dn n =G− A . p dt τnr

(6.5b)

155

By comparing eqns (6.4a), (6.4b) with (6.5a), (6.5b) we obtain 1 τnrAn

= An n 2 ,

1 A

τnr p

= Ap p 2 .

(6.6)

Typical values of the Auger coefﬁcient in semiconductors are of the order of A ∼ 10−31 –10−29 cm6 /s, exceptionally (for the no-phonon process k = 0) up to 10−26 cm6 /s. The quadratic dependence of (τnrA )−1 on the carrier concentration in eqn (6.6) signiﬁes an important fact: the intrinsic Auger effect occurs mainly for high concentrations of free carriers. The (eeh) is type is expected to be found mainly in n-type semiconductors, while (ehh) is predominantly in p-type materials. Non-radiative Auger recombination obviously plays an important role in luminescence processes under high excitation and also whenever multiple free electron–hole pairs are localized in a small volume, e.g. in nanocrystals. Auger lifetimes τnrA for n, p = 1018 cm−3 are of the order of 10−6 s, but for n, p = 1019 cm−3 they drop to only 10−8 s (!). It is worth noting that intrinsic Auger recombination contributes to the fact that luminescence of narrow-bandgap semiconductors is weak. The reason is that easy thermal generation of free carriers across the bandgap leads to a relatively high free carrier concentration already in unexcited material. In addition to intrinsic Auger recombination, there also exists extrinsic Auger recombination when carriers localized at impurities also play a role. An example of such a process is displayed in Fig. 6.4: a non-radiative process accompanying luminescence originating in the transitions (e–A0 ) and (h–D0 ) and therefore decreasing its efﬁciency. Again a high concentration of free carriers or impurity atoms is essential here because the interaction of, for example, a free electron with an electron localized on a donor must occur, which is conditioned by the close proximity to each other. A slightly different type of extrinsic Auger process (accompanying bound exciton recombination) will be discussed in Chapter 7. Let us now return to the question of non-radiative bimolecular recombination of free carriers. We know that bimolecular recombination, both radiative and non-radiative, is characterized by the quadratic nature of the recombination terms in kinetic equations of the type (6.3) or (3.9). We have already noted that the probability of such non-radiative processes in an ideal pure semiconductor (Fig. 6.1(a)) is in fact zero. In spite of this, it has been discovered experimentally that bimolecular non-radiative recombination occurs in a wide range of materials. We will show that the reason for this may lie in the existence of strongly localized states approximately in the middle of the bandgap (a suitably located ‘deep level’) and their co-actions with Auger recombination. (One therefore deals with the extrinsic effect because deep levels are due either to a defect or an impurity.) This mechanism has been proposed by Juˇska et al. [3].

Fig. 6.4 Extrinsic nonradiative Auger recombination competing with radiative transitions (e − A0 ) and (h − D0 ). Compare with Fig. 5.7.

156

Fig. 6.5 Bimolecular nonradiative recombination mediated by a deep level (with concentration N ) in the forbidden band in cooperation with Auger recombination of electrons (n) and holes ( p) in respective extremes of the valence and conduction bands. h¯ k stands for quasi-momentum change, h¯ ω is phonon energy.

Non-radiative recombination The process is clariﬁed by the schematic sketch in Fig. 6.5. Its basis consists in Auger recombination of free electrons and holes in relevant bands; however, the ﬁnal state of the transition of the particle releasing energy becomes the deep level within the forbidden gap. At the same time, if this energy state is strongly localized in r-space, it is strongly delocalized in k-space, which facilitates automatic satisfaction of the quasi-momentum conservation law. The probability of such processes is therefore high. Furthermore, its rate in comparison with the Auger recombination across the full bandgap (Fig. 6.3) is enhanced because of the smaller required change k in the Auger particle wavevector (for the Auger recombination matrix element MA we have MA ≈ 1/(k)2 ). Let N be the concentration of the localized states, n = p the concentration of the excited free carriers and n N the momentary concentration of electrons on the localized level; the corresponding kinetic equations for electrons read dn = −An n 2 (N − n N ) dt

(6.7)

and for holes dp = −Ap p2 n N = −Ap n 2 n N . dt We eliminate n N : An dn dn = −An n 2 N − , dt Ap dt dn An = −(An N ) n 2 , 1+ dt Ap dn An N =− n 2 = −βnr n 2 . dt (1 + An /Ap )

(6.8)

Therefore, the process depicted in Fig. 6.5 indeed has a bimolecular character, as reﬂected in the quadratic dependence ∼ n 2 . If An = Ap = 10−27 cm6 /s (k = 0, the Auger coefﬁcients therefore have high values) and N = 1018 cm−3 , we get from (6.8) for the bimolecular coefﬁcient of non-radiative recombination βnr = 5 × 10−10 cm3 /s, a value in order-of-magnitude agreement with both experiment and the typical magnitude of the radiative bimolecular coefﬁcient βr , see Section 3.3. Let us emphasize that the effective functioning of this model assumes a relatively high concentration of the deep traps, because there has to be a positive value (N – n N ) on the right side of eqn (6.7). This model was originally proposed for amorphous silicon where the role of the deep levels is played by valence band tail states, which fulﬁl the above condition. Also a relatively high excitation is indispensable because it is in principle necessary to fulﬁl another condition n, p > N in order to ensure a sufﬁcient concentration of electrons and holes in the extremes of the bands during rapid carrier capture in the deep trap.

Creation of lattice defects

6.2 Creation of lattice defects The principle of this excitation energy dissipation lies in the following mechanism: An electronic excitation is localized at some atom occupying a regular lattice position. Relaxation of such an excited atom into the ground state can proceed in the following way: the released excitation energy is transferred to the relevant atom as a whole, which is thus ‘kicked off’ into an interstitial lattice position, creating a so-called Frenkel defect (a vacancy plus an interstitial atom). This defect can be either transient or permanent depending on whether the interstitial atom does or does not return into its original lattice site once the excitation is terminated. In order to make this non-radiative recombination process possible, the following criteria must be fulﬁlled, [4]: (a) Localization of the electronic excitation must occur. Expressed quantitatively, the lifetime of such an excitation at the atom in question must be higher than the effective vibration period of the lattice, because the creation of the Frenkel defect is conditioned by relatively slow displacements of surrounding heavy atoms or ions. Strong localization of the excitation happens most easily if photoexcited electrons and holes or excitons move slowly throughout the crystal lattice. This occurs most probably when they have high effective masses, thus polarons with non-zero coupling constants αe , αh (Table 4.2) appear to be good candidates. It can be shown that the polaron mass m ∗p is connected with the effective mass of a ‘bare’ quasi-particle m ∗ by the expression m ∗p =

1 − 0.08α 2 α ∗ ∗ m ≈ 1 + m , 1 − α/6 + 0.0034 α 2 6

(6.9)

therefore m ∗p > m ∗ (the approximation on the right side holds for α ≤ 0.5). Such a localized excitation is usually called a self-trapped exciton; we will address self-trapped excitons in the next chapter. One can immediately infer from Table 4.2 that the creation of self-trapped excitons is to be expected in II–VI and I–VII semiconductors, which have considerable ionic binding, a strong exciton–phonon interaction and a relatively wide forbidden gap. (b) Energy criterion. The energy of the self-trapped exciton E e (which does not differ too much from the bandgap width E g ) must of course be higher than the energy E d of formation of the defect Eg ≥ Ee > Ed .

(6.10)

The energy E d required by an atom or ion to jump to an interstitial position is very weakly dependent on the type of semiconductor and is mostly in the range of 1.5–3.5 eV. Relation (6.10) tells us, in accordance with criterion (a), that the creation of a lattice defect is mainly a feature of wide-bandgap semiconductors with a high fraction of ionic binding. (c) Protection against degradation to heat—phonons. Local vibrations in the vicinity of an atom around which the self-trapped exciton gets localized

157

158

Non-radiative recombination must have a frequency ω higher than the highest LO-phonon frequency LO , i.e. ω > ω LO , which guarantees that phonons do not ‘spread’ the ωmax

max localized energy over the whole crystal. The phonon mode concerned must thus belong, referring to Fig. 4.7(d), among the so-called local modes, resulting from an increase of the effective spring constant f = M ω 2 around the localized excitation; redistribution of the charge density accompanied by changes of the equilibrium atom positions may indeed often lead to the required increase of f . (d) Orientation criterion. The self-trapped exciton (its charge density) should have a suitable symmetry in the crystal lattice so that the creation of the interstitial atom is energetically favourable. An example of a semiconductor material in which such defect formation owing to the localized electronic excitation very probably occurs is AgCl. Here, the exciton–phonon interaction is so strong that a self-trapped exciton (in the form of an autolocalized hole on a silver ion (AgCl6 )4− in the lattice, which subsequently attracts a photoelectron via Coulomb interaction) is created at low temperatures very rapidly (in the order of picoseconds). In addition to radiative recombination, presenting itself as a broadband bluegreen luminescence, this localized exciton can recombine also non-radiatively causing the relevant Ag+ ion to be pushed out (probably only transiently) into an interstitial position. Therefore a Frenkel defect is created. Interstitial silver ions Ag+ in silver halides can also be created by heating; these materials are characterized by a rather high concentration of these interstitial ions, about 1013 –1014 cm−3 at room temperature. Their presence, hand in hand with their mobility, plays a fundamental role in photolysis and the formation of latent photographic images.

6.3 Photochemical changes In silver halides AgCl, AgBr and AgI at sufﬁciently high temperatures (T ≥ 200 K) there exists, besides defect formation, another channel dissipating energy of the optically created electron–hole pairs. A photoelectron becomes captured at a certain ‘photosensitivity centre’ while a hole gets localized on a Cl− ion. The captured electron then attracts an interstitial Ag+ ion which is able to diffuse rather freely through the lattice (the diffusion coefﬁcient of the Ag+ ions at room temperature is of the order of 10−12 cm2 /s, while that of Cl− ions is by several orders lower, basically unmeasurable). A neutral Ag0 atom results, and successive trapping of other electrons and Ag+ ions may lead to the growth of a metallic silver cluster—a seed of the latent photographic image: Ag+ → Ag0 → Ag− → 2Ag0 → 3Ag+ → 3Ag0 → 3Ag− . . . e

e

Ag+

Ag+

e

e

(6.11)

Sufﬁcient mobility both of the electrons and of the interstitial metal ions, Ag+ (the speciﬁcity of silver halides resides just in this) is therefore essential, and also a sufﬁciently high temperature is required because the ion mobility grows exponentially with T . The captured holes neutralize the Cl− ions and chlorine

Problems

159

gas leaks out, at least from the surface layers of the crystal. Therefore, a photochemical dissociation of the solid occurs. At low temperatures (T ≤ 100 K) the motion of the interstitial Ag+ obviously becomes strongly limited (‘freezes’), the formation of the latent image fades away and silver halides become, on the contrary, relatively efﬁcient phosphors. Their properties under UV irradiation are then very stable. (Hardly anybody is aware of the impossibility of taking photographs at cryogenic temperatures.) There exists a rather wide range of temperatures (100–200 K) where all three actions, i.e. radiative recombination, defect formation and photochemical reaction, may coexist. It is interesting that, although silver halides have been widely used in photography for as long as 150 years, a detailed understanding of all the steps in the reaction described by scheme (6.11) is still lacking. In particular, what is not fully clear is the microscopic nature of the primary photosensitivity centres. Similar photographic processes occur, nevertheless with much lower efﬁciency, in halides of lead (PbCl2 ), thallium (TlCl, TlBr) and mercury (Hg2 Cl2 , Hg2 Br2 ); all these materials show luminescence in the visible region at low temperatures.

6.4 Problems 6/1: If a bimolecular radiative recombination ∼ βn 2 and Auger non-radiative recombination ∼ An 3 are simultaneously active in a semiconductor, the non-equilibrium carrier concentration n(= p) is driven by the kinetic equation dn = −β n 2 − A n 3 . dt In the case when non-radiative recombination prevails (i.e. β An), it will be possible to detect a very weak luminescence, whose kinetic behaviour will be described by the equation dn/dt ∼ =–An 3 . Show that the luminescence decay curve can then be expressed as I (t) = I (0)/[1 + 2AI (0)t/β], where I (0) = βn 2 (0) is the intensity at time t = 0. 6/2: Quick graphical test of the type of recombination mechanism. From the experimentally measured curve of a luminescence decay I (t) (Fig. 6.6) it is possible to deduce the dominating type of carrier recombination by making use of the following method: We plot the curve on a semilogarithmic scale and at several points we draw a tangent, thereby obtaining several values of its slope tan α. Then we plot ln | tan α| as a function of ln I (t). If this plot is constant, independent of I (t), the dominating recombination is monomolecular, if it constitutes a straight line with slope 1/2 then a bimolecular recombination dominates, and a straight line with slope 1 indicates that non-radiative Auger recombination prevails. Prove this. (Hint: Start from the explicit expressions for I (t). Employ the results of Problem 6/1.) 6/3: Discuss the experimental methods applied to study the Auger effect in semiconductors according to [2]; see also [5].

Fig. 6.6

160

Non-radiative recombination

References 1. Abakumov, V. N., Perel, V. I., and Yassievich, I. N. (1991). Nonradiative recombination in semiconductors. In Modern Problems in Condensed Matter Sciences, Vol. 33 (ed. V. M. Agranovich and A. A. Maradudin). North Holland, Amsterdam. 2. Pilkuhn, M. H. (1981). Light emitting diodes. In Handbook on Semiconductors (ed. T. S. Moss), Vol. 4 (ed. C. Hilsum), p. 539. North Holland, Amsterdam. 3. Juˇska, G., Viliunas, M., Arlauskas, K., and Koˇcka, J. (1995-I). Phys. Rev. B, 51, 16668. ˇ B. and Luˇscˇ ik, A. C. ˇ (1989). Decay of electronic excitations with defect 4. Luˇscˇ ik, C. formation in solids (in Russian: Raspad elektronnych vozbuˇzdˇenij s obrazovaniem defektov v tverdych telach). Nauka, Moskva. 5. Dziewior, J. and Schmid, W. (1977). Appl. Phys. Lett., 31, 346; Benz, G. and Conradt, R. (1977). Phys. Rev. B, 16, 843.

Luminescence of excitons

In an ideal pure semiconductor, the primary electronic excitation is a free electron–hole pair, the energy required for its creation (supplied, for example, by an incident photon) being equal—at the very minimum—to the bandgap value E g . In a simpliﬁed way, an exciton may be visualized as a couple consisting of an electron and the associated hole, attracted to each other via Coulomb forces. Therefore, such a bound electron–hole pair no longer represents two independent quasi-particles and its internal energy is lower than E g . The exciton is thus a quasi-particle representing the lowest electronic excitation in a semiconductor. There exist three basic types of excitons: 1. Frenkel exciton or a small-radius exciton. The spatial extension of the excitation is approximately restricted to a single unit cell. These excitons are to a large extent localized at a speciﬁc atom or molecule, and their movement through the crystal is limited to a hopping mechanism. They occur in molecular crystals. 2. A charge transfer exciton occurs primarily in ionic crystals. One can imagine its creation as follows: An electron is transferred from a lattice anion to a nearest neighbour cation, thereby creating there a maximum of the electron charge density. The radius of the charge transfer exciton can therefore be somewhat larger than that of the Frenkel exciton. 3. Wannier exciton or a large-radius exciton. The electron and hole are separated over many lattice constants, the exciton wavefunction is strongly delocalized and the exciton can move freely inside the crystal. Such a quasi-particle is also called a free exciton. The free exciton transfers the excitation energy, however, not the electric charge, because—as a whole— it is electrically neutral. Wannier excitons occur mainly in semiconductors. The annihilation of an exciton is accompanied by a characteristic luminescence due to radiative recombination of the electron with the hole. In this chapter, we shall explain in detail the concept of the Wannier exciton and expound how it manifests itself in luminescence. Afterwards, we shall discuss the characteristic features of luminescence of the so-called bound excitons (i.e. excitons localized at impurity atoms or self-trapped owing to the strong exciton–phonon interaction).

7 7.1 Concept of the Wannier exciton

162

7.2 Bound excitons

180

7.3 Problems

201

162

Luminescence of excitons

7.1 Concept of the Wannier exciton The Wannier exciton can be conceived, in a ﬁrst approximation, as a weakly bound electron–hole pair at which an electron and a hole circulate around each other; the attractive force results from the Coulomb potential U (r ) = −

Fig. 7.1 (a) Schematic of the Wannier exciton in a two-dimensional crystal lattice with lattice constant a. Here h¯ K stands for the quasi-momentum belonging to the translational movement of the exciton centre of mass, and the effective masses of the electron (e) and hole (h) are denoted m e and m h , respectively. (b) The exciton dispersion relations E = E(K). Optical absorption transitions are also marked; ‘non-vertical’ transitions are not allowed. (c) An incorrect plot of the exciton levels within the energy band scheme of a semiconductor (see text).

e2 , 4πε0 ε r

(7.1)

where r is the electron–hole distance and ε stands for the dielectric constant of the substance. A striking resemblance with the hydrogen atom is already evident at ﬁrst sight; the role of the proton is played here by the hole. If we regard the electron and hole as point charges characterized by their charge and effective masses (the so-called effective mass approximation), we can apply a modiﬁed Bohr model of the hydrogen atom. We shall see that this illustrative approximation can explain the majority of the principal features observed in the optical spectra of Wannier excitons in semiconductors. Let us rotate the electron around the hole (which is always heavier, see Fig. 7.1(a)), thus circulating an orbit with radius r given by eqn (7.1). With regard to the Bohr radius of the hydrogen atom aB ≈ 5 × 10−2 nm, however, we encounter here two factors which impose the necessity of rescaling this characteristic length. Firstly, now we have a substantially different ratio of the (effective) masses. Unlike the pair of a light electron and a very heavy proton, the exciton is composed of two light quasi-particles with comparable masses m e , m h which entails a lower stability of the exciton in comparison with the hydrogen atom, and thus to a larger radius of the electron orbit. Secondly, the attractive electrostatic force between the electron and hole in a semiconductor is shielded by the dielectric constant ε,1 which reduces further the attractive force and results in an increase in the orbital radius. It turns out that we may write ε ε rn = (7.2) aBn = n 2 aB , (m r /m 0 ) (m r /m 0 ) where n = 1, 2, 3, . . . is the principal quantum orbit number, m r = (m e m h )/ (m e + m h ) is the reduced mass of the exciton and m 0 stands for the free electron mass. The commonly understood Bohr radius of the hydrogen atom aB corresponds to the ground state, i.e. to the quantum number n = 1(aB ≡ aB1 ). Considering typical values ε ≈ 10 and (m r /m 0 ) ≈ 0.1 for a semiconductor, an order-of-magnitude estimate of the Wannier exciton ground state radius thus yields aX ≡ r1 ≈ 100aB ≈ 5 nm. Let us rescale in a similar way the binding (or ionization) energy of the hydrogen atom. It is well known that this energy, commonly known as one Rydberg, amounts to 13.6 eV and refers to the ground state of the hydrogen atom. Let us denote Ry(H) = 13.6 eV. As noted above, the low value of the 1 A completely independent issue is whether the static ε or high-frequency ε s ∞ dielectric constant is to be applied. This question has not yet been clariﬁed up to now. It depends on whether the volume occupied by the exciton is large enough in order to be regarded as a homogeneous dielectric. Most frequently, the so-called Haken correction which interpolates between εs and ε∞ is used.

Concept of the Wannier exciton Table 7.1 The binding energy and Bohr radius of free excitons in selected semiconductors. The width (E g ) and type (d–direct, i–indirect) of the bandgap are indicated. Semiconductor

Binding energy E X (meV) experimental

CuCl CuBr Cu2 O ZnS AgBr GaN ZnO TlCl AgCl TlBr GaP ZnSe CdS ZnTe CdSe CdTe GaAs InP Si Ge GaSb InSb SiC

190 108 150 36 ∼ 22 28 61 23i , 11d 23 19i , 9d 18 19 30 13 15 10.5 4.2 5.1 14.7 4.15 2.8

Radius aX (nm)

E g (eV) i/d

calculated 0.7 1.25 0.5

23 ∼ 58

∼3 3.1

2.6i 4.1d 21 20 28 13 15 12 4.9 4.8 14.7 4.17 2 0.4

4.5 2.7 5.5 5.4 6.7 13 12 4.9 11.4 23 100

28

3.395 d 3.077 d 2.17 d 3.78 d 2.71 i 3.49 d 3.44 d 3.22i/3.42d 3.27 i 2.66i/3.02d 2.35 i 2.8 d 2.58 d 2.39 d 1.83 d 1.60 d 1.52 d 1.42 d 1.17 i 0.74 i 0.81 d 0.23 d 2.42i

reduced mass (m r /m 0 ) along with the high dielectric constant reduces the stability of the exciton. The exciton energy levels are therefore expected to lie markedly closer to the ionization continuum in comparison with the hydrogen atom: E X(n) =

(m r /m 0 ) 1 EX Ry(H) = 2 . ε2 n2 n

(7.3)

The binding energy, denoted E X in eqn (7.3), corresponds to the exciton ground state n = 1, therefore E X ≡ E X(1) =

(m r /m 0 ) Ry(H). ε2

(7.4)

A typical value of E X thus amounts to E X ≈ (0.1/102 ) × 13.6 eV ≈ 13 meV. The Wannier exciton binding energy is therefore of the order of tens of meV. The exciton is stable only if the attractive potential (7.1) is strong enough to prevent the exciton from breaking up owing to collisions with phonons. The binding energy E X must thus be higher than ∼ k B T . Because the value kB T = 10 meV is associated with T ≈ 110 K, one comes to the important conclusion that excitons in semiconductors occur only at low temperatures. Table 7.1 summarizes the basic exciton parameters in selected semiconductors.

163

164

Luminescence of excitons To understand the next properties of the Wannier exciton, we have to go a step beyond the effective-mass approximation. From the point of view of wave–particle duality, it is possible to describe an exciton by its wavefunction and to tackle the problem of ﬁnding its stationary energy states using the standard methods of solid-state quantum theory [1, 2]; they lead to expressions (7.2) and (7.3). The exciton wavefunction, which is constructed as a linear combination of atomic functions of the crystal, has the same translational symmetry as the crystal lattice. The larger or smaller extent of the exciton’s spatial localization (corresponding to its Bohr radius aX ) is described in quantum mechanics by the so-called envelope wavefunction. Free excitons may thus move throughout the lattice. The following quantities are associated with such a translational movement: the exciton wavevector K, quasi-momentum h¯ K and kinetic energy E kin = h¯ 2 K 2 /2(m e + m h ). Considering eqn (7.3), the total exciton energy can then be written in the form (m r /m 0 ) Ry(H) h¯ 2 K 2 + . 2 2 ε n 2(m e + m h ) (7.5) For the ground state, n = 1, energy we thereby get E (n) (K) = E g − E X(n) + E kin = E g −

E (1) (K) = E g − E X +

h¯ 2 K 2 h¯ 2 K 2 , = Eg − EX + 2(m e + m h ) 2m exc

(7.6)

where m exc = m e + m h is the total (or effective) exciton mass. Here, it is necessary to stress that, in addition to low temperatures, also sufﬁcient purity of the crystal is essential for free excitons to exist. That is, the impurity atoms represent very efﬁcient traps for the free excitons propagating through the crystal, which then get localized at the impurities (losing their kinetic energy) and bound excitons are created. Equations (7.5) or (7.6) are nothing but the dispersion relations of a free exciton. They are depicted in Fig. 7.1(b). This ﬁgure looks very similar to a commonly used representation of the semiconductor band structure, just some extra discrete exciton levels within the bandgap appear. However, there is a substantial difference—the common energy band scheme of a semiconductor follows from the so-called one-electron approximation in which one chosen test electron moves in the effective potential of electric forces exerted by all of the other electrons and periodically arranged atomic cores. The exciton concept goes beyond this one-electron approximation because it takes into consideration the extra inﬂuence of a positive hole. Therefore, the scheme in Fig. 7.1(b) no longer belongs to the one-electron approximation and the K = |0 point cannot be identiﬁed with the top of the valence band; it represents the ground state of the whole ideal pure crystal where all the spin and orbital electron momenta are compensated. What may be somewhat misleading is that these exciton levels can in fact be formally drawn also into the one-electron scheme, which is depicted in Fig. 7.1(c). Even if one can meet similar pictures in renowned textbooks, this approach is not fully accurate and might lead to an incorrect interpretation of such schemes, as we shall see in Chapter 8.

Concept of the Wannier exciton

7.1.1 Absorption spectrum of the Wannier exciton Before we set about the exposition of exciton luminescence (i.e. light emission) properties accompanying the annihilation of the exciton, we describe how the creation of an exciton due to the absorption of an appropriate incident photon manifests itself in the optical absorption spectra of semiconductors. Let us ﬁrst consider a direct-bandgap semiconductor. It is well known that the onset of the absorption edge here is described (in the so-called dipole approximation and without considering the exciton effects) by the square-root law [2–4] α(hν) ≈ (hν − E g )1/2 ,

hν ≥ E g .

(7.7)

The photons possessing energy hν smaller than the bandgap width E g therefore should not be absorbed at all. In fact, however, very distinctive absorption lines at certain discrete energies hν < E g are observed experimentally at low temperatures. Their origin is depicted by the upward arrows in Fig. 7.1(b), namely, they arise from transitions from the |0 state to the n = 1 state (creation of the exciton in its ground state) and to the higher exciton levels n = 2, 3, . . . This is thus the characteristic and famous hydrogen-like series in the absorption spectra, comprising lines at energies hν = E g −

EX , n2

n = 1, 2, 3, . . . ∞;

(7.8)

the band-to-band absorption to the states labelled in Fig. 7.1(b) as ‘continuum’ begins by transitions to n = ∞. It becomes clear by comparing (7.5) and (7.8) that the excitons created by this kind of light absorption have zero kinetic energy. In other words, the excitons at K = |0 are created by vertical transitions. The question arises as to whether also ‘non-vertical’ transitions as indicated in Fig. 7.1.(b) can occur. The answer is no; they cannot, because the relation λ a holds between the optical wavelength λ = c/ν and the lattice constant a. The magnitude of the photon wavevector 2π/λ is therefore negligible compared with the characteristic dimension of the Brillouin zone 2π/a and, consequently, the quasimomentum of the absorbed photon, is not sufﬁcient to ensure the necessary change of K required for the non-vertical transition. Such a transition would thus have to incorporate a third quasi-particle—phonon—and the absorption act would then be classiﬁed as a higher-order process, the probability of which is many orders of magnitude lower. A textbook example of the direct-bandgap absorption spectrum in the exciton region is given in Fig. 7.2 (pure GaAs at T = 1.2 K) [5]. Two additional important facts follow from this ﬁgure. Firstly, the intensity of the absorption lines drops with increasing n (proportionally to ∼ 1/n 3 ), and, secondly, the optical absorption for hν ≥ E g becomes enhanced under the inﬂuence of excitons (the absorption edge shape without considering the exciton effects, as given by eqn (7.7), is depicted by the dashed line). In a direct-bandgap semiconductor in which the dipole transitions in the vicinity of the absorption edge are not allowed owing to the symmetry of the wavefunction in the band extrema (Cu2 O), the absorption spectrum has

165

166

Luminescence of excitons

Fig. 7.2 Optical absorption spectrum of a very pure GaAs sample at T = 1.2 K in the vicinity of the absorption edge. Marked absorption lines, leading to the creation of the free exciton in the state n = 1, 2 and 3, dominate the spectrum. Absorption into higher exciton states merges gently into the absorption continuum; the value of the forbidden gap E g = 1.5194 eV is determined by extrapolating the series to n = ∞. The dashed line at the bottom right represents the absorption edge shape (hν–E g )1/2 expected in the absence of the electron–hole interaction. D0 –X stands for the absorption on residual impurities. After Weisbuch and Benisty [5].

Fig. 7.3 Exciton dispersion relations in a semiconductor with indirect bandgap of width E gi . The arrows indicate optical absorption transitions from the |0 point. The inset shows the relevant electronic band structure in the one-electron approximation.

a somewhat different character (the line intensity decreases proportionally to (n 2 –1)/n 5 and the n = 1 line is missing). However, the marked absorption lines still dominate the spectrum. In indirect-bandgap semiconductors, however, a substantially different spectral dependence around the onset of the intrinsic absorption edge occurs. The situation is schematically depicted in Fig. 7.3. The K = |0 point again represents the crystal ground state, however, the exciton dispersion curves have a minimum at Ki = |Kc –Kv |, where Kc (Kv ) stands for the wavevector of the conduction (valence) band extremum, respectively; see the inset in Fig 7.3. A stable exciton can be created only when the group velocities of the electron and hole are the same; only in this case can the electron and hole move together as a bound pair. Since the electron or hole group velocity in the band is equal to Vg =

1 ∂E , h¯ ∂k

(7.9)

the claim for equality of the group velocities (zero gradient) will undoubtedly be fulﬁlled in the valence Kv and conduction Kc band extrema, therefore the

Concept of the Wannier exciton

167

exciton created with a minimum energy will be characterized by the wavevector K i = |Kc –Kv |.2 The onset of optical absorption should thus turn up at the photon energy hν = E gi –E X (transition (1) in Fig. 7.3). However, because now a phonon h¯ ω with a wavevector |Kc –Kv | must obviously participate in the absorption process in order to meet the quasi-momentum conservation law, the threshold value of the photon energy will shift to hν = E gi –E X + h¯ ω (we consider only low temperatures and hence the phonon emission into the lattice reservoir). Besides, the values of the absorption coefﬁcient will be much lower compared with direct-gap semiconductors and—what is most important—there is no reason to observe any absorption lines, because the transitions (2) in Fig. 7.3 will have the same probability as the transition (1), both types of process being of the same order. Then the density of states in the exciton bands, proportional to [E–(E gi –E X(n) )]1/2 , enters the play and the absorption coefﬁcient will increase with increasing hν starting from the threshold values E gi –E X(n) + h¯ ω. Such a spectral course of the absorption coefﬁcient is schematically depicted in Fig. 7.4(a). Instead of discrete lines, it contains characteristic ‘shoulders’ at the energies E gi –E X(n) + h¯ ω. An example of a simple experimental exciton absorption spectrum of an indirect-bandgap semiconductor (AgBr) is shown Fig. 7.4(b) [6]. In reality, the experimental spectrum often shows a somewhat richer structure than that displayed in Fig. 7.4(b)—for instance in Si and Ge—as a consequence of the higher number of various types of participating phonons. Then, however, the analysis of such a spectrum is not an easy task. Fig. 7.4 (a) Schematic drawing of the low-temperature exciton absorption spectrum in an indirect-bandgap semiconductor. (b) Measured temperature dependence of the exciton absorption spectrum in AgBr. The drawing (a) corresponds to the curve recorded at T = 4.7 K. The value of (E gi + h¯ ω) ≈ 2.714 eV (determined with the help of the binding energy value E X ≈ 22 meV established from other measurements) is indicated. As the temperature rises, a shift of E gi towards lower energies occurs on the one hand and, on the other, absorption processes with phonon annihilation begin to operate, resulting in the occurrence of another shoulder red-shifted by 2h¯ ω. Thence it is possible to determine the energy of the quasi-momentum conserving phonon: h¯ ω ∼ = 8 meV (TO(L)). After Joesten and Brown [6].

2 In direct-bandgap semiconductor K = K = 0 holds and thus the exciton is created at c v K = |0, in accordance with the previous discussion.

168

Luminescence of excitons It is worth noting that the transitions of type (2) result in the appearance of excitons with non-zero kinetic energy, unlike direct-bandgap semiconductor where the resonant condition (7.8) leads to the creation of excitons with zero kinetic energy. However, it is important to realize that in both the types of semiconductors, excitons with non-zero kinetic energy can be created easily by optical absorption in the ‘non-resonant’ way. By means of photons hν > E g one creates free electron–hole pairs which are very quickly, in the order of picoseconds, bound to excitons. These thermalize rapidly, getting rid of the excess energy through the emission of phonons into the lattice. Such an exciton gas can be described statistically by its kinetic energy distribution with a certain effective temperature, as was explained in Section 5.3.

7.1.2 Direct bandgap: resonant luminescence of free exciton–polaritons Looking at Fig. 7.1(b), an idea about exciton luminescence may cross our mind, namely, that luminescence transitions accompanying exciton annihilation can be depicted simply by turning upside down the arrows pointing up from |0 to n = 1, 2, . . . . In the emission spectrum thereby a series of lines fully analogous to the lines shown in the absorption spectrum in Fig. 7.2 will appear (at least, it works like this in the case of a hydrogen atom). Unfortunately, this is not quite true. Here, the difference between a gas of noninteracting hydrogen atoms and the collective properties of the solid state will reveal itself, as well as the inﬂuence of residual impurities which are present even in nominally pure undoped semiconductor materials. The situation around the luminescence of free excitons thus becomes rather complicated. The luminescence photon, created during exciton annihilation due to the radiative recombination of the electron with a hole, will be resonantly reabsorbed while travelling through the lattice (the absorption coefﬁcient for exciton absorption lines is very high – see Fig. 7.2) and transformed back into an exciton; this exciton, when its lifetime is out, annihilates emitting a photon which is again reabsorbed, and so on. Such an oversimpliﬁed ‘mechanistic’ view is evidently untenable; however, it points to the fact that the concepts of the exciton and photon inside a solid can hardly be separated from each other. We speak of a mixed electronic-polarization and optical wave propagating through the crystal, for which the term polariton (not to be confused with polaron!) or more strictly exciton–polariton is used.3 A more solid idea about polaritons and their luminescence can be obtained from the graphical representation of their dispersion curves E(K). The dispersion curves of the exciton E(K) = E g –E X + h¯ 2 K 2 /2m exc and of a √ bare photon E(K ) = hν = h¯ c K / ε∞ (i.e. the straight line with slope √ h¯ c / ε∞ ) without considering the above mentioned interaction are schematically depicted in Fig. 7.5(a). Both curves must necessarily cross each other. However, it is known that in a degenerate quantum system, the degeneracy is 3 Analogously, one can encounter a phonon–polariton in the infrared part of the spectrum in polar crystals.

Concept of the Wannier exciton

Fig. 7.5 √ (a) Dispersion curve of a ‘bare’ exciton and ‘bare’ photon (straight line with slope of h¯ c( ε∞ )−1 ), i.e. without considering their mutual interaction. (b) Schematic of the exciton–polariton dispersion curves. ΔLT stands for the longitudinal-transverse exciton splitting. (c) Thermalization of LPB polaritons owing to the cascade emission of optical (h¯ ωO ) and acoustic (h¯ ωA ) phonons. (d) Schematic of the luminescence spectrum of polaritons.

lifted owing to the interaction. Here, it means simply that a splitting of the curves in the vicinity of this point of intersection will appear, as suggested in Fig. 7.5(b). Moreover, the so-called longitudinal-transverse splitting ΔLT of the exciton gains importance in polar cubic semiconductors, in analogy with the energy difference between LO- and TO-phonons (Section 4.2). The resulting polariton dispersion curves are drawn by solid lines in Fig. 7.5(b). One can indeed recognize around the intersection point a region having the character of mixed exciton-photon states, while far from this point the curves have a character very similar to a bare photon (the so-called ‘photon-like’ straight lines with a slope close to the value of h¯ multiplied by the light velocity) or to a bare exciton with the characteric parabolic dependence E ∼ K 2 . The entire dispersion curve is then composed of two branches, namely, the upper polariton branch (UPB) and the lower polariton branch (LPB). The existence of these two branches and, in particular, of the strong LPB curvature around the point where the ‘photon-like’ straight line turns into the ‘exciton-like’ parabola ∼ h¯ 2 K 2 /2m exc , is essential for understanding the shape of the polariton emission spectra. This region in the (E, K) plane is often termed a bottleneck. Let us consider a common situation during which the polaritons are created (non-resonantly) via absorption of photons with energy high above the bandgap as, for example, at A point in Fig. 7.5(c). Thermalization of these polaritons runs initially—far away from the ‘bottleneck’—very efﬁciently via emission of the optical phonons possessing a high energy h¯ ω0 at K ≈ 0; close to the bottleneck, however, the scattering to lower energy states can be mediated only via emission of the acoustic phonons with very low energy h¯ ωA . Naturally, the thermalization process is slowing down signiﬁcantly and a considerable accumulation of the polariton population on the LPB in the vicinity of the bottleneck will occur. A similar accumulation is likely to happen also near the bottom of the UPB. After a lapse of their lifetime of the order of

169

170

Luminescence of excitons 10−9 s, these accumulated polaritons ‘recombine’ to give rise to a no-phonon4 exciton–polariton luminescence that, localized spectrally in the close vicinity of hν ≈ (E g –E X ), emerges from the crystal. The emission spectrum thus consists, according to what has just been said, of two lines separated by ∼ LT . This is schematically depicted in Fig. 7.5(d). The line originating from the LPB branch is usually more intense, as may be inferred from thermodynamic considerations. It is necessary to emphasize, however, that no simple analytic formula describing the corresponding spectral lineshape like, e.g., eqns (5.9) or ( 5.13) exists, in spite of numerous attempts to deduce such a lineshape formula theoretically. It may be interesting to mention that this spectral shape actually complies with the original simple concept of the excitonic luminescence reabsorption— the central part of a narrow emission line is (seemingly?) reabsorbed and only both of the wings survive (see also Appendix H). Figure 7.6 shows an example of the experimental emission spectrum of the exciton–polariton in GaAs at T = 4.2 K [7]. The thick arrow marks the position of the n = 1 absorption line (i.e. hν = E g –E X ), taken from Fig. 7.2. A qualitative agreement with Fig. 7.5(d) is evident. The above discussed model of the exciton–polariton luminescence was reﬁned by Koteles et al. [8] who noticed that the occurrence of the ‘UPB/LPB doublet’ was affected to a large extent by the concentration of residual impurities, in particular donors. The authors assume that all the excitons, after having thermalized, accumulate exclusively on the LPB branch and, accordingly, their luminescence spectrum should consist of a single line only. However, if donors are present at a relatively high concentration (≥ 1015 cm−3 ), the exciton–polaritons are scattered on their way from the bulk by elastic collisions just with these donors (not by acceptors because their Bohr radius—which means, in this case, their effective scattering cross-section—is

Fig. 7.6 Luminescence spectrum of free exciton–polariton X in very pure GaAs at T = 4.2 K (impurity concentration of the order of 1013 cm−3 ). Lines due to the upper (UPB) and lower (LPB) polariton branch in the n = 1 state are clearly evident. The thick arrow marks the position of the absorption line n = 1. The line labelled (h–D0 ) is caused by the recombination of a hole with a neutral donor (Section 5.3); lines (D0 –X) and (A0 –X) are due to recombination of bound excitons (Section 7.2). On the right, a weak indication of a line arising from recombination of the n = 2 state of the exciton–polariton can also be seen. After Razeghi et al. [7].

4 That is, phonons do not participate in the actual emission process. However, it is possible to conceive of a process (depicted by the lower wavy line in Fig. 7.5(c)), during which emission of another phonon h¯ ω0 occurs and, at the same time, the polariton moves to the photon part of the dispersion curve. This means that the radiative decay of the exciton–polariton is accompanied by emission of an optical phonon. We shall treat this mechanism shortly.

Concept of the Wannier exciton

171

substantially lower!). This scattering leads, according to detailed calculations, to a ‘hole burning’ in the luminescence line proﬁle and to the emergence of the doublet. In sufﬁciently pure samples polariton scattering does not occur. Very convincing support for this theory is given in Fig. 7.7, which depicts three photoluminescence spectra of nominally undoped epitaxial GaAs layers with different residual donor concentrations. Incontestably, the free exciton (X) line splitting fades away with increasing sample purity. The effect seems to be conﬁrmed by more and more frequent observation of a simple and intense luminescence line at the n = 1 position of the free exciton also in other materials, e.g. InP (Fig. 7.8) [9]. This tendency is likely to be closely related to the incessant improvement of a wide range of preparation techniques of ultrahigh-purity semiconductors, such as molecular beam epitaxy (MBE) or metal organic vapour phase epitaxy (MOVPE), etc. Figures 7.6–7.8 can serve as examples of a photoluminescence assessment of the semiconductor purity that shows a considerable application impact, and is de facto a unique and irreplaceable method used even in the microelectronics industry. Application of this photoluminescence impurity analysis in the case of silicon, where it even gives quantitative information, will be discussed in detail in Subsection 7.2.2.

7.1.3 Direct bandgap: luminescence of free excitons with emission of optical phonons The previous subsection might have evoked an impression that the entire spectral manifestation of free exciton luminescence in a direct-bandgap semiconductor is characterized by a kind of not-very-exactly deﬁned lineshape which often almost disappears in the background of plenty of other emission lines. Nevertheless, there exists another intrinsic free exciton recombination channel in direct-bandgap semiconductors, signiﬁcant especially in II-VI type semiconductors, namely, luminescence with simultaneous emission of LO-phonons (possibly TO-phonons, as well). Speciﬁc for this channel is a pronounced emission line (or even a series of lines) with a well-deﬁned spectral shape. This process, as we have already mentioned, is depicted by the lower wavy line in Fig. 7.5(c). From here we can at once estimate the spectral position of the relevant line as hνX−m LO ≈ (E g − E X ) − m h¯ ω0 ,

m = 1, 2, 3, . . .

(7.10)

This relation formulates nothing but the law of energy conservation, expressing that the lines are shifted, with respect to the exciton–polariton resonant line (or ‘doublet’), towards lower energies by a multiple of the phonon energy h¯ ω0 . (Figure 7.5(c) shows this recombination for m = 1 only.) In the literature these lines are sometimes marked as A–LO, A–2LO, . . . , or X–LO, X–2LO, etc. Their intensity is relatively high but, at the same time, the reason for this is not obvious at ﬁrst sight—after all, one deals with a process incorporating the participation of a third quasi-particle and thus its probability to occur should

Fig. 7.7 Emission spectra of three undoped epitaxial layers of GaAs with different residual donor concentrations. The bottom spectrum belongs to the sample with the highest concentration of donors, and this concentration decreases towards the middle and upper spectra. At the same time it can be seen that the free exciton-polariton line (X) is losing its splitting into the UPB and LPB. Bath temperature is 5 K. Labelling of the remaining lines is the same as in Fig. 7.6. After Koteles et al. [8].

172 Fig. 7.8 Emission spectrum of a pure epitaxial layer of InP (residual impurity concentration below 1014 cm−3 ). The spectrum is dominated by an unsplit line of the exciton–polariton ground state (Xn=1 ); a weak trace of the ﬁrst exciton–polariton excited state (Xn=2 ) is also present. Other lines on the low-energy side of the spectrum are attributed to recombination of an exciton bound to a neutral donor in the ground state (D0 –X)n=1 , an exciton bound to an ionized donor (D+ –X), exciton bound to a neutral acceptor (A0 –X) and to recombination of a hole with a neutral donor (h–D0 ). Notice that the bound exciton linewidth is much narrower in comparison with the linewidth of the free exciton–polariton; the latter reﬂects the kinetic energy distribution in the free exciton gas. After Bose et al. [9].

Fig. 7.9 (a) Radiative recombination of a free exciton accompanied by emission of one optical phonon. The photon energy is hν ≈ (E g − E X ) − h¯ ω0 , the quasi-momentum conservation law Kexc ∼ = qphoton is satisﬁed. The shaded area labels the Maxwell–Boltzmann distribution of the exciton kinetic energies. In the vicinity of K = 0, a splitting of polariton states into UPB and LPB for both n = 1 and n = 2 is indicated. (b) Corresponding phonon dispersion curves.

Luminescence of excitons

be substantially lower than that of the resonant emission itself. The reasons for this are in fact two: 1. The emitted phonon delivers part of the energy of the decaying exciton– polariton into the lattice, thereby lowering the energy of the luminescence photon by multiples of h¯ ω0 . The photon may thus escape to a large degree (but not completely) from the bottleneck region and circumvent number the resonant polariton complications (reabsorption and scattering). Therefore, a large number of photons ﬁnally reaches the sample surface and leaves the semiconductor. 2. The participation of phonons makes it possible for all the free excitons residing at the LPB (which have a certain distribution of their kinetic energy 2 /2m h¯ 2 K exc exc characterizing their propagation through the crystal) to take part in the radiative recombination process. This is because the participating phonons ensure the quasi-momentum conservation law Kexc ≈ qphonon to be satisﬁed for the whole exciton population, while it is only exciton– polaritons with virtually zero kinetic energy, i.e. a zero wavevector Kexc = Kphoton ≈ 0, that can undergo resonant no-phonon radiative recombination. Such excitons, however, represent only a small fraction of the whole free exciton population, as shown in Fig. 7.9(a) (see also Problem 7/1). This is therefore the second reason why phonon participation in the emission process substantially increases the (X − mLO) line intensity. (Sometimes one speaks of ‘recoil’ phonons released during the radiative annihilation of excitons.) Now, one can anticipate intuitively that shapes of the emission lines with phonon participation will reﬂect the Maxwell–Boltzmann distribution of the free exciton kinetic energy and will thus be analogous to eqn (5.9). Basically this is the case; nevertheless, some small differences appear. The lineshape should reﬂect in some way the probability of phonon(s) creation W (m) (mqphonon ); this is a new factor that we did not have to take into

Concept of the Wannier exciton

173

account while deriving the relation (5.9); phonons did not participate there. We thus write formally (m) (hν) ≈ (hν − [(E g − E X ) − m h¯ ω0 ])1/2 Isp hν − [(E g − E X ) − m h¯ ω0 ] ×exp − kB T

W (m) (mqphonon ≈ K exc ),

(7.11)

considering simultaneously that the low-energy threshold of the line is given by eqn (7.10). Let us pay attention only to the (X–LO) and (X–2LO) lines, i.e. m = 1, 2. The quasi-momentum conservation law for one- and two-phonon assisted radiative annihilation of a free exciton is depicted in Fig. 7.10. During the one-phonon process (Fig. 7.10(a)), each exciton with a given Kexc can create only phonons with essentially a discrete spectrum of magnitudes of their wavevectors |qphonon |. The important question now reads: will the probability W (1) (qphonon ) be the same for all excitons with different kinetic energy, i.e. with a different vector Kexc ≈ qphonon ? The answer is no, because the moduli of all these vectors are small in comparison with the dimensions of the ﬁrst Brillouin zone, and any of their relative variations |q|/|q|, however small they may be, is important. It can be expected that phonons whose wavelengths are comparable with the linear dimension of the exciton will be emitted most probably; therefore, the modulus of their wavevector will correspond to the modulus of the exciton wavevector. More accurate theoretical 2 . considerations lead to a scaling of the type W (1) (qphonon ≈ Kexc ) ∼ K exc (1) is proportional to the exciton kinetic energy which In other words, W

Fig. 7.10 Vector diagrams depicting the quasi-momentum conservation law during radiative annihilation of a free exciton: (a) with emission of one phonon, (b) with emission of two phonons.

174

Luminescence of excitons is (hν − [(E g − E X ) − h¯ ω0 ]). Therefore, for the (X–LO) process we obtain from (7.11) (1) Isp (hν) ≈ (hν − [(E g − E X ) − h¯ ω0 ])3/2 hν − [(E g − E X ) − h¯ ω0 ] exp − . kB T

(7.12)

We emphasize once more that the scaling W (1) ∼ |Kexc |2 follows from the fact that the moduli of the exciton and phonon wavevectors are in this case comparable. Two-phonon radiative recombination (X–2LO) satisﬁes the quasimomentum conservation law in a slightly different way. The number of corresponding combinations of wavevectors (qphonon , qphonon ) for each recombining exciton is high, and their moduli may be much larger than |Kexc |, as can be seen in Fig. 7.10(b). Such phonons no longer ‘feel’ the spatial extent of the exciton, and one can expect W (2) (qphonon , qphonon ) to be no longer dependent upon the energy or upon the wavevector of the recombining exciton; thus W (2) = const. It is this fact which causes the important difference between the one- and two-phonon process, and from (7.11) it follows immediately that the two-phonon lineshape (m = 2) will be Maxwell-like: (2) Isp (hν) ≈ (hν − [(E g − E X ) − 2h¯ ω0 ])1/2 hν − [(E g − E X ) − 2h¯ ω0 ] exp − . kB T

(7.13)

These qualitative considerations were put forward for the ﬁrst time by Gross et al. [10] and conﬁrmed by quantum-mechanical calculations by Segall and Mahan [11]. Figure 7.11 reproduces (a) one of the ﬁrst published emission spectra by Gross et al. in the spectral range of the (X − m LO) lines in CdS [10], and (b) a comparison of the experiment with the theoretical lineshape (7.12) in CdSe [12]. The second important feature of the emission lines (X–LO), (X–2LO),. . . , contributing to their identiﬁcation, is their intensity dependence. The free exciton recombination, as a typical intrinsic ‘monomolecular’ process, increases with the excitation linearly in a wide interval of excitation intensities (no saturation is observed). We have not yet given a full account of why just the optical phonons have to participate in phonon-assisted free exciton luminescence. In fact acoustic phonons could not make the relevant effect possible because at low values of |qphonon |, their energy is close to zero (Fig. 7.9(b)) and would not be sufﬁcient to release photons from the bottleneck region, or—if you like—to enable them to escape from the resonant reabsorption. The optical phonons have a constant non-zero energy h¯ ω0 in the vicinity of |qphonon | = 0 and do not introduce any additional factor which could complicate the emission lineshape (7.12) or (7.13). But then the ‘legal’ question arises: Is the participation of the ‘welcome’ optical phonons allowed also by selection rules imposed by the crystal symmetry?

Concept of the Wannier exciton

175

Fig. 7.11 (a) Emission spectrum of n = 1 free excitons (9 –7 ) in CdS at T = 4.2 K (lower curve) and T = 42 K (upper curve). The lower curve from the left: a weak resonant line of the exciton–polariton (485.3 nm), a very intense and broad line (486–492 nm, intensity out of scale) due to an exciton bound to a residual impurity, a X–LO line at 492.8, once more an intense line of bound excitons (494–498) nm and ﬁnally a X–2LO line at 500.5 nm. At a temperature of T = 42 K, the lines of bound excitons almost disappear, the free exciton emission dominates the spectrum and the lines X–LO, X–2LO show the characteristic asymmetry described by relations (7.12) and (7.13). After Gross et al. [10]. (b) Comparison of the experimental lineshape X–LO, solid line, with the theoretical one (7.12), dashed line. Crystal CdSe at a temperature of T = 44 K. After Gross et al. [12].

In order to answer this question, a short excursion into the irreducible representations of point groups will be of use [3, 13]. Let α, β, μ be the irreducible representations (in general, of three different point groups of symmetry), corresponding to the wavefunction of the initial and ﬁnal electron states and to the matrix element operator of the corresponding optical transition, respectively. Matrix elements of the type β| μ| α are then non-zero (i.e. the transition is allowed) if and only if the direct product(α ⊗ μ)includes β

(7.14a)

or, equivalently, the direct product( α ⊗ β ⊗ μ)includes a fully symmetric representation1 .

(7.14b)

Next, by using (7.14), we shall ﬁnd the selection rule concerning LO-phonon participation in the excitonic luminescence of a commonly occurring hexagonal wurtzite modiﬁcation of CdS crystals. Let us denote as c the six-fold rotation axis of the highest symmetry. The band structure is schematically shown in Fig. 7.12. The corresponding point group of crystal symmetry is C 6v .

Fig. 7.12 Schematic of the energy band structure of hexagonal wurtzite CdS crystals. Δ stands for the spin–orbit splitting and δ is the splitting of the highest valence band by the crystal ﬁeld. The transitions between three valence bands and the conduction band are usually marked as A, B, C. The emission lines in Fig. 7.11 belong to the A transitions.

176

Luminescence of excitons Because the spin–orbit splitting of the valence band at the point plays an important role here, irreducible representations of the double group are used for labelling the symmetry of the electron states. Let us ﬁrst study the onset of the absorption edge 9 → 7 , neglecting for a while the exciton states. The CdS crystals have a direct bandgap. In the relevant notation, the highest valence band maximum at k = 0 has a symmetry α = 9 , and the conduction band minimum at the same value of k has a symmetry β = 7 . In crystals with the point group C6v , the photon operator for light polarization E ⊥c (in the dipole approximation) transforms according to the irreducible representation μ = 5 . If we calculate the direct product α ⊗ μ = 9 ⊗ 5 employing the character tables of the irreducible representations (or we may consult previously published multiplication tables [3]), we obtain 9 ⊗ 5 = 7 ⊕ 8 . This product contains the representation 7 (= β) and, according to (7.14a), this means the interband transitions in the vicinity of the absorption edge are dipole allowed.5 Finally, let us pursue the luminescence of excitons with phonon participation. Because the interband transitions are dipole allowed, the exciton envelope function must be s-like (λ = 0) with a full 1 symmetry. Therefore, the initial electronic state of the transition is α = 1 ⊗ 7 ⊗ 9

(7.15)

(i.e. a free exciton), the ﬁnal state being the crystal ground state |0, which is certainly spherically symmetric: β = 1 . The overall operator of the transition matrix element transforms like μ = photon ⊗ phonon = 5 ⊗ phonon . In CdS, the LO-phonon has an energy of h¯ ω0 = 37 meV and symmetry 5 . Taking into consideration (7.15) and using the multiplication table we therefore obtain α ⊗ β ⊗ μ = (1 ⊗ 7 ⊗ 9 ) ⊗ 1 ⊗ (5 ⊗ 5 ) = (7 ⊗ 9 ) ⊗ (5 ⊗ 5 ) = (5 ⊕ 6 ) ⊗ (1 ⊕ 2 ⊕ 6 ) = 1 ⊕ 2 ⊕ 3 ⊕ 4 +3 5 +3 6 . From the last expression it is evident that the product α ⊗ β ⊗ μ includes 1 , therefore, according to condition (7.14b), the corresponding transition is allowed. The LO-phonon assisted radiative recombination of free excitons in crystals of CdS type is thus allowed by the selection rules. We shall close this subsection with a brief summary: The participation of optical phonons in free exciton radiative annihilation in direct semiconductors removes polariton effects and leads to the appearance of luminescence lines with a characteristic shape described by relations (7.12) and (7.13). Their intensity dependence is linear in a wide range of excitation intensities. Prominent participation of LO-phonons in exciton luminescence, which cannot be overlooked particularly in II-VI materials, follows from the fact that these phonons have in polar semiconductors the strongest coupling—Fr¨ohlich 5 Sometimes the term ‘ﬁrst-class dipole-allowed’ direct transitions is used; see the book by Peyghambarian, N., Koch, S. W., and Mysyrowicz, A. (1993), Introduction to Semiconductor Optics. Prentice Hall, Englewood Cliffs N.J.

Concept of the Wannier exciton

177

coupling—with excitons (Section 4.2). In I-VII semiconductors, which are even more polar, the LO-phonon assisted luminescence of free excitons also occurs (for example in CuCl), but some of them have an indirect bandgap (AgBr, TlBr) and the mechanism of exciton luminescence is rather different there; we will explain this now.

7.1.4 Luminescence of free excitons in indirect-bandgap semiconductors The ﬁrst important fact affecting quite essentially (and basically in a positive sense) luminescence processes in indirect-bandgap semiconductors is the absence of polariton states. This is documented in Fig. 7.13. The energy minimum of the exciton states is located at the Ki , a point sufﬁciently distant from |0 and the exciton and photon dispersion curves therefore do not cross each other. This phenomenon markedly simpliﬁes the discussion of exciton luminescence in these materials. A second important factor, following from the very nature of the indirect bandgap and also from Fig. 7.13, is the indispensability of participation of non-zero qphonon ∼ = Ki phonons in the radiative recombination process. This is, as we already know, a positive aspect—it enables the whole population of free excitons to recombine radiatively because a suitable ‘recoil phonon’ provides the momentum mismatch ∼ h¯ Ki . This time, however, the approximate equality qphonon ∼ = Kexc is no longer valid, unlike the case of a direct semiconductor. The reason for this consists in the fact that the Ki point is de facto in all known indirect semiconductors situated at the ﬁrst Brillouin zone boundary or in its close vicinity, thus |qphonon | ∼ = |Ki | |Kexc |, as indicated in Fig. 7.13. In this case, as we discussed in the preceding section, the probability W (1) of phonon creation does not depend on qphonon , and it follows immediately from eqn (7.11) that the spectral lineshape of the one-phonon assisted free exciton luminescence will reﬂect exactly the Maxwell–Boltzmann distribution of exciton kinetic energies. Now we can rewrite expression (7.11) as

Fig. 7.13 Dispersion curves of a free exciton and a photon in an indirect-bandgap semiconductor. The polariton states do not exist. On the right: schematic of the exciton luminescence spectrum (INP stands for a no-phonon line).

178

Luminescence of excitons hν − [(E gi − E X ) − h¯ ω] (1) Isp(i) (hν) ∼ , = (hν − [(E gi − E X ) − h¯ ω])1/2 exp − kB T (7.16)

Fig. 7.14 Band structure of AgBr. The valence band maximum at the L point has a symmetryL 3 , and the conduction band minimum with a symmetry 1 is located at the Brillouin zone centre ( point, k = 0). An ion of Br− is placed at the origin of the coordinate system. Energy is plotted in units of Ry(H) ≈ 13.6 eV. After Kunz [14].

where the index (i) indicates the indirect bandgap. Appendix B features in detail the way in which the shape (7.16) or (7.12) can be modiﬁed in experiment by the inﬂuence of a ﬁnite slit width of the spectral apparatus and by so-called phonon broadening. What remains to be considered is what kind of a phonon will take part in the recombination process. In strongly polar crystals of AgBr one would a priori expect participation of an LO-phonon. Surprisingly, this is not the case (that is why we have also omitted the index (0) in the phonon energy h¯ ω in (7.16)). Why? Selection rules arising from the symmetry of phonon and electron states will apply, analogously to Subsection 7.1.3. Crystals of AgBr have a cubic structure belonging to the point group Oh . The valence band maximum is situated at the boundary of the ﬁrst Brillouin zone and has a L 3 symmetry, while the conduction band minimum is at the Brillouin zone centre and has a 1 symmetry (see Fig. 7.14) [14]. A photon in the crystal structure Oh transforms according to the irreducible representation 15 . (Relativistic effects and thus the spin–orbit splitting of the highest valence state in AgBr can be disregarded; thus the electronic states are classiﬁed according to a single point group.) Considering the symmetry of the exciton envelope to be 1 , the initial state of the transition related to the exciton recombination has a symmetry α = 1 ⊗ 1 ⊗ L 3 . The crystal ground state 1 represents the transition ﬁnal state β (thus β = 1 ), and the transition matrix element belongs to the representation μ = photon ⊗ L phonon = 15 ⊗ L phonon . Then, in accordance with (7.14a), the direct product ( α ⊗ μ) = (1 ⊗ 1 ⊗ L 3 ) ⊗ (15 ⊗ L phonon ) = L 3 ⊗ 15 ⊗ L phonon (7.17) must contain β = 1 if the phonon-assisted transition is to be allowed. Because L 3 and 15 are odd representations, L phonon must be an even representation if the direct product (7.17) is to contain an even (1 ) representation. At the L point, AgBr has two types of phonons transforming according to an even representation: L 1 (LA) and L 3 (TO), see Fig. 4.6 (and also Problem 4/4). We perform the multiplication indicated in (7.17), using the tables of irreducible representations of points with symmetries L and [13], for both types of phonons in question: phonon L 1 : (L 3 ⊗ 15 ) ⊗ L 1 = L 3 ⊗ (15 ⊗ L 1 ) = L 3 ⊗ (L 1 ⊕ L 3 ) = 1 ⊕ 2 ⊕ 212 ⊕ 3 25 ⊕ 3 15 ,

(7.18a)

phonon L 3 : (L 3 ⊗ 15 ) ⊗ L 3 = L 3 ⊗ (15 ⊗ L 3 ) = L 3 ⊗ (L 1 ⊕ L 2 ⊕ 2L 3 ) = 2 (1 ⊕ 2 ⊕ 212 ⊕ 3 25 ⊕ 3 15 ).

(7.18b)

Concept of the Wannier exciton Indeed, both eqns (7.18a) and (7.18b) contain 1 on their right side, therefore the participation of both the L 1 (LA) and L 3 (TO) phonons in the radiative recombination of an indirect free exciton in AgBr is allowed. On the contrary, the LO-phonon in AgBr has symmetry L 2 at the L point and therefore its participation in the exciton luminescence is forbidden. Selection rules derived in this way are in perfect agreement with experiment [15], as documented in Fig. 7.15. The dominant line in the low-temperature edge emission of pure AgBr crystals is a TO(L)-phonon replica of free exciton luminescence (ITO (FE)),6 and, in addition, also a markedly weaker line ILA (FE) is present. This is due to the higher density of states of the TO-phonons in the L point along with a stronger coupling of these phonons with excitons over that of TA-phonons. In Fig. 7.15, also the theoretical lineshape (7.16) calculated using h¯ ωTO ∼ = 8 meV, h¯ ωLA ∼ = 12 meV and an effective temperature of T = 10 K is depicted (symbols; the height of the theoretical curves is always normalized to the maximum of the measured line). Agreement between theory and experiment, as far as the lineshape is concerned, appears also to be very good. We point out the characteristic asymmetry towards higher photon energies. In this context, we refer the reader also to Fig. 8.20. Figure 7.15 contains another two interesting pieces of information. Firstly, also a weak line INP (FE) corresponding to the radiative recombination of an indirect free exciton without phonon participation is present. This process is theoretically forbidden in an ideal periodic lattice, however, due to the presence of residual impurities and lattice defects breaking the strictly periodic arrangement of atoms, it becomes partially allowed. Secondly, these residual impurity atoms manifest themselves in the luminescence spectrum very distinctly: free excitons get localized at the impurities, creating bound excitons (BE) which also decay radiatively. The corresponding lines are, contrary to free exciton luminescence, of extrinsic origin and this is reﬂected in their labelling: EXTO (BE), EXLA (BE). It is expected that in this case the intensity ratio ITO (FE)/EXTO (BE) varies signiﬁcantly from sample to sample. In silicon and germanium, similar symmetry-driven selection rules apply like in the case of AgBr. It turns out that in phonon-assisted free exciton radiative recombination in silicon all types of phonons (LO, TO, LA, TA) are allowed. Experimentally, though, only three lines ITA (FE), ILO (FE) and ITO (FE) are observed, as can be seen in Fig. 1.1. The reason for this consists in the degeneration of the LA, LO phonon dispersion curves at the X point of the Brillouin zone (Fig. 4.3), in the close vicinity of which the conduction band minimum in silicon is situated (Fig. 7.16). The weak ILA (FE) line thus de facto merges with the ILO (FE) line. In germanium, two allowed free exciton luminescence lines, namely ILA (FE) and ITO (FE), are observed, again in accord with the selection rules. Here, the spectral lineshape is more complicated due to the exciton ground state splitting (interaction of the anisotropic conduction band minima with degenerate hole states) and non-parabolicity of the density of states. If the theoretical description of the lineshape (7.13) is to be used to ﬁt exactly the experiment, it needs substantial corrections. Further information on this issue can be found in [16, 17]. 6 This labelling is sometimes used in order to stress the intrinsic (I) character of the free exciton (FE) emission.

179

Fig. 7.15 Photoluminescence edge emission spectrum of pure AgBr (residual impurities ≤ 1 ppm) at a bath temperature of T = 4.2 K. Starting from the highest photon energy: a line of no-phonon recombination of a free exciton INP (FE), a TO-phonon ITO (FE) and LA-phonon ILA (FE) assisted luminescence of a free exciton, respectively. Normalized emission lineshapes, calculated using (7.16) with an effective temperature of 10 K, are denoted by circles. (Compare with Fig. 7.13.) The EXTO (BE) and EXLA (BE) lines originate in the radiative annihilation of an exciton bound to an unknown residual impurity. The last three weak lines are two-phonon replicas. After von der Osten and Weber [15].

180

Luminescence of excitons Finally, one important note: Similarly to the case of (X − m LO) lines (Section 7.1.3), a signiﬁcant additional guideline to identify various free exciton luminescence lines in indirect semiconductors is their linear dependence on pump intensity. We shall close this subsection by stressing once more what has already been mentioned repeatedly: a single microscopic luminescence centre in an indirect-bandgap semiconductor may manifest itself through several emission lines of comparable intensities (phonon replicas).

7.2 Bound excitons

Fig. 7.16 Band structure of Si and Ge. In silicon, an indirect forbidden gap E gi ∼ = 1.17 eV is formed between the top of the valence band ( 25 ) and the conduction band minimum situated along the line, close to the X 1 point. In germanium, there is an indirect bandgap 8+ − L + 6 of the magnitude of E gi ∼ = 0.745 eV. Because Ge is heavier than Si, the spin–orbit splitting of the valence band maximum is more distinct and a double group notation is used for labelling the symmetry of the electronic states.

We have already noted that lattice defects, and especially impurity atoms, present in the crystal either intentionally (doping) or as residual impurities which the preparation technology fails to get rid off, make very efﬁcient potential wells—traps—for free excitons. The exciton loses its kinetic energy owing to localization at these traps and such excitons are then called bound excitons (BE), to be distinguished from free excitons (FE).7 Afterwards, a radiative or non-radiative recombination of the bound exciton, accompanied in the former case by emission of a characteristic luminescence photon, occurs again. It is a typical extrinsic luminescence. As a rule, the efﬁciency of the bound exciton luminescence is substantially higher than that of free excitons. Emission spectra of medium-level doped or sometimes also nominally pure semiconductors are usually dominated by the bound exciton luminescence. Why? Two reasons are of importance. 1. First of all, it is the large radius of the Wannier exciton aX itself, representing in this context a large capture cross-section σX for capturing of 2 ≈ 10−12 cm2 if we consider an exciton at the potential well (σX ≈ πaX a typical Bohr radius aX = 5 nm). Let us estimate the mean free exciton lifetime τtr before trapping. Obviously, it is expected that the higher the cross-section σX , the higher the impurity concentration N and the faster the free exciton movement, the smaller is τtr : τtr ≈

1 , σX Nv

(7.19)

where v is the thermal velocity of exciton diffusion through the lattice. Let us assume N = 1015 cm−3 (corresponding to a nominally pure semiconductor, except silicon perhaps, where purity of N ≤ 1011 cm−3 can be reached), σX = 10−12 cm2 and v = 106 cm/s (corresponding to a temperature of approximately 2 K); from (7.19) we obtain τtr ≈ 10−9 s. This value of τtr is comparable with the radiative recombination lifetime τr in direct-bandgap semiconductors. This means the chance of a free exciton in such a semiconductor to emit its characteristic luminescence is roughly the same as that of being trapped at an impurity and then to recombine with emission of BE luminescence. 7 In the case of exciton localization at an impurity atom, the term ‘bound exciton’ is in fact synonymous with the term ‘excited state of the impurity atom’.

Bound excitons

181

In an indirect-bandgap semiconductor τr ≥ 10−4 s holds, thus we get τtr τr . Therefore, the chance of a free exciton to be trapped, forming in this way a bound exciton, is far higher than to recombine radiatively with emitting the characteristic free exciton luminescence (hν ≈ E gi –E X –h¯ ω). This simple estimate implies immediately that the low-temperature free exciton luminescence—for instance in silicon at a doping level of the order of 1015 cm−3 —should not appear at all. Indeed, Fig. 1.1 corroborates this conjecture: The bottom spectrum (C) originates in a sample with a total concentration of boron and arsenic atoms of approximately 8×1015 cm−3 and it is evident that the free exciton lines ITO (FE)/ILO (FE) at ∼ 1130 nm and ITA (FE) at ∼ 1090 nm (i.e. the intrinsic emission) are totally missing, while the extrinsic emission of excitons localized at boron atoms (e.g. BTO (BE), BLO (BE)) is very intense. We will return to this point in more detail in Subsections 7.2.1 and 7.2.2. 2. The bound exciton luminescence is characterized by the so-called ‘giant oscillator strength’, as shown by Rashba and Gurgenishvili [18]. In principle this means that all the unit cells inside a ‘volume’ of approximately 3 around the impurity atom or defect contribute to the radiative ∼ aX recombination of the bound exciton. The probability of this radiative recombination (and, consequently, the relevant oscillator strength f ) is thus increased by several orders of magnitude, and the radiative lifetime τr ∼ 1/ f decreases proportionally. These two effects can also be expressed in the following way: The crystal lattice, serving as a ‘matrix’ for impurity atoms or defects, plays, during photoluminescence processes, the role of an ‘antenna’ that ‘harvests’ the excitation radiation and transfers the excitation energy efﬁciently—with the help of the motion and trapping of free excitons—to the extrinsic luminescence centres. Expressed concisely, photoluminescence is a very sensitive tool to study impurities and defects in semiconductors. How do we identify the bound exciton luminescence in the emission spectrum? One deals with a localized excitation, characterized very often (but not always!) by a small Huang–Rhys factor. This is owing to the large radius of a typical bound exciton, or owing to the fact that the excited area is spread in the host lattice over a considerable volume. Therefore, the spectra are composed of very narrow emission lines (FWHM of the order of 0.1 meV) which, moreover, do not broaden with increasing temperature (because the bound exciton lacks kinetic energy). Figure 7.17 represents the ﬁrst emission spectrum of a bound exciton published in 1960 [19], which clearly demonstrates these characteristic features. A very narrow AsTO (BE) line originates in the TO-phonon assisted radiative recombination of an exciton bound to an arsenic atom (donor impurity in silicon). Its narrow width contrasts sharply with the neighbouring free exciton line ITO/LO (FE), broadened considerably at the experimental temperature of T = 25 K. A narrow no-phonon line of the bound exciton AsNP (BE) is also present. There are two additional important features contributing to the reliable identiﬁcation of the extrinsic bound exciton luminescence. The ﬁrst one is the

Fig. 7.17 The ﬁrst published emission spectrum of a bound exciton: crystalline silicon containing an arsenic impurity with a controlled concentration of 8 × 1016 cm−3 (full line) in comparison with a silicon sample containing negligible concentration of impurities (dashed line). Silicon doped with arsenic shows a new line AsTO (BE) due to radiative decay of excitons bound to As atoms. An intense ILO/TO (FE) line is a ﬁngerprint of the free exciton luminescence; AsNP (BE) denotes no-phonon emission of the bound exciton. After Haynes [19].

182

Luminescence of excitons linear intensity dependence with the expected tendency to saturation at higher excitation power densities, as outlined in Section 3.5. Next, the speciﬁc spectral position of the bound exciton line may be considered to be the second feature. Because the free exciton during its localization hands over part of its energy to the surroundings (and the rest is later emitted), the bound exciton emission line must be shifted—with respect to the corresponding free exciton replica— towards lower photon energies. This is clearly demonstrated in Fig. 7.17. In the next subsections we shall explain in more detail the physical origin of this energy shift.

7.2.1 Excitons bound to shallow impurities Shallow donors and acceptors, controlling in a principal way the electric conductivity of semiconductors, are of fundamental importance in semiconductor technology. These impurities can reveal themselves in a characteristic way also in luminescence radiation; this is naturally proﬁtable because it enables the donors and acceptors to be investigated also by optical means. We shall point to the slightly different luminescence behaviour of excitons bound to ionized donors or acceptors, and that of excitons bound to these impurities in a neutral state. Excitons bound to ionized donors (D+ –X) or acceptors (A− –X) This is the simplest type of bound exciton. To describe the processes of free exciton capture and subsequent radiative annihilation of the bound exciton, it is advantageous to use quantum-chemistry notation. Let us thus denote e. . . . . . . . . . . . . . . . . . electron, h. . . . . . . . . . . . . . . . . .hole, ⊕e. . . . . . . . . . . . . . . . neutral donor; also D0 , h. . . . . . . . . . . . . . . .neutral acceptor; also A0 , FE. . . . . . . . . . . . . . . . free exciton, ⊕. . . . . . . . . . . . . . . . . ionized donor; also D+ , . . . . . . . . . . . . . . . . . ionized acceptor; also A− , ⊕ eh. . . . . . . . . . . . . . exciton bound to ionized donor; also (D+ –X) or (D+ , X), eh. . . . . . . . . . . . . . exciton bound to ionized acceptor; also (A− –X) or (A− , X), ⊕ eeh. . . . . . . . . . . . . exciton bound to neutral donor; also (D0 –X) or (D0 , X), ⊕ heh. . . . . . . . . . . . . exciton bound to neutral acceptor; also (A0 –X) or (A0 , X). The capturing event of a free exciton by an ionized donor can be described schematically as ⊕ + FE → ⊕ eh + D1 ,

(7.20a)

where D1 is the dissociation or binding energy of the exciton in the relevant complex. It is thus the energy released by the exciton during localization or, alternatively, the energy required to tear the exciton off the ionized donor and make it free again, i.e. the energy necessary to start the reaction (7.20a) going in the opposite direction. (D1 is not to be confused with the binding energy E X of an electron–hole pair in a free exciton!) The radiative decay of such a bound

Bound excitons

183

exciton ⊕eh, resulting in emission of a photon hνBE , then reads ⊕ eh → ⊕ + hνBE .

(7.20b)

By combining both eqns (7.20) we obtain immediately hνBE = FE − D 1 ∼ = (E g − E X ) − D 1 ,

(7.21)

where the meaning of the spectral shift of the bound exciton line is clear, i.e. the energy separation between the low-energy threshold of the free exciton line and the maximum of the bound exciton line is equal to the dissociation (binding) energy D1 of the exciton at the impurity. Luminescence measurements therefore provide a simple way to ﬁnd out this crucial parameter via optical experiments. Among others, this is important also because theoretical calculations are not able to cope with D1 completely. The problem of fundamental importance related to excitons bound to ionized impurities concerns their existence depending on the ratio of the effective masses of the carriers σ = m e /m h . It appears that neither (D+ –X) nor (A− –X) can exist (i.e. be a stable complex) at arbitrary values of σ . The following qualitative consideration may help us to unravel this claim. In order for the exciton bound to an ionized donor ⊕eh to be stable, it is required that the hole is sufﬁciently heavy (has small kinetic energy), otherwise it will break away from the neutral remainder ⊕e. In other words, the kinetic energy of the hole will surmount the gain in potential energy accomplished during localization of the exciton and the complex (D+ –X) will disappear. The theoretical dependence of the dissociation energy D1 on σ is shown qualitatively in Fig. 7.18. It is seen that there exists a critical ratio σc ∼ = 0.43 and the complex (D+ –X) is stable only for σ ≤ σc . Similar consideration can be repeated also for an exciton bound to an ionized acceptor (A− –X); merely the electron and hole exchanging their roles. Such an exciton will thus be stable for σ > 1/σc ≈ 2.33, as is also shown in Fig. 7.18. (In reality, theoretical computations of the complex stability calculate, in analogy with a H+ 2 molecular ion, a slightly different dissociation energy, namely, the energy needed to break away only a hole, thus a neutral donor remains there, or only an electron, when a neutral acceptor remains.) A more detailed discussion can be found, e.g. in [20]. Several interesting consequences can be extracted from the above exposition: (a) In a given material, there cannot exist simultaneously both (D+ –X) and (A− –X). (b) The existence of (A− –X) in general is very unlikely because, as a rule, the hole is usually heavier than the electron (σ < 1). (c) In silicon (σ ∼ = 0.61), no excitons bound to ionized impurities can exist at all, neither (D+ –X) nor (A− –X). This is illustrated for instance in Fig. 1.1; lines of this origin occur in none of the three panels. (d) In GaAs (σ ∼ = 0.11) and InP (σ ∼ = 0.0944) we ﬁnd σ < σc , therefore the (D+ –X) exciton should exist in these materials, unlike the (A− –X) one. Also this conclusion is conﬁrmed by experiment. The (D+ –X) line can be identiﬁed in the emission spectrum of InP shown in Fig. 7.8; this line

Fig. 7.18 Qualitative illustration of the dissociation energy of an exciton bound to an ionized donor (acceptor)—i.e. the energy needed to tear the free exciton off the complex—as a function of the effective masses ratio σ = m e /m h . The exciton at an ionized donor (D + –X) may exist only for σ ≤ σc ∼ = 0.43, the exciton at an ionized acceptor (A− –X) only for σ > 1/σc ∼ = 2.33.

184

Luminescence of excitons

Fig. 7.19 Emission spectrum of a thin layer of GaAs (prepared by chemical epitaxy in vacuum) at a temperature of T = 2 K. After Bernussi et al. [21].

occurs also in GaAs but coincides spectrally with the (h–D0 ) line (see, e.g., Figs 7.6 and 7.19 [21]). No line which could be attributed to (A− –X) occurs in the mentioned ﬁgures. Excitons bound to neutral donors (D0 –X) or neutral acceptors (A0 –X) Numerous theoretical computations and experiments have shown that excitons bound to a neutral impurity are stable at an arbitrary σ ratio. This is a substantial difference in regard to the previous case. One can speculate qualitatively about the reasons in the following way. An exciton bound to a neutral donor ⊕eeh is—in the limit of a heavy hole σ → 0 (i.e. m h → ∞)—an analogy to the hydrogen molecule H2 , which is a very well known and stable particle with a dissociation energy (the energy necessary for decomposing H2 into two hydrogen atoms) equal to 0.33 Ry(H) = 4.5 eV. By analogy, we can conclude that the dissociation energy E BX of an exciton localized at a neutral donor will be E BX ≈ 0.33 E D , where E D is the ionization energy of the relevant donor. In the opposite limit of a light hole σ → ∞, only the electron part of the exciton is bound to the impurity, which is actually an analogy to the H− ion. This ion is also a stable object with dissociation energy of approximately 0.055 Ry (H); the corresponding exciton binding energy will thus be E BX ≈ 0.055 E D . A variety of interpolations between these two limit cases exist, nevertheless, it appears that E BX , despite passing through a minimum, stays permanently above zero. To describe the creation and subsequent radiative decay of a bound exciton, equations analogous to eqn (7.20) can be written: ⊕ e + FE → ⊕ eeh + E BX ,

(7.22a)

⊕ eeh → ⊕ e + hνBE .

(7.22b)

By eliminating ⊕ eeh we obtain hνBE = FE − E BX = (E g − E X ) − E BX (in a direct-bandgap semiconductor), hνBE = FE − E BX = (E gi − E X − h¯ ω) − E BX (in an indirect-bandgap semiconductor).

Bound excitons The emission line of a bound exciton is thus again red-shifted by an amount equal to the binding (dissociation) energy E BX . As an example we give in Fig. 7.19 the emission spectrum of GaAs at T = 2 K which, being measured in a sufﬁciently wide range of wavelengths, incorporates a number of lines. We have already discussed previously the origin of all of them, starting from the (D0 –A0 ) band at the longest wavelengths and terminating with the polariton emission (X) on the opposite side. At this moment, let us pay attention to the (D0 –X), (A0 –X) and (D+ –X) lines. The binding energy E BX of the (D0 –X) exciton is, as can be deduced from Fig. 7.19, substantially smaller than that of (A0 –X). This is understandable because m h (≈ 0.61 m 0 ) is signiﬁcantly larger than m e (≈ 0.066 m 0 ). What is less understandable at ﬁrst sight is why the (D+ –X) line is more distant from the free exciton line than the (D0 –X) one, or—in our notation—why D1 > E BX . Then, a related question arises as whether a similar relation holds universally in all materials. The answer is: No, it does not. The relation between D1 and E BX depends strongly on the ratio σ , as demonstrated qualitatively in Fig. 7.20. The exciton bound to an ionized donor is, as noted above, a stable complex only for σ < σc ; however, D1 increases rather abruptly with further decrease of σ . On the other hand, it is true that E BX > 0 holds for arbitrary σ but the increase in E BX is rather slow with decreasing σ and both curves cross each other somewhere. Therefore, the relation between D1 and E BX is material-dependent; σ is sufﬁciently small in GaAs as well as in most direct semiconductors and therefore D1 > E BX applies there. There is a very important law related to excitons bound to neutral donors and acceptors, usually referred to as Haynes’ rule. It can be seen in Figs 7.6, 7.8 or 7.19 that the binding energy of excitons localized at acceptors differs in general from that of excitons localized at donors, as we have already discussed. Nevertheless, Haynes in 1960 found out empirically—just with the help of luminescence spectroscopy—an even more delicate relation, namely, that E BX depends on the chemical nature of the donor or acceptor atom. Or, the energy E BX depends (slightly) on whether the exciton is bound to an atom of, for example, phosphorus or arsenic in silicon (both the impurities being donors in silicon). Till now, we have not taken this fact into account in our exposition, in other words, we used the effective mass approximation and we were interested only in the ratio σ = m e /m h of the host material, but the possible inﬂuence of the chemical nature of the impurity was disregarded. Haynes’ rule thus points to the fact that the localized exciton ‘feels’ the chemical identity of the impurity atom and can bear witness to it via the speciﬁc energy of the emitted luminescence photon. This phenomenon is sometimes referred to as the ‘central cell correction’. The standard quantitative formulation of Haynes’ rule in case of donors reads E BX = a + b E D ,

(7.23)

which, expressed verbally, tells that us the binding energy E BX of an exciton localized at a neutral donor increases linearly with increasing binding energy

185

Fig. 7.20 The ratio of the binding energies of an exciton localized at an ionized (D1 ) and neutral (E BX ) donor.

186

Luminescence of excitons

Fig. 7.21 (a) Haynes’ rule: the binding energy E BX of an exciton localized at a neutral impurity as a function of the binding energy of the corresponding donor (E D ) or acceptor (E A ) in Si and GaP. Full lines apply for the linear relation (7.23) in silicon. After Hayes and Stoneham [22]. (b) Modiﬁed Haynes’ 1.6 , rule for donors in GaP: E BX ∼ E D after Herbert [24].

of the donor E D itself. As for donors in silicon, a = 0 and b ≈ 0.1, thus the binding energy of a localized exciton is approximately equal to one-tenth of the binding energy of the donor itself, which corresponds reasonably to the above mentioned estimates based on the analogy with a molecule H2 or ion H− . The dependence (7.23) is plotted in Fig. 7.21(a) [22]. An equation fully analogous to (7.23) holds also for the acceptors in silicon, the only difference being that there appears E A instead of E D and values of the constants a, b will be slightly different. A corresponding plot is also shown in Fig. 7.21(a), together with data relevant to GaP where eqn (7.23) also holds true but a = 0 and, moreover, this parameter has the opposite sign for donors and acceptors. The simple Haynes’ rule in the form of (7.23) was later explained theoretically through a chemical shift of the short-range force potential [23]. Unfortunately, this rule is not of universal validity. It turned out to be inapplicable for example to some III-V compounds such as GaAs or InP. The binding energy E BX differs there for different donors and acceptors non-systematically and only very little. Therefore, if the line due to an exciton bound to a neutral donor is marked simply (D0 –X) in Figs 7.6, 7.7 or 7.19, this means that it may incorporate spectrally unresolved contributions from several donor species. A modiﬁed Haynes’ rule E BX ∼ E D1.6 was proposed for GaP, as shown in Fig. 7.21(b) [24]. This modiﬁcation resulted in particular from extending the

Bound excitons

data in Fig. 7.21(a) to deep donors Ge and O. The validity of Haynes’ rule (7.23) is also commonly not accepted in II-VI semiconductors. Bound multiexciton complexes (BMEC) At the beginning of the 1970s, Kaminskii and Pokrovskii discovered experimentally with the aid of luminescence spectroscopy that more than one exciton can be localized at a neutral donor or acceptor [25]. Later the term bound multiexciton complex (BMEC) became common to denote such objects. Here, the situation differs a bit against single excitons bound to neutral impurities (D0 –X) and (A0 –X), because the existence of (D0 –X), (A0 –X) was predicted theoretically (together with predicting the existence of excitonic molecules— Section 8.2 [26]), while the discovery of bound multiexciton complexes was, from the theoretical point of view, unexpected. A BMEC is created in a photoexcited semiconductor in such a way that one, two, three or more excitons with step by step diminishing binding (localization) energy are successively ‘wrapped around’ a neutral donor D0 or acceptor A0 . They later annihilate radiatively emitting narrow luminescence lines as depicted in Fig. 7.22(a), drawn speciﬁcally for a BMEC at a neutral donor. If m stands for the number of bound excitons, then the energy level of the mth bound exciton is denoted as m BE (m = 1, 2, 3, . . .) in Fig. 7.22.

187 Fig. 7.22 (a) Schematic shell model of a bound multiexciton complex localized at a neutral donor. Transitions denoted αm result from radiative decay of the mth exciton, while the exciton number in the complex decreases to (m – 1). (b) Energy balance for luminescence of a BMEC consisting of two bound excitons. EX stands for either the binding energy of the bound exciton in the case of a direct-bandgap semiconductor ≡ E ) or at no-phonon emission, (E X X = E + h ω for phonon replicas or E X ¯ X in a semiconductor with an indirect bandgap. (c) Low-temperature (T = 4.2 K) emission spectrum demonstrating the occurrence of α1 –α4 lines in a BMEC localized at a phosphorus atom in silicon. The lines are no-phonon (NP) replicas. Also the hypothetic spectral position of a no-phonon free exciton luminescence INP (FE) is depicted. Correlation with the notation used in panel (a) reads PNP (BE) ≡ α1 , PNP (α2 ) ≡ α2 , PNP (α3 ) ≡ α3 , PNP (α4 ) ≡ α4 . In addition to the said lines, the spectrum comprises also a weak no-phonon line As NP (BE) ≡ (D0 –X) originating in exciton annihilation at another neutral donor (arsenic), and also a TA-replica of luminescence of a single exciton bound at phosphorus PTA (BE). The silicon sample was doped by P and As to a total donor concentration exceeding 1016 cm−3 .

188

Luminescence of excitons Conformingly to previous notation 1 BE ≡ (D0 –X). During the radiative annihilation of m BE, an emission line αm arises and the number of excitons in the BMEC lowers by one (m BE → (m–1)BE). The energy balance of the multiexciton trapping and subsequent radiative recombination can be obtained by generalizing relations (7.22): (1)

⊕ e + FE → ⊕ e(eh) + E BX (1) (2) ⊕ e(eh) − E BX + FE → ⊕ e(2eh) + E BX

(1) (2) (3) ⊕ e(2eh) − E BX + E BX + FE → ⊕ e(3eh) + E BX

.. . ⊕ e ((m − 1) eh) −

(m−1)

( j)

(m)

E BX + FE → ⊕ e(m eh) + E BX . (7.24a)

j=1 (m)

In eqns (7.24a), describing the gradual trapping of free excitons FE, E BX (1) stands for the binding energy of the mth localized exciton (E BX ≡ E BX in our previous notation). (m) The radiative decay of the mth exciton leading to emission of a photon hνBE (αm line) proceeds in accordance with the scheme (m) ⊕ e(meh) → ⊕ e [(m − 1) eh] + hνBE ,

(7.24b)

which, by means of the last equation of (7.24a), gives immediately (m)

hνBE = FE −

m

( j)

E BX .

j=1

This relation tells us that the αm lines are shifted with respect to the position of the free exciton emission line FE (= E gi – E X – h¯ ω in an indirect-bandgap semiconductor) by a sum of binding energies of all of the localized excitons. Figure 7.22(b) illustrates the energy balance (7.24) for the m = 1 and m = 2 lines; the notation E X = E X + h¯ ω is introduced there for brevity’s sake. (m) (m−1) Considering that E BX < E BX , the αm lines make a series densifying with increasing m. At the same time, the intensity of these lines decreases, because (m) the number of localized excitons with higher m due to the condition E BX < (m−1) decreases monotonically. This is nicely illustrated in Fig 7.22(c) which E BX displays the low-temperature emission lines α1 –α4 originating from a BMEC at a phosphorus atom in silicon. The schematic displayed in Fig. 7.22(a) represents a considerably simpliﬁed version of the so-called shell model which was put forward by Kirczenow for explaining the luminescence in BMECs [27]. In reality, the levels in Fig. 7.22(a) are split as a result of the higher number of electron and hole states differing slightly in energy. Using a very sensitive detection system with

Bound excitons

189

Fig. 7.23 Photoluminescence spectra of two samples of crystalline Si doped with phosphorus to approximately the same donor concentration NP ≈ 3 × 1014 cm−3 . Bath temperature T = 4.2 K. (a) Continuous-wave excitation 488 nm from an Ar+ -laser (excitation intensity ∼ 20 W/cm2 ), a scanning detection monochromator HRD-1 and a cooled photomultiplier with a photocathode of S1 type. After Pelant et al. [29]. (b) Continuous-wave excitation 514 nm from an Ar+ -laser (estimated excitation intensity ∼ 2 W/cm2 ), detection with the help of a Nicolet Fourier spectrometer with a cooled North Coast Ge detector. The inset shows the enlarged area of NP replicas. After Colley and Lightowlers [30].

a high S/N ratio, one can, in addition to the series of αm lines, observe also weaker emission lines βm —they can be seen for instance in Fig. 7.23(b).8 It is worth noting that the αm lines in Fig. 7.22(c) represent no-phonon luminescence and, surprisingly, are more intense than the corresponding series of lines in the region of TO/LO- or TA-replicas, as one can make sure of by looking at Fig. 1.1(A) where a similar series of phosphorus-related α1 –α4 lines occurs, too. At this point it may appear suitable to make a small deviation in a more general sense: when discussing recombination processes in indirectbandgap semiconductors we encounter certain competition between the conﬁgurational coordinate model and the principle of quasi-momentum conservation (the conﬁgurational coordinate model was introduced in Sections 4.4 and 4.5 by assuming tacitly a direct-bandgap material). As far as silicon donors are concerned, there is a very weak exciton–phonon interaction, thus the Huang–Rhys factor is small (S ∼ = 0.1) implying that the no-phonon lumines(m)

8 True values of the binding energies then differ from those of the quantities E BX introduced by us, and need not satisfy the condition of monotonic decrease with increasing m. Details can be found in Thewalt, M. L. W. (1983). Bound multiexciton–impurity complexes. In Excitons (ed. E. I. Rashba and M. D. Sturge). Modern Problems in Condensed Matter Sciences, Vol. 2, Chap. 10. North Holland, Amsterdam.

190

Luminescence of excitons cence lines of a localized impurity centre (phosphorus atom) are expected to be relatively intense, as indeed is observed experimentally; the ﬁrst phonon replicas are substantially weaker. However, we cannot forget that in an indirect semiconductor this phenomenon is conditioned by relaxation of the quasimomentum conservation law owing to the phoshorus-atom-induced breaking of the lattice translational symmetry. Hereby, the inﬂuence of the indirect bandgap is de facto annulled in this way.9 A similar scheme of energy levels as in Fig. 7.22 (shell model) can be introduced also in the case of a BMEC at a neutral acceptor. A corresponding series of emission lines, characteristic for a BMEC localized at boron in silicon is clearly noticeable in Fig. 1.1(C). Somewhat stronger exciton–phonon coupling in an acceptor-related BMEC causes the ﬁrst phonon replicas to be more intense than no-phonon lines here. The BTO (BE) line, is analogous to a TO-replica of the donor α1 line, BTO (b1 ) corresponds to a TO-replica of the α2 line, BTO (b2 ) corresponds to a TO-replica of the α3 line, etc. Fully analogous notation is used for TA-replicas in Fig. 1.1(C). BMECs were studied in detail mainly in silicon. Lines that can be attributed to radiative decay of a BMEC were observed also in Ge, β-SiC and GaP. These are all indirect-bandgap semiconductors where the occurrence of a BMEC is quite understandable, for two reasons. First, the excitons have a relatively long lifetime in indirect semiconductors (which enhances the probability for trapping of several excitons at one centre), and second is the N -fold degeneracy of the conduction band minimum (N = 4 in Ge and N = 6 in Si) allowing up to 2N electrons to be placed in one molecular orbital without violating Pauli’s exclusion principle. Some emission lines, observed in the direct-bandgap semiconductor GaAs, were also attributed to a BMEC; however, deﬁnitive conﬁrmation of the existence of BMECs in these materials is missing. The radiative recombination of various types of excitons bound to donors and acceptors represents a strong rival channel to the (D0 –A0 ) luminescence.

7.2.2 Quantitative luminescence analysis of shallow impurities in silicon The utilization of low-temperature photoluminescence spectroscopy over the exciton spectral range to determine the concentration of shallow donors and acceptors in crystalline silicon was proposed in 1982 by Tajima [28]. In Table 7.2 we give the wavelengths of the luminescence lines originating in various complexes (D0 –X), (A0 –X) in silicon. These are TO-phonon assisted lines of excitons bound to commonly applied donors and acceptors. As will become clear hereafter, the TO-replicas are those used most frequently for the quantitative luminescence analysis of silicon. 9 Strictly speaking, however, the presence of impurity atoms should also allow the intrinsic no-phonon luminescence of free exciton INP (FE) to appear, like in AgBr, see Fig. 7.15. In spite of this, no line like INP (FE) has ever been reported in silicon; this difference between AgBr and Si is probably given by the much higher concentration of both point and line defects (dislocations) in AgBr.

Bound excitons It follows from Table 7.2 that the spectral positions of the lines characteristic of donors and acceptors vary—according to Haynes’ rule—with the chemical nature of the dopants; the variations range from fractions of nanometres to several nanometres. Such differences are in principle large enough for the individual lines to be distinguished, provided a scanning monochromator with resolving power of R ≈ 5 × 103 is used. However, if there are several types of impurities in a given sample, their lines will very probably merge together due to their natural linewidth and due to possible line broadening by the ﬁnite monochromator slit, and will form an almost irresolvable band. Any effort to identify the individual lines then would not probably attain the target. Fortunately, silicon technology is highly advanced so that a very low level of residual (introduced unintentionally) impurities—down to 1010 cm−3 —can be reached by zone-reﬁning. In order to achieve the desired type and value of electric conductivity, mostly phosphorus (donor) and boron (acceptor), possibly also As, Sb, Al and Ga, are used as dopants. In practise, their concentrations usually range from 1012 cm−3 to 1018 cm−3 and knowledge of the exact values of the concentration is basic information for both the producers and purchasers of Si ingots and wafers. Photoluminescence analysis enabling us to determine such a concentration in the range of approximately 1011 –1015 cm−3 was developed primarily for boron and phosphorus. In this concentration range—i.e. for nominally pure or weakly doped Si wafers—this technique has an important role to play in supplementing the wide range of diagnostic methods (temperature-dependent Hall effect, resistivity measurements, infrared absorption spectroscopy, etc.) being commonly applied at higher concentrations of donors and acceptors. It can be stated that photoluminescence diagnostics is nowadays the only analytic method of weakly doped Si crystals that is used routinely in practice. The essence of the method is very simple and is based on the following use of the emission lines BTO (BE), PTO (BE) and ITO (FE), shown for example in Fig. 1.1 or Fig. 7.23 [29, 30]. It is, undoubtedly, reasonable to assume the Table 7.2 Spectral positions of luminescence lines (TO-replicas) due to excitons bound at various impurities in Si; T = 4.2 K∗) Impurity P As Sb Bi Li B Al Ga In Tl C free exciton

Type SD SD SD SD ID SA SA SA SA SA I –

Wavelength (nm) 1135.13 1135.97 1135.04 1138.32 1133.74 1134.39 1135.60 1136.15 1144.83 1177.59 1164.36 1129.76

∗) SD stands for a substitutional donor, ID interstitial donor, SA substitutional

acceptor, I isoelectronic impurity.

191

192

Fig. 7.24 Calibration curves for the quantitative determination of B and P concentrations in silicon from photoluminescence spectra at T = 4.2 K (dependence of the ratio of intensities PTO (BE)/ITO (FE) and BTO (BE)/ITO (FE) on phosphorus and boron concentrations, respectively). After Pelant et al. [31].

Luminescence of excitons intensities of the lines BTO (BE) and PTO (BE) to be proportional to the relevant concentrations of boron NB or phosphorus NP , respectively. On the other hand, the intrinsic emission ITO (FE) line, as we have already stressed several times, is characteristic of those parts of the crystal where these dopants are not present. The ratio of the line intensities BTO (BE)/ITO (FE) or PTO (BE)/ITO (FE) is surely an increasing function of the concentrations NB , or NP , respectively. If we determine experimentally this dependence (the so-called calibration curve) via luminescence measurements performed on samples with a known content of boron and phosphorus, the dopant concentrations NB and NP in unknown samples can then be determined easily from the relevant luminescence spectra using these calibration curves. An example of such calibration curves is displayed in Fig. 7.24 [31]. It should be stressed that these curves—as shown—are not applicable universally because the intensity ratio of the bound to free exciton lines depends slightly on the excitation power density. Measurements of calibration curves and experimental investigation of samples in which the dopant concentration is to be determined thus have to be always performed using the same experimental setup and keeping all the experimental parameters constant. In this case, it is not even necessary to take into account spectral corrections. The calibration curves in Fig. 7.24 were obtained using the experimental set-up drawn in Fig. 2.2(a). It is worth stressing that the measurement of intensities of the BTO (BE) or PTO (BE) lines alone is not sufﬁcient to determine the unknown concentrations because the overall luminescence intensity is sample-dependent (being affected by surface treatment, reproducibility of the sample position with respect to the optical collecting system, etc.); it is thus always necessary to determine the ratio BE/FE. This fact then speciﬁes the above mentioned limits of applicability of the method: in strongly doped samples (NB , NP ≥ 1015 cm−3 ) the ITO (FE) line becomes undetectable, as clearly demonstrated in Fig. 1.1(C); in very pure samples (NB , NP ≤ 1011 cm−3 ), on the other hand, the BTO (BE) and PTO (BE) lines disappear. While the essence of the method is simple, its experimental realization is not quite trivial. There are several reasons for this. First of all, the luminescence of silicon is very weak, several orders of magnitude below that of direct-bandgap materials (GaAs). Moreover, judged from the point of view of detectors of weak photon ﬂuxes, this luminescence is situated in a very unsuitable spectral range. As for photomultipliers, only types with an S1 photocathode are sensitive in the range 1100–1200 nm, but also for them this wavelengths represent the red limit of their sensitivity. Similar arguments can be applied as for silicon CCD detectors. It is possible to use a germanium detector, however, only special high-sensitive types with efﬁcient noise suppression are suitable (Edinburgh Instruments, formerly North Coast). The problem is all the more difﬁcult because it is necessary to measure the spectra with a high resolution Rreal , therefore with a relatively narrow slit of the spectral apparatus (λ = L −1 ≈ 0.25 nm). The possibility to circumvent the mentioned difﬁculties by using a very intense excitation source (e.g. a pulsed laser) is also out of the question because, under strong pumping, a qualitative change

Bound excitons of the emission spectrum occurs—a novel broad band at ∼1143 nm labelled ILO,TO (EHL) in Fig. 1.1 begins to prevail, whose origin, consisting in radiative recombination of an electron–hole liquid, is discussed in detail in Section 8.4. This band to a large degree masks the lines of bound excitons, particularly in very pure samples. It is therefore necessary to choose a certain optimal level of (continuous) pumping and pay attention to the proper choice of monochromator, detector and also of efﬁcient collection of an optical system. What follows from the above discussed difﬁculties is the particular choice of TO replicas for the method under discussion, because in their spectral range, both the lines originating from the impurities and the free exciton line ITO (FE) are relatively intense. This method can serve as an example to demonstrate clearly some advantages of Fourier luminescence spectroscopy. Figure 7.23 shows a comparison of (a) an emission spectrum obtained in a conventional experimental set-up [29] with (b) an emission spectrum measured by a Fourier spectrometer [30]. It becomes evident that the Fourier-measured spectrum exhibits a markedly higher S/N ratio, even under lower excitation intensity (as reﬂected among others in the total absence of the ILO,TO (EHL) band). The accuracy achieved in the Fourier approach is substantially better (± 10%) compared with that obtained with a scanning monochromator (± 30%). The sensitivity in the Fourier arrangement can attain almost unbelievable levels—it enables us to distinguish safely a tiny spectral shift and ﬁne structure in the emission lines of bound excitons in Si crystals with different content of silicon isotopes [32]! This opens further diagnostic possibilities. Another experimental aspect deserves special attention, namely, the method of sample cooling. It is mandatory that the samples must be immersed in a cooling medium (liquid He), an optical bath He cryostat is thus a necessity. We emphasize this because there is sometimes a tendency to replace the bath cryostat by a cheaper option—a continuous ﬂow cryostat with a closed He cycle where the cooling is mediated only by the heat transfer in He vapour. In this case, however, the cooling power is incomparably lower and the samples are strongly heated by the absorbed excitation radiation (the reader is reminded that silicon has low luminescence efﬁciency—the prevailing part of the excitation energy is converted, owing to non-radiative transitions, into heat!). This results in ‘evaporating’ bound excitons from the impurity atoms and in a corresponding increase of the free exciton concentration, which entails an appreciable drop in intensity of the BTO (BE) and PTO (BE) lines and, vice versa, an increase in the ITO (FE) line intensity. The signiﬁcance of this effect is demonstrated in Fig. 7.25 [33, 34]: upon an increase in temperature by a mere three kelvin the intensity ratio BTO (BE)/ITO (FE) is decreased by more than one order of magnitude! Insufﬁcient cooling therefore leads to a rapid deterioration of the measurement sensitivity, loss of the required spectral resolution and the method ﬁnally declines in importance. Upon introducing the photoluminescence analysis of silicon by Tajima, the method was independently developed and conﬁrmed at several other laboratories [30, 31, 35, 36]. The results were identical as far as the principal features

193

194

Luminescence of excitons were concerned, even if Colley and Lightowlers [30] proposed a modiﬁcation to consider the NP replicas instead of TO ones for the bound excitons, and the TO replica to employ for free excitons only. Besides calibration curves for boron and phosphorus, they presented calibration curve also for aluminium; Schumacher and Whitney [36] in addition for gallium and Broussel et al. [37] for arsenic. An effort is being made to extend similar photoluminescence diagnostics of dopants to other semiconductor materials. However, serious problems are often encountered owing either to high residual impurity concentrations or insufﬁcient resolved lines from different donor species. Nevertheless, the determination of luminescence of shallow impurity concentrations in CdTe has been published [38] and attempts to develop characterization methods of GaAs with the help of Fourier photoluminescence and magneto-photoluminescence spectroscopy have been reported, e.g. [39].

7.2.3 Excitons bound to isoelectronic impurities The exciton can be trapped—besides the above discussed cases of localization at ionized or neutral donors and acceptors—also at isovalent or isoelectronic impurities. By an impurity like this we understand a substitutionally built-in atom from the same group (column) of the periodic table of elements which the original constituent of the host lattice comes from. Unlike donors or acceptors, we do not encounter here a weakly bound ‘extra’ electron or hole that could inﬂuence the electric conductivity. Typical examples to be discussed in more detail are a nitrogen atom in place of phosphorus in GaP (GaP/N) and an iodine ion I− substituting bromine in AgBr (AgBr/I− ). In most cases, as we shall see, the exciton bound to an isoelectronic trap presents a highly efﬁcient channel of radiative recombination. (Also thallium activated alkali halides (KCl/Tl, CsI/Tl), often quoted in older literature as examples of efﬁcient phosphors and scintillators, belong to a certain extent to this category [40].)

Fig. 7.25 (a) Temperature dependence of intensities of the BTO (BE) and ITO (FE) lines and of their ratio in silicon in the temperature range 9–12 K, measured in a continuous-ﬂow cryostat. After Pelant et al. [33]. (b) Emission spectra of a very pure Si sample at T = 4.2 K (bath cryostat, lower spectrum) and at a nominal temperature of T ∼ 9 K (continuous ﬂow cryostat, upper spectrum). The spectra are normalized at 1130 nm. After Pelant et al. [34].

Bound excitons The physical mechanism of free exciton trapping is based on the electronegativity difference between the original and substituting atom. For example, a nitrogen atom N has higher electronegativity X (i.e. the ability to attract an electron) than a phosphorus atom P (X N = 3.0 > X P = 2.2). Therefore, if free photoelectrons and photoholes are created in GaP by an external excitation, the N atom may capture a nearby photoelectron with the help of short-range forces. The negatively charged N atom then attracts—now via long-range Coulomb forces—a free photohole, thereby a bound exciton localized at the nitrogen atom is created. Its radiative recombination gives a characteristic luminescence emission. Similarly, one can imagine the process to take place in AgBr crystals doped with an iodine impurity I− ; the iodine electronegativity is lower than that of bromine (X I = 2.7 < X Br = 3.0) and thus iodine has a higher capability to capture a photohole. A bound exciton is created again, owing to the subsequent Coulomb interaction of the positively charged centre with a photoelectron. What is the spectral shape of the luminescence emission accompanying the recombination of an exciton bound to an isoelectronic trap? The Maxwell– Boltzmann lineshape can be certainly excluded since possible broadening due to the kinetic energy of either a free carrier or a free exciton is missing. One deals with a localized excitation; a qualitative answer can thus be obtained by applying the conﬁgurational coordinate model. It is essential in this context that the initial photocarrier capture is by short-range forces. Localization of the excitation is thus basically mediated by alteration in the occupation of the electronic shell in a single (impurity) atom. The corresponding change in the conﬁgurational coordinate r Q = (Q e0 –Q g0 )/Q g0 (see Fig. 4.8) can then vary according to the strength of the exciton–phonon interaction. If this strength is relatively weak, which is the case of III-V semiconductors and thus also of GaP, r Q is small (small Huang–Rhys factor S ∼ = 0) and the emission line will be narrow. This is demonstrated in Fig. 7.26(a) where sharp lines A, B can be seen in the edge emission of a nominally pure sample of GaP [41]; both the lines are attributed to an exciton localized at a residual impurity N, being present in a concentration of ∼ 1015 cm−3 . The A line originates from an exciton with a total quantum number J = 1, the B line belongs to the exciton in the J = 2 state (in principle, a forbidden transition J = 2). The splitting is caused by the electron–hole exchange interaction; also the terms singlet and triplet exciton are often used. Both no-phonon lines and phonon replicas involving emission of optical phonons are present. (Looking at Fig. 5.10 we may ﬁnd out that the lines in question are very distinct also in a GaP sample doped with Si and S.) In strongly polar AgBr, the exciton–phonon coupling is much stronger, the surrounding host lattice reacts to the hole trapping by a sizable change of r Q and the emission due to the iodine presence reveals itself through a broad band rather than a narrow line. The emission spectrum of the exciton localized at I− (which is again a residual impurity in a nominally pure material, similarly to N in GaP) was already mentioned brieﬂy in the context of our discussion of the exciton–phonon interaction (see Figs 1.2(b) and 4.10(b)). The HuangRhys factor S can be estimated, based on the serial number of phonon replicas located at the band maximum, to be S = 8–9. A similar spectrum is shown

195

196

Luminescence of excitons

Fig. 7.26 (a) Emission spectra of nominally pure GaP under cw pumping with a dye laser 2.409 eV. The A and B lines (no-phonon ones) and their TA-, TO- and LO-phonon replicas, occurring in the edge emission range, are due to radiative decay of the excitons localized at the residual isoelectronic impurity of nitrogen (∼ 1015 cm−3 ). Band V originates from a similar exciton which is, moreover, inﬂuenced by the presence of distant donors and acceptors. After Gershoni et al. [41]. (b) Emission spectrum of nominally pure AgBr under cw pumping with a Kr+ -laser 3.53 eV. A weak indication of edge emission in the vicinity of 2.7 eV (enlarged in the circle) contains the free exciton line ITO (FE). An intense broad band at ∼ 2.5 eV is due to an exciton bound to a residual isoelectronic impurity of iodine (∼ 1016 cm−3 ). After Pelant [42]. The position of the indirect bandgap E gi is marked. Note the different energy scales in (a) and (b).

again in Fig. 7.26(b) [42]. This ﬁgure is, however, rather exceptional in two respects. Firstly, unlike the spectra in Figs 1.2(b) and 4.10(b), the bound exciton band at ∼2.5 eV lacks any ﬁne structure. This is, however, an experimental artefact due to a not-entirely-suitable choice of the time constant of the detecting lock-in ampliﬁer (over-damped state). On the other hand, however, this facilitated the discovery of the second—and more interesting—aspect: a weak emission of the free exciton ITO (FE) at ∼2.678 eV. What made recording this extremely weak line possible was just the strong noise suppression, together with a certain exceptionality of the investigated sample. The result enables us now to estimate in an illustrative way the extraordinary efﬁciency of the radiative recombination of excitons localized at an isoelectronic trap. From Fig. 7.26(b), we can estimate the ratio of the spectrally integrated intensities of the bound exciton line IodLO (BE) to the free exciton line ITO (BE) as [IodLO (BE)/ITO (FE)]≈ 104 .10 The corresponding luminescence 10 It is worth noticing that while the free exciton line is, owing to the strict selection rules (Section 7.1.4), accompanied by emission of TO-phonons (h¯ ωTO ≈ 8meV) satisfying the quasimomentum conservation law, the ﬁne phonon structure at the iodine band points to participation of primarily LO-phonons since separation between the individual peaks in Fig. 1.2(b) is very close to the energy of h¯ ωLO ∼ = 16 meV. The reason is basically twofold: ﬁrstly, the free and bound

Bound excitons decay times found experimentally are τIod ≈ 2 × 10−5 s [43] and τFE ≈ 6 × 10−8 s [44]. We write down simple relations for the intensities: IodLO (BE) =

NIod NFE , ITO (FE) = FE , Iod τr τr

(7.25)

FE where τ Iod r and τ r are the radiative lifetimes and NIod , NFE are the concentrations of ‘excited iodine ions’ and of free excitons at the given pumping level, respectively. By using relation (3.3) for the luminescence efﬁciencies ηIod , ηFE , we obtain from (7.25)

IodLO (BE) NIod ηIod τFE . = ITO (FE) NFE ηFE τIod

(7.26)

Now, we introduce an effective enhancement factor z ef = (NIod /NFE ) (ηIod /ηFE ) which comprises both the ratio of bound and free exciton concentrations (and thus takes into consideration the high effective cross-section of the free exciton trapping at impurity ions) and the ratio of quantum efﬁciencies of both the radiative processes. The factor z ef then follows from relation (7.26) as

IodLO (BE) τIod ≈ 104 × 103 /3 ∼ z ef = = 3 × 106 (!). ITO (FE) τFE This is an extremely high enhancement factor. The concentration of residual iodine in a nominally pure sample AgBr is ∼ 1016 cm−3 . Considering the host lattice contains ∼ 6 × 1022 molecules of AgBr per cubic centimetre, there is a single iodine ion per approximately 107 ions of the host lattice and, at the same time, ‘its’ own luminescence is by many orders of magnitude more intense than the intrinsic free exciton luminescence characterizing the pure host lattice! How is this possible? In addition to the efﬁcient trapping of free excitons itself (which has already been discussed when introducing the bound excitons at the beginning of Section 7.2), two other factors contribute to the high efﬁciency of the radiative recombination of an already trapped exciton. The ﬁrst one is the absence of Auger non-radiative recombination. An exciton bound to a neutral donor or acceptor represents three quasi-particles localized in a relatively small volume—either two electrons and one hole or two holes and one electron. This promotes a high probability of Auger recombination, therefore the luminescence of BE at neutral donors and acceptors is not particularly intense. On the contrary, the third quasi-particle is missing in the case of an exciton in an isoelectronic trap, therefore, Auger recombination does not take place at all. A second factor, important mainly in indirect-bandgap semiconductors (both AgBr and GaP), is the already mentioned strong localization of one quasiparticle at the impurity atom. The Heisenberg uncertainty relations xk ≥ 1/2 (where x is the uncertainty in the spatial coordinate and k that in the wavevector) imply, however, that a strong localization in real space (x → 0) excitons have different symmetry and, secondly, in radiative recombination of the impurity centre also local vibrations may participate. More detailed discussion of the phonon structure of the AgBr/I luminescence can be found in Czaja, W. and Baldereschi, A. (1979). J. Phys. C: Solid State Phys., 12, 405.

197

198

Fig. 7.27 Energy band structure of the GaP doped with nitrogen. Black ﬁlled areas denote the amplitude of the electron wavefunction ψN (k). It is seen that |ψN (k = 0)|2 = 0. Quasi-direct transitions at the point lead to intense luminescence (the lines A and B in Fig. 7.26(a)). E N stands for the binding energy of the electron at the isoelectronic trap N. After Holonyak et al. [45].

Luminescence of excitons inevitably introduces a strong delocalization of the wavefunction in k-space. Figure 7.27 depicts the situation as can be visualized in the energy band scheme of GaP:N [45]. The uncertainty k in localization of the modulus squared of the wavefunction |ψ N (k)|2 of an electron trapped at the N atom, i.e. an electron occupying the energy level just below the conduction band minimum at k ∼ = π/a(100), extends up to the (k = 0) point. This makes quasi-direct radiative recombination of the electron with hole possible. The probability of such transitions—taking place without the need of phonon assistance— is naturally by several orders of magnitude higher than that of the indirect transitions. This leads therefore to an exceptionally intense luminescence even in indirect-bandgap materials. It might be perhaps useful to emphasize once more the principal difference between the luminescence of shallow impurities (donors and acceptors) and the radiative decay of an exciton bound to an isoelectronic trap. At the shallow impurities, the electron or hole is attracted to a donor or acceptor, respectively, by the long-range Coulomb force. The emission spectrum of the exciton bound at a shallow impurity always bears the character of narrow lines. On the other hand, the isoelectronic trap captures the electron or hole through a short-range force and the wavefunction of the corresponding quasi-particle is strongly delocalized in momentum space. According to the type of the exciton–phonon interaction, the emission spectrum may take the form of either narrow lines (GaP, S ∼ = 0) or a phonon wing with a few phonon replicas in the case of medium exciton–phonon coupling (ZnTe/O, S ∼ = 3), or possibly a broad band in the case of very strong coupling (AgBr, S ∼ = 9). The luminescence of the isoelectronic impurity N has found widespread use in the production of green-emitting electroluminescence diodes based on GaP/N. The emission spectrum of this kind of diode is shown in Fig. 7.28 [46]. In commercially produced diodes, ternary alloys GaAs1−x Px (x = 0.4 to 1) are often used as the active medium which enables, apart from other things, the emission wavelength to be tuned. At high nitrogen doping, another radiative recombination channel due to the presence of coupled nitrogen atoms (NNpair states) appears. A detailed discussion of the physics of the isoelectronic impurity N in GaAs1−x Px can be found in the review article by Craford and Holonyak [47]. The question arises here as to whether it is possible to apply the principle of the isoelectronic trap also in homopolar semiconductors of group IV. It is a topical problem, in particular relevant to the search for light-emitting materials on a Si basis for future silicon photonics (Chapter 15). The doping of silicon with germanium or tin can hardly lead to any effect because the electronegativities of these chemical elements are almost the same (X Si = 1.9; X Ge = 2.0; X Sn = 2.0). As for doping with carbon (X C = 2.6), the desirable effect of strong luminescence is expected—according to what was explained above—to occur. Unfortunately, this is not the case. The carbon-related luminescence in crystalline silicon, represented by a narrow line at ∼ 0.97 eV, is very weak and, moreover, in order to appear, the material must ﬁrst be activated by electron beam irradiation. The reasons for this are not fully clear. Both the small atomic radius of the carbon atom and the weak exciton– phonon interaction have a possible role to play. A closer analysis of issues of isoelectronic traps in silicon can be found in [48].

Bound excitons

199

7.2.4 Self-trapped excitons In polar semiconductors with sufﬁciently strong exciton–phonon interaction, free exciton trapping can occur also in a pure and unperturbed crystal lattice. This process is called self-trapping or auto-localization of the exciton; radiative recombination of such a self-trapped exciton (STE) then evidently represents an intrinsic luminescence process. One can infer—from the fact that the exciton–phonon interaction is strong—that the corresponding luminescence emission spectrum will be broad. An intuitive illustrative idea of exciton self-trapping can be drawn in the following way: the translational movement of the exciton through the lattice is driven by its heavier constituent, i.e. the hole. If the polaron coupling constant of the hole αh is high, the hole–polaron is heavy; its effective mass is described by relation (6.9). The movement of the heavy hole is then very slow, the hole thus strongly polarizes the surrounding lattice, and thereby its movement is further slowed down and, ﬁnally, a total localization of the hole close to some atom constituting the host lattice can occur owing to positive feedback. A light electron accompanying the hole will then describe its orbit in the close vicinity. A more exact phenomenological description of the self-trapping of free quasi-particles as well as that of the entire exciton was put forward by Toyozawa [49]. In the case of an electrically neutral particle—an exciton— the interaction with the host lattice is, according to Toyozawa, caused not directly by the electric forces but mainly by the short-range (s) forces, and a redistribution of atoms (lattice relaxation—LR) occurs in the close vicinity of the exciton. This redistribution is within the conﬁgurational coordinate model accompanied by the lattice relaxation energy E R given by relation (4.14). For the purpose of more exact identiﬁcation, we denote here this relaxation energy s s ; thus E LR = S0 h¯ ω, where S0 is the Huang–Rhys factor. The shortas E LR s /B, where B is range interaction is characterized by the parameter gs = E LR the total energy width of the exciton band. The interaction of charged quasi-particles, electrons and holes, with the lattice is mediated by the Fr¨ohlich mechanism employing LO-phonons. Consequently, long-range ( ) forces are involved and Toyozawa introduces

the parameters ELR and g = E LR /B for their characterization. The Fr¨ohlich interaction is naturally completely absent in homopolar semiconductors of group IV (Si, Ge), and therefore g = 0 there. Toyozawa showed that excitons can occur really in two stable states that occupy local energy minima in the conﬁgurational coordinate model: free (F) and self-trapped (S) states. A self-trapped exciton gets localized in a potential well, created as a consequence of the strong lattice deformation over the exciton’s surroundings. Toyozawa assigns this exciton to an effective mass m = m exc exp S0 , where m exc is the free exciton effective mass (thus the case of a strong exciton–phonon interaction, when S0 1, entails m → ∞). The steady state switches rapidly from F to S as soon as the value of the coupling s /B exceeds unity. constant gs = E LR The resulting phase diagram in the plane (gs , g ) is shown in Fig. 7.29. The coupling of electrons, holes and excitons with phonons increases in the direction of rising gs , g . The F–S boundary is depicted by a solid line, and sections marked F(S) and S(F) indicate regions in which the self-trapped and free states

Fig. 7.28 Emission spectrum of the green electroluminescence from a GaP/N diode at room temperature. The GaN content in the melt is shown in percent at the individual curves. The positions of the individual lines from Fig. 7.26(a) are indicated; these lines merge into a single band at higher temperature. The red-shift of the lines in comparison with Fig. 7.26(a) is caused by the bandgap narrowing upon temperature increase 4 K → 300 K. After Vishnevskaya et al. [46].

Fig. 7.29 Phase diagram in the (gs , g ) plane for electrons, holes and excitons in a deformable lattice. The boundary F (free state)–S (self-trapped state) is depicted by a solid line. It is seen that self-trapping does not occur in IV, III-V and II-VI semiconductors. In AgCl and alkali halides, the hole and subsequently also the exciton become self-trapped. After Toyozawa [49].

200 Fig. 7.30 (a) Emission spectrum of AgCl under pumping with laser pulses 351 nm (∼ 1 ps) at T = 2 K. The position of the expected free exciton luminescence line is indicated by the arrow F. The broad band S at ∼490 belongs to the self-trapped exciton. (b) Time integrated luminescence in the region of the expected free exciton emission. Its intensity is extremely weak (∼ 70 counts/s) and the luminescence decays very quickly (∼ 20 ps). This line has been attributed to the radiative decay of the free exciton. Points represent experiment; the full line is the Maxwell–Boltzmann shape (7.16) with an effective temperature of 19.7 K. After Kobayashi et al. [50].

Fig. 7.31 Schematic of the microscopic structure of a self-trapped hole in AgCl depicting tetragonal distortion of the surrounding lattice. After von der Osten [51].

Luminescence of excitons

can coexist (more details later). It can be clearly seen that a break occurs in silver halides—while both the carriers and the exciton are still free in AgBr (and also in TlBr), in AgCl the hole becomes self-trapped and, consequently, self-trapping of the exciton also occurs. Therefore, the luminescence of a (free) exciton in AgBr consists of a narrow resonant emission line (Fig. 7.15), while the emission spectrum of STE with S0 ≥ 50 1 in AgCl is represented by a broad band at ∼490 nm (Fig. 7.30(a) [50] or Fig. 4.10(c)). Although AgBr and AgCl differ very little only in most physical, chemical and photochemical properties, the difference in their low-temperature luminescence is substantial! Various microscopic mechanisms of hole self-trapping can exist. In AgCl the hole becomes self-trapped—even though it may seem strange at ﬁrst sight— at an already positively charged cation Ag+ [51], thereby a ‘molecular ion’ 4− is created, see Fig. 7.31. The reason for such hole localization (Ag+ Cl− 6) lies, in the ﬁrst place, in the fact that the valence band maximum of AgCl at L 3 comprises contributions both from 3p states of Cl− and 4d states of Ag+ ; therefore the self-trapped hole must be constructed from both the states of chlorine and silver. The Jahn–Teller effect leads to a lowered symmetry of the created complex, because of lifting the geometrical equivalence of the six chlorine ions—four of them move towards the central Ag2+ ion while the other two move in the opposite direction. In this way a prolonged axis of the complex in one of the equivalent [100] directions is created (Fig. 7.31).11 Free and self-trapped excitons may coexist. This holds true in segments marked as F(S) and S(F) in Fig. 7.29. One can imagine such coexistence in the framework of the conﬁgurational coordinate model as depicted in Fig. 7.32. In the particular case of AgCl, it is possible to interpret the conﬁgurational coordinate Q as the separation of Cl− ligands from the central Ag2+ ion in the (AgCl6 )4− complex. The free exciton (minimum F in Fig. 7.32) is separated from the deeper minimum (S) of the self-trapped exciton by a potential barrier Δ. Free excitons created by light must overcome this barrier in order to reach the energetically favourable self-trapped state (by tunnelling at low temperatures); to do this, they need some time. Because the barrier is 11 In alkali halides, on the other hand, the hole becomes self-trapped in the form of a molecular ion X− 2 (X = F, Cl, Br, I), which is the so-called Vk - centre oriented along the [110] direction.

Problems low (Δ ∼ = 5 meV) and thin in AgCl, it is easy to overcome. Therefore, the free exciton ‘stays’ in the F minimum only for a very short time and the probability of its radiative recombination there is negligible in comparison with penetrating the barrier and subsequently radiating an intense luminescence from the S minimum. In the standard steady-state luminescence experiment we thus record only a broad STE emission band at ∼ 490 nm (Fig. 7.30(a)). A time-resolved luminescence experiment taking advantage of short enough excitation pulses (∼ 1 ps) together with a very sensitive detection system, however, permits us to verify the presence of an extremely weak emission line due to the free exciton radiative annihilation at the F minimum. Besides the fast pumping, also a sufﬁciently low temperature (T = 2–4 K) is necessary because higher temperatures rapidly promote the probability of thermally overcoming the barrier Δ. This delicate experiment was performed by Kobayashi and coworkers [50] and the result agreed exactly with expectation—they succeeded in detecting a weak line with spectral proﬁle corresponding to the Maxwell– Boltzmann distribution at a wavelength of about 383 nm (which corresponds to the indirect exciton gap 3.248 eV decreased by the energy h¯ ω TO = 8 meV of the quasi-momentum conserving phonon), see Fig. 7.30(b). It is interesting to note that nanosecond pumping pulses are not sufﬁciently short for that purpose because the time required to penetrate the barrier appears to be very short, around 70 ps. However, also under pumping with relatively long (∼10 ns) pulses time-resolved luminescence spectroscopy found a clear indication of short-living emission on the high-energy side of the STE emission band at ∼425 nm (Fig. 1.2(a)). This emission can be attributed to hot luminescence of STE (see the arrows H in Fig. 7.32) and to transient fusion of the free exciton with the self-trapped [52]. In general, the occurrence of exciton self-trapping in semiconductors is the exception rather than the rule. Experimental attention was, in addition to AgCl, paid to CdI2 [53] and ZnSe1−x Tex (x ≈ 0.01) [54]. The latter case is, however, a ternary alloy containing defects of the disordered lattice that contribute signiﬁcantly to the localization effect. Such a localization is no longer an intrinsic process, and is therefore called extrinsic self-trapping (the self-trapping occurs neither in pure ZnSe nor in pure ZnTe, in agreement with Fig. 7.29). Otherwise, it is possible to meet the intrinsic self-trapping of excitons in a variety of wide-bandgap non-semiconducting materials, both inorganic and organic. An overview of these phenomena is given in the monograph [55].

7.3 Problems

√ 7/1: Show, employing the slope of the photon dispersion curve h¯ c( ε∞ )−1 , that states corresponding to the polariton effects occupy within the ﬁrst Brillouin zone only a very small volume around k = 0. (This justiﬁes why we consider h¯ ω(k ∼ = 0) as the energy of phonons taking part in the thermalization and radiative recombination of the exciton–polariton, and it means also that the polariton effects play mostly a negligible role in the total emitted luminescence.)

201

Fig. 7.32 Potential energy curve of a free (F) and self-trapped (S) exciton in the conﬁgurational coordinate model. Vertical lines depict luminescence processes, and Δ stands for the potential barrier against self-trapping. After Kobayashi et al. [50].

202

Luminescence of excitons 7/2: Show that the maximum of the (X–LO) emission line is shifted from the energy of the free exciton ground state n = 1 towards lower energies not exactly by h¯ ω0 , but by a temperature variable quantity (h¯ ω0 –(3/2)kB T ). 7/3: The quasi-momentum conservation law is formulated differently depending on whether the free exciton radiative decay is one- or two-phonon assisted. This leads not only to a slightly different shape of the corresponding emission lines (eqns (7.12) and (7.13)) but also to different temperature dependences of both the lines. Show that the ratio of the integral (1) (2) intensities Isp and Isp of the X–LO and X–2LO lines, respectively, can (1) (2) be expressed as (Isp )/(Isp ) = γ T , where γ is a constant. Proceed from relations (7.12) and (7.13). 7/4: Free excitons and the conﬁgurational coordinate model. A free exciton, considering its translational movement, surely does not represent a localized luminescence centre. Can we discuss its luminescence behaviour in the framework of the conﬁgurational coordinate model? According to what was formulated in Section 4.4 obviously not. However, the existence of the LO-phonon assisted radiative decay of free excitons points to the fact that an intrinsic exciton–phonon interaction occurs here. We can then consider the (X–LO), (X–2LO), etc. lines as being phonon satellites of the resonant exciton–polariton (no-phonon) line. Therefore, also here we are in principle allowed to use formally the conﬁgurational coordinate model, and the reason for this is the ﬁnite spatial extent of the exciton wavefunction. The rise and decay of the related electronic polarization then causes a moderate lattice deformation. The Huang–Rhys factor S is, . naturally, very small (S = 0.1). Deal with the Huang–Rhys factor of free excitons after Zhao and Kalt [56]. 7/5: We have derived the symmetry-driven selection rules for indirect exciton transitions in AgBr by making use of (7.17). The applied approach was, however, somewhat simpliﬁed. That is, we tacitly assumed the vertical photon-related transitions to the nearby ‘virtual’ states (whose involvement results from second-order perturbation theory) to be dipole allowed, see transitions L 1 − L 3 and 1 –15 in Fig. 7.33. Show, using relation (7.14), that this assumption was justiﬁed. (You need not know either the tables of characters of point groups or to be proﬁcient in their usage. You will ﬁnd all the necessary relations throughout Subsections 7.1.3 and 7.1.4. We recall only that 1 ⊗ X = X holds for an arbitrary representation X , because the 1 representation is spherically symmetric.)

Fig. 7.33

References 1. Knox, R. S. (1963). Theory of Excitons. Academic Press, New York; Bassani, F. and Pastori Parravicini, G. (1975). Electronic States and Optical Transitions in Solids. Pergamon Press, Oxford. 2. Velick´y, B., Tauc, J., Trlifaj, M., and Prosser, V. (1965). Interaction of electromagnetic radiation with solids (In Czech: Interakce elektromagnetick´eho z´aen´ı s pevnou l´atkou). In Solid State Theory (In Czech: Teorie pevn´ych l´atek), p. 229. ˇ NCSAV, Prague.

References 3. Klingshirn, C. F. (1995). Semiconductor Optics. Springer, Berlin. 4. Peyghambarian, N., Koch, S. W., and Mysyrowicz, A. (1993). Introduction to Semiconductor Optics. Prentice Hall, Englewood Cliffs, N.J. 5. Weisbuch, C. and Benisty, H. (2005). phys. stat. sol. (b), 424, 2345. 6. Joesten, B. L. and Brown, F. C. (1966). Phys. Rev., 148, 919. 7. Razeghi, M., Omnes, F., Nagle, J., Defour, M., Acher, O., and Bove, P. (1989). Appl. Phys. Lett., 55, 1677. 8. Koteles, E. S., Lee, J., Salerno, J. P., and Vassel, M. O. (1985). Phys. Rev. Lett., 55, 867. 9. Bose, S. S., Kim, M. H., and Lee, B. (1988). J. Electr. Mater., 17, S36. 10. Gross, E., Permogorov, S., and Razbirin, B. (1966). J. Phys. Chem. Solids, 27, 1647. 11. Segall, B. and Mahan, G. D. (1968). Phys. Rev., 171, 935. 12. Gross, E. F., Permogorov, S. A., and Razbirin, B. S. (1971). Sov. Phys. Usp., 14, 104. 13. Bassani, F. and Pastori-Parravicini, G. (1975). Electronic States and Optical Transitions in Solids. Pergamon Press, Oxford. 14. Kunz, A. B. (1982). Phys. Rev. B, 26, 2070. 15. von der Osten, W. and Weber, J. (1974). Solid State Comm., 14, 1133. 16. Thomas, G. A., Frova, A., Hensel, J. C., Miller, R. E., and Lee, P. A. (1976). Phys. Rev. B, 13, 1692. 17. Hensel, J. C., Phillips, T. G., and Thomas, G. A. (1977). The electron–hole liquid in semiconductors: experimental aspects. In The Electron–Hole Liquid in Semiconductors (ed. H. Ehrenreich, F. Seitz and D. Turnbull), p. 88. Solid State Physics Vol. 32. Academic Press, New York. 18. Rashba, E. I. and Gurgenishvili, G. E. (1962). Sov. Phys. – Solid State, 4, 759. 19. Haynes, J. R. (1960). Phys Rev. Lett., 4, 361. 20. Bebb, H. B. and Williams, E. W. (1972). Photoluminescence I. Theory. In Semiconductors and Semimetals (ed. R. K. Willardson and A. C. Beer ), Vol. 8, p. 181. Academic Press, New York and London, 21. Bernussi, A. A., Barreto, C. L., Carvalho, M. M. G., and Motisuke, P. (1988). J. Appl. Phys., 64, 1358. 22. Hayes, W. and Stoneham, A. M. (1985). Defects and Defect Processes in Nonmetallic Solids. John Wiley, New York. 23. H¨onerlage, B., R¨ossler, U., and Schr¨oder, U. (1975). Phys. Rev. B, 12, 2355. 24. Herbert, D. C. (1984). J. Phys. C: Solid State Phys., 17, L901. 25. Kaminskii, A. S. and Pokrovskii, Ya. E. (1970). JETP Lett., 11, 255. 26. Lampert, M. A. (1958). Phys. Rev. Lett., 1, 450. 27. Kirczenow, G. (1977). Canad. J. Phys., 55, 1787. 28. Tajima, M.(1982). Quantitative impurity analysis in Si by the photoluminescence technique. In Semiconductor Technologies (ed. J. Nishizawa), p. 1. North Holland, Amsterdam. 29. Pelant, I., H´ala, J., Ambroˇz, M., V´acha, M., Valenta, J., Adamec, F., Kohlov´a, V., and Matouˇskov´a, J. (1990). Impurity analysis in Si crystals by the photoluminescence method V (In Czech: Anal´yza pˇrimˇes´ı v krystalech Si fotoluminiscenˇcn´ı metodou V). Research Report for Tesla Roˇznov, k.p., Charles University in Prague, Faculty of Mathematics & Physics, Prague. 30. Colley, P. McL. and Lightowlers, E. C.(1987). Semicond. Sci. Technol., 2, 157. 31. Pelant, I., H´ala, J., Ambroˇz, M., Kohlov´a, V., and Vacek, K. (1989). Czech. J. Phys A (In Czech), 39, 142. 32. Karaiskaj, D., Thewalt, M. L. W., Ruf, T., and Cardona, M. (2003). phys. stat. sol. (b), 235, 63. 33. Pelant, I., H´ala, J., Ambroˇz, M., and Kohlov´a, V. (1988). Photoluminescence of impurities and photoluminescence assessment of boron and phoshorus in silicon (In Czech: Fotoluminiscence pˇrimˇes´ı a fotoluminiscenˇcn´ı stanoven´ı boru a fosforu v kˇrem´ıku). In Kˇrem´ık ’88, part 2, p. 86. General Head Ofﬁce Tesla–ES, Roˇznov pod Radhoˇstˇem.

203

204

Luminescence of excitons 34. Pelant, I., H´ala, J., Ambroˇz, M., and Kohlov´a, V. (1988). Quantitative analysis of low concentrations of boron and phosphorus in silicon by the laser luminescence spectroscopy—experimental aspects (In Czech: Kvantitativn´ı anal´yza n´ızk´ych koncentrac´ı boru a fosforu v kˇrem´ıku laserovou luminiscenˇcn´ı spektroskopi´ı – experiment´aln´ı aspekty). In Lasers in Research and Industry (6th Czechoslovak Conferˇ CSSP ˇ ence), p. 252. Raˇckova dolina, SVST Liptovsk´y Mikul´asˇ. 35. Kaminskii, A. S., Kolesnik, L. I., Leiferov, B. M., and Pokrovskii, Ya. E. (1982). J. Appl. Spectros., 36, 516. 36. Schumacher, K. L. and Whitney, R. L. (1989). J. Electron. Mater., 18, 681. 37. Broussell, I., Stolz, J. A. H., and Thewalt, M. L. W. (2002). J. Appl. Phys., 92, 5913. 38. Zimmermann, H., Boyn, R., Michel, C., and Rudolph, P. (1990). phys. stat. sol. (a), 118, 225. 39. Thewalt, M. L. W., Nissen, M. K., Beckett, D. J. S., and Lungren, K. R. (1989). High-performance photoluminescence spectroscopy using Fourier-transform interferomety, MRS Meeting Boston November/December, Symp. G. MRS Symposium Proceedings, 163, (1990), 221. 40. Dekker, A. J. (1963). Solid State Physics. Prentice-Hall, Englewood Cliffs, N.J.; Curie, D. (1960). Luminescence Cristalline. Dunod, Paris. 41. Gershoni, D., Cohen, E., and Ron, A. (1985). J. Luminescence, 34, 83. 42. Pelant, I. (1988). Laser luminescence spectroscopy of some crystalline semiconductors and ionic crystals (In Czech: Laserov´a luminiscenˇcn´ı spektroskopie vybran´ych krystalick´ych polovodiˇcu˚ a dielektrik), DSc Thesis, Charles University in Prague, Faculty of Mathematics and Physics, Prague. 43. Tsukakoshi, M. and Kanzaki, H. (1971). J. Phys. Soc. Japan, 30, 1423. 44. Stolz, H., von der Osten, W., and Weber, J. (1976). Lifetime and time-resolved spectra of indirect excitons in AgBr. In Physics of Semiconductors (ed. F. G. Fumi), p. 865. Proceedings of the 13th International Conference on the Physics of Semiconductors, Rome. 45. Holonyak, N. Jr., Campbell, J. C., Lee, M. H., Verdeyen, J. T., Johnson, W. L., Craford, M. G., and Finn, D. (1973). J. Appl. Phys., 44, 5517. 46. Vishnevskaya, B. I., Korneev, V. M., Kogan, L. M., and Yunovich, A. E. (1973). Soviet Phys. Semicond., 6, 1372. 47. Craford, M. G. and Holonyak, N. Jr. (1976). The optical properties of the nitrogen isoelectronic trap in GaAs1−x Px . In Optical Properties of Solids. New Developments (ed. B. O. Seraphin), p. 187. North Holland, Amsterdam. 48. Brown, T. G. and Hall, D. G. (1998). Radiative isoelectronic impurities in silicon and silicon–germanium alloys. In Light Emission in Silicon: From Physics to Devices (ed. D. J. Lockwood), Semiconductors and Semimetals Vol. 49, p. 77. Academic Press, San Diego. 49. Toyozawa, Y. (1970). J. Luminescence, 1, 632; Toyozawa, Y. (1981). J. Luminescence, 24/25, 23. 50. Kobayashi, M., Matsushima, Y., Nishi, O., Mizuno, K., and Matsui, A. H. (1995). SPIE, 2362 (Exciton processes in condensed matter), 225. 51. von der Osten, W. (1984). Excitons and exciton relaxation in silver halides. In Polarons and Excitons in Polar Semiconductors and Ionic Crystals (ed. J. T Devreese and F. Peeters), p. 293. Plenum Press, New York. 52. Pelant, I. and H´ala, J. (1991). Solid State Comm., 78, 141. 53. Nakagawa, H., Muneda, Y., and Matsumoto, H. (1988). J. Luminescence, 40/41, 485. 54. Lee, D., Mysyrowicz, A., Nurmikko, A. V., and Fitzpatrick, B. J. (1987). Phys. Rev. Lett., 58, 1475. 55. Song, K. S. and Williams, R. T. (1996). Self -Trapped Excitons. Springer Series in Solid State Sciences Vol. 105. Springer, Berlin. 56. Zhao, H. and Kalt, H. (2003). Phys. Rev. B, 68, 12.

Highly excited semiconductors

8 8.1 Experimental considerations 206 8.2 Excitonic molecule or biexciton

The channels of radiative recombination, discussed in Chapters 5 and 7, are characteristic of conventional (weak) optical excitation when the excitation power densities on the sample surface amount to 0.01–10 W/cm2 . When the excitation intensity is increased to kW/cm2 –MW/cm2 (which is attainable almost exclusively with the aid of pulsed lasers) the emission spectrum undergoes substantial modiﬁcations: New emission lines or bands appear. Figure 8.1 shows a typical example [1]. These lines or bands signify novel luminescence processes occurring in highly excited semiconductors, in particular: radiative decay of excitonic molecules (biexcitons), collisions between excitons, luminescence of the electron–hole liquid or electron–hole plasma and Bose– Einstein condensation of excitons or biexcitons. We are going to discuss these

207

8.3 Collisions of free excitons

218

8.4 Electron–hole liquid (EHL)

220

8.5 Electron–hole plasma (EHP) 230 8.6 Bose–Einstein condensation of excitons 234 8.7 Problems

239

Fig. 8.1 Edge emission spectrum of CdS under various intensities of optical excitation (temperature T = 1.8 K). The lowermost spectrum was acquired at a conventional Hg-lamp excitation (λex = 365 nm) and is dominated by I1 and I2 lines, which are due to excitons bound to residual impurities. The X-line belongs to the resonant emission of an exciton–polariton (compare with Fig. 7.11(a)). The remaining spectra were excited by a pulsed N2 -laser (λex = 337 nm), relative excitation power densities being indicated to the right along with normalization factors. The ﬁgure illustrates that the I1 , I2 lines gradually saturate with increasing excitation intensity while novel M and P lines appear. After Shionoya et al. [1].

206

Highly excited semiconductors phenomena in the present chapter. Optical properties of highly excited semiconductors are dealt with also, e.g. in special issues of Physics Reports [2, 3].

8.1 Experimental considerations To understand the underlying physical nature of the novel luminescence processes occuring under high excitation, it appears advantageous to characterize the concentration level of created free excitons n X . We can start with eqn (3.4) from which it follows that in steady-state conditions nX ∼ = Iex α τ,

(8.1)

where Iex stands for the excitation photon ﬂux (photon/cm2 s) of energy hνex , α(cm−1 ) denotes the absorption coefﬁcient at energy hνex and τ (s) means the exciton lifetime. For a typical case of band → band excitation we consider α ∼ = 105 cm−1 , τ = 10−9 s (direct semiconductor) and the excitation photon ﬂux Iex can be derived from the excitation intensity Pex — usually expressed in watts per cm2 —using the relation Iex = (Pex / hνex ). For Pex = 1 W/cm2 (conventional weak excitation) and hνex = 3 eV we have Iex ∼ = 2 × 1018 photon/cm2 s and the density of photogenerated excitons (8.1) 2 × 1014 cm−3 . becomes n X ∼ =√ Given X ∼ = 3 (1/n X )) as the mean interexciton separation, we get in this case X ∼ = 170 nm. Comparing this value with a typical exciton Bohr radius aX ∼ 5 nm (Table 7.1) implies X aX , and therefore free excitons are sufﬁ= ciently separated from each other and do not enter into interactions. However, if we increase their density so that X approaches the exciton diameter 2aX , the situation becomes completely different. The condition X ∼ = 2aX yields (keeping aX = 5 nm) the exciton density n X ∼ = 1018 cm−3 and the corresponding excitation photon ﬂux is, using (8.1), equal to Iex ≈ 1022 photon/cm2 s or, equivalently, to the excitation intensity Pex = Iex hνex ≈ 5 kW/cm2 .1 At such excitation intensities one can already expect the occurence of interactions between excitons. These, as we shall see, may dramatically modify the luminescence behaviour of the material under study. It is worth stressing, however, that relation (8.1) is not exact; the density of excitons or electron–hole pairs under standard one-photon excitation is considerably inhomogeneous. The concentration gradient pushes them from a thin subsurface layer with thickness α −1 < 1μm deeper into the sample, thereby rapidly reducing their concentration. Besides, excitons close beneath the surface undergo efﬁcient surface non-radiative recombination (Fig. 6.2). That is why the excitation intensities Pex applied in experiments must in fact be higher than the above order-of-magnitude estimate—they usually range from ∼ 1 kW/cm2 up to 1–10 MW/cm2 , where the upper bound is driven by the threshold of mechanical destruction of the sample by powerful laser pulses.

1 For expressing the density of excitons or electron–hole pairs, one sometimes exploits the dimensionless parameter rs = (3/4π n X )1/3 (1/aX ); high densities n X are characterized by values rs < 1.

Excitonic molecule or biexciton Two remarks may be in order. The ﬁrst one refers to most indirect-bandgap semiconductors (Si, Ge, GaP). Here, the exciton lifetime is much longer than 10−9 s and high exciton densities rs < 1 can already be achieved using cw lasers or even conventional high-pressure lamps. The second remark points to the principal superiority of two-photon excitation for studying luminescence of high-density excitonic systems. Owing to the very slow decrease of excitation intensity along the penetration depth inside the sample (Fig. 5.15(a)), relation (8.1) holds—contrary to the onephoton case—very accurately. We can thus achieve a pre-determined value of homogeneous exciton concentration over the whole volume of the sample, which is highly desirable for comparing the experimentally deduced density with various models of excitonic interactions discussed below. Of course, we have to replace the one-photon absorption coefﬁcient α in (8.1) by its twophoton analogue α (2) , deﬁned in the context of eqn (5.22) as α (2) = aI 0 = aPex (cm−1 )

(8.2)

(that is, we denote the excitation power density as Pex in this chapter). The reader is reminded that a is a material constant with a typical value of a ∼ = 10−3 cm/MW. However, there is one hitch in this, namely, if we realize how low the amount of energy deposited generally into the electronic system of the sample under two-photon excitation is. Introducing α (2) from (8.2) to (8.1) and expressing Pex as a function of the required exciton concentration, we get (8.3) Pex = n X h νex /τ a. Therefore, if we wish to generate a homogeneous exciton concentration n X = 1017 cm−3 , using typical values of hνex = 3 eV ≈ 5 × 10−19 J, τ = 10−9 s and a = 10−3 cm/MW, it follows from (8.3) that the required excitation power density Pex reaches ∼ 100 MW/cm2 ! Such a high value of excitation power density is already comparable with the threshold of sample destruction. We have to carefully look up all possible material parameters (especially the value of a) in advance, as well as evaluate all the capabilities of our experimental set-up. Only then can we decide whether the possible advantage of achieving a homogeneous density of exciton gas would not be nulliﬁed by damaging the sample.

8.2 Excitonic molecule or biexciton Referring to the similarity between a free exciton and a hydrogen atom, discussed in Section 7.1, we can expect that with increasing free exciton density a ‘fusion’ of two excitons into an excitonic molecule (EM) or biexciton will occur, in analogy with the fusion of two hydrogen atoms into a hydrogen molecule. An EM is a quasi-particle consisting of two electrons and two holes and propagating freely through the crystal lattice (more exactly, we should designate it as a free biexciton). It is obvious that the very existence of EMs in a given semiconductor will be critically dependent upon the ratio of the electron and hole effective masses σ = m e /m h , much like as in bound exciton

207

208

Fig. 8.2 Examples of theoretically calculated dependencies of the biexciton binding energy E B upon the ratio of the electron and hole effective masses σ = m e /m h . E B is expressed in units of the free exciton binding energy E X . Small letters denote results obtained by different authors. Adapted from Quattropani and Forney [4], where the reader can ﬁnd a more detailed discussion.

Highly excited semiconductors complexes discussed in Subsection 7.2.1. Both an electron and a hole are very light quasi-particles and thus the resulting large amplitude of biexciton zeropoint vibrations will have a tendency to dissociate the excitonic molecule even at low temperatures. The measure of EM stability against dissociation into two free excitons is its binding energie E B . Theoretical calculations of E B using diverse variation methods have been performed by many authors; the results, as compiled by Quattropani and Forney, are depicted in Fig. 8.2 [4]. It is observed that an EM is a stable entity (E M ≥ 0) for an arbitrary value of σ , even if, quite naturally, the binding energy strongly increases in the case of heavy holes. It is important to note that the calculations predict, for typical values of σ in semiconductors (σ ≈ 0.1–0.5), that the magnitude of the binding energy E B will be approximately equal to one-tenth of the free exciton binding energy: EB ∼ = 0.1E X . A biexciton is therefore substantially less resistant to thermal dissociation than an exciton. An important message for experiments is that for studying biexcitons very low temperatures are required in most cases (about 1.3–50 K), accessible in liquid helium cryostats only. Radiative recombination of EMs is a process in which one of the excitons forming the molecule undergoes a transition to the free exciton n = 1 state while the second one recombines, emitting a photon hνM . This process gives rise to a novel emission line (e.g. the M-line in Fig. 8.1). In order to be able to assign reliably an experimentally observed line to excitonic molecule decay, we have to analyse its lineshape, intensity dependence, spectral position and temperature behaviour.

8.2.1 Identiﬁcation of the EM emission line The basic guideline for the indentiﬁcation of an emission line as being due to radiative decay of an EM is its characteristic lineshape. It turns out to be suitable to discuss the EM emission lineshape separately in direct-bandgap and indirect-bandgap semiconductors. Luminescence of excitonic molecule in a direct semiconductor To begin, we determine the approximate spectral position of the EM emission line, neglecting the kinetic energies of all participating quasi-particles. The formation of an EM through the ‘fusion’ of two excitons with energies (E g –E X ), accompanied by a simultaneous release of binding energy E B , leads to a biexciton in its ground state with an energy of 2(E g –E X )–E B (see Fig. 8.3(a)). Radiative decay of the biexciton generates one photon, hν M , and leaves behind one free exciton, therefore the total energy of the system reads hνM + (E g –E X ). Comparing the above mentioned energies yields the overall energy balance 2 (E g − E X ) − E B = hνM + (E g − E X )

(8.4)

hνM = (E g − E X ) − E B .

(8.5)

or

Excitonic molecule or biexciton

209

Fig. 8.3 Radiative decay of an excitonic molecule in an E(K) diagram for (a) a direct-bandgap semiconductor and (b) an indirect-bandgap semiconductor with the indirect bandgap situated at K0 . The scheme goes, of course, beyond the limit of the one-electron approximation (otherwise the energy level of the excitonic molecule would be ‘submerged’ high up into the conduction band).

Hence, the emission line of the EM is shifted with respect to the position of the free exciton absorption line (E g –E X ) (or the luminescence line of an exciton– polariton) by the binding energy E B towards low photon energies. Now we take into consideration also the kinetic energies in the ensemble of excitonic molecules and free excitons. We shall arrive at important informaM (hν), tion on the characteristic biexciton spontaneous emission lineshape Isp namely, that it is of a mirror-like appearance with regard to the free exciton emission lineshape described by expressions (7.13) or (7.16). We speak of the inverse Maxwell–Boltzmann distribution (with effective temperature TM of the biexciton gas), i.e. M Isp (hν) ∼ = [(E g − E X − E B ) − hν]1/2

exp {−[(E g − E X − E B ) − hν] /kB TM }.

(8.6)

Prior to deriving expression (8.6) rigorously, we shall attempt to understand this lineshape qualitatively employing Fig. 8.3(a). The biexciton dispersion curve ŒM (K) = h 2 K 2 /4m exc (where m exc = m e + m h is the exciton mass) is less curved compared with the exciton curve ŒX (K) = h2 K2 /2mexc . The highest emitted photon energy thus belongs to the downward transition at K = |0 and is, according to (8.5), equal to (E g –E X )–E B ; radiative decay of

210

Highly excited semiconductors biexcitons with non-zero kinetic energy at K = |0 results in luminescence photons with lower energy, which is depicted in Fig. 8.3(a) by the transition M between states E 2 and E 1 . Therefore, the emission line will have an asymmetric shape characterized by a high-energy edge at (E g –E X )–E B followed by a low-energy tail. To derive (8.6) we shall apply a procedure similar to that utilized in Subsection 5.2.1 for deducing the Maxwell–Boltzmann distribution (5.9a). Spontaneous emission of a luminescence photon pertaining to radiative decay M (hν) is driven by (i) the optical joint density of states ρ (hν), of a biexciton Isp M coming from the relevant densities of states in the exciton and biexciton bands,2 (ii) the population fraction f M (hν) of the biexciton states and (iii) the transition matrix element MM : M Isp (hν) ∼ ρM (hν) f M (hν)|MM |2 .

(8.7)

The matrix element MM is considered to be independent of hν. Referring to Fig. 8.3(a) we can write E 2 = 2(E g − E X ) − E B + h¯ 2 K 2 /4 m exc ,

(8.8a)

E 1 = (E g − E X ) + h¯ 2 K 2 /2 m exc ,

(8.8b)

which immediately implies hν = E 2 − E 1 = (E g − E X − E B ) − h¯ 2 K 2 /4 m exc ,

(8.8c)

hence K2 =

4 m exc [(E g − E X − E B ) − hν]. h¯ 2

(8.9)

Inserting for K 2 from (8.9) to (8.8b) yields E 1 = 2[(E g − E X − E B ) − hν] + (E g − E X ).

(8.10)

Let us suppose now that the density of states in the exciton band ρX has the common square-root form, fully analogous to the densities of states in the conduction and valence bands, expressed by formula (5.4): (2 m exc )2/3 ρ X (E 1 ) = E 1 − (E g − E X ). (8.11) 2 π2 h¯ 3 By using the incremental relation ρ X (E 1 ) dE 1 = −ρ M (hν) d(hν) (the ‘–’ sign means here that the loss of one free exciton state is equivalent to the generation of one photon hν) along with (8.10) and (8.11) we ﬁnd the optical joint density of states ρ M (hν) = −ρ X (E 1 ) dE 1 /d(hν) = −ρX (E 1 )(−2) √ 2(2m exc )3/2 (E g − E X − E B ) − hν. = π2 h¯ 3

(8.12)

2 The reader is reminded that the possibilty of introducing the joint density of states follows from the verticality of the transitions depicted in Fig. 8.3(a).

Excitonic molecule or biexciton Finally, the population factor f M (hν) in (8.7) can be determined quite easily: Since both biexcitons and excitons are composed of an even number of fermions, they have integer spin and are, therefore, bosons. Then, there is no need—contrary to direct interband e–h transitions—to formulate any mathematical condition concerning the occupancy of the exciton dispersion curve; the population fraction is driven exclusively by the occupation probability of the upper (biexciton) level. This is given by the Boltzmann factor f M (hν) ≈ exp(−h¯ 2 K 2 /4 m exc kB TM ) = exp −(E g − E X − E B − hν)/kB TM . By combining this expression with (8.12) we obtain, according to (8.7), the emission lineshape of biexciton luminescence (8.6). The reader will have certainly noticed that the above considerations were conducted under the tacit assumption of the validity of not only energy conservation, but also quasi-momentum conservation for the whole recombining biexciton population. In other words, all biexcitons are supposed to take part in the radiative decay, independently of the magnitude of their wavevector K. This represents a fundamental difference from the free exciton luminescence in direct-bandgap materials, where the radiative recombination can occur only for K ∼ = |0 and when the polariton effects play an important role, as we have clariﬁed in Subsection 7.1.2. When dealing with biexcitons we have not been speaking about polaritons at all. Is this standpoint correct? And if it is the case, then why? Yes, this approach is basically correct for the following reason: The biexciton momentum h¯ K is carried away by the so-called recoil exciton, which is released during the luminescence process h¯ K = h¯ Kphoton (∼ = 0) + h¯ Kexc ,

(8.13)

thereby ensuring the momentum conservation law for any value of K. For the same reason the inﬂuence of the polariton effects (being limited to a small region |K| ≤ 105 cm−1 ) on the overall emission lineshape can be, in a good approximation, neglected. From what has just been said it follows immediately that biexciton luminescence can become a very effective channel of radiative recombination in highly excited semiconductors, and may even take part in stimulated emission. The typical asymmetry of the free biexciton emission lineshape in direct-gap semiconductors is documented—in addition to Fig. 8.1—also in Fig. 8.4(a) [5]. The investigated material is crystalline copper chloride, CuCl; the solid curve denotes experimental data, the dashed curve represents the theoretical lineshape (8.6) with effective temperature TM = 18 K and binding energy E B = 28 meV. The presence of two lines is due to transitions to the longitudinal and transverse exciton states, split by ΔLT ≈ 5 meV. The relevant excitation photon (hνex ∼ = 3.7 eV) ﬂux was Iex = 8 × 1021 photon/cm2 s (Pex ≈ 2 4.8 kW/cm ). A further increase in excitation intensity leads to biexciton collisions accompanied by a deviation of the experimental lineshape from (8.6); the line becomes more symmetric. A temperature increase entails a similar effect. For the sake of comparison, Fig. 8.4(b) displays the biexciton emission line

211

212

Highly excited semiconductors

Fig. 8.4 (a) Biexciton emission spectrum in CuCl (direct-gap semiconductor) at a bath temperature of 4.2 K, excited by a pulsed N2 -laser (337 nm). Solid curve – experiment, dashed curve – theoretical lineshape after (8.6). The line MT (ML ) is due to a transition to the transversal (longitudinal) exciton level, respectively. After Grun et al. [5]. (b) Spectrum of edge emission of AgBr (indirect-gap semiconductor) at a bath temperature of 3 K under N2 -laser excitation, comprising a free exciton line ITO (FE) and a biexciton line M. This ﬁgure demonstrates clearly the mirror symmetry of both lines. Solid curve – experiment, symbols – theoretical ﬁt of the ITO (FE) line employing (7.16) and of the M line according to (8.16), using the 2 m parameter = (h¯ 2 /2 aM exc )/k B TM equal to 4. The effective temperatures of the exciton and biexciton gases turn out to be equal: TX = TM = 19 K. After Baba and Masumi [6].

in an indirect-gap semiconductor (AgBr [6]); the corresponding lineshape will now be discussed. Luminescence of excitonic molecule in an indirect semiconductor Given the exciton band minimum located at a wavevector K0 = 0, then biexcitons are characterized by wavectors around 2K0 . Consequently, phonons with momentum ∼ h¯ K0 (and energy h¯ ω) have to participate in the process of radiative biexciton decay. This is certainly an important difference with respect to the biexciton luminescence in direct-bandgap materials; nevertheless, we shall see that this fact has no principal impact upon the emission lineshape. The line will be—at low temperatures—of a shape very similar to the inverse Maxwell–Boltzmann distribution. We can draw such a conclusion by looking at Fig. 8.3(b). Downward transitions from the minimum of the EM dispersion curve (where at T ≈ 0 K the entire biexciton population occurs, having kinetic energy ŒM = 0) give rise to photons with maximum available energy hνM = E gi –E X –E B –hω, provided the ﬁnal state of the transition is located at the exciton dispersion minimum, i.e. at ŒX = 0; all other transitions (to higher exciton states) may result in lower photon energies only. Consequently, the emission line will have a sharp high-energy threshold on the one side, and a low-energy tail on the other—as yet, everything is basically the same as in biexcitons in direct-gap semiconductors. Even so, with rising temperature now the high-energy edge will become broader, because biexcitons will gradually occupy also higher states ŒM > 0 on their dispersion curve, and downward

Excitonic molecule or biexciton transitions from these states to the minimum of the exciton states ŒX = 0 yield photon energies higher than hνM = E gi − E X − E B − hω ≡ E 0 − hω. It is obvious that also in the indirect bandgap the entire population of biexcitons is participating in the luminescence process, because the law of momentum conservation is met again, this time owing to participating phonons hω. Let us now attempt to indicate how one can formulate a mathematical description of the emission lineshape. The concept of joint density of states cannot be—unlike the direct bandgap—introduced here. We have to deal with the task in a slightly different way, namely, in analogy with expression (5.10) that determines the luminescence lineshape of recombining free electron–hole pairs in an indirect bandgap. This expression is sufﬁciently universal. We can thus, making use of (5.10), write down for the case of EM luminescence in the indirect bandgap M 2 M ∼ (8.14) Iin (hν) = ρM (ŒM ) f M (ŒM )ρX (ŒX ) f X (ŒX ) Min dŒM , where ŒM and ŒX stand for the biexciton and exciton kinetic energy, ρ M (ŒM ) and ρ X (ŒX ) denote the densities of states in the biexciton and exciton bands, respectively, and f M and f X mean the relevant occupation factors. Meanwhile, M |2 within the integral and we have we keep the squared matrix element | Min not explicitly shown the integration limits. These can be found easily from Fig. 8.3(b). For a given constant value of hν we have to perform the integration with respect to ŒM obviously from a certain lower limit to inﬁnity; the lower limit can be derived from energy consideration (Fig. 8.3(b)) ŒX + (hν + h¯ ω) = ŒM + (E gi − E X − E B )

(8.15)

applied for ŒX = 0. Accordingly, making use of (8.15) yields for the lower limit ŒM = (hν + h¯ ω) − (E gi − E X − E B ) = hν + h¯ ω − E 0 . We denote this lower limit as hν = hν + h¯ ω − E 0 .3 In addition, with the aid of (8.15) one can write down ŒX = ŒM − hν and for the densities of states in the parabolic approximation of Œ(K) √ we obtain ρM (Œ M ) ≈ ŒM , ρX (ŒX ) ≈ (ŒM − hν). Thereby, expression (8.14) becomes ∞ IinM (hν) ≈

√ M 2 ŒM ŒM − hν f M (ŒM ) f X (ŒX ) Min dŒM.

hν

In the case of bosons occupying their ground state (i.e. excitons on their dispersion curve with a local minimum at K0 ) the occupation factor f X does not need to be taken into account. The biexciton population factor referring to the 3 It might be of interest to note that this lower limit hν may be considered an analogue of the upper limit in the integral (5.10). This ‘exchange’ of limits arises because here the parabolas of the excited (EM) and ground (FE) states are curved in the same sense.

213

214

Highly excited semiconductors upper dispersion curve reads f M (ŒM ) ≈ exp(–ŒM /kB TM ) and the biexciton emission line is therefore described by the integral ∞ IinM (hν) ≈

√ ŒM ŒM ŒM − hν exp − kB TM

M 2 Min dŒM.

(8.16)

hν

Until now we have always considered the matrix element M of the optical transition in integrals of the type (8.16) to be a constant, which can be put in front of the integral. However, this appears hardly acceptable here, for the simM |2 = const, then (8.16) would result in a monotonic increase ple reason: if |Min of the emission spectrum towards low-photon energies, which is physically impossible. Indeed, with decreasing hν (and thus also hν) the second term in the integrand (8.16) is increasing and, simultaneously, the integration range is getting broader while keeping all other parameters constant. Hence, various phenomenological models have been proposed to establish the dependence of M on Œ or K, i.e. M M = M M (Œ ) ≈ M M (K); this dependence should Min M M in in in M at K = 2K . Cho [7] has proposed produce a rather sharp maximum of Min M X a matrix element of the form 2 C0 M 2 , = | (8.17) | Min 2 2 (KM /2 − KX ) + (1/aM ) where C0 = const and aM stands for ‘biexciton radius’, or the average separation of the two holes in a biexciton. In other words, aM is a quantity determining the spatial extent of the biexciton wavefunction; as such, it is of the same order of magnitude as the exciton Bohr radius aX . The underlying physical background of expression (8.17) consists in the fact that the matrix element drops rapidly from its maximum value at KM = 2KX down to −1 . This reﬂects the ‘magnitude’ of the almost zero just for | KM /2 − KX | ≈ aM biexciton in real space. The radius aM thus becomes a crucial factor driving the emission lineshape; this factor is usually embodied in the dimensionless 2 m parameter = (h¯ 2 /2 aM exc )/k B TM . A detailed discussion of the emission lineshape (8.16) employing the matrix element (8.17) together with a hint for numerical integration can be found in Appendix C. Figure 8.4(b) shows the emission spectrum of AgBr in the edge emission region, acquired under high photoexcitation with a pulsed nitrogen laser. The spectrum contains two lines—an ITO (FE) line, ascribed to radiative decay of a free exciton accompanied with the emission of a TO-phonon, and an M-line being due to radiative decay of a biexciton. It is commonly supposed that biexciton annihilation is, apart from photon emission, accompanied with the emission of the same type of phonon as free exciton decay, i.e. a TO-phonon in this case. The biexciton line here therefore would have been correctly denoted as ITO (M) or ITO (EM) rather than simply M, if one insisted on strictly adhering to notation.4 Theoretical ﬁts (symbols) follow the experimental 4 It can be shown that a biexciton has in most cases the same full symmetry as the crystal ground state (1 ), hence the selection rules for biexciton and exciton luminescence are similiar to each other.

Excitonic molecule or biexciton data more than satisfactorily. It is seen that the typical M-line asymmetry— broadening towards the long-wavelength side, i.e. a resemblance to the inverse Maxwell–Boltzmann distribution—is indeed conserved even in indirect-gap semiconductors. M-line intensity dependence Apart from the lineshape analysis, the behaviour of the M-line as a function of the photoexcitation power density represents an important auxiliary guideline for ﬁrm identiﬁcation of the experimentally observed biexciton emission line. Intuitively we should expect this dependence to be quadratic. Although experiment does conﬁrm the dependence of the biexciton luminescence intensity n , the exponent n upon the excitation intensity to be superlinear, I M ∼ Iex amounts to only n ∼ = 1.4–1.6 in most cases. This rule holds independently of whether the forbidden gap is direct or indirect; n = 2 is seldom attained. An explanation has been put forward by the Knox et al. [8] through a kinetic theory, similar to the model discussed in Section 3.5, which describes the simultaneous occurrence of both monomolecular (here exciton) and bimolecular (here biexciton) luminescence. The authors [8] divide excitons photogenerated by band → band transitions into ‘optical’ and ‘thermal’ ones, supposing that biexcitons can be created by fusing thermal excitons only. They arrive at the M-line intensity dependence I M ≈ const( 1 + Iex /I0 − 1)2 ,

(8.18)

excitation intensity. where I0 stands for the characteristic material-dependent √ Evidently, for Iex I0 we can approximate 1 + Iex /I0 ≈ 1 + Iex /2 I0 and I M scales with Iex quadratically, while for Iex I0 the dependence (8.18) turns out to be linear: I M ∼ Iex . This corroborates qualitatively the experimental observations; the reader is reminded about the resemblance of (8.18) to relations (3.24) and (3.26). Simultaneously the model [8] predicts that the intensity dependence of free exciton luminescence should be linear, also in accordance with experiment. Figure 8.5 shows the superlinear growth of biexciton luminescence in AgBr 1.5 ). It may be of interest to specify the relevant experimental condi(I M ∼ Iex tions [9]. The excitation was performed by ∼ 2 ns pulses of a dye laser, the ITO (FE) and M lines were observable only in a temporal window coincident with the laser pulse; then the emission spectra and the intensity dependence were recorded. Further development of the spectra with increasing delay after the excitation pulse, recorded with the use of time-resolved spectroscopy, is displayed in Fig. 2.48. It can be seen how the fast edge emission ITO (FE) and M fades away, free excitons and biexcitons become gradually localized on the iodine ions and a slower emission band emerges at 500 nm, due to excitons localized on the isoelectronic impurity I− . To conﬁrm further the interpretation of the emission M-line as being due to EM decay, it is highly recommended to analyse its spectral position and temperature behaviour. They are closely connected with the determination of two important EM parameters: the binding energy E B and the radius aM .

215

216

Highly excited semiconductors

Fig. 8.5 Edge emission of AgBr under pulsed laser excitation at a bath temperature of T ≈ 10 K. The nonlinear growth of the biexciton M-line with increasing excitation intensity Iex (Im corresponds to ≈ 0.7MW/cm2 ) is clearly observable. The inset demonstrates the dependence of the integral M-line intensity 1.5 . The I (FE) line is due to I M ∼Iex TO free exciton decay, and the EHL line originates in the electron–hole liquid. After Pelant et al. [9].

8.2.2 Determination of biexciton parameters The biexciton binding energy E B in direct-bandgap semiconductors can be extracted readily and quite accurately from the emission spectrum. According to (8.5), E B is equal to the energy separation between the emission line of a free exciton–polariton and that of a biexciton, or more precisely, to the separation between the centre of the polariton line and the high-energy edge of the biexciton line. Less obvious is how to determine E B in a semiconductor with an indirect bandgap. There, the high-energy edge of the M-line gets broader at T > 0 K, as discussed in the context of Fig. 8.3(b). Fortunately the model [7], making use of the matrix element (8.17), comprises in the theoretical curve not only the relevant lineshape but also an energy position pertinent to the minimum of the biexciton dispersion ŒM (K). This position is indicated in Fig. 8.4(b) by a vertical line at 2.669 eV (∼ 464.5 nm). The determination of E B is then the same as mentioned above: as the energy separation of this line from the energy coordinate pertinent to the minimum of the exciton dispersion ŒX (K), i.e. from the vertical line at 2.676 eV (∼ 463.2 nm). This is how we get E B ≈ 7 meV in AgBr. This mode of assessing the EM binding energy is designated as spectroscopic. An independent determination of E B consists in investigating the intensity variations of the FE and M lines with varying temperature and can thus be called a thermodynamic method. It is applicable above all in indirect bandgap semiconductors where the free exciton emission line is sufﬁciently strong. The principle is as follows: In the course of sample heating, biexcitons undergo thermal dissociation more easily than free excitons do, because their binding energy is always smaller, E B < E X . Due to this, the M-line intensity

Excitonic molecule or biexciton

217

drops substantially faster compared with the intensity fall of the FE-line. In 2 ∼ thermodynamic equilibrium, and provided a quadratic proportion I M ∼ Iex FE 2 FE 2 M (I ) is valid, we can anticipate that the intensity ratio R = (I ) /I will be apparently driven by a factor exp(–E B /kB TM ). A more exact derivation leads to the even sharper dependence EB (I FE )2 k , (8.19) ≈ T exp − R= M IM kB TM where the value of the exponent k varies depending on whether the free movement of the quasi-particles FE, EM is not limited in any way (k = 3/2) or whether they are localized in a certain place of the sample, for instance in a potential well created by a local deformation of the sample (k = 3) [10]. A semi-logarithmic plot of R ∗ = (I FE )2 /I M TMk against 1/kB TM then yields E B as the slope of the straight line. Such a plot is shown in Fig. 8.6 for crystalline silicon at three different levels of laser excitation [10]. It can be seen that the slope, i.e. the binding energy E B , is independent of the excitation intensity (in fact, there is no reason why it should be dependent); we get E B = 1.53 meV, in good agreement with spectroscopic value E B = 1.46 meV. In this case the exponent k = 3 was applied in (8.19), because the gas of free excitons and biexcitons was spatially localized in a potential well. This localization made it possible to attain sufﬁciently elevated concentrations of both FE and EM under not excessive optical pumping levels. As a consequence of this approach a purely 2 ∼ (I FE )2 was observed in experiment—since quadratic dependence I M ∼Iex the condition Iex I0 was fulﬁlled in (8.18)—justifying the use of eqn (8.19). It is worth mentioning that experimentally observed binding energies E B in various materials systematically exceed theoretical values. This is documented in Table 8.1 (the only exception to this rule being copper halides CuCl and CuBr). The reasons are not clear. Often one blames the theoretical approaches for not taking into account at least two factors: (i) the effect of lattice polarization in polar semiconductors, which may raise E B substantially and (ii) the process of creating a biexciton from two excitons located at different valleys of the conduction (valence) band in indirect semiconductors. For in this way one can generate a two-electron triplet spin function connected with a lower Table 8.1 Comparison of the experimental and theoretical values of EM binding energy in several semiconductors (d – direct bandgap, i – indirect bandgap). The values of E B are given in meV. Semicondutor CuCl (d) AgBr (i) CdS (d) ZnO (d) GaAs (d) Si (i) Ge (i) HgI2 (d)

E B experimental

E B calculated

28–34 ∼7 ∼5 12–16 ∼ 0.7 1.2–1.5 ∼ 0.3 ∼6

41–44 1.3–2.5 2–5 5–9 ∼ 0.4 0.45–1.1 ∼ 0.1 ∼ 2.5

Fig. 8.6 Thermodynamic determination of the EM binding energy in silicon at three levels of laser excitation. Symbols— experiment, lines—ﬁt by the quantity 3 with the use of (8.19). R ∗ = R/TM Taking into consideration the relatively long lifetimes of participating quasi-particles along with not too high excitation, TM = T (bath temperature) holds. After Gourley and Wolfe [10].

218

Highly excited semiconductors lying energy level compared with a singlet state of two excitons located in the same valley (there, conforming to the Pauli exclusion principle, two electrons must be of antiparallel spins, i.e. total spin S = 0). Thereby the EM dispersion curve in Fig. 8.3(b) may shift downwards, raising the binding energy E B . The above considerations are in qualitative agreement with Table 8.1. The most marked difference between the experimental and theoretical values of E B occurs in AgBr, where—as in a polar, indirect-gap semiconductor—both factors enter the play. Any quantitative theoretical estimates are lacking, though. The second biexciton parameter, the radius aM , can be found relatively easily from luminescence measurements in indirect semiconductors. When ﬁtting the experimental lineshape with relations (8.16) and (8.17), the variable para2 m meters are = (h¯ 2 /2aM exc )/k B TM together with the reduced wavelength axis hν/kB TM = (hν + h¯ ω − E 0 )/kB TM [7]. This enables an independent determination of both TM and aM . The ﬁt shown in Fig. 8.4(b) yields, for AgBr, = 4, TM = 19 K and aM ≈ 2.6 nm. In direct-bandgap semiconductors, on the other hand, there is no similar straightforward and commonly accepted method to establish aM experimentally. The last remark in this section concerns bound (localized) biexcitons. It has been found that free biexcitons, similarly to free excitons, can get localized close to impurity atoms. Actually, this is not surprising if we recall bound multiexciton complexes (Subsection 7.2.1). A bound biexciton can be regarded as a limiting case of a bound exciton complex composed of two excitons, even though the process of creation (localization) may be slightly different. In the case of high excitation, biexcitons as a whole get localized preferentially. The relevant emission line, originating in radiative decay of bound biexcitons, is red-shifted with regard to (E g(i) –E X –E B ) and features properties analogous to other extrinsic radiative channels, namely, its shape is symmetric, does not vary either with excitation intensity or temperature and the line exhibits saturation behaviour. Bound biexcitons have been discovered via luminescence measurements in GaP, CuCl and AgBr.

8.3 Collisions of free excitons

Fig. 8.7 Free exciton collisions in the E(K) scheme. K, K denote the exciton wavevectors before the collision, k is pertinent to internal e–h pair movement (h 2 k 2 /2m r ) and K to its translation movement (h 2 K 2 /2(m e + m h )) after the collision.

Another type of interexciton interaction that can manifest itself in luminescence spectra at higher excitation power densities is inelastic collisions between free excitons (X–X collisions). Two FEs, instead of fusing and creating an EM, collide with one another while one of the two FEs dissociates into a free e–h pair and the remaining one recombines radiatively emitting a photon hν P . This photon energy, however, is reduced compared to the n = 1 FE state by an amount passed over to the ﬁrst exciton and making it dissociate—and this is the very exciton binding energy E X . Let us consider a direct-bandgap semiconductor, Fig. 8.7. Energy balance then reads 2 free excitons → photon + free e–h pair kin ), (E g − E X ) + (E g − E X ) ≈ hνP + (E g + E e,h

Collisions of free excitons

219

and thus kin , hνP ≈ (E g − 2 E X ) − E e,h

(8.20)

kin = h 2 k 2 /2 m +h 2 K 2 /2 (m + m ) stands for the kinetic energy where E e,h ¯ r ¯ e h of the created electron–hole pair. A new emission P-line therefore appears, redshifted from the spectral position of an exciton–polariton (which is E g –E X ) roughly by E X (see Fig. 8.1 and Problem 8/1). Experiment reveals that the ﬁnal state in this collision process does not necessarily have to be always a free e–h pair. The exciton, acquiring energy at the collision, may happen to be excited only to some higher lying but still bounded exciton state (n = 2, 3, 4, . . .) and the energy of the emitted photon is then

hνPn ≈ (E g − E X ) − E X (1 − 1/n 2 ), n = 2, 3, . . . , ∞,

(8.21)

which is nothing but a generalization of (8.20) with simultaneous neglect of kinetic energy. In Fig. 8.8 there are emission spectra of a high-purity monocrystalline ZnO sheet under high excitation with an electron beam at T = 10 K [11]. Owing to the extreme purity, the emission line of the exciton localized on a residual impurity (denoted I9 ) is strongly suppressed, enabling the observation of two lines in the P-band, corresponding to photon energies hν P2 and hν P∞ according to (8.21). The basic features of the spectral shape of the emission line accompanying the creation of a free e–h pair (n = ∞) can be readily guessed: The P∞ line should have a high-energy threshold at E g –2E X and is expected to be asymmetrically broadened towards the low-energy side, since for the e–h pairs there exists a continuum of energy states. The creation of an e–h pair with high kin then leads, in compliance with (8.20), to the emission of kinetic energy E e,h lower-energy photons. Moriya and Kushida studied this lineshape theoretically in the framework of perturbation theory and found that [12] P∞ Isp (hν)

∞ ∞ P 2 3 2 ≈ M h ν n X dξ dt

1 × exp −t − 4t

0

0

ξ 1/2 (1 + ξ/E X )4

E g − 2 E X − hν − ξ kB T

2 (8.22)

(M P denotes the optical matrix element and n X the concentration of free excitons). The physical meaning of the double integration in (8.22) consists in the fact that photons with a given energy hν may originate from numerous combinations of initial (K, K ) and ﬁnal (k, K ) wavevector pairs. In practise, however, this theoretical lineshape is seldom compared with experiment. There are several reasons for this. On the one hand, a background composed of many lines due to impurities (BE, e–A0 , h–D0 , etc.) often occurs in this spectral region, which makes the lineshape analysis of the P-line difﬁcult; on the other hand, the very theoretical expression (8.22) is based on a simpliﬁed approximation of the interaction potential between the two excitons which is,

Fig. 8.8 Emission spectra of pure ZnO under electron beam excitation (40 kV, ∼ 100 ns pulses) with two different current densities Jex . Apart from the P-band, the bound exciton line I9 and its LO-phonon replicas can be seen. The P-band grows superlinearly with increasing excitation current density at the expense of other lines. Arrows indicate emission wavelengths calculated using (8.21) for n = 2, 3, 4, and ∞. T = 10 K. After Hvam [11].

220

Highly excited semiconductors in reality, rather complicated. It is worth noting that (8.22) contains a term n 2X , P upon the excitation therefore one can expect a quadratic dependence of Isp intensity; Fig. 8.8 basically conﬁrms this expectation. The close resemblance of the M- and P-lines (superlinear growth, line asymmetry) invokes the following questions: When can we in an experiment expect the creation of excitonic molecules and when are inelastic exciton collisions more likely to occur? Or do both of these mechanisms take place always simultaneously, as Fig. 8.1 indicates? The answer to these questions is neither simple nor unambiguous. There is no strict theoretical prediction as to when (at what excitation level) and where (in what material) we should expect this mechanism or that one to occur. Of course, in a qualitative manner we can come to the conclusion that the fusion of two excitons into an EM will prevail at relatively lower excitation power densities and provided E B is sufﬁciently large. For if we create a very high concentration of free excitons possessing, moreover, a non-equilibrium excess kinetic energy (‘optical excitons’ introduced in Subsection 8.2.1), then the collision process will probably predominate. (The interacting excitons will ‘have no time’ to fuse; only a collision followed by one exciton annihilation will set in.) The observed predominance of exciton collisions under pumping with high current density electron beams seems to support this conjecture. However, there is certainly a relatively broad range of laser excitation power densities where both ‘M’ and ‘P’ actions occur simultaneously. Radiative decay of the EM as well as luminescence due to exciton collisions can easily result in stimulated emission, as we shall see later. All considerations held in this section concerned direct-badgap semiconductors. Till now the P-line has not been observed in any indirect-bandgap material (Problem 8/3). On the contrary, in the next section we shall discuss a luminescence process taking place exclusively in indirect semiconductors, namely, radiative annihilation of an electron–hole liquid.

8.4 Electron–hole liquid (EHL) Another qualitative alteration of luminescence (but not only luminescence) behaviour of a semiconductor, linked with high exciton densities, is exciton condensation into a new state of matter, named an electron–hole liquid, EHL. We have already introduced the concept of an exciton gas; the condensation of excitons represents a phase transition that can be regarded as a quantummechanical analogue of the well-known classical gas condensation into a liquid (water vapour molecules in the atmosphere condense into droplets constituting fog or rain). In the case of excitons one speaks of a Fermi liquid—a degenerate electron–hole system—composed of free fermions, electrons and holes. Similarly to the classical case, also particles of this particular liquid form spherical drops, inside which they are held together by means of internal forces and surface tension; hence also the term electron–hole drops (EHD) is sometimes used. The typical diameter of these drops amounts to several μm. It should be stressed again that the drops do not contain excitons but free electrons and

Electron–hole liquid (EHL)

221

Fig. 8.9 The phase diagram of photoexcited electrons and holes in silicon. It can be deduced, e.g., that for an average e–h pair density of ∼ 1017 cm−3 and T = 15 K a saturated free exciton gas with a density about 1016 cm−3 coexists with drops of EHL; in each of these drops there is a concentration of e–h pairs ∼ 3 × 1018 cm−3 . The dashed curve and open symbols denote theoretical and experimental values of the Mott insulator–metal transition (Section 8.5). After Shah et al. [13].

holes. The thing is that excitons in the condensate immediately ‘break up’, therefore the designation ‘exciton drops’, which is sometimes used, is not correct. The density of e–h pairs inside the drops may be higher by several orders of magnitude than the concentration of excitons remaining in the surrounding gas phase, as we shall see shortly. To liquefy a classical gas, it is necessary to reach a critical pressure and to descend below a critical temperature, the whole process being advantageously sketched in a p, T (pressure, temperature) diagram. As for the exciton concentration, it appears more illustrative to apply an n, T (density, temperature) coordinate system and to speak about the critical density n c of e–h pairs and the critical temperature Tc of the liquid. The phase diagram of an electron–hole system in silicon is shown in Fig. 8.9. The values of the critical temperature and the critical density are Tc = 25 K and n c = 1.2 × 1018 cm−3 , respectively. An EHL cannot survive for T > Tc . The e–h pair density in EHL at a given temperature is driven by the liquid interface of the two-phase coexistence region (shadowed area), where the e–h system separates into a liquid and the surrounding gas phase. It can be seen that this density is n 0 ≈ 3 × 1018 cm−3 and is only weakly temperature dependent in the range 0–15 K. On the left and above the coexistence region only the gas of free excitons may subsist. Similarly to the case of excitonic molecules, of fundamental importance is now to ask about the stability of the EHL, or to ask which parameter plays the role of the binding energy E B here. Prior to establishing such a parameter, we deﬁne the ground state energy E G (n) of the liquid, allotted per one e–h pair. This energy is given by the sum of the kinetic, exchange and correlation energies and it exhibits, as a function of the e–h pair density, its minimal value at the equilibrium density n 0 . Should the EHL be a stable and energetically favourable phase compared to the free exciton gas, this minimum must be located deeper than the ground exciton state level, referred to the bottom of the e–h continuum of states. In Fig. 8.10, this means that the relation |E G (n 0 )| > E X must hold. The difference ϕ = |E G (n 0 )|–E X then represents the (material dependent) EHL stability parameter we are looking for. ϕ is called the binding energy of the condensate with respect to free excitons (or, in analogy with thermionic electron emission, the work function). It is the energy

Fig. 8.10 Schematic drawing of the EHL ground state energy per electron–hole pair as a function of the reciprocal pair density.

222

Highly excited semiconductors required to ‘evaporate’ one e–h pair from the liquid.5 The condensate is stable if and only if ϕ > 0. Various theoretical approaches to calculate E G (n) or ϕ, along with obtained results, are summarized, e.g., in [14] and [15]. Theory reveals that the EHL stability may proﬁt from speciﬁc features of the energy band structure of indirect-bandgap semiconductors. In particular, the long exciton lifetime and several equivalent conduction band minima νc , in, e.g., Si and Ge (or several equivalent valence band maxima νv in AgBr) promote the chance of photoelectrons (photoholes) to reduce efﬁciently their kinetic energy. This entails an important increase in stability and cohesiveness of the condensed phase. Quantitatively, the increased number of equivalent band extremes νc (νv ) appears in the expression for the density of states in the bands. Instead of (5.4) we have to be more speciﬁc now and write down ρc (E) = νc

(2 m de )3/2

ρv (E) = νv

2 π2 h¯ 3

1/2

Ee ,

(2 m dh )3/2 1/2 Eh . 2 π2 h¯ 3

(8.23)

The factors νc and νv describe the fact that the electrons and holes have at their disposal νc -times or νv -times more available states, respectively, in comparison with a semiconductor having a single band extreme. (In a semiconductor characterized by a simple band structure with a direct bandgap at the point, νc = νv = 1 holds, while in silicon νc = 6, νv = 2.) Furthermore, instead of simple effective masses m e , m h , which belong to idealized parabolic bands, we have to consider now the so-called density-of-states effective masses m de , m dh that take into account the complex band structure of real semiconductors Si, Ge, AgBr, etc. Namely, they involve the anisotropy of the effective mass and the existence of heavy and light holes with markedly different masses [14]. The kinetic energy of photocarriers gets reduced because its mean value is equal to 3/5Fe and 3/5Fh (Fe , Fh being the Fermi energies of electrons and holes, respectively), see Problem 8/4. A pure mechanical analogue may be invoked: if we pour a liquid (here the photoexcited electron–hole ﬂuid) uniformly into several vessels (here several valleys of the conduction or the valence band) instead of a single one, the liquid levels in the vessels become inversely proportional to the number of vessels used. It has been demonstrated that further promotion of ϕ arises from the interaction of electrons and holes with LO-phonons. A very stable EHL with a high Tc therefore occurs in polar semiconductors with an indirect bandgap (AgBr, GaP). On the contrary, the short exciton lifetime along with the single conduction band valley in the point of direct semiconductors do not allow the necessary conditions for exciton condensation to be reached, even though this issue had been intensively discussed throughout the 1970s and 1980s.

5 Upon leaving the condensate, such a pair is immediately bound and creates a free exciton.

Electron–hole liquid (EHL)

223

8.4.1 Luminescence determination of EHL parameters The EHL represents an electronic excited state of a semiconductor, which fades away rapidly (10−9 –10−6 s) after the cessation of the excitation effect. However, the EHL emits its characteristic luminescence radiation that originates (even in the steady state) through the radiative recombination of electrons and holes constituting the condensate. The probability of radiative recombination in the EHL is even increased several times compared to a system of free carriers of the same density (due to the so-called enhancement factor) because of the correlation existing between the electrons and holes. The EHL luminescence is of intrinsic type and its emission spectrum features a relatively broad band rather than a single narrow line; this reﬂects the Pauli exclusion principle, according to which each level in a system of fermions can be occupied by two electrons (or holes) at the most (Fig. 8.11). Referring to what has been discussed above, this band appears in the emission spectrum as soon as the pumping level exceeds a certain threshold level, provided the condition T < Tc holds at the same time. Let us now discuss what the emission bandshape looks like; simultaneously we shall learn how we can, by analysing the emission spectrum, extract the two most important EHL parameters, namely, n 0 and ϕ. These are listed, for selected semiconductors, in Table 8.2. The formation of EHL luminescence is evident from Fig. 8.11. The emission lineshape is deﬁned through a combination of all the occupied electron states with all the occupied hole states, the momentum conservation rule for all recombining e–h pairs being ensured through the participation of a phonon h¯ ω. Formally therefore we can start with the convolution integral (5.10) that has been derived for allowed indirect recombination processes

I

EHL

hν √ (hν) ≈ |M| E hν − E f c (E) f v (hν − E)dE, 2

(8.24)

0

and where hν = hν + h¯ ω − E g . Now we perform in (8.24), compared to (5.10), two formal adjustments and then one essential physical modiﬁcation. Table 8.2 The basic EHL parameters of selected semiconductors (experimental values); n 0 , ϕ and Tc denote the equilibrium density, the binding energy and the critical temperature, respectively. Semiconductor

n 0 (cm−3 )

ϕ (meV)

Tc (K)

Ge Si GaP AgBr TlBr (2)

2.4 × 1017 3.3 × 1018 6 × 1018 8 × 1018 1.4 × 1019

1.5 8 15 55 –2.2

6.5 25 40 ∼ 60 (Tef ≈ 100)(1) –

Note: (1) Owing to the short lifetime, the effective critical temperature Tef is higher than the bath Tc . (2) Theoretically calculated values.

Fig. 8.11 Schematic of EHL recombination radiation. A photon hν originates via the recombination of an electron with a hole from the corresponding Fermi seas. Electrons occupy the conduction band up to the electron Fermi level Fe ; in a similar manner levels in the valence band are occupied by holes up to the hole Fermi level Fh . E g means a reduced bandgap (< E g ). For the sake of simplicity the transitions are drawn as direct transitons. μ = E g + Fe + Fh stands for the EHL chemical potential.

224

Highly excited semiconductors Under formal adjustments we omit the phonon energy h¯ ω in (8.24) and replace E g by the so-called reduced or renormalized bandgap E g < E g ; therefore we put hν = hν − E g . The omission of h¯ ω serves only to simplify our reasoning; this step does not affect the emission spectral shape, shifting it only— as a whole—on the photon energy axis. Graphically, we can then illustrate the EHL recombination radiation as if it were due to direct transitions (Fig. 8.11); we shall see later that this simpliﬁcation will turn into a certain beneﬁt. Introducing the reduced bandgap E g has a deeper physical meaning: it tells us that the high density of e–h pairs inside the condensate droplets entails a reduction of the bandgap E g (calculated within the one-electron approximation or found experimentally, e.g. with the aid of optical measurements using lowintensity light) down to a value E g < E g . We shall investigate this effect more closely in Section 8.5. For luminescence measurements, this has a practical consequence, namely, the recombination radiation originating inside the drops is not absorbed in the surrounding lattice and can be easily detected. The essential physical modiﬁcation, indicated above, compared to the luminescence of an e–h system under weak excitation (Subsection 5.2.2) consists now in introducing into (8.24) for f c and f v the relevant Fermi–Dirac distribution functions in the conduction and the valence bands, respectively. Therefore, (8.24) becomes

I

EHL

−1 hν √ E − Fe +1 (hν) ≈ E hν − E exp kB T 0

exp

hν − E − Fh kB T

−1 +1

dE.

(8.25)

The integrand does not contain any singularities and thus to calculate (8.25) for ﬁtting the experimental emission spectrum, any simple numerical method may be used.

Fig. 8.12 (a) Schematic of the emission spectrum comprising the EHL band and a free exciton line FE, indicating at the same time how to determine the binding energy ϕ. (b) Experimental and theoretical (eqn 8.25) lineshapes of the EHL band (LA-phonon replica) in pure Ge. The FE line is not displayed. The less-intense band at ∼ 0.7 eV is a TO-phonon replica of the EHL luminescence. After Benoit a` la Guillaume and Voos [16].

Determination of the reduced bandgap Eg and the potential μ Close to the temperature T = 0 K, the emission spectrum obviously starts on the short wavelength side at hν = μ and terminates on the long-wavelength side at hν = E g (let the reader compare Figs 8.11 and 8.12(a)). Photoluminescence therefore turns out to be a unique method for a direct determination of auxiliary EHL parameters such as the reduced bandgap E g and the chemical potential of the electron–hole liquid μ = E g + Fe + Fh . The ﬁt parameters6 in (8.25) are Fe , Fh and T . They are not independent of each other, however, which somewhat complicates the ﬁtting procedure based on eqn (8.25). This procedure is connected with the extraction of the density n 0 from the luminescence spectrum, a process that we are now going to describe. 6 E appears to be also a ﬁt parameter, however, it does not affect the bandshape but shifts g the overall spectrum on the wavelength axis only. It can be extracted from the ﬁnal ﬁtting of the calculated curve on the experimental spectrum.

Electron–hole liquid (EHL) Determination of the electron–hole density n0 The simplest way to determine n 0 can be realized at very low temperatures. Let us consider the limit case T = 0 K. The EHL emission band has a full width (at its foot) E F = Fe + Fh = μ − E g (Figs 8.11 and 8.12). From here, n 0 will be extracted as follows: The electron density n e (= the hole density n h ) is given by summing over all occupied states in unit volume, which is generally expressed as ∞ n0 = ne = nh =

∞ ρc (E) f c (E, Fe ) dE =

0

ρv (E) f v (E, Fh ) dE 0

and, by considering explicitly the densities of states (8.23), the above expression transforms into −1 ∞ √ νc(v) (2 m de(h) )3/2 E − Fe(h) + 1 n0 = ne = nh = E exp dE. kB T 2 π2 h¯ 3 0

(8.26) For T = 0 K (and solely in this case) the integration can be performed analytically which yields νc νv (2 m de Fe )3/2 = (2 m dh Fh )3/2 (8.27a) n0 = 3 2 3 π h¯ 3 π2 h¯ 3 or 2/3

νc

m de Fe = νv2/3 m dh Fh .

(8.27b)

Ultimately the relationship between the full width of the band E F and the concentration n 0 follows from E F = Fe + Fh , which combined with (8.27b) gives −1 2/3 m de νc Fe = 1 + EF. (8.28) νv m dh Therefore, upon obtaining experimentally the full width E F of the emission band we are able, making use of (8.27a), (8.28) and of the band structure 3/2 parameters, to calculate n 0 immediately. It can be seen that n 0 ∼ E F ; the wider the luminescence band, the denser the EHL. For T = 0 K the procedure is similar, the expression (8.26) being no longer computable analytically, though. The integration has to be performed numerically. The method of determining n 0 then cannot be separated from ﬁtting the emission bandshape, as we have already mentioned. The experimental EHL band is ﬁtted with the aid of (8.25), letting the values of the couple Fe , Fh vary, but keeping their ratio ﬁxed, as follows from the numerical integration of (8.26) or, in other words, from the condition of the electroneutrality of the condensate n e = n h . (This means that the e–h pair density n 0 = n e = n h enters the spectral shape (8.25) implicitly.) The temperature T represents the next ﬁt parameter, as already mentioned above; this effective temperature can again be higher than the lattice temperature. It should be noted, however, that at a sufﬁciently low bath temperature the simple

225

226

Highly excited semiconductors determination of n 0 through a combination of (8.27) with an iterative analytical calculation of the bandshape (8.25) for T = 0 K is often applicable. That is to say, the spectral shape undergoes only an insigniﬁcant modiﬁcation around μ , as demonstrated in Fig. 8.12(b) [16]. Determination of the binding energy ϕ From the above ﬁtting procedure one gets the value of the reduced bandgap E g together with Fe (T ) and Fh (T ). Their sum deﬁnes the chemical potential: μ (T ) = E g + Fe (T ) + Fh (T ). We shall show before long that μ is the spectroscopic energy characterizing the EHL ground state, i.e. it corresponds to the energy E G (n 0 ). Then it is readily seen in Figs 8.10 and 8.12(a) that the condensate binding energy ϕ (with respect to a free exciton) may be extracted very simply as the separation between μ and the low-energy edge of the FE emission line, whose spectroscopic position is denoted E X in Fig. 8.12(a): ϕ(T ) = E X − μ (T ).7

(8.29)

Why, then, does μ (T ) characterize the EHL ground state? We come to this conclusion by means of simpliﬁed reasoning, the origin of which is ascribed to Keldysh: the maximum EHL luminescence photon energy at T = 0 K is determined by the radiative recombination of an electron with a hole which reside on their Fermi levels; in other words, such recombination leaves the EHL in its ground state (any other recombination event leaves behind the EHL in an excited state, because for instance an unoccupied state at energy lower than Fe appears in the electron Fermi sea, and a redistribution of the population on electron levels must follow to restore the ground state). Consequently, μ is the spectroscopic energy relevant to the EHL ground state. This can also be shown computationally (Problem 8/5). This determination of ϕ is essentially spectroscopic, much like the case of the determination of the binding energy E B of an excitonic molecule. Similarly, also here the possibility exists to set ϕ thermodynamically. In this case ϕ is obtained as the activation energy from plotting, e.g., the exciton density on the gas–liquid boundary against temperature (Fig. 8.9). The excellent treatise of these methods as well as of other luminescence manifestations of the EHL can be found in the monograph [17].

8.4.2 Identiﬁcation of the EHL emission band Now we can summarize the typical spectral features that differentiate EHL luminescence from plenty of other lines or bands in the emission spectrum: 1. With increasing excitation intensity (even over several orders of magnitude) the EHL band ﬁrmly keeps its shape and position, i.e. neither band broadening nor a spectral shift occurs. This is due to the fact that the liquid density n 0 is constant at a given temperature (Fig. 8.9). An increase in the 7 Also E and E are dependent on temperature but this dependence is weak in comparison g X with the temperature dependencies Fe (T ), Fh (T ) and μ (T ).

Electron–hole liquid (EHL)

227

pump power density entails—no doubt—an increase in the total volume occupied by the drops and thus naturally also an increase in the emission intensity I EHL , but the relevant spectral shape, driven by the density n 0 , does not vary. 2. With increasing temperature two contradictory effects happen: the highenergy edge broadens (because more and more electrons and holes are excited above the respective Fermi levels), but, at the same time, the FWHM of the band gets slightly narrower (because the liquid density with increasing temperature drops slightly due to thermal expansion—see the liquid boundary of the phase diagram in Fig. 8.9). Consequently, the chemical potential μ (T ) = E g + Fe (T ) + Fh (T ) is a decreasing function of T , or ϕ(T ) becomes, according to (8.29), an increasing function of temperature; it turns out that this function can be written as ϕ(T ) = ϕ(0) + a(kB T )2 , where a is a constant of the order of 1 meV−1 . 3. The EHL phase diagram implies the existence of two distinct thresholds connected with EHL luminescence. The EHL band appears in the emission spectrum upon reaching an intensity threshold, which is nicely demonstrated in Fig. 8.13 [18]. On the other hand, the EHL band disappears

Fig. 8.13 Emission spectrum of ultrapure Ge at T = 2.1 K under excitation with a tungsten lamp. (a) Excitation intensity is below the threshold for exciton condensation into the EHL. Only LAand TO- phonon replicas of the free exciton are present. (b) Excitation intensity has been 2.2× increased. Suddenly the EHL band (LA-replica) at ∼ 708.5 meV appears. After Westervelt [18].

228

Highly excited semiconductors

Fig. 8.14 Fast component of AgBr luminescence under pulsed laser excitation (380 nm, 6 ns). (a) Excitation intensity 50 kW/cm2 . Only the ITO (EHL) band and a weak free exciton line ITO (FE) occur. (b) Excitation intensity of 5 MW/cm2 . This high excitation induces, apart from the ITO (EHL) and ITO (FE) lines, also a very strong M-line due to excitonic molecules. Bath temperatures are indicated. The critical bath temperature is Tc ∼ 60 K, which corresponds to the effective critical temperature of the e–h system of about 120 K. Symbols denote the theoretical shape (8.25) for n 0 = 8 × 1018 cm−3 . The intensity scales in (a) and (b) are not comparable. After Hulin et al. [19].

sharply upon reaching a temperature threshold (the critical temperature Tc ), as can be seen in Fig. 8.14 [19]. The occurrence of both thresholds follows also from a simple kinetic model of nucleation and decay of electron–hole drops, see Appendix D. The salient features (1.–3.) are very characteristic and enable one, as a rule, to make a facile identiﬁcation of the EHL luminescence. Moreover, the considerable bandwidth of the EHL luminescence compared with, e.g., exciton lines may serve as primary guidance (see Fig. 1.1 where the replicas ILO,TO (EHL) and ITA (EHL) in silicon contrast with the narrow lines of free, FE, and bound, BE, excitons). On the other hand, neither the analysis of the luminescence decay curves nor the shape of the intensity dependence of the EHL band is a reliable guide in this case. EHL luminescence decays faster than the free exciton emission (owing to Auger recombination in drops), but the shape of the decay curves as well as that of the intensity dependence may be strongly affected by the presence of parallel recombination processes (EM, BE, etc.).

8.4.3 Coexistence of excitonic molecules with electron–hole liquid We have seen that under strong excitation various exciton interactions take place, among which especially EM and EHL affect signiﬁcantly the lowtemperature emission spectrum. Let us now ask whether in a semiconductor both the condensation of excitons into an EHL and the fusion of excitons into an excitonic molecule can occur simultaneously, or whether these are two

Electron–hole liquid (EHL) ‘disjunctive’ processes in the sense that in a given material these may exist— depending upon the speciﬁc band structure—always just one of them.8 The attentive reader already knows the answer, of course. Comparison of Tables 8.1 and 8.2 shows that in AgBr, Si and Ge simultaneously E B > 0 and ϕ > 0 hold, hence the gas of excitonic molecules can indeed coexist with the electron–hole liquid, In spite of this, there are certain points here—ﬁrstly, the remarkable historical context (the interpretation of the ﬁrst luminescence experiments in highly excited Si and Ge crystals in the 1960s and 1970s oscillated between the EHL and EM models, because the correct answer to the above question was not known) and, secondly, interesting experimental aspects—which are worth mentioning. Figure 8.14 compares AgBr emission spectra under a relatively low pulsed photoexcitation (50 kW/cm2 , panel (a)) with those taken with the excitation power density two orders of magnitude higher (5 MW/cm2 , panel (b)). Somewhat surprising is the occurrence of the M-line at the higher excitation only, while the EHL band is present in both these cases. It follows from these observations that, ﬁrstly, the equilibrium between the biexciton gas and the EHL (and, possibly, also the FE gas) may be limited to only a certain part of the phase diagram in the (n, T ) plane, the so-called biexciton pocket [19]. Secondly, it turns out that the exciton condensation into an EHL is not entirely a typical ‘high excitation effect’; a comparable, or perhaps an even more important role is played by a sufﬁciently low temperature. Condensation may often be achieved by making use of cw incandescent lamp excitation (see, e.g., Fig 8.13). In Ge and Si the biexciton binding energy EB is very small, not only in comparison with ϕ, but also absolutely. Consequently, at sufﬁciently low temperatures excitons very willingly condense into an EHL and thus the M-line cannot be observed at all, see Figs 1.1, 8.12 or 8.13. This is because the density of the surrounding free exciton gas, n X , is low and biexcitons cannot form. If we simply decide to heat the sample in order to increase n X and thus create biexcitons (which was realized in AgBr through heating the e–h system with powerful laser pulses, see Fig. 8.14(b)), we shall be faced with a problem. It is true that upon increasing the temperature by a couple of degrees we shall ‘evaporate’ more excitons, but at the same time we might already prevent biexciton formation because kB T ≈ E B will hold. Ultimately, at T > Tc we shall dissolve the EHL entirely. Such a straightforward route cannot be applied, therefore the issue of the coexistence of EM with EHL remained unresolved for a long time. We have to make the conditions for exciton condensation difﬁcult, i.e. to make the EHL less stable, e.g. via stressing a Si sample along the [100] direction. In this way we lower the crystal symmetry and reduce the number of equivalent conduction band valleys νc from six to two. Therefore—according to what has been outlined above—we reduce the condensate binding energy ϕ. This means that the exciton gas surrounding the EHL drops gets denser, biexcitons can thus be created and, in the luminescence, the M-line appears. This is documented in Fig. 8.15 [20].

8 With regard to what has been outlined in the introduction to Section 8.4, this inquiry concerns indirect-bandgap semiconductors.

229

Fig. 8.15 Time-resolved emission spectra of a pure Si crystal, stressed along [100] at T = 8 K. Numbers at the curves indicate delay times (μs) after the excitation pulse. Besides the coexistence of all three phases—EHL, gas of FE and gas of EM—the ﬁgure also demonstrates the very rapid decay of the EHL luminescence. After Kulakovskii and Timofeev [20].

230

Highly excited semiconductors

Fig. 8.16 Schematic cross-section of a (indirect-bandgap) semiconductor sample excited by light at low temperatures. Various luminescence processes are shown. After Westervelt [18].

An illustration of several parallel luminescence channels in semiconductors is given in Fig. 8.16. Let us add that, by using a special luminescence technique, the coexistence of an EHL with free polyexcitons (apart from biexcitons, with triexcitons and tetraexcitons) has been observed, particularly in silicon [21].

8.5 Electron–hole plasma (EHP) 8.5.1 Mott transition Let us disregard for a moment the fact that the condensation of excitons can give rise to EHL drops. We thus have a gas of free excitons, the density of which, n X , is continuously increased through the enhancement of excitation intensity. At the same time we also increase the number of free electron–hole pairs N , for a certain number of excitons always become ionized, even at low temperatures. In this way we reach a density NM at which excitons as bound e–h pairs cease to exist. The reason for this resides in the effective screening of the Coulomb interaction between electrons and holes owing to the surrounding free carriers;9 instead of (7.1), the interaction potential becomes Us (r ) = −

e2 exp(−ksr ), 4 π ε0 ε r

(8.30)

where ks = ks (N ) > 0 is the so-called screening factor. Alternatively, λs = ks−1 is called the screening length. Relation (8.30) is known, e.g., from plasma physics. The screening length λs (N ) gets shorter with increasing e–h pair density N . When λs approaches the free exciton radius aX , excitons become unstable— the attraction between the electron and the hole is destroyed. As a ﬁrst consequence of the screening (8.30), therefore, the transition of the exciton gas 9 The proximity of other excitons operates in the same sense but it is commonly accepted that the main contribution to the screening comes from free electrons and holes.

Electron–hole plasma (EHP)

231

(composed of bosons) through ionization to an electron–hole plasma (EHP) of a metallic character (i.e. driven by Fermi statistics) appears. This process represents one of a variety of possible realizations of the so-called Mott insulator– metal transition. The relevant density NM is called the Mott density. Bandgap renormalization arises as a second consequence. We have to realize that now we are far beyond the one-electron approximation. Due to Coulomb correlation and exchange effects, at high density of electron–hole pairs/excitons the semiconductor bandgap reduces to E g (N ) < E g . This can be demonstrated via a simple calculation, which compares the self-energy of a point charge in a many-electron system with that derived in the one-electron approximation [22] E g (N ) = E g (N ) − E g = lim [Us (r ) − U (r )]

r →0

exp (−ksr ) − 1 = lim 4 π ε0 ε r →0 r e2

=

e2 e2 lim −ks exp(−ks r ) = − ks (N ) < 0, (8.31) 4 π ε0 ε r →0 4 π ε0 ε

where we have used l’Hospital’s rule. It follows immediately that E g (N ) < E g ; the renormalization therefore entails a reduction of the bandgap (‘gap shrinkage’) in a dense electron–hole ensemble compared to the oneelectron value E g . The Mott transition in an excitonic system is displayed schematically in Fig. 8.17. Already at densities N smaller than NM by two orders of magnitude the value E g begins to drop; at the Mott density NM the curves E g (N ) and the ground exciton level n = 1 cross each other, which means that E g (N ) < E g (0) − E X for N > NM . In other words, for the e–h system it becomes energetically more favourable to be in the continuum of states of free e–h pairs than to be bound into excitons. It might seem strange that the exciton n = 1 level is independent of N . In fact, however, this indicates that the binding energy E X also drops with increasing N (due to screening) and this drop in E X is just compensated by the drop in E g (N ). This information is very important because it tells us that the Mott transition to EHP is—unlike EHL nucleation—gradual, i.e. excitons do not disappear suddenly upon reaching NM , but their concentration decreases slowly as a function of the increasing excitation intensity.10 The Mott density NM can be calculated within various approximations. The calculation is fairly easy to perform considering a non-degenerate EHP with relevant Fermi distribution functions approximated by Boltzmann tails. The screening length λs is then called the Debye–H¨uckel screening length and one gets

10 Gap shrinkage and the corresponding loss of excitonic resonances entail important qualitative changes in the optical absorption spectrum. Their features are obviously dependent on the excitation intensity and thus these spectral modiﬁcations represent a typical example of nonlinear optical phenomena.

Fig. 8.17 The renormalized bandgap E g as a function of the e–h pair density N . The exciton binding energy of the n = 1 state is denoted E X . The transition from the dielectric free exciton gas to ionized plasma EHP, proceeds smoothly. The EHP luminescence spectrum is depicted on the right; μ stands for the plasma chemical potential, NM is the Mott density.

232

Highly excited semiconductors λ s ∼N −1/2 , NM ≈

kB T kB T ε0 ε = . 3 E 2 e2 aX 8 π aX X

(8.32)

The Debye–H¨uckel model happens to be a viable approximation in semiconductors with large aX , except at low temperatures. The temperature T in (8.32) may designate the effective temperature.

8.5.2 Luminescence of EHP

Fig. 8.18 (a). Onset of the EHP emission band in highly excited GaN at T = 6 K upon reaching the Mott density (NM ≈ 1019 cm−3 ). Triangles label the positions of the reduced bandgap Eg at the indicated densities of e–h pairs. Panel (b) displays the overall shape of the emission spectrum. Apart from the EHP band, also the M-line due to biexciton luminescence and the P-line due to exciton collisions are present. The free exciton spectral position is given by the reﬂection spectrum R/R. After Nagai et al. [23].

Electrons and holes in an EHP can recombine radiatively, of course. We are interested in what the EHP luminescence emission spectrum looks like. To begin, however, we have to answer an important question: What is the difference between an electron–hole plasma, EHP, and an electron–hole liquid, EHL, the existence of the latter having been—for the sake of simplicity—disregarded at the beginning of this section? EHL and EHP are two similar phases of the e–h system. However, while the condensation exciton gas → EHL starts abruptly and the liquid is concentrated into spatially clearly separated regions—spherical drops with a constant e–h pair density n 0 , the transition exciton gas → EHP proceeds smoothly, continuously. Also, the plasma gradually ﬁlls the whole excited volume (there are no drops) and may diffuse both laterally and into the depth of the sample, due to the concentration gradient. The e–h pair density therefore is not, unlike EHL, spatially constant and, moreover, rises with increasing excitation intensity. And perhaps the most important: the EHP may exist—unlike EHL—at arbitrary temperatures, neither is there an EHP critical temperature nor binding energy. The EHP is therefore a ‘less ordered’ relative of EHL. There is no radiative recombination enhancement factor in EHP, unlike EHL. It is worth stressing, however, that the concept of the renormalized gap, as introduced in Subsection 8.4.1, holds equally for both EHP and EHL! If condensation into an EHL happens, the e–h system simply ‘jumps’ somewhere to the right in Fig. 8.17, far beyond the NM density, and remains there. Equally, we can imagine that Fig. 8.11 is valid for both EHL and EHP, but while E g (n 0 ) is constant inside EHL drops, E g (N ) in EHP varies as a function of N (see Fig. 8.17). The scenario under growing optical excitation intensity, e.g., in silicon at T = 15 K, can then be described as follows (see the horizontal arrow in Fig. 8.9): First, a gas of excitons with increasing density n X is created, but before the Mott transition sets in, n X reaches a critical value for exciton condensation into EHL drops with a very high equlibrilum e–h pair density N = n 0 ≈ 3 × 1018 cm−3 . The density of the surrounding gas, n X , henceforth remains constant11 (∼ 1016 cm−3 ) and the gradual Mott transition will not occur. Generally it turns out that in indirect-bandgap materials, EHP and its luminescence reveal themselves only at temperatures T = Tc or higher. To differentiate the contributions to the emission spectrum from EHL, EHP and possibly from other luminescence channels (biexcitons, etc.) under these 11 The average density of the e–h system (all phases) will rise with the continuing growth of the excitation level, though, due to the growth the total volume of the EHL drops.

Electron–hole plasma (EHP)

233

conditions is not easy. Some authors even take the view that EHP can also undergo its own condensation process, characterized by a second critical point in the phase diagram. Currently, there is no consensus on this issue and further discussion goes beyond the scope of this book. In this respect, the situation is much simpler in direct-bandgap semiconductors, where EHL does not occur. The onset of EHP luminescence under sufﬁciently strong excitation is straightforward there, and according to the foregoing discussion this light emission has very speciﬁc spectral features: 1. A wide emission band (much like an EHL—radiative recombination in an ensemble of fermions), gradually emerging in the spectrum when the density of e–h pairs, N , approaches NM . 2. The low-energy emission band boundary (determined by E g (N )) undergoes a red shift with increasing excitation intensity; for an EHL, this boundary does not shift. 3. With increasing excitation intensity the EHP emission band gets broader, because the plasma density increases; the EHL bandwidth remains ﬁxed. Examples are shown in Figs 8.18 (GaN [23]) and 8.19 (TlBr [24]). The gradual increase of the EHP band around N = NM —the salient feature (1)— can be nicely seen in Fig. 8.18, while Fig. 8.19 demonstrates features (2) and (3).12 Open circles in Fig. 8.19 represent a theoretical ﬁt from which the displayed EHP densities were derived. It is important to stress that, although in TlBr the direct bandgap is concerned here, expression (8.25) together with the procedure described in Subsection 8.4.1 were applied for ﬁtting. This is surprising because the convolution (8.25) was derived for an indirect bandgap. Here, strictly speaking, its application is not justiﬁed. Nevertheless, this phenomenological approach is currently being used because it is simple and provides us with both a reasonable reproduction of the emission bandshape and a realistic effective temperature and density of EHP. (This was one of the reasons to depict transitions in Fig. 8.11 as direct ones.) More elaborate routines for spectral modelling that comprise k-conservation have been proposed, of course, but they are rather sophisticated and the resulting spectral shape is almost the same, except for more accurate determination of E g [25]. Let us recall once more that the densities obtained through ﬁtting are average EHP densities, unless we create in some way a spatially uniform plasma which, in fact, is highly desirable for the comparison of theory with experiment. To this end for example, two-photon excitation discussed in Section 5.5 can be used, as well as various spatial localizations of EHP in low-dimensional structures. Finally, let us note that radiative recombination of EHP in direct semiconductors may easily lead to stimulated emission (Chapter 10), which is of basic importance for light-emitting diodes and semiconductor lasers.

12 Let the reader compare Fig. 8.19 with Fig. 8.14, where the I (EHL) spectral position TO remains ﬁxed in spite of the variation in excitation power density by two orders of magnitude.

Fig. 8.19 EHP emission spectra in a highly excited TlBr crystal (a pulsed N2 -laser, 2 ns, 3.4 eV) at a bath temperature of 8.5 K. The excitation intensity I0 corresponds to ∼ 0.6 MW/cm2 . In TlBr, radiative recombination can occur both in indirect as well as in direct bandgaps; the displayed spectra originate in the direct are one, whose reduced values E gd labelled by arrows. After Kohlov´a et al. [24]. (Fig. 2.38(b) represents the EHP emission spectrum of TlBr at T = 25 K both in direct—A-line—and indirect—B-line—bandgaps. Arrows at ∼ 3.02 eV and ∼ 2.66 eV denote the spectral positions of relevant non-renormalized gaps corresponding to the one-electron approximation. The respective plasma densities and effective temperatures are also shown.)

234

Highly excited semiconductors

8.6 Bose–Einstein condensation of excitons An exciton as a quasi-particle consisting of two fermions (an electron and a hole) always has an integer total spin S = 0 or 1. An exciton is thus a boson and these can undergo, at high densities, so-called Bose–Einstein condensation. It is worth stressing that Bose–Einstein condensation represents a fundamentally different process with regard to exciton condensation into an EHL discussed above. In order to understand the fundamentals of Bose–Einstein condensation and to discover how this kind of exciton condensation can manifest itself in luminescence, we ﬁrst recall the basic properties of Bose–Einstein statistics.

8.6.1 Properties of the Bose–Einstein distribution The distribution or occupation function of ideal (non-interacting) bosons, determining the mean boson’ number in a state with energy E, reads

f BE (E, T ) = exp

1 E−μ kB T

−1

,

(8.33)

where μ is the chemical potential. This function is called the Bose–Einstein distribution. Unlike the Fermi–Dirac distribution, where μ is more often known as the Fermi energy and has quite an illustrative meaning of an energy level with the occupation probability equal to 1/2, the chemical potential μ in (8.33) is less familiar. Its properties are: 1. μ < 0 must be satisﬁed, otherwise the distribution function (8.33) in the ground state (E = 0) would acquire a negative value, which is not admissible. 2. |μ| is large at low boson densities, while with increasing density |μ| decreases and gradually approaches zero. This also follows directly from (8.33); a large value of |μ| implies a low mean number of bosons in a given state. Let us now ask a question: Can the boson’ number in the investigated system reach an arbitrary value? The total boson’ number (per unit volume) ntot can be found by summing over all occupied states and all possible energies: ∞ n tot =

ρ(E) f BE (E) dE.

(8.34)

0

For bosons with a mass m and total spin S = 0 we shall consider the density of states of the form13 ρ(E) = (2m)3/2 E 1/2 /4π2 h 3 . The maximum available number of bosons, n CB , can be obtained if we introduce into (8.34) a maximum value of f BE , which, according to the foregoing discussion, occurs in the limiting case μ → 0. By performing the relevant calculation (Appendix E) we get 13 The difference 1/2 compared to (5.4) is due to the difference in the spin degeneracy factor g between fermions (g = 2) and bosons with spin S = 0(g = 1).

Bose–Einstein condensation of excitons 2.31 (2m)3/2 (kB T )3/2 4 π2 h¯ 3 3/2 m kB T 3/2 ∼ m 15 ∼ T 3/2 (cm−3 ), (8.35) 6.4 × 10 = 2.61 = 2 m0 2 π h¯ where m 0 stands for the free electron mass. Obviously, this is a ﬁnite number, thus a very important message from (8.35) is: an ensemble of bosons may always contain only a ﬁnite number of particles (dependent on temperature). What happens now if we continuously add further particles into the ensemble? (In particular, if we keep creating a higher and higher exciton density through increasing the optical excitation?) Einstein, shortly after the formulation of quantum statistics by the Indian physicist Bose, deduced: the excess particles must ‘condense’ to the ground state E = 0, which, in this way, somehow separates from other states. Relation (8.35) thus deﬁnes a critical concentration n CB for the onset of this so-called Bose–Einstein condensation,14 which occurs primarily in energy or momentum space (k-space), not in real space—unlike exciton condensation to an EHL. Before we discuss manifestation of luminescence the of this peculiar condensation, we shall derive one simple mathematical consequence of (8.35). Upon reaching n CB we can obviously express the boson density as n CB (T ) =

n tot = n 0 + n CB (T ). The ground state population n 0 will thus grow with a further increase of pumping, while n CB at a given T remains constant. This relation can be rewritten as n CB 6.4 × 1015 (m/m 0 )3/2 T 3/2 n0 =1− =1− , n tot n tot n tot from which the critical temperature T CB for the Bose–Einstein condensation can be deﬁned via 1 3/2

TCB

=

6.4 × 1015 (m/m 0 )3/2 . n tot

The announced mathematical follow-up of (8.35) then reads n0 T 3/2 =1− . n tot TCB

(8.36)

(8.37)

From (8.37) we can easily infer the meaning of the critical temperature: For T > TCB . . . . . . . . . . . . . . . . . . (8.37) has no physical meaning, T = TCB . . . . . . . . . . . . . . . . .n 0 = 0 and the condensation just begins, 14 At the same time a condition must be satisﬁed, namely, that the energy and the number of bosons can vary independently. This is possible, e.g., for atoms, excitons and biexcitons but not for photons and phonons; their chemical potential equals zero but, despite this fact, one cannot speak of a Bose–Einstein condensation. An equivalent statement reads that bosons undergoing Bose–Einstein condensation must have non-zero rest mass (see (8.35)), which holds neither for photons nor phonons.

235

236

Highly excited semiconductors T < TCB . . . . . . . . . . . . . . . . .n 0 according (8.37) sharply increases, T = 0 K . . . . . . . . . . . . . . . . .n tot = n 0 . On the basis of (8.36) and (8.37) we can quite clearly imagine what the Bose– Einstein condensation of excitons looks like in an experiment. Let us apply, e.g., a ﬁxed excitation intensity, i.e. a ﬁxed exciton density n X = n tot , and let us start the experiment at a relatively high temperature when, according to (8.35), n X < n CB (T ). Therefore there is no condensation. In the course of cooling we reduce n CB (T ) till we drop to the critical temperature TCB when n X = n CB . The condensation sets in and if we keep cooling, the concentration of ‘condensed’ excitons rises according to (8.37) up to the limit value n 0 = n X at T = 0 K. Then, all of the photogenerated excitons occur in the condensate with energy E = 0.

8.6.2 Luminescence experiment: Bose–Einstein condensation yes or no? The Bose–Einstein condensation represents the macroscopic population of a single state E = 0 or k = 0. It is one of the fundamental consequences of quantum mechanics that leads—among others—to important, application-related effects like superﬂuidity of liquid He and superconductivity. The development of efﬁcient laser and magnetic cooling of atoms has recently led to a fruitful investigation of experimental features of this condensation in an atomic gas, but at extremely low temperatures below 100 nK. Semiconductor luminescence proposes unique conditions for a detailed study of Bose–Einstein condensation. If we adjust (8.36) to express explicitly the critical temperatures

m 0 2/3 (8.38) n tot (K), TCB ∼ = 2.9 × 10−11 m it is observed that the critical temperature for an atomic gas (m m 0 ) is by many orders lower compared with a gas of excitons (m ≈ m 0 ) of the same density. Considering this density to be n tot = 1017 cm−3 (easily attainable under optical pumping), we obtain from (8.38) for m = m 0 a critical temperature TCB ≈ 6.3 K. This is a ‘reasonable’ temperature that can be achieved in a current helium cryostat. Pumping of 4 He vapour enables going down to T ≈ 1.3 K commonly. There are additional advantages: the exciton density and thus, according to (8.38), also TCB can be varied readily via the variation of excitation intensity, or vice versa, at a given excitation power density we can ﬁnely tune the sample temperature in the environs of TCB . And, most importantly, the exciton condensate reveals itself through a dramatic modiﬁcation of the semiconductor emission spectrum. For all of these reasons the search for the Bose–Einstein condensation of excitons using luminescence methods has represented a worldwide challenge for more than 30 years. How the condensation should manifest itself in the emission spectrum can be predicted ﬁrst with the aid of simple reasoning. Since it arises from the accumulation of excitons in the E = 0 state, which corresponds to the bottom of the exciton band, we expect the recombining ‘condensed’ excitons to emit

Bose–Einstein condensation of excitons

237

Fig. 8.20 (a) Low-temperature free exciton photoluminescence in AgBr accompanied with the emission of a TO(L)-phonon (i.e. ITO (FE) line), in two samples #451 and #421. Open circles denote the theoretical lineshape ﬁt based on (7.16). The very narrow peak labelled FE0 has been identiﬁed as being due to the Bose–Einstein condensation of the free exciton gas. Panel (b) shows a sudden intensity increase of this peak in the course of cooling below 3 K. After Czaja and Schwerdtfeger [26]. Later experiments revealed that this interpretation was probably incorrect, though.

a very narrow peak on the low-energy edge of the free exciton line (hν = E gi –E X –h¯ ω in an indirect-bandgap semiconductor). This peak should appear in the spectrum suddenly in the course of cooling, upon reaching TCB . Exactly this kind of behaviour can be recognized in the spectra shown in Fig. 8.20(a), which come from two nominally pure AgBr crystals at T = 2.08 K and T = 1.49 K. The lower panel (b) shows that the intensity behaviour of the sharp FE0 peak at ∼ 2.6754 eV complies perfectly with (8.37), provided we put TCB = 3 K. This represents one of the ﬁrst luminescence observations interpreted in terms of the excitonic Bose–Einstein condensation [26]. Everything looks very convincing. However, a series of subsequent papers revealed this interpretation to be untenable, by ﬁnding the origin of the FE0 peak in an exciton bound to a residual shallow impurity (Subsection 7.2.1). This indicates that the experimental realization of the Bose–Einstein exciton condensation is not a simple task and that such a straightforward way as the one shown in Fig. 8.20 is hardly viable. A ‘jump’ from the Maxwell–Boltzmann distribution (circles on the experimental curves in Fig. 8.20(a)) immediately to the spectrally narrow condensate is unrealistic. The Maxwell–Boltzmann distribution is a classical limit, shared both by bosons and fermions. With

238

Highly excited semiconductors

Fig. 8.21 (a) Product √ of the density of states ρ (E) ≈ E with the Bose–Einstein distribution function (8.33) where α = –μ/kB T . The lower curve (MB) is the Maxwell–Boltzmann approximation valid for low exciton densities (α > 4). In the limit α → 0 a narrow peak remains only at Œ = 0. The curves are normalized at high values of Œ. (b) Narrowing down of the exciton emission line (a phonon replica) in Cu2 O at high exciton density. The sample was immersed in liquid He (T = 2K) and excited by 10 ns pulses of an Ar+ -laser with excitation intensity of ∼ 40 MW/cm2 . The dashed curve (Maxwell–Boltzmann distribution) is considerably wider. After Snoke et al. [27].

increasing density n X (therefore with decreasing |μ|) the excitons should at ﬁrst prove that they start to behave as genuine bosons. Consequently, the exciton statistics and also the emission lineshape should gradually transform to true Bose statistics. In this case, the lineshape width would undergo dramatic but gradual narrowing, which can be easily shown by calculating ρ(E) f BE (E) and which is displayed in Fig. 8.21(a). This is the so-called Bose narrowing. The reader is reminded that the FWHM of the Maxwell–Boltzmann distribution (7.16) is invariable, equal to about 1.8 kB T . This Bose narrowing has indeed been found in exciton luminescence of Cu2 O [27], as demonstrated in Fig. 8.21(b). Nevertheless, till now, no unambiguous experimental evidence of Bose–Einstein condensation has been achieved either in this material or in bulk semiconductors in general (at least unconditional evidence that would be accepted without taking exceptions to). Taking into consideration everything discussed above in this chapter, we understand why this is so. First of all, excitons have a ﬁnite lifetime. The ideal Bose– Einstein distribution (8.33) holds exactly for excitons as non-interacting quasiparticles with inﬁnite lifetime in thermodynamic equilibrium only. Moreover, with increasing exciton density the important exciton–exciton interactions occur in most semiconductors (biexcitons, EHL, EHP). For instance, prior to reaching the critical concentration n CB , the Coulomb e–h attraction may happen to be screened and the exciton gas transformed into EHP or EHL. (This is one of the reasons why especially Cu2 O appears to be a good candidate

Problems for the exciton Bose–Einstein condensation—owing to speciﬁc features of the Cu2 O band structure the interaction between excitons is repulsive, thus biexcitons do not originate here. Moreover, because the Bohr radius aX is very small, see Table. 7.1, EHP does not occur in this material at high excitation.) Another complication preventing excitons from Bose–Einstein condensation may be insufﬁcient sample purity, as we have seen in the case of AgBr (Fig. 8.20)—the presence of bound excitons reduces n X and, in the spectrum, may either mask a possible emission line arising from the Bose–Einstein condensate or cause an incorrect interpretation of the experimental observations. Finally, high optical excitation levels can both evoke spatial exciton diffusion and entail a high effective temperature of the exciton gas that hinders reaching TCB . A more detailed discussion goes beyond scope of this book. It is worth mentioning though, that also biexcitons are bosons and one can expect their Bose–Einstein condensation together with its speciﬁc luminescence manifestation. The most investigated material in this regard is copper chloride, CuCl. The whole topic is covered by a special monograph [28]. It is worth noting that, strictly speaking, the above discussed ‘classical’ Bose–Einstein condensation may exist in inﬁnite bulk materials only. In lowdimensional systems, a generalized deﬁnition of Bose–Einstein should be applied. In particular in two-dimensional structures the concept of condensation is linked to the phase-coherent superﬂuid movement of a bosonic system rather than to boson accumulation in the lowest energy level [29]. Recent results concerning Bose–Einstein condensation of exciton–polaritons in semiconductor low-dimensional microcavities will be brieﬂy mentioned in Chapter 16.

8.7 Problems 8/1: Based on Fig. 8.1: (a) Estimate the binding energy E B of an excitonic molecule in CdS. (b) Check that the spectral position of the P-band, which is due to inelastic exciton–exciton scattering, is in accord with the binding energy E X in Table 7.1. 8/2: Luminescence of excitonic molecules in indirect-bandgap semiconductors, discussed in Subsection 8.2.1, has been described in the framework of allowed dipole transitions. Nakahara and Kobayashi [30] have generalized this approach for the case of indirect forbidden transitions, when the relevant transition matrix element is composed of two terms, the ﬁrst of which is proportional to the magnitude of the biexciton wavevector Q and the second one to the magnitude of the wavevector q of the remaining exciton. Making use of the formalism applied in Appendix C, adjust the expression describing the emission lineshape to a form suitable for numerical integration (analogy with (C-15)) and show that the contribution of the second term is negligible. 8/3: Prove, using the E(K) diagram (in analogy with Fig. 8.7), that in common semiconductors with indirect bandgap the luminescence channel due to inelastic free exciton collisions (P-line) cannot occur. Hint: consider that the indirect bandgap in common semiconductors is always deﬁned by an

239

240

Highly excited semiconductors extreme of the conduction or valence band situated at the boundary of the ﬁrst Brillouin zone. 8/4: Show that the average kinetic energy (per electron) in a Fermi gas at T = 0 K is equal to (3/5)Fe (Fe = Fermi energy of electrons). 8/5: An electron–hole liquid (EHL) in the form of electron–hole drops (EHDs) represents an open system exchanging quasi-particles, i.e. the electron– hole pairs, with its surroundings. Open systems in thermodynamics are characterized, among others, by their chemical potential μ. Show that here μ is characteristic of the EHL ground state. Hint: start from the deﬁnition of the chemical potential as the energy required for passing from the ground state with N electron–hole pairs in a drop to the ground state with (N + 1) pairs in the drop. See also [31]. 8/6: By using the relationship (8.32) and exploiting the parameters from Table. 7.1, calculate the Mott density NM in selected semiconductors for kB T /E X = 0.1. Compare the obtained results with a rough estimate 3 /3)−1 . Discuss the derived on the basis of the criterion NM ∼ = (4 π aX illustrative meaning of this criterion.

References 1. Shionoya, S., Saito, H., Hanamura, E., and Akimoto, O. (1973), Solid State Comm., 12, 223. 2. Klingshirn, C. and Haug, H. (1981). Phys. Rep., 70, 315. 3. Hanamura, E., and Haug, H. (1977). Phys. Rep., C, 33, 209. 4. Quattropani, A. and Forney, J. J. (1977). Nuovo Cimento B, 39, 569. 5. Grun, J. B., L´evy, R., Ostertag, E., Vu Duy Phach, H., and Port, H. (1976). Biexciton luminescence in CuCl and CuBr. In: Physics of Highly Excited States in Solids (ed. M. Ueta and Y. Nishina), Lecture Notes in Physics Vol. 57, p. 49. Springer, Berlin. 6. Baba, T. and Masumi, T. (1977). Nuovo Cimento B, 39, 609. 7. Cho, K. (1973). Optics Comm., 8, 412. 8. Knox, R. S., Nikitine, S., and Mysyrowicz, A. (1969). Optics Comm., 1, 19. 9. Pelant, I., H´ala, J., Parma, L., and Vacek, K. (1980). Solid State Comm., 36, 729. 10. Gourley, P. L. and Wolfe, J. P. (1979). Phys. Rev. B, 20, 3319. 11. Hvam, J. M. (1973). Solid State Comm., 12, 95. 12. Moriya, M. and Kushida, T. (1976). J. Phys. Soc. Japan, 40, 1668. 13. Shah, J., Combescot, M., and Dayem, A. H. (1977). Phys. Rev. Lett., 38, 1497. 14. Rice, T. M. (1977). The electron–hole liquid in semiconductors: theoretical aspects. In: The Electron–Hole Liquid in Semiconductors (ed. H. Ehrenreich, F. Seitz and D. Turnbull), Solid State Physics Vol. 32, p. 1. Academic Press, New York. 15. Vashista, P., Kalia, R. K., and Singwi, K. S. (1983). Electron–hole liquid: theory. In: Electron–Hole Droplets in Semiconductors (ed. C. D. Jeffries and L. V. Keldysh), Modern Problems in Condensed Matter Sciences Vol. 6, p. 1. North Holland, Amsterdam. 16. Benoit a` la Guillaume, C. and Voos, M. (1973). Phys. Rev. B, 7, 1723. 17. Hensel, J. C., Phillips, T. G., and Thomas, G. A. (1977). The electron–hole liquid in semiconductors: experimental aspects. In: The Electron–Hole Liquid in Semiconductors (ed. H. Ehrenreich, F. Seitz and D. Turnbull), Solid State Physics Vol. 32, p. 88. Academic Press, New York. 18. Westervelt, R. M. (1983). Kinetics of electron–hole drop formation and decay. In: Electron–Hole Droplets in Semiconductors (ed. C. D. Jeffries and L. V. Keldysh),

References

19. 20.

21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31.

Modern Problems in Condensed Matter Sciences Vol. 6, p. 187. North Holland, Amsterdam. Hulin, D., Mysyrowicz, A., Combescot, M., Pelant, I., and Benoit a` la Guillaume, C. (1977). Phys. Rev. Lett., 39, 1169. Kulakovskij, V. D. and Timofeev, V. B. (1983). Thermodynamics of electron-hole liquid in semiconductors. In: Electron–Hole Droplets in Semiconductors (ed. C. D. Jeffries and L. V. Keldysh), Modern Problems in Condensed Matter Sciences Vol. 6, p. 95. North Holland, Amsterdam. Steele, A. G., McMullan, W. G., and Thewalt, M. L. W. (1987). Phys. Rev. Lett., 59, 2899. Haug, H. (1988). Introduction. In: Optical Nonlinearities and Instabilities in Semiconductors (ed. H. Haug ), p. 1. Academic Press, New York. Nagai, T., Inagaki, T. J., and Kanemitsu, Y. (2004). Appl. Phys. Lett., 84, 1284. Kohlov´a, V., Pelant, I., H´ala, J., Ambroˇz, M., and Vacek, K. (1987). Solid State Comm., 62, 105. Capizzi, M., Modesti, S., Frova, A., Staehli, J. L., Guzzi, M., and Logan, R. A. (1984). Phys. Rev. B, 29, 2028. Czaja, W. and Schwerdtfeger, C. F. (1974). Solid State Comm., 15, 87. Snoke, D. W., Wolfe, J. P., and Mysyrowicz, A. (1990). Phys. Rev. B, 41, 11171. Moskalenko, S. A. and Snoke, D. W. (2000). Bose–Einstein Condensation of Excitons and Biexcitons. Cambridge University Press, Cambridge. Kavokin, A. V., Baumberg, J. J., Malpuech, G., and Laussy F. P. (2007). Microcavities. Oxford University Press, Oxford. Nakahara, J. and Kobayashi, K. (1976). J. Phys. Soc. Japan, 40, 189. Combescot, M. and Nozi´eres, P. (1972). J. Phys. C, 5, 2369.

241

Luminescence of disordered semiconductors

9 9.1 Densities of states in bands

242

9.2 Temperature dependence of luminescence 244 9.3 Distribution of luminescence lifetimes 248 9.4 Spectral shape of the emission band

250

9.5 Some other properties of luminescence of disordered semiconductors

255

9.6 Problems

261

Disordered (amorphous) semiconductors are characterized by the absence of an ordered atomic arrangement over long distances from a chosen atom (‘longrange order’). One is thus not allowed to employ the concepts familiar from the crystalline state such as the electron or hole wavevector k, the Bloch theorem or the energy band structure perceived as the energy dependence of the charge carrier on the wavevector k, i.e. E = E(k). However, because the short range order (i.e. basically the periodic arrangement in the close surroundings of the given site) is kept, also the concepts of the conduction and valence bands, the forbidden gap and the density of states are basically conserved. These again are of decisive importance for understanding the luminescence processes, but the microscopic luminescence features in disordered solids differ quite considerably from the mechanisms that operate in their crystalline counterparts and that were discussed in Chapters 5, 7 and 8.

9.1 Densities of states in bands The commonly accepted scheme of the electron and hole energy distribution in disordered semiconductors is depicted in Fig. 9.1(a): The electrons with energy higher than the so-called mobility edge E cm are considered free and may take part in the charge transport; their movement is characterized by the so-called microscopic mobility μm . The electrons having energy E < E cm are not free; they are spatially localized in traps whose microscopic origin consists in deﬂections of the bond lengths and angles from their ﬁxed values in a regular crystalline lattice. Upon applying an electric ﬁeld these carriers can participate in the charge transport only via the so-called hopping mechanism, when the electrons tunnel between nearby potential wells that act as charge traps, or by means of so-called multiple trapping. In that case the localized electrons are thermally excited above the mobility edge E cm , migrate with the mobility μm , fall down into a distant trap, are thermally re-excited, etc. A mirror-like picture may be applied to the holes with relevant mobility edge E vm . The difference E cm –E vm roughly corresponds to the energy bandgap in crystalline semiconductors. The density of states of the electrons with energy E > E cm is described by a square-root function ρ(E) (E − E cm )1/2 , anal-

Densities of states in bands ogously to crystals. In an ideal crystalline semiconductor, however, the density of states within the bandgap is zero, while in disordered materials it remains non-zero even for E < E cm . It has been established that the density of these states (originating, as already mentioned, owing to variations of the bonding parameters between atoms), g(E), drops exponentially downwards from the mobility edge [1] gc (E) = gc0 exp(−E/E c0 ).

(9.1)

In this expression the energy E is referred to Ecm and considered positive downwards, see Fig. 9.1. A similar convention for the holes yields gv (E) = gv0 exp(−E/E v0 ).

(9.2)

The quantities E c0 , E v0 stand for the energy widths of the tail states (i.e. the states extending into the ‘energy gap’) of the conduction and valence bands, respectively. They amount typically to tens of meV. Nonequilibrium electron– hole pairs, created with the generation rate G, rapidly thermalize (within 10−13 –10−12 s) towards the corresponding mobility edges, then deeper into the tail states and eventually—on a much longer timescale—they may recombine radiatively via tunnelling between nearby sites with a recombination rate 1/τr (Fig. 9.1(b)). This is generally believed to be the main radiative recombination channel in disordered semiconductors. Within the bandgap of disordered semiconductors one can ﬁnd other electron states. The deformed covalent bonds between neighbouring atoms are exposed to mechanical strain and may break. This rupture gives rise to so-called dangling or unsaturated bonds. They are very often passivated by hydrogen atoms (especially in hydrogenated amorphous silicon, a-Si:H), but some remain unpassivated, may capture an electron and thereby introduce deep localized electron states approximately in the middle of the bandgap. Important, from the luminescence standpoint, is that these deep defect levels act as efﬁcient centres of non-radiative recombination (Fig. 9.1(b)), which is, after all, a general property of all deep defect states (see Chapter 6). It should be noted also that the total density of the dangling bonds is not constant in time. It grows upon irradiating the sample with photons hν ≥ E cm − E vm that create free electron–hole pairs. Subsequent non-radiative recombination of these e–h pairs may release energy sufﬁcient to break the weakened bonds, as explained already in Section 6.2. The process has been known for a long time as the Staebler–Wronski effect [2] but its microscopic mechanism has not been understood in all details till now. Recent results indicate that it is basically due to bimolecular non-radiative recombination [3]. The dangling bonds can be either empty (i.e. positively charged, D+ , because the negative electron charge is missing there), or occupied with one electron (D0 ), or with two electrons of opposite spins (negatively charged dangling bond, D− ). The energy required to add the second electron to an already occupied dangling bond is called the correlation energy U , see Fig. 9.1(a).

243

244

Luminescence of disordered semiconductors

Fig. 9.1 (a) Schematic of the electron density of states in disordered semiconductors. Luminescence properties are mainly driven by occupation of the localized, so-called tail states gc (E), gv (E) that drop exponentially down from the relevant mobility edges into the ‘forbidden’ gap. The electrons above the mobility edge E cm occupy free states, whose density is described approximately by a square-root shape (like the holes below the E vm edge). Approximately in the middle of the bandgap there are levels D+ , D0 , D− arising from the dangling bonds. These levels represent efﬁcient non-radiative centres. (b) Schematic of thermalization and recombination of non-equilibrium electrons and holes in amorphous semiconductors. The radiative recombination of an e–h pair localized in the tail states (1/τr ) competes with non-radiative tunnelling to a deep defect (2) level (1/τnr ) or with non-radiative recombination due to thermal carrier excitation and subsequent diffusion towards the non-radiative centres (1) (1/τnr ).

The last types of energy levels in disordered semiconductors are possible impurity levels in doped materials. These are located, similarly to crystalline counterparts, within the bandgap close below the relevant mobility edges (donors and acceptors in Fig. 9.1(a)).

9.2 Temperature dependence of luminescence We have seen that the disorder does not introduce any new kinds of recombination processes fundamentally different from crystalline solids. However, the radiative recombination in the tail states exhibits a typical experimental dependence whose provenance can be simply derived. We start with the expression for luminescence quantum efﬁciency (3-2) by rewriting it as a relation suitable for the luminescence intensity as a function of temperature I (T ): I (T ) = I0

pr (T ) 1/τr . = I0 pr (T ) + pnr (T ) (1/τr + 1/τnr )

(9.3)

Here pr and pnr stand for the probability of radiative and non-radiative recombination, respectively, and τr and τnr denote the corresponding recombination times. I0 is a constant quantity whose meaning will be discussed below.

Temperature dependence of luminescence Expression (9.3) simply connects the luminescence intensity with its quantum efﬁciency η, namely, I (T ) = I0 η(T ). At a ﬁxed temperature, the electron (or hole) in the tail state with energy E can, according to Fig. 9.1(b), either recombine radiatively (1/τr ) or be excited thermally above the mobility edge and subsequently diffuse towards a non(1) radiative centre (1/τnr ≡ 1/τnr ).1 Thermal excitation causing luminescence quenching is described by the known relation (4.17) that now reads 1/τnr = p0 exp (−E/kB T ) ,

(9.4)

1012 s−1

is the so-called frequency factor. The electrons and holes where p0 ≈ in shallow states (E small) thus recombine mainly non-radiatively, while the photocarriers deep below the relevant mobility edge have no chance to ‘escape non-radiatively’ and rather they give rise to recombination luminescence radiation. It is thus possible to deﬁne a temperature dependent demarcation energy E D (T ); carriers at this energy have the rate of radiative recombination just equal to the rate of non-radiative recombination given by (9.4): 1/τr = p0 exp (−E D (T )/kB T ) .

(9.5)

The signiﬁcance of the demarcation energy therefore consists in separating light-emitting states from non-radiative (‘dark’) states. Now we can express the quantum efﬁciency through the tail state densities as ∞ gv (E)dE pr (T ) ED = e−E D (T )/Ev0 . = ∞ η= (9.6) pr (T ) + pnr (T ) gv (E)dE 0

∞ The integrals in (9.6) mean summing over all the tail states ( dE) and over the states below the demarcation energy (

∞

0

dE). Note that we sum over the

ED

valence band states (9.2) only. This is justiﬁed by different widths of the tail states: The valence band tail states are usually wider than the conduction band ones (E v0 > E c0 ). Consequently, even if both kinds of photocarriers located above the relevant demarcation energy may be thermally released, decisive for the efﬁciency of the non-radiative process is the release of deeper lying holes— the electrons liberated easily from their shallower states cannot recombine unless free holes, upon migrating through the sample, occupy the deep centres of non-radiative recombination. Supposing further that η is very small compared with unity (i.e. pnr (T ) pr (T ), or η = pr /( pr + pnr ) ≈ pr / pnr ), expression (9.3) becomes pr + pnr I0 pnr ∼ 1 I0 = =1+ = =1+ I (T ) I0 pr /( pr + pnr ) pr pr η 1 For the sake of simplicity we neglect here the (temperature independent) channel of direct (2) non-radiative recombination 1/τnr .

245

246

Luminescence of disordered semiconductors or

I0 ∼ 1, −1 = I (T ) η

which, with the aid of (9.6), yields the required expression for the characteristic temperature dependence of luminescence E D (T ) I0 T −1 = ln ≡ . (9.7) I (T ) E v0 T0 In (9.7) we have introduced, to a certain extent formally, the characteristic temperature T0 via E v0 = kB T0 ln ( p0 τr ) .

(9.8)

Such a deﬁnition of T0 can be justiﬁed by a formal similarity of E v0 and E D (T ), provided we express the latter quantity from eqn (9.5). The parameter T0 characterizes the width of the tail states. Therefore, plotting the experimentally acquired values of ln(I0 /I (T )–1) against T should yield—provided the above model is correct—a straight line with slope 1/T0 . The curves in Fig. 9.2(a), measured in various samples of hydrogenated amorphous silicon, nicely demonstrate that this is the case [4]. The reciprocal slope value T0 , extracted from this ﬁgure, amounts to T0 = 22–23 K. The parameter T0 is very sensitive to the degree of disorder: In amorphous alloys, where, besides the topological disorder, also composition disorder occurs (e.g. in a-Si:H with high hydrogen content ≥ 10 at. %) the tail states are much wider. Figure 9.2(b) shows the dependence (9.7) for a-Si:H with 19 at. % of hydrogen [5]. The slope of the linear plot yields T0 = 62 K. This means that, among others, the photocarriers after thermalization get localized in deep states and thus the thermal luminescence quenching is less effective. This corroborates Fig. 9.2(b)—it becomes evident that I (T ) = 0 even at room temperature while in ‘standard’ a-Si:H with hydrogen content of about 5–10 at.% only, photoluminescence at T = 295 K in fact does not occur. The presence of room-temperature luminescence in amorphous alloys is supported probably also by a low carrier mobility, which makes the ‘search’ of released carriers for non-radiative centres more difﬁcult. Till now, we have not speciﬁed how to assess the constant I0 and what is its meaning. This can be easily anticipated—since monotonic thermal luminescence quenching is involved with increasing temperature, as indicated, e.g. by the growth of the demarcation energy with temperature (9.5), I0 should mean the luminescence intensity at the lowest temperature of measurement. (After all, it can be deduced from (9.7) that I0 /I (T ) > 1 must always hold, for formal reasons.) Despite this, the assessment of I0 may be ambiguous in some cases, because in disordered semiconductors the form of I (T ) at the lowest temperatures (about 4–70 K) is not always simple: Sometimes in this temperature range a ‘plateau’ is found; another time even a moderate increase of I (T ) with increasing temperature is observed. The question then arises which value of I (T ) to select as I0 . This selection may inﬂuence the left part of the curve [I0 /I (T )–1], as becomes evident in Fig. 9.2(b) for the

Temperature dependence of luminescence

247

Fig. 9.2 (a) Plot of [I0 /I (T )–1] against T in samples of a-Si:H prepared in various ways. After Collins et al. [4]. (b) The same plot () obtained in an a-Si:H alloy with high hydrogen content. Also the direct dependence of I (T ) on temperature is shown (). After Luterov´a et al. [5]. The symbols denote experimental data, and the lines are ﬁts according to (9.7).

data at T ≤ 125 K. For a more detailed discussion, the reader is referred to the literature [4]. Of course, I0 is only a certain experimental parameter, not (unlike the ﬁt parameter T0 ) a characteristic material constant. The model under discussion leads to the following consequence: The demarcation energy E D (T ) increases with increasing temperature. Therefore, the luminescence emission spectrum as a whole (or its maximum) must shift to the red and, what is of the essence, this shift must exceed the temperature redshift of the bandgap. Figure 9.3 shows that this is the case [6]. Let us now attempt to summarize all assumptions applied in deriving the temperature behaviour (9.7) and to determine the limits of its validity. First, as we have just stated, this model can be applied only in a temperature range where the luminescence intensity drops with increasing T . Besides, we have (2) neglected the channel of direct non-radiative tunnelling (1/τnr = 0). This, it is true, means implicitly that within the model the quantum efﬁciency η is equal to unity, provided the photocarriers thermalize into states lying below the demarcation energy. This may occur at sufﬁciently low temperatures when no carriers can be thermally excited to the free states, and thus all they can do

Fig. 9.3 Temperature shift of the emission band maximum in a-Si:H (with rate of 1.8 × 10−3 eV/K; different symbols denote different samples or different excitation modes) in comparison with the temperature shift of the absorption edge (4.3 × 10−4 eV/K). After Tsang and Street [6].

248

Luminescence of disordered semiconductors is to recombine radiatively. This fact, however, gets involved in a contradiction with the second assumption applied in deriving (9.7), namely, that η 1. Is the model thus inconsistent? It is better to say one should be cautious in making use of it. The mentioned (2) contradiction may be removed if we admit 1/τnr = 0. The overall character of I (T ) remains unchanged, but the left-hand side of the deﬁnition (9.5) of the demarcation energy will comprise the low-temperature luminescence decay (2) rate 1/τL0 = 1/τr + 1/τnr instead of the reciprocal radiative lifetime 1/τr . Similarly, τL0 will substitute for τr in expression (9.8) for E v0 . We have to keep this in mind when deriving E v0 from the experimentally determined T0 , and also in a possible reciprocal procedure: if, for instance, we assess E v0 via optical absorption or photoelectric measurements (in addition to evaluating T0 from luminescence experiments), we have to carefully analyse every time whether eqn (9.8) will yield τr or τL0 . This difference is not always sufﬁciently accentuated in the literature.

9.3 Distribution of luminescence lifetimes

Fig. 9.4 Illustrating the distribution of luminescence decay times. The conduction band tail states are depicted by short horizontal lines, those of the valence band by squares (the tail state widths are exaggerated for the sake of clarity). Oblique arrows represent radiative recombination via tunnelling, horizontal arrows denote the escape of carriers towards non-radiative centres and the wavy lines indicate carrier thermalization.

In the preceding section we implemented for disordered semiconductors a single luminescence decay time τL , in full analogy with their crystalline counterparts. This is, however, an oversimpliﬁcation that does not correspond to the facts. In disordered materials, generally speaking, a large range of luminescence decay times occurs, spanning from 10−9 s up to 10−1 s, in strong dependence upon temperature. The reason for this consists in the fact that the tail states, in which luminescence originates, are very broad and have a very variable spatial density. The non-equlibrium electrons sitting in energy states close to the mobility edge E cm can ﬁnd in their close neighbourhood many ‘deep’ hole states (in proximity to E vm ) for tunnelling radiatively. That is, near the mobility edges the densities of states (9.1) and (9.2) acquire their maximal values per unit volume. Because the probability of radiative tunnelling can be expressed as 1/τr ≈ exp (−2R/R0 ), where R is the localized electron– localized hole separation and R0 is a characteristic constant, this probability is large for small R. Therefore, high-energy luminescence photons hν1 , corresponding to a small distance R1 , will decay faster than photons hν2 < hν1 and hν3 < hν2 that belong to the tunnelling separations R2 > R1 and R3 > R2 (Fig. 9.4). Furthermore, energetically higher lying carriers ﬁnd more chance to thermalize (wavy lines) and also to escape non-radiatively into the free states (Fig. 9.4, left part). This, altogether, makes the high-photon-energy luminescence radiation decay faster that the low-energy radiation. Consequently, a continuous distribution of luminescence decay times g(τL ) must exist; taking into account its considerable width, it is usually plotted as a function of the logarithm of the decay time g(log τL ). The luminescence of every electron–hole pair localized in the tail states can certainly be regarded as a ‘monomolecular’ type of radiative recombination,

Distribution of luminescence lifetimes

249

i.e. according to (3.5) we shall consider the individual decay curves in the form i L (t) = i(0)e−t/τL =

N0 η −t/τL e , τL

(9.9)

where N0 denotes the number of excited centres (e–h pairs with the decay time τL ) and η stands for the luminescence efﬁciency. However, owing to the existence of g(log τL ), instead of (9.9) we now have to consider the sum over all possible τL : +∞ exp(−t/τL ) i L (t) = ηN0 d(log τL )g(log τL ) . τL

(9.10)

−∞

An example of an experimentally acquired distribution g(log τL ) is shown in Fig. 9.5 [7]. Now we analyse how to determine the distribution function g(log τL ) experimentally. One of the possible ways is as follows. We have mentioned in Section 3.4 that the luminescence decay curve in disordered systems can be in most cases described phenomenologically by the temporal stretched exponential function i L (t) = i(0) exp[− (t/τ )δ ],

(9.9a)

where τ is called the decay time and δ ∈ (0, 1 is the so-called dispersion factor. Now, let us recall the deﬁnition of the Laplace transform of a function f (x) ∞ F(t) =

f (x)e−t x dx ;

0

x is a real argument and F(t) is called image of the Laplace transform. Substituting x = 1/τ yields ∞ f (1/τ ) exp(−t/τ )

F(t) = 0

dτ τ2

and, if in (9.10) we write d (log τL ) ≈ dτL /τL and replace formally g(log τL ) → f (1/τL ), eqn (9.10) becomes ∞ i L (t) ≈

f (1/τL ) exp(−t/τL ) 0

dτL . τL2

(9.10a)

By comparing (9.9a) with (9.10a) it turns out that, under suitable normalization, one can write

δ

exp −(t/τ )

∞ f (1/τL ) exp(−t/τL )

= 0

dτL . τL2

(9.10b)

The last equation implies that, in order to reveal the distribution function f (1/τL ), ﬁrst of all we should determine τ , δ by virtue of ﬁtting the

Fig. 9.5 Temporal shape of the decay of the spectrally integrated photoluminescence of a-Si:H at a temperature T = 77 K (symbols) and the relevant decay time distribution g(log τL ) (full curve) deﬁned via (9.10). After Wang and Fritzsche [7].

250

Luminescence of disordered semiconductors experimental decay curve i L (t), and then we can calculate f (1/τL ) as the inverse Laplace transform of the stretched exponential function.2 This procedure is applied whenever the distribution functions g(τL ) or f (1/τL ) are relatively narrow. An example will be given in Chapter 15 (Fig. 15.1). When the distribution function is sufﬁciently broad (g(log τL )), it can be determined by making use of a much simpler way, namely, directly from the measured decay curve iL (t) as g(log τL ) i L (t)t (Problem 9/3). The preceding discussion on the continuous character of g(log τL ) has not been fully exhausting. Even if we study the ‘monochromatized’ luminescence of disordered semiconductors, i.e. if we measure the decay time on a single selected wavelength, we obtain curves g(log τL ) similar to those displayed in Fig. 9.5, see Fig. 9.6(a) [8]. Referring to what has been said above this could hardly be expected (!) How, then, is it possible? The answer is given in Fig. 9.4. The recombination of the e–h pairs (a) and (c) will be faster than that of the pair (b), because both the electron in case (a) and the hole in case (c) can be easily thermally excited into delocalized states and subsequently ﬁnd a counterpart to recombine non-radiatively. At the same time the photon energy hν may be in all three cases (a), (b) and (c) identical. Moreover, the random statistical distribution of the electron–hole separation R, occurring also for hν = const, will manifest itself. In materials where the tail state widths E v0 and E c0 are large enough, the luminescence is present till room temperature. This is expected to be due to participation in the radiative recombination of predominantly those electrons and holes which are localized deepest in the bandgap. In this case we may expect a sizeable narrowing of g(log τL ). The inset in Fig. 9.6(b) [5] or its comparison with the curves shown in Fig. 9.6(a) demonstrate that this is indeed the case.

9.4 Spectral shape of the emission band Figure 9.7 displays examples of photoluminescence emission spectra of several pure amorphous semiconductors [9–11]. All of these spectra exhibit a simple structureless band of considerable width (FWHM ≈ 200–400 meV). Its shape is approximately Gaussian—with a minor asymmetry towards low photon energies—and does not exhibit any indications of a potential ﬁne structure. To explain this spectral shape, ﬁrstly we shall attempt to apply some of the models discussed in previous chapters. However, because of the different microscopic essence and different density of the electronic states, participating in the radiative recombination in the amorphous and crystalline phases, it is not at all obvious whether we shall succeed. For instance, it stands to reason that the model of free e–h pairs (Section 5.2) is inapplicable, since now the light emission originates in localized states. Besides, the observed bandwidth is much larger than the corresponding Boltzmann factor ∼ k B T 2 It is worth stressing that if the left-hand side of (9.10b) contains the stretched exponential function, the distribution f (1/τL ) cannot be analytically expressed via simple functions such as the Gaussian distribution, etc.

Spectral shape of the emission band

251

Fig. 9.6 (a) The distribution function g(log τL ) of photoluminescence of a-Si:H for various emitted photon energies at T = 50 K, after Oheda [8]. To acquire τL , the method of phase shift (Subsection 2.9.2) was used; the lower abscissa represents the modulation frequency of the excitation radiation. (b) The photoluminescence decay curve in an amorphous alloy a-Si:H with 19 at.% of hydrogen, room temperature. The inset demonstrates narrow distribution function g(log τL ). After Luterov´a et al. [5].

(≈ 25 meV at room temperature). For a similar reason we have to reject the radiative recombination of type e–A0 or h−D0 (Section 5.3). Excitons as the quasi-particles with a well-deﬁned wavevector do not exist in amorphous materials, thus we are not allowed to apply any of the channels of the exciton luminescence, discussed in Chapter 7. The broad emission band could perhaps correspond to electron–hole liquid EHL (Section 8.4) or electron–hole plasma EHP luminescence (Section 8.5), but these are high-excitation effects while in disordered semiconductors this kind of light emission occurs independently of the excitation intensity and, moreover, it exhibits its speciﬁc temperature behaviour (Section 9.2) that is incompatible with the EHL or EHP models.

252

Luminescence of disordered semiconductors And yet, there remains one possibility. A broad structureless emission band can occur at the localized optical centre with a strong electron–phonon coupling (Section 4.5). In disordered semiconductors, the non-equlibrium carriers actually become localized before recombination and, to employ the conﬁguration coordination concept, there is no need to meet the presumption about the long-term ordering (i.e. a regular crystalline lattice). This is the basic idea underlying the phonon broadening model, which has been submitted to interpret the broad emission band in a-Si:H by Street [12]. This concept therefore assumes that each e–h pair localized in the tail states has a strong phonon interaction with the surrounding matrix, which leads to a large Huang– Rhys factor S 1 (or to a Debye–Waller factor u DW = 0), to the absence of the no-phonon line and the appearance of a broad Gaussian emission band with a considerable Stokes shift. The bandshape is then described by (Appendix F) [hν − (E 0 − E R )]2 a , (9.11) Isp (hν) ≈ const exp − 2σ 2 where E 0 is the transition no-phonon energy, E R = S h¯ ω stands for the relaxation energy (h¯ ω being the phonon energy) and σ denotes the band halfwidth at the points of inﬂection. Indeed, the emission band maximum in a-Si:H peaks at ∼ 1.4 eV (Fig. 9.7), while the optical bandgap width amounts to ∼ 1.9 eV. The shift in the luminescence maximum from the absorption edge thus amounts to 2E R ∼ 0.5 eV. Enumerating the FWHM of the√band, which is described by eqn (9.11), through relation (F-4), yields σF = 4 ln 2E R h¯ ω ≈ 370 meV if we consider E R = 250 meV and adopt h¯ ω = 50 meV as a typical phonon energy. Everything

Fig. 9.7 Examples of the emission spectra of undoped hydrogenated amorphous semiconductors. From the top downwards: a-C:H (after Ko´os et al. [9]), a-Si:H (after Street and Biegelsen [10]) and multilayers a-Si:H (5 nm)/a-Ge:H (1 nm) (after Deki et al. [11]). The lowermost curve documents independency of the spectral shape of the excitation wavelength (λex = 488 nm and λex = 790 nm were applied). Notice also different measurement temperatures.

Spectral shape of the emission band

253

corresponds well to experimental data. The phonon broadening model thus reasonably describes the dominant spectral features, however, at the same time it involves implicitly the assumption about a ﬁxed value of the no-phonon energy of all of the recombining e–h pairs (at most, the model can allow for a very narrow distribution of these energies only); otherwise an additional inhomogeneous broadening due to disorder would arise. This assumption is open to discussion and, in fact, denies to a large extent the effect of the ﬁnite width of the tail states. Moreover, the experimentally observed emission band is not fully symmetric but exhibits a slight low-energy tail. Therefore, a diametrically opposite approach to the interpretation of the emission band—particularly in a-Si:H again—has been taken by Dunstan and Boulitrop [13, 14]. They have proposed a model of disorder broadening in which the tail states are supposed to be quite ‘solid’, i.e. without any electron– phonon interaction, and the sizeable emission bandwidth is interpreted as being due to a wide distribution of these states. Here, an idea might cross our mind, namely, that the authors copy the procedure we used previously to derive the spectral shape of the luminescence of free e–h pairs in indirect crystalline semiconductors (Subsection 5.2.2): the convolution of occupied electron and hole states, this time in the relevant tail states instead of in the conduction and valence bands.3 It is thus tempting to adopt relation (5.10) in which we merely replace the square root functions by the exponential expressions (9.1) and (9.2). However, we are not allowed to proceed in this way. Amorphous semiconductors, as already stressed several times, have their speciﬁc features. Above all, the tunnelling radiative lifetime τr is not constant but depends strongly on the electron–hole separation. The transition matrix element thus cannot be put outside the integral. In addition, in amorphous materials it is possible, no doubt, to introduce the Fermi–Dirac distribution function for electrons and holes, but not all the non-equilibrium e–h pairs are able to recombine radiatively (owing to the random spatial distribution of the tail states, see below). This is why the Fermi–Dirac function is not applicable to calculate the occupation of luminescence-active states. The crucial problem of the disorder broadening model is thus to determine the distribution function of carriers recombining radiatively in the tail states. To this end, Boulitrop and Dunstan [13] suppose that a very fast thermalization of non-equilibrium carriers down to the lowest states within a critical volume (surroundings) Vc takes place before the recombination occurs. This volume is driven by the rate of hopping carrier diffusion, i.e. the rate of the non-radiative tunnelling transitions to lower unoccupied states. Let this neighbourhood contain N states (Fig. 9.8) and let us select one reference couple of e–h states. The probability pn of another couple, next to the reference couple, having a lower energy (E 0 –E) decreases exponentially with increasing

3 Of course, now the wavevector concept and thus the notion of direct and indirect transitions are useless and, moreover, the recombining carriers are localized. Nevertheless, the e–h recombination is indirect in real space, because the electron and the hole cannot get localized on the same place; see Fig. 9.1(b) or Fig. 9.4.

Fig. 9.8 Illustrating the calculation of the luminescence occupation probability of the tail states. In a volume Vc around an e–h pair with the lowest energy (i.e. with the maximum value of E) there are N other couples of states.

254

Luminescence of disordered semiconductors E, i.e. pn = e−E/E c 0(v 0) . This means that the probability of the occurrence of a neighbouring couple with a higher energy (E 0 –E) is pm = (1 − pn ) = (1 − e−E/E c 0 (v 0) ). Should the number of such neighbours be N , then the occupancy probability of the relevant states will be pec(v) (E) = (1 − e−E/Ec 0(v 0) ) N .

(9.12)

The density of occupied electron states Rc (E), as a product of the total density of states gc (E) with the relevant occupation function pec , then reads Rc (E) = gc (E) pec (E) ≈ e−E/E c0 (1 − e−E/E c 0 ) N .

(9.13a)

Similarly, for the states occupied by holes we get Rv (E 0 − hν − E) ≈ e−(E 0 −hν−E)/E v0 [1 − e−(E 0 −hν−E)/E v0 ] N

(9.13b)

and the shape of the emission spectrum is described, in analogy with (5.10), by the convolution E 0 −hν a (hν) Isp

≈

Rc (E)Rv (E 0 − hν − E)dE.

(9.14)

0

Let us note that expression (9.14) does not involve a distribution of radiative lifetimes; it holds for a single value of τr . The material parameters of a-Si:H yield the value of the important parameter N to be N ≈ 50 (see Problem 1/4). An arbitrary electron thus must not be combined with an arbitrary hole, unlike the recombination of free e–h pairs in an indirect bandgap crystalline semiconductor. The values of the occupied tail state densities, calculated with the aid of (9.13),4 are shown in Fig. 9.9(a). a (hν), obtained with the use of (9.14), is compared The theoretical lineshape Isp with two experimental spectra in Fig. 9.9(b). Obviously the calculated spectrum (curve c) follows well the experimental asymmetry (curves a, b) but is considerably narrower compared to the measured spectra. Taking into account the experimentally determined distribution of radiative lifetimes makes the cala (hν) rather elaborate [14] and the result is represented by curve culation of Isp (d) in Fig. 9.9(b). This curve is wider than the theoretical spectrum (c), but still narrower than the experimental curves. Therefore, the ‘disorder broadening’ model does not do full justice to the microscopic nature of the luminescence band in disordered semiconductors, and clearly is to be combined with Street’s phonon broadening model. A detailed analysis of the applicability of both models in the case of a-Si:H and related alloys can be found in [15]. Another way to improve the disorder broadening model consists in the following reasoning: The involved assumption about full thermalization of 4 The approximation [1 − exp(−x)] N ∼ = exp[−N exp(−x)] has been used.

Some other properties of luminescence

255

Fig. 9.9 (a) The densities of occupied tail states of the conduction and valence bands in a-Si:H (dashed lines) that participate in the radiative recombination. (b) Comparison of two experimental photoluminescence spectra of a-Si:H (curves a, b, T = 8 K) with the theoretical shape by Dunstan and Boulitrop, calculated both employing (9.14) for a single value of τr (= 10 ms, curve c) and taking into account the experimental distribution function of τr with non-zero width (curve d). After Dunstan and Boulitrop [14].

carriers before recombining in fact discriminates the potential radiative recombination of ‘hot carriers’, represented by the left transition in Fig. 9.4 (and, to explain the broad distribution curve of lifetimes, the model offers merely a distribution of distances between the localized electrons and holes, like, after all, most other authors). If we admit the existence of the hot luminescence, then the theoretical curves in Fig. 9.9(b) will obviously broaden. The relevant mathematical description, however, would be rather complicated.

9.5 Some other properties of luminescence of disordered semiconductors 9.5.1 Correlation effects Excitonic effects play an important role in the luminescence of crystalline solids. The Wannier exciton, a large-radius correlated electron–hole pair moving freely through the lattice, does not exist in disordered materials. However, one may think of an electron–hole correlation of another type. As the wavevector k of a non-equilibrium carrier is not a good quantum number, its uncertainty can be considered to be inﬁnitely large, k → ∞, and the uncertainty relations then for the spatial coordinate x predict x → 0. One can

256

Luminescence of disordered semiconductors thus, unlike the crystalline semiconductors, attribute to an electron and a hole a certain space coordinate. We have already met this concept in Figs 9.1 and 9.4 and when discussing the Boulitrop and Dunstan model. Many authors in this context consistently distinguish between recombination of the so-called geminate and non-geminate e–h pairs. Under the geminate pair one understands an electron–hole couple created through the absorption of a given photon in a given site (which means the recombining electron and hole are correlated to a certain extent). The non-geminate pair is represented by an electron and a hole that have originated in different parts of the sample as a consequence of two separated photon absorption events. Because the photocarrier diffusion length in disordered semiconductors is short, obviously the recombination of geminate pairs dominates at low optical excitation levels when the created e–h pairs are sufﬁciently separated from each other, while at high excitation levels the e–h pairs may ‘mix up’ and the non-geminate recombination may no longer be negligible. One of the central issues of the luminescence of amorphous semiconductors has been for a long time the question of whether radiative recombination (i.e. the tunnelling in the tail states) takes place in arbitrary pairs or in geminate pairs only. Without going into details (we refer to the monograph by Street [1]), at present it is believed that it is the geminate pairs that dominate in luminescence while the annihilation of the non-geminate pairs represents a channel of non-radiative recombination and can be detected for instance via light-induced electron spin resonance. It is worth noting, however, that Dunstan and Boulitrop in their model [14] do not explicitly differentiate between geminate and non-geminate recombination (even if it can be deduced that implicitly they had in mind the recombination of geminate pairs only). Besides, in the injection electroluminescence, as a matter of fact all e–h pairs ought to be considered non-geminate and, consequently, the electroluminescence of amorphous semiconductors would not occur at all. At the same time the very occurrence of electroluminescence in a-Si:H p-i-n structures has been established beyond any doubt for a long time [16] and, even if its intensity is comparatively low, it is applied for instance to studying the microscopic mechanisms of photocarrier recombination and their relations to charge transport processes [17]. Moreover, the electroluminescence of LED structures based on the p-i-n junction in amorphous hydrogenated silicon carbide a-SiC:H exhibits at room temperature a relatively high quantum efﬁciency (∼ 10−3 %) and high brightness (of the order of 10 cd/m2 ). The emission is situated in the visible region and these devices have been considered potential candidates for optoelectronic light sources [18]. All these facts are hard to explain if we accept unreservedly the non-radiative recombination of non-geminate pairs.

9.5.2 Non-radiative recombination Multiple passages in this chapter have mentioned possible paths of the nonradiative recombination of e–h pairs in amorphous semiconductors. These have been:

Some other properties of luminescence

257

1. A recombination mediated by the dangling bonds, i.e. the Shockley–Read recombination at defect levels located approximately in the middle of the bandgap; 2. thermal quenching; 3. recombination of non-geminate e–h pairs. Two additional mechanisms (occurring also in crystalline solids) should be attached, namely: 4. Auger recombination; 5. surface recombination. Auger recombination gains importance at high excitation intensities (Subsection 6.1.2). Figure 9.10 [19] shows how the relative photoluminescence quantum efﬁciency ηL in a-Si:H and the relevant decay time (τL ) distribution depend on the excitation photon ﬂux φ; obviously for φ above a certain level a marked decrease in the luminescence quantum efﬁciency (not intensity!) occurs and, simultaneously, the decay time gets shorter. This undoubtedly indicates the opening of a new channel of non-radiative recombination, which may be plausibly identiﬁed with the Auger process (Problem 9/5): under comparatively high excitation, not only the deep tail states but also shallow localized states close to the mobility edge will be occupied. The latter are characterized by a high spatial density and are thus located close to each other. Under these circumstances the energy of such a recombining e–h pair may be transferred either to an electron or to a hole residing in the close neighbourhood. The rate of such an Auger process may even be increased in

Fig. 9.10 (a) The distribution of photoluminescence decay times τL , in a-Si:H features, at a very low temperature (here T = 2 K), two maxima (see also Fig. 9.6(a)). (b) Plot of the temporal location of these maxima and of the relative luminescence quantum efﬁciency ηL versus the excitation photon ﬂux φ. It can be seen how, under high excitation, τL gets shorter and ηL is reduced. After Stachowitz et al. [19].

258

Luminescence of disordered semiconductors comparison with crystalline counterparts because of the breakdown of the kconservation rule. There is, however, also an alternative point of view. Stachowitz and coworkers [19] have concluded, by analysing the experimental data in Fig. 9.10 that, instead of the Auger process, it is the non-radiative recombination of nongeminate pairs which is responsible for the observed drop of τL and ηL . They proceed even further, rejecting even the concept of geminate pair radiative recombination and proposing the only possible luminescence centre in a-Si:H to be e–h pairs with extremely small separation R between the electron and the hole (R ∼ 0.5–1 nm), therefore a kind of ‘small-radius localized exciton’. The occurrence of two maxima in the luminescence decay time distribution (Fig. 9.10(a)) they propose to interpret via recombination of singlet and triplet ‘excitons’ (whose existence is based on the exchange interaction between spins of closely spaced carriers in the ‘exciton’). However, neither can this opinion be easily reconciled with the existence of electroluminescence mentioned in Subsection 9.5.1. Surface recombination in a thin subsurface layer, owing to the presence of speciﬁc unsaturated bonds near the surface, was treated in Subsection 6.1.1. Microscopic features of this non-radiative recombination remain unchanged in disordered materials but, because the thickness of the luminescence ‘dead’ layer close to the surface depends on the photocarrier diffusion coefﬁcient D which is small in disordered semiconductors, the thickness of this non√ luminescent layer L = Dτ is also very small, typically L ∼ 0.01 μm at low temperatures. Thus, although the concentration of the subsurface defects is large, the impact of the surface non-radiative recombination on the total luminescence intensity reduction is small (∼ 10%). Examining once more all of the ﬁve mechanisms of non-radiative recombination put forward above, we notice that from the microscopic point of view items (1), (2), (3) and perhaps even (5) can be reduced to a shared basis, which is the occurrence of dangling bonds: In thermal quenching, in surface recombination and perhaps even in non-geminate pair non-radiative recombination, the ﬁnal dissipation stage of the electronic excitation energy proceeds via a deep defect level. Both kinds of photocarriers meet there in the end, upon accomplishing the diffusion motion, provided they did not ﬁnd a way to recombine radiatively. A full consensus does not exist in this respect (an alternative chance for the non-geminate pairs is to recombine through direct non-radiative tunnelling between localized states), in any case, however, the role of the dangling non-saturated bonds in non-radiative recombination is substantial.

9.5.3 Luminescence of impurities and defects Till now we have occupied ourselves with the luminescence of pure disordered semiconductors. It is legitimate to ask whether doping of amorphous semiconductors with donors and acceptors can induce novel luminescence processes, similarly to the crystalline analogues (e.g. e–A0 , h–D0 , etc.). Even though the donor and acceptor energy levels in amorphous materials are broadened due to

Some other properties of luminescence

259

Fig. 9.11 Sketch of the density of the donor states (beneath the conduction band bottom, E D stands for the donor binding energy) and of the deep defect states located approximately in the middle of the bandgap. One conceivable transition representing the defect-related luminescence (hν ∼ 0.8–0.9 eV in a-Si:H) is shown. E f denotes the Fermi level; G indicates the photogeneration rate of non-equilibrium electrons. The shadowed states are occupied in a non-excited semiconductor.

disorder (there is a distribution of the binding energies E D , E A ), as indicated in Fig. 9.11, one can certainly imagine for instance a recombination of the type h–D0 , when an electron from some of the donor levels recombines radiatively with a hole residing in the valence band tail states. It has been established experimentally that, e.g., a-Si:H doped with phosphorus or boron actually exhibits a new emission band in the near-infrared region (at ∼ 0.8–0.9 eV against the ‘intrinsic’ emission peaked at ∼ 1.4 eV), whose intensity is linked with the presence of the dopants, but the band is due to luminescence of deep defect levels rather than due to transitions e–A0 or h–D0 . The introduction of dopants produces new dangling bonds and, accordingly, corresponding deep defect levels roughly in the middle of the band appear. These levels, as we have already stressed several times, mediate predominant non-radiative recombination, but if their concentration is sufﬁciently increased due to doping, they can manifest themselves through a weak but measurable luminescence (Fig. 9.11). This luminescence therefore originates owing to the radiative recombination of a photocarrier that is localized in the tail states with an oppositely charged photocarrier trapped at the defect level.5 It should be stressed, of course, that the overall intensity of this long-wavelength emission amounts to a few percent of the principal luminescence band intensity only; the defect levels predominantly quench the ‘intrinsic’ luminescence and only then substitute it partially by a new channel of radiative recombination. Figure 9.12(a) displays emission photoluminescence spectra of a-Si:H doped with phosphorus [20]. Obviously, the defect luminescence at ∼ 0.85 eV can be excited, in line with Fig. 9.11, even by absorption of photons whose energy is considerably less compared to the bandgap width (E g ≈ 1.5 eV)). Since the band at ∼ 0.85 eV is fairly large, the relevant transition has been suggested to be characterized by a strong electron–phonon interaction. This is qualitatively illustrated by the conﬁgurational coordinate model sketched 5 The doping has to be relatively high (> 1017 cm−3 ). The Fermi level thereby shifts from the middle of the bandgap close to the relevant mobility edge, and charged dangling bonds along with their correlation energies enter the play. Details go beyond the scope of this book, see Street, R. A. (1991). Hydrogenated Amorphous Silicon. Cambridge University Press, Cambridge.

260

Luminescence of disordered semiconductors

Fig. 9.12 (a) Low-temperature emission spectra of a-Si:H doped with phosphorus (∼ 1018 cm−3 ), under various excitation photons hνex . Numbers in parentheses denote relative intensities of the maxima. (b) Conﬁgurational coordinate diagram for the defect luminescence in a-Si:H:P. After Tajima et al. [20].

in Fig. 9.12(b). A note may be in order pointing to the resemblance with Fig. 6.1(c), which elucidates an analogous process in a localized centre of a crystalline phosphor. However, the question of why radiative processes like (e−A0 ) or (h–D0 ) have not been observed in amorphous semiconductors is still to be answered here. The reason lies again in the unique feature of these materials—the occurrence of the tail states. From the luminescence point of view, the donor and acceptor states in an excited sample become in fact indistinguishable from the overlapping tail states, ‘fusing’ with them (see Fig. 9.1(a) or 9.11). This implies that the potential manifestation of their radiative recombination—if any—is included in the main emission band at ∼ 1.4 eV. Provided the concentration of donors or acceptors is very high (∼ 1019 –1020 cm−3 ), comparable to or even higher than the total density of the tail states, one could perhaps expect some structure superimposed on this emission band. In this case, however, complete quenching of the ∼ 1.4 eV luminescence due to the high concentration of the defects mostly prevails.

9.5.4 Luminescence ‘fatigue’ Photoluminescence in amorphous semiconductors may be accompanied by an undesirable adverse effect: gradual fading away of the main emission band, which is observable mainly under relatively high excitation. This is, as generally accepted, due to the Staebler–Wronski effect or the light-induced formation of the dangling bonds; these bonds represent, as already stressed,

Problems powerful quenching centres. An example is displayed in Fig. 9.13, which shows luminescence decay curves of a-Si:H, measured before and after illuminating the sample with an intense cw argon-ion laser (514 nm; 0.54 W; 45 min) [21].6 A decrease of the luminescence intensity upon illuminating down to about 60 % of the initial value is evident, along with decay shortening. This corresponds to an increased rate of non-radiative transitions. It is worth mentioning that similar experiments performed in nominally pure a-Si:H revealed a moderate increase in intensity of the weak defect luminescence at ∼ 0.85 eV [22], which ﬁts well the concept of the Staebler–Wronski effect as a phenomenon caused by enhancement of the dangling bond density. Annealing of the sample at a temperature of 150–200◦ C for one hour usually leads to a complete recovery of the initial photoluminescence intensity. It is well known that the application potential of amorphous semiconductors has overtaken—already a long time ago—our detailed microscopic understanding of their physical and chemical properties. The present knowledge of the luminescence processes conﬁrms this state of the art—we have been emphasizing throughout this chapter that, as yet, no consensus has been achieved about many issues of both radiative and non-radiative recombination.

9.6 Problems 9/1: In expression (9.6) for η it has been tacitly supposed that all the tail states are occupied, otherwise in the integrals ﬁguring in (9.6) an occupation function f would have appeared (here we apply f = 1). Prove that in case this supposition is not valid, one obtains the resulting temperature dependence formally identical with eqn (9.7), only instead of T a temperature T > T will appear. Determination of the slope 1/T0 therefore is not affected. 9/2: Assess the tail state width E v0 in hydrogen-rich a-Si:H, on the basis of the temperature dependence shown in Fig. 9.2(b). Values of the parameters p0 , τr can be found throughout the text of Chapter 9. 9/3: Show that (a) if the distribution of luminescence decay times g(log τL ) is very narrow, then expression (9.10) transforms into (9.9), while (b) if g(log τL ) is very broad, it can be approximated as g(log τL ) = g(log t) ≈ i L (t)t, or simply via multiplying the luminescence intensity i L (t) by the relevant time decay t related to the end of the excitation event. (For example the curve g(log τL ) in Fig. 9.5 has been determined in this way.) Start from eqn (9.10). 9/4: By making use of [13] explain how to estimate the value of the parameter N appearing in eqns (9.12)–(9.14), which represents the number of highenergy (E 0 –E) tail states in the neighbourhood of a particular lowerenergy site with a trapped thermalized photocarrier. 6 The photoluminiscence decay by itself was measured under excitation with a low-peak-power pulsed laser (0.8 kW) in order to avoid distortion of the results owing to the fatigue effect.

261

Fig. 9.13 Photoluminescence decay curves in a-Si:H (the emission band at ∼ 1.4 eV, energy of excitation photons hνex = 2.53 eV, pulsed excitation 10 ns). Circles and diamonds denote measurements before and after light-induced degradation, respectively. After Hirabayashi et al. [21].

262

Luminescence of disordered semiconductors 9/5: With the aid of the equation dn/dt = G–n/τr –βn 2 comprising Auger non-radiative recombination prove that, at a very high photogeneration rate G, drops both in the luminescence decay time and quantum yield occur, driven by a proportion ∼ G −1/2 . Comment: A speciﬁc ‘extrinsic’ Auger recombination of bimolecular type (see eqn (6.8)) in disordered semiconductors is considered.

References 1. Street, R. A. (1991). Hydrogenated Amorphous Silicon. Cambridge University Press, Cambridge. 2. Staebler, D. and Wronski, C. (1977). Appl. Phys. Lett., 31, 292. ˇ ep´anek, J., Lechner, T., Pelant, I., Meier, J., 3. Kudrna, J., Mal´y, P., Troj´anek, F., Stˇ and Kroll, U. (2000). Mater. Sci. Eng. B, 69–70, 238. 4. Collins, R. W., Paesler, M. A., and Paul, W. (1980). Solid State Comm., 34, 833. 5. Luterov´a, K., Pelant, I., Fojt´ık, P., Nikl, M., Gregora, I., Koˇcka, J., Dian, J., ˇ ep´anek, J., Poruba, A., and Horv´ath, P. (2000). Phil. Mag. Valenta, J., Mal´y, P., Stˇ B, 80, 1811. 6. Tsang, C. and Street, R. A. (1979). Phys. Rev. B, 19, 3027. 7. Wang, W. and Fritzsche, H. (1989). Photoluminescence in a-Si:H ﬁlms and multilayers. In Advances in Semiconductors, Vol. 1, Amorphous Silicon and Related Materials, Vol. B (ed H. Fritzsche), p. 779. World Scientiﬁc, Singapore. 8. Oheda, H. (1993). J. Non-Crystal. Solids, 164–166, 559. 9. Ko´os, M., P´ocsik, I., and T´oth, L. (1993). J. Non-Crystal. Solids, 164–166, 1151. 10. Street, R. A. and Biegelsen, D. K. (1980). Solid State Comm., 33, 1159. 11. Deki, H., Miyazaki, S., Ohmura, M., and Hirose, M. (1993). J. Non-Crystal. Solids, 164–166, 841. 12. Street, R. A. (1978). Phil. Mag. B, 37, 35. 13. Boulitrop, F. and Dunstan, D. J. (1983). Phys. Rev. B, 28, 5923. 14. Dunstan, D. J. and Boulitrop, F. (1984). Phys. Rev. B, 30, 5945. 15. Searle, T. M. and Jackson, W. A. (1989). Phil. Mag. B, 60, 237. 16. Pankove, J. E. and Carson, D. E. (1976). Appl. Phys. Lett., 29, 620. 17. Wang, K., Han, D., Kemp, M., and Silver, M. (1993). Appl. Phys. Lett., 62, 157. 18. Kruangam, D. (1991). Amorphous and microcrystalline silicon–carbide alloy light–emitting diodes: physics and properties. In: Amorphous & Microcrystalline Semiconductor Devices (ed J. Kanicki), p. 195. Artech House, Boston. 19. Stachowitz, R., Schubert, M., and Fuhs, W. (1998). J. Non-Crystal. Solids, 227– 230, 190. 20. Tajima, M., Okushi, H., Yamasaki, S., and Tanaka, K. (1986). Phys. Rev. B, 33, 8522. 21. Hirabayashi, I., Morigaki, K., and Nitta, S. (1980). Jap. J. Appl. Phys. 19, L357. 22. Tajima, M., Okyama, H., Okushi, H., Yamasaki, S., and Tanaka, K. (1989). Jap. J. Appl. Phys., 28, L1086.

Stimulated emission

Stimulated emission can be viewed as a special case of luminescence. Its character conforms to the deﬁnition of luminescence (the excess electromagnetic radiation when compared to the equilibrium radiation as described by Planck’s law, featuring simultaneously a ‘sufﬁciently long’ lifetime), although the thermodynamic conditions necessary for its occurrence differ fundamentally from the common occupancy of electronic states in spontaneous luminescence processes. A population inversion of energy levels, a state diametrically opposed to thermodynamic equilibrium, needs to be achieved. That is why, among other things, the spectral distribution of stimulated emission cannot be described using relations (5.9), (7.11) or (7.16), as these relations are valid provided that only minute variations from the equilibrium occupancy of states occur. It is thus obvious that the description of stimulated emission needs to be based on a completely different principle. Apart from the thermodynamic non-equilibrium, the nonlinear character of this optical process starts to be of particular importance. In this chapter, we will ﬁrst formulate the conditions necessary for the occurrence of stimulated emission in bulk semiconductors. Then, we will show how stimulated emission can originate in an electron–hole plasma (EHP) and discuss possible contributions of excitons and excitonic complexes to stimulated emission. Finally, the methods employed for the study of optical gain will be described.

10.1 Spontaneous versus stimulated emission. Optical gain The phenomenon of stimulated emission is generally unconsciously perceived as the fundamental principle underlying the operation of all lasers. In luminescence spectroscopy, stimulated emission can be treated from two diametrically opposed points of view. If a particular phosphor is studied as a potential new active laser medium, any manifestation of stimulated emission is warmly welcome. If, on the other hand, importance is put on the basic research of the fundamentals of radiative recombination processes, should (unintentionally) stimulated emission arise, the emission spectrum or luminescence dynamics

10 10.1 Spontaneous versus stimulated emission. Optical gain

263

10.2 Optical gain in semiconductors

267

10.3 Spectral shape of the optical gain

271

10.4 Stimulated emission in an indirect-bandgap semiconductor

278

10.5 Participation of excitons in stimulated emission

282

10.6 Experimental techniques for measuring the optical gain 287 10.7 Problems

299

264

Fig. 10.1 Emission spectra of an electron–hole plasma (EHP) in various kinds of CdS crystals with different sizes of the excited area (bath temperature 4.2 K, excitation with a nanosecond dye laser 470 nm). (a) Thin ﬁlm, 0.2 mm, excited area 0.8 × 0.8 mm2 . (b) Thin ﬁlm, 0.2 mm, excited area 0.1 × 0.1 mm2 . (c) Bulk crystal with thickness of 5 mm, excited area 0.8 × 0.8 mm2 . Excitation intensity was 5 MW/cm2 in all cases. After Yoshida et al. [1].

Fig. 10.2 EHP emission spectra of thin-ﬁlm CdS. Excitation intensities of a pulsed nitrogen laser (337 nm, 10 ns) are noted at the corresponding curves. Although the excited area is extremely small, approximately 10 × 10 μm2 , an indication of several lasing modes appears at 16 MW/cm2 . After Lysenko et al. [2].

Stimulated emission can be inﬂuenced in such a way that they give rise to the formulation of an incorrect model of the luminescence centre and to erroneous conclusions. This can easily happen when measurements are carried out at low temperatures and in direct-bandgap semiconductors, which typically exhibit high radiative recombination rates. Consequently, it is indispensable to know, in the ﬁrst place, what experimental conditions are favourable for making the occurrence of stimulated emission in experiment highly probable, and thus what measures can be taken to prevent it if necessary. An immensely important role in this context is played even by the shape of the sample and the applied geometry of the experiment (Fig. 10.1) [1]. If the excited spot is a relatively large (diameter ≈ 1 mm) area of a sample with a surface of high optical quality (e.g. a semiconductor thin ﬁlm, either freestanding or on a polished substrate), the spontaneous luminescence, travelling in the plane of the sample within the excitation spot, will very likely stimulate the emission of other photons. This situation is illustrated in Fig. 10.1(a), where the hatched area demonstrates the contribution of stimulated emission from an electron–hole plasma (EHP) in a thin CdS slab with the excited area of 0.8 × 0.8 mm2 at T = 4.2 K. The spontaneous EHP emission itself is represented by a broad background band. The contribution of stimulated emission can even be enhanced if the detection system also collects the photons emitted from the edge of the sample (the waveguiding effect in the ‘reﬂection’ geometry at 90◦ angle mentioned in Section 2.1). Reducing the excitation area to 0.1 × 0.1 mm2 (Fig. 10.1(b)) obviously results in the suppression of EHP stimulated emission, however, a new M line appears due to the radiative decay of excitonic molecules. On the other hand, if a bulk crystal of relatively large dimensions with irregular edges is used, pure EHP spontaneous emission can be detected (Fig. 10.1(c)). It is important to point out the fact that at very high excitation ﬂuences even a radical decrease in size of the excited area to the order of 10 × 10 μm2 does not necessarily prevent the onset of stimulated emission, as is demonstrated in the top curve in Fig. 10.2; this graph again displays low-temperature light emission of a CdS thin ﬁlm under pulsed laser excitation [2]. Let us come back for a short while to Fig. 10.1. The identiﬁcation of the hatched area in the spectrum with actual stimulated emission is deﬁnitely not straightforward; the assignment might be made clearer, however, by employing, e.g., time-resolved luminescence spectroscopy. The results of such measurements, carried out on an EHP in a material related to cadmium sulphide, namely in cadmium selenide CdSe, are shown in Fig. 10.3. Whereas the timeintegrated spectrum (top curve) comprises both spectral components (i.e. those originating in both spontaneous and stimulated emission), spectra measured at different time delays after the 20-ps excitation pulse conﬁrm that the longwavelength component decays much faster, which is a strong indication of stimulated emission [3]. Our goal for now will be to formulate a relation describing the spectral lineshape or, more speciﬁcally, the shape of the emission band corresponding to stimulated emission in semiconductors. First, we will make a short digression into atomic spectroscopy to recall the basic concepts of spontaneous and stimulated transitions in the optical region. Based on an analogy with a two-level atomic system, the concept of optical gain will be introduced.

Spontaneous versus stimulated emission

265

Fig. 10.3 Time-resolved emission spectra of EHP in a thin-ﬁlm CdSe slab (0.3 mm). Excitation was performed using a pulsed Nd:YAG laser system (532 nm, 20 ps, diameter of the beam 2–3 mm); excitation intensity was 10 MW/cm2 . A relatively high bath temperature of 260 K was chosen so that the contributions of spontaneous and stimulated emission were more or less comparable; at higher temperatures, the conditions necessary to achieve stimulated emission can be met only with difﬁculty, while at sufﬁciently low temperatures the stimulated-emission contribution dominates. After Yoshikuni et al. [3].

This concept, along with the relevant emission spectra, is commonly exploited in spectroscopy for characterizing active laser media; in many cases, especially in semiconductor lasers, gain is used even more frequently than the spectrum. To a large extent, we will follow the reasoning used in [4] and [5]. In a two-level atomic system (Fig. 10.4(a)), the rate of transitions from level |2 to level |1, accompanied by spontaneous emission of a photon hν and being independent of external conditions, is equal to the Einstein coefﬁcient of spontaneous emission A 21 = 1/τsp (s−1 ), where τsp is the spontaneous lifetime of the level |2.1 Stimulated emission between levels |2 and |1, as well as the inverse transition |1 → |2 (i.e. the absorption of a photon hν), are conditioned by the presence of a resonant radiation with the spectral energy density u(ν)(J/cm3 s−1 ). The corresponding rates of optical transitions can then be expressed as W21 = B21 u (ν)

(s−1 )

(stimulated emission)

and W12 = B12 u (ν)

(s−1 )

(absorption),

1 In a single atom, this lifetime is equivalent to the ‘radiative’ lifetime, because energy dissipation (through its transformation into heat) is not possible in this case.

Fig. 10.4 Schematic of possible optical transitions (a) in a two-level atomic system and (b) in a direct-bandgap semiconductor close to the absorption edge (in the absence of excitonic effects).

266

Stimulated emission where B12 is the Einstein coefﬁcient of absorption and B21 the Einstein coefﬁcient of stimulated emission. The relation connecting the coefﬁcients reads A21 8πh ν 3 = B21 c3

(10.1)

(c being the velocity of light in vacuum) and in the simplest case of nondegenerate levels also B12 = B21 holds. The densities of corresponding electron transitions then depend on the populations of the individual levels. If N1 and N2 denote the population densities of levels |1 and |2, then the numbers of atoms participating in the corresponding transitions per unit volume and unit time are psp = A21 N2 (cm−3 s−1 )

spontaneous emission, (10.2a)

p21 = W21 N2 = B21 u(ν)N2 (cm−3 s−1 ) p12 = W12 N1 = B12 u(ν)N1 (cm

−3 −1

s

)

stimulated emission,

(10.2b)

absorption.

(10.2c)

In atomic spectroscopy, the description of these processes involves the introduction of a normalized emission or absorption lineshape function γ (ν–ν0 ) (1/Hz = s), which takes into account the narrow, though ﬁnite linewidth around the ν0 maximum.2 Subsequently, the energy spectral density can be expressed as u(ν) = u ν γ (ν–ν0 ), where u ν stands for the energy per unit volume, and formulas (10.2) take on the form psp = A21 N2 ,

(10.3a)

p21 = W21 N2 = B21 N2 u ν γ (ν–ν0 ),

(10.3b)

p12 = W12 N1 = B12 N1 u ν γ (ν–ν0 ).

(10.3c)

Applying these equations, we can easily derive a formula for the absorption coefﬁcient α(ν) in the Lambert–Beer law or, as the case may be, for the so-called optical gain coefﬁcient g(ν). Let a (probe) parallel beam of photons hν, whose power ﬂux density, or intensity, is given by Iν = cuν (W/cm2 ), impinge on our atomic system in the z- direction from an external source (such as a spectral lamp). The variation in the intensity on the path element dz can obviously be written as dIν = hν(A21 N2 + W21 N2 –W12 N1 )dz. Usually, the contribution of isotropic spontaneous emission in the given direction can be assumed to be much smaller than the contribution of stimulated emission, i.e. A21 N2 W21 N2 and thus dIν = hν(W21 N2 − W12 N1 )dz.

(10.4a)

It follows from B12 = B21 and (10.1) that c2 dIν γ (ν − ν0 )Iν . = (N2 − N1 ) dz 8πν 2 tsp

(10.4b)

2 Besides, it is of importance in many cases whether γ (ν–ν ) describes a homogeneously or 0 inhomogeneously broadened spectral line.

Optical gain in semiconductors From the phenomenological point of view, the assumption about the validity of the Lambert–Beer law Iν (z) = Iν (0) exp(–α(ν)z) is fully justiﬁed, immediately leading to dIν = −Iν α(ν). dz

(10.5)

The comparison of the microscopic (10.4b) and macroscopic (10.5) approaches ﬁnally yields the formula for the absorption coefﬁcient α(ν) = (N1 − N2 )

c2 γ (ν − ν0 ) (cm−1 ). 8πν 2 tsp

(10.6)

If the levels |1 and |2 are occupied in a standard way, i.e. N1 > N2 , the probe beam is attenuated since α(ν) > 0. If, on the other hand, population inversion, i.e. N2 > N1 , is achieved, it follows from (10.5) that the intensity Iν can rise exponentially along the z-direction, since α(ν) < 0. Under such circumstances, the quantity g(ν) = –α(ν) > 0 is referred to as the optical gain. This term will be speciﬁed shortly. Please note here that in the atomic case the spectral lineshape of the optical gain is determined by the shape of the corresponding (spontaneous) emission line.

10.2 Optical gain in semiconductors In many of the preceding chapters, the theoretical spontaneous emission lineshape for various mechanisms of radiative recombination was discussed. As regards stimulated emission, which is the case being analysed right now, neither a general theoretical description of the lineshape nor its comparison with experiment can be applied in most cases. In principle, two underlying reasons can be found. First of all, the strongly nonlinear character of stimulated emission makes the process, and naturally also its emission spectral lineshape, extremely dependent on the intensity of the stimulating light. Moreover, as was shown in the preceding section, spontaneous and stimulated emission in semiconductors often occur simultaneously in luminescence experiments (Figs 10.1–10.3), which brings even more difﬁculties in attempts at spectral separation of stimulated emission and its comparison with a theoretical lineshape. Nevertheless, a theoretical guideline exists even in this case; it should not be based on the emission spectrum itself but, instead, on the spectral distribution of the optical gain, which can often be both theoretically well described and—as will be shown in Section 10.6—in many cases reliably experimentally determined.3 Our goal for now will be the formulation of a general formula for the spectral shape of the optical gain in semiconductors. We proceed from the mechanism of EHP radiative recombination, a process which ﬁnds application in the operation of semiconductor injection lasers. The issue of how to mathematically formulate the optical gain in semiconductors 3 Even if the spectral distribution of the optical gain depends also on the excitation intensity, this dependence can be quantiﬁed, and, moreover, the optical gain does not contain any ingredient of spontaneous emission.

267

268

Stimulated emission dates back to the beginning of the 1960s [6, 7], which is the time when the very ﬁrst lasers of this type were built [8, 9]. One can easily ﬁnd that, unlike the atomic case, stimulated transitions between the quasi-continua of electron and hole states (Fig. 10.4(b))—not between discrete energy levels—need to be taken into account. Factors playing important roles will thus be the densities of states in the conduction ρc (E 2 ) and valence ρv (E 1 ) bands, respectively. For the case of a direct-bandgap semiconductor, in Section 5.2 we replaced these densities with the joint density of electron and hole states in the bands ρ(ν). Let us recall that under lowﬂuence excitation (i.e. without EHP) the formula for the probability density of spontaneous band-to-band emission reads Isp (hν) =

1 ρ(ν) f e (ν), τr

(10.7a)

where f e (ν) stands for the probability of ‘suitable occupancy of states’ in the conduction and valence bands. The role of the spontaneous lifetime tsp is, in semiconductors, taken on by the radiative lifetime of electron–hole recombination τr . When deriving f e (ν), we considered only a small deviation from thermodynamic equilibrium (due to the low-ﬂuence excitation), a situation that could be described satisfactorily by a single Fermi level E f pinned in the middle of the bandgap, as described by the well-known Fermi–Dirac distribution function f (E) =

1 . exp(E − E f /kB T ) + 1

(10.8)

The probability f e (ν) of (or the condition for the occupancy of levels for) emission of a photon was then given as the product f e (ν) = f c (E 2 )[1– f v (E 1 )], standing for the co-occurrence of an electron in the conduction band and a hole (with the same wavevectors) in the valence band. In other words, relation (10.7a) was rearranged into the form Isp (hν) =

1 ρ(ν) f c (E 2 ) [1 − f v (E 1 )] , τr

(10.7b)

resulting then in the Maxwell–Boltzmann lineshape of spontaneous emission. Let us now try to ﬁnd a formula analogous to eqn (10.7a) or (10.7b), but suitable for stimulated emission under high-ﬂuence excitation. We proceed from relations (10.2) or (10.3). Before starting we have to realize that this time the concept of the volume density of atoms N2 cannot be applied; instead, a term proportional to the product ρ(ν) f e (ν) and characterizing the ‘occupied joint states per unit volume (1 cm3 ) which are about to emit a photon’ will take on its role. Please note also that the quantities W21 and W12 in (10.2) represent the rates of optical transitions in an isolated atom or molecule, being thus in s−1 units. In a semiconductor, however, the closely packed atoms in a solid need to be taken into account, which results in the quasi-continuous distribution of energy levels, and the possibility of emission or absorption of a photon has to be related to some frequency interval (ν, ν + dν); therefore, we can specify that the role of N2 will be taken on by the factor ρ(ν) f e (ν)dν, having the same units as N2 (cm−3 ). Finally, it follows also that it will not be possible to study

Optical gain in semiconductors the optical gain (or absorption) employing quasi-monochromatic light with a single frequency ν0 and a spectral density of energy u ν γ (ν–ν0 ), but it will be necessary to employ, in general, light with a broad spectral distribution u(ν). It follows from what has been said above that the probability density of (hν), often referred to as the stimulated emission rate stimulated emission rstim (i.e. the number of photons hν = E 2 –E 1 emitted per second per 1 Hz and per 1 cm3 of the semiconductor [10]), can be expressed, in analogy with (10.3b), as rstim (hν0 ) dν0 = B21 u(ν0 ) γ (ν − ν0 ) ρ(ν0 ) f e (ν0 ) dν0 (cm−3 ).

The overall stimulated emission rate can then be obtained by integrating over all the allowed frequencies ν 0 , or rstim (hν) = rstim (hν0 ) dν0 = B21 u(ν0 )ρ(ν0 ) f e (ν0 ) γ (ν − ν0 ) dν0 and, as the linewidth of the individual energy levels from the quasi-continuum of electronic states in semiconductors is much smaller than the frequency band of stimulated emission, the approximation γ (ν − ν0 ) → δ(ν − ν0 ) can be exploited, yielding rstim (hν) = B21 u(ν) ρ(ν) f e (ν).

(10.9a)

Taking into account the ‘reciprocity’ of stimulated emission and absorption transitions, the photon absorption rate can be obtained by replacing the probability f e (ν) in (10.9a) by the occupancy condition for absorption f a (ν) = f v (E 1 )[1– f c (E 2 )]: rabs (hν) = B12 u(ν) ρ(ν) f a (ν).

(10.9b)

Consequently, the resulting rate of observable stimulated emission (taking into account the absorption-related losses) can be derived from (10.9a) and (10.9b), considering the equality B12 = B21 = B, as Rstim (hν) = rstim (hν) − rabs (hν) = B u (ν)ρ(ν) [ f c (E 2 ) − f v (E 1 )] . (10.10) Finally, an equation analogous to (10.4a) will now be of the form dI (ν) = hν [rstim (hν) − rabs (hν)] dz = hν Rstim (hν) dz,

(10.11)

where I (ν) = (c/n)u(ν) is the spectral distribution of intensity, i.e. the energy of optical radiation per 1 Hz per area of 1 cm2 per second. Taking into account the fact that I (ν) again satisﬁes the Lambert–Beer law (10.5) dI (ν) = −α(ν) I (ν) dz, we ﬁnd, making use of the comparison of the last two formulas, that the absorption coefﬁcient in this case reads α(ν) = −

hν Rstim (hν) , I (ν)

269

270

Stimulated emission which can, using (10.10), (10.1) and A21 = 1/τr , be easily transformed to express the optical gain as g(ν) = −α(ν) =

hν B u(ν)ρ(ν) [ f c (E 2 ) − f v (E 1 )] I (ν)

=

1 c2 ρ(ν) [ f c (E 2 ) − f v (E 1 )] τr 8πν 2 n 2

=

1 λ20 ρ(ν) [ f c (E 2 ) − f v (E 1 )] ; τr 8πn 2

(10.12)

λ0 is the wavelength of light in vacuum and n stands for the refractive index of the semiconductor. Thus, we have succeeded in ﬁnding a formula for stimulated emission, which is analogous to eqn (10.7b) describing the spectral shape of spontaneous emission at low excitation ﬂuences.4 Obviously, the spectral shape of the gain is inﬂuenced largely by the factor in square brackets (sometimes also referred to as the Fermi inversion factor), i.e. by the occupancy of the electron states in the conduction band and the hole states in the valence band, in other words, by the pump intensity. Before we discuss the spectral shape of g(ν) on the basis of (10.12), let us stop for a while to examine the time characteristics of stimulated emission. By formally comparing (10.10) with (10.7b), we can easily see that instead of the reciprocal spontaneous radiative lifetime τr−1 we can write for the case of stimulated emission 1 τstim

= B u(ν),

which can, using (10.1), be rearranged to 1 τstim

=

1 c2 I (ν) 1 λ20 φ(ν) , = 2 2 τr 8πn ν hν τr 8πn 2

(10.13)

when we have applied the substitution tsp → τr and deﬁned the mean spectral density of photons φ(ν) = I (ν)/ hν(cm−2 ) in units of the number of photons per second per cm2 per 1 Hz. Let us for now imagine an experiment in which the stimulated emission transitions are just setting in, causing the simultaneous occurrence of both spontaneous and stimulated transitions in the detected emission spectrum. The overall radiative lifetime τov at the chosen wavelength can then be expected to behave as λ20 φ(ν) 1 1 1 1 1 1+ξ > . = +ξ = (10.14) 2 τov τr τstim τr τ 8πn r 4 The role of the probe beam is, in luminescence experiments, taken on by the spontaneous emission in a given direction Isp (hν). By solving an equation similar to (10.11) it is possible to derive a formula for the ampliﬁcation of stimulated emission in the given direction Istim (hν, z) ∼ Isp (hν) exp[g(ν)z], which then in fact describes the spectral shape of the stimulated emission band. This illustrates, among other things, the above-mentioned nonlinearity of the process. This problem will be treated in more detail in Section 10.6.

Spectral shape of the optical gain The factor 0 < ξ(t) < 1 here stands for the relative part of the excited volume of material that takes part in the stimulated emission along the direction under investigation. Consequently, the onset of stimulated emission effectively shortens the radiative lifetime and thus also the experimentally measured luminescence lifetime. This shortening is a feature typical of the onset of stimulated emission (see Fig. 10.3) and can become quite signiﬁcant, indeed, as a result of the positive feedback implicit in eqn (10.14). Nevertheless, stimulated emission typically depletes the population inversion very quickly, fading itself away as a result, and the whole process of luminescence decay ﬁnishes through the slower spontaneous emission. We should point out, however, that the above discussion is valid only near the very threshold of the onset of stimulated emission, whereas in the case of real laser action inside a resonator it no longer serves any useful purpose. In the latter case, the rapid ‘emptying’ of electron states in the conduction band, rather than being directly linked to τr , is in a decisive way inﬂuenced by the quality and construction of the resonator, along with the level of pumping.

10.3 Spectral shape of the optical gain Let us now treat in more detail the spectral shape of function g(ν) deﬁned in eqn (10.12). In this case, obviously, the quasi-equilibrium state characterized by a single Fermi energy level cannot be applied, but we need to deﬁne (as indicated also in Fig. 10.4(b)) separate (quasi-)Fermi levels for electrons Fe , or μe and for holes Fh , or μh . We thus write f c (E 2 ) = (exp f v (E 1 ) = (exp

E 2 − μe kB T E 1 − μh kB T

+ 1)−1

(10.15)

+ 1)−1 .

In order to be more speciﬁc, let us add that the energies E 1 , E 2 , μe and μh share a common system of coordinates whereas Fe and Fh are values relative to the corresponding band extremes. At the same time, the Fermi energies are linked through the relation E g + Fe + Fh = μe − μh (= μ , the plasma chemical potential). An easy derivation of the Fermi inversion factor Γ (ν) = f c (E 2 )– f v (E 1 ) by making use of (10.15) shows that Γ (ν) can be expressed as a fraction with a positive denominator, possessing a numerator in the form of 1 − exp [(hν − E g − Fe − Fh )/kB T ].

(10.16)

In order to achieve positive optical gain (i.e. to describe the ampliﬁcation of light by stimulated emission, and not attenuation through absorption), the factor Γ (ν) = f c (E 2 )– f v (E 1 ) has to be positive according to (10.12), which, based on (10.16), implies hν < E g + Fe + Fh .

271

272

Stimulated emission Since the lowest photon energy hν which can be ampliﬁed in a given case is hν = E g , we obtain the following formulation of the condition for the occurrence of optical gain in semiconductors E g < hν < E g + Fe + Fh = μe − μh .

Fig. 10.5 Schematic sketch of the Bernard-Duraffourg condition for the inverse occupancy of energy states. Ampliﬁcation of radiation through stimulated emission can occur only between electron states with occupancy higher than 1/2 ( f c (E 2 ) > 1/2), and an analogous condition applies also for holes (1 − f v (E 1 > 1/2). States denoted by hatched areas are occupied largely by electrons.

(10.17)

This is the well-known Bernard–Duraffourg condition for inverse population of states and ampliﬁcation of radiation through stimulated emission in a degenerate semiconductor [6]. It is valid for any temperature. This condition can be reformulated to better illustrate the bottom line: The ampliﬁcation of light through stimulated emission in semiconductors can occur only for photons which arise from radiative transitions between states in the conduction band with the probability of being occupied by electrons larger than 1/2, and states in the valence band with probability of being occupied by electrons lower than 1/2. The corresponding states in the valence band are thus largely occupied by holes, as depicted in Fig. 10.5. This case is in fact an analogy to the case of inversion population in discrete atomic levels shown in Fig. 10.4(a) (N2 > N1 ). One can easily get the basic idea about the spectral dependence of the optical gain by looking at formula (10.12). This dependence is determined in a crucial way by the spectral behaviour of the factor Γ (ν) = f c (E 2 )– f v (E 1 ) and of the joint density of states ρ(ν); the parameter λ20 , or ν −2 , on the other hand, does not inﬂuence the spectral shape of g(ν), as will be shown shortly. Based on (10.15), it is easy to show that Γ (ν) monotonically decreases with ν (i.e. dΓ (ν)/dν < 0, see also Problem 10/3) and intersects zero at hν = E g + Fe + Fh , which is shown in Fig. 10.6(a). The very same ﬁgure also illustrates the well-known square-root shape ρ(ν) ∼ hν − E g and the resulting curve ρ(ν)Γ (ν) (solid circles). The shape of the curve ρ(ν)Γ (ν)ν −2 is also shown for comparison by open circles; this curve denotes the accurate shape of the optical gain g(ν) according to (10.12). The comparison proves that the factor ν −2 in fact does not inﬂuence the shape of the product ρ(ν)Γ (ν) (for hν of the order of 1 eV and for typical widths of gain curves of the order of tens of meV); it can thus be considered constant and g(ν) ∼ = ρ(ν)Γ (ν) can be used as a good approximation. Now, however, we encounter a problem: Experimentally obtained spectral gain shapes in most cases do not copy the symbols-denoted curve in Fig. 10.6(a). Rather, the experimental data can be better ﬁtted using the curve shown as circles in Fig. 10.6(b), which starts with a slow increase of g(ν) near the threshold value hν = Eg . We generated this curve by replacing ad hoc the square-root dependence ρ(ν) ∼ hν − E g by a quadratic dependence ρ(ν) ∼ (hν − E g )2 . We have already met this factor in the previous chapters in the text on band-to-band recombination of electron–hole pairs in an indirect semiconductor, i.e. in the case when the recombination of any electron–hole pair is allowed irrespective of the corresponding wavevectors. This implies that during EHP stimulated emission in a direct semiconductor the quasimomentum conservation law probably is not satisﬁed. We have already come across a similar effect—we mentioned in Subsection 8.5.2 that the emission

Spectral shape of the optical gain

273

Fig. 10.6 (a) Spectral dependence of the Fermi inversion factor Γ (ν), the joint density

of states ρ(ν) ∼

hν − E g , and the

products ρ(ν)Γ (ν) and ρ(ν)Γ (ν)/ν 2 . Curves correspond to direct transitions with the quasi-momentum conservation law ‘on’. (b) The same dependencies as in case (a) but considering the density of states in the form ρ(ν) ∼ (hν − E g )2 . Parameters of the calculation: E g = 1 eV, m e = m h , Fe + Fh = 20 + 20 = 40 meV, T ≈ 60 K.

spectrum of spontaneous EHP luminescence in a direct semiconductor can be well ﬁtted with a mathematical model ignoring the quasi-momentum conservation law. Now, we came to a similar conclusion also for the EHP stimulated emission. If this is really the case, however, we are not allowed to describe the shape of g(ν) simply by substituting ρ(ν) ∼ (hν − E g )2 in (10.12). The proper treatment in this case is to integrate over all suitable pairs of states in the conduction and valence bands. We can exploit formula (8.24) or (8.25), in which, however, the spontaneous-emission occupancy condition f c (E) f v (hν − E) will be replaced by the condition for stimulated emission [ f c (E) − f v (hν − E)]: hν=hν−E g

g(ν)

√ E hν − E f c (E) − f v (hν − E) dE

(10.18)

0 hν=hν−E g

=

√ E hν − E f c (E) + f h (hν − E) − 1 dE.

0

In this relation, the occupancy probability of the corresponding state by a hole is denoted as f h = 1– f v . Figure 10.7 demonstrates the results of a calculation carried out according to (10.18). Panel (a) shows one of the ﬁrst detailed theoretical calculations of

274

Stimulated emission

Fig. 10.7 (a) Optical gain g(ν), or absorption coefﬁcient α(ν), calculated for GaAs within the model of the relaxation of the k-vector, qualitatively described by the relation (10.18). Parameters shown next to the curves stand for the relative level of electrical pumping. Curves are calculated for room temperature. After Stern [11]. (b) EHP optical gain in GaAs (measured using the technique of thin-ﬁlm optical transmission: laser pump and probe) at a bath temperature of TL = 2 K. Points denote experimental data, the solid curve is a theoretical ﬁt considering k-vector relaxation according to (10.18). μ = μe − μh is the plasma chemical potential. After Hildebrand and G¨obel [12].

gain in GaAs by Stern [11]. It is obvious that the overall shape of the curves is in very good accord with the dependence g(ν) ∼ ρ(ν)Γ (ν) in Fig. 10.6(b). In addition, we can easily see that in the absence of pumping, i.e. when the conduction band is empty ( f c (E) = 0), the valence band is completely ﬁlled ( f v (hν − E) = 1) and E g = E g , the gain attains negative values, which means that by applying this approach, we can obtain the onset of the absorption coefﬁcient α(ν) = –g(ν) near the absorption edge. In panel (b) of Fig. 10.7 the theory is compared to experiment, showing nice agreement [12]; see also Appendix G. Before moving on it is useful to take note of one more thing. Figure 10.7(a) depicts not only the shape of the gain curves but also the numerical values of g(ν), which are of the order of hundreds of cm−1 . Up to now in luminescence spectroscopy, we have come across only the shape of spectra in arbitrary units; the optical gain, however, in fact a counterpart of the optical absorption coefﬁcient, can be quantiﬁed and is, in this sense, an exception for us. Nevertheless, in order to carry out a correct calculation of g(ν) values it would be indispensable ﬁrstly to add the squared modulus of the transition matrix element |M|2 to (10.18) and, secondly, to insert a numerical factor in front of the integral, containing, apart from universal constants, also the effective masses of the carriers. This means that in the case of a particular material it would be necessary to take into account the existence of several valence bands (light and heavy holes) and obtain the resulting values of g(ν) via summing over all bands. At the same time, a sufﬁciently accurate calculation of |M|2 for a given band structure represents a problem on its own. Such procedures are, however, beyond the scope of the present textbook and anyone interested in this problem should refer to the specialized literature [13, 14], containing further references.

Spectral shape of the optical gain A simple estimate of at least an order of magnitude of g(ν) according to (10.12) is, on the other hand, within our powers. Considering that the typical densities of states at the band edges (usually expressed in units of cm−3 eV−1 ) attain values of 1017 cm−3 eV−1 , we can approximate the joint density of states to be of the same order ρ(hν) ≈ 1017 cm−3 eV−1 . This implies that ρ(ν) = ρ(hν)d(hν)/dν = hρ(hν) ≈ 4 × 102 cm−3 /s−1 . The optical frequencies are of the order of ν ≈ 1014 Hz and in a direct-bandgap semiconductor τr ≈ 1 ns. As the Fermi inversion factor Γ (ν) = f c (E 2 )– f v (E 1 ) near the extreme of the gain-curve maximum is of the order of unity (see Fig. 10.6), we can approximate Γ (ν) = 1, and relation (10.12) ﬁnally yields g(ν) ≈ 200 cm−1 . This conﬁrms the values of the vertical axis in Fig. 10.7(a), i.e. it shows that the peak values of the optical gain in semiconductors are of the order of 102 –103 cm−1 . Now, let us come back to the model (10.18) ignoring the quasi-momentum conservation law, or, put more simply, the k conservation law. Although, in most cases, the model describes well the optical-gain spectrum, the physical reason underlying its application is not clear. What may cause the k conservation law to be violated? The answer can lie, e.g., in the large number of inhomogeneously distributed electron–hole pairs in an EHP, which distorts the ideal translational symmetry of the lattice and thus violates the k conservation law. A similar effect arises from, as we already know, the presence of impurity atoms, which might in fact be a description closer to reality: semiconductor lasers are based on a p-n junction, which inevitably requires doping. Other explanations include the opinion that, during radiative EHP recombination, the k conservation law is actually being satisﬁed locally, through multiple collisions between electrons and holes. These—or similar—arguments, however, always have their weaknesses. If, for example, the high concentration of electron–hole pairs were the most important reason underlying the relaxation of the k conservation law, the shape of the gain curve would naturally have to depend on the intensity of pumping and, at the transition to the negative values of g(ν), it would have to change to a square-root dependence −g(ν) hν − E g , which is not backed up by experimental observations. If, on the other hand, the doping of the semiconductor is the cause, the mentioned ‘smearing’ of the absorption edge can be explained by the existence of tail states inside the bandgap, but the characteristic shape of the gain curve described by (10.18) should not be observed under optical pumping of high-purity samples, which actually does happen. The applicability of the k-vector relaxation model has thus been a hotly debated topic ever since the beginnings of semiconductor-laser research, see e.g. [15]. Over time, even models respecting the k conservation law were proposed as an explanation of the shape of the gain curve [16]. The currently accepted opinion is that the k conservation law is satisﬁed during EHP radiative recombination, in accordance with the basic laws of quantum physics; the gentle increase of g(ν) close to E g instead of a square-root dependence and the overall asymmetry of the gain curve are believed to be due to two ‘correction’ factors. The ﬁrst one is the so-called ﬁnal state damping in the EHP while the second one is referred to as excitonic enhancement. The ﬁnal state damping can

275

276

Fig. 10.8 EHP optical gain in thin-ﬁlm (60 μm) ZnSe under pulsed laser pumping (Iex = 2 MW/cm2 ), measured by a pump and probe method. The dashed curve represents a theoretical ﬁt, taking into account the k-vector conservation law and including both the ﬁnal state damping and excitonic enhancement. TL = 8 K, effective EHP temperature Tef = 20 K. After Kunz et al. [18].

Stimulated emission be understood as a phenomenon when, once the recombination of an electron with a hole in the EHP is accomplished, one unoccupied state remains among the conduction-band electrons and an electron with higher energy quickly relaxes towards it (while, at the same time, among the holes close to the top of the valence band one state ﬁlled with an electron appears, which leads to an analogous relaxation via rearrangement of holes). Such a relaxation is very fast and, as a result of the uncertainty principle, manifests itself as a spectral broadening of the gain curve. This, however, would lead to a more or less systematic smearing of the curve shown in Fig. 10.6(a). The observed shift of the centre of gravity of the curve towards (μe − μh ) − E g is then the result of excitonic enhancement. Roughly speaking, the excitonic enhancement means that electron–hole pairs with high energy, i.e. close to μ = μe − μh where ﬁlled and empty states are in close neighbourhood, are—at least partially— describing relative circular orbits, which evokes memories of a bound excitonic state [17]. This effect entails an enhancement in EHP luminescence and the relevant gain curves on their high-energy edge. Figure 10.8 then conﬁrms that the above ideas are correct, as it represents an experimentally obtained spectrum of EHP optical gain in ZnSe as well as a theoretical ﬁt taking into account the k conservation law, ﬁnal state damping and excitonic enhancement [18]. The agreement between experiment and theory is once again good; obviously, both the models, i.e. both the k-vector relaxation and the k conservation law, are able to model the experimental curves of gain more than satisfactorily. In this ‘spectral’ sense, the argument about which of the models is the correct one can be viewed more as an academic debate, because the values of the basic ﬁtting parameters of the theoretical gain curves (the density of the plasma entering the ﬁt through μ and the effective plasma temperature) turned out to be practically identical in both approaches. Finally, let us address three more issues: the spectral position of the gain with respect to the maximum of the spontaneous emission band, the behaviour of the gain with varying temperature and—once again—the ν −2 factor in eqn (10.12). As for the spectral position of gain: looking at Fig. 10.5 or even better at Fig. 10.9(a) we can immediately see that the stimulated emission in the EHP is always situated on the longer-wavelength part of the spontaneous emission band, because stimulated emission can occur only for photon energies hν < μe − μh , whereas regarding spontaneous luminescence, even electron– hole pairs with energy higher than μ = μe − μh contribute to the signal. Moreover, the possible onset of optical absorption, e.g. from the absorptionband tail, can negatively inﬂuence the higher-energy side, competing with the stimulated recombination transitions. Corresponding spectra of spontaneous emission and gain are schematically sketched in 10.9(b) and, in addition, the whole situation is very well documented by a series of EHP emission spectra in Fig. 10.3. A word of caution, however, is that in the case of lowdimensional semiconductor structures, the onset of stimulated emission on the longer-wavelength side of the spontaneous emission band is not necessarily the rule. Now, let us move on to the inﬂuence of temperature on optical gain. Most experimental curves shown in this section correspond to low temperatures

Spectral shape of the optical gain

277

Fig. 10.9 (a) EHP radiative recombination with highlighted spontaneous and stimulated transitions, which are separated by the Bernard–Duraffourg EHP (ν) for a semiconductor with parabolic energy bands, condition. (b) Calculated spectra of the optical gain g(ν) and spontaneous emission Isp Fermi energies of Fe = 15 meV, Fh = 11.8 meV and EHP temperature equal to 80 K. The calculation was performed in the same units for both curves in the approximation of k-vector relaxation (10.18) or (8.25). After Lasher and Stern [7].

(2–80 K). As the most important applications of stimulated emission in semiconductors are injection lasers functioning at T = 295 K, the question arises of how the conditions for achieving stimulated emission vary with increasing temperature. The answer to this question is as easy as pie: the conditions worsen. Let us recall that the inevitable condition for light ampliﬁcation by stimulated emission in EHP is a degenerate electron–hole plasma, i.e. a plasma obeying Fermi–Dirac statistics. Speaking more accurately, the plasma chemical potential μ = μe − μh needs to be, according to condition (10.17), larger than the reduced bandwidth, μ > E g .5 The higher the temperature, however, the more difﬁcult it is to fulﬁl this condition, because electrons and holes are thermally excited to higher states, the occupancy of lower states decreases and, consequently, the Fermi levels μe , μh shift towards the middle of the bandgap and their difference is reduced. What is more, thermal quenching of luminescence sets in. Let us formulate a simple mathematical condition for EHP degeneration. The Fermi–Dirac distribution functions can be written in the coordinate systems of the corresponding bands as f c = {exp [(E 2 − E c − Fe ) /kB Tef ] + 1}

−1

f v = {exp [(E v − E 1 − Fh ) /kB Tef ] + 1}

−1

, .

When the temperature Tef is high enough so that both the Fermi energies happen to be situated within the bandgap (i.e. Fe , Fh < 0), and, at the same time, not extremely high so that exp[( E e (h) − Fe (h) )/kB Tef ] 1 applies, 5 This, however, does not necessarily mean that both the Fermi levels need to be situated within the corresponding bands, as is the case, e.g., in Figs 10.4 or 10.5—just a single Fermi level sufﬁces to be immersed within a band. This is a common situation for achieving optical gain in GaAs: μe is situated in the conduction band (Fe > 0) while μh lies inside the bandgap (Fh < 0). The underlying reason for this situation is that in GaAs m h (∼ 0.52m 0 ) m e (∼ 0.067m 0 ) holds. See also Problem 10/4.

278

Stimulated emission Fermi–Dirac statistics are transformed into Maxwell–Boltzmann statistics and the Bernard–Duraffourg condition does not make sense any more; it cannot be employed (E e = E 2 –E c , E h = E v –E 1 are the energies of carriers inside the bands). Since the energies E e , E h are of the order of kB Tef , the condition for a transition of the EHP from quantum statistics (degenerate gas) to classical statistics (non-degenerate gas) reads exp (−Fe (h) /kB Tef ) 1.

(10.19)

Finally, as regards the ν −2 factor in eqn (10.12), although it does not inﬂuence the shape of the g(ν) curve, as was shown in Fig. 10.6, it deﬁnitely enhances its magnitude. This effect is more pronounced at low frequencies, which can be considered one of the reasons why the very ﬁrst laboratory semiconductor lasers generated long-wavelength radiation in the near-infrared spectral region (> 800 nm) and, moreover in accordance with the preceding discussion, solely at low temperatures (∼ 80 K). It was not until the concept of semiconductor heterostructures that the problem of laser action at room temperature was successfully solved.

10.4 Stimulated emission in an indirect-bandgap semiconductor Up to now, we have been discussing optical gain and stimulated emission in direct-bandgap semiconductors only. Can we, however, eliminate a priori indirect-bandgap semiconductors from this discussion? Naturally, we know that their radiative lifetime τr is by several orders of magnitude longer than in direct-bandgap materials and, accordingly, we would expect the optical gain to scale to lower values, in conformity with relation (10.12). This does not necessarily imply, however, that a (at least very low) positive optical gain coefﬁcient cannot in principle occur in indirect-bandgap semiconductors. By the way, the peak value of the optical gain in ruby (optical transitions in a Cr3+ ion) is very low, about 0.2 cm−1 only at the typical concentration of Cr3+ ions of 1019 cm−3 . In spite of this, the ruby laser was the very ﬁrst realized laser type and in some laboratories is still being used. In indirect-bandgap semiconductors, or at least in the most common materials such as silicon and germanium, there is another obstacle that needs to be overcome in order to achieve stimulated emission, namely, free carrier absorption (FCA). Before we start a detailed discussion of stimulated emission in an indirect-bandgap semiconductor, let us concisely recall the basics of FCA. In an ideal pure semiconductor at T = 0 K the conduction band is empty and the valence band is ﬁlled with electrons. If, however, free electrons are introduced into the minimum of the conduction band by any means, photons of electromagnetic radiation can be absorbed and the excess energy can be exploited for transferring these electrons to allowed higher lying states in the very same band (this type of absorption is thus not restricted to energies given by the well-known condition hν > E g ; it can occur even at lower photon energies).

Stimulated emission in an indirect-bandgap semiconductor

279

A quantitative description of free carrier absorption can be most easily given in the framework of the classical Drude model. If a free electron gas with the free electron concentration N0 , mass m 0 and a relaxation time τ (in the simplest solid-state approximation it can be the mean time between collisions of the electron with either the lattice, i.e. phonons, or impurities) is inserted into a ﬁeld of optical radiation at the frequency ν, the imaginary part of the dielectric constant ε2 is described by the relation [19] ε2 (ν) ≈

2πε∞ νp2 ντ (4π2 ν 2 + 1/τ 2 )

,

(10.20)

where ε∞ is the high-frequency (real) dielectric constant and νp2 = N0 e2 / 4π2 ε0 ε∞ m 0 is the plasma frequency νp squared. In the visible or near-infrared spectral regions, for semiconductors ν 1/2πτ holds and (10.20) is reduced to ε2 (ν) ≈ ε∞ νp2 /2πν 3 τ . The absorption coefﬁcient αFCA (ν) as a function of frequency ν then reads αFCA (ν) =

2πν N0 ε2 (ν) ≈ 2 ≈ N0 λ2 . c n(ν) ν

(10.21)

This implies that free carrier absorption is of a non-resonant character and rises monotonically with wavelength λ (in (10.21) c stands for the light velocity in vacuum and n(ν) is the refractive index, whose dependence on frequency is quite weak). Possible deviations in (10.21) in wavelength power from the value of two, which are sometimes observed in certain materials, can be due to variations of τ as a function of ν. The absorption cross-section of free carriers σFCA , a material constant, is then introduced by the relation αFCA = σFCA N0 .6 . It is of the order of σFCA = 10−18 − 10−17 cm2 . The absorption of radiation in a system of free electrons residing in the conduction band minimum is schematically sketched in Fig. 10.10(a); an analogous mirror scheme applies for holes in the valence band. The fact that one deals with an intraband type of absorption is evident. An important piece of information stemming from Fig. 10.10(a) is the non-verticality of the transition, which signiﬁes that a phonon h¯ ω has to take part in the process apart from a photon hν (and an electron or a hole, of course) in order to compensate for the change in quasi-momentum h¯ k (alternatively, relaxation of the quasi-momentum conservation law might occur as a result of the presence of impurities).7 From the point of view of perturbation theory, these processes are of second order, which will shortly turn out to be very important. The importance of free carrier absorption for lasing in semiconductors becomes clearer if we realize that the absorption transitions in Fig. 10.10(a) coexist with the radiative recombination of electrons and holes across the bandgap. This scenario is shown in Fig. 10.10(b). We can immediately notice that generated photons hν = E 2 –E 1 can be in no time (re)absorbed by free electrons and holes in the corresponding bands without ever leaving the 6 When an electron–hole plasma is present in the semiconductor, N denotes the concentration 0 of electron–hole pairs. 7 This implies that free carrier absorption is not allowed in vacuum.

Fig. 10.10 (a) Illustrating the absorption of photons hν on free EHP electrons in the minimum of the conduction band; the electrons are raised to free states above the Fermi level. A change in quasi-momentum h¯ k needs to be compensated for. (b) A process when radiative EHP recombination across the bandgap takes place and resulting luminescence photons are reabsorbed by free carriers. Only low temperatures are considered, with the optical transition being accompanied by the emission of a phonon ω.

280

Stimulated emission material. The corresponding absorption coefﬁcient αFCA (ν) will then compete with the optical gain g(ν) and as long as the former is high enough, the difference G(ν) = g(ν) − αFCA (ν)

(10.22)

becomes negative. According to the Lambert–Beer law, the generated luminescence will thus be attenuated instead of being enhanced via stimulated emission. This process will prevent the material from becoming an active medium for a semiconductor laser. The quantity G(ν) deﬁned by relation (10.22) can be referred to as the ‘net’ optical gain; additional subtle distinctions will be mentioned in Subsection 10.6.1. To be more speciﬁc, the situation in two typical examples of direct (GaAs) and indirect (Si) semiconductors is compared in Fig. 10.11. The radiative recombination in GaAs (even though some doubts were discussed in the preceding section) occurs via direct transitions, whereas the free carrier absorption is due to, as was emphasized above, indirect transitions, i.e. due a secondorder process. In Si, on the other hand, both these transitions are indirect, conditioned by phonon participation, and thus their rates will be comparable. This fundamental difference when it comes to laser action was pointed out for the ﬁrst time by Dumke in 1962 [20] and the values of g(ν) and αFCA (ν), calculated based on his theory, are quoted in Fig. 10.11 for T = 4 K. In GaAs at photon energies hν ≈ E g ≈ 1.5 eV we get g(ν) αFCA (ν) and the inﬂuence of free carrier absorption is thus negligible, resulting in G(ν) ≈ g(ν) > 0. On the other hand, in Si for hν ≈ E g ≈ 1.1 eV one gets g(ν) smaller than αFCA (ν) by about an order of magnitude, i.e. G(ν) < 0. Let us point out that this fact is not obvious a priori; it is determined by the band structure of a particular semiconductor and only a detailed calculation or an experiment can decide.8 Similarly, the calculation yields G < 0 for germanium, which implies that neither Si nor Ge can be exploited for the construction of a semiconductor

Fig. 10.11 Competition between the optical gain g and free carrier absorption, characterized by the absorption coefﬁcient αFCA , for (a) GaAs and (b) Si. The coefﬁcients g and αFCA were calculated according to theoretical work [20] for pumping levels giving rise to an EHP with the density of e–h pairs N = 1018 cm−3 and for T ≈ 4 K.

8 For example in Al Ga x 1−x As, which is an indirect-bandgap semiconductor for x ≥ 0.44, the occurrence of stimulated emission was proved experimentally by Kalt, H., Smirl, A. L., and Boggess, T. F. (1989). J. Appl. Phys., 65, 294.

Stimulated emission in an indirect-bandgap semiconductor laser operating via electronic transitions across the bandgap at low temperatures. This signiﬁes, however, that laser action is even less probable at room temperature, when the conditions for achieving optical gain, as we already know, generally worsen and, besides, the luminescence quantum yield in both Si and Ge is extremely low, η ≈ 10−6 . Up to now, no experiment has cast doubts on the results of these calculations. This conclusion about silicon not being suitable as a laser medium puts severe restrictions on the application potential of this material, which otherwise represents the cornerstone of nearly all present-day microelectronics. A large number of authors therefore tried to circumvent this situation by applying more or less sophisticated approaches. For example Rediker [21] ﬁled a patent for an electrically pumped injection laser based on a p-n junction in an indirect semiconductor, with the bottom line being the introduction of a pulsed phonon ‘avalanche’ into the junction just at the moment when sufﬁciently high population inversion is reached. These phonons should have caused a fast radiative electron ‘sweeping down’ across the bandgap, presumably accompanied with emission of a laser pulse (the principle was thus very like the generation of giant pulses, commonly exploited in optically pumped lasers). The idea was never experimentally realized, though. Recently Trupke et al. [22] theoretically analysed Dumke’s calculations and concluded that in the case of indirect-bandgap semiconductors Dumke [20] underestimated the possibility of radiative recombination accompanied with the absorption of phonons, which in principle could help to overcome the losses caused by free carrier absorption. Up to now, however, the idea has not met with a positive response, and all functional injection lasers are still based on III-V direct-bandgap semiconductors such as GaAs. The issue of a silicon laser still remains open and is hotly debated, though, mostly due to the intense development of so-called silicon photonics, which will be treated in more detail in Chapter 15. Recently, a very interesting idea of how to attain direct radiative recombination in germanium has been proposed [23]. It is based on the fact that the absolute minimum of the conduction band at L + 6 is not excessively deep (Fig. 10.12). If this minimum were fully ﬁlled with electrons from ionized donors, under optical or electrical pumping the excess non-equilibrium electrons in the conduction band would prefer fast scattering to the 7− minimum, and radiative recombination with a hole via 7− → 8+ direct transitions, or even laser action, would follow. Obviously, a high level of doping with donors is required. If, at the same time, a suitable mechanical deformation is applied in order to reduce the number of equivalent minima at the L point, estimates show that the necessary doping level would still be realistic—around 8×1019 cm−3 . The question of whether an analogous approach is feasible in silicon is left for the reader to answer (Problem 10/5).9

9 Optically pumped lasing in germanium at room temperature, based on this scheme, has recently been achieved (Liu, J., Sun, X., Camacho-Aguilera, R., Kimerling, L. C., and Michel, J. (2010). Optics Letters, 35, 679).

281

Fig. 10.12 Part of the band structure of germanium, demonstrating how to realize direct radiative recombination and lasing.

282

Stimulated emission

10.5 Participation of excitons in stimulated emission So far, stimulated emission has been discussed with regard to the high-density system of free electrons and holes, namely, the electron–hole plasma EHP. In the previous chapters of this book, however, the luminescence of bound electron–hole pairs, excitons, has been widely covered. It is thus only logical to ask if and how stimulated emission can occur in various radiative recombination processes involving excitons, or their complexes. We will focus here on semiconductors with direct bandgap and, most importantly, we will show that luminescence arising from the recombination of a system containing solely free excitons (i.e. without the participation of other quasi-particles) cannot be ampliﬁed through stimulated emission; if LO-phonons (radiative A–LO or X–LO recombination) are present, however, stimulated emission can be achieved. In addition, we will also explain that stimulated emission can occur in the luminescence accompanying collisions of free excitons (X–X collisions) and during the radiative decay of excitonic molecules (EMs). These effects, however, are usually related to low temperatures without a direct application potential for optoelectronic components. In order to simply but adequately describe stimulated emission in a system of free excitons (hν ≈ E g –E X , Fig 10.13(a)) we will apply, like in the previous chapters of this book, kinetic equations [24]. For this purpose, they need to contain explicitly the intensity of generated radiation; this can be achieved

Fig. 10.13 Schematic of radiative decay of (a) a free exciton–polariton, (b) a free exciton with the emission of an LO-phonon, and (c) a biexciton or an excitonic molecule. Arrows directed upwards illustrate reabsorption. In contrast to (a), in (b) and (c) ampliﬁcation by stimulated emission can occur. The similarity of (a) to a two-level atomic system, or (b) and (c) to a three-level atomic system is conspicuous. It is well known that whereas the three-level system (e.g. Cr3+ in sapphire, i.e. ruby) makes lasing possible, a two-level system does not. Such an analogy, however, has to be viewed with caution, because the lower level |1 denotes the ground state of the entire crystal, which makes it difﬁcult to deﬁne the concept of population inversion.

Participation of excitons in stimulated emission by employing the number of photons n f . The overall number of excitons (generated in the system under investigation e.g. via optical pumping), which are allowed to recombine radiatively, satisfying quasi-momentum conservation and emitting a photon to a given mode of the electromagnetic ﬁeld, will be denoted as NX . If τr stands for the exciton radiative lifetime, the rate of increase in the number of photons in the given electromagnetic mode through spontaneous emission is equal to NX /τr . Stimulated emission, taking place in parallel, contributes to the increase in the number of photons by n f NX /τr and the overall rate of photon generation will then read NX (n f + 1). τr

(10.23a)

These photons, however, undergo resonant reabsorption, as was mentioned in Subsection 7.1.2. The important thing now is that both excitons and photons are bosons and the roles they play can be considered symmetric (i.e. we are not restricted by the Pauli exclusion principle imposing constraints on the occupancy of levels, see e.g. the occupancy condition in (10.9) or (10.10)). This fact can also be rephrased as ‘the absorption of a photon is accompanied by both stimulated and spontaneous emission of an exciton’ and the corresponding term in the kinetic equations can be derived from (10.23a) by interchanging NX and n f : nf − (NX + 1). (10.23b) τr Finally, some photons have to leave the investigated sample (or laser resonator) so that we could obtain a measurable luminescence signal, which can be described with a loss coefﬁcient γ and a term −γ n f .

(10.23c)

All in all, the kinetic equation for photons then contains all three terms (10.23a), (10.23b), and (10.23c): 1 dn f 1 = NX (n f + 1) − n f (NX + 1) − γ n f dt τr τr =

1 (NX − n f ) − γ n f . τr

(10.24)

This brings us to an important conclusion: as the number of photons on the right-hand side of (10.24) stands with a negative sign, the number of photons in a given mode cannot grow in time, i.e. ampliﬁcation of free exciton luminescence via stimulated emission cannot occur. This fact was recognized both experimentally and theoretically in the early 1960s in connection with the very ﬁrst luminescence experiments in semiconductors under high pumping. This conclusion is in fact not very surprising if we recall the previous discussion on polaritons in Chapter 7; in this sense, excitons and photons can also be seen as a system of bound oscillators. In other types of radiative decay of excitons—i.e. those involving another quasi-particle—stimulated emission, on the other hand, can occur. Let us

283

284

Stimulated emission consider the radiative annihilation of an exciton accompanied by the emission of an LO-phonon (X–LO, see Subsection 7.1.3). The approximate energy of the emitted photons derives from the energy conservation law and amounts to hν ∼ = E g − E X − h¯ ωLO , where E X is the exciton binding energy and h¯ ωLO is the LO-phonon energy, see also Fig. 10.13(b). The key here is that the energy of the luminescence photon is now lower by h¯ ωLO with respect to the exciton energy, which prevents reabsorption-related losses (at low temperatures, when the phonon population is negligible). Let us keep denoting by n f the number of photons. Then n q will stand for the number of phonons with wavevector q, and Nq for the number of excitons with the same wavevector (or, more accurately speaking, these are always mean occupation numbers in the given state or mode). We know that excitons with any value of q can participate in the process, since their quasi-momentum q is taken on by phonons. Therefore, the overall number of initial states contributing to the radiative process is much larger than in the preceding case of simple excitonic recombination, which is an additional factor facilitating the onset of stimulated emission. Let the overall number of excitons be NX , Nq . implying NX = q

As photons, phonons and excitons are bosons, the rate of their generation is proportional to their numbers increased by unity: (n f + 1), (n q + 1) and (Nq + 1). The rate of annihilation, on the other hand, is proportional only to their numbers: n f , n q and Nq . The contribution of relevant terms to the kinetic equation will thus read: • The rate of generation of photons (emitted together with phonons) Cq Nq (n f + 1)(n q + 1), where Cq > 0 is the corresponding rate constant. • The rate of losses due to an inverse process Cq (Nq + 1)n f n q . • Losses caused by the escape of photons from the sample (resonator) −γLO n f . Hence, the kinetic equation for the number of photons reads dn f Cq Nq (n f + n q + 1) − n f n q . = −γLO n f + dt q

(10.25)

This equation can be simpliﬁed provided the excitonic gas is in thermal equilibrium and can be described by a thermal distribution Nq = NX f q (T );10

10 If we assume, for the sake of simplicity, the effective gas temperature to be equal to the lattice temperature T , it follows for low temperatures and not too high densities of exci-

Participation of excitons in stimulated emission further, at low temperatures we can approximate exp(h¯ ωLO /kB T ) 1 and thus it follows from (4.6) that n q ≈ exp(−h¯ ωLO /kB T ) 1, n q Nq . Equation (10.25) then takes on the form dn f = −γLO n f + Cq NX f q (n f + 1) − n f n q dt q where β =

≈ −γLO n f + β NX (n f + 1),

(10.26)

Cq f q . Now it is obvious that ampliﬁcation of luminescence by

q

stimulated emission is possible. Whether it occurs or not depends on which one of the factors on the right-hand side of eqn (10.26) prevails. Conditions supporting stimulated emission may be achieved through maximizing the positive-sign term comprising the number of photons, i.e. through sufﬁciently high excitation (maximizing NX ) and under fast radiative recombination (maximizing β). A similar approach can conﬁrm that stimulated emission can inﬂuence a number of other luminescence processes: Luminescence of free excitons with emission of multiple phonons, collisions of free excitons (X–X), collisions of free exciton–electrons or free exciton–holes, annihilation of free excitons accompanied by emission of plasmons and, most of all, the radiative decay of an excitonic molecule (EM) into a photon and a free exciton, see Fig. 10.13(c). In all these cases, the decrease in energy of a luminescence photon by the energy of a participating quasi-particle (phonon, free carriers, plasmon, recoil exciton) prevents photons from being reabsorbed and, moreover, makes it possible for the whole excitonic population to take part in the radiative recombination. Let us now attempt to estimate the spectral shape of the optical-gain curve G LO (hν) in the process of X–LO luminescence. In analogy between the system of free excitons and an atomic gas this process can be viewed (Fig. 10.13(b)) as a (quasi-)atomic process, in which the shape of the gain g LO (hν) is determined by the shape of the corresponding (spontaneous) spectral line. In the case of X–LO luminescence, the spontaneous emission lineshape is described by relation (7.12) hν − E 0 LO LO 3/2 ∼ ∼ , (10.27) Isp (hν) = g (hν) = NX (hν − E 0 ) exp − kB T where E 0 = (E g − E X ) − h¯ ωLO and, moreover, now the overall number of excitons NX has been added as a coefﬁcient. The reason is that this expression needs to be compared to a competing reabsorption process, which increases proportionally to the occupancy number of phonons n q ∼ exp(−h¯ ωLO /kB T )

tons that f q (T ) (kB T )−3/2 exp(−h¯ 2 q 2 /2m exc kB T ), i.e. the Boltzmann distribution can be employed.

285

286

Stimulated emission at the level |2, Fig. 10.13(b). The rate of these absorption processes will, in addition to that, be proportional to the relevant joint density of states, which can be considered here to be represented by the term (hν − E 0 )3/2 , and the expression for the absorption coefﬁcient thus reads α LO (hν) ≈ (hν − E 0 )3/2 n q .

(10.28)

The net gain coefﬁcient can then be obtained as the difference between (10.27) and (10.28), yielding G LO (hν) = g LO (hν)−α LO (hν) hν−E 0 ≈ ANX (hν−E 0 )3/2 exp − −B(hν − E 0 )3/2 n q kB T hν−E 0 hν−E 0 3/2 1 − η exp , (10.29) = ANX (hν−E 0 ) exp − kB T kB T where A, B are constants independent of photon energy hν and η = Bnq /ANX . A more theoretically detailed calculation [25] yields a very similar formula. One can easily see from (10.29) that at low temperatures, when n q → 0, the gain coefﬁcient will be positive G LO (hν) > 0; with rising temperature, however, η rapidly grows and the term in the last bracket will quickly acquire a negative value. The reader can show, by employing analogous reasoning, that the gain coefﬁcient in the process of EM radiative decay can be written down in the form of (Problem 10/6) G EM (hν) ≈ A NXX (E 0 − hν)1/2 E 0 − hν E 0 − hν exp − 1 − η exp − , (10.30) kB T kB T

Fig. 10.14 Optical gain in EM luminescence: experimental (solid line) and theoretical (dashed line) gain curves, the latter being calculated using relation (10-30), in thin-ﬁlm ZnO. The letter M denotes the position of the high-energy edge of the spontaneous emission line E 0 = E g − E X − E B . Effective temperature of the gas of excitons and excitonic molecules as one of the ﬁtting parameters yields Tef = 39 K, bath temperature was T = 1.8 K, excitation was carried out with a pulsed N2 laser (337 nm). After Hvam [28].

where A and B are again constants, NXX is the number of excitonic molecules, E 0 = E g –E X –E B and η = (B /A )(NX /NXX ); E X and E B stand for the binding energy of an exciton and an excitonic molecule, respectively (Subsection 8.2.1). Anyone interested in more details about relation (10.30) is referred to the literature [26, 27]. One more thing to bear in mind is that, even though for the sake of simplicity thermal equilibrium of all the quasiparticles with the lattice was assumed, in reality T in (10.29) and (10.30) denotes the effective temperature of the excitonic or biexcitonic gas, which is always higher than the lattice temperature. Figures 10.14 and 10.15 demonstrate the above discussion. Figure 10.14 shows both the experimentally obtained and theoretically calculated (using eqn (10.30)) shape of the excitonic-molecule gain in ZnO [28]. It is obvious that the gain shape keeps the typical asymmetry of the spontaneous EM emission line (Subsection 8.2.1): a tail extended towards lower photon energies. The high-energy edge of the gain curve is simultaneously shifted towards lower energies with respect to the edge of spontaneous emission E 0 = E g –E X –E B .

Experimental techniques for measuring the optical gain This shift is due to a process in which high-energy photons are those which are most strongly reabsorbed; this is quantitatively described by the coefﬁcient η in (10.30). Similarly to EHP stimulated emission, the gain curve is thus situated on the long-wavelength side of the spontaneous emission line. This red-shift is easily discernible in Fig. 10.15, where one can immediately compare the spectrum of spontaneous emission (a) with the gain curve (shaded area in (b)) in thin-ﬁlm ZnS [29]. While the spontaneous EM luminescence in (a) peaks at ∼ 3.785 eV, the corresponding gain attains its maximum value at ∼ 3.781 eV. Also, there is one more feature which makes this ﬁgure interesting: it contains optical-gain features due to two other mechanisms of radiative exciton recombination. The ﬁrst one is gain at the line of free exciton collisions X–X, which was already mentioned in this section, and in addition to that, gain at the line of a bound exciton D0 –X is present. The latter mechanism of optical gain has not yet been mentioned; its existence is not at all surprising, though. An exciton bound at an impurity atom or ion is, as we already know, a synonym for an excited electronic state of such an atom. In principle, a similar laser mechanism is encountered, e.g., in a ruby or neodymium laser (even if the differences, e.g. in the concentration of impurities or the strength of their interaction with the lattice–matrix, may be substantial). Now, let us move on to experimental techniques which yield the spectra of optical gain, shown, e.g., in Figs 10.14, 10.15 and other in Sections 10.3 and 10.5.

10.6 Experimental techniques for measuring the optical gain At the beginning of this chapter, the experimental manifestation of the optical gain in luminescence experiments was discussed mostly as a phenomenon slightly difﬁcult to control, which can (but not necessarily) appear accidentally under conditions of strong excitation. The availability of an experimental method which is focused intentionally on conﬁrming the presence of stimulated emission and enabling the value of the optical gain to be quantiﬁed is certainly desirable. We will now focus on two such methods: the so-called variable stripe length (VSL) method and a pump and probe (P&P) method. Both of these techniques are based on a direct measurement of the ampliﬁcation of a weak probe beam propagating through an optically pumped sample of the material under study. The most signiﬁcant difference between these two methods lies in the origin of the probe beam.

10.6.1 Variable stripe length (VSL) technique This method is in principle a photoluminescence method: the spontaneous emission itself, coming from an optically excited area of the sample, is exploited as the probe beam; the excited spot has the shape of a thin stripe of small width t. Such a shape can be obtained by focusing a pumping laser beam with a cylindrical lens. This method was introduced in the early 1970s by Shaklee et al. [30, 31] and its principle is depicted in Fig. 10.16. The length of

287

Fig. 10.15 (a) Spontaneous emission and (b) spectral shape of net optical gain in thin-ﬁlm epitaxially grown ZnS on a GaAs substrate. The optical gain contains three contributions: from the luminescence of a bound exciton (D0 –X), excitonic molecule (EM) and free exciton collisions (X–X). Circles represent the theoretical shape of the gain, calculated for EM according to relation (10.30). Effective temperature of the gas of excitons and excitonic molecules was Tef = 36 K, bath temperature T ≈ 5 K, excitation was carried out with a pulsed laser (308 nm; 4.02 eV). After Valenta et al. [29].

288

Stimulated emission

Fig. 10.16 (a) Schematic of the VSL method for measuring optical gain in a stripe characterized by length l and width t. (b) Typical experimental setup. After Shaklee et al. [31], reproduced courtesy of Elsevier.

the excitation stripe l varies in a deﬁned way during the measurement (utilizing an adjustable slit or a shifting razor blade) and, at the same time, the radiation emanating from the edge of the sample in the direction of the axis of the stripe is detected, i.e. the measured signal corresponds to ampliﬁed spontaneous emission (ASE). Provided its intensity scales with increasing stripe length l superlinearly, the ampliﬁcation of the (spontaneous) emission actually occurs through stimulated emission, i.e. net optical gain is present.11 Before we point out the characteristic features (and also some drawbacks) of this method, the whole process will be described quantitatively provided the stripe can be considered inﬁnitely narrow (l t) and thus treated as a onedimensional object in the direction of the x axis. Spontaneous luminescence radiation arising in the stripe is emitted randomly in all directions and the spontaneous photons can initiate acts of stimulated emission along the x axis, which is then monitored by recording the output intensity of radiation IASE from the edge of the sample. The excited stripe thus serves (provided that sufﬁciently high population inversion was reached) as a single-passage ampliﬁer12 for photons travelling along the x axis. Consequently, the net gain G(ν) can be deﬁned as a relative change in the intensity of radiation I (x, ν) on an inﬁnitesimal path element dx: G(ν) = [g(ν) − K (ν)] =

dI (x, ν) 1 . dx I (x, ν)

(10.31)

11 Referring to Section 2.1, this experimental set-up can be viewed as a special case of a ‘reﬂection’ arrangement under an angle of 90◦ . The sample needs to have both its excitation area together with its output edge polished, or it should be prepared as a thin ﬁlm on a similarly treated substrate. 12 Generally speaking, such a device is not a common laser (laser oscillator), because the positive feedback, in a laser realized by inserting the active medium into a resonator, is intentionally left out. The ampliﬁcation of spontaneous emission is also often classiﬁed as lasing without mirrors.

Experimental techniques for measuring the optical gain The coefﬁcient K (ν) now describes all the losses that in a real material act against ampliﬁcation, i.e. not only the free carrier absorption as in (10.22), but also the absorption on residual impurities, light scattering on possible inhomogeneities of the sample, etc. The overall increase in the detected intensity dIASE (x, ν), related to the increase in the stripe length dx, is then dIASE (x, ν) = G(ν)IASE (x, ν) dx + Isp (ν) dx;

(10.32)

as compared with relation (10.31), the term Isp (ν)dx, originating from (nonampliﬁed) spontaneous emission, has been added to this equation. The quantity Isp (ν) thus stands for the intensity of spontaneous emission coming from unit length of the stripe and being independent of x; the latter is also presumed to be a property of the gain coefﬁcient G(ν). By solving (10.32)—an inhomogeneous linear differential equation—we obtain the intensity IASE (l, ν) coming out of the stripe. The general solution of the corresponding homogeneous equation (when putting Isp (ν) = 0) is simple and yields IASE (l, ν) = const × exp(Gl), the application of the initial condition IASE (l = 0, ν) = 0 implying const = 0. Thus, in order to solve the equation, one has no choice but to ﬁnd the particular solution with a ‘non-zero right-hand side’ Isp (ν) = 0 and the variation of constants method [32] leads to the solution ⎡ l ⎤ l ⎣ ⎦ IASE (l, ν) = Isp (ν) exp −G(ν)dx dx exp G(ν)dx 0

=

Isp (ν) G(ν)l (e − 1). G(ν)

0

(10.33)

Consequently, by measuring the dependence of IASE on l and by subsequently ﬁtting this dependence using relation (10.33) we obtain values of the gain coefﬁcient G(ν) as a ﬁtting parameter for chosen wavelengths λ(= c/ν). It is also possible to retrieve the overall spectral proﬁle of the gain by measuring, for two particular stripe lengths l1 and l2 = 2l1 , relevant emission spectra and dividing them. For this case, we can get from (10.33) IASE (l2 , ν) 1 −1 . (10.34) G(ν) = ln l1 IASE (l1 , ν) From the terminological point of view, it is useful to comment on the net gain coefﬁcient here. A waveguiding effect can be present in the sample as a result of either intentional preparation of the sample in the form of a planar (or any other) waveguide, or because of an increase in the refractive index within the area of the stripe due to the high concentration of photoexcited carriers that may occur. Under such circumstances, it is necessary to take into account the mode conﬁnement factor ΓM , deﬁned as the fraction of the radiant power conﬁned in the core of the waveguide (0 < ΓM < 1, ΓM = 0.8–0.9 in highquality waveguides). Instead of the term ‘net gain’, G(ν) is then referred to as the modal gain, g(ν) is called the material gain and one can write down G(ν) ≡ G modal = ΓM g(ν) − K (ν).

(10.35)

289

290

Stimulated emission

Fig. 10.17 (a) GaN at T = 2 K: dependence of IASE (hν = 3.458 eV) on the stripe length l in a log–lin scale. The gain G(ν) can be determined from the slope of the linear parts of the curves. The values of G(ν) and of the excitation intensity (a pulsed N2 -laser) are shown at each curve. (b) GaN at T = 2 K: development of the emission spectrum IASE (l, ν) with increasing stripe length at an excitation intensity of 1.25 MW/cm2 . The emission originates in radiative EHP recombination. After Dingle et al. [33]. (c) CdS at T = 2 K: intensity dependence of IASE (hν = 2.527 eV) at a constant stripe length l = 500 μm. Different symbols denote different samples. In this case, gain occurs at the P-line (X–X collisions). After Shaklee and Leheny [30].

One of the very ﬁrst applications of the VSL method is depicted in Fig 10.17 [30, 33]. There is one more aspect which makes this ﬁgure noteworthy: it dates back to as long ago as 1971 when it demonstrated an exceptionally high optical gain in GaN. Although this demonstration singled out GaN as an ideal material to serve as an active medium in an injection laser, it took 30 more years before an InGaN-based laser was put on the market. The journey from basic research to commercially available application output is not necessarily straightforward and various obstacles of technological problems might be encountered on the way. The story of the ‘blue’ GaN-based laser is summarized in a monograph [34]. In addition to that, one more thing catches the eye in Fig. 10.17(a). The ﬁtted curves determined by (10.33)—dashed lines—systematically deviate from experimental dependencies (solid lines) upon exceeding a certain critical stripe length lc , which gets shorter with increasing excitation intensity. This effect is due to gain saturation, a phenomenon well-known from laser physics: at high photon densities, the rapid onset of stimulated emission is quickly depleted, which, in this case, leads to only a linear increase in IASE with increasing l

Experimental techniques for measuring the optical gain for l > lc .13 The saturation effect is not included in the assumptions applied when deriving (10.33) and the occurrence of the saturation deviation in the VSL curve such as that in Fig. 10.17(a) can be considered another proof supporting the onset of stimulated emission. Frequently, an abrupt increase in the slope of the intensity dependence of IASE (l, ν) at a constant stripe length l (Fig. 10.17(c)), and a corresponding narrowing of the emission spectrum, are also viewed as additional supporting arguments. As for the narrowing, however, it does not have to be necessarily evident in every sample (we should not forget that resonator feedback is not employed); it can be missing, e.g. if the luminescence originates in the EHP or if several parallel emission mechanisms take place. Moreover, what deﬁnitely cannot be left out and what is of fundamental importance in evaluating spectral narrowing here is a careful determination of the zero-signal level. Nevertheless, it is obvious this method works ﬂawlessly for high values of the gain G(ν). If G(ν)l ≥ 2.5, then exp(G(ν)l) 1, the IASE intensity rises purely exponentially with increasing l and the occurrence of stimulated emission cannot be doubted. The reliability of VSL, however, gets worse at low net gain values. This can be simply deduced from the fact that at | G | l1 the exponential factor can be approximated as exp(Gl) ≈ 1 + Gl and from (10.33) it follows that IASE (l, ν) ≈ Isp (ν)l. The emission intensity scales only linearly with increasing l and, consequently, the method is unable to distinguish small positive gain (G > 0) from weak attenuation (G < 0). Generally, already on condition that Gl ≈ 1, a large number of experimental parameters can negatively inﬂuence the measurement, which did not have to be considered up to now: (a) Finite stripe width t; if it is too large, the one-dimensional approximation (10.33) is no longer valid. (Widths below approximately 10–20 μm cannot commonly be achieved, without employing specialized equipment, however.) (b) Constant pump intensity along the whole stripe length. From this point of view, what appears to be ideal in the VSL method is the application of lasers or excitation sources with a rectangular beam proﬁle and uniformly distributed pump energy density over the entire beam cross-section (N2 -laser 337 nm, XeCl excimer laser 308 nm). Such a beam is transformed into a stripe of constant t and constant excitation intensity over the whole length l via focusing by means of a cylindrical lens (Fig. 10.16(b)). If other types of lasers are exploited (with a Gaussian beam proﬁle), only a small central part of the beam needs to be selected, using, e.g., an expander. (c) Constant efﬁciency of coupling of the IASE emission to the monochromator, or the detector, from any part of the stripe. (d) Diffraction of the pump beam on the slit or a razor blade, limiting the utilizable stripe length.

13 For l ≤ l , the term ‘small-signal gain coefﬁcient’ is sometimes used. c

291

292

Stimulated emission Unsuitably chosen parameters (a) through (c) or diffraction effects can lead to experimental artefacts (artiﬁcial nonlinear IASE growth), which can be mistakenly interpreted as the manifestation of stimulated emission. Can this be prevented? Yes, to a certain extent, and the corresponding instructions on how to do it can be found in [35, 36]. Let us start with a short overview of diffraction effects, which are inevitably present, but whose inﬂuence can be minimized by choosing a suitable imaging system between the cylindrical lens and the sample. As a rule, the imaging system is usually chosen so that it geometrically reduces the length of the stripe 2–3 times with regard to its length in the focal plane of the cylindrical lens, where the slit is inserted (Fig. 10.16(b)). This reduces correspondingly the overall length of the diffraction area as against the case when the slit is positioned directly on the sample surface. In addition, the diffraction pattern can be easily detected directly during the experiment by collecting, together with the IASE emission, the scattered pump radiation for every ﬁxed stripe length l. The relevant part at the beginning of the stripe with a distinctive diffraction pattern will then be excluded from analysis of the experiment, see Fig. 10.18 [37]. Now, let us focus on item (c) from the list, i.e. the coupling of the emission from the stripe to the detector. In principle, two undesirable effects can cause the signal to be collected preferentially from a certain spot or area of the excited stripe. They are the waveguiding effect and the confocal effect. Firstly, the waveguiding effect can occur in samples in which the luminescence stripe is excited in the core of a planar, or any other type of waveguide, having a primarily positive inﬂuence on the ampliﬁcation of spontaneous emission. On the other hand, both guided and substrate modes can leave the edge of the sample under particular angles, see Fig. 10.19(a). These angles can be different for different stripe lengths l, being larger for short stripes near the edge of the sample. Consequently, part of the radiation leaving the stripe might happen

Fig. 10.18 Inﬂuence of pump light diffraction in the VSL method. The stripe begins at the coordinate l0 ≈ 0.11 cm. (a) Diffraction pattern of the pump radiation (Ar+ laser 365 nm) at the beginning of the stripe obtained experimentally (symbols) as well as computationally (solid curve), (b) VSL measurement (symbols) and ﬁt according to eqn (10.33)—solid curve. The exponential growth is an artefact and with ﬁtting parameter G = 84 cm−1 means apparent gain only. (c) Theoretical VSL ﬁt outside the diffraction area yields G = –40 cm−1 , i.e. in reality the sample exhibits only optical losses. Silicon nanocrystals are the material under investigation. After Dal Negro et al. [37].

Experimental techniques for measuring the optical gain

293

Fig. 10.19 (a) Waveguiding effect in the VSL method. Guided modes are highlighted in the cross-section of a planar waveguide; emission leaves the waveguide towards a detection system characterized by a numerical aperture NA. (b) Confocal effect in the VSL method.

not to be collected by the numerical aperture (NA) of the collecting lens, while all the radiation is collected for longer stripe lengths l. Therefore, the IASE (l) dependence can appear to contain a nonlinear increase in its initial parts, posing as false gain. Secondly, the confocal effect is depicted in Fig. 10.19(b). It consists in the fact that the very edge of the sample (spot a in Fig. 10.19(b)) is usually the area which is imaged by the optical system onto the detector or the entrance slit of the spectrometer. Commonly, a combination of a large NA and a short focal length of the collecting lens is applied in order to maximize the collecting system’s efﬁciency while a longer focal length of the imaging lens is often preferred to ﬁt the NA of the spectrometer (Section 2.5). The image is thus magniﬁed in the detection plane, as also indicated in Fig. 10.19(b). During the measurements of small gains, a long stripe needs to be excited, leading to a situation when the image of emitting spots distant from the output edge (spot b in Fig. 10.19(b)) is formed in front of the detector or slit. If the detector area is small or if the entrance slit is narrow, part of the emitted radiation will be lost for detection. The larger the NA of the collecting lens (i.e. the smaller the depth of focus) and the larger the magniﬁcation of the optical system, the more signiﬁcant inﬂuence this effect has. In principle, the very same effect is successfully exploited in confocal microscopes to gain depth resolution; in the VSL method, however, this is an undesirable phenomenon. In particular, if the focal point of the collecting lens is not located exactly at the edge of the sample but lies a bit deeper inside, artefacts posing as false growth of IASE (l) with increasing l can appear. What would help to prevent this problem is to use a collecting lens with small NA, and therefore with long depth of focus; however, such a collecting system signiﬁcantly reduces the collection efﬁciency of IASE . Fortunately, both the confocal and waveguiding effects can be to a large extent corrected for by combining the VSL method with a method called shifting excitation spot (SES) [38]. The SES approach represents in fact a modiﬁcation of the VSL method. It is based on employment of the same experimental setup with a solitary

294

Stimulated emission

Fig. 10.20 Comparison of the VSL (left) and SES (right) methods.

change: only a very short part (a segment) of the stripe is excited instead of exciting the whole length of the stripe, and this segment is shifted along the axis of the stripe, see Fig. 10.20. At the same time, the radiation leaving the edge of the sample is detected; this radiation, however, certainly remains nonampliﬁed by stimulated emission, because it propagates only through the nonexcited part of the sample. On the contrary, it can be attenuated via various loss mechanisms (residual absorption, scattering) on its way through the sample, as demonstrated on the right-hand side of Fig. 10.20. Let the intensity of this emission be ISES (x, ν); by summing up the contributions of all the segments over the path l we obtain l ISES (l, ν) =

ISES (x, ν)dx

(10.36)

0

and then we can compare this curve (as a function of l) with the IASE (l, ν) curve described by relation (10.33). If we ﬁnd that both the curves coincide along the whole length of the stripe (including the possible false exponential part), i.e. ISES (l, ν) ≡ IASE (l, ν), the investigated material obviously does not exhibit optical gain. If, on the other hand, a deviation of the IASE (l, ν) curve from the ISES (l, ν) curve towards higher intensity values is observed, especially for longer stripe lengths, this can be considered proof of the occurrence of optical gain. Nevertheless, if the curves are to be compared, they need to be normalized ‘in a suitable way’, the intensity dependence of emission needs to be taken into account and the inﬂuence of possible absorption bleaching remains to be clariﬁed thoroughly. Several examples will be given in Chapter 15 and the reader is referred to [36] and [38] for a more detailed discussion. Finally, we have to mention one more, equally important application of the SES method. It can be easily employed to determine the loss coefﬁcient K of the material under study. If a ‘point-like’ segment is excited with a weak excitation beam and if the spontaneous-emission signal leaving the edge of the sample is detected at the same time, the intensity of this emission is attenuated as the photons propagate a non-excited medium, according to the

Experimental techniques for measuring the optical gain

295

well-known relation exp (−Kx), where x stands for the distance of the segment from the edge. Thus K can be directly obtained by ﬁtting the decrease of the spontaneous emission (measured for different values of x) with the abovementioned exponential function.

10.6.2 Pump and probe (P&P) method The P&P method exploits, like the VSL method, optical pumping of a certain part of the sample with a strong laser beam. It does not, however, rely on the occurrence of spontaneous photoluminescence, but monitors the processes in the excited area using a weak external probe beam (Fig. 10.21). Changes in the absorption coefﬁcient of the probe beam (or the sample optical transmittance) are then analysed. Let I0 be the intensity of the incident probe beam. The intensity of this beam after passing through the sample (no pumping is applied) will be denoted as IOFF . In the presence of the pump beam let the intensity of the probe behind the sample be ION . Furthermore, let α0 (νs ) denote the absorption coefﬁcient at the frequency νs of the probe beam in the absence of pumping (also referred to as the linear absorption coefﬁcient), and α0 (νs ) + α(νs ) will denote this absorption coefﬁcient altered by α(νs ) as a result of nonlinear processes induced by the pump beam. In most cases, the so-called differential transmittance is then the investigated quantity. It is deﬁned as TD = (ION –IOFF )/IOFF , which can be rewritten using the Lambert–Beer law in the form TD (νs ) =

(1 − R)I0 (νs ) exp [−(α0 (νs ) + α(νs ))d] − (1 − R)I0 (νs ) exp(−α0 (νs )d) (1 − R)I0 (νs ) exp(−α0 (νs )d)

= exp(−α(νs )d) − 1,

(10.37)

Fig. 10.21 Typical schematic of the pump and probe method for the measurement of optical gain.

296

Stimulated emission where d is the thickness of the sample and R its reﬂectivity. The possible change of R as a result of sample irradiation with the pump beam was not taken into account in (10.37); such an approximation is, however, usually considered reasonable. If experiment reveals TD > 0, thus α < 0, then—at ﬁrst glance—we could deduce that ampliﬁcation of the intensity of the probe beam by stimulated emission was achieved in the sample, which implies that positive optical gain was measured. In such a case, however, we should exercise prudence. Two different scenarios are possible: (1) |α| ≤ α0 . Therefore, only a nonlinear decrease in absorption at the frequency νs is present as a result of bleaching. (2) |α| > α0 . Only now has the gain overcome the losses and real ampliﬁcation by stimulated emission takes place. The difference G = |α| − α0 is then called the net gain G.14 Thus, it is necessary to compare quantitatively the linear absorption α0 with the differential absorption α in order to conﬁrm conﬁdently the presence of net optical gain. (If we are sure that |α| α0 we naturally do not have to subtract the ‘background’ due to linear absorption.) Figure 10.22 [39] serves as an example of a P&P measurement. We would just like to remind the reader that the gain spectra displayed in Figs 10.7(b) and 10.8 were also obtained using the P&P method. Now, let us focus on the experimental details. The pump beam usually comes from a high-power pulsed laser and it is advantageous to send it to the sample at an inclined angle, so that the transmitted and scattered pump radiation does not hit the detector monitoring the intensity of the probe behind the sample. The diameter of the excited spot should be several times larger than that of the probe beam on the sample (e.g. 500 μm/50 μm) in order to detect only in the area of homogeneous excitation within the pumped spot. To ensure spatial overlap of the two beams, a spatial ﬁlter (pinhole) can be applied, or the area can be checked using a camera or a microscope with a long working distance. The probe beam intensity needs to be at least one order of magnitude weaker than that of the pump beam not to cause nonlinear optical effects on its own. Both the faces of the sample should be of high optical quality and the sample should have the form of either a self-standing membrane or a thin ﬁlm on a transparent substrate. The thickness of the sample d is limited by both the necessity to ensure perfect overlap of the pump and probe beams within the whole excited volume, and by the requirement imposed by the pump frequency νp on the sample to appear optically thin: the product α0 (νp )d has to be sufﬁciently small to allow the pump beam to penetrate the entire depth of the

14 The P&P method yields in most cases material gain, because the beam is not sensitive to waveguiding effects during its passage through a thin ﬁlm. In correct terminology, we should therefore write g = |α| − α0 . In principle, it is thus possible to encounter a situation when g > 0, with low optical quality of the ﬁlm (waveguide), causing the modal gain G to be negative, preventing the onset of stimulated emission or lasing. Even in custom-made laser structures, the material gain can be much higher than the modal gain (Chapter 14). For the sake of simplicity, in the following discussion we shall not turn our attention to the difference between g and G.

Experimental techniques for measuring the optical gain

297

Fig. 10.22 Comparison of the P&P and VSL methods. Measurements were carried out on CuBr nanocrystals embedded in a glass matrix under an excimer 308-nm laser at T = 15–20 K. (a) Linear absorption coefﬁcient α0 in the exciton region and negative differential absorption −α = |α|. (b) Net optical gain G(ν) given by the difference G = |α| − α0 . (c) Net gain spectrum G(ν) (circles) and spontaneous emission spectrum Isp (ν) (squares), determined by the VSL method. Both methods yield nearly the same magnitude and spectral dependence of G(ν). After Valenta et al. [39].

sample and thus to generate a homogeneous population of photocarriers also in the direction normal to the surface. For example, by allowing the maximum acceptable decrease of the pumping intensity due to interaction with the sample to be 10%, we obtain ln(I /I0 ) ≈ –α0 (νp )d; since ln(0.9) ≈ –0.105, then the upper bound of the thickness is d ≈ 1 μm for α0 (ν p ) = 103 cm−1 . Now, we wish to estimate the sensitivity of this method. First, we realize that the lowest detectable change in the absorption coefﬁcient α is determined mostly by the dynamic range of the detection system. The dynamic range as such is deﬁned as the ratio of the maximum detectable signal Smax to the noise level of the detector, i.e. to the noise equivalent power NEP (Section 2.2). Besides, there √ is a limitation due to shot noise, which scales with the measured signal like S. In other words, the induced relative change in transmission TD has to be larger√than the reciprocal value of the effective dynamic range r = Smax /(NEP + S). It thus follows from (10.37) that √ NEP + S I0 exp [−(α0 + α)d] − I0 exp(−α0 d) ≥ = r −1 , I0 exp(−α0 d) Smax or exp(−αd) − 1 ≥ r −1 .

(10.38)

To simplify the problem, let us consider |α| α0 and therefore G = –α(> 0). This converts (10.38) to Gd ≥ ln(1 + r −1 ),

298

Stimulated emission which for r 1 enables us to apply the well-known approximation ln (1 + 1/r ) ≈ r −1 , yielding Gd ≥ r −1 .

Fig. 10.23 Schematic of the pump and probe method applied to a thick sample in the form of a channel waveguide.

By inserting a typical value r = 103 we obtain the sensitivity limit of the P&P method in the form Gd ≥ 10−3 and if d ≈ 1 μm, the minimum detectable gain amounts to G min ≈ 10 cm−1 . Last but not least, let us try to compare the P&P and VSL/SES methods. From the experimental point of view, it is easier to employ the VSL method as it requires a single (pump) laser beam and, besides, in principle it is applicable even to samples prepared on non-transparent substrates. Because of the possible occurrence of artefacts, discussed in Subsection 10.6.1, the threshold sensitivity of the VSL method—expressed in terms of the product of Gl—is worse compared to the case of the P&P method; it can be estimated to be Gl ≈ 1. However, since usually the relation l d applies, l can reach values as high as l ≈ 1 cm if the sample is large enough and of sufﬁciently high quality, implying the lower limit of detectable gain is roughly about G min ≈ 1 cm−1 . Nevertheless, the VSL method features also an upper bound of applicability, stemming from two phenomena: ﬁrstly, saturation of the IASE signal limits the method to Glc ≤ 5 and, secondly, diffraction effects on the slit (razor blade) make it impossible to measure gain reliably if the stripe is shorter than about 10 μm. Thus, the maximum detectable net gain value (producing saturation of the IASE signal for stripes as short as l = 10 μm) amounts to G max ≈ 5 × 103 cm−1 . This upper limit does not, however, cause problems in real-life measurements, because gains reaching higher values are in reality rarely encountered, except perhaps for, e.g., GaN (see Fig. 10.17). All these considerations are summed up in Table 10.1. To close, the P&P method is more suitable for materials with higher optical gain, while the VSL method (combined with the SES approach) is more advantageous if the values of G are lower. Obviously, a relatively wide interval of the values of G in which both methods are applicable exists, as demonstrated in Fig. 10.22. The handicap of lower sensitivity of the P&P method can be overcome if the sample is prepared in a special way, i.e. in the form of a channel waveguide. The thickness of such a sample, or—more precisely in this particular case—the length of the waveguide d, can reach values from several millimetres to centimetres (Fig. 10.23). The preparation of these special samples (of sufﬁciently high quality), however, is not at all simple, which is probably why such samples are, for the time being, only scarcely used. They can be exploited for measuring modal gain by the P&P method. Table 10.1 Limits of applicability of the P&P and VSL methods for measurements of optical gain. Method

Lower limit

Upper limit

Note

P&P VSL

Gd > 10−3 Gl ≥ 1

– G ≤ 5 × 103 cm−1

α(νp )d ≤ 0.1, d ≤ 1 μm

Problems

10.7 Problems 10/1: Try to ﬁnd the reasons for the M line being present in Fig. 10.1(b), in contrast to the spectra shown in Figs 10.1(a) and 10.1(c). 10/2: Show that if electron levels |1 and |2 are degenerate (the corresponding degeneracy factors being g1 and g2 ), the relation B12 = B21 (g2 /g1 ) applies for the Einstein coefﬁcients. This implies that the higher the degeneracy of the upper level |2, the harder it is to achieve stimulated emission. 10/3: Using relation (10.14) and Fig. 10.4(b), give a derivation of the Bernard– Duraffourg condition (10.16) by calculating the Fermi inversion factor Γ (ν). Next, show that dΓ (ν)/dν < 0. For the sake of simplicity, assume equality of the effective masses m e = m h . 10/4: Show that degeneracy of the electron or hole gas in a semiconductor can result from either (a) light masses of quasi-particles or (b) low (effective) temperature of the gas or (c) high density of the gas; it can evidently be due to a combination of all three factors. (Hint: express the density of particles as a function of the Fermi energy Fe or Fh and apply relation (10.19).) 10/5: Making use of the energy band structure of silicon (e.g. Fig. 7.16) estimate the concentration of donors necessary for ﬁlling all the equivalent minima of the conduction band near the X point. Would it then be possible for direct e–h recombination at the point to occur? Apply the parabolic approximation of the conduction band and use m de = 0.322m 0 for the electron density-of-states effective mass. 10/6: Consider the luminescence decay of an excitonic molecule to a free exciton FE and a photon: EM(K) → FE(K) + hν. The inverse process of EM generation via reabsorption of a photon by an exciton (FE(K) + hν → EM(K), i.e. optical absorption induced by a strong excitation), constitutes losses during ampliﬁcation of spontaneous luminescence by stimulated emission. Show that the corresponding optical gain coefﬁcient arising from the EM line can be described by relation (10.30). Hint: start with the inverse Maxwell–Boltzmann shape of the spontaneous emission line (8.6) and, in addition to that, consider that the thermal distribution of excitons on level |2 in Fig. 10.13(c) is proportional to exp(−h¯ 2 K 2 /2m exc kB T ). 10/7: Answer qualitatively the following questions: (1) Why is the gain curve arising from the EHP luminescence line considerably broader (full width at half maximum is the order of tens of meV) than in exciton-based gain mechanisms (the order of meV)? (2) Why are high-energy photons those being mostly reabsorbed in the loss process (FE + hν → EM) that reduces gain on the line of an excitonic molecule? (3) Is it in principle possible to achieve positive optical gain on the line of the radiative decay of an excitonic molecule in an indirectbandgap semiconductor?

299

300

Stimulated emission

References 1. Yoshida, H., Saito, H., Shionoya, S., and Timofeev, V. B. (1980). Solid State Comm., 33, 161. 2. Lysenko, V. G., Revenko, V. I., Tratas, T. G., and Timofeev, V. B. (1975). JETP, 68, 335. 3. Yoshikuni, Y., Saito, H., and Shionoya, S. (1979). Solid State Comm., 32, 665. 4. Liu, J.-M. (2005). Photonic Devices. Cambridge University Press, Cambridge. 5. Yariv, A. (1967). Quantum Electronics. John Wiley, New York. 6. Bernard, M. G. A. and Duraffourg, G. (1961). phys. stat. sol., 1, 699. 7. Lasher, G. and Stern, F. (1964). Phys. Rev. A, 133, 553. 8. Hall, R. N., Fenner, G. E., Kingsley, J. D., Soltys, T. J., and Carlson, R. O. (1962). Phys. Rev. Lett., 9, 366. 9. Nathan, M. I., Dumke, W. P., Burns, G., Hill, F. D., and Lasher, G. J. (1962). Appl. Phys. Lett., 1, 62. 10. Saleh, B. E. A. and Teich, M. C. (1991). Fundamentals of Photonics. John Wiley, New York. 11. Stern, F. (1976). J. Appl. Phys., 47, 5382. 12. Hildebrand, O. and G¨obel, E. (1976). Investigations on the ground state energy of the electron–hole plasma in GaAs. In: Physics of Semiconductors (ed. F. G. Fumi), p. 942. Proceedings of the 13th international conference on the physics of Semiconduct, Rome. 13. Cassey, H. C. Jr. and Panish, M. B. (1978). Heterostructure Lasers. Part A: Fundamental Principles. Academic Press, New York. 14. Thompson, G. H. B. (1980). Physics of Semiconductor Laser Devices. John Wiley, Chichester. 15. G¨obel, E. (1974). Appl. Phys. Lett., 24, 492. 16. Majumder, F. A., Swoboda, H.–E., Kempf, K., and Klingshirn, C. (1985). Phys. Rev. B, 32, 2407. 17. Klingshirn, C. (2005). Semiconductor Optics. Springer, Berlin. 18. Kunz, M., Pier, T., Bhargava, R. N., Reznitsky, A., Kozlovskii, V. I., M¨uller-Vogt, G., Pﬁster, J. C., Pautrat, J. L., and Klingshirn, C. (1990). J. Crystal Growth, 101, 734. 19. Peyghambarian, N., Koch, S. W., and Mysyrowicz, A. (1993). Introduction to Semiconductor Optics. Prentice-Hall, Englewood Cliffs, N.Y.; Yu, P. Y. and Cardona, M. (1996). Fundamentals of Semiconductors. Springer, Berlin. 20. Dumke, W. P. (1962). Phys. Rev., 127, 1559. 21. Rediker, R. H. (1972). United States Patent No 3 636 471. 22. Trupke, T., Green, M. A., and V¨urfel, P. (2003). J. Appl. Phys., 93, 9058. 23. Michel, J., Liu, J., Sun, X., Bernardis, S., Hong, C.-Y., Beals, M. A., and Kimerling, L. C. (2008). Advanced Ge devices for electronic-photonic integration. E-MRS Spring Meeting, Strasbourg. 24. L´evy, R., Bivas, A., Grun, J. B., and Nikitine, S. (1975). Interaction between excitons at high concentrations. In Excitons at High Density (ed. H. Haken and S. Nikitine), Springer Tracts in Modern Physics, Vol. 73, p. 171. Springer, Berlin. 25. Haug, H. (1968). J. Appl. Phys., 39, 4687. 26. Kushida, T. and Moriya, T. (1975). phys. stat. sol (b), 72, 385. 27. Saito, H. and G¨obel, E. O. (1985). Phys. Rev. B, 31, 2360. 28. Hvam, J. M. (1978). Solid State Comm., 26, 987. 29. Valenta, J., Guennani, D., Manar, A., H¨onerlage, B., Cloitre, T., and Aulombard, R. L. (1996). Solid State Comm., 98, 695. 30. Shaklee, K. L. and Leheny, R. F. (1971). Appl. Phys. Lett., 18, 475. 31. Shaklee, K. L., Nahory, R. E., and Leheny, R. F. (1973). J. Luminescence, 7, 284. 32. Arfken, G. B. and Weber, H. J. (1995). Mathematical Methods for Physicists, 4th edn. Academic Press, San Diego. 33. Dingle, R., Shaklee, K. L., Leheny, R. F., and Zetterstrom, R. B. (1971). Appl. Phys. Lett., 19, 5.

References 34. Nakamura, S., Pearton, S., and Fasol, G. (2000). The Blue Laser Diode. The Complete Story. Springer, Berlin. 35. Valenta, J., Luterov´a, K., Tomaˇsiunas, R., Dohnalov´a, K., H¨onerlage, B., and Pelant, I. (2003). Optical gain measurements with variable stripe length technique. In Towards the First Silicon Laser (ed. L. Pavesi, S. Gaponenko and L. Dal Negro), NATO Science Series, Vol. 93, p. 223. Kluwer Academic Publishers, Dordrecht. 36. Dal Negro, L., Bettotti, P., Cazzanelli, M., Paciﬁci, D., and Pavesi, L. (2004). Optics Commun., 229, 337. 37. Dal Negro, L., Cazzanelli, M., Daldosso, N., Gaburro, Z., Pavesi, L., Priolo, F., Paciﬁci, D., Franz`o, G., and Iacona, F. (2003). Physica E, 16, 297. 38. Valenta, J., Pelant, I., and Linnros, J. (2002). Appl. Phys. Lett., 81, 1396. 39. Valenta, J., Dian, J., Gilliot, P., and H¨onerlage, B. (2001). phys. stat. sol. (b), 224, 313.

301

Electroluminescence

11 11.1 Historical notes

302

11.2 High-ﬁeld electroluminescence

304

11.3 Injection electroluminescence

321

11.4 Electroluminescence of a p-n junction biased in the reverse direction

333

11.5 Problems

336

Most of the previous chapters dealt with luminescence processes excited by optical means, i.e. with photoluminescence. This prevalence closely correlates with the fact that the number of scientiﬁc publications related to photoluminescence problems highly outnumbers that focusing on the rest of the luminescence processes, i.e. cathodoluminescence, thermoluminescence, chemiluminescence, etc. It mainly stems from the relative simplicity of the photoluminescence technique and the minimal requirements on the shape, surface treatment and, among other things, also the electrical conductivity of the studied samples. This approach fully meets the requirements of basic research. However, from the point of view of the present-day applications of luminescence processes in electronics, optoelectronics or our everyday life, the privileged status is given to electroluminescence as a technique of a direct, i.e. nonthermal transformation of electric energy into light. Let us devote this chapter both to the explanation of the basic terms of electroluminescence processes and to the corresponding experimental techniques. We will not, however, go into details of commercial displays, electroluminescence or LED diodes,1 let alone semiconductor injection lasers. In this context, the reader is referred, e.g. to publications [1–4].

11.1 Historical notes Electroluminescence radiation arises from the application of an electric ﬁeld to a luminescent material.2 If we adhere to historical terminology, we distinguish two categories of electroluminescence in semiconductors: the so-called 1 We use the term ‘LED’ diode despite its being an evident pleonasm (LED = light-emitting diode). It is, however, quite a common collocation, which helps to distinguish the light-emitting diode from other diodes. Besides, the term ‘LED’ is sometimes used as an abbreviation for a ‘light-emitting device’ and, in this sense, can also refer to other types of light sources. 2 The term ‘electroluminescence’ does not include gas discharge. The term photoelectroluminescence stands for a process when a phosphor, excited by means of an electric ﬁeld, is simultaneously irradiated by light. Electrophotoluminescence then stands for luminescence excited by light, while its intensity is increased or decreased by an additional electric ﬁeld.

Historical notes Destriau effect and injection electroluminescence. Firstly, the Destriau effect, also referred to as high-ﬁeld electroluminescence, is based on the excitation of certain luminescence centres by free (majority) carriers accelerated in a high electric ﬁeld (of the order of up to MV/cm); both direct (DC) and alternating ﬁelds (AC) are possible. This process was ﬁrst observed by Destriau in the 1930s during the application of an electric ﬁeld to a suspension of zinc sulphide (ZnS) luminescent particles in an insulator [5]. These materials, in particular ZnS:Mn together with rare earth chalcogenides (SrS, SrSe, CaS), remain at the focus of electroluminescence research up to now. The application stimulus behind this research lies in a search for new materials for special types of ﬂat displays, which have now been commercially available for about 20 years. The second type of electroluminescence, namely injection electroluminescence, is characterized by the radiative interband recombination of majority and minority carriers injected into a semiconductor p-n junction. Although the ﬁrst observation of a similar effect dates back to as early as 1907 (in a Schottky rectifying junction in silicon carbide, SiC), it is widely accepted that a thorough investigation of this effect had to await the birth of the p-n junction and transistor between 1947 and 1948, and the correct explanation was provided as late as four years later, in the beginning of the 1950s in the USA [6, 7]. Until then, light emitted by a rectifying metal–semiconductor contact had been perceived only as an unimportant curiosity and had not been well-known in the wider scientiﬁc community. However, the remarkable contribution of the almost forgotten Soviet physicist Losev is deﬁnitely noteworthy. Although he never formally graduated from a university, during the 1920s and 1930s he published (just by himself, without any co-author) a series of publications on the observation of light emission in ZnO and SiC rectifying diodes used, in those days, in radio receivers [8]. Moreover, he correctly explained the nature of this effect as the ‘inversion photoelectric effect’. As is indicated in a recent memorial article [9], it is probable that even signs of stimulated emission can be traced in his work. Losev starved to death as a technician in Leningrad Medical Institute in 1942 during the Leningrad blockade and the effect of injection electroluminescence had to await its rediscovery for another ten years [6, 7].3 Nevertheless, although the origin and main features of injection electroluminescence were determined reliably in the 1950s, its application potential was not fully appreciated at ﬁrst. The renowned textbook of Solid State Physics by Dekker in its seventh edition from 1963 [10] devotes only a short closing paragraph in the chapter on Luminescence to this effect: When a p-n junction of germanium or silicon is biased in the forward direction, electrons from the n-region penetrate into the p-region and holes ﬂow from p to n. The minority 3 A similarity with the story of Nakamura immediately comes to mind. Nakamura, as an unknown scientist in the laboratories of the Nichia Corporation, developed just by himself an LED and injection laser based on GaN (Nakamura, S., Pearton, S., and Fasol, G. (2000). The Blue Laser Diode. The Complete Story. Springer, Berlin). After all, similar features can also be traced back in the story of Maiman who, in 1960 as a young researcher at the Hughes Aircraft Laboratories, almost alone fabricated the very ﬁrst functioning laser (Maiman, T. (1960). Nature, 187, 493) in spite of being disdained and underestimated by world-leading laboratories aiming at the same target. The question arises if such scenarios are the rule rather than a rare exception.

303

304

Electroluminescence carriers so injected will recombine with their counterparts and one might expect emission of photons. This has indeed been observed by Haynes and Briggs. The emitted radiation has a wavelength which agrees well with the optical absorption associated with band-to-band transitions. For Ge and Si the radiation lies in the infrared (λ = 1.77 μm and 1.12 μm, respectively). The emission is localized in the junction region. The physical phenomenon which by means of the discoveries of LED diodes and injection lasers radically contributed to a revolutionary change not only in telecommunications (optoelectronic light sources for optical communications) but also in many aspects of our everyday life (CD-ROM disks, bar code readers, trafﬁc lights, etc.) had thus to await the full exploitation of its potential for another decade. The observation of the high quantum yield of electroluminescence emitted from a p-n junction in GaAs upon injection of minority carriers, published by Keyes and Quist in 1962 [11], is often viewed as an important milestone here. Those interested in further reading are referred to the review articles [12, 13].

11.2 High-ﬁeld electroluminescence High-ﬁeld electroluminescence can be divided into three subcategories: • electroluminescence of powder phosphors (the original discovery by Destriau falls into this category—the phosphor particles were dispersed in a dielectric); • electroluminescence of thin ﬁlms (a homogeneous thin layer of a phosphor ﬁlling up the space between capacitor plates—electrodes); • electroluminescence of a reverse-biased p-n junction. Firstly, we will examine several experimental questions, such as the sample structure and properties, and we will also mention some particularities of electrical excitation. Then, we will explain the principles of the excitation mechanism of luminescence centres in high ﬁelds; the explanation of electroluminescence of the reverse-biased p-n junction is left to Section 11.4.

11.2.1 Experimental considerations The collection of electroluminescence radiation, its dispersion into a spectrum and subsequent detection proceeds wholly analogously to the photoluminescence case, and we can therefore refer the reader to Chapter 2. The fundamental difference here, however, is the excitation technique itself, which is reﬂected primarily in the sample shape and structure. They can no longer be as simple as in the case of photoluminescence. A typical cross-section of a sample for a high-ﬁeld electroluminescence measurement is depicted in Fig. 11.1 (which describes mainly the case of powder phosphors and thin ﬁlms). The substrate can be a non-conductive solid slab covered with a metal electrode, as in Fig. 11.1(a). However, a semiconductor (silicon) wafer with adequate electrical conductivity substituting simultaneously the bottom electrode is often exploited. Thin insulator layers are

High-ﬁeld electroluminescence

305

Fig. 11.1 (a) Principal schematic of a sample for high-ﬁeld electroluminescence studies. (b) Arrangement of the electroluminescent panel for excitation by an alternating ﬁeld. The phosphor is completely encapsulated in a dielectric, which stabilizes its properties and prevents electrical breakdown. The phosphor layer thickness ranges from hundreds of nanometres to several micrometres in both cases.

sometimes inserted in between the phosphor and the electrodes. Then, strictly capacitance coupling, not a galvanic connection, arises (Fig. 11.1(b)), and it is thus necessary to apply AC or pulsed voltage. The active layer thickness is typically hundreds of nm to several micrometres. Tin oxide, SnO2 , sometimes with indium alloy (indium-tin-oxide, ITO) usually serves as a transparent electrode. It is also possible to use a thin ﬁlm of many other metals (Au, Ag, Al, . . . ); in the form of a thin ﬁlm, they are transparent to visible light, however, they are soft and can be damaged easily. Naturally, to analyse the emission spectrum in the correct way, it is necessary to take into account, besides the spectral sensitivities of the dispersion element and the detector, also the spectral dependence of the optical transmission of the transparent electrode. As for the preparation of these types of samples, technical equipment for thin ﬁlm deposition (evaporation, sputtering, plasma-enhanced chemical vapour deposition (PECVD), etc.) has to be available. It is also possible to apply, in particular for the preparation of the active phosphor layer, a wide range of other techniques, for example spin-coating or deposition from a liquid phase. As was mentioned earlier, both AC and DC ﬁelds can be applied for the excitation of electroluminescence; it is related, to a considerable extent, to the phosphor structure and the microscopic excitation mechanism (details will be speciﬁed in Subsection 11.2.2). It is often advantageous to work with a pulsed excitation since long-term loading with a high DC ﬁeld can lead, in particular in novel and unknown materials, to fast degradation of the sample. The pulsed excitation, however, can also cause difﬁculties in many cases. We will mention qualitatively one of them, namely, a consequence of polarization effects.

306

Electroluminescence The pulsed electric ﬁeld perceives most phosphor samples as if they were capacitors because the bandgap width of typical phosphors (ZnS, etc.) is close to that of dielectrics. On the other hand, these dielectrics are far from being ideal insulators as impurities (introduced both unintentionally or intentionally) or defects cause a non-zero concentration of free carriers. As a result of polarization by free carriers, electric-ﬁeld shielding occurs upon application of an external voltage, which is depicted in Fig. 11.2 [14]. The ﬁeld is then attenuated in the sample body or inside a particular grain of the phosphor, whereas the ﬁeld becomes enhanced close to the electrodes or near the grain boundaries (Fig. 11.2(b)). On switching the external ﬁeld off (Fig. 11.2(c)), a ﬁeld of opposite polarity suddenly appears, due to the polarized free carriers. Therefore, even if we apply for example an ideal rectangular voltage pulse with very fast rise time (which is easily done with present-day pulse generators) and with repetition rate f = 1/T , the ﬁeld exciting the luminescence centres inside the sample may have a considerably different shape—see Figs 11.2(d) and (e). This electric ﬁeld behaviour obviously manifests itself also in the electroluminescence kinetics (rise and decay). The rate of the changes shown in Figs 11.2(d), (e) is driven by the time lag required to establish the equilibrium between free carrier drift and diffusion. This time lag τM , referred to as the dielectric relaxation time (or Maxwell relaxation time, respectively),

Fig. 11.2 Impact on the electric ﬁeld distribution of semiconducting phosphor polarization by free carriers in the case of non-injecting electrodes or grain boundaries (capacitance coupling). (a) Spatial distribution of the electron potential energy at the moment of application of the external voltage U0 . Polarization has not yet set in; there is still a homogeneous electric ﬁeld distribution in the sample. (b) The voltage is switched on; the phosphor becomes polarized after an elapsed time τM due to the free carrier displacement and the formation of the space charge near electrodes. (c) Moment of switching off the external voltage. A transient ﬁeld of opposite polarity decaying with time constant τM emerges in the phosphor bulk. (d) Time dependence of the internal electric ﬁeld under a periodic external pulsed voltage (with a period T ), fulﬁlling the condition τM T . (e) Same as (d) but at τM T . After Henisch [14].

High-ﬁeld electroluminescence can be deﬁned also as the mean time necessary for an extra volume charge in an insulator or semiconductor to disperse—due to the DC electric conductivity σDC , not as a result of recombination. It can be written in the form τM = ε∞ ε0 /σDC , where ε∞ is the relative high-frequency dielectric constant of the material [15]. Whereas ε∞ of electroluminescent materials lies in a narrow range of values from 2 to 10, σDC can vary by many orders of magnitude. For ε∞ = 10 and in relatively strongly conductive materials, where σDC = 1 −1 cm−1 = 102 Sm−1 , we therefore obtain (considering ε0 = 8.85 × 10−12 C2 /Nm2 ) τM 9 × 10−13 s, therefore τM is in the order of picoseconds. In this case, complete shielding of the electric ﬁeld inside the phosphor will probably occur (high free carrier concentration); the time dependence of the internal ﬁeld is depicted in Fig. 11.2(d). For less conductive samples, which is more typical, though, τM can be by many orders of magnitude longer (microseconds to milliseconds) and the ﬁeld shielding will be weaker; the internal ﬁeld time relaxation for τM T is shown in Fig. 11.2(e). How these effects manifest themselves in the electroluminescence intensity and temporal behaviour will be discussed in Subsection 11.2.3. However, it becomes evident that the sample preparation, the mode of high-ﬁeld electroluminescence excitation and the subsequent interpretation of results are, as a consequence of a combination of both electrical and optical effects, considerably more complicated in comparison with photoluminescence. In fact, a wide range of other phenomena can moreover play an important role here, e.g. the very high electric ﬁelds at grain boundaries and in the vicinity of the electrodes (see Fig. 11.2(b)) and the presence of hot electrons in these regions; the processes of the recombination of electrons with holes and of surface recombination, which can lead to deviations from the equilibrium state; inhomogeneities of the phosphor and the presence of potential barriers, etc. Obviously, a sufﬁciently general analysis of the conditions of the excitation by an electric ﬁeld is in fact impossible. What is also worth mentioning is the question of the measurement temperature. We remember that the rate of non-radiative processes in semiconductors commonly decreases rapidly with decreasing temperature and therefore the luminescence intensity increases (Section 4.6). From this point of view, it appears favourable for basic research to perform experiments at low temperatures. On the other hand, the electrical conductivity σDC = enμn + epμp decreases with decreasing temperature. The reason for this lies in the decrease of both the free electron n and hole p concentrations and (at very low temperatures ≤ 100 K) also in the decrease of the corresponding mobilities μn and μp . This may adversely affect the efﬁciency of excitation of luminescence centres (Subsection 11.2.2). For this reason, studies of electroluminescence at low temperatures are not nearly as common as photoluminescence studies. Besides, the importance of applications of electroluminescence requires that electroluminescence processes are investigated at room temperature or at least in its close vicinity. In other words, if we want to investigate the microscopic nature of a luminescence process, the almost exclusive approach is by means of photoluminescence; electroluminescence and its investigation, on the other hand, have signiﬁcance as a tool of targeted or applied optoelectronic research.

307

308

Electroluminescence From this point of view, the electroluminescence efﬁciency is undoubtedly one of the important parameters. It is also referred to as the quantum yield in the case of photoluminescence (Section 3.1); for electroluminescence there is no point in using this term (although it is still sometimes used anyway). The electroluminescence efﬁciency is deﬁned in a different way and in the case of high-ﬁeld electroluminescence even several different efﬁciencies are introduced [16]: 1. Excitation efﬁciency ηex =

Number of excited luminescence centres (cm−3 ) Q/e (cm−2 )

where Q is the total transferred electric charge per unit area and e is the elementary electron charge. 2. Radiative efﬁciency ηrad =

Number of centres decaying radiatively (cm−3 ) Number of excited centres (cm−3 )

3. Outcoupling (external) efﬁciency ηout =

Number of photons emitted through the surface (cm−2 ) Generated photons (cm−3 )

The number of photons emitted from the surface is limited mainly by the optical transmission of the semitransparent output electrode, total internal reﬂection and by the surface morphology. 4. The product of the above-mentioned partial efﬁciencies determines the total electroluminescence efﬁciency ηtot = ηex ηrad ηout =

Number of photons emitted through the surface (cm−2 ) Q/e (cm−2 )

Although a little in advance, we can mention here also an expression for the total efﬁciency of the injection electroluminescence: ηtot =

Number of photons emitted through the surface (cm−2 ) Number of injected electron–hole pairs (cm−2 )

11.2.2 Mechanisms of high-ﬁeld electroluminescence To begin with, it may be useful to reﬂect brieﬂy on which of the numerous mechanisms of radiative recombination discussed in the previous chapters can apply in electroluminescence. As mentioned earlier, the study of lowtemperature electroluminescence is rather exceptional; hence we can exclude all luminescence processes occurring only at low temperatures. This, to be speciﬁc, stands for all the channels of radiative recombination of free and most bound excitons (Chapter 7) and luminescence of the electron–hole liquid, EHL (Section 8.4). Next, the effects of high excitation are also excluded (Chapter 8) because it is hardly possible to attain high current densities without damaging

High-ﬁeld electroluminescence

309

the phosphor in high-ﬁeld electroluminescence.4 Hence, there is not much left—in fact, only three potential radiative recombination channels remain: (1) Extrinsic luminescence of localized centres, primarily ions of the transient metals and rare-earth ions (Section 5.6). (2) Recombination processes involving the participation of neutral donors and acceptors, in particular the luminescence of donor–acceptor pairs (Section 5.4). The prerequisite here, however, is that the ionization energy of donors and acceptors is sufﬁciently high for the impurities to exist in their neutral state also at room temperature. (3) Intrinsic recombination of free electron–hole pairs. The probability of such a process is, however, in comparison with processes (1) and (2) very low at room temperature. A condition necessary for high-ﬁeld electroluminescence is then the presence of free carriers. They are accelerated in an electric ﬁeld and due to collisions they can transfer a portion of their energy to the above-mentioned luminescence centres, exciting them in this way. Possibly also free electron– hole pairs, which subsequently recombine radiatively or pass their energy to the above-mentioned extrinsic centres, can be generated during this process. In the case of a sufﬁciently conductive phosphor and galvanic coupling, carriers can be introduced into the luminescent material via injection from electrodes; in the capacitively coupled thin ﬁlms of phosphors, on the other hand, carrier injection can be realized, e.g. from surface states located in the vicinity of the electrodes or by thermal release (with the assistance of the electric ﬁeld) from deep traps in the material volume, which is the so-called Poole–Frenkel effect. Let us leave these considerations for now and assume that free electrons or holes are present in the luminescent layer. We will now explain in more detail the essence of the excitation mechanism. Let us emphasize here that, unlike photoluminescence experiments and theoretical work which—thanks to development of laser technology in the 1960s and 1970s—boosted the discovery and interpretation of a series of new recombination processes in semiconductors, the past 40 or 50 years did not bring any fundamentally new results in electroluminescence. Strictly speaking, we will recapitulate the classical knowledge summarized comprehensively, e.g., in the review chapters of monographs [16] and [17]. Impact ionization and excitation Typical luminescence centres behind the luminescence of thin ﬁlms of ZnS are Mn2+ ions, where photons are emitted owing to the electron transitions between levels of the not fully occupied 3d shell. A similar role can also be played by di- and trivalent rare earth ions. Processes of excitation of such centres occurring in high electric ﬁelds are depicted in Fig. 11.3. The electric ﬁeld accelerates the free carriers propagating in the ZnS lattice; we will speciﬁcally 4 The maximum attainable steady-state drift velocity of carriers in most semiconductors (in a ﬁeld intensity ≥ 100 kV/cm) is of the order of v = 107 cm/s and typical current densities are j = 4 A/cm2 , the relevant carrier density being n = j/ev ≈ 2 × 1012 cm−3 (e is the electron charge). The high excitation effects set in at carrier densities of at least three or four orders higher.

Fig. 11.3 Possible electroluminescence processes in high ﬁelds. (a) Impact excitation of an extrinsic luminescence centre (the transition metals or rare earth type of ions) by an accelerated electron: the most important electroluminescence process in ZnS:Mn. (b) Excitation of a donor–acceptor pair via impact ionization of the lattice. (c) Intrinsic electroluminescence process: Impact ionization of the pure semiconductor lattice. With a certain probability, it is possible to detect luminescence photons with energy both much higher and lower than E g .

310

Electroluminescence speak of electrons because they are the majority carriers in semiconductors of this type. The electrons transfer their energy to the luminescence centres by inelastic collisions and relax to the bottom of the conduction band (so-called impact excitation, Fig. 11.3(a)). This is the excitation mechanism that occurs in a ‘standard’ electroluminescence material ZnS:Mn2+ . For completeness, two additional types of excitation processes which can occur in high ﬁelds in other semiconductors are shown in Figs 11.3(b) and (c), namely, impact lattice ionization leading to the luminescence of donor–acceptor pairs or to a speciﬁc intrinsic emission. It is apparent that the minimum energy of an accelerated electron in ZnS:Mn2+ must amount to at least ∼ 2 eV, which corresponds to the wavelength of about 600 nm of the radiation emitted by the Mn2+ centre. Electrons with such a high energy (measured relative to the bottom of the conduction band) do not occur at standard conditions of charge transport in semiconductors. The temperature Tef , participating in the energy distribution function of the electrons, is then much higher than the lattice temperature T . We speak of so-called hot electrons (or holes).5 In order to better understand their role in electroluminescence processes, we have to discuss them in more detail. Most convenient will be to begin with classical electrical conduction in semiconductors in weak electric ﬁelds (≤ 103 V/cm). In weak ﬁelds F, as is well-known, the statistical energy distribution of the electrons at the bottom of the conduction band is described by the (nondegenerate) Boltzmann distribution. Under these conditions (sufﬁciently low concentration, sufﬁciently high temperatures), electrons travel for the mean free path l = v T τm

(11.1)

isotropically in all directions between collisions; here, τm is the mean time between collisions due to electron scattering and v T is the mean velocity of the thermal motion. The mean velocity follows from the thermal equilibrium of the electron gas with the lattice as descibed by the equipartition theorem m e v T 2 /2 = (3/2)kB T , or

3kB T . (11.2) v T = me The electric force −eF affects the equilibrium distribution of velocities only as a small perturbation, the drift velocity of electrons v d in the ﬁeld direction being much smaller than v T and Ohm’s law holding true. We may write down this law in the form j = σ F, where σ = enμn 5 Hot carriers can be generated equivalently both by accelerating them in high electric ﬁelds or exciting by light highly above the gap (even if the detailed mechanisms through which the carriers acquire energy may be different). In Section 5.3 we put the accent on the concept of the effective temperature Tef of the exciton or photocarrier gas rather than on that of hot carriers. Such terminology was employed because the term ‘hot carriers’ is used more commonly in the narrower sense of the word just for the case of high-ﬁeld charge transport in semiconductors.

High-ﬁeld electroluminescence

311

Fig. 11.4 Path evolution of an electron that is ‘heated up’ in a semiconductor in an electric ﬁeld with increasing intensity F. Beginning with low ﬁelds and increasing F from (a) via (b) to (c), the drift velocity vd increases, however, the mobility decreases (see text).

is the electrical conductivity, n stands for the electron concentration and μn =

eτm el = me m e vT

(11.3)

is their mobility, representing a proportion between the drift velocity and the electric ﬁeld intensity vd = μn F.

(11.4)

The transport of electrons in low ﬁelds is shown schematically in Fig. 11.4(a). The drift velocity vd is much lower than the mean thermal velocity vT . Now, let us have a look at what happens when increasing the ﬁeld intensity F. This represents a rather sophisticated complex of processes, in which the decisive role is played by scattering mechanisms (collisions) in which electrons change the direction of their movement and lose part of their energy [15, 18, 19]. Starting from a certain ﬁeld intensity F0 , the electrons begin to ‘feel’ the accelerating pull of the electric ﬁeld along their free path l, and the mean velocity between collisions vT begins to rise (unlike the thermal velocity (11.2)), which means that the electron system heats up. The electron drift velocity increases; however, as long as one may still regard the ﬁeld as not too high, electrons do not gain too much energy and the decisive collision mechanism in that case remains the scattering on acoustic phonons. The mean free path l remains constant (does not increase with increasing electron energy) and we may deduce from (11.1) and (11.3) that a decrease in τm and thus also a decrease in the mobility of electrons μn occurs for vT > vT . Mobility is thus no longer a constant, but starts to be a function of F:μn = μn (F). The increase in the drift velocity is depicted in Fig. 11.4(b), and the accompanying decrease in mobility μn , which, at a ﬁrst glance, might seem somewhat paradoxical, is demonstrated in Fig. 11.5 via decreasing the slope of the vd (F) plot in segment (b). A further increase in the ﬁeld intensity leads to a further, although slower, increase in the free electron energy. Once this energy becomes comparable with the energy of the optical lattice vibrations h¯ ω0 , the generation of optical phonons becomes the prevailing mechanism of electron scattering. Since the energy h¯ ω0 is rather high, an electron loses almost all its energy during such a ‘collision’ or inelastic scattering. Therefore, a further increase in vd with increasing F is now slow and approaches saturation characterized by a further decrease in mobility (Fig. 11.5, segment (c)). Only a very small number of hot electrons manage to retain an energy exceeding h¯ ω0 during

Fig. 11.5 Approximate sketch of the dependence of the electron drift velocity on the electric ﬁeld intensity in a semiconductor (at room temperature). The segments (a), (b), (c) correspond to the labelling in Fig. 11.4.

312

Fig. 11.6 Energy band structure of ZnS. After Luo et al. [20].

Electroluminescence the given time interval. The magnitude of the saturated drift velocity is, in most semiconductors, of the order of 107 cm/s (Problem 11/2) and, at such a high value, not only the impact excitation of luminescence centres but also the lattice ionization accompanied by the generation of free electron–hole pairs can occur. These effects were, by the way, already demonstrated in Fig. 11.3. High-ﬁeld electroluminescence processes therefore generally lie at the edge of semiconductor avalanche breakdown. A full development of the electric breakdown is, however, prevented by both the presence of active luminescence impurities and also of a suitable energy band structure (see below). Moreover, a critical issue here is the high homogeneity of the material. In the standard ZnS:Mn2+ material, however, lattice ionization is very improbable, as we will see shortly. Let us keep following with our eyes the plot μn = μn (F) in Fig. 11.5. In some semiconductors with a suitable band structure, even a decrease in the drift velocity can occur under the highest ﬁelds (dashed curve in Fig. 11.5). This is a rather astonishing effect, characterized also by the term negative differential conductivity, arising from transitions of the accelerated electrons from the absolute minimum of the conduction band at the point (k = (0, 0, 0)) to a higher-situated minimum at some other points of the ﬁrst Brillouin zone. Such a transition between band minima (intervalley scattering) is not, of course, possible at thermal equilibrium of electrons with the lattice and in low ﬁelds. Besides the presence of a high ﬁeld, another condition must therefore be fulﬁlled, namely, that the energy separation between the minima is much higher than kB T and, at the same time, smaller than the bandgap width E g , otherwise electron–hole pair generation by impact ionization across the forbidden gap prevails. The lateral energy minima usually exhibit smaller band curvature and therefore higher effective mass m e . This, according to (11.3), means yet another decrease in electron mobility and, consequently, a lower drift velocity vd . It was believed for rather a long time that the transfer of hot electrons between valleys of the conduction band occurs solely in the case of GaAs and InP, where the so-called Gunn effect takes place based on this principle, facilitating the production of tiny microwave generators. However, the ZnS band structure, depicted in Fig. 11.6 [20], shows that ZnS also fulﬁls the above-stated criteria for electron transitions from the central minimum to side valleys, namely to X (k = (1, 0, 0)) and L (k = (1, 1, 1)). At the same time, it can be clearly seen that these valleys are in fact much shallower than the valley at the point, and that hot electrons appreciably decrease their drift velocity there. An important question is, then, whether the transfer of hot electrons → X , L, which is now believed to exist in ZnS, is of any importance for electroluminescence processes. It actually turns out to be of substantial importance. That is to say, it increases the efﬁciency of impact excitation of the Mn2+ centres. This efﬁciency is quantitatively described by a quantity referred to as the impact excitation cross-section σim . Recent calculations [21] have shown that there is a wide range of parameters which the impact excitation cross-section depends on; in particlar σim scales with the free electron effective mass m e and its drift velocity vd as

High-ﬁeld electroluminescence σim ≈

me ; 2 v E ge d

(11.5)

E ge stands for the energy loss of electrons corresponding to the excitation of the Mn2+ centre from its ground to the excited state. From relation (11.5), it is immediately clear that a heavy mass m e and a low velocity vd in the side valleys lead to the increase in σim . For many years, another supporting factor to which ZnS:Mn2+ and related semiconductors owe their leading role among inorganic electroluminescent materials—as the ideal combination of host lattice and extrinsic luminescence centre—is found in the suitable energy separation of the X and L valleys from the absolute minimum at the point: this separation is much lower than Eg (≈ 3.7 eV at room temperature). The energy distribution of hot electrons then, as calculations show, just matches the absorption spectrum of the Mn2+ ions in ZnS and, consequently, only a tiny fraction of electrons can reach energies high enough to be able to ionize the ZnS lattice. Therefore, there is no immediate danger of avalanche breakdown of the material. It is necessary to stress one more fact: Although the decrease in mobility of hot electrons with increasing F turns out to be a prerequisite for efﬁcient and safe electroluminescence, we have to realize that the initial high mobility μn in low ﬁelds (the high initial slope (a) in Fig. 11.5) is no less important. It helps to attain the desired energy of hot electrons in ﬁelds of a reasonable intensity F. Now, let us move on to the question of free carrier generation in high-ﬁeld electroluminescence. Generation of free carriers Several mechanisms of free carrier generation for impact excitation of luminescence exist: (1) injection of majority carriers from electrodes; (2) release of carriers from deep traps localized in the phosphor, due to both high electric ﬁeld and tunnelling; (3) release of carriers from traps on the boundary between a dielectric and the phosphor. The mechanism (1) is active at the direct galvanic contact of a conductive electrode with the semiconductor-phosphor, while the carriers release (3) will apparently apply in an electroluminescence device with capacitance coupling and AC excitation. Carrier generation (2) can occur for both galvanic and capacitance coupling, with very variable importance with respect to the two above-mentioned possibilities. We will now explain the physics underlying these mechanisms. (1) Injection of majority carriers from electrodes. One deals essentially with a process occurring in the well-known rectifying metal–semiconductor Schottky junction. However, in this case, the junction is exploited in a speciﬁc way. Firstly, let us recapitulate what is to be understood under the concept of ‘charge carrier injection’. This is a disturbance of the equilibrium space distribution of carriers by a local increase of their concentration beneath the

313

314

Fig. 11.7 Energy band scheme of a metal–semiconductor junction (Schottky barrier) for an n-type semiconductor. (a) Steady state without external bias, characterized by a built-in potential barrier ΦBZ. . (b) Bias U is applied in the forward direction. Minority carrier (hole) injection into the semiconductor takes place. (c) Bias U applied in the reverse direction. Majority carrier (electron) injection into the semiconductor takes place either thermally across the lowered barrier (transition 1) or via tunnelling (transition 2). Simultaneous lowering and narrowing of the barrier is shown in the enlarged inset.

Electroluminescence surface, or at an interface with another material or, in particular, near a contact with a metal. The depth into which this disturbance penetrates depends on the magnitude of the injection current and carrier lifetime (at low current and low lifetime, injected charges will be localized only in the close vicinity of the injecting contact, and in a negligible concentration). Now, it is important to distinguish between the injection of minority and majority carriers. It usually goes without saying that the term ‘injection’ refers to the injection of minority carriers, because injecting minority carriers is much simpler than injecting majority carriers. This stems from the following reasons: In both the cases, an additional local electric ﬁeld and consequently also the drift currents are generated by the injection, introducing a compensating charge of opposite sign into the area of injection. At the same time, the diffusion current of the injected carriers ﬂows in the opposite direction. Speciﬁcally, in an n-type semiconductor (where n 0 p0 holds true for the carrier concentrations), we generate a local increase in hole concentration p during minority carrier injection; these holes will tend to diffuse into the material volume. Simultaneously, as a result of the relation n 0 p0 , the drift current of majority carriers—electrons—will be comparatively higher. Therefore, if we keep the p concentration constant with the aid of an external activity, other electrons are attracted to the area of injection and the excess concentration of minority carriers—holes—remains relatively stable. If, on the contrary, in an n-type semiconductor we increase locally via charge injection the electron concentration by n, then the diffusion electron current ﬂowing all around into the surrounding lattice overwhelms (again) the current caused by attracted holes; thus compensation of the negative space charge is realized mostly via spreading of the electron cloud. Therefore, the excess concentration n tends to vanish very rapidly and it is indeed very difﬁcult to keep it constant. In order to do so, a very high rate of the electrons is indispensable. In order to achieve electroluminescence in high ﬁelds, however, it is just the injection of majority carriers that is the crucial process. In the typical case of ZnS:Mn2+ , as we mentioned earlier, it is the injection of electrons because ZnS is inherently an n-type semiconductor. Let us now have a look at Fig. 11.7, which shows the carrier energy scheme in the vicinity of a contact between a metal and an n-type semiconductor. Steady state is depicted in panel (a). In the forward direction (panel (b), negative bias U applied to the semiconductor), injection of the holes, i.e. minority carriers occurs. Unfortunately, such an injection is not suitable for excitation of electroluminescence. Consequently, it is necessary to apply reverse bias (panel (c)) when, due to an electric ﬁeld F, the built-in potential barrier for electrons is decreased from its initial value ΦBZ by the quantity Δ = (eF/4πε0 εs )1/2 [22, 23] and electron injection occurs (this effect is sometimes referred to as the Schottky effect). The effect of the high electric ﬁeld F is twofold: ﬁrstly, this ﬁeld keeps the injected electron current at a magnitude sufﬁcient to sustain the stability the electron concentration (as explained above), in spite of the very small number of injected electrons (reverse bias!). Secondly, this ﬁeld has a major role to play also in the impact excitation of luminescence centres by accelerated electrons, as is also indicated in Fig. 11.7(c).

High-ﬁeld electroluminescence The electron injection current density in this case reads [22, 23]

j∼ = T 2 exp −e(ΦkBBZT−Δ) πε0 εs )1/2 ) = T 2 exp − e(ΦBZ −(eF/4 kB T

1/2 BZ = T 2 exp aUT − eΦ kB T ,

315

(11.6)

where εs stands for the static dielectric constant of the semiconductor. Therefore, the current density increases exponentially with the square root of the applied bias U = Fd. Let us emphasize that (11.6) describes the injection of thermal electrons across the lowered potential barrier (arrow 1 in Fig. 11.7(c)). Under the application of a very high ﬁeld, however, the injection of electrons can be enhanced due to their tunnelling through the barrier (arrow 2 in Fig. 11.7(c)). That is to say, the barrier not only gets lower but also narrower with increasing ﬁeld F, as depicted in the enlarged inset in Fig. 11.7(c). Thus, the barrier penetrability for electrons quickly increases (so-called Fowler–Nordheim tunnelling). The effect sets in at a barrier width below about 0.01μm. (2) Release of carriers from deep traps. Lattice defects in semiconductors act as deep traps (potential wells) for charge carriers. The concentration of these defects is relatively high mainly in wide-bandgap materials (ZnS, CaS, SrS), which have appropriate band-structure parameters for electroluminescence in high ﬁelds. Especially electron traps, as we know, are essential in this context. Similarly to the above-discussed case of injection from contacts, upon the application of an electric ﬁeld, a decrease in the potential barrier of the trap occurs as is shown in Fig. 11.8. This leads to the thermal release of trapped electrons into the conduction band, which is known as the Poole– Frenkel effect. An expression for the electron current density is very similar to

Fig. 11.8 Energy band scheme of an electron in a deep trap described by the potential −e/4πε0 εs x. (a) Without external bias. (b) A high external ﬁeld of intensity F is switched on. A decrease of the potential barrier height by Δ = (eF/πε0 εs )1/2 and ﬁeld-assisted thermal emission of the electron from the trap occur (Poole–Frenkel effect.)

316

Electroluminescence eqn (11.6) and has the form of [22, 23] e ΦBZ −(eF/πε0 εs )1/2 j∼ F exp − = kB T

1/2 ≈ U exp bUT ,

(11.7)

where U is the voltage across the luminescent layer. Moreover, also in this case the electrons can be injected from the trap into the conduction band via direct tunnelling through the narrowed barrier at ﬁelds F of the order of 106 Vcm−1 . Under such conditions, the current density naturally does not depend on temperature and is given by [22–24] b j∼ , (11.8) = U 2 exp − U where b is a constant. It is widely believed that this type of tunnelling constitutes the dominant contribution to the electron emission into the conduction band in very high ﬁelds. (3) Release of carriers from traps on the boundary between a dielectric and a phosphor. If a semiconductive phosphor is in contact with an insulator (which is typically the case of AC powered electroluminescent components where the phosphor is sandwiched between two insulating layers—see the scheme in Fig. 11.1(b)) – lattice defects are formed at the interface. The corresponding electronic states are localized within the forbidden band, as is indicated in Fig. 11.9. Under application of an electric ﬁeld, electrons captured in these traps can be injected into the conduction band, again either thermally owing to the Poole–Frenkel effect or by tunnelling. Fig. 11.9 Band scheme of the interface between a dielectric and a luminescent layer. Electron injection can happen both thermally (1) and via tunnelling (2).

11.2.3 Intensity, spectral and temporal characteristics Throughout this subsection we give several examples of typical experimental results, also paying attention to the question of whether and how it is possible to use the experimental demonstration of high-ﬁeld electroluminescence to identify the relevant excitation mechanism, and potentially also to help uncover the luminescence centre. Concentrating here on the basic physics—we are to investigate a sample of a new material exhibiting electroluminescence—we leave the purely application-related aspects aside. The dependence of the electroluminescence intensity (often referred to as the electroluminescence ﬁlm brightness B) on the applied voltage U is evidently an easily measurable characteristic. If we make the assumption that the brightness B is proportional to the injection current density j, it springs to mind to inspect the differences in the dependencies (11.6), (11.7) and (11.8) as functions of the applied voltage U . These curves are (in a convenient normalization and suitable choice of the constants a, b and b ) depicted in Fig. 11.10. It is evident that the differences between the overall curve shapes are not too important. Thus, if we plot B directly as a function of U (both quantities in linear scale), it is very difﬁcult to determine the injection mechanism, especially if these mechanisms happen to occur simultaneously. An

High-ﬁeld electroluminescence

317

Fig. 11.10 Dependence of the high-ﬁeld electroluminescence brightness B on the applied voltage U for three different mechanisms of free carrier generation. The inset shows the same curves, just plotted in a different way. The calculation parameters, i.e. the values of the constants a, b and b in eqns (11.6), (11.7) and (11.8), were chosen as close to a typical experiment as possible, and room temperature was considered.

Fig. 11.11 Examples of experimental curves of the electroluminescence brightness B against the applied voltage U (at room temperature). (a) In linear scale (different curves correspond to different powder materials dispersed in a dielectric matrix, AC voltage was applied. After Henisch [14]). (b) In the √ form of log B = f (1/ U ) for a ZnS ﬁlm of thickness of ∼ 1 μm doped with Cu, Mn, Cl; DC bias, after Thornton [26].

example of several experimental curves B = B(U ) in a linear scale is given in Fig. 11.11(a) [14]. We might seem closer to solving the problem, however, if we plot in a logarithmic scale B/U 2 ∼ j/U 2 as a function of 1/U according to (11.8): see the inset in Fig. 11.10. This way we obtain the so-called Fowler–Nordheim straight line for the case of tunnelling and if the experimental data follow such a dependence, some authors conclude that Fowler–Nordheim tunnelling is the primary source of free carriers. However, a very careful examination of data is indispensible and the measurements should be performed, if possible, in a sufﬁciently wide interval of voltages. Quite frequently, in particular in older works, one can meet the dependence √ B ≈ exp(−b / U ). (11.9)

318

Electroluminescence This relation was derived by Zalm in his doctoral thesis [25] devoted to zinc sulphide, ZnS, doped with different ‘activators’. Exploiting the speciﬁc conditions of this semiconductor, he assumed that under the negative electrode near the ZnS surface a potential barrier (depletion layer) of the Schottky type (Subsection 11.2.2) emerges from ionized donors. Despite the barrier being relatively thick (∼ 100 nm), the author considers that tunnelling of electrons into ZnS under the inﬂuence of external bias from the cathode occurs, followed by their acceleration in the high-ﬁeld region of the barrier and subsequent impact excitation or ionization of the luminescence centres, rather than thermal overcoming of the barrier by the electrons. From our modern terminology, this is a speciﬁc case of Fowler–Nordheim tunnelling. For ZnS, the relation (11.9) holds very precisely over several orders of magnitude (Fig. 11.11 (b) [26]), both for DC and AC excitation. The given assumptions, however, considerably limit the general validity of this model, which was relatively widely discussed from its early days. In addition, breaks on the curve sometimes occur, which may indicate either a non-exact model or the participation of more injection mechanisms. It is therefore evident that the study of the B = B(U ) dependence on its own can be a sufﬁciently reliable approach for the determination of the transport or injection mechanisms in electroluminescence in exceptional cases only, rather than as a routine tool.6 It might have crossed the reader’s mind that the temperature behaviour of the brightness B can be considered an important additional piece of information because relations (11.6)–(11.8) show different temperature behaviour. However, the corresponding luminescence experiment cannot differentiate the temperature dependence of the excitation current density from that of the radiative process itself. Parallel measurements of the current density j and brightness B under varying temperature can of course be performed, if we have at our disposal an instrument sufﬁciently sensitive for measuring small currents. However, such an experiment is already more complex and an unambiguous result (i.e. separation of the temperature dependence of the charge transport from the temperature dependence of the radiative recombination) is, remembering the above mentioned possible superposition of more transport processes and the occurrence of polarization effects, by no means guaranteed. As for the spectral composition of electroluminescence, the situation simpliﬁes substantially. If we measure (at the same temperature) the emission spectrum of a given electroluminescence sample under both electrical and optical pumping (the latter realized, e.g. by illuminating the transparent electrode with ultraviolet radiation) and both the spectra look the same in their salient features, we can quite reliably conclude that in both cases the same luminescence centre is active. A wide range of methods offered by photoluminescence spectroscopy, which were discussed in detail in the previous chapters, can then be employed. This approach has been adopted from the very beginning of 6 It is also necessary to be aware of the simplifying assumptions. Firstly, is the assumption about linear scaling of the electroluminescence brightness with current density; here, however, it is not easy to determine the effective area of the injecting electrodes and, in addition, we have to rely on homogeneity of the ﬂowing current. Further, the probability of the excitation or ionization process itself may depend on the applied voltage, etc.

High-ﬁeld electroluminescence

319

electroluminescence research, as is indicated by the examples in Fig. 11.12, showing a comparison of a photoluminescence and electroluminescence spectrum of ZnS/CdS powder from 1940 in panel (a) [27] and analogous curves used during a contemporary study of the properties of silicon nanocrystals in panel (b) [28]. Generally speaking, we cannot expect complete identity of both spectra because, e.g., the photoluminescence emission spectrum can slightly depend on the excitation wavelength, and, similarly, the electroluminescence spectrum can depend on the applied voltage, frequency of the AC ﬁeld, etc. Neither can the inﬂuence of the semitransparent electrode be neglected. By the way, these effects are also demonstrated in Fig. 11.12. Attention must be paid—we cannot help but emphasize again—to the main features of the spectra, and to the occurrence of several similar bands, even though their relative intensities may differ. It is also necessary to keep in mind that the emission spectrum of a thin layer can have an interference structure modulated on it. An example of the temporal characteristics of electroluminescence in high ﬁelds is given in Fig. 11.13 [29]. It refers to thin ﬁlms of the so-called IIa– VIb compounds, doped with rare earth ions: blue-green emitting SrS:Ce3+ , and CaS:Eu2+ luminescing in the red.7 A double-isolating sandwich sample

Fig. 11.12 (a) Comparison of a photographic record of the photoluminescence emission spectrum of mixed ZnS/CdS crystals (1, 2) with their electroluminescence spectrum (3) excited by an AC ﬁeld of amplitude 5 × 105 V/cm. Spectrum 1 is sandwiched between reference spectra of argon lines. Wavelength increases from right to left, measured at room temperature, after Destriau and Loudette [27], dated 1940. Reproduced with kind permission of EDP Sciences. (b) Electroluminescence (points) and photoluminescence (line) emission spectra of an electroluminescence diode manufactured from porous silicon. Room temperature, after Linnros and Lalic [28], dated 1995. Among other things, this ﬁgure represents an interesting comparison of the level of presentation of results in scientiﬁc journals 70 years ago and nowadays.

7 Such phosphors are sometimes called Lenard phosphors and have been the subject of study for a long time. With regard to their hygroscopicity, it is necessary to passivate the electroluminescence ﬁlms of these materials well to prevent direct contact with air. These semiconductors are attractive primarily because of their ability to accept a wide range of dopants including rare earth

320

Fig. 11.13 Time behaviour of electroluminescence of thin ﬁlms (a) SrS:Ce,K, (b) CaS:Eu and (c) ZnS:Ce,F. The top panel depicts the shape of the applied voltage pulses, measurements performed at room temperature. After Tanaka [29].

Fig. 11.14 (a) Cross-section of an AgCl thin sheet fabricated for electroluminescence measurements and (b) oscillographic record of the temporal behaviour of the electroluminescence (upper trace) during excitation by electric pulses (lower trace) with a duration of 100 μs. For the sake of transparency, both waveforms are mutually phase shifted. Measurement temperature T = 77 K (sample in liquid nitrogen). After Vacek [31], reproduced with kind permission of Wiley-VCH Verlag GmbH&Co. KGaA.

Electroluminescence structure, similar to that in Fig. 11.1(b), is employed. The characteristic feature in this particular case is that the luminescence, pumped with electrical pulses, has the form of short ﬂashes both during switching on and off the voltage. This means that the second ﬂash appears in a ﬁeld of opposite polarity, as a result of the polarization effects occurring near the interface between the phosphor and the insulating layers, as depicted in Fig. 11.2. From this one can infer the excitation mechanism: the ﬁrst thing which most probably occurs is the impact excitation of the Ce3+ and Eu2+ centres by the electrons accelerated in the applied pulsed ﬁeld, then their ionization in high electric ﬁeld takes place, thereby creating Ce4+ and Eu3+ ions. Electrons released into the conduction band in this way get subsequently localized in traps. At the moment when the pulsed voltage is switched off, these electrons are again released into the conduction band, captured back by ionized rare earth centres, and ﬁnally, the electroluminescence photon is emitted due to the radiative transition 4fn−1 5d → 4fn inside the luminescence centre. Such temporal behaviour of electroluminescence (when the frequency of the luminescence ﬂashes is doubled with respect to the frequency of the pumping pulses) is not of course observed in all materials, as is demonstrated in panel (c) in Fig. 11.13, representing the electroluminescence of Ce3+ centres in ZnS. Here, just a single luminescence pulse corresponds to a given polarity of the electric pulses. This means that no ionization of the Ce3+ centres occurs, but, like the ‘classical’ case of ZnS:Mn2+ , impact excitation by the accelerated electrons should be considered instead. This substantial difference between electroluminescence of ZnS and CaS or SrS is caused by both the differences in the energy band structure and the differences between ionic radii of the lattice cation constituents and their ratio to the ionic radii of dopants–activators (Ce3+ , Eu2+ ). Details can be found in [29, 30]. In the previous chapters we quite often mentioned crystals of silver halides as suitable model materials. We shall close this subsection with a brief remark on the electroluminescence of AgCl. The temporal behaviour of the electroluminescence of a sheet of pure silver chloride (excited at a temperature of liquid nitrogen T = 77 K by electric pulses of duration 100 μs) is, together with the sample cross-section, shown in Fig. 11.14 [31]. It is obvious that the luminescence brightness exhibits two short ﬂashes, which are in phase with the leading and trailing edges of the electric pulse (the luminescence and voltage traces are intentionally shifted with respect to one another in Fig. 11.14); the ﬁrst ﬂash is substantially weaker than the second one. The applied voltage has a negative polarity on the point electrode, which is in direct contact with the sample surface. On the basis of the contemporary understanding of mechanism of low-temperature AgCl photoluminescence, consisting in the radiative decay of the self–trapped exciton (see Subsection 7.2.4), we may qualitatively interpret the observed kinetics of AgCl electroluminescence from Fig. 11.14(b) in the following way.

ions and thus cover with their luminescence the whole visible spectrum, which is ideal for colour thin ﬁlm electroluminescent displays.

Injection electroluminescence The negative point electrode injects electrons into the sample. They are immediately strongly accelerated because the ﬁeld under the point electrode is very high, as is indicated by the ﬁeld lines (dashed curves) in Fig. 11.14(a). These electrons can therefore ionize the lattice, thereby generating free electron–hole pairs. The holes in AgCl immediately become self-trapped and the electrons soon become localized at the traps, which occur in sufﬁcient concentration in AgCl (e.g. interstitial ions, Ag+ ). At the same time, a certain number of secondary electrons may bind with the holes to create self-trapped excitons, which subsequently recombine radiatively with a typical decay time of ∼ 10 μs. This is how the ﬁrst weak electroluminescence ﬂash arises. During the application of the external voltage, however, an internal ﬁeld appears at the same time, due to both the generation of a space charge of free carriers and to ionic lattice polarization. Therefore, upon switching off the voltage pulse, a ﬁeld of opposite polarity appears inside the sample for a moment (Fig. 11.2(c)). This ﬁeld may subsequently release the localized electrons via the Poole–Frenkel mechanism; the electrons then come back to the point electrode. They are captured owing to Coulomb forces by the holes previously self-trapped beneath the surface, thereby creating self-trapped excitons. Their radiative decay then gives rise to the second, more intense electroluminescence ﬂash. This result can serve as a rather atypical example of low temperature intrinsic electroluminescence. The kinetics itself depicted in Fig. 11.14 would not of course sufﬁce for an unambiguous identiﬁcation of the origin of this electroluminescence; we should at least add that it is observed that the emission spectra of photoluminescence and electroluminescence are almost identical in AgCl.

11.3 Injection electroluminescence What is meant by the term ‘injection electroluminescence’ is in fact the radiative recombination induced by the injection of minority carriers into a semiconductor p-n junction. Since the description of the rectifying mechanism of a p-n junction and its electrical properties are included in every basic textbook on solid-state physics, we will keep our exposition on this topic to a minimum. In order to get a more detailed description of the effects connected with charge transport and light emission in a semiconductor p-n junction, the reader is referred, e.g. to textbooks [1–4]. The energy band scheme of a semiconductor p-n junction is depicted in Fig. 11.15. If the p and n semiconductors are in contact, the diffusion of electrons from the n region to the p region as well as the diffusion of holes from the p region to the n region occur—without any application of an external bias. The n region thus gets charged with a positive space charge; the p region, on the other hand, charges negatively. An electric ﬁeld, preventing further diffusion of carriers, therefore arises in the vicinity of the interface; this ﬁeld has the direction from the n towards the p region. Thus, a steady state is reached afterwards, Fermi levels are equalized and a potential barrier UD (also

321

322

Electroluminescence

Fig. 11.15 Energy band scheme of a p-n junction (homojunction), i.e. the dependence of the electron energy on the space coordinate x. (a) Separated semiconductors p and n, (b) both parts in contact without applying an external bias, (c) voltage U is applied, the junction is biased in the forward direction, and minority carrier injection and their possible radiative recombination with the majority carriers occur.

called the diffusion potential) sets in, see Fig. 11.15(b). Its electric ﬁeld is localized in a narrow region near the interface, from where all free carriers disappeared because of diffusion. This region is therefore called a depletion layer and its electrical conductivity is substantially lower than the conductivity of unaffected p and n regions. The width of the depletion layer will be denoted as WD . Upon applying a suitable external voltage U (positive polarity on the p region, i.e. the forward direction), the coincidence of the Fermi levels is perturbed, the internal potential barrier decreases to a value (UD –U ) and excess electrons are injected from the n region to the p region. Symmetrically, excess holes are injected into the n region. This ‘mixing’ of high concentrations of minority and majority carriers leads to their recombination and if such recombination is radiative, it gives rise to injection electroluminescence. Before we focus on its closer description, we will sum up the electrical properties of a p-n junction.

11.3.1 Electrical properties of a p-n junction The potential barrier height UD , its width WD and their variations as a function of the applied bias are the determining factors of the behaviour of the p-n junction. For the sake of simplicity, we will assume (as is common in this context) that all dopants, i.e. donors of concentration ND in the n region and acceptors of concentration NA in the p region, are fully ionized, thus

Injection electroluminescence n = ND , p = NA holds for the free electron (n) and hole ( p) concentrations, respectively. We can then expect that the diffusion voltage UD in the depletion layer will be in some way proportional to the concentration of both donors and acceptors; by solving the equations describing the equality of the drift and diffusion currents of electrons and holes (e.g. [24]) one can obtain UD =

k B T NA N D , ln e n 2i

(11.10)

where n i is the intrinsic carrier concentration in the semiconductor under study. The width of the depletion layer WD depends also on the concentrations NA and ND . The higher these concentrations are, the narrower the region of the semiconductor that has to be depleted of free carriers, originating from ionized dopants, in order to form the given diffusion potential UD . Therefore, WD decreases with increasing NA and ND . By applying an external bias in the forward direction, we actually ‘return’ the electrons to the n region and the holes to the p region; consequently, we can expect that WD will decrease with increasing U . The resulting expression has the form

2ε0 εr 1 1 (UD − U ) ( WD = + ). (11.11) e NA ND From this expression it is, among other things, evident that in the case of a different level of doping of the n and p regions the space charge will be concentrated predominantly in the region with a lower concentration of impurities. Naturally, application of the reverse bias (positive polarity on the n region) will have the opposite effect and the depletion layer’s width will increase on √ increasing (absolute value of) the reverse bias as WD ≈ (UD + U ). As the depletion region has a high electrical resistance, the applied bias easily decreases or increases the potential barrier height. As mentioned earlier, under forward bias the electrons and holes are injected as minority carriers into the regions of opposite conductivity type, which makes a current ﬂow across the p-n junction; this current increases with increasing bias. By solving the continuity equation—and taking into account the generation and recombination mechanisms of carriers [24]—it is possible to obtain an expression for the current density (sometimes referred to as the Shockley equation) 1 1 2 exp(eU/kB T − 1) Dp /τp + Dn /τn j = eni ND NA = js exp(eU/kB T − 1).

(11.12)

Here, Dn or Dp stand for the diffusion coefﬁcient of electrons or holes, respectively; τn or τp denote the lifetime of electrons or holes as minority carriers, respectively. If a reverse bias (U = –U < 0) is applied, the approximation exp(eU /kB T ) 1 can be written for a sufﬁciently high absolute value of this bias and eqn (11.12) yields, for this case, a current ﬂowing in the opposite

323

324

Electroluminescence direction, whose magnitude no longer depends on the bias: 1 1 2 = − js. Dp /τp + Dn /τn j = eni ND NA

(11.13)

The current of density js is called the saturation current; it is usually much lower than the forward current. A p-n junction therefore has, as is of course well-known, rectifying properties and is thus the cornerstone of semiconductor diodes. A typical current–voltage characteristic (11.12) in the vicinity of the origin of the coordinate system is shown in Fig. 11.16(a). Equation (11.13) can be rewritten in a slightly different way which very well illustrates the physical meaning of the saturation current. Let us ﬁrst consider that the carrier diffusion length is determined by the relation L n,p = Dn,p τn,p . Then, the left term in parentheses of eqn (11.13) can be expressed as Dp /τp (1/ND ) = L p /(τp ND ). Also, it is known that the square of the intrinsic concentration of carriers in semiconductors is given by the product of the free electron and free hole concentrations (law of mass action), for the n region of the investigated p-n junction we can therefore write n 2i = n n0 p0n ; in this formula, n n0 and p0n stand for the equilibrium densities of electrons or holes in this region, respectively.8

Fig. 11.16 (a) Current–voltage characteristic of a p-n junction calculated in the vicinity of the origin of the coordinate system using expression (11.12). (b) Current–voltage characteristic in the forward direction of p-n junctions manufactured from different semiconductors. Room temperature, arrows mark the corresponding threshold biases. After Schubert [2].

8 We consider the reverse direction. In the forward direction, the injection of minority carriers occurs in the vicinity of the depletion layer, which is a non-equilibrium state and the law of mass action thus cannot be applied.

Injection electroluminescence However, in this region we assumed that n n0 = ND and thus the hole component of the saturation current density will—considering what was just said—be equal to epn L p 1 js(p) = en2i Dp /τp = 0 . ND τp

(11.14)

From this, a microscopic interpretation of the saturation current follows: p0n /τp stands for the number of holes recombining per second; therefore, in steady state it means also the rate of thermal generation of holes. Holes generated in this way diffuse from their place of birth and recombine after travelling a mean distance L p . Consequently, under reverse bias, the electrons in the n region do not contribute to the current at all (do not overcome the potential hill UD + U ); as for the holes, only those generated in a distance shorter than L p from the depletion layer contribute to the current. Similar reasoning can also be applied to the electrons in the p region. The magnitude of the saturation current is therefore driven by the diffusion length and lifetime of minority carriers and the external bias has no impact on it. In the special case of sufﬁciently high forward bias U kB T /e it is possible to further modify (11.12) to j = js exp(eU/kB T ), which, using (11.12) and (11.10) and considering the fact that the voltages UD and U have opposite polarities, gives j = e( Dp /τp NA + Dn /τn ND ) exp((U − UD )/kB T ). (11.15) This expression shows that a signiﬁcant increase of current density in the forward bias does not occur until U ≈ UD . This bias is often referred to as the threshold bias Uth (≈ UD ). Looking at Fig. 11.15(c), one may guess that this increase in current can be expected the moment that the edges of the conduction and valence bands begin to equalize on both sides of the junction, so that the potential barrier almost disappears and the minority carrier injection increases rapidly. Using the same ﬁgure, we can easily see that E g = e(UD − U ) + (E c − E fn ) + eU + (E fp − E v ). In the common case of highly doped semiconductors, the differences (E c − E fn ) and (E fp − E v ) are negligible with respect to the bandgap width E g . Using the previous equation, we obtain UD ≈ Uth ≈ E g /e.

(11.16)

The threshold bias Uth (and also the energy of emitted photons) thus substantially depends on the material from which the p-n junction is manufactured; see Fig. 11.16(b) and also Problem 11/4. To end this subsection we wish to add two notes. The ﬁrst one is related to the Shockley equation (11.12); this equation describes the ideal theoretical current–voltage characteristics of a p-n junction. In order to characterize a real experimental curve, a dimensionaless ideality factor n ideal ≥ 1 is introduced and relation (11.12) gains the form j = js exp(eU/n ideal kB T − 1). For

325

326

Electroluminescence a ‘theoretical’ p-n junction, n ideal = 1 holds true; in real diodes n ideal can reach values up to n ideal = 6. The second note is to point out the facts that commercial electroluminescence (LED) diodes are not based on a simple p-n (homo)junction, which we analysed hitherto and a schematic of which is depicted in Fig. 11.15, but they use the principle of a heterojunction. In heterojunctions, two different semiconductors are in contact: an active (luminescent) region with narrower bandgap (e.g. GaAs) and a barrier region with wider bandgap (Alx Ga1−x As). Such a structure commonly consists of two highly doped barriers—therefore two parts with wider bandgaps—surrounding the central active narrower-gap region, which is usually doped lightly or left completely undoped, see Fig. 11.17. Such a structure is known as a double heterostructure. The double heterostructure introduces two factors that signiﬁcantly improve the luminescence performance of p-n junctions. First, is the spatial localization of the injected electrons and holes in a relatively narrow active region (WDH ≈ 0.1–1 μm, see Fig. 11.17(b)). The material volume in which the radiative recombination occurs is no longer determined by the diffusion length of minority carriers, which can reach values of up to 10–15 μm. An increased concentration of electrons and holes in active region then manifests itself in increased electroluminescence efﬁciency. A second factor is then a waveguiding effect in the active region, which is due to the higher refractive index of semiconductors possessing narrower bandgaps [32]; the whole structure then represents a thin planar waveguide with efﬁcient spatial conﬁnement of the radiant power. As a result, double heterostructures represent a technological base not only for LED diodes but also for semiconductor injection lasers. The optical transparency of the barrier layers—owing to the wider bandgap—for luminescence radiation generated in the active region (i.e. much smaller absorption losses in comparison with homojunctions) can also be put on the list of the beneﬁts of heterojuntions.

Fig. 11.17 Double heterostructure of P-p-N type. (a) Band scheme of the non-interacting components, (b) heterostructure biased in the forward direction.

Injection electroluminescence

327

11.3.2 Intensity, spectral and temporal characteristics of LEDs Nowadays, injection electroluminescence is not (and in fact has never been) a tool for basic research in the sense of obtaining basic information about the mechanisms of radiative recombination in a luminescent material.9 Thus, a treatise on injection electroluminescence goes, to a large degree, beyond the scope of this book, namely teaching the reader to decode the information carried by luminescence radiation (mainly by its spectral composition) about the place and the mechanism of its origin. On the other hand, injection luminescence presents, as we have already pointed out several times, an important application output from the basic research of the optical properties of solids towards electronic devices achieving a direct transformation of electric energy into light. The main application domains of LED diodes emitting in the visible spectral region are light indicators of various colours, and recently also energysaving interior lighting or high-brightness trafﬁc lights. Another wide ﬁeld of application of LED diodes, this time those emitting in the infrared region, is represented by optical telecommunications systems. Let us focus in this subsection on several illustrative examples of the emission characteristics of LED diodes biased in the forward direction. Only data obtained at room temperature will be presented. Intensity characteristics An example of the dependence of the electroluminescence intensity on injection current is shown in Fig. 11.18 [33]. The onset of photon emission is conditioned by reaching the threshold bias ∼ E g /e (although weak luminescence is already observable at lower bias, see also Problem 11/5), and afterwards, a linear increase of the electroluminescence intensity with increasing injection current follows in most cases. An indication of saturation often occurs at higher current values. Saturation can generally be caused by several factors; ﬁrstly, it can indicate an extrinsic origin of the emission: the luminescence labelled as ‘blue’ in Fig. 11.18 is thought to be due to the recombination of donor– acceptor pairs (Section 5.4) in the active InGaN layer doped with silicon and zinc as a substitutional donor and acceptor, respectively. On the other hand, the ‘violet’ emission with maximum at 385 nm originates from band-to-band intrinsic bimolecular recombination in the active layer free from any donor– acceptor pairs and does not exhibit saturation.10 However, saturation can also be caused for example by so-called carrier overﬂow, i.e. leakage of injected carriers from the fully occupied potential well represented by the active layer in the heterostructure. If a markedly superlinear increase of the output power with increasing current occurs when investigating light emission from a laboratory sample of a p-n junction, this probably indicates that an excitation mechanism other than 9 Among many other reasons which we will emphasize soon, this is so because the preparation of high-quality p-n junctions or heterostructures with both sufﬁcient luminescence intensity and durability often goes beyond the capabilities of basic research. 10 The occurrence of injection electroluminescence of various origins at room temperature is, ﬁrst of all, due to the efﬁcient spatial localization of carriers in the heterostructure.

Fig. 11.18 Output light power of double heterostructure InGaN/AlGaN LED diodes as a function of the forward current. After Nakamura et al. [33].

328

Electroluminescence minority carrier injection (e.g. impact ionization in a high electric ﬁeld, see also Section 11.4) is taking place. Spectral characteristics This is the right place to point out that the material basis for the fabrication of commercial LED diodes has undergone a certain evolution since the 1960s. From the beginning of the 1960s, parallel research was conducted by different laboratories, both on light diodes for the visible region prepared from gallium phosphide, GaP (red emission when doped with donor–acceptor pairs, O–Zn, and yellow or green emission when doped with nitrogen, N) and diodes on the basis of GaAs for the near-infrared region (this research was given a signiﬁcant boost by the observation of stimulated emission in a GaAs p-n junction as early as in 1962). These devices were put on the market in the late 1960s. Ternary alloys of GaAs1−x Px appeared shortly afterwards. In the 1980s, AlGaAs alloys were developed for high-brightness red diodes. None of these semiconductor materials, however, was able to cover the blue spectral region. Blue-emitting diodes had been manufactured from silicon carbide, SiC, for some time but their brightness had been low and, moreover, the high temperatures necessary for the synthesis of this material had posed a problem. Then, for a long time hopes were pinned on wide-bandgap II-VI semiconductors, in the ﬁrst place on ZnSe. Although the fundamental problem of suitable doping for reaching p-type conductivity in this material was successfully solved and laboratory samples of light-emitting diodes on the basis of a p-n junction were prepared, fast degradation of these devices as a result of non-radiative recombination on lattice defects prevented their commercial implementation. In the end, mastering the technology of producing high-quality layers of gallium nitride, GaN, and of related ternary compounds (InGaN, AlGaN) for diodes emitting in both the blue and near-ultraviolet region turned out to be a revolutionary solution in the beginning of the 1990s. Consequently, nowadays III-V semiconductors have thus taken over the market with electroluminescence optoelectronic light sources and their research keeps continuing, mainly towards the infrared region to ﬁt the needs of optical communication systems. Figure 11.19 presents examples of normalized emission spectra of LED diodes by different manufacturers. As we mentioned previously, the minimum wavelength λm of the emitted radiation is determined by the bandgap width as λm = hc/E g , however, the injected electrons and holes in most cases do

Fig. 11.19 Normalized emission spectra of LEDs by different manufacturers. Active layers and the corresponding colour perceptions are: (a) GaInN (blue 470 nm), (b) GaInN (green 525 nm), (c) GaP:N (green 565 nm), (d) AlGaInP (red 625 nm) and (e) AlGaAs (infrared 850 nm).

Injection electroluminescence

329

not recombine radiatively via a bimolecular mechanism across the bandgap, but extrinsic luminescence due to donor–acceptor pairs or an exciton bound to an intentionally introduced impurity occurs instead. The maximum of the emission band is then shifted towards longer wavelengths in comparison with λm . Moreover, the emission spectra of LED diodes may be inﬂuenced by light absorption and scattering at impurities and in the materials surrounding the active region, including the plastic encapsulation. The spectral shape is also inﬂuenced (in ternary and quaternary compounds) by broadening of the emission band owing to random ﬂuctuations in the chemical composition of the active layer (so-called alloy broadening). A typical spectral width is 50–100 meV and this increases slightly with increasing current.11 In most cases, the spectra are smooth curves, however, e.g. curve (c) in Fig. 11.19 corresponding to GaP:N is an exception from the rule and demonstrates the fact that gallium phosphate is an indirect-bandgap semiconductor: the short-wavelength peak is often attributed to the emission of the X–TO type and the neighbouring peak to the X–LO process. An indication of structure on the long-wavelength wing corresponds to the so-called NN luminescence due to the recombination of an excited pair of nearest neighour nitrogen atoms. From the physical point of view, the process of how the isoelectronic nitrogen impurity in GaP and GaAs1−x Px radically inﬂuences the luminescence properties of these materials is very interesting (as discussed already in Subsection 7.2.3) and, what is no less important, how substantial the impact of this phenomenon on applications in optoelectronics is. The N impurity together with the variable composition of the ternary GaAs1−x Px compounds contributes to the possibility of continuous tuning of the emission wavelength

Fig. 11.20 Total (external) efﬁciency of injection electroluminescence in GaAs1−x Px as a function of the phosphorus molar fraction x. Symbols stand for experimental data. A sharp decrease of the efﬁciency in the vicinity of x = 50% in GaAs1−x Px without nitrogen is due to the direct → indirect bandgap transformation. Doping with nitrogen compensates to a large degree for this inconvenient effect. After Campbell [34].

11 Typical values of the total efﬁciency of LED diodes η (here also referred to as the external tot efﬁciency) are ηtot = 1–10% and the luminous efﬁciency (i.e. the emitted light ﬂux at an input power of 1 W) is of the order of 10–100 lm/W. Further technical parameters can be found, e.g. in [2].

330

Electroluminescence in the range from about 550 to 690 nm. That is, the bandgap E g and thus the energy of the emitted photon varies with the molar fraction x, this energy being lowered with respect to E g by the localization energy of an exciton at the isoelectronic impurity N. The reabsorption of the emitted radiation is thus signiﬁcantly reduced. Most importantly, however, the presence of the N atoms induces quasi-direct radiative transitions in GaAs1−x Px alloys for x ≥ 0.5, which is a boundary for transformation from direct to indirect bandgaps. These effects are demonstrated in Fig. 11.20 [34]. This is, in fact, one of the ﬁrst practical applications of the Heisenberg uncertainty relations. It might also be of interest to mention also white-emitting LED diodes, which are nowadays a commonly available commodity. White emission can be obtained by means of so-called luminescence converters, i.e. phosphors covering the active p-n junction of a blue LED diode in the form of a thin layer. Blue injection electroluminescence, originating e.g. in an InGaN chip, excites in an appropriately chosen converter photoluminescence emission spectrally located in the green, yellow or red regions. Part of the blue electroluminescence which was not absorbed in the converter leaves the diode and additive colour mixing then invokes a white perception in the human eye. The principle is thus very similar to a classical ﬂuorescent tube containing mercury vapour and phosphor deposited on the inner surface of the tube. A commonly used converter is yttrium-aluminium garnet (YGd)3 (AlGa)5 O12 doped with cerium (YAG:Ce3+ ), which has yellow luminescence. An example of the emission spectrum of such an LED diode is shown in Fig. 11.21. A certain drawback of the YAG:Ce3+ converter is the absence of a red spectral component, resulting in a ‘cold’ white spectrum. In order to achieve ‘warm’ white light (with a yellowish tint), a combination of two converters—YAG:Ce3+ and CaS:Eu2+ —is used. New types of converters on the basis of (oxy)nitrides doped with Ce3+ and Eu2+ , exhibiting almost 100% photoluminescence quantum efﬁciency, are being studied nowadays. Temporal characteristics Upon opening or closing the electrical circuit with an LED diode, transient electronic processes manifest themselves in different temporal behaviours of the current passing through the diode, the diode voltage and the rise or decay of the luminescence emission. These processes are inﬂuenced by a wide range

Fig. 11.21 Emission spectrum of a white LED diode on the basis of GaInN with a YAG:Ce3+ converter. Produced by Nichia Chemical Industries Corporation. After Schubert [2]. This diode already contains a low-dimensional element—one quantum well (Chapter 12).

Injection electroluminescence of factors; apart from the rates of radiative and non-radiative recombinations themselves, electrical parameters and the geometry of the p-n junction as well as of the external circuit have an important role to play. An example is shown in Fig. 11.22 [35]. One can see that, quite logically, the emission of light sets in with a certain delay after the current (about 1.5 μs here): minority carrier injection across the depletion region, possible ﬁlling of the electron and hole traps and carrier capture at active impurities—all these effects take some time. On the other hand, the fact that also the voltage across the diode is delayed after the current can be rather surprising; however, this suggests that a p-n junction represents, to a large extent, a capacitance load for the external source. This capacitance is, moreover, owing to the variable depletion layer width (11.11), dependent on the bias and thus, because of the transient effects, also on time. A simple theoretical description of the curves shown in Fig. 11.22 is then almost impossible. The only thing that can be said here is that the rise of luminescence begins roughly when the voltage approaches its saturated value and that this delay of the light-emission rise time does not depend on the resistance of the external circuit. The speeds of the rise and decay of electroluminescence are of course very important parameters for assessing the suitability of LED diodes to be used in optical communications, when their light emission is directly modulated by the ﬂowing current. In technical practice, the rise in time of the light output under an electric pulsed excitation may be formally described by the relation (see Fig. 11.23(a))

331

Fig. 11.22 Example of temporal behaviour of the characteristic quantities of an LED diode: current, voltage across the diode and the electroluminescence intensity. After Kogan [35].

Ir (t) = I0 (1 − exp(−t/τ1 )) and its decay by Id (t) = I0 exp(−t/τ2 ). Then, it is common to introduce the rise time τr and the decay time τd as time intervals between the points corresponding to the 90% and 10% levels of the

Fig. 11.23 (a) Deﬁnition of the rise time τr and decay time τd of LED-diode emission for the determination of its frequency bandwidth. (b) An example of the frequency response of an LED diode. After Liu [1].

332

Electroluminescence signal, as indicated in Fig. 11.23(a). The bandwidth of the LED frequency response is then deﬁned by means of these quantities. The determination of τr and τd is very simple. Using the deﬁnition of τr we write I0 × 0.1 = I0 (1 − exp(−t10 /τ1 )),

(11.17a)

I0 × 0.9 = I0 (1 − exp(−t90 /τ1 ))

(11.17b)

and from eqn (11.17a) we obtain by elementary adjustments t10 = −τ1 ln 0.9; similarly, it follows from (11.17b) that t90 = −τ1 ln 0.1 and thus τr = t90 − t10 = τ1 ln 9 ∼ = 2.2 τ1 . In a similar way one can get τd = τ2 ln 9 ∼ = 2.2 τ2 .

(11.18)

If we look on the LED diode as a linear system (which is naturally a simpliﬁcation), a transfer function H (ν) can be assigned to the diode; this function is, generally speaking, complex and is equal to the ratio of the output to the input signal as a function of frequency ν. (The function H (ν) is determined via Fourier transformation of the impulse response function.) Because an LED diode is a system characterized by an exponential impulse response exp (–t/τ2 ), its power transfer function reads [36] (p)

HLED (ν) =

1 . 1 + i2πντ2

The upper bound of the diode frequency band is then determined as the (p) frequency at which the modulus of the transfer function |HLED | drops to half of its low-frequency value (the signal level decreases by 3 decibels (dB) because log (1/2) = –0.3 B = –3 dB). This frequency limit (cut-off) ν3dB is thus determined from the condition 1 1 1 + i2πν τ = 2 , 3dB 2

from which we immediately obtain √

ν3dB =

3 , 2πτ2

√ which, using (11.18), yields ν3dB = 3 ln 9/2πτd . If in addition we consider the rising edge with the time constant τr , we obtain √ 1.2 3 ln 9 ∼ ν3dB = . = π(τd + τr ) (τr + τd )

Electroluminescence of a p-n junction

333

For example, if τr = τd = 2 ns, we get ν3dB ∼ = 300 MHz. The cut-off frequencies of LED diodes range from 10 MHz to 1 GHz, see Fig. 11.23(b); higher frequencies of the modulating current cannot be transferred by the diode without substantial distortion.

11.4 Electroluminescence of a p-n junction biased in the reverse direction As early as in the 1950s, a surprising fact was experimentally discovered, namely, that a p-n junction biased even in the reverse direction emits electroluminescence radiation. This kind of behaviour can a priori hardly be expected; after all, the diode is a rectifying element, which almost does not transmit electric current under reverse bias! The relevant emission spectrum was found to be quite broad and located—again unexpectedly—at photon energies substantially exceeding the bandgap width. This was a very unusual observation and if the electroluminescence exhibits any new, speciﬁc mechanism of radiative recombination in comparison with photoluminescence, it is just this emission. Let us devote this short independent section to this amazing effect. The emission electroluminescence spectrum of a reverse-biased p-n junction in silicon and germanium extends to the visible region (Fig. 11.24 [37]). At the same time, it was discovered that this radiation originates ﬁrst in the isolated spots in the close vicinity of the junction area, and with increasing reverse bias these spots merge into a single homogeneous emitting area. The explanation of this effect is based on the close link between electroluminescence and the electrical (pre-)breakdown of a reverse-biased p-n junction, as depicted in Fig. 11.25(a). At reverse bias, as we know, the ‘correct injection’ of carriers, i.e. the injection of electrons from the n region to the p region and of holes from the p region to the n region, cannot be achieved. The saturation current across the junction arises from thermally generated minority carriers on both sides of the junction. They at ﬁrst diffuse towards the depletion region, are dragged in its high electric ﬁeld and ﬁnally are accelerated in this ﬁeld. Then, processes emerge there which we met earlier in avalanche diodes (Section 2.2) or when

Fig. 11.24 Electroluminescence spectrum of a silicon p-n junction, biased in the reverse direction at room temperature. The spectrum is corrected for reabsorption in the material. The position of the bandgap E g is marked. The inset shows an example of the dependence of the overall intensity of this light emission on the current density across the junction. After Newman [37].

334

Electroluminescence discussing the mechanisms of high-ﬁeld electroluminescence: an accelerated electron or hole ionizes the lattice, a free e–h pair is created and an avalanchelike increase in the number of free carriers evolves. The current is increasing substantially; however—as the total number of the carriers taking part in this process is low—the total electric breakdown and device destruction do not occur, provided the bias does not exceed a critical value. Electron–hole pairs with substantial excess energy gained by the acceleration can, naturally, recombine radiatively. Several mechanisms of this recombination have been proposed in the course of time (band-to-band recombination of hot electrons and holes, bremsstrahlung of the electrons corresponding to transitions within the conduction band, recombination of holes within the valence band). Nowadays, it is widely believed that the luminescence photons are created via the band-to-band recombination of hot e–h pairs (Fig. 11.25(b)); various estimates of the effective carrier temperature in Si yield values between 3800 and 7500 K. Such a high effective temperature is exactly what underlies the speciﬁcity of this recombination mechanism, because the recombination of such carriers does not commonly occur in the steady-state electroluminescence (let alone photoluminescence) regime. In the case of photoluminescence excited high up into the bands it is the high rate of thermalization of hot carriers which prevents such recombination from taking place. In high-ﬁeld electroluminescence, conditioned by impact excitation of the impurity ions in phosphors of ZnS:Mn2+ type, the energy of the accelerated electrons is effectively lost in collisions with the active impurity ions and thus photons with energy higher than E g do not appear in the emission spectra either.12

Fig. 11.25 Light emission in a reverse biased p-n junction. (a) The current–voltage characteristic; (b) energy band scheme which demonstrates current ampliﬁcation due to impact ionization and depicts radiative recombination of an e–h pair giving hν > E g .

12 Calculations and various experiments show that the threshold kinetic energy E for the th generation of a free e–h pair by impact excitation across the bandgap is in common semiconductors appreciably higher than E g . Estimates give E th ≈ 1.2 eV for silicon. This means that the emission spectrum should begin to decrease rapidly for the energy of emitted photons hν = (E th + E g ) ≈ 2.3 eV. This is in agreement with Fig. 11.24. In ZnS, ﬁeld-accelerated electrons can hardly achieve the high threshold energy E th > E g ≈ 3.7 eV, as we already mentioned in Subsection 11.2.2.

Electroluminescence of a p-n junction

335 Fig. 11.26 Electroluminescence spectrum of a commercial GaAs LED diode biased in the reverse direction. The dip at ∼ 1.9 eV is an experimental artefact. After Lahbabi et al. [38]. (b) Corresponding interband recombination of hot carriers in the band scheme of GaAs. The emission band denoted A arises from direct transitions at the point (6 —8 ), and the B band is due to the indirect recombination of electrons from the local minimum of the conduction band L 6 with holes in 8 .

In silicon, indirect band-to-band recombination of the e–h pairs (with phonon assistence) occurs, otherwise the spectrum would have to contain photons with energy higher than the direct forbidden gap E gd (15 − 25 ) ≈ 3 eV. In p-n junctions made of GaAs, the emission spectrum contains a component due to both direct and indirect interband transitions of hot electrons and holes (Fig. 11.26), which is the result of the speciﬁc GaAs band structure [38]. The random and highly nonlinear character of avalanche ionization is reﬂected also in the intensity dependence of electroluminescence, which can, in a log-log scale, show high values of the slope as well as breaks on the curve (inset in Fig. 11.24). The message for basic research is then: if a markedly nonlinear intensity dependence of electroluminescence occurs in an experiment performed on a sample of a new material (whose thin layer is surrounded by—not very well characterized—oxide barriers, metal electrodes, a covering layer, etc.), it is always necessary to think of the occurrence of avalanche (pre-) breakdown in one of the involved reverse biased depletion layers. Although the total efﬁciency of this electroluminescence is very low (∼ 10−6 %), it does not pose any problem for contemporary highly sensitive photodetectors and even various potential applications of this electroluminescence have been proposed. Most important is the luminescence emission microscopy of these devices, i.e. the connection of the microscopic monitoring of semiconductor devices (with high spatial resolution) with the spectral investigation of electroluminescence arising in different zones of both discrete elements and silicon CMOS integrated circuits. That is, the discussed light emission is not restricted, as it could perhaps seem from the previous explanation, only to standard electric or LED diodes, but it occurs also in other p-n barriers and similar structures, whose miniature dimensions themselves naturally lead to high electric ﬁelds: in memory integrated circuits, the conductive channel of MOSFET transistors, etc. In this way, the phenomenon makes it possible for us to monitor optically the homogeneity of details, prebreakdown states in the diodes and transistors and to analyse their causes, to test integrated circuits, etc. More information can be obtained in the review articles [39, 40]. Impact electroluminescence in the region of avalanche breakdown, for instance, contributed to a large extent to the discovery of rapid crystallization of hydrogen-rich a-Si:H, induced by local electric breakdown in p-i-n structures [41].

336

Electroluminescence Finally, let us brieﬂy mention one more thing, namely the dynamics of this impact electroluminescence. Obviously, it must be a very fast luminescence process (even in silicon) because it is the hot carriers in highly non-equilibrium states that are recombining. This opens up the possibility of manufacturing a fast pulsed LED diode, destined, e.g. for the above-mentioned diagnostic purposes [40]. Systematic steps in this direction have been missing for a long time. Recently, however, a report on the laboratory realization of such a diode has appeared [42].

11.5 Problems 11/1: Unlike semiconductors, hot electrons do not occur in metals. Try to explain qualitatively why this is so. 11/2: Show that the saturation drift velocity of hot electrons is vsd = (h¯ ω0 /m e )1/2 , where h¯ ω0 is the optical phonon energy and m e is the effective electron mass. Using typical values of h¯ ω0 = 40 meV and m e = 0.1m 0 , one obtains vsd ∼ = 2 × 107 cm/s. Hint: assume that in high electric ﬁelds F, the rate of electron energy increase is fully compensated by the energy loss rate owing to the emission of optical phonons, thus dE/dt = eFvs − h¯ ω0 /τen , where τen is the energy relaxation time. Write an analogous equation also for the electron quasimomentum m e vs . See also [19]. 11/3: By virtue of the energy band structure of Si and Ge (e.g. Fig. 7.16), discuss the suitability of these semiconductors for possible infrared luminescence panels based on high-ﬁeld electroluminescence (impact excitation and ionization). 11/4: One might conclude from Fig. 11.15(c) that total equalization of the band edges occurs upon increasing the forward bias up to the value U = UD , the depletion layer then completely disappearing (WD = 0, see relation (11.11)). In other words, this would mean that the full voltage equal to E g /e will be applied to the junction at that moment. This situation, however, cannot in fact be achieved; considering the widths of the forbidden gaps of the most common semiconductors at room temperature to be E g (Ge) ≈ 0.67 eV, E g (Si) ≈ 1.12 eV and E g (GaAs) ≈ 1.425 eV, this fact is illustratively depicted in Fig. 11.16(b). Explain qualitatively the reason for this. 11/5: Electroluminescence in a forward biased p-n junction emerges already at very low currents when the bias applied to the junction is lower than the threshold voltage ≈ E g /e. This means that the barrier of the junction is overcome by a small fraction of electrons (or holes) with energy high above the bottom of the conduction band or below the top of the valence band, respectively (Fig. 11.27). These charge carriers gain their energy from the lattice. The release of this energy in the form of photons then, of course, leads to inevitable cooling of the close vicinity of the junction. Discuss this effect after [43] or [44]. 11/6: Figure 11.26 shows electroluminescence spectra of a reverse biased LED diode manufactured from GaAs. Some of the recombining hot

References

337

Fig. 11.27

electrons originating during the avalanche diode breakdown are localized at the absolute minimum of the conduction band at the point (A emission band) and, at the same time, others can be found in the local minimum at the L point (B emission band). Theoretical modelling of the experimental emission spectra yields the effective temperature TefA of electrons at the minimum to be much lower than the temperature TefB of the electrons at the L minimum [38]. This contradicts the intuitive concept, namely, that the electrons should be hotter in the electric ﬁeld owing to their lower effective mass (m = 0.064 m 0 , m L ≈ 0.22 m 0 ) and thus their higher mobility. Explain this apparent contradiction.

References 1. Liu, J.-M. (2005). Photonic Devices. Cambridge University Press, Cambridge. 2. Schubert, E. F. (2003). Light-Emitting Diodes. Cambridge University Press, Cambridge. 3. Moss, T. S., Burrell, G. J., and Ellis, B. (1973). Semiconductor Opto-Electronics. Butterworth, London. 4. Carroll, J., Whiteaway, J., and Plumb, D. (1998). Distributed Feedback Semiconductor Lasers. IEE Circuits, Devices & Systems series, Vol. 10. The Institution of Electrical Engineers/SPIE Optical Engineering Press, London. 5. Destriau, G. (1936). J. de Chim. Phys., 33, 597. 6. Lehovec, K., Accardo, C. A., and Jamgochian, E. (1951). Phys. Rev., 83, 603. 7. Haynes, J. R. and Briggs, H. B. (1952). Phys. Rev., 86, 647. 8. Losev, O. (1928). Phil. Mag., 6, 1024. 9. Zheludev, N. (2007). Nature Photonics, 1, 189. 10. Dekker, A. J. (1963). Solid State Physics. Prentice-Hall, Englewood Cliffs, N.J. 11. Keyes, R. J. and Quist, T. M. (1962). Proc. IRE, 50, 1822. 12. Rediker, R. H. (2000). IEEE J. Selected Topics Quant. Electron., 6, 1355. 13. Grimmeiss, H. G. and Allen, J. W. (2006). J. Non-Crystal. Solids, 352, 871. 14. Henisch, H. K. (1962). Electroluminescence. Pergamon Press, Oxford. 15. Sah, C.-T. (1991). Fundamentals of Solid-State Electronics, World Scientiﬁc, Singapore. 16. Gumlich, H.-E., Zeinert, A., and Mauch, R. (1998). Electroluminescence. In Luminescence of Solids (ed D. R. Vij), p. 221. Plenum Press, New York. 17. Tanaka, S., Kobayashi, H., and Sasakura, H. (1999). Fundamentals of luminescence. In Phosphor Handbook (ed. S. Shionoya and W. M. Yen), p. 123. CRC Press, Boca Raton. 18. Blakemore, J. S. (1985). Solid State Physics. Cambridge University Press, Cambridge. 19. Yu, P. Y. and Cardona, M. (1996). Fundamentals of Semiconductors. Springer, Berlin. 20. Luo, W., Ismail-Beigi, S., Cohen, M. L., and Louie, S. G. (2002). Phys. Rev. B, 66, 195215.

338

Electroluminescence 21. Allen, J. W. (1989). Developments in the theory of electroluminescence mechanisms. In Electroluminescence. Proceedings of the Fourth International Workshop (ed. S. Shionoya and H. Kobayashi), Springer Proceedings in Physics Vol. 38, p. 10. Springer, Berlin. 22. Sze, S. M. (1981). Physics of Semiconductor Devices. 2nd edn. John Wiley, New York. 23. Kasap, S. and Capper, P., eds. (2006). Springer Handbook of Electronic and Photonic Materials, Chap. 29. Springer Science and Business Media, New York. 24. B¨oer, K. W. (1992). Survey of Semiconductor Physics. Volume II: Barriers, Junctions, Surfaces, and Devices. Van Nostrand Reinhold, New York. 25. Zalm, P. (1956). Philips Res. Rep., 11, Part I p. 353, Part II p. 417. 26. Thornton, W. A. (1961). Phys. Rev., 122, 58. 27. Destriau, G. and Loudette, P. (1940). J. Phys. Rad., 1, 51. 28. Linnros, J. and Lalic, N. (1995). Appl. Phys. Lett., 66, 3048. 29. Tanaka, S. (1988). J. Luminescence, 40&41, 20. 30. Tanaka, S. (1990). J. Crystal Growth, 101, 958. 31. Vacek, K. (1967). phys. stat. sol., 23, 105. 32. Moss, T. S. (1985). phys. stat. sol. (b), 131, 415. 33. Nakamura, S., Pearton, S., and Fasol, G. (2000). The Blue Laser Diode. The Complete Story. Springer, Berlin. 34. Campbell, J. C. (1974). J. Appl. Phys., 45, 4543. 35. Kogan, L. M. (1983). Semiconductor Light Emitting Diodes (in Russian: Poluprovodnikovyje svetoizluajuˇsije diody). Energoatomizdat, Moscow. 36. Saleh, B. E. A. and Teich, M. C. (1991). Fundamentals of Photonics. John Wiley, New York. 37. Newman, R. (1955). Phys. Rev., 100, 700. 38. Lahbabi, M., Ahaitouf, A., Fliyou, M., Abarkan, E., Charles, J.-P., Bath, A., Hoffmann, A., Kerns, S. E., and Kerns, D. V., Jr. (2004). J. Appl. Phys., 95, 1822. 39. Deboy, G. and K¨olzer, J. (1993). Semicond. Sci. Technol., 9, 1017. 40. Kramer, J., Seitz, P., Steigmeier, E. F., Auderset, H., Delley, B., and Baltes, H. (1993). Sensors and Actuators A, 37–38, 527. 41. Luterov´a, K., Pelant, I., Fojt´ık, P., Nikl, M., Gregora, I., Koˇcka, J., Dian, J., Mal´y, ˇ ep´anek, J., Poruba, A., and Horv´ath P. (2000). Phil. Mag. B, 80, P., Kudrna, J., Stˇ 1811. 42. Kuai, S. and Meldrum, A. (2009). Physica E, 41, 916. ˇ cˇ as. fyz. (in Czech), 7, 246. 43. Tauc, J. (1957). Cs. 44. Dousmanis, G. C., Mueller, C. W., Nelson, H., and Petzinger, K. G. (1964). Phys. Rev., 133, A316.

Electronic structure and luminescence of low-dimensional semiconductors All the previous chapters described in detail the luminescence properties of the so-called ‘bulk’ semiconductors, either crystalline or amorphous. This term applies to materials which are in principle homogenous and whose dimensions (in all directions) are substantially larger than the exciton Bohr radius. The properties of such bulk semiconductor samples are determined by their chemical composition, crystalline structure, and certainly also by structural defects and impurities. The number of stable, ‘natural’ semiconducting materials, which can be grown, investigated, and prospectively exploited in electronics and optoelectronics is somewhat limited to, let us say, 30 or so. In addition to that, however, a tempting approach to change the discrete spectrum of available semiconductor properties into a nearly continuous spectrum exists. To start with, the de Broglie wavelength of electrons λe and holes λh in semiconductors as well as the Bohr radius of Wannier excitons aX (typically 1–10 nm) are fortunately many times larger than the lattice constant of the corresponding semiconductor crystal (typically 0.5–0.6 nm). Therefore, it is in principle possible to decrease the size of the crystal (in one or more directions) down to a size comparable to (or even smaller than) the Bohr radius of an exciton while keeping the basic structure of the semiconductor crystal unaltered. In such a spatially conﬁned crystal, its ‘chemically determined’ electronic states become dependent on its size—the so-called quantum conﬁnement effect sets in. The principle of quantum conﬁnement lies in the quantization of the kinetic energy of a quasi-particle whose motion is restricted to a region comparable with its de Broglie wavelength. Thanks to the advanced semiconductor technology and the highly developed theoretical models in the semiconductor ﬁeld, it is now possible to fabricate structures with custom-designed properties tailored to speciﬁc applications. Such procedures are sometimes referred to as quantum engineering or band engineering. Starting from the end of the 1980s, semiconductor research gradually diverted away from bulk semiconductors, which are almost perfectly understood, to the investigation of low-dimensional semiconductor structures. As this chapter is of fundamental importance for the further comprehension of luminescence properties and the application potential of semiconductor nanostructures, which are the subject of the remainder of the book, we shall

12 12.1 Basic types of low-dimensional semiconductors

340

12.2 Density of states in low-dimensional semiconductors

344

12.3 Quantum wells (layers)—two-dimensional semiconductors

347

12.4 Quantum wires

359

12.5 Quantum dots—nanocrystals 363 12.6 Exciton–phonon interaction. Phonon bottleneck 371 12.7 Some special phenomena

374

12.8 Problems

378

340

Low-dimensional semiconductors have to delve deeper into the theory of the electronic energy structure and optical properties of low-dimensional semiconductors. However, we will put aside other aspects, such as the important ﬁeld of electrical transport properties. The reader can ﬁnd more details in a number of monographs and textbooks which are currently available and cover the whole ﬁeld. We can recommend the textbook by Davies as an excellent introductory treatise [1].

12.1 Basic types of low-dimensional semiconductors

Fig. 12.1 Basic types of low-dimensional semiconductor nanostructures characterized by the number of dimensions which are restricted to the size where quantum conﬁnement effects start to play an important role.

Primarily, low-dimensional semiconductors can be divided into groups according to the number of dimensions in which the characteristic size is small enough to ﬁt into the quantum conﬁnement limit. The structures conﬁned in one, two or three dimensions are called quantum layers (or quantum wells), quantum wires, and quantum dots or nanocrystals, see Fig. 12.1. Alternatively, we can speak of ‘quasi-’ two-dimensional (2D), one-dimensional (1D) and zero-dimensional (0D) structures, in contrast to a bulk, three-dimensional (3D) material. As mentioned above, the quantum-conﬁnement effect sets in if the structures under consideration have dimensions on the order of tens of nanometres or less, which means that the fabrication technology for preparing such materials belongs to the area of nanotechnologies. These technologies are based on the application of two approaches: a synthesis of materials in the ‘bottom-up’ direction and the patterning of materials in the ‘top-down’ direction. Bottom-up growth is a chemistry-based procedure of the synthesis of the desired material from appropriate precursors. In contrast to conventional technologies, the size of the growing structure needs to be controlled so that the growth can be terminated in due time. The top-down disintegration process again proceeds chemically, when chunks of the original material are transformed from the initial solid structure to a mobile phase (gas or liquid) and removed. Most frequently, various types of lithographic techniques are applied; in these procedures, a mask typically protects parts of the surface from erosion, giving rise to nano-patterned structures. In fact, lithography is the basic method for the fabrication of semiconductor integrated circuits. However, in the case of nanostructures, the masks have to be accurate with nanometric accuracy, indicating that conventional optical lithography cannot be employed (as its wavelength is of the order of hundreds of nanometres) but electron-beam or ion-beam lithography (or perhaps a scanning tunnelling microscope) needs to be exploited.

12.1.1 Semiconductor heterostructures Low-dimensional semiconductor structures usually do not contain a single type of material conﬁned into small dimensions but they tend to combine several types of semiconductors (or even metals and insulators) of various composition. The reasons for this are multiple: (i) the need for passivation and

Basic types of low-dimensional semiconductors

341

protection of the nanostructured surface by another material; (ii) embedding of a nanostructure into a macrostructure, which is, in contrast to a nanostructure, suitable for manipulation; and (iii) the necessity to fabricate the appropriate energy structure, which meets the functionality requirements put on the low-dimensional structure. Such compound materials are commonly referred to as heterostructures. The simplest example of a low-dimensional heterostructure is a quantum well—a small segment of a semiconductor (thin layer, spherical nanocrystal, etc.) surrounded by a different semiconductor with wider bandgap. Excited electrons and holes (excitons) are localized in the corresponding extremes of the conduction or valence band, i.e. inside the quantum well, which is constituted by a semiconductor with a narrower bandgap. The surrounding material with wider bandgap acts as a potential barrier. The basic technologies for the fabrication of such semiconductor heterostructures are epitaxial methods for thin-ﬁlm depositions. During epitaxial deposition, one type of semiconductor is deposited onto a (typically) crystalline substrate of the same (homoepitaxy) or a different (heteroepitaxy) semiconductor. The growing semiconductor chemically bonds to atoms of the substrate, thus accepting its crystalline structure. Consequently, heteroepitaxy is well suited only to the combinations of semiconductors with the same crystalline structure, appropriate lattice match and similar properties of chemical bonds. If a semiconductor is forced to grow on a structure much different from its natural form, mechanical strain is introduced into the growing layer. When the layer exceeds a certain critical thickness, the strain is relaxed through the formation of structural defects (see Fig. 12.2 [2]). Strain in a heterostructure induces changes in the semiconductor band structure, which can sometimes be constructively exploited for proper engineering of the energy structure of the device. Other subtypes of low-dimensional heterostructures include the so-called multiple quantum wells, i.e. several quantum wells side by side. If the number of neighbouring quantum wells is very large (the order of hundreds) and the barriers in between them are very thin, so-called superlattices arise. Due to the thin potential barriers, the wavefunctions of carriers in neighbouring quantum

Fig. 12.2 Simpliﬁed scheme of epitaxial growth of a ZnSe layer on a GaAs substrate. The epitaxial layer is strained due to the lattice mismatch (∼ 0.27%) and the difference in thermal expansion coefﬁcients of the two materials. When the layer becomes thicker than a certain critical thickness (around 150 nm in this case), the strain is released as a result of forming dislocations; a layer with a thickness of about 1 μm is already fully relaxed. Adapted from Yao et al. [2].

342

Low-dimensional semiconductors

Fig. 12.3 Overview of semiconductor materials sorted by their low-temperature lattice constants and bandgap values. The materials forming stable alloys are connected by lines. White circles and dashed lines indicate indirect-bandgap materials, while black circles and solid lines denote direct-bandgap materials. (The negative bandgap values in HgS, HgSe, and HgTe signify that these materials are near the border between metals and semiconductors.) The grey vertical rectangles highlight groups of materials with close lattice constants, suitable for the fabrication of heterostructures. Adapted from Davies [1] and Yu and Cardona [4].

wells signiﬁcantly overlap, thus allowing for tunnelling between wells. This means that a brand new energetic band structure, together with speciﬁc electric transport properties, emerges. The most important epitaxial techniques are molecular beam epitaxy (MBE), liquid phase epitaxy (LPE), metal-organic chemical vapour deposition (MOCVD), and metal-organic vapour-phase epitaxy (MOVPE). A description of these techniques is beyond the scope of this book, and the reader is referred to, for example, the monograph by Kelly [3]. What kind of materials can be combined in heterostructures and how broad is the range? The range is indeed plentiful, as is illustrated in Fig. 12.3, which displays the lattice constants and bandgaps of the most common semiconductors and their alloys [1, 4]. The archetypal example of a ‘traditional’ hetero-system is deﬁnitely GaAs–Alx Ga1−x As, which has negligible lattice mismatch and which was the cornerstone of the ﬁrst operating devices with heterojunctions.1

12.1.2 Basic types of quantum-well heterostructures Now, we will inspect the electronic energy levels in heterostructures in more detail. The essential factor which determines the properties of a heterostructure is the relative shift between the conduction and the valence bands, the so-called band offset. A ﬁrst estimate of band offsets can be obtained by applying the Anderson rule, which states that the vacuum levels of both materials connected 1 Interestingly, AlAs is an indirect semiconductor, chemically unstable and reacts with air moisture. As a result of lucky chance, it was found that the Alx Ga1−x As alloy is stable enough and, moreover, it has a direct bandgap for x < 0.45. This discovery opened the door to heterostructure devices towards the end of the 1960s. Alferov and Kroemer were awarded half the Nobel Prize in physics in 2000 for the development of semiconductor heterostructures.

Basic types of low-dimensional semiconductors

343

Fig. 12.4 Basic types of quantum wells and illustration of the band-offset calculation from electron afﬁnities—the Anderson rule: (a) type I, (b) type II, and (c) type IIb, sometimes called type III.

in a heterojunction must be aligned, as illustrated by Fig. 12.4(a). Let the two interconnected semiconductors A and B have electron afﬁnities (i.e. the energy required to release an electron from the bottom of the conduction band into vacuum—out of the crystal) χ A , χ B and bandgap widths E gA , E gB . Then, the conduction and valence band offsets E c and E v are given by E c = χ A − χ B , E v = E gB − E gA − E c = E g − E c . For example, GaAs and Al0.3 Ga0.7 As have electron afﬁnities 4.07 and 3.74 eV, respectively, and the difference in bandgap widths is E g = 0.37 eV. Consequently, the offsets are E c = 0.33 eV for the conduction bands and only E v = 0.04 eV for the valence bands. Sometimes, a relative offset of the conduction band with respect to the bandgap is introduced as the factor Q = E c /E g . For the above example, we obtain Q 0.89. However, in real heterostructures, the situation tends to be more complicated; experiments revealed that Q = 0.62 for GaAs/Alx Ga1−x As with x < 0.45. The exact determination of band offsets in a heterostructure is quite difﬁcult, in contrast to the measurement of bandgap widths (the values of which can be obtained for example from optical absorption data). Quantum wells may be divided into two basic groups, according to their band offsets. If the minimum of the conduction band and the maximum of the valence band are both situated in the same layer, we speak of a quantum well of the ﬁrst type (Fig. 12.4(a)). If, on the other hand, these extremes lie in different (neighbouring) layers (materials), it is a so-called quantum well of the second type (Fig. 12.4(b)), whose energy structure reminds as of that of an indirectbandgap semiconductor. However, here the band extremes are not misaligned in k-space, but in real space, implying that electrons and holes are spatially separated. A special case of the type II structure arises when the conduction and valence bands of neighbouring materials partially overlap (Fig. 12.4(c)). Then, the neighbouring materials can freely exchange electrons and holes until equilibrium due to induced local ﬁelds is reached (similarly to p-n junctions). Such structures are sometimes referred to as quantum wells of the third type.

344

Low-dimensional semicon